268 22 15MB
English Pages 701 Year 2006
Marius Grundmann The Physics of Semiconductors
Marius Grundmann
The Physics of Semiconductors An Introduction Including Devices and Nanophysics
With 587 Figures, 6 in Color, and 36 Tables
123
Marius Grundmann Institut für Experimentelle Physik II Universität Leipzig Linnéstraße 5 04103 Leipzig email: [email protected]
Library of Congress Control Number: 2006923434
ISBN10 354025370X Springer Berlin Heidelberg New York ISBN13 9783540253709 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com © SpringerVerlag Berlin Heidelberg 2006 Printed in Germany The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: ProtagoTEXProduction GmbH, Berlin Production: LETEX Jelonek, Schmidt & Vöckler GbR, Leipzig Cover design: eStudio Calamar S.L., F. SteinenBroo, Pau/Girona, Spain Printed on acidfree paper
57/3100/YL
543210
To Michelle, Sophia Charlotte and Isabella Rose
Preface
Semiconductor devices are nowadays commonplace in every household. In the late 1940s the invention of the transistor was the start of a rapid development towards ever faster and smaller electronic components. Complex systems are built with these components. The main driver of this development was the economical beneﬁt from packing more and more wiring, transistors and functionality on a single chip. Now every human is left with about 100 million transistors (on average). Semiconductor devices have also enabled economically reasonable ﬁberbased optical communication, optical storage and highfrequency ampliﬁcation and have only recently revolutionized photography, display technology and lighting. Along with these tremendous technological developments, semiconductors have changed the way we work, communicate, entertain and think. The technological sophistication of semiconductor materials and devices is progressing continuously with a large worldwide effort in human and monetary capital, partly evolutionary, partly revolutionary embracing the possibilities of nanotechnology. For students, semiconductors offer a rich, diverse and exciting ﬁeld with a great tradition and a bright future. This book is based on the two semester semiconductor physics course taught at Universit¨ at Leipzig. The material gives the students an overview of the subject as a whole and brings them to the point where they can specialize and enter supervised laboratory research. For the interested reader some additional topics are included in the book that are taught in subsequent, more specialized courses. The ﬁrst semester contains the fundamentals of semiconductor physics (Part I – Chaps. 1–17). Besides important aspects of solidstate physics such as crystal structure, lattice vibrations and band structure, semiconductor speciﬁcs such as technologically relevant materials and their properties, electronic defects, recombination, hetero and nanostructures are discussed. Semiconductors with electric polarization and magnetization are introduced. The emphasis is put on inorganic semiconductors, but a brief introduction to organic semiconductors is given in Chap. 16. In Chap. 17 dielectric structures are treated. Such structures can serve as mirrors, cavities and microcavities and are a vital part of many semiconductor devices. The second part (Part II – Chaps. 18–21) is dedicated to semiconductor applications and devices that are taught in the second semester of the
VIII
Preface
course. After a general and detailed discussion of various diode types, their applications in electrical circuits, photodetectors, solar cells, lightemitting diodes and lasers are treated. Finally, bipolar and ﬁeldeffect transistors are discussed. The course is designed to provide a balance between aspects of solidstate and semiconductor physics and the concepts of various semiconductor devices and their applications in electronic and photonic devices. The book can be followed with little or no preexisting knowledge in solidstate physics. I would like to thank several colleagues for their various contributions to this book, in alphabetical order (if no aﬃliation is given, from Universit¨ at Leipzig): Klaus Bente, Rolf B¨ ottcher, Volker Gottschalch, Axel Hoffmann (Technische Universit¨ at Berlin), Alois Krost (OttovonGuericke Universit¨at Magdeburg), Michael Lorenz, Thomas Nobis, Rainer Pickenhain, HansJoachim Queisser (MaxPlanckInstitut f¨ ur Festk¨ orperforschung, Stuttgart), Bernd Rauschenbach (LeibnizInstitut f¨ ur Oberﬂ¨ achenmodiﬁzierung, Leipzig), Bernd Rheinl¨ ander, Heidemarie Schmidt, R¨ udiger SchmidtGrund, Mathias Schubert, Gerald Wagner, Holger von Wenckstern, Michael Ziese, and Gregor Zimmermann. Their comments, proof reading and graphic material improved this work. Also, numerous helpful comments from my students on my lectures and on preliminary versions of the present text are gratefully acknowledged. I am also indebted to many other colleagues, in particular to (in alphabetical order) Gerhard Abstreiter, Zhores Alferov, Levon Asryan, G¨ unther Bauer, Manfred Bayer, Immanuel Broser, J¨ urgen Christen, Laurence Eaves, Ulrich G¨ osele, Alfred Forchel, Manus Hayne, Frank Heinrichsdorff, Fritz Henneberger, Detlev Heitmann, Robert Heitz† , Nils Kirstaedter, Fred Koch, Nikolai Ledentsov, Evgeni Kaidashev, Eli Kapon, Claus Klingshirn, J¨ org Kotthaus, Axel Lorke, Anupam Madhukar, Bruno Meyer, David Mowbray, Hisao Nakashima, MatsErik Pistol, Fred Pollak, Volker Riede, Hiroyuki Sakaki, Lars Samuelson, Vitali Shchukin, Maurice Skolnick, Oliver Stier, Robert Suris, Volker T¨ urck, Konrad Unger, Victor Ustinov, Leonid Vorob’jev, Richard Warburton, Alexander Weber, Eicke Weber, Peter Werner, Ulrike Woggon, Roland Zimmermann and Alex Zunger, with whom I have worked closely, had enjoyable discussions with and who have posed questions that stimulated me. I reserve special thanks for Dieter Bimberg, who supported me throughout my career. I leave an extra niche – as the Romans did, in order not to provoke the anger of a God missed in a row of statues – for those who had an impact on my scientiﬁc life and that I have omitted to mention. Leipzig, January 2006
Marius Grundmann
Contents
Abbreviations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .XXI Symbols . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .XXVII .. Physical Constants . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .XXXI . 1
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Timetable . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Nobel Prize Winners . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 General Information . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
1 1 7 9
Part I Fundamentals 2
Bonds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Covalent Bonds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.1 ElectronPair Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.2 sp3 Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.3 sp2 Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Ionic Bonds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4 Mixed Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5 Metallic Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6 vanderWaals Bond . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7 Hamilton Operator of the Solid . . . . . . . . . . . . . . . . . . . . . . . . .
15 15 15 15 15 19 21 23 25 26 27
3
Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Crystal Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Lattice . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.1 Unit Cell . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.2 Point Group . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.3 Space Group . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.4 2D Bravais Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.5 3D Bravais Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.6 Polycrystalline Semiconductors . . . . . . . . . . . . . . . . . .
29 29 29 30 30 31 33 34 34 39
X
Contents
3.3.7 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . Important Crystal Structures . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Rocksalt Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 CsCl Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.3 Diamond Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.4 Zincblende Structure . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.5 Wurtzite Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.6 Chalcopyrite Structure . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.7 Delafossite Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.8 Perovskite Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.9 NiAs Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Polytypism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Reciprocal Lattice . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.1 Reciprocal Lattice Vectors . . . . . . . . . . . . . . . . . . . . . . 3.6.2 Miller Indices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.3 Brillouin Zone . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.1 Random Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.2 Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.3 Virtual Crystal Approximation . . . . . . . . . . . . . . . . . . 3.7.4 Lattice Parameter . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.5 Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
39 40 41 41 41 42 43 45 46 48 48 48 50 51 52 54 54 55 57 59 59 61
4
Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Point Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Thermodynamics of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 Stacking Faults . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6 Grain Boundaries . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7 Antiphase and Inversion Domains . . . . . . . . . . . . . . . . . . . . . . . 4.8 Disorder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
63 63 63 65 67 71 72 73 76
5
Mechanical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Lattice Vibrations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Monoatomic Linear Chain . . . . . . . . . . . . . . . . . . . . . . 5.2.2 Diatomic Linear Chain . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.3 Lattice Vibrations of a ThreeDimensional Crystal . 5.2.4 Phonons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.5 Localized Vibrational Modes . . . . . . . . . . . . . . . . . . . . 5.2.6 Phonons in Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.7 Electric Field Created by Optical Phonons . . . . . . . . 5.3 Elasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Stress–Strain Relation . . . . . . . . . . . . . . . . . . . . . . . . .
77 77 77 77 80 84 86 87 89 91 94 94
3.4
3.5 3.6
3.7
Contents
5.3.2 Biaxial Strain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.3 ThreeDimensional Strain . . . . . . . . . . . . . . . . . . . . . . 5.3.4 Substrate Bending . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.5 Scrolling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.6 Critical Thickness . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Cleaving . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
99 100 102 103 105 109
Band Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Bloch’s Theorem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 FreeElectron Dispersion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Kronig–Penney Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Electrons in a Periodic Potential . . . . . . . . . . . . . . . . . . . . . . . . 6.5.1 Approximate Solution at the Zone Boundary . . . . . . 6.5.2 Solution in the Vicinity of the Zone Boundary . . . . 6.5.3 Kramer’s degeneracy . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6 Band Structure of Selected Semiconductors . . . . . . . . . . . . . . 6.6.1 Silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.2 Germanium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.3 GaAs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.4 GaP . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.5 GaN . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.6 Lead Salts . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.7 Chalcopyrites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.8 Delafossites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6.9 Perovskites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.7 Alloy Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.8 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.9 Systematics of Semiconductor Bandgaps . . . . . . . . . . . . . . . . . 6.10 Temperature Dependence of the Bandgap . . . . . . . . . . . . . . . . 6.11 Equation of Electron Motion . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.12 Electron Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.12.1 Effective Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.12.2 Polaron Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.12.3 Nonparabolicity of Electron Mass . . . . . . . . . . . . . . . . 6.13 Holes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.13.1 Hole Concept . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.13.2 Hole Dispersion Relation . . . . . . . . . . . . . . . . . . . . . . . 6.13.3 ValenceBand Fine Structure . . . . . . . . . . . . . . . . . . . 6.14 Strain Effect on the Band Structure . . . . . . . . . . . . . . . . . . . . . 6.14.1 Strain effect on Band Edges . . . . . . . . . . . . . . . . . . . . 6.14.2 Strain Effect on Effective Masses . . . . . . . . . . . . . . . . 6.15 Density of States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.15.1 General Band Structure . . . . . . . . . . . . . . . . . . . . . . . . 6.15.2 FreeElectron Gas . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
111 111 111 112 114 116 117 118 119 119 119 119 119 120 120 121 122 123 123 124 125 125 129 131 132 132 135 136 136 136 138 140 142 143 144 144 144 145
5.4 6
XI
XII
Contents
7
Electronic Defect States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Fermi Distribution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3 Carrier Concentration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4 Intrinsic Conduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Shallow Impurities, Doping . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.1 Donors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.2 Acceptors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.3 Compensation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.4 Amphoteric Impurities . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.5 High Doping . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.6 QuasiFermi Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7 Deep Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7.1 Charge States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7.2 Jahn–Teller Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7.3 NegativeU Center . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7.4 DX Center . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7.5 EL2 Defect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7.6 Semiinsulating Semiconductors . . . . . . . . . . . . . . . . . 7.7.7 Surface States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.8 Hydrogen in Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . .
149 149 149 151 153 156 157 164 167 170 171 174 175 176 177 178 180 182 183 184 185
8
Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Conductivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 LowField Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.1 Mobility . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.2 Microscopic Scattering Processes . . . . . . . . . . . . . . . . 8.3.3 Ionized Impurity Scattering . . . . . . . . . . . . . . . . . . . . . 8.3.4 Deformation Potential Scattering . . . . . . . . . . . . . . . . 8.3.5 Piezoelectric Potential Scattering . . . . . . . . . . . . . . . . 8.3.6 Polar Optical Scattering . . . . . . . . . . . . . . . . . . . . . . . . 8.3.7 Temperature Dependence . . . . . . . . . . . . . . . . . . . . . . . 8.4 Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.5 HighField Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.5.1 DriftSaturation Velocity . . . . . . . . . . . . . . . . . . . . . . . 8.5.2 Velocity Overshoot . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.5.3 Impact Ionization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 HighFrequency Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.7 Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.8 Continuity Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.9 Heat Conduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.10 Coupled Heat and Charge Transport . . . . . . . . . . . . . . . . . . . . 8.10.1 Seebeck Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.10.2 Peltier Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
189 189 190 191 191 192 193 193 194 194 194 197 200 200 201 202 205 205 206 207 209 209 210
Contents
XIII
9
Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1 Spectral Regions and Overview . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Reﬂection and Diffraction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Electron–Photon Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4 Band–Band Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.1 Joint Density of States . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.2 Direct Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.3 Indirect Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.4 Urbach Tail . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.5 IntravalenceBand Absorption . . . . . . . . . . . . . . . . . . . 9.4.6 Amorphous Semiconductors . . . . . . . . . . . . . . . . . . . . 9.4.7 Excitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.8 Exciton Polariton . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.9 BoundExciton Absorption . . . . . . . . . . . . . . . . . . . . . 9.4.10 Biexcitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.11 Trions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.12 Burstein–Moss Shift . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.13 Bandgap Renormalization . . . . . . . . . . . . . . . . . . . . . . 9.4.14 Electron–Hole Droplets . . . . . . . . . . . . . . . . . . . . . . . . 9.4.15 TwoPhoton Absorption . . . . . . . . . . . . . . . . . . . . . . . . 9.5 Impurity Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.6 FreeCarrier Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7 Lattice Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.1 Dielectric Constant . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.2 Reststrahlenbande . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.3 Polaritons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.4 Phonon–Plasmon Coupling . . . . . . . . . . . . . . . . . . . . .
213 213 214 216 219 219 219 221 223 225 225 225 229 232 234 235 235 236 238 239 240 242 245 245 246 248 249
10
Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Band–Band Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2.1 Spontaneous Emission . . . . . . . . . . . . . . . . . . . . . . . . . 10.2.2 Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2.3 Stimulated Emission . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2.4 Net Recombination Rate . . . . . . . . . . . . . . . . . . . . . . . 10.2.5 Recombination Dynamics . . . . . . . . . . . . . . . . . . . . . . . 10.2.6 Lasing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.3 FreeExciton Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4 BoundExciton Recombination . . . . . . . . . . . . . . . . . . . . . . . . . 10.5 Alloy Broadening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6 Phonon Replica . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.7 Donor–Acceptor Pair Transitions . . . . . . . . . . . . . . . . . . . . . . . 10.8 InnerImpurity Recombination . . . . . . . . . . . . . . . . . . . . . . . . . 10.9 Auger Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.10 Band–Impurity Recombination . . . . . . . . . . . . . . . . . . . . . . . . .
251 251 251 251 252 253 253 254 256 256 258 260 261 265 267 267 268
XIV
Contents
10.11 Field Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.11.1 Thermally Activated Emission . . . . . . . . . . . . . . . . . . 10.11.2 Direct Tunneling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.11.3 Assisted Tunneling . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.12 Multilevel Traps . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.13 Surface Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.14 ExcessCarrier Proﬁles . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
272 272 273 273 273 274 274
11
Heterostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 Growth Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3 Material Combinations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3.1 Pseudomorphic Structures . . . . . . . . . . . . . . . . . . . . . . 11.3.2 Heterosubstrates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.4 Band Lineup in Heterostructures . . . . . . . . . . . . . . . . . . . . . . . 11.5 Energy Levels in Heterostructures . . . . . . . . . . . . . . . . . . . . . . 11.5.1 Quantum Well . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.2 Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.3 Single Heterointerface Between Doped Materials . . 11.6 Recombination in Quantum Wells . . . . . . . . . . . . . . . . . . . . . . 11.7 Isotope Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.8 Wafer Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
277 277 277 280 280 280 285 286 286 293 293 295 299 300
12
External Fields . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1 Electric Fields . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1.1 Bulk Material . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1.2 Quantum Wells . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2 Magnetic Fields . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.1 FreeCarrier Absorption . . . . . . . . . . . . . . . . . . . . . . . . 12.2.2 Energy Levels in Bulk Crystals . . . . . . . . . . . . . . . . . . 12.2.3 Energy Levels in a 2DEG . . . . . . . . . . . . . . . . . . . . . . . 12.2.4 Shubnikov–de Haas Oscillations . . . . . . . . . . . . . . . . . 12.3 Quantum Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.1 Integral QHE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.2 Fractional QHE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.3 Weiss Oscillations . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
303 303 303 305 306 307 308 309 310 313 313 317 318
13
Nanostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.2 Quantum Wires . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.2.1 Preparation Methods . . . . . . . . . . . . . . . . . . . . . . . . . . 13.2.2 Quantization in TwoDimensional Potential Wells . 13.3 Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.3.1 Quantization in ThreeDimensional Potential Wells . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
321 321 321 321 328 328 328
Contents
13.3.2 13.3.3 13.3.4
XV
Electrical and Transport Properties . . . . . . . . . . . . . . 331 SelfAssembled Preparation . . . . . . . . . . . . . . . . . . . . . 336 Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 341
14
Polarized Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2 Spontaneous Polarization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3 Ferroelectricity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.1 Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.2 Soft Phonon Mode . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.3 Phase Transition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.4 Domains . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.5 Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.4 Piezoelectricity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
345 345 345 346 348 348 348 352 353 353
15
Magnetic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.2 Magnetic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.3 Diluted Magnetic Semiconductors . . . . . . . . . . . . . . . . . . . . . . 15.4 Spintronics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.4.1 Spin Transistor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.4.2 Spin LED . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
359 359 359 361 365 366 367
16
Organic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 369 16.1 Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 369 16.2 Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 371
17
Dielectric Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.1 PhotonicBandgap Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.1.2 General 1D Scattering Theory . . . . . . . . . . . . . . . . . . 17.1.3 Transmission of an N Period Potential . . . . . . . . . . . 17.1.4 The QuarterWave Stack . . . . . . . . . . . . . . . . . . . . . . . 17.1.5 Formation of a 3D Band Structure . . . . . . . . . . . . . . . 17.1.6 Defect Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.1.7 Coupling to an Electronic Resonance . . . . . . . . . . . . 17.2 Microscopic Resonators . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2.1 Microdiscs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2.2 Purcell Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2.3 Deformed Resonators . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2.4 Hexagonal Cavities . . . . . . . . . . . . . . . . . . . . . . . . . . . .
375 375 375 375 377 379 382 385 387 390 390 392 393 395
XVI
Contents
Part II Applications 18
Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2 Metal–Semiconductor Contacts . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.1 Band Diagram in Equilibrium . . . . . . . . . . . . . . . . . . . 18.2.2 SpaceCharge Region . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.3 Schottky Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.4 Capacitance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.5 Current–Voltage Characteristic . . . . . . . . . . . . . . . . . . 18.2.6 Ohmic Contacts . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.7 Metal Contacts to Organic Semiconductors . . . . . . . 18.3 Metal–Insulator–Semiconductor Diodes . . . . . . . . . . . . . . . . . . 18.3.1 Band Diagram for Ideal MIS Diode . . . . . . . . . . . . . . 18.3.2 SpaceCharge Region . . . . . . . . . . . . . . . . . . . . . . . . . . 18.3.3 Capacity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.3.4 Nonideal MIS Diode . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.4 Bipolar Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.4.1 Band Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.4.2 SpaceCharge Region . . . . . . . . . . . . . . . . . . . . . . . . . . 18.4.3 Capacitance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.4.4 Current–Voltage Characteristics . . . . . . . . . . . . . . . . 18.4.5 Breakdown . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5 Applications and Special Diode Devices . . . . . . . . . . . . . . . . . 18.5.1 Rectiﬁcation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.2 Frequency Mixing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.3 Voltage Regulator . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.4 Zener Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.5 Varactors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.6 FastRecovery Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.7 StepRecovery Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.8 pinDiodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.9 Tunneling Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.10 Backward Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5.11 Heterostructure Diodes . . . . . . . . . . . . . . . . . . . . . . . . .
401 401 402 402 407 409 410 412 421 424 425 427 428 432 435 435 436 437 442 443 454 457 457 460 462 463 463 466 466 468 469 471 471
19
LighttoElectricity Conversion . . . . . . . . . . . . . . . . . . . . . . . . . . 19.1 Photocatalysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2 Photoconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2.2 Photoconductivity Detectors . . . . . . . . . . . . . . . . . . . . 19.2.3 Electrophotography . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2.4 QWIPs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2.5 Blocked ImpurityBand Detectors . . . . . . . . . . . . . . .
473 473 475 475 475 477 477 482
Contents
19.3
Photodiodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.3.2 pn Photodiodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.3.3 pin Photodiodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.3.4 PositionSensing Detector . . . . . . . . . . . . . . . . . . . . . . 19.3.5 MSM Photodiodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.3.6 Avalanche Photodiodes . . . . . . . . . . . . . . . . . . . . . . . . 19.3.7 TravelingWave Photodetectors . . . . . . . . . . . . . . . . . . 19.3.8 Charge Coupled Devices . . . . . . . . . . . . . . . . . . . . . . . . 19.3.9 Photodiode Arrays . . . . . . . . . . . . . . . . . . . . . . . . . . . . Solar Cells . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.4.1 Solar Radiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.4.2 Ideal Solar Cells . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.4.3 Real Solar Cells . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.4.4 Design Reﬁnements . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.4.5 SolarCell Types . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.4.6 Commercial Issues . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
484 484 484 487 489 490 495 498 501 509 511 511 513 516 516 517 520
ElectricitytoLight Conversion . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.1 Radiometric and Photometric Quantities . . . . . . . . . . . . . . . . 20.1.1 Radiometric Quantities . . . . . . . . . . . . . . . . . . . . . . . . 20.1.2 Photometric Quantities . . . . . . . . . . . . . . . . . . . . . . . . 20.2 Scintillators . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.2.1 CIE Chromaticity Diagram . . . . . . . . . . . . . . . . . . . . . 20.2.2 Display Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.2.3 Radiation Detection . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.2.4 Luminescence Mechanisms . . . . . . . . . . . . . . . . . . . . . . 20.3 LightEmitting Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.3.2 Spectral Ranges . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.3.3 Quantum Eﬃciency . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.3.4 Device Design . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4 Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.2 Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.3 Gain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.4 Optical Mode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.5 Loss Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.6 Threshold . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.7 Spontaneous Emission Factor . . . . . . . . . . . . . . . . . . . 20.4.8 Output Power . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.9 Temperature Dependence . . . . . . . . . . . . . . . . . . . . . . . 20.4.10 Mode Spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.11 Longitudinal SingleMode Lasers . . . . . . . . . . . . . . . . 20.4.12 Tunability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
523 523 523 523 524 525 528 528 530 531 531 531 532 533 539 539 542 543 547 552 554 555 555 559 560 560 562
19.4
20
XVII
XVIII Contents
20.4.13 Modulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.4.14 Surfaceemitting Lasers . . . . . . . . . . . . . . . . . . . . . . . . 20.4.15 Optically Pumped Semiconductor Lasers . . . . . . . . . 20.4.16 Quantum Cascade Lasers . . . . . . . . . . . . . . . . . . . . . . . 20.4.17 HotHole Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Semiconductor Optical Ampliﬁers . . . . . . . . . . . . . . . . . . . . . .
564 568 571 573 573 575
Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2 Bipolar Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.1 Carrier Density and Currents . . . . . . . . . . . . . . . . . . . 21.2.2 Current Ampliﬁcation . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.3 Ebers–Moll Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.4 Current–Voltage Characteristics . . . . . . . . . . . . . . . . . 21.2.5 Basic Circuits . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.6 HighFrequency Properties . . . . . . . . . . . . . . . . . . . . . 21.2.7 Heterobipolar Transistors . . . . . . . . . . . . . . . . . . . . . . . 21.2.8 Lightemitting Transistors . . . . . . . . . . . . . . . . . . . . . . 21.3 FieldEffect Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.4 JFET and MESFET . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.4.1 General Principle . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.4.2 Static Characteristics . . . . . . . . . . . . . . . . . . . . . . . . . . 21.4.3 Normally On and Normally Off FETs . . . . . . . . . . . . 21.4.4 FieldDependent Mobility . . . . . . . . . . . . . . . . . . . . . . 21.4.5 HighFrequency Properties . . . . . . . . . . . . . . . . . . . . . 21.5 MOSFETs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.5.1 Operation Principle . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.5.2 Current–Voltage Characteristics . . . . . . . . . . . . . . . . . 21.5.3 MOSFET Types . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.5.4 Complementary MOS . . . . . . . . . . . . . . . . . . . . . . . . . . 21.5.5 LargeScale Integration . . . . . . . . . . . . . . . . . . . . . . . . . 21.5.6 Nonvolatile Memories . . . . . . . . . . . . . . . . . . . . . . . . . . 21.5.7 Heterojunction FETs . . . . . . . . . . . . . . . . . . . . . . . . . . 21.6 ThinFilm Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
577 577 577 579 582 583 585 588 589 590 590 592 593 593 594 597 598 601 601 601 602 606 608 610 614 615 619
20.5 21
Part III Appendices A
Tensors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 623
B
Kramers–Kronig Relations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 627
C
Oscillator Strength . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 629
D
Quantum Statistics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 635
Contents
XIX
E
The k · p Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . 639
F
EffectiveMass Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 643
References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 645 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 669
Abbreviations
2DEG
twodimensional electron gas
AAAS AB ac AFM AIP AM APD APD APS AR ASE AVS
American Association for the Advancement of Science antibonding (position) alternating current atomic force microscopy American Institute of Physics air mass antiphase domain avalanche photodiode American Physical Society antireﬂection ampliﬁed spontaneous emission American Vacuum Society (The Science & Technology Society)
BC bcc BEC BGR
bond center (position) bodycentered cubic Bose–Einstein condensation bandgap renormalization
CAS CCD CD CEO CIE CIS CL CMOS CMY COD CPU CRT CVD
calorimetric absorption spectroscopy charge coupled device compact disc cleavededge overgrowth ´ Commission Internationale de l’Eclairage CuInSe2 material cathodoluminescence complementary metal–oxide–semiconductor cyanmagentayellow (color system) catastrophical optical damage central processing unit cathode ray tube chemical vapor deposition
XXII
Abbreviations
cw CZ
continuous wave Czochralski (growth)
DAP DBR dc DFB DH(S) DLTS DMS DOS DPSS DRAM DVD
donor–acceptor pair distributed Bragg reﬂector direct current distributed feedback double heterostructure deep level transient spectroscopy diluted magnetic semiconductor density of states diodepumped solidstate (laser) dynamic random access memory digital versatile disc
EEPROM EHL EL ELO EMA EPROM ESF EXAFS
electrically erasable programmable readonly memory electron–hole liquid electroluminescence epitaxial lateral overgrowth effective mass approximation erasable programmable readonly memory extrinsic stacking fault extended Xray absorption ﬁne structure
fcc FeRAM FET FIR FKO FPA FQHE FWHM FZ
facecentered cubic ferroelectric random access memory ﬁeldeffect transistor far infrared Franz–Keldysh oscillation focal plane array fractional quantum Hall effect full width at halfmaximum ﬂoatzone (growth)
GLAD GRINSCH GSMBE
glancingangle deposition gradedindex separate conﬁnement heterostructure gassource molecular beam epitaxy
HBT hcp HCSEL HEMT HIGFET HJFET hh
heterobipolar transistor hexagonally close packed horizontal cavity surfaceemitting laser high electron mobility transistor heterojunction insulating gate FET heterojunction FET heavy hole
Abbreviations XXIII
HOMO HR HRTEM HWHM
highest occupied molecular orbital high reﬂection highresolution transmission electron microscopy halfwidth at halfmaximum
IC IDB IF IPAP IQHE IR ISF ITO
integrated circuit inversion domain boundary intermediate frequency Institute of Pure and Applied Physics, Tokyo integral quantum Hall effect infrared intrinsic stacking fault indium tin oxide
JDOS JFET
joint density of states junction ﬁeldeffect transistor
KKR KTP
Kramers–Kronig relation KTiOPO4 material
LA LCD LDA LEC LED lh LO LPE LPCVD LPP LST LT LUMO LVM
longitudinal acoustic (phonon) liquid crystal display local density approximation liquid encapsulated Czochralski (growth) lightemitting diode light hole longitudinal optical (phonon), local oscillator liquid phase epitaxy lowpressure chemical vapor deposition longitudinal phonon plasmon (mode) Lyddane–Sachs–Teller (relation) low temperature lowest unoccupied molecular orbital local vibrational mode
MBE MEMS MESFET MIGS MIOS MIR MIS MHEMT ML MMIC
molecular beam epitaxy microelectromechanical system metal–semiconductor ﬁeldeffect transistor midgap (surface) states metal–insulator–oxide–semiconductor midinfrared metal–insulator–semiconductor metamorphic HEMT monolayer millimeterwave integrated circuit
XXIV Abbreviations
MO MODFET MOMBE MOPA MOS MOSFET MOVPE MRS MS MSM MWQ
master oscillator modulationdoped FET metalorganic molecular beam epitaxy master oscillator power ampliﬁer metal–oxide–semiconductor metal–oxide–semiconductor ﬁeldeffect transistor metalorganic chemical vapor deposition Material Research Society metal–semiconductor (diode) metal–semiconductor–metal (diode) multiple quantum well
NDR NEP NIR NMOS NTSC
negative differential resistance noise equivalent power near infrared nchannel metal–oxide–semiconductor (transistor) national television standard colors
OPSL
optically pumped semiconductor laser
PA PBG pc PFM PHEMT PL PLD PLE PMMA PMOS PPC PPLN PV PWM PZT
power ampliﬁer photonic bandgap primitive cubic piezoresponse force microscopy pseudomorphic HEMT photoluminescence pulsed laser deposition photoluminescence excitation (spectroscopy) polymethyl methacrylate pchannel metal–oxide–semiconductor (transistor) persistent photoconductivity perodically poled lithium niobate photovoltaic pulsewidth modulation PbTix Zr1−x O3 material
QCL QCSE QD QHE QW QWIP QWR
quantum cascade laser quantum conﬁned Stark effect quantum dot quantum Hall effect quantum well quantumwell intersubband photodetector quantum wire
Abbreviations
RAM RAS REI RF RGB RHEED RKKY rms ROM
random access memory reﬂection anisotropy spectroscopy random element isodisplacement radio frequency redgreenblue (color system) reﬂection highenergy electron diffraction Ruderman–Kittel–Kasuya–Yoshida (interaction) root mean square readonly memory
SAGB SAM sc SCH SEL SEM SET SGDBR SHG si SIA SIMS SL so SOA SPD SPIE SPS sRGB SRH SSR STM
smallangle grain boundary separate absorption and ampliﬁcation (structure) simple cubic separate conﬁnement heterostructure surfaceemitting laser scanning electron microscopy singleelectron transistor sampled grating distributed Bragg reﬂector secondharmonic generation semiinsulating Semiconductor Industry Association secondary ion mass spectroscopy superlattice spinorbit (or splitoff) semiconductor optical ampliﬁer spectral power distribution International Society for Optical Engineering shortperiod superlattice standard RGB Shockley–Read–Hall (kinetics) sidemode suppression ratio scanning tunneling microscopy
TA TCO TE TEGFET TEM TES TF TFT TM TO TOD TPA
transverse acoustic (phonon) transparent conductive oxide transverse electric (polarization) twodimensional electron gas FET transmission electron microscopy twoelectron satellite thermionic ﬁeld emission thinﬁlm transistor transverse magnetic (polarization) transverse optical (phonon) turnon delay (time) twophoton absorption
XXV
XXVI Abbreviations
UHV UV
ultrahigh vacuum ultraviolet
VCA VCO VCSEL VFF VGF VIS VLSI
virtual crystal approximation voltagecontrolled oscillator verticalcavity surfaceemitting laser valence force ﬁeld vertical gradient freeze (growth) visible very large scale integration
WGM WKB WS
whispering gallery mode Wentzel–Kramer–Brillouin (approximation or method) Wigner–Seitz (cell)
XSTM
crosssectional STM
Symbols
α α(ω) αm αn αp β γ, Γ γ1 , γ2 , γ3 Δ0 ǫ(ω) ǫ0 ǫr ǫxy η ηd ηw ΘD κ λ μ μ0 μh μn ν Π ρ σ σn σp σP σxy τ
Madelung constant, disorder parameter, linewidth enhancement factor absorption coeﬃcient mirror loss electron ionization coeﬃcient hole ionization coeﬃcient used as abbreviation for e/(kB T ), spontaneous emission coeﬃcient broadening parameter Luttinger parameter spinorbit splitting dielectric function permittivity of vacuum relative dielectric function strain components quantum eﬃciency differential quantum eﬃciency wallplug eﬃciency Debye temperature imaginary part of index of refraction, heat conductivity wavelength mobility magnetic susceptibility of vacuum hole mobility electron mobility frequency Peltier coeﬃcient mass density, charge density, resistivity standard deviation, conductivity electron capture cross section hole capture cross section polarization charge stress components lifetime, time constant
XXVIII Symbols
φ φBn χ χ(r) Ψ (r) ω Ω
phase Schottky barrier height electron aﬃnity, electric susceptibility envelope wavefunction wavefunction angular frequency interaction parameter
a a A A, A A∗ A∗∗ a0 b b B B, B c C Cn , Cp Cij d D D, D De (E) Dh (E) Dn Dp e E E, E, E EA b EA EC ED b ED EF EFn EFp Eg EP EV EX
hydrostatic deformation potential accelaration area vector potential Richardson constant effective Richardson constant (cubic) lattice constant bowing parameter, deformation potential Burger’s vector bimolecular recombination coeﬃcient, bandwidth magnetic ﬁeld velocity of light in vacuum, lattice constant (along caxis) capacity, spring constant Auger recombination coeﬃcient elastic constants distance, shear deformation potential density of states, diffusion coeﬃcient displacement ﬁeld electron density of states hole density of states electron diffusion coeﬃcient hole diffusion coeﬃcient elementary charge energy electric ﬁeld energy of acceptor level acceptor ionization energy energy of conductionband edge energy of donor level donor ionization energy Fermi energy electron quasiFermi energy hole quasiFermi energy bandgap energy parameter energy of valenceband edge exciton energy
Symbols XXIX b EX f F F, F F (M ) fe fi Fn Fp g G G gm h H H, H H i I Is j js k, kB k kF l L L LD Lz m m∗ M M, M me mh mj n
n N (E) n∗ NA Nc
exciton binding energy oscillator strength free energy force excess noise factor Fermi–Dirac distribution function ionicity electron quasiFermi energy hole quasiFermi energy degeneracy, gfactor, gain free enthalpy, generation rate vector of reciprocal lattice transconductance Planck constant enthalpy magnetic ﬁeld Hamiltonian h/(2π) imaginary number current saturation current current density, orbital momentum saturation current density Boltzmann constant wavevector Fermi wavevector angular orbital momentum length of line element line vector (of dislocation) diffusion length quantumwell thickness mass effective mass mass, multiplication factor magnetization effective electron mass effective hole mass magnetic quantum number electron concentration (in conduction band), ideality factor normal vector number of states complex index of refraction (= nr + iκ) acceptor concentration critical doping concentration
XXX
NC ND ni nr ns Nt ntr nthr NV p p, p P P, P pcv pi q q, q Q r r R R rH RH s S Sij t T u unk U v, v vs V V (λ) Va vg vs vth w Wm X Y Z
Symbols
conductionband edge density of states donor concentration intrinsic electron concentration index of refraction (real part) sheet electron density trap concentration transparency electron concentration threshold electron concentration valenceband edge density of states pressure, free hole density momentum power electric polarization momentum matrix element intrinsic hole concentration charge heat ﬂow charge, quality factor radius spatial coordinate resistance, radius, recombination rate vector of direct lattice Hall factor Hall coeﬃcient spin entropy, Seebeck coeﬃcient, total spin stiffness coeﬃcients time temperature displacement, cellinternal parameter Bloch function energy velocity driftsaturation velocity volume, voltage, potential (standardized) sensitivity of human eye unitcell volume group velocity velocity of sound thermal velocity depletionlayer width work function electronegativity Young’s module, CIE brightness parameter partition sum, atomic order number
Physical Constants
constant
symbol
speed of light in vacuum c0 permeability of vacuum μ0 permittivity of vacuum ǫ0 = (μ0 c20 )−1 elementary charge electron mass Planck constant
Boltzmann constant vonKlitzing constant Rydberg constant Bohr radius
e me h = h/(2π) kB RH aB
numerical value
unit
2.99792458 × 108 4π × 10−7 8.854187817 × 10−12 8.617385 × 10−5 1.60217733 × 10−19 9.1093897 × 10−31 6.6260755 × 10−34 1.05457266 × 10−34 6.582122 × 10−16 1.380658 × 10−23 25812.8056 13.6056981 5.29177249 × 10−11
m s−1 N A−2 F m−1 eV K−1 C kg Js Js eV s J K−1 Ω eV m
1 Introduction
The proper conduct of science lies in the pursuit of Nature’s puzzles, wherever they may lead. J.M. Bishop [1]
The historic development of semiconductor physics and technology began in the second half of the 19th century. In 1947, the realization of the transistor was the impetus to a fastpaced development that created the electronics and photonics industries. Products founded on the basis of semiconductor devices such as computers (CPUs, memories), opticalstorage media (CD, DVD), communication infrastructure (opticalﬁber technology, mobile communication) and lighting (LEDs) are commonplace. Thus, fundamental research on semiconductors and semiconductor physics and its offspring in the form of devices has contributed largely to the development of modern civilization and culture.
1.1 Timetable
In this section early important milestones in semiconductor physics and technology are listed. 1821 T.J. Seebeck – discovery of semiconductor properties of PbS [2]. 1833 M. Faraday – discovery of the temperature dependence of the conductivity of AgS (negative dR/dT ) [3]. 1873 W. Smith – discovery of photoconductivity in selenium [4].
2
1 Introduction
1874 F. Braun1 – discovery of rectiﬁcation in metal–sulﬁde semiconductor contacts [6], e.g. for CuFeS2 and PbS. The current through a metal–semiconductor contact is nonlinear (as compared to that through a metal, Fig. 1.1), i.e. a deviation from Ohm’s law. Braun’s structure is similar to a MSM diode.
Fig. 1.1. Current through a silver–CuFeS2 –silver structure as a function of the current through the metal only, 1874. Data points are for diﬀerent applied voltages. Experimental data from [6]
1876 W.G. Adams and R.E. Day – discovery of the photovoltaic effect in selenium [7]. 1883 Ch. Fritts – ﬁrst solar cell, based on an Au/selenium rectiﬁer [5]. The eﬃciency was below 1%. 1907 H.J. Round – discovery of electroluminescence investigating blue light emission from SiC [8]. 1911 The term ‘Halbleiter’ (semiconductor) is introduced for the ﬁrst time by J. K¨ onigsberger and J. Weiss [9].
1
F. Braun made his discoveries on metal–semiconductor contacts in Leipzig while a teacher at the Thomasschule zu Leipzig. He conducted his famous work on vacuum tubes later as a professor in Strasbourg, France.
1.1 Timetable
3
1925 J.E. Lilienfeld2 – proposal of the ﬁeldeffect transistor (Fig. 1.2) (Method and Apparatus for Controlling Electric Currents, US patent 1,745,175, 1930, ﬁled 1926). J.E. Lilienfeld was also awarded patents for a depletion mode MOSFET (US patent 1,900,018, 1933) and current ampliﬁcation with nppnand pnnptransistors (US patent 1,877,140, 1932).
Fig. 1.2. Sketch of a ﬁeldeﬀect transistor, 1926. From [12]
1927 A. Schleede and Baggisch – impurities are of decisive importance for conductivity. 1931 R. de L. Kronig and W.G. Penney – properties of periodic potentials in solids [13]. A.H. Wilson – development of bandstructure theory [14]. C. Zener – Zener tunneling [15]. 1936 J. Frenkel – description of excitons [16]. 1938 B. Davydov – theoretical prediction of rectiﬁcation in Cu2 O [17]. W. Schottky – theory of the boundary layer in metal–semiconductor contacts [18], being the basis for Schottky contacts and ﬁeldeffect transistors (FETs). 2 After obtaining his PhD in 1905 from the FriedrichWilhelmsUniversit¨ at Berlin, J.E. Lilienfeld joined the Physics Department of University of Leipzig and worked on gas liquiﬁcation and with Lord Zeppelin on hydrogenﬁlled blimps. In 1910 he became professor at the University of Leipzig where he mainly researched on Xrays and vacuum tubes. To the surprise of his colleagues he left in 1926 to join a US industrial laboratory [10, 11].
4
1 Introduction
N.F. Mott – metal–semiconductor rectiﬁer theory [19]. R. Hilsch and R.W. Pohl – proposal of a threeelectrode crystal (from NaCl). 1941 R.S. Ohl – Si rectiﬁer with point contact (Fig. 1.3) (US patent 2,402,661).
Fig. 1.3. Characteristics of a silicon rectiﬁer, 1941. From [20]
1942 K. Clusius, E. Holz and H. Welker – rectiﬁcation in germanium (Elektrische Gleichrichteranordnung mit Germanium als Halbleiter und Verfahren zur Herstellung von Germanium f¨ ur eine solche Gleichrichteranordnung, German patent DBP 966 387, 21g, 11/02) 1945 H. Welker – patents for JFET and MESFET (Halbleiteranordnung zur kapazitiven Steuerung von Str¨ omen in einem Halbleiterkristall, German patent DBP 980 084, 21g, 11/02) 1947 W. Shockley, J. Bardeen and W. Brattain fabricate the ﬁrst transistor in the AT&T Bell Laboratories, Holmdel, NJ in an effort to improve hearing aids [21].3 Strictly speaking the structure was a pointcontact transistor. A 50µm wide slit was cut with a razor blade into gold foil over a plastic (insulating) triangle and pressed with a spring on ntype germanium (Fig. 1.4). The one 3
Subsequently, AT&T, under pressure from the US Justice Department’s antitrust division, licensed the transistor for $25,000. This action initiated the rise of companies like Texas Instruments, Sony and Fairchild.
1.1 Timetable
5
gold contact controls via the ﬁeld effect (depletion of a surface layer) the current from Ge to the other gold contact. For the ﬁrst time, ampliﬁcation was observed [22]. More details about the history and development of the semiconductor transistor can be found in [23], written on the occasion of the 50th anniversary of its invention.
Fig. 1.4. The ﬁrst transistor, 1947 (length of side of wedge: 32 mm)
1952 H. Welker – fabrication of compound semiconductors [24] (Verfahren zur Herstellung eines Halbleiterkristalls aus einer A III  B V  Verbindung mit Zonen verschiedenen Leitungstyps, German patent DBP 976 791, 12c, 2) W. Shockley – today’s version of the (J)FET [25]. 1953 G.C. Dacey and I.M. Ross – ﬁrst realization of a JFET [26]. D.M. Chapin, C.S. Fuller and G.L. Pearson – invention of the silicon solar cell at Bell Laboratories [27]. A single 2cm2 photovoltaic cell from Si, Si:As with an ultrathin layer of Si:B, with about 6% eﬃciency generated 5 mW of electrical power.4 Previously existing solar cells based on selenium had very low eﬃciency (< 0.5%). 4
A solar cell with 1 W power cost $300 in 1956 ($3 in 2004). Initially, ‘solar batteries’ were only used for toys and were looking for an application. H. Ziegler proposed the use in satellites in the ‘space race’ of the late 1950s.
6
1 Introduction
1958 J. Kilby made the ﬁrst integrated circuit at Texas Instruments. The simple oscillator consisted of one transistor, three resistors and a capacitor on a 11 × 1.7 mm2 Ge platelet (Fig. 1.5a). J. Kilby ﬁled in 1959 for US patent 3,138,743 for miniaturized electronic circuits. At practically the same time R. Noyce from Fairchild Semiconductors, the predecessor of INTEL, invented the integrated circuit on silicon using planar technology (US patent 2,981,877, 1959, for a siliconbased integrated circuit).
(a)
(b)
Fig. 1.5. (a) The ﬁrst integrated circuit, 1958 (germanium, 11 × 1.7 mm2 ). (b) The ﬁrst planar integrated circuit, 1959 (silicon, diameter: 1.5 mm)
Figure 1.5b shows a ﬂipﬂop with four bipolar transistors and ﬁve resistors. Initially, the invention of the integrated circuit5 met scepticism because of concerns regarding yield and the achievable quality of the transistors and the other components (such as resistors and capacitors). 1959 J. Hoerni and R. Noyce – ﬁrst realization of a planar transistor (Fig. 1.6) [29]. 1960 D. Kahng and M.M. Atalla – ﬁrst realization of a MOSFET [30]. 1962 The ﬁrst semiconductor laser on GaAs basis at 77 K at GE [28] and at IBM [31]. 1963 Proposal of a double heterostructure laser (DH laser) by Zh.I. Alferov [32] and H. Kroemer [33]. 5
The two patents led to a decadelong legal battle between Fairchild Semiconductors and Texas Instruments. Eventually, the US Court of Customs and Patent Appeals upheld R. Noyce’s claims on interconnection techniques but gave J. Kilby and Texas Instruments credit for building the ﬁrst working integrated circuit.
1.2 Nobel Prize Winners
7
base base
base contact
emitter contact emitter
collector
Fig. 1.6. Planar pnp silicon transistor, 1959. The contacts are Al surfaces (not bonded)
1966 Zh.I. Alferov – report of the ﬁrst DH laser on the basis of GaInP at 77 K [34]. C.A. Mead – proposal of the MESFET (‘Schottky Barrier Gate FET’) [35]. 1967 W.W. Hooper and W.I. Lehrer – ﬁrst realization of a MESFET [36]. 1968 DH laser on the basis of GaAs/AlGaAs at room temperature by Zh.I. Alferov [37] and I. Hayashi [38].
1.2 Nobel Prize Winners Several Nobel Prizes6 have been awarded for discoveries and inventions in the ﬁeld of semiconductor physics (Fig. 1.2). 1909 Karl Ferdinand Braun ‘in recognition of his contributions to the development of wireless telegraphy’ 1914 Max von Laue ‘for his discovery of the diffraction of Xrays by crystals’ 1915 Sir William Henry Bragg William Lawrence Bragg ‘for their services in the analysis of crystal structure by means of Xrays’
6
www.nobel.se
8
1 Introduction
1909
1914
1915
Karl Ferdinand Braun
Max von Laue
Sir William Henry Bragg
1915 William Laurence Bragg
(1850–1918)
(1879–1960)
(1862–1942)
(1890–1971)
1953
1946
1953
1953
Percy Williams Bridgman
William B. Shockley
John Bardeen
Walter Hauser Brattain
(1882–1961)
(1910–1989)
(1908–1991)
(1902–1987)
1973
1985
1998
1998
Leo Esaki
Klaus von Klitzing
Robert B. Laughlin
Horst L. St¨ ormer
(*1925)
(*1943)
(*1930)
(*1949)
1998
2000
2000
2000
Daniel C. Tsui
Zhores I. Alferov
Herbert Kroemer
Jack St. Clair Kilby
(*1939)
(*1938)
(*1928)
(1923–2005)
Fig. 1.7. Winners of Nobel Prize in Physics and year of award with great importance for semiconductor physics
1.3 General Information
9
1946 Percy Williams Bridgman ‘for the invention of an apparatus to produce extremely high pressures, and for the discoveries he made therewith in the ﬁeld of high pressure physics’ 1953 William Bradford Shockley John Bardeen Walter Houser Brattain ‘for their researches on semiconductors and their discovery of the transistor effect’ 1973 Leo Esaki ‘for his experimental discoveries regarding tunneling phenomena in semiconductors’ 1985 Klaus von Klitzing ‘for the discovery of the quantized Hall effect’ 1998 Robert B. Laughlin Horst L. St¨ ormer Daniel C. Tsui ‘for their discovery of a new form of quantum ﬂuid with fractionally charged excitations’ 2000 Zhores I. Alferov Herbert Kroemer ‘for developing semiconductor heterostructures used in highspeed and optoelectronics’ Jack St. Clair Kilby ‘for his part in the invention of the integrated circuit’
1.3 General Information In Fig. 1.8, the periodic table of elements is shown. In Table 1.1 the physical properties of various semiconductors are summarized.
10
1 Introduction
Fig. 1.8. Periodic table of elements. From [39] with permission
1.3 General Information
11
Table 1.1. Physical properties of various semiconductors at room temperature. ‘S’ denotes the crystal structure (d: diamond, w: wurtzite, zb: zincblende, ch: chalcopyrite, rs: rocksalt) ZnS, Cds and CdTe can realize zb and w structures S a0 (nm) C Si
d 0.3567 d 0.5431
Ge
d
αSn d 3CSiC zb 4HSiC w 6HSiC w w
AlP AlAs
zb zb
AlSb GaN
zb 0.61335 w 0.3189 (a) 0.5185 (c) zb 0.54506 zb 0.56533
GaSb InN InP InAs InSb ZnO ZnS ZnSe ZnTe CdO CdS CdSe CdTe
m∗e
5.45 (Γ ) 1.124 (X) 0.98 0.19 0.6461 0.67 (L) 1.58 0.08 0.64892 0.08 (Γ ) 0.02 0.436 2.4 0.3073 (a) 3.26 1.005 (c) 0.30806 (a) 3.101 1.5117 (c) 0.3111 (a) 6.2 0.4978 (c) 0.54625 2.43 (X) 0.13 0.56605 2.16 (X) 0.5
AlN
GaP GaAs
Eg (eV)
zb 0.60954 w 0.3533 (a) 0.5693 (c) zb 0.58686 zb 0.60584 zb 0.64788 w 0.325 (a) 0.5206 (c) zb 0.54109 zb 0.56686 zb 0.61037 rs 0.47 w 0.416 (a) 0.6756 (c) zb 0.6050 zb 0.64816
1.52 X) 3.4 (Γ )
m∗h
(ml ) (mt ) (ml ) (mt )
0.11 0.2
2.26 (Γ ) 0.13 1.43 (Γ ) 0.067 0.72 (Γ ) 0.045 0.9 (Γ ) 1.35 (Γ ) 0.36 (Γ ) 0.18 (Γ ) 3.4 (Γ )
0.07 0.028 0.013 0.28
3.6 (Γ ) 2.58 (Γ ) 2.25 (Γ ) 2.16 2.42 (Γ )
0.3 0.17 0.15 0.2
1.73 (Γ ) 0.13 1.50 (Γ ) 0.11
0
nr
μe μh (cm2 /V s) (cm2 /V s)
5.5 2.42 2200 0.16 (mlh ) 11.7 3.44 1350 0.5 (mhh ) 0.04 (mlh ) 16.3 4.00 3900 0.3 (mhh ) 2000 9.7 2.7 1000 9.6 2.7 10.2 2.7 1140
1600 480 1900 1000 50 120 850
8.5 3.32 9.8 3.0 80 0.49 (mlh ) 12 1000 1.06 (mhh ) 0.39 11 3.4 200 0.8 12 2.4 1500
80 300
0.67 10 3.37 300 0.12 (mlh ) 12.5 3.4 8500 0.5 (mhh ) 0.39 15 3.9 5000
150 400
0.4 0.33 0.18 0.59
600 200 1700
12.1 12.5 18 6.5
3.37 3.42 3.75 2.2
4000 22 600 100 000 220
1000
8.3 2.4 110 8.1 2.89 600 9.7 3.56 0.7
8.9 2.5 250
0.4 0.35
10.6 650 10.9 2.75 1050
100
12
1 Introduction Table 1.1. (continued) S a0 (nm)
Eg (eV)
MgO HgS HgSe HgTe PbS PbSe
rs zb zb zb rs rs
7.3 2.0 (Γ ) −0.15 (Γ ) −0.15 (Γ ) 0.37 (L) 0.26 (L)
PbTe
rs 0.645
0.421 0.5852 0.6084 0.64616 0.5936 0.6147
ch 0.54 (a) 1.0441 (c) ZnGeP2 ch 0.5465 (a) 1.0771 (c) ZnSnP2 ch 0.5651 (a) 1.1302 (c) CuInS2 ch 0.523 (a) 1.113 (c) CuGaS2 ch 0.5347 (a) 1.0474 (c) CuInSe2 ch 0.5784 (a) 1.162 (c) CuGaSe2 ch 0.5614 (a) 1.103 (c)
ZnSiP2
0.29 (L) 2.96 (Γ ) 2.34 (Γ ) 1.66 (Γ ) 1.53 (Γ ) 2.5 (Γ ) 1.0 (Γ ) 1.7 (Γ )
m∗e
m∗h
0
nr μe μh (cm2 /V s) (cm2 /V s)
10.3 3.0 0.045 0.029 0.1 0.07 (mlh ) 0.039 (mhh ) 0.24 (mlh ) 0.02 (mhh ) 0.07
50 25 18 500 0.3 20 3.7 22 000 0.1 170 3.7 500 0.06 (mlh ) 250 1800 0.03 (mhh ) 0.3 (mlh ) 412 1400 0.02 (mhh )
0.5
100 600 930 1100
Part I
Fundamentals
2 Bonds
2.1 Introduction The positively charged atomic nuclei and the electrons in the atomic shells of the atoms making up the semiconductor (or any other solid) are in a binding state. Several mechanisms can lead to such cohesiveness. First, we will discuss the homopolar, electronpair or covalent bond, then the ionic bond and subsequently the mixed bond. We will only brieﬂy touch on the metallic bond and the vanderWaals bond.
2.2 Covalent Bonds Covalent bonds are formed due to quantummechanical forces. The prototype covalent bond is the bonding of the hydrogen molecule due to overlapping of the atomic shells. If several electron pairs are involved, directional bonds can be formed in various spatial directions, eventually making up a solid. 2.2.1 ElectronPair Bond The covalent bond of two hydrogen atoms in a H2 molecule can lead to a reduction of the total energy of the system, compared to two single (distant) atoms (Fig. 2.1). For fermions (electrons have spin 1/2) the twoparticle wavefunction of the two (indistinguishable) electrons A and B must be antisymmetric, i.e. Ψ (A, B) = −Ψ (B, A) (Pauli principle). The wavefunction of each electron has degrees of freedom in real space (r) and spin (σ), Ψ (A) = Ψr (A)Ψσ (A). The twoparticle wavefunction of the molecule is nonseparable and has the form Ψ (A, B) = Ψr (rA , rB )Ψσ (σA , σB ). The binding state has a wavefunction with a symmetric orbital and antiparallel spins, i.e. Ψr (rA , rB ) = Ψr (rB , rA ) and Ψσ (σA , σB ) = −Ψσ (σB , σA ). The antisymmetric orbital with parallel spins is antibinding for all distances of the nuclei (protons). 2.2.2 sp3 Bond Elements from group IV of the periodic system (C, Si, Ge, . . . ) have 4 electrons on the outer shell. Carbon has the electron conﬁguration 1s2 2s2 2p2 .
16
2 Bonds
A
S
(a)
(b)
Fig. 2.1. Binding of the hydrogen molecule. (a) Dashed line: classical calculation (electrostatics), ‘S’, ‘A’: quantummechanical calculation taking into account Pauli’s principle (S: symmetric orbital, antiparallel spins, A: antisymmetric orbital, parallel spins. The distance of the nuclei (protons) is given in units of the Bohr radius aB = 0.053 nm, the energy is given in Rydberg units (13.6 eV). (b) Schematic contour plots of the probability distribution (Ψ ∗ Ψ ) for the S and A states
For an octet conﬁguration bonding to four other electrons would be optimal (Fig. 2.2). This occurs through the mechanism of sp3 hybridization.1 First, one Selectron of the ns2 np2 conﬁguration is brought into a p orbital, such that the outermost shell contains one s, px , py , and pz orbital each (Figs. 2.3a–e). The energy necessary for this step is more than regained in the subsequent formation of the covalent bonds. The four orbitals can be reconﬁgured into four other wavefunctions, the sp3 hybrids (Figs. 2.3f–i), i.e. Ψ++++ = (s + px + py + pz )/2
(2.1a)
Ψ++−− = (s + px − py − pz )/2 Ψ+−+− = (s − px + py − pz )/2 Ψ+−−+ = (s − px − py + pz )/2 .
(2.1b) (2.1c) (2.1d)
These orbitals have a directed form along tetrahedral directions. The binding energy (per atom) of the covalent bond is large, for H–H 4.5 eV, for C–C 3.6 eV, for Si–Si 1.8 eV, and for Ge–Ge 1.6 eV. Such energy is, for neutral atoms, comparable to the ionic bond, discussed in the next section. In Fig. 2.4a the energy of a crystal made up from silicon atoms is shown for various crystal structures or phases (see Chap. 3). The lattice constant with the lowest total energy determines the lattice spacing for each crystal 1 It is debated in femtosecond chemistry whether the bond really forms in this way. However, it is a picture of overwhelming simplicity.
2.2 Covalent Bonds
17
Fig. 2.2. Octet, the favorite card game of the ‘Atomis’ (trying to reach octet conﬁguration in a bond by swapping wavefunctions). The bubble says: ‘Do you c have a 2p?’. Reprinted with permission from [40], 2002 WileyVCH 1
2
1
0
2
1
0
1
1
0
1
0
1 1
1
2
2
1
1
1 0 0 1
1
2
0
0
1
1
1 0
1 0
(a)
1
(e)
2px
2s
1
2py
1 0
(c)
2
2pz
2pz
1
0
0
1
1
2
2
1
2py
1
1
0 1 2
2
2px
2s
0
(d)
1
1
0 1 2
2
2
1
2
1
1
0
0
0
0
1
1
1
1
2
2 2
2 2
1
(f)
1
1
(b)
1
(g)
2 2
1 0
2 1
0 1
(h)
1 0 1
(i)
0 1
Fig. 2.3. (a) s orbital, (b,c,d) px , py and pz orbital, (e) hybridization, (f,g,h,i) orbitals of the sp3 hybridization: (f ) (s+px +py +pz )/2, (g) (s+px −py −pz )/2, (h) (s−px +py −pz )/2, (i) (s−px −py +pz )/2
structure. The thermodynamically stable conﬁguration is the phase with the lowest overall energy for given external conditions. The covalent bond of a groupIV atom to other groupIV atoms has a tetrahedral conﬁguration with electronpair bonds, similar to the hydrogen molecule bond. In Fig. 2.4b the energy states of the n = 2 shell for tetrahedrally bonded carbon (diamond, see Sect. 3.4.3) are shown as a function of the distance from the nuclei. First, the energetically sharp states become a band
18
2 Bonds conduction band 6 states per atom
4 states per atom
2p
Energy
2s 2 states per atom
valence band 4 states per atom
(a)
(b)
observed lattice constant
lattice constant
Fig. 2.4. (a) Energy per atom in silicon for various crystal structures. Reprinted c with permission from [41], 1980 APS. (b) Electron energy levels in (diamond structure) carbon as a function of the distance of the atomic nuclei (schematic). Adapted from [42]
due to the overlap and coupling of the atomic wavefunctions (see Chap. 6). The mixing of the states leads to the formation of the ﬁlled lower valence band (binding states) and the empty upper conduction band (antibinding states). This principle is valid for most semiconductors and is shown schematically also in Fig. 2.5. The conﬁguration of bonding and antibinding p orbitals is depicted schematically in Fig. 2.6. The bonding and antibinding sp3 orbitals are depicted in Figs. 2.7a,b and 2.13. We note that the energy of the crystal does not only depend on the distance of the nuclei but also on their geometric arrangement (crystal structure). Per carbon atom there are (in the second shell) four electrons and four unoccupied states, altogether eight. These are redistributed into four states (ﬁlled) per atoms in the valence band and four states per atom (empty) in the lowest conduction bands. Between the top of the valence band and the bottom of the conduction band there is an energy gap, later called the bandgap (see Chap. 6).
Fig. 2.5. Schematic of the origin of valence and conduction band from the atomic s and p orbitals. The bandgap Eg and the position of the Fermi level EF are indicated
2.2 Covalent Bonds
(a)
19
(b)
Fig. 2.6. Schematic representation of (a) bonding and (b) antibinding p orbitals. The signs denote the phase of the wavefunction 2
2
1
1
0
0
1
1
32
2
1
2
1
0 1 32
2
32
2
1
2
1
1
0
0
0
0
1
1
1
1
2 2
2 2
1 0
(a)
2
1
0 1 32
2 2
1 0
1 2
(b)
2 2
1 0
1 2
(c)
1 0
1 2
(d)
1 2
Fig. 2.7. Schematic representation of (a,c) bonding and (b,d) antibinding symmetric (a,b) and nonsymmetric (c,d) sp3 orbitals
2.2.3 sp2 Bond Organic semiconductors (see Chap. 16) are made up from carbon compounds. While for inorganic semiconductors the covalent (or mixed, see Sect. 2.4) bond with sp3 hybridization is important, the organic compounds are based on the sp2 hybridization. This bonding mechanism, which is present in graphite, is stronger than the sp3 bond present in diamond. The prototype organic molecule is the benzene ring2 (C6 H6 ), shown in Fig. 2.8. The benzene ring is the building block for small organic molecules and polymers. In the benzene molecule neighboring carbon atoms are bonded within the ring plane via the binding σ states of the sp2 orbitals (Fig. 2.8a). The wavefunctions (Fig. 2.9) are given by (2.2a–c).
2 Supposedly, the chemist Friedrich August Kekul´e von Stadonitz had a dream about dancing carbon molecules and thus came up with the ringlike molecule structure [43]. Kekul´e remembered: ‘During my stay in Ghent, I lived in elegant bachelor quarters in the main thoroughfare. My study, however, faced a narrow sidealley and no daylight penetrated it. . . . I was sitting writing on my textbook, but the work did not progress; my thoughts were elsewhere. I turned my chair to the ﬁre and dozed. Again the atoms were gamboling before my eyes. This time the smaller groups kept modestly in the background. My mental eye, rendered more acute by the repeated visions of the kind, could now distinguish larger structures of manifold conformation; long rows sometimes more closely ﬁtted together all twining and twisting in snakelike motion. But look! What was that? One of the snakes had seized hold of its own tail, and the form whirled mockingly before my eyes. As if by a ﬂash of lightning I awoke; and this time also I spent the rest of the night in working out the consequences of the hypothesis.’
20
2 Bonds
(b)
(a)
(c)
Fig. 2.8. Schematic representation of the (a) σ and (b) π bonds in benzene, (c) schematic symbol for benzene
√
√ 2px )/ 3 √ Ψ2 = (s − 1/2px + 3/2py )/ 3 √ Ψ3 = (s − 1/2px − 3/2py )/ 3 .
Ψ1 = (s +
(2.2a) (2.2b) (2.2c)
The ‘remaining’ pz orbitals do not directly take part in the binding (Fig. 2.8b) and form bonding (π, ﬁlled) and antibinding (π*, empty) orbitals (see Fig. 2.10). The π and π* states are delocalized over the ring. Between the highest populated molecular orbital (HOMO) and the lowest unoccupied molecular orbital (LUMO) is typically an energy gap (Fig. 2.11). The antibinding σ ∗ orbitals are energetically above the π* states.
1
2
1
0
2
1
0
1
1
0
1
0
1 1
1
2
2
1
1
1 0 0 1
1
2
0
0
1
1
1 0
1
(a)
0
(e)
2px
2s
1
1
(b)
1
2py
2pz
2s
1
(d)
1
2px
2py
0 1 2
2
1
2
1
1
0
0
0
1
1
1
2
2 2
2 2
1
2 1
0 1
(g)
1
1
0 1 2
2
0
2pz
1
0 1 2
(f)
1 0
(c)
2
1 0 1
(h)
0 1
Fig. 2.9. (a) s orbital, (b,c,d) px , py√and pz√orbital, (e) (f,g,h) hybridization, √ orbitals of the sp2 hybridization: 2p 1/2p 3/2p (f ) (s+ x )/ 3, (g) (s− x+ y )/ 3, √ (h) (s− 1/2px − 3/2py )/ 3
2.3 Ionic Bonds
21
Fig. 2.10. Orbitals due to binding and antibinding conﬁgurations of various π orbitals
s* 6´ pz 18´ sp2
} p* }p
LUMO HOMO
s Fig. 2.11. Schematic energy terms of the benzene molecule
2.3 Ionic Bonds Ionic crystals are made up from positively and negatively charged ions. The heteropolar or ionic bond is the consequence of the electrostatic attraction between the ions. However, the possibly repulsive character of next neighbors has to be considered. For I–VII compounds, e.g. LiF or NaCl, the shells of the singly charged ions are complete: Li: 1s2 2s1 → Li+ : 1s2 , F: 1s2 2s2 2p5 → F− : 1s2 2s2 2p6 .
22
2 Bonds
Compared to ions in a gas, a Na–Cl pair in the crystal has a binding energy of 7.9 eV that mostly stems from the electrostatic energy (Madelung energy). VanderWaals forces (see Sect. 2.6) only contribute 1–2%. The ionization energy of Na is 5.14 eV, the electron aﬃnity of Cl is 3.61 eV. Thus the energy of the NaCl pair in the solid is 6.4 (=7.9−5.1+3.6) eV lower than in a gas of neutral atoms. The interaction of two ions with distance vector rij is due to the Coulomb interaction C Uij =
qi q j 1 e2 1 =± 4πǫ0 rij 4πǫ0 rij
(2.3)
and a repulsive contribution due to the overlap of (complete) shells. This contribution is typically approximated by a radially symmetric core potential core Uij = λexp(−r/̺)
(2.4)
that only acts on next neighbors. λ describes the strength of this interaction and ρ parameterizes its range. The distance of ions is denoted as rij = pij R, where R denotes the distance of next neighbors and the pij are suitable coeﬃcients. The electrostatic interaction of an ion with all its neighbors is then written as C = −α Uij
e2 1 , 4πǫ0 R
(2.5)
where α is the Madelung constant. For an attractive interaction (as in a solid), α is positive. It is given (calculated for the ith ion) as Na
Cl
Cl
Cl
(a) Na
Na
Cl
Na
Na
Cl
Cl
Cl
(b) Na
Na
Cl
Na
Fig. 2.12. (a) Experimental and (b) theoretical charge distribution in the (100) plane of NaCl. The lowest contour in the interstitial region corresponds to a charge √ density of 7 e/nm3 and adjacent contours diﬀer by a factor of 2. Diﬀerences are mainly due to the fact that the Xray experiments have been made at room temc perature. Reprinted with permission from [45], 1986 APS
2.4 Mixed Bond
α=
±1 ij
pij
.
23
(2.6)
For a onedimensional chain α = 2 ln 2. For the rocksalt (NaCl) structure (see Sect. 3.4.1) it is α ≈ 1.7476, for the CsCl structure (see Sect. 3.4.2) it is α ≈ 1.7627, and for the zincblende structure (see Sect. 3.4.4) it is α ≈ 1.6381. This shows that ionic compounds prefer the NaCl or CsCl structure. The charge distribution for NaCl is shown in Fig. 2.12. For tetragonal and orthorhombic structures, the Madelung constant has been calculated in [44].
2.4 Mixed Bond The groupIV crystals are of perfectly covalent nature, the I–VII are almost exclusively ionically bonded. For III–V (e.g. GaAs, InP) and II–VI compounds (e.g. CdS, ZnO) we have a mixed case. The (screened) Coulomb potentials of the A and B atoms (in the AB compound) shall be denoted VA and VB . The origin of the coordinate system is in the center of the A and B atom (i.e. for the zincblende structure (see Sect. 3.4.4) at (1/8, 1/8, 1/8)a). The valence electrons then see the potential Vcrystal = VA (r − rα ) + VB (r − rβ ) , (2.7) α
β
where the sum α (β) runs over all A (B) atoms. This potential can be split into a symmetric (Vc , covalent) and an antisymmetric (Vi , ionic) part (2.8b), i.e. Vcrystal = Vc + Vi 1 VA (r − rα ) + VB (r − rα ) Vc = 2 α α ⎫ ⎬ + VB (r − rβ ) + VA (r − rβ ) (2.8a) ⎭ β β 1 VA (r − rα ) − VB (r − rα ) Vi = 2 α α ⎫ ⎬ + VA (r − rβ ) . (2.8b) VB (r − rβ ) − ⎭ β
β
For homopolar bonds Vi = 0 and the splitting between bonding and antibinding states is Eh , which mainly depends on the bond length lAB (and the related overlap of atomic wavefunctions). In a partially ionic bond the orbitals are not symmetric along A–B, but the center is shifted towards the more electronegative atom (Figs. 2.7c,d and 2.13).
24
2 Bonds
(a)
(b)
Fig. 2.13. Schematic representation of (a) bonding and (b) antibinding sp3 orbitals. From [46]
The band splitting3 between the (highest) bonding and (lowest) antibinding state Eba is then written as Eba = Eh + iC ,
(2.9)
where C denotes the band splitting due to the ionic part of the potential and depends only on VA − VB . C is proportional to the difference of the
Fig. 2.14. Values of Eh and C for various AN B 8−N compounds. The dashed line fi = 0.785 separates 4fold from 6fold coordinated structures. Most data taken from [47] 3
This energy should not be confused with the bandgap ΔEcv , the energy separation of the highest valenceband state and the lowest conductionband state. The energy splitting Eba is the energy separation between the centers of the valence and conduction bands. Mostly, the term Eg is used for ΔEcv .
2.5 Metallic Bond
25
electronegativities X of the A and B atoms, C(A, B) = 5.75(XA − XB ). A material thus takes a point in the (Eh ,C) plane (Fig. 2.14). The absolute 2 value for the band splitting is given as Eba = Eh2 + C 2 . The ionicity of the bond is described with the ionicity (after Phillips) fi , deﬁned as [48] fi =
Eh2
C2 . + C2
(2.10)
The covalent part is 1 − fi . In Table 2.1 the ionicity is given for a number of binary compounds. The ionicity can also be interpreted as the angle tan φ = C/Eh in the (Eh ,C) diagram. The critical value of fi = 0.785 for the ionicity separates quite exactly (for about 70 compounds) the 4fold (diamond, zincblende and wurtzite) from the 6fold (rocksalt) coordinated substances (fi = 0.785 is indicated by a dashed line in Fig. 2.14). Table 2.1. Ionicity fi (2.10) for various binary compounds C Si Ge Sn BAs BP BeTe SiC AlSb BN GaSb BeSe
0.0 0.0 0.0 0.0 0.002 0.006 0.17 0.18 0.25 0.26 0.26 0.26
AlAs BeS AlP GaAs InSb GaP InAs InP AlN GaN MgTe InN
0.27 0.29 0.31 0.31 0.32 0.33 0.36 0.42 0.45 0.50 0.55 0.58
BeO ZnTe ZnO ZnS ZnSe HgTe HgSe CdS CuI CdSe CdTe CuBr
0.60 0.61 0.62 0.62 0.63 0.65 0.68 0.69 0.69 0.70 0.72 0.74
CuCl CuF AgI MgS MgSe CdO HgS MgO AgBr LiF NaCl RbF
0.75 0.77 0.77 0.79 0.79 0.79 0.79 0.84 0.85 0.92 0.94 0.96
2.5 Metallic Bond In a metal, the positively charged atomic cores are embedded in a more or less homogeneous sea of electrons. The valence electrons of the atoms become the conduction electrons of the metal. These are freely moveable and at T = 0 K there is no energy gap between ﬁlled and empty states. The bonding is mediated by the energy reduction for the conduction electrons in the periodic potential of the solid compared to free atoms. This will be clearer when the band structure is discussed (Chap. 6). In transition metals the overlap of (partially ﬁlled) inner shells (d or f) can also contribute to the bonding.
26
2 Bonds
2.6 vanderWaals Bond The vanderWaals bond is a dipole bond that leads to bonding in the noblegas crystals (at low temperature). Ne, Ar, Kr and Xe crystallize in the densely packed fcc lattice (see Sect. 3.3.5). He3 and He4 represent an exception. They do not solidify at zero pressure at T = 0 K due to the large zeropoint energy. This quantummechanical effect is especially strong for oscillators with small mass. When two neutral atoms come near to each other (distance of the nuclei R), an attractive dipole–dipole interaction −AR−6 arises (London interaction) the vanderWaals interaction. The quantummechanical overlap of the (ﬁlled) shells leads to a strong repulsion +BR−12 . Altogether, a binding energy minimum results for the Lennard–Jones potential VLJ (see Fig. 2.15) VLJ (R) = −
B A + 12 . R6 R
(2.11)
The energy minimum Emin = −A2 /(2B) is at R = (2B/A)1/6 .
Fig. 2.15. Lennard–Jones potential (2.11) for A = 1 and two values of B
The origin of the attractive dipole–dipole interaction can be understood from a onedimensional (1D) model as follows: Two atoms are modeled by their ﬁxed positively charged nuclei in a distance R and their negatively charged electron shells that are polarizable, i.e. can be displaced along one direction x. Additionally, we assume (two identical) 1D harmonic oscillators for the electron motion at the positions 0 and R. Then, the Hamilton operator H0 of the system without interaction (R is very large) H0 =
1 2 1 2 p + Cx21 + p + Cx22 . 2m 1 2m 2
(2.12)
2.7 Hamilton Operator of the Solid
27
The indices 1 and 2 denote the two electrons of atoms. x1 and x2 are the displacements ofthe electrons. Both harmonic oscillators have a resonance frequency ω0 = C/m, and the zeropoint energy is ω0 /2. Taking into account the Coulomb interaction of the four charges, an additional term H1 arises H1 =
e2 e2 e2 e2 2e2 + − − ≈ − 3 x1 x2 . R R + x1 + x2 R + x1 R − x2 R
(2.13)
The approximation is valid for small amplitudes xi ≪ R. A separation of variables can be achieved by transformation to the normal modes x1 + x2 x1 − x2 xs = √ , xa = √ . (2.14) 2 2 Then we ﬁnd H = H0 + H1
1 2 1 1 2 1 2e2 2e2 pa + C − 3 x2s + C − 3 x2a . (2.15) ps + = 2m 2 R 2m 2 R This equation is the Hamiltonian of two decoupled harmonic oscillators with the normal frequencies
2 1 2e2 1 2e2 2e2 − C ± 3 /m ≈ ω0 1 ± ω± = + ... . R 2 CR3 8 CR3 (2.16)
The coupled system thus has a lower (zeropoint) energy than the uncoupled. The energy difference per atom is (in lowest order) proportional to R−6 .
2 1 2e2 A 1 =− 6 . (2.17) ΔU = ω0 − (ω+ − ω− ) ≈ −ω0 3 2 8 CR R The interaction is a true quantummechanical effect, i.e. the reduction of the zeropoint energy of coupled oscillators.
2.7 Hamilton Operator of the Solid The total energy of the solid, including kinetic and potential terms, is H=
P2j p2 i + 2mi 2Mj i j +
Zj Zj e2 e2 1 1 + 2 4πǫ0 Rj − Rj  2 4πǫ0 ri − ri  j,j
−
i,j
Zj e2 , 4πǫ0 Rj − ri 
i,i
(2.18)
28
2 Bonds
where ri and Ri are the position operators and pi and Pi are the momentum operators of the electrons and nuclei, respectively. The ﬁrst term is the kinetic energy of the electrons, the second term is the kinetic energy of the nuclei. The third term is the electrostatic interaction of the nuclei, the fourth term is the electrostatic interaction of the electrons. In the third and fourth terms the summation over the same indices is left out. The ﬁfth term is the electrostatic interactions of electrons and nuclei. In the following, the usual approximations in order to treat (2.18) are discussed. First, the nuclei and the electrons tightly bound to the nuclei (inner shells) are united to form ion cores. The remaining electrons are the valence electrons. The next approximation is the Born–Oppenheimer (or adiabatic) approximation. Since the ion cores are much heavier than the electrons (factor ≈ 103 ) they move much slower. The frequencies of the ion vibrations are typically in the region of several tens of meV (phonons, see Sect. 5.2), the energy to excite an electron is typically 1 eV. Thus, the electrons always ‘see’ the momentary position of the ions; the ions, however, ‘see’ the electron motions averaged over many periods. Thus, the Hamiltonian (2.18) is split into three parts: H = Hions (Rj ) + He (ri , Rj0 ) + He−ion (ri , δRj ) .
(2.19)
The ﬁrst term contains the ion cores with their potential and the timeaveraged contribution of the electrons. The second term is the electron motion around the ion cores at their averaged positions Rj0 . The third term is the Hamiltonian of the electron–phonon interaction that depends on the electron positions and the deviation of the ions from their average position δRj = Rj − Rj0 . The electron–phonon interaction is responsible for such effects as electrical resistance and superconductivity.
3 Crystals
3.1 Introduction The economically most important semiconductors have a relatively simple atomic arrangement and are highly symmetric. The symmetry of the atomic arrangement is the basis for the classiﬁcation of the various crystal structures. Using group theory, basic and important conclusions can be drawn about the physical properties of the crystal, such as its elastic and electronic properties. The presence of highly symmetric planes is obvious from the crystal shape of the minerals and their cleavage behavior. Polycrystalline semiconductors consist of grains of ﬁnite size that are structurally perfect. The grain boundaries are a lattice defect (see also Sect. 4.6). Amorphous semiconductors are disordered on the atomic scale, see Sect. 3.3.7.
3.2 Crystal Structure The crystals are built up by the (quasi) inﬁnite periodic repetition of identical building blocks. This lattice (Bravais lattice) is generated by the three fundamental translation vectors a1 , a2 and a3 . These three vectors may not lie in a common plane. The lattice (Fig. 3.1) is the set of all points R (ni are integer numbers)
(a)
(b)
Fig. 3.1. (a) Twodimensional lattice. It can be generated by various pairs of translation vectors. (b) Elementary cells of the lattice. Primitive elementary cells are shaded
30
3 Crystals
R = n1 a1 + n2 a2 + n3 a3 .
(3.1)
The crystal structure is made up by the lattice and the building block that is attached to each lattice point. This building block is called the base (Fig. 3.2). In the simplest case, e.g. for simple crystals like Cu, Fe or Al, this is just a single atom (monoatomic base). In the case of C (diamond), Si or Ge, it is a diatomic base with two identical atoms (e.g. Si–Si or Ge–Ge), in the case of compound semiconductors, such as GaAs or InP, it is a diatomic base with nonidentical atoms such as Ga–As or In–P. There exist far more involved structures, e.g. NaCd2 where the smallest cubic cell contains 1192 atoms. In protein crystals, the base of the lattice can contain 10 000 atoms. In summary: Crystal structure = Lattice × Base.
Base
Fig. 3.2. Crystal structure, consisting of a lattice and a base
3.3 Lattice As described in Sect. 3.2 the lattice is spanned by three translation vectors ai . The lattice symmetry is decisive for the physical properties of the semiconductor. It is completely described by the appropriate groups of the symmetry operations. 3.3.1 Unit Cell The choice of the vectors ai making up the lattice is not unique (Fig. 3.1). The volume that is enclosed in the parallelepiped spanned by the vectors a1 , a2 and a3 is called the elementary cell. A primitive elementary cell is an elementary cell with the smallest possible volume (Fig. 3.1b). In each primitive elementary cell there is exactly one lattice point. The coordination number is the number of nextneighbor lattice points. A primitive cubic (pc) lattice, e.g. has a coordination number of 6. The typically chosen primitive elementary cell is the Wigner–Seitz (WS) cell that reﬂects the symmetry of the Bravais lattice best. The Wigner–Seitz cell around a lattice point R0 contains all points that are closer to this lattice
3.3 Lattice
31
point than to any other lattice point. Since all points fulﬁll such a condition for some lattice point Ri , the Wigner–Seitz cells ﬁll the volume completely. The boundary of the Wigner–Seitz cell is made up by points that have the same distance to R0 and some other lattice point(s). The Wigner–Seitz cell around R0 is constructed by drawing lines from R0 to the next neighbors Rj , taking the point at half distance and erecting a perpendicular plane at (Rj + R0 )/2. The WS cell is the smallest polyhedra circumscribed by these planes. A twodimensional construction is shown in Fig. 3.3.
(b)
(a)
Fig. 3.3. (a) Construction of a twodimensional Wigner–Seitz cell, (b) ﬁlling of space with WS cells
3.3.2 Point Group Besides the translation there are other operations under which the lattice is invariant, i.e. the lattice is imaged into itself. These are: Identity. The neutral element of any point group is the identity that does not change the crystal. It is denoted as 1 (E) in international (Sch¨ onﬂieß) notation. Rotation. The rotation around an axis may have a rotation angle of 2π, 2π/2, 2π/3, 2π/4 or 2π/6 or their integer multiples. The axis is then called n = 1, 2, 3, 4 or 6fold, respectively, and denoted as n (international onﬂieß). Objects with Cn symmetry are depicted in notation) or Cn (Sch¨ Fig. 3.4. Mirror operation with respect to a plane through a lattice point. Different mirror planes are discerned (Fig. 3.5) (after Sch¨ onﬂieß) σh : a mirror plane
C1
C2
C3
C4
C6
Fig. 3.4. Twodimensional objects with perpendicular rotation axis Cn . Note that the circles do not exhibit σh symmetry with respect to the paper plane, i.e. they are diﬀerent on the top and bottom side
32
3 Crystals C4
C2 sv
C2
sv
O
F
H
sd
H
H (b)
(a)
C2
C2
H
F
(c)
Fig. 3.5. Mirror planes: (a) σv (at H2 O molecule), (b) σh (at F2 H2 molecule) and (c) σd
perpendicular to a rotational axis, σv : a mirror plane that contains a rotational axis, and σd : a mirror plane that contains a rotational axis and bisects the angle between two C2 axes. The international notation is ¯2. Inversion. All points r around the inversion center are replaced by −r. The inversion is denoted ¯ 1 (i) in international (Sch¨ onﬂieß) notation. Improper rotation. The improper rotation Sn is a rotation Cn followed immediately by the inversion operation i denoted as n ¯ in international notation. There are ¯ 3, ¯ 4 and ¯ 6 and their powers. Only the combined operation n ¯ is a symmetry operation, while the individual operations Cn and i alone are not symmetry operations. In the Sch¨ onﬂieß notation the improper rotation is deﬁned as Sn = σh Cn , with σh being a mirror operation with a plane perpendicular to the axis of the Cn rotation, denoted as Sn . There are S3 , S4 and S6 and ¯ 3 = S65 , ¯ 4 = S43 and ¯ 6 = S35 . For successive applications, the Sn yield previously known operations, e.g. S42 = C2 , S44 = E, S62 = C3 , S63 = i, S32 = C32 , S33 = σh , S34 = C3 , S36 = E. We note that formally S1 is the inversion i and S2 is the mirror symmetry σ. Objects with Sn symmetry are schematically shown in Fig. 3.6. These symmetry operations form 32 point groups. These groups are shown (with their different notations and elements) in Table 3.1. The highest symmetry is the cubic symmetry Oh = O × i. The tetraeder group Td (methane molecule) is a subgroup of Oh .
S1
S2
S6
S4
S3
Fig. 3.6. Twodimensional objects with perpendicular improper rotation axis Sn . Note that the white and black circles do not exhibit σh symmetry with respect to the paper plane, i.e. they are white on the top and black on the bottom. The circles with a dot in the center exhibit σh symmetry, i.e. they look the same from top and bottom
3.3 Lattice
33
Table 3.1. The 32 point groups System
Class InterSch¨ onnational ﬂieß
Symmetry elements
triclinic
1 ¯ 1
C1 Ci
E Ei
monoclinic
m 2 2/m
Cs C2 C2h
E σh E C2 E C2 i σh
orthorhombic
2mm 222 mmm
C2v D2 D2h
E C2 σv′ σv′′ E C2 C2′ C2′′ E C2 C2′ C2′′ i σh σv′ σv′′
tetragonal
4 ¯ 4 4/m 4mm ¯ 42m 422 4/mmm
C4 S4 C4h C4v D2d D4 D4h
E E E E E E E
2C4 C2 2S4 C2 2C4 C2 i 2S4 σh 2C4 C2 2σv′ 2σd C2 C2′ C2′′ 2σd 2S4 2C4 C2 2C2′ 2C2′′ 2C4 C2 2C2′ 2C2′′ i 2S4 σh 2σv′ 2σh
3 ¯ 3 3m 32 ¯ 3m ¯ 6 6 6/m ¯ 6m2 6mm 622 6/mmm
C3 S6 C3v D3 D3d
E E E E E
2C3 2C3 2C3 2C3 2C3
C3h C6 C6h D3h C6v D6 D6h
E 2C3 σh 2S3 E 2C6 2C3 C2 E 2C6 2C3 C2 i 2S3 2S6 σh E 2C3 3C2 σh 2S3 3σv E 2C6 2C3 C2 3σv 3σd E 2C6 2C3 C2 3C2′ 3C2′′ E 2C6 2C3 C2 3C2′ 3C2′′ i 2S3 2S6 σh 3σd 3σv
23 m3 ¯ 43m 432 m3m
T Th Td O Oh
E E E E E
trigonal (rhombohedral)
hexagonal
cubic
4C3 4C3 8C3 8C3 8C3
i 2S6 3σv 3C2 3C2 i 2S6 3σd
4C32 3C2 4C32 3C2 i 8S6 3σh 3C2 6σd 6S4 3C2 6C2′ 6C4 3C2 6C2 6C4 i 8S6 3σh 6σd 6S4
3.3.3 Space Group The space group is formed by the combination of the elements of the point group with translations. The combination of a translation along a rotational axis with a rotation around this axis creates a screw axis nm . In Fig. 3.7a, a socalled 41 screw axis is shown. The ﬁrst index n indicates the rotation angle, i.e. 2π/n, the second index indicates the translation, i.e. c/m, c being the periodicity along the axis. There are eleven crystallographically allowed screw rotations.1 1
21 , 31 , 32 , 41 , 42 , 43 , 61 , 62 , 63 , 64 , 65 .
34
3 Crystals
c
(a)
c/2
c/2
c/4
41
42
(b)
glide
21
Fig. 3.7. (a) Schematic drawing of a 41 and 42 screw axis. (b) Schematic drawing of an axial glide reﬂection. The mirror plane is shown with dashed outline. Opposite faces of the cube have opposite color. For comparison a 21 screw axis is shown
The combination of the mirror operation at a plane that contains a rotational axis with a translation along this axis creates a glide reﬂection (Fig. 3.7b). For an axial glide (or bglide) the translation is parallel to the reﬂection plane. A diagonal glide (or dglide) involves translation in two or three directions. A third type of glide is the diamond glide (or dglide). There are 230 different space groups [49].
3.3.4 2D Bravais Lattices There are ﬁve twodimensional (2D) Bravais lattices (Fig. 3.8). These are very important for the description of symmetries at surfaces. The 2D Bravais lattices are the square, hexagonal, rectangular and centeredrectangular lattice.
3.3.5 3D Bravais Lattices In three dimensions, the operations of the point group results in fourteen 3D Bravais lattices (Fig. 3.9), that are categorized into seven crystal classes (trigonal, monoclinic, rhombic, tetragonal, cubic, rhombohedral and hexagonal). These classes are discerned by the conditions for the lengths and the mutual angles of the vectors that span the lattice (Table 3.2). Some classes have several members. The cubic crystal can have a simple (sc), facecentered (fcc) or bodycentered (bcc) lattice. In the following, some of the most important lattices, in particular those most relevant to semiconductors, will be treated in some more detail.
3.3 Lattice
a b
35
a
f
f
b
(a)
(b)
a b
a
f
b
(c)
a b
f
(d)
Fig. 3.8. The twodimensional Bravais lattices with the primitive unit cells: (a) square lattice (a = b, φ = 90◦ ), (b) hexagonal lattice (a = b, φ = 60◦ ), (c) rectangular lattice (a = b, φ = 90◦ ), (d) centeredrectangular lattice (a = b, φ = 90◦ , for the (nonprimitive) rectangular unit cell shown on the right) Table 3.2. Conditions for lengths and angles for the 7 crystal classes. Note that only the positive conditions are listed. The rhombohedral system is a special case of the trigonal class. Conditions for the trigonal and hexagonal classes are the same, however, trigonal symmetry includes a single C3 or S6 axis, while hexagonal symmetry includes a single C6 or S65 axis System
#
triclinic monoclinic orthorhombic tetragonal cubic trigonal (rhombohedral) hexagonal
1 2 4 2 3 1 1 1
lattice symbol
s, s, s, s,
c c, bc, fc bc bc, fc
conditions for the usual unit cell none α = γ = 90◦ or α = β = 90◦ α = β = γ = 90◦ a = b , α = β = γ = 90◦ a = b = c , α = β = γ = 90◦ a = b , α = β = 90◦ , γ = 120◦ a=b=c,α=β=γ a = b , α = β = 90◦ , γ = 120◦
Cubic fcc and bcc Lattices The primitive translation vectors for the cubic facecentered (fcc) and the cubic bodycentered (bcc) lattice are shown in Fig. 3.10 and Fig. 3.11, respectively. Many metals crystallize in these lattices, e.g. copper (fcc) and tungsten (bcc).
36
3 Crystals
cubic, sc
tetragonal
bcc
bc tetragonal
orthorhombic
c orthorhombic
monoclinic
c monoclinic
rhombohedral
fcc
bc orthorhombic
fc orthorhombic
triclinic
hexagonal
Fig. 3.9. The 14 threedimensional Bravais lattices: cubic (sc: simple cubic, bcc: bodycentered cubic, fcc: facecentered cubic), tetragonal (simple and bodycentered), orthorhombic (simple, centered, bodycentered and facecentered), monoclinic (simple and centered), triclinic, rhombohedral and hexagonal
In the fcc lattice, one lattice point sits in the center of each of the six faces of the usual cubic unit cell. The vectors spanning the primitive unit cell are a (3.2) a′ = (ex + ey − ez ) 2 a b′ = (−ex + ey + ez ) 2 a ′ c = (ex − ey + ez ) . 2 In the bcc lattice, one extra lattice point sits at the intersection of the three body diagonals at (a1 + a2 + a3 )/2. The vectors spanning the primitive unit cell are a a′ = (ex + ey − ez ) (3.3) 2 a b′ = (−ex + ey + ez ) 2 a ′ c = (ex − ey + ez ) . 2
3.3 Lattice
37
c' b'
a a'
Fig. 3.10. Primitive translations of the fcc lattice. These vectors connect the origin with the facecenter points. The primitive unit cell is the rhombohedron spanned by these vectors. The primitive translations a′ , b′ and c′ are given in (3.2). The angle between the vectors is 60◦
a
b'
c'
a'
Fig. 3.11. Primitive translations of the bcc lattice. These vectors connect the origin with the lattice points in the cube centers. The primitive unit cell is the rhombohedron spanned by these vectors. The primitive translations a′ , b′ and c′ are given in (3.3). The angle between the vectors is ≈ 109.5◦
Hexagonally Close Packed Lattice (hcp) The 2D hexagonal Bravais lattice ﬁlls a plane with spheres (or circles) with maximum ﬁlling factor. There are two ways to ﬁll space with spheres and highest ﬁlling factor. One is the fcc lattice, the other is the hexagonally close packed (hcp) structure. Both have a ﬁlling factor of 74%. For the hcp, we start with a hexagonally arranged layer of spheres (A), see Fig. 3.12. Each sphere has six nextneighbor spheres. This could, e.g., be a plane in the fcc perpendicular to the body diagonal. The next plane B is
38
3 Crystals
(a)
(b)
Fig. 3.12. Structure of the (a) hcp and (b) fcc lattice. For hcp the stacking is (along the caxis) ABABAB. . . , for fcc (along the body diagonal) ABCABCABC. . .
put on top in such a way that each new sphere touches three spheres of the previous layer. The third plane can now be added in two different ways: If the spheres of the third layer are vertically on top of the spheres of layer A, a plane A’ identical to A has been created that is shifted from A along the stacking direction (normally called the caxis) by chcp = (8/3)1/2 a ≈ 1.633a .
(3.4)
The hcp stacking order is ABABAB. . . , the coordination number is 12. In the fcc structure, the third layer is put on the thus far unﬁlled positions and forms a new layer C. Only the forth layer is again identical to A and is shifted by √ cfcc = 6a ≈ 2.45a . (3.5) The fcc stacking order is ABCABCABC. . . . In the hexagonal plane of the fcc lattice (which will √ later be called a {111} plane) the distance between lattice points is a = a 2, where a0 is the cubic / 0 √ lattice constant. Thus c = 3a0 , just what is expected for the body diagonal. For real materials with hexagonal lattice the ratio c/a deviates from the ideal value given in (3.4). Helium comes very close to the ideal value, for Mg
3.3 Lattice
39
it is 1.623, for Zn 1.861. Many metals exhibit a phase transition between hcp and fcc at higher temperatures. 3.3.6 Polycrystalline Semiconductors A polycrystalline material consists of crystal grains that are randomly oriented with respect to each other. Between two grains a (largeangle) grain boundary (see also Sect. 4.6) exists. An important parameter is the grain size and its statistical distribution. It can be inﬂuenced via processing steps such as annealing. Polycrystalline semiconductors are used in cheap, largearea applications such as solar cells (e.g. polysilicon, CuInSe2 ) or thinﬁlm transistors (polySi) or as nconducting contact material in MOS diodes (polySi) as shown in Fig. 3.13 (see also Fig. 18.23).
150 nm
150 nm
(a)
(b)
150 nm
(c)
Fig. 3.13. Transmission electron micrographs of polycrystalline silicon (polySi). (a) Asdeposited material from lowpressure chemical vapor deposition (LPCVD) at about 620◦ C, grain size is about 30 nm. (b) After conventional processing (annealing at 1150◦ C), average grain size is about 100 nm. (c) After annealing in HCl that provides enhanced point defect injection (and thus increased possibility to form larger grains), average grain size is about 250 nm. Reprinted with permission c from [50], 1989 AIP
3.3.7 Amorphous Semiconductors An amorphous material lacks the longrange order of the direct lattice. It is disordered on the atomic scale. Amorphous silicon is, e.g., denoted as ‘aSi’. The local quantum mechanics provides almost rigorous requirements for the bond length to next neighbors. The constraints for the bond angle are less strict. Covalently bonded atoms arrange in an open network with correlations up to the third and fourth neighbors. The shortrange order is responsible
40
3 Crystals Ge a=0.07
Probability
a=0.09 a=0.12
exp.
4 0.1
(a)
(b)
0.2
12
12
0.3 0.4 0.5 Atom distance (nm)
0.6
Fig. 3.14. (a) A continuous random network model of amorphous silicon containing one dangling bond. Reprinted with permission from [51]. (b) Calculated radial atomic distribution functions of amorphous Ge (solid lines) for three diﬀerent values of the disorder parameter α (3.6) as labeled and experimental result (dashed line). The positions of next, secondnext and thirdnext neighbors are indicted by vertical bars with numbers of their multiplicity (4, 12, and 12). Adapted from [52], reprinted with permission
for the observation of semiconductor properties such as an optical absorption edge and also thermally activated conductivity. In Fig. 3.14a a model of a continuous random network (with a bondangle distortion of less than about 20%) of aSi is depicted. The diameter dSR of the shortrange order region is related to the disorder parameter α via [52] dSR =
a , 2α
(3.6)
where a is the nextneighbor interatomic distance. For a diamond structure √ it is related to the lattice constant by a = 3a0 /4. Typically, a signiﬁcant number of dangling bonds exists. Bonds try to pair but if an odd number of broken bonds exists locally, an unsaturated, dangling bond remains. This can be passivated by a hydrogen atom. Thus, the hydrogenation of amorphous semiconductors is very important. A hydrogen atom can also break an overlong (and therefore weak) bond, saturate one side and eventually leave a dangling bond.
3.4 Important Crystal Structures Now the crystal structures that are important for semiconductor physics will be discussed. These are the rocksalt (PbS, MgO, ....), diamond (C, Si, Ge), zincblende (GaAs, InP, ...) and wurtzite (GaN, ZnO, ...) structures.
3.4 Important Crystal Structures
41
3.4.1 Rocksalt Structure The rocksalt (rs, NaCl) structure (Fig. 3.15a) consists of a fcc lattice with the period a and a diatomic base in which the Cl atom is √ positioned at (0,0,0) and the Na atom at (1/2,1/2,1/2)a with a distance 3a/2. Materials that crystallize (under normal conditions) in the rocksalt lattice are, e.g., KCl, KBr, PbS (galena), PbSe, PbTe, AgBr, MgO, CdO, MnO. AlN, GaN and InN undergo, under high pressure, a phase transition from the wurtzite into the rocksalt structure.
(a)
(b) Fig. 3.15. (a) Rocksalt (NaCl) structure, (b) CsCl structure
3.4.2 CsCl Structure The CsCl structure (Fig. 3.15b) consists of a simple cubic lattice. Similar as for the rocksalt structure, the base consists of different atoms at (0,0,0) and (1/2,1/2,1/2)a. Typical crystals with CsClstructure are TlBr, TlI, CuZn (βbrass), AlNi. 3.4.3 Diamond Structure The diamond structure (Fig. 3.16a) has the fcc lattice. The base consists of two identical atoms at (0,0,0) and (1/4,1/4,1/4)a. Each atom has a tetrahedral conﬁguration. The packing density is only about 0.34. The materials that crystallize in the diamond lattice are C, Ge, Si and αSn. The diamond structure (point group Oh ) has an inversion center, located between the two atoms of the base, i.e. at (1/8,1/8,1/8)a. The radii of the wavefunctions for various groupIV elements increases with the order number (Table 3.3), and accordingly increases the lattice constant.
42
3 Crystals
(b)
(a)
Fig. 3.16. (a) Diamond structure and (b) zincblende structure (black spheres: A atoms, white spheres: B atoms). The tetragonal bonds are indicated Table 3.3. Radii of the wavefunctions in the diamond structure, rs and rp are related to s1 p3 , rd to s1 p2 d1 and lattice constant a0
C Si Ge
rs (nm)
rp (nm)
rd (nm)
a0 (nm)
0.121 0.175 0.176
0.121 0.213 0.214
0.851 0.489 0.625
0.356683 0.543095 0.564613
In Fig. 3.17a the unit cell with tetragonal symmetry of three places along the 111 direction is shown. In Fig. 3.17b the arrangement of atoms along 111 is depicted. The symmetry along this line is at least C3v . At the atoms sites it is Oh . The bond center (BC) and the hexagonal (H) position are a center of inversion and have D3d symmetry. The unoccupied ‘T’ positions have Td symmetry. 3.4.4 Zincblende Structure The zincblende (sphalerite, ZnS) structure (Fig. 3.16b) has a fcc lattice with a diatomic base. The metal (A) atom is at (0, 0, 0) and the nonmetal (B) atom is at (1/4, 1/4, 1/4)a. Thus the cation and anion sublattices are shifted with respect to each other by a quarter of the body diagonal of the fcc lattice. The atoms are tetrahedrally coordinated, a Zn atom is bonded to four S atoms and vice versa. However, no inversion center is present any longer (point group Td ). In the zincblende structure the stacking order of diatomic planes along the body diagonal is aAbBcCaAbBcC. . . . Many important compound semiconductors, such as GaAs, InAs, AlAs, InP, GaP and their alloys (see Sect. 3.7), but also the II–VI compounds ZnS, ZnSe, ZnTe, HgTe, CdSe and CdTe crystallize in the zincblende structure.
3.4 Important Crystal Structures
43
3a 0
A
(a)
BC B BAB T
H
T AAB A
(b) Oh D3d Oh C3v Td D3d Td C3v Oh
Fig. 3.17. (a) Unit cell of the zincblende structure with the indication of tetragonal symmetries. The position of the small white (black ) sphere is the tetrahedrally conﬁgured unoccupied positions of the A (B) sublattice, denoted with ‘T’ in part (b). (b) Line along 111 in the zincblende structure. Full circles denote the positions of the A and B atoms as labeled. Other positions are called the bond center (‘BC’), antibonding (‘AB’) relative to A and B atoms (‘A–AB’, ‘B–AB’), hexagonal (‘H’) and tetrahedral position (‘T’). The point symmetries of the various locations are given in the lower line
Fourfold coordinated materials (zincblende and wurtzite) typically undergo a phase transition into 6fold coordinated structures upon hydrostatic pressure [53]. For GaAs under pressure see [54]. 3.4.5 Wurtzite Structure The wurtzite structure is also called the hexagonal ZnS structure (because ZnS has both modiﬁcations). It consists (Fig. 3.18) of a hcp lattice with a diatomic base. The c/a ratio typically deviates from the ideal value ζ0 = (8/3)1/2 ≈ 1.633 (3.4) as listed in Table 3.4. The Zn atom is located at (0, 0, 0), the S atom at (0, 0, 3/8)a. This corresponds to a shift of 3/8c along the caxis. This factor is called the cellinternal parameter u that has the value u0 = 3/8 = 0.375 for the ideal wurtzite structure. For real wurtzite crystals u deviates from the ideal value, e.g. for groupIII nitrides u > u0 . The ZnS diatomic planes have a stacking order of aAbBaAbB. . . in the wurtzite structure. In Fig. 3.19 the different local structural environment of the atoms in the zincblende and wurtzite structure is shown. Many important semiconductors with large bandgap crystallize in the wurtzite structure, such as GaN, AlN, InN, ZnO, SiC, ZnS2 , CdS und CdSe. 2 For ZnS, CdS and CdTe the hightemperature phase is cubic and the lowtemperature phase hexagonal.
44
3 Crystals
Table 3.4. c/a ratio of various wurtzite semiconductors. Listed is ξ = (c/a−ζ0 )/ζ0 . Data based on [55] material
ξ (%)
material
ξ(%)
material
ξ (%)
material
ξ (%)
AlN GaN InN ZnS ZnSe
−2.02 −0.49 −1.35 0.25 0.06
CdS CdSe CdTe MgS MgSe
−0.61 −0.18 0.25 −0.80 −0.67
CuBr CuCl CuI AgI ZnTe
0.43 0.55 0.74 0.12 0.74
BeO ZnO 6HSiC BN MgTe
−0.61 −1.9 0.49 0.74 −0.67
uc
c
Zn S
a
(b)
(a)
Fig. 3.18. (a) Top view (along the caxis) and (b) side view of the wurtzite structure with the tetragonal bonds indicated. The top (bottom) surface of the depicted structure is termed the Znface, (00.1) (Oface, (00.¯ 1))
(a)
[111]
[0001]
i
m
(b)
Fig. 3.19. Comparison of the tetragonal bonds in the (a) zincblende and (b) wurtzite structure (i: inversion center, m: symmetry plane)
3.4 Important Crystal Structures
45
3.4.6 Chalcopyrite Structure The chalcopyrite (ABC2 , named after ‘fool’s gold’ CuFeS2 ) structure is relevant for I–III–VI2 (with chalcogenide anions) and II–IV–V2 (with pnictide anions) semiconductors such as, e.g., (Cu,Ag)(Al,Ga,In)(S,Se,Te)2 and (Mg,Zn,Cd)(Si,Ge,Sn)(As,P,Sb)2 . A nonmetallic anion atom (‘C’) is tetrahedrally bonded to two different types of cation atoms (‘A’ and ‘B’) as shown in Fig. 3.20. The local surrounding of each anion is identical, two of both the A and B atoms. The structure is often tetragonal, i.e. η = c/(2a) deviates from the ideal value 1; typically η < 1 [56, 57].
Fig. 3.20. Chalcopyrite structure, black and white spheres denote the metal species. The bigger grey spheres represent the nonmetal anion
If the C atom is in the tetrahedral center of the two A and two B atoms, the bond lengths RAC and RBC of the A–C and B–C bonds, respectively, are equal. Since the ideal A–C and B–C bond lengths dAC and dBC are typically unequal, this structure is strained. The common atom C is therefore displaced along [100] and [010] such that it is closer (if dAC < dBC ) to the pair of A atoms and further away from the B atoms. The displacement parameter is 2 2 − RBC 1 RAC + (3.7) 4 a2 and it deviates from the ideal value u0 = 1/4 for the zincblende structure as listed in Table 3.5 for a number of chalcopyrite compounds. In the chalcopy
u=
46
3 Crystals
rite structure RAC RBC
1/2 1 + η2 2 = u + a 16 1/2
2 1 1 + η2 = a. + u− 2 16
(3.8a) (3.8b)
The minimization of the microscopic strain yields (in ﬁrst order) [58] 1 3 d2AC − d2BC + . 4 8 d2AC + d2BC
u∼ =
(3.9)
Compounds with u > uc , uc = 0.265 being a critical displacement parameter, (or u < 1/2 − uc = 0.235) are stable with regard to cation disorder [57]. In Fig. 3.21 the correlation of the calculated value for u according to (3.9) and the experimental values is shown. 0.30
ue px
0.28
0.26
0.24 IIIIVI2 IIIVV2 IVIIIVI2
0.22 0.22
0.24
0.26 ucalc
0.28
0.30
Fig. 3.21. Experimental values uexp of the displacement parameter for various chalcopyrites vs. the calculated value ucalc according to (3.9). Adapted from [58], c reprinted with permission, 1984 APS
3.4.7 Delafossite Structure The I–III–O2 materials crystallize in the trigonal delafossite (CuFeO2 , space group 166, R¯ 3m) structure (Fig. 3.22). This structure is also called caswellsilverite (NaCrS2 ). In Table 3.6 the lattice parameters of some delafossite compounds are given. The (Cu,Ag) (Al,Ga,In)O2 materials are transparent conductive oxides (TCO). We note that Pt and Pd as groupI component create metallike compounds because of the d9 conﬁguration as opposed to the d10 conﬁguration of Cu and Ag.
3.4 Important Crystal Structures
47
Table 3.5. Lattice nonideality parameters η and u (from (3.9)) of various chalcopyrite compounds and their experimentally observed disorder stability (+/− indicates compound with/without order–disorder (D–O) transition, respectively). Data from [57]
CuGaSe2 CuInSe2 AgGaSe2 AgInSe2 CuGaS2 CuInS2 AgGaS2 AgInS2
η
u
D–O
0.983 1.004 0.897 0.96 0.98 1.008 0.895 0.955
0.264 0.237 0.287 0.261 0.264 0.236 0.288 0.262
+ + − +
ZnSiAs2 ZnGeAs2 CdSiAs2 CdGeAs2 ZnSiP2 ZnGeP2 CdSiP2 CdGeP2
+ −
η
u
D–O
0.97 0.983 0.92 0.943 0.967 0.98 0.92 0.939
0.271 0.264 0.294 0.287 0.272 0.264 0.296 0.288
− + − − + − −
Table 3.6. Lattice parameters a, c, and u of some delafossite compounds. Theoretical values are shown with asterisk. Data from [59]
CuAlO2 CuGaO2 CuInO2
a (nm)
c (nm)
u (nm)
0.2858 0.2980 0.3292
1.6958 1.7100 1.7388
0.1099 0.1073∗ 0.1056∗
Ga Cu O ES c
DB ES 2uc
a Fig. 3.22. Hexagonal unit cell of delafossite CuGaO2 . Oxygen atoms are bonded to the Cu in a dumbbell (‘DB’) conﬁguration. In the edgesharing (‘ES’) layer the Ga atoms are octahedrally conﬁgured as GaO6
48
3 Crystals
3.4.8 Perovskite Structure The perovskite structure (calcium titanate, CaTiO3 ) (Fig. 3.23) is relevant for ferroelectric semiconductors (see Sect. 14.3). It is cubic with the Ca (or Ba, Sr) ions (charge state 2+) on the corners of the cube, the O ions (2−) on the face centers and the Ti (4+) in the body center. The lattice is simple cubic, the base is Ca at (0,0,0), O at (1/2,1/2,0), (1/2,0,1/2) and (0,1/2,1/2) and Ti at (1/2,1/2,1/2). The ferroelectric polarization is typically evoked by a shift of the negatively and positively charged ions relative to each other.
O
O2
Ba Ti4+
Ti
(a)
(b)
Ba2+
Fig. 3.23. Perovskite structure (BaTiO3 ), (a) A cell with 12fold (cuboctahedrally) conﬁgured Ba, (b) B cell with octahedrally conﬁgured Ti
3.4.9 NiAs Structure The NiAs structure (Fig. 3.24) is relevant for magnetic semiconductors, such as MnAs, and also occurs in the formation of Ni/GaAs Schottky contacts [60]. The structure is hexagonal. The arsenic atoms form a hcp structure and are trigonal prismatically conﬁgured with six nearest metal atoms. The metal atoms form hcp planes and ﬁll all octahedral holes of the As lattice. For a cubic close packed, i.e. fcc, structure this would correspond to the rocksalt crystal. The stacking is ABACABAC... (A: Ni, B,C: As).
3.5 Polytypism In polytype materials the stacking order is not only hcp or fcc but takes different sequences, such as, e.g., ACBCABAC as the smallest unit cell along the stacking direction. A typical example is SiC, for which in addition to hcp and fcc 45 other stacking sequences are known. The largest primitive unit
3.5 Polytypism
(a)
49
(b)
Fig. 3.24. NiAs structure, metal atoms: dark grey, chalcogenide atoms: light grey C A
B A 2H wurtzite Zn S
C B
B
C
B
C
B
B
A
B
C
C
A
C
A
A
A
B
A
C
C
B
B
A
C
A
B
A
A
B
B
A 3C zincblende
C
A 4H 6H
B C A C B C
A
A
8H
B
10H
A 15R
Fig. 3.25. Polytypes of the zincblende and wurtzite lattice (found in SiC), the letters A, B and C denote the three possible positions of the diatomic layers (see Fig. 3.12)
cell of SiC contains 594 layers. Some of the smaller polytypes are shown in Fig. 3.25. In Fig. 3.26 cubic diamond crystallites and metastable hexagonal and orthorhomic phases (in silicon) are shown. For the ternary alloy (see Sect. 3.7) Zn1−x Cdx S the numbers nh of diatomic layers with hexagonal stacking (AB) and nc of layers with cubic stacking (ABC) have been investigated. CdS has wurtzite structure and ZnS mostly zincblende structure. The hexagonality index α as deﬁned in (3.10) is shown in Fig. 3.27 for Zn1−x Cdx S nh α= . (3.10) nh + nc
50
3 Crystals
(a)
(b)
(c)
Fig. 3.26. Polytypes of diamond found in crystallites (metastable phases in silicon). (a) cubic type (3C) with stacking ABC, inset shows a diﬀractogram and the alignment of the C and Si lattice, (b) rhombohedral 9R crystallite with ABCBCACABA stacking, (c) 9R phase with interface to a hexagonal 2H (AB stacking) c phase. Reprinted with permission from Nature [61], 2001 Macmillan Magazines Limited
1.0 0.8
a
0.6 0.4 0.2 0 0
Zn1xCdxS 0.01 0.02 0.03 0.04 0.05 0.06 x
Fig. 3.27. Hexagonality index α (3.10) of Zn1−x Cdx S for various ternary compositions. Dashed line is a guide to the eye
3.6 Reciprocal Lattice The reciprocal lattice is of utmost importance for the description and investigation of periodic structures, in particular for Xray diffraction, surface electron diffraction, phonons and the band structure. It is the quasiFourier transformation of the crystal lattice. The crystal lattice is also called the direct lattice, in order to distinguish it from the reciprocal lattice.
3.6 Reciprocal Lattice
51
3.6.1 Reciprocal Lattice Vectors When R denotes the set of vectors of the direct lattice, the set G of the reciprocal lattice vectors is given by the condition3 exp (iGR) = 1
(3.11)
for all R ∈ R and G ∈ G. Therefore, for all vectors r and a reciprocal lattice vector G exp (iG(r + R)) = exp (iGr) .
(3.12)
Each Bravais lattice has a certain reciprocal lattice. The reciprocal lattice is also a Bravais lattice, since when G1 and G2 are two reciprocal lattice vectors, then this is obviously true also for G1 + G2 . For the primitive translation vectors a1 , a2 and a3 of the direct lattice, the vectors b1 , b2 and b3 that span the reciprocal lattice can be given directly as 2π (a2 × a3 ) Va 2π b2 = (a3 × a1 ) Va 2π (a1 × a2 ) , b3 = Va b1 =
(3.13a) (3.13b) (3.13c)
where Va = a1 (a2 × a3 ) is the volume of the unit cell spanned by the vectors ai . The volume of the unit cell in the reciprocal space is Va∗ = (2π)3 /Va . The vectors bi fulﬁll the conditions ai bj = 2πδij .
(3.14)
For an arbitrary reciprocal lattice vector G = k1 b1 + k2 b2 + k3 b3 and a vector R = n1 a1 + n2 a2 + n3 a3 in direct space we ﬁnd GR = 2π (n1 k1 + n2 k2 + n3 k3 ) .
(3.15)
The number in brackets is an integer. Thus, it is clear that (3.11) is fulﬁlled. Additionally, we note that the reciprocal lattice of the reciprocal lattice is again the direct lattice. The reciprocal lattice of the fcc is bcc and vice versa. The reciprocal lattice of hcp is hcp (rotated by 30◦ with respect to the direct lattice). For later, we note two important theorems. A (suﬃciently well behaved) function f (r) that is periodic with the lattice, i.e. f (r) = f (r + R) can be expanded into a Fourier series with the reciprocal lattice vectors according to 3
The dot product a · b of two vectors shall also be denoted as ab.
52
3 Crystals
f (r) =
aG exp (iGr) ,
(3.16)
where aG denotes the Fourier component of the reciprocal lattice vector G, aG = V f (r) exp (−iGr) d3 r. If f (r) is lattice periodic, the integral given in (3.17) is zero unless G is a reciprocal lattice vector. aG . (3.17) f (r) exp (−iGr) = 0, G∈ /G V 3.6.2 Miller Indices A lattice plane is the set of all lattice points in a plane spanned by two independent lattice vectors R1 and R2 . The lattice points on that plane form a twodimensional Bravais lattice. The entire lattice can be generated by shifting the lattice plane along its normal n = (R1 × R2 )/R1 × R2 . The plane belongs to the reciprocal lattice vector Gn = 2πn/d, d being the distance between planes. This correspondence between reciprocal lattice vectors and sets of planes allows the orientation of planes to be described in a simple manner. The shortest reciprocal lattice vector perpendicular to the plane is used. The coordinates with respect to the primitive translation vectors of the reciprocal space bi form a triplet of integer numbers and are called Miller indices. The plane described by Gn r = A fulﬁlls the condition for a suitable value of A. The plane intersects the axes ai at the points x1 a1 , x2 a2 and x3 a3 . Thus we ﬁnd Gn xi ai = A for all i. From (3.15) follows Gn a1 = 2πh, Gn a2 = 2πk and Gn a3 = 2πl, where h, k and l are integers. The triplet of integer numbers (hkl), the reciprocal values of the axis intersections in the direct lattice, are the Miller indices. An example is shown in Fig. 3.28.
3 2 1 a3 1 2
a1
a2
1
2
3
3
Fig. 3.28. The plane intersects the axes at 3, 2, and 2. The inverse of these numbers is 1/3, 1/2, and 1/2. The smallest integer numbers of this ratio form the Miller indices (233)
3.6 Reciprocal Lattice
53
Planes are denoted as (hkl) with parentheses. The (outward) normal direction is denoted with [hkl] (square brackets). A set of equivalent planes is denoted with curly brackets as {hkl}. For example, in the simple cubic lattice (100), (010), (001), (−1 00), (0−1 0) are (00−1 ) equivalent and are denoted by {100}. (−1 00) can also be written as (¯ 100). A set of equivalent directions is denoted with hkl. In a cubic lattice the faces of the cubic unit cell are {001}, the planes perpendicular to the area diagonals are {110} and the planes perpendicular to the body diagonals are {111} (Fig. 3.29). In the zincblende lattice the {111} planes consist of diatomic planes with Zn and S atoms. It depends on the direction whether the metal or the nonmetal is on top. These two cases are denoted by A and B. We follow the convention that the (111) plane is (111)A and the metal is on top (as in Fig. 3.16b). For each change of sign the type changes from A to B and vice versa, e.g. (111)A, (1−1 0)B, (−1 − 11)A and (−1 − 1 − 1)B.
Fig. 3.29. Miller indices of important planes for the cubic lattice
In the wurtzite lattice the Miller indices are denoted as [hklm] (Fig. 3.30). Within the (0001) plane three indices hkl are used that are related to the three vectors a1 , a2 and a3 (see Fig. 3.30a) rotated with respect to each other by 120◦ . Of course, the four indices are not independent and l = −(h+k). The third (redundant) index can therefore be denoted as a dot. The caxis [0001] is then denoted as [00.1]. Wurtzite (and trigonal, e.g. sapphire) substrates are available typically with a ([11.0]), r ([01.2]), m ([01.0]) and c ([00.1]) surface orientations (Fig. 3.30b).
54
3 Crystals
[0001] (0001)
a4
(0110) a3
(1100)
(a)
r
m
c
a2
a1
[2110]
a
[0110] [1120]
(b)
Fig. 3.30. (a) Miller indices for the wurtzite (or hcp) structure. (b) Orientation of the a, r, m, and cplane in the wurtzite structure
3.6.3 Brillouin Zone The Wigner–Seitz cell in reciprocal space is called the (ﬁrst) Brillouin zone. In Fig. 3.31, the Brillouin zones for the most important lattices are shown. Certain points in the Brillouin zone are labeled with dedicated letters. The Γ point always denotes k = 0 (zone center). Certain paths in the Brillouin zone are labeled with dedicated Greek symbols. In the Brillouin zone of the fcc lattice (Si, Ge, GaAs, ...) the X point denotes the point at the zone boundary √ in [001] direction (at a distance π/a from Γ ), K for [110] (at a distance (3 2/4)π/a) and L for the [111] direction (at a distance 3/4π/a ≈ 0.87π/a). The straight paths from Γ to X, K, and L are denoted as Δ, Σ, and Λ, respectively.
3.7 Alloys When different semiconductors are mixed various cases can occur: – The semiconductors are not miscible and have a socalled miscibility gap. They will tend to form clusters that build up the crystal. The formation of defects is probable. – They form an ordered (periodic) structure that is called a superlattice. – They form a random alloy.
3.7 Alloys
55
kz
kz
X W
X
D
R
L
S
L
G
D T
S
U
L G
M
Z
X
S
ky
ky
K
kx
kx
(b)
(a) H
kz
D
G kx
G
L R A
P
H
F
L D
D
P
ky
N
S
K
S
L
M
S M
P T'
K
A
(d)
L
H
kz
X
Z
T
T
U
G
G
N
X
(e)
S' H
U G
T
H
(c)
H
Y
ky
S
(f)kx
Fig. 3.31. Brillouin zones and special k points for the (a) primitive cubic (pc), (b) fcc, (c) bcc, and (d) hcp lattice. (e) Brillouin zone for chalcopyrite structure with fcc Brillouin zone shown as dashed outline. (f ) Brillouin zone for orthorhombic lattice with one quadrant shown with dashed lines.
3.7.1 Random Alloys Alloys for which the probability to ﬁnd an atom at a given lattice site is given by the fraction of these atoms (i.e. the stoichiometry) are called random alloys. Deviations from the random population of sites is termed clustering. For a Gex Si1−x alloy this means that any given atom site has the probability x to have a Ge atom and 1 − x to have a Si atom. The probability pn that a Si atom has n nextneighbor Ge atoms is
56
3 Crystals
4 pn = xn (1 − x)4−n , n
(3.18)
and is depicted in Fig. 3.32 as a function of the alloy composition. The symmetry of the Si atom is listed in Table 3.7 for these ﬁve cases. If it is surrounded by four of the same atoms (either Ge or Si), the symmetry is Td . If one atom is different from the other three next neighbors, the symmetry is reduced to C3v since one bond is singled out. For two atoms each the symmetry is lowest (C2v ).
Fig. 3.32. Probability that a Si atom has n nextneighbor Ge atoms in a random Gex Si1−x alloy
In an alloy from binary compound semiconductors such as Alx Ga1−x As the mixing of the Al and Ga metal atoms occurs only on the metal (fcc) sublattice. Each As atom is bonded to four metal atoms. The probability Table 3.7. Probability p (3.18) and symmetry of an A atom being surrounded by n B atoms in a tetrahedrally conﬁgured Bx A1−x random alloy n
p
symmetry
0 1 2 3 4
p4 4p3 (1 − p) 6p2 (1 − p)2 4p(1 − p)p3 (1 − p)4
Td C3v C2v C3v Td
3.7 Alloys
57
that it is surrounded by n Al atoms is given by (3.18). The local symmetry of the As atom is also given by Table 3.7. For AlAsx P1−x the mixing occurs on the nonmetal (anion) sublattice. If the alloy contains three atom species it is called a ternary alloy. If the binary end components have different crystal structure, the alloy shows a transition (or transition range) from one structure to the other at a particular concentration. An example is the alloy between wurtzite ZnO and rocksalt MgO. The Mgx Zn1−x O alloy exhibits wurtzite structure up to about x = 0.5 and rocksalt structure for x > 0.6 [64]. If the alloy contains four atom species it is called a quaternary. A quaternary zincblende alloy can have the mixing of three atom species on one sublattice, such as Alx Gay In1−x−y As or GaAsx Py Sb1−x−y or the mixing of two atom species on both of the two sublattices, such as Inx Ga1−x Asy N1−y . The random placement of different atoms on the (sub)lattice in an alloy represents a perturbation of the ideal lattice and causes additional scattering (alloy scattering). In the context of cluster formation, the probability of an atom having a direct neighbor of the same kind on its sublattice is important. Given a Ax B1−x C alloy, the probability pS to ﬁnd a single A atom surrounded by B atoms is given by (3.19a). The probability pD1 to ﬁnd a cluster of two neighbored A atoms surrounded by B atoms is given by (3.19b). pS = (1 − x)12 pD1 = 12x(1 − x)18 .
(3.19a) (3.19b)
These formulas are valid for fcc and hcp lattices. For larger clusters [65, 66], probabilities in fcc and hcp structures differ. 3.7.2 Phase Diagram The mixture Ax B1−x with average composition x between two materials A and B can result in a single phase (alloy), a twophase system (phase separation) or a metastable system. The molar free enthalpy ΔG of the mixed system is approximated by ΔG = Ωx(1 − x) + kT [x ln(x) + (1 − x) ln(1 − x)] .
(3.20)
The ﬁrst term on the righthand side of (3.20) is the (regular solution) enthalpy of mixing with the interaction parameter Ω, which can depend on x. The second term is the ideal conﬁgurational entropy based on a random distribution of the atoms. The function is shown for various ratios of kT /Ω in Fig. 3.33a. In an equilibrium phase diagram (see Fig. 3.33b) the system is above the binodal curve in one phase (miscible). On the binodal line Tb (x) in the (x, T ) diagram the A and Brich disordered phases have equal chemical potentials, i.e. ∂G/∂x = 0. For Ω independent of x the temperature Tb is given by (3.21a). A critical point is at the maximum temperature Tmg and concentration xmg of the miscibility gap. For Ω independent of x it is given by
58
3 Crystals
Δ
Ω
(a)
(b)
Fig. 3.33. (a) Free enthalpy ΔG of mixed binary system (3.20) in units of Ω for Ω =const. and various values of kT /Ω as labeled. (b) Schematic phase diagram for binary mixture. The temperature is given in units of Ω/k. The solid (dashed) denotes the binodal (spinodal) line
Tmg = Ω/2 and xmg = 1/2. In the region below the spinodal boundary, the system is immiscible and phases immediately segregate (by spinodal decomposition). On the spinodal line Tsp (x) the condition ∂ 2 G/∂x2 = 0 is fulﬁlled. For Ω independent of x the temperature Tsp is given by (3.21b). The region between the binodal and spinodal curves is the metastable region, i.e. the system is stable to small ﬂuctuations of concentration or temperature but not for larger ones. 2x − 1 ln(x) − ln(1 − x) kTsp (x) = 2Ωx(1 − x) .
(3.21a)
kTb (x) = Ω
(3.21b)
In Fig. 3.34 calculated diagrams for GaAsAlAs and GaAsGaP [62] are shown. The arrows denote the critical point. These parameters and the inter350 GaPxAs1x
(a)
AlxGa1xAs
90
Temperature (K)
Temperature (K)
100
80 70
binodal
60 spinodal
50 40 GaAs
x=0.5
AlAs
(b)
300 250 200 150 100 GaAs
x=0.5
GaP
Fig. 3.34. Calculated phase diagrams for (a) Alx Ga1−x As and (b) GaPx As1−x . The binodal (spinodal) curve is shown as solid (dashed) line. Adapted from [62]
3.7 Alloys
59
action parameters for a number of ternary alloys are given in Table 3.8. For example, for Alx Ga1−x As complete miscibility is possible for typical growth temperatures (> 700 K), but for Inx Ga1−x N the In solubility at a typical growth temperature of 1100 K is only 6% [63]. Table 3.8. Calculated interaction parameter Ω(x) (at T = 800 K, 1 kcal/mol= 43.39 meV), miscibilitygap temperature Tmg and concentration xmg for various ternary alloys. Data for InGaN from [63], other data from [62] alloy
Tmg (K)
xmg
Ω(0) kcal/mol
Ω(0.5) kcal/mol
Ω(1) kcal/mol
Alx Ga1−x As GaPx As1−x Gax In1−x P GaSbx As1−x Hgx Cd1−x Te Znx Hg1−x Te Znx Cd1−x As Inx Ga1−x N
64 277 961 1080 84 455 605 1505
0.51 0.603 0.676 0.405 0.40 0.56 0.623 0.50
0.30 0.53 2.92 4.51 0.45 2.13 2.24 6.32
0.30 0.86 3.07 3.96 0.80 1.88 2.29 5.98
0.30 1.07 4.60 3.78 0.31 2.15 2.87 5.63
3.7.3 Virtual Crystal Approximation In the virtual crystal approximation (VCA) the disordered alloy ABx C1−x is replaced by an ordered binary compound AD with D being a ‘pseudoatom’ with properties that are conﬁguration averaged over the properties of the B and C atoms, e.g. their masses or charges. Such an average is weighted with the ternary composition, e.g. the mass is MD = xMB + (1 − x)MC . For example, the A–D force constant would be taken as the weighted average over the A–B and A–C force constants. 3.7.4 Lattice Parameter In the VCA for an alloy a new sort of effective atom is assumed that has an averaged bond length that depends linearly on the composition. Typically, Vegard’s law (3.22), which predicts that the lattice constant of a ternary alloy Ax B1−x C depends linearly on the lattice constants of the binary alloys AC and BC, is indeed fulﬁlled a0 (Ax B1−x C) = a0 (BC) + x[a0 (AC) − a0 (BC)] .
(3.22)
In reality, the bond length of the AC and BC bonds changes rather little (Fig. 3.35a) such that the atoms in the alloy suffer a displacement from
60
3 Crystals
(b) √ Fig. 3.35. (a) Nearneighbor distance ( 3a0 /4) of Inx Ga1−x As as measured by standard Xray diﬀraction (Bragg reﬂection, solid squares) and VCA approximation (dashdotted line). Nearneighbor Ga–As and In–As distances as determined by EXAFS (extended Xray absorption ﬁne structure, solid squares). Dashed lines are guides to the eye. Data from [67]. (b) Secondneighbor distances for Inx Ga1−x As as determined from EXAFS, top: anion–anion distance (for As–As), bottom: cation– cation distance (for In–In, Ga–Ga, and Ga–In). Solid lines in both plots are the √ VCA (a0 / 2). Data from [68] (a)
their average position and the lattice is deformed on the nanoscopic scale. In a lattice of the type Inx Ga1−x As the anions suffer the largest displacement since their position adjusts to the local cation environment. For Inx Ga1−x As a bimodal distribution, according to the As–Ga–As and As–In–As conﬁgura
Fig. 3.36. Theoretical values (T = 0 K) for the cellinternal parameter u as a function of the composition for groupIII nitride alloys. The solid lines are quadratic curves (bowing parameter b is shown) through the points for x = 0, 0.5, and 1.0. Data from [69]
3.7 Alloys
61
tions, is observed (Fig. 3.35b). The cation–cation secondneighbor distances are fairly close to the VCA. While the average lattice parameter in alloys changes linearly with composition, the cellinternal parameter u (for wurtzite structures, see Sect. 3.4.5) exhibits a nonlinear behavior as shown in Fig. 3.36. Therefore physical properties connected to u, such as the spontaneous polarization, will exhibit a bowing. 3.7.5 Ordering Some alloys have the tendency for the formation of a superstructure [70]. Growth kinetics at the surface can lead to speciﬁc adatom incorporation leading to ordering. For example, in In0.5 Ga0.5 P the In and Ga atoms can be ordered in subsequent (111) planes (CuPt structure) instead of being randomly mixed (Fig. 3.37). This impacts fundamental properties such as the phonon spectrum or the bandgap. CuPt ordering on (111) and (¯1¯11) planes 111) and (1¯ 11) planes CuPtB ordering. In Fig. 3.38, a is called CuPtA , on (¯ TEM image of a Cd0.68 Zn0.32 Te epilayer is shown with simultaneous ordering in the CuPt structure (doublet periodicity along [1¯11] and [¯111]) and in the CuAuI structure4 (doublet periodicity along [001] and [¯110]).
Ga In P Td Disordered or “random” alloy
C3v CuPt ordered
Fig. 3.37. CuPtordered ternary alloy In0.5 Ga0.5 P; the lattice symmetry is reduced from Td to C3v 4 The CuAuI structure has tetragonal symmetry. There exists also the CuAuII structure that is orthorhombic.
62
3 Crystals
(b)
(a)
Fig. 3.38. (a) Crosssectional transmission electron microscope image along the [110] zone axis of a Cd0.68 Zn0.32 Te epilayer on GaAs showing ordered domains having a doublet periodicity on the {111} and {001} lattice planes. Two diﬀerent {111} variants are labeled ‘a’ and ‘b’. The doublet periodicity in the [001] is seen in the ‘c’ region. (b) Selectedarea diﬀraction pattern along the [110] zone. Strong peaks are fundamental peaks of the zincblende crystal, weak peaks are due to CuPt ordering, labeled A and B, and CuAuI ordering, labeled C and D. The latter are the weakest due to a small volume fraction of CuAuordered domains. Reprinted c with permission from [71], 2001 AIP [001] [110]
(a)
Cd Zn Se
(b)
(c)
Fig. 3.39. Schematic diagrams of zincblende Cdx Zn1−x Te along [110] with (a) CuAuI type ordering and (b,c) two types of the CuPtB type ordering. Doublet periodicity is along (a) [001] and [¯ 110], (b) [1¯ 11] and (c) [¯ 111]. Reprinted with c permission from [71], 2001 AIP
4 Defects
4.1 Introduction In an ideal lattice each atom is at its designated position. Deviations from the ideal structure are called defects. In the following, we will brieﬂy discuss the most common defects. The electrical activity of defects will be discussed in Sects. 7.5 and 7.7. For the creation of a defect a certain free energy GD is necessary. At thermodynamical equilibrium a (point) defect density proportional to e−GD /kT will always be present (see Sect. 4.3).
4.2 Point Defects Point defects are deviations from the ideal structure involving essentially only one lattice point. The simplest point defect is a vacancy, a missing atom at an atomic position. If an atom is at a position that does not belong to the crystal structure an interstitial (or Frenkel defect) is formed. The formation energy for line or area defects scales with N 1/3 and 2/3 N , respectively, N being the number of atoms in the crystal. Therefore, these defects are not expected in thermodynamic equilibrium. However, the path into thermodynamical equilibrium might be so slow that these defects are metastable and must be considered quasifrozen. There may also exist metastable point defects. By annealing the crystal, the thermodynamic equilibrium concentration might be reestablished. If an atom site is populated with an atom of different order number, an impurity is present. If the number of valence electrons is the same as for the original (or correct) atom, then it is an isovalent impurity and quasi ﬁts into the bonding scheme. If the valence is different, the impurity adds extra (negative or positive) charge to the crystal bonds, which is compensated by the extra, locally ﬁxed charge in the nucleus. This mechanism will be discussed in detail in the context of doping (Chap. 7). If in an AB compound an A atom sits on the B site, the defect is called an antisite defect AB . A point defect is typically accompanied by a relaxation of the surrounding host atoms. As an example, we discuss the vacancy in Si (Fig. 4.1a). The missing atom leads to a lattice relaxation with the next neighbors moving some way into the void (Fig. 4.1b). The bond lengths of the next and secondnext
64
4 Defects
neighbor Si atoms around the neutral vacancy are shown in Fig. 4.1c. The lattice relaxation depends on the charge state of the point defect (Jahn–Teller effect) that is discussed in more detail in Sect. 7.7. In Fig. 4.1d the situation for the positively charged vacancy with one electron missing is shown. One of the two bonds is weakened since it lacks an electron. The distortion is therefore different from that for V 0 .
(a)
(b)
(c)
(d)
Fig. 4.1. (a) Schematic diamond lattice with vacancy, i.e. a missing Si atom without relaxation. (b) Si with neutral vacancy (V 0 ), lattice relaxation and formation of two new bonds. (c) Schematic diagram showing the relaxation of the neighbors around the neutral Si vacancy defect site calculated by an ab initio method. The distances (in ˚ A) on the outer shell of atoms show the distance from the vacant site. The lengths of the two new bonds are also indicated. The bond length in bulk Si is 2.352 ˚ A, the secondneighbor distance 3.840 ˚ A. (d) Si unit cell with positively charged vacancy (V + ). Parts (a,b,d) reprinted with permission from [72]
As an example, we depict in Fig. 4.2a the lowestenergy conﬁguration of a boronrelated defect in silicon. It is Bs –SiT i , i.e. boron on a substitutional site and a selfinterstitial Si on the ‘T’ place with highest symmetry1 (cf. Fig. 3.17). Due to its importance as an acceptor in Si, the conﬁguration and diffusion of B in Si has found great interest [73, 74]. The diffusion of boron 1 The positive charge state is stable, the neutral charge state is metastable since the defect is a negativeU center (see Sect. 7.7.3).
4.3 Thermodynamics of Defects
65
has been suggested [74] to occur via the following route: The boron leaves its substitutional site and goes to the hexagonal site (‘H’) (Fig. 4.2b) with an activation energy of about 1 eV. It can then relax (∼ 0.1 eV) without barrier to the tetrahedral ‘T’ position (Fig. 4.2c). It could then diffuse through the crystal by going from ‘H’ to ‘T’ to ‘H’ and so on. However, longrange diffusion seems to be not possible in this way because the kickin mechanism will bring back the boron to its stable conﬁguration. The pair diffusion mechanism Bs – H T SiT i → Bi → Bs –Sii provides an activation energy of about 1 eV.
(b)
(a)
(c)
eV (d) Fig. 4.2. Conﬁgurations of boron in Si. (a) Substitutional boron and Si selfinterstitial at ‘T’ site. (b) Boron at ‘H’ and (c) boron at ‘T’ site, each with the Si atoms on the Si lattice sites. The large bright ball represents the boron atom, large and small dark balls represent Si atoms. (d) Diﬀusion of the positively charged B– Si state, conﬁguration vs. total energy, with two pathways, kickout (dasheddotted line) and pair diﬀusion (solid line); the activation energy is labeled. Reprinted with c permission from [74], 2001 APS
4.3 Thermodynamics of Defects For a given temperature the free enthalpy G of a crystal (a closed system with regard to particle exchange) G = H − TS
(4.1)
is minimum. H is the enthalpy and S the entropy. The enthalpy H = E + pV is the thermodynamic potential for a system whose only external parameter
66
4 Defects
is the volume V . It is used when the independent variables of the system are the entropy S and pressure p. The free enthalpy is used when the independent parameters are T and p. G0 (H0 ) is the free energy (enthalpy) of the perfect crystal. Hf is the formation enthalpy of an isolated defect. This could be, e.g., the enthalpy of a vacancy, created by bringing an atom from the (later) vacancy site to the surface, or an interstitial, created by bringing an atom from the surface to the interstitial site. In the limit that the n defects do not interact with each other, i.e. their concentration is suﬃciently small, they can be considered independent and the enthalpy is given by H = H0 + nHf .
(4.2)
The increase of entropy due to increased disorder is split into the conﬁgurational disorder over the possible sites, denoted as Sd , and the formation entropy Sf due to localized vibrational modes. The total change ΔG of the free energy is ΔG = G − G0 = n(Hf − T Sf ) − T Sd = nGf − T Sd ,
(4.3)
where Gf = Hf − T Sf denotes the free enthalpy of formation of a single isolated defect. In Table 4.1 experimental values for the formation entropy and enthalpy are given for several defects. The defect concentration is obtained by minimizing ΔG, i.e. ∂ΔG ∂Sd = Gf − T =0. ∂n ∂n
(4.4)
Table 4.1. Formation enthalpy Hf and entropy Sf of interstitials (I) and vacancy (V ) in Si and the Ga vacancy in GaAs. Data for Si from [75], for GaAs from [76] Material
defect
Hf (eV)
Sf (kB )
Si Si GaAs
I V VGa
3.2 2.0 3.2
4.1 ∼1 9.6
The entropy Sd due to disorder is given as Sd = kB ln W ,
(4.5)
where W is the complexion number, usually the number of distinguishable ways to distribute n defects on N lattice sites
N! N . (4.6) W = = n n!(N − n)!
4.4 Dislocations
With Stirling’s formula ln x! ≈ x(ln x − 1) for large x we obtain
∂Sd N N N −n = kB ln + ln . ∂n n N −n n
67
(4.7)
If n ≪ N and ∂N/∂n = 0, the right side of (4.7) reduces to kB ln(N/n). The condition (4.4) reads Gf + kB T ln(n/N ), or
Gf n = exp − . N kB T
(4.8)
In the case of several different defects i with a degeneracy Zi , e.g. a spin degree of freedom or several equivalent conﬁgurations, (4.8) can be generalized to
ni Gif = exp − . Zi N kB T
(4.9)
4.4 Dislocations Dislocations are line defects along which the crystal lattice is shifted. The vector along the dislocation line is called line vector L. A closed path around the dislocation core differs from that in an ideal crystal. The difference vector is called the Burger’s vector b. Since the energy of a dislocation is proportional to b2 , only dislocations with the shortest Burger’s vector are stable. The plane spanned by L and b is called the glide plane. In Fig. 4.3 a highresolution image of the atoms around a dislocation and the phase and amplitude of the (111) reﬂection are shown. The phase corresponds to the atomic columns, the amplitude to the displacement of the atoms at the dislocation core (see also Fig. 5.18). For an edge dislocation (Fig. 4.4a) b and L are perpendicular to each other. An extra halfplane spanned by L and b × L is inserted. For a screw dislocation (Fig. 4.4b) b and L are collinear. The solid has been cut along a halfplane up to the dislocation line, shifted along L by the amount b and reattached. The most important dislocations in the zincblende lattice (Fig. 4.5) have the line vector along 110. With the Burger’s vector 1/2a 110 three different types of dislocations can be formed: edge, screw and 60◦ dislocations. The vicinity of the core of the latter is shown in more detail in Fig. 4.5d. We note that the atomistic structure of 60◦ dislocations is different for L along [110] and [−1 10]; depending on whether the cation or anion are in the core, they are labeled α or β dislocations. When materials with different lattice constants are grown on top of each other, the strain can plastically relax via the formation of misﬁt dislocations. A typical network of such dislocations is shown in Fig. 4.6 for InGaAs on InP.
68
4 Defects
(b)
(a)
(c)
(d)
Fig. 4.3. (a) Highresolution transmission electron microscopy image (HRTEM) in the 110 projection of a network of misﬁt dislocations at a GaAs/CdTe/ZnTe interface. Substrate: GaAs (001), 2◦ oﬀ 110, ZnTe buﬀer layer is 2 monolayers thick. (b) Fourier transform with round mask around the (111) Bragg reﬂection. (c) Phase and (d) amplitude images for the mask from (b). From [77]
b b
L (a)
L
(b)
Fig. 4.4. Model of (a) an edge and (b) a screw dislocation. The Burger’s vector b is indicated
4.4 Dislocations
69
[110]
L
b L
(a)
(b)
=0°
(c)
=60°
=90°
(d)
Fig. 4.5. Dislocations in the zincblende structure. The line vector is along [100]. The Burger’s vector 1/2a 110 can create an (a) screw dislocation, a (b) 60◦ dislocation, and (c) an edge dislocation. (d) Atomistic structure of a 60◦ dislocation
Fig. 4.6. Planview transmission electron microscopy image of a network of 110 dislocation lines in InGaAs on InP (001) with a lattice mismatch of about 0.1%. The TEM diﬀraction vector is g = [220]. Reprinted with permission from [78], c 1989 AIP
Around the intersection of a screw dislocation with a surface, the epitaxial growth occurs typically in the form of a growth spiral that images the lattice planes around the defect. It has been found that the addition of impurities can lead to a substantial reduction of the dislocation density. This effect is known as impurity hardening and is caused by a hardening of the lattice due to an increase of the socalled critical resolved shear stress [80]. In Fig. 4.8 the dependence of the dislocation density in GaAs and InP is shown as a function of the carrier density that is induced by the incorporation of (electrically active) groupII
70
4 Defects
(a)
(b)
Etch pit density (cm2)
Fig. 4.7. (a) Atomic force microscopy image of growth spiral around a screw dislocation on a silicon surface; image width: 4 µm. (b) STM image (width: 75 nm) of a screwtype dislocation with a Burgers vector of [0001] on the Nface. The reconstruction is c(6×12). The c(6×12) row directions correspond to ¯ 1100. Reprinted c with permission from [79], 1998 AVS
10
4
10
3
102
101 17 10
InP
GaAs
S Te Zn
S Te Zn 10
18
19
20
17
18
10 10 10 10 3 Carrier concentration (cm )
10
19
10
20
Fig. 4.8. Dislocation density (as revealed by etch pits) for GaAs and InP as a function of the carrier concentration for various concentrations of impurities (S, Se, and Zn). Adapted from [81].
or groupVI atoms (acceptors or donors, cf. Sect. 7.5). The high carrier concentration is unwanted when semiinsulating substrates (cf. Sect. 7.7.6) or low optical absorption (cf. Sect. 9.6) are needed. Thus the incorporation of isovalent impurities, such as In, Ga or Sb in GaAs and Sb, Ga or As in InP, has been investigated and found to be remarkably effective. Material contain
4.5 Stacking Faults
71
ing such impurities in high concentration (> 1019 cm−3 ) must be considered a lowconcentration alloy. The lattice constant is thus slightly changed, which can cause problems in the subsequent (latticemismatched) epitaxy of pure layers.
4.5 Stacking Faults The ideal stacking of (111) planes in the zincblende structure, ABCABC. . . , can be disturbed in various ways and creates area defects. If one plane is missing, i.e. the stacking is ABCACABC, an intrinsic stacking fault is present. If an additional plane is present, the defect is called an extrinsic stacking fault, i.e. ABCABACABC. An extended stacking fault in which the order of stacking is reversed is called a twin lamella, e.g. ABCABCBACBABCABC. If two regions have inverted stacking order they are called twins and their joint interface is called a twin boundary, e.g. . . . ABCABCABCBACBACBA. . . The various types of stacking faults are shown in Fig. 4.9. In Fig. 4.10 a crosssectional image of stacking faults in GaAs on Si is shown. They block each other and thus partially annihilate with increasing thickness. A stacking fault is bounded by two partial dislocations formed by the dissociation of a perfect dislocation. A perfect dislocation with Burger’s vector a/2[110] in a III–V compound is dissociated into two Shockley partials according to [83] a a a ¯¯ [0 1 1] → [1 2 1] + [¯1 1 2] . 2 6 6
(a)
(4.10)
(b)
Fig. 4.9. HRTEM images of (a) thinﬁlm silicon with intrinsic (labeled ‘ISF’) and extrinsic (‘ESF’) stacking faults and twin boundary (‘Twin’). (b) Six monolayer thick hexagonal (wurtzite) CdTe layer in cubic (zincblende) CdTe. Stacking order (from bottom to top) is: ABCABABABABC. . . Reprinted with permission from [86]
72
4 Defects
Fig. 4.10. Crosssectional TEM image showing stacking faults in heteroepitaxial GaAs on Si. Adapted from [82]
Since the dislocation energy is proportional to b2 , the dissociation is energetically favored. The stackingfault energy in undoped GaAs is about 50 mJ m−2 . It is reduced upon doping, e.g. to 6 mJ m−2 for GaAs:Sn with [Sn]≈ 1017 cm−3 .
4.6 Grain Boundaries The boundaries of crystal grains are called grain boundaries. Such defects can have a large impact on the electric properties. They can act as barriers for transport or as carrier sinks. Details of their structure and properties can be found in [84, 85]. The two crystal grains meet each other with a relative tilt and/or twist. The situation is shown schematically in Fig. 4.11a for a small angle between the two crystals. A periodic pattern of dislocations forms at the interface that is called a smallangle grain boundary (SAGB) (Fig. 4.11b). In
(a)
(b)
(c)
(d)
(e)
(f)
Fig. 4.11. Schemes of (a,b,c) pure tilt and (d,e,f ) pure twist boundary, dislocation formation in (c) pure tilt and (f ) twist boundaries.
4.7 Antiphase and Inversion Domains
73
6
Dislocation spacing (μm)
5 4 3 2 1 0
(b)
(a)
(d)
0
(c)
1
2 3 4 Tilt angle (104 rad)
5
(e)
Fig. 4.12. (a) Scheme of a smallangle (pure tilt) grain boundary. (b) Model of edge dislocations in a {110} plane in Ge. (c) Relation of dislocation distance d and tilt angle θ for various smallangle grain boundaries in Ge. Solid line is relation d = 4.0 × 10−8 /θ. (d) Optical image of an etched (CP–4 etch) Ge sample with a c smallangle grain boundary. Reprinted with permission from [87], 1953 APS. (e) HRTEM image of a smallangle grain boundary in Si with dislocations highlighted. From [88]
Fig. 4.12, experimental results for pure tilt SAGB are shown. The dislocation spacing is inversely proportional to the tilt angle θ. An image of a twist SAGB is shown in Fig. 4.13.
4.7 Antiphase and Inversion Domains Antiphase domains occur when one part of the crystal is shifted with respect to another by an antiphase vector p. This does not form a twin. If the polar direction changes between two domains they are called inversion domains.
74
4 Defects
Fig. 4.13. Brightﬁeld TEM image of pure twist boundary with network of pure twist dislocations fabricated by wafer bonding of two Si (001) surfaces with a relative twist. From [89]
¯ In the zincblende structure the [110] and [110] directions are not equivalent. In one case there is a ZnS lattice and in the other a SZn lattice. Both lattices vary by a 90◦ rotation or an inversion operation (which is not a symmetry operation of the zincblende crystal). If, e.g., a zincblende crystal is grown on a Si surface with monoatomic steps (Fig. 4.14), adjoint regions have a different phase; they are called antiphase domains (APD). The antiphase vector is (0, 0, 1)a0 /4. At the boundaries a twodimensional defect,
Fig. 4.14. Monoatomic step on the Si (001) surface and subsequent formation of an antiphase boundary in InP (zincblende)
4.7 Antiphase and Inversion Domains
75
Fig. 4.15. Antiphase domains in InP on Si. HCl etchs InP anisotropically and prepares A planes. The etch patterns of layers with (without) APDs are crossc hatched (linear). Reprinted from [90], 1991, with permission from Elsevier
an antiphase domain boundary, develops. The APD boundary contains bonds between identical atom species. In Fig. 4.15, intertwinning APD boundaries are shown on the surface of InP layers on Si. The antiphase domains can be visualized with an anisotropic etch. In Fig. 4.16a, inversion domains in irondoped ZnO are shown. Between domains the direction of the caxis is reversed. The iron is found preferentially
(21 15
)
(0001)
(a)
(b)
Fe
Fig. 4.16. Transmission electron microscopy of inversion domains in ZnO:Fe. (a) Inversion domains in irondoped ZnO (ZnO:Fe2 O3 =100:1). Arrows denote the orientation of the caxis in the respective domains. (b) Top: bright ﬁeld TEM, bottom Fe distribution from energyﬁltered image. Adapted from [92]
76
4 Defects
in the inversion domain boundary (IDB) (Fig. 4.16b) and plays an important role in its formation [91].
4.8 Disorder Disorder is a general term for deviations from the ideal structure on a microscopic scale. Examples are – The presence of various isotopes of an element. This introduces disorder with regard to the mass of the atoms and impacts mostly phonon properties (see, e.g., Fig. 8.15). – The occupation of lattice sites in alloys (Sect. 3.7) ranging from a random alloy, clustering to (partially) ordered phases.
5 Mechanical Properties
5.1 Introduction The atoms making up the solid have an average position from which they can deviate since they are elastically bonded. The typical atomic interaction potential looks like the one shown in Fig. 2.1. The atoms thus perform a vibrational motion and the solid is elastic. The potential is essentially asymmetric, being steeper for small distances due to quantummechanical overlap of orbitals. However, for small amplitudes around the minimum a harmonic oscillator is assumed (harmonic approximation).
5.2 Lattice Vibrations In the following we will discuss the dispersion relations for lattice vibrations, i.e. the connection between the frequency ν (or energy E = hν = ω) of the wave and its wavelength λ (or kvector k = 2π/λ). 5.2.1 Monoatomic Linear Chain The essential physics of lattice vibrations can best be seen from a onedimensional model that is called the linear chain. The mechanical vibrations will also be called phonons, although technically this term is reserved for the quantized lattice vibrations resulting from the quantummechanical treatment. In the monoatomic linear chain the atoms of mass M are positioned along a line (xaxis) with a period (lattice constant) a at the positions xn0 = na. This represents a onedimensional Bravais lattice. The Brillouin zone of this system is [−π/a, π/a]. The atoms will interact with a harmonic potential, i.e. the energy is proportional to the displacement un = xn − xn0 to the second power. The total potential energy of the system is then: U=
1 C (un − un+1 )2 . 2 n
(5.1)
78
5 Mechanical Properties
The model assumes that the mass points are connected via massless, ideal springs with a spring constant C. If φ(d) is the interaction energy between two atoms as a function of their distance d, C is given by C = φ′′ (a). Again, the harmonic approximation is only valid for small displacements, i.e. un ≪ a. The displacement of the atoms can be along the chain (longitudinal wave) or perpendicular to the chain (transverse wave), see Fig. 5.1. We note that for these two types of waves the elastic constant C must not be the same.
k=1/4 /a
a T L
k=1/2 /a
T L
k=/a T L Fig. 5.1. Visualization of transverse (‘T’) and longitudinal (‘L’) waves in a linear monoatomic chain at diﬀerent wavevectors
When the sum in (5.1) has a ﬁnite number of terms (n = 0,. . . ,N − 1), the boundary conditions have to be considered. There are typically two possibilities: The boundary atoms are ﬁxed, i.e. u0 = uN −1 = 0, the boundary conditions are periodic (Born–von Karman), i.e. ui = uN +i . If N ≫ 1, the boundary conditions play no signiﬁcant role anyway, thus those with the greatest ease for subsequent math are chosen. In solidstate physics typically periodic boundary conditions are used. Boundary phenomena, such as at surfaces, are then treated separately. The equations of motion derived from (5.1) are Mu ¨ n = Fn = −
∂U = −C(2un − un−1 − un+1 ) . ∂un
(5.2)
5.2 Lattice Vibrations
79
We solve for solutions that are periodic in time (harmonic waves), i.e. un (x, t) = un exp(−iωt). Then the time derivative can be executed immediately as u ¨n = −ω 2 un and we obtain: M ω 2 un = C(2un − un−1 − un+1 ) .
(5.3)
If, also, the solution is periodic in space, i.e. is a (onedimensional) plane wave, i.e. un (x, t) = v0 exp[i(kx − ωt)] with x = na, we ﬁnd from the periodic boundary condition exp(ikN a) = 1 and thus k=
2π n , n∈N. a N
(5.4)
It is important that, when k is altered by a reciprocal space vector, i.e. k ′ = k + 2πn/a, the displacements un are unaffected. This property means that there are only N values for k that generate independent solutions. These can be chosen as k = −π/a, . . . , π/a, so that k lies in the Brillouin zone of the lattice. In the Brillouin zone there is a total number of N kvalues, i.e. one 2π 2π for each lattice point. The distance between adjacent kvalues is N a = L , L being the lateral extension of the system. The displacements at the lattice points n and n + m are now related to each other via un+m = v0 exp(ik(n + m)a) = v0 exp(ikna) exp(ikma) = exp(ikma)un .
(5.5)
Thus, the equation of motion (5.3) reads M ω 2 un = C(2 − exp(−ika) − exp(ika))un .
(5.6)
Using the identity exp(ika)+exp(−ika) = 2 cos(ka), we ﬁnd the dispersion relation of the monoatomic linear chain (Fig. 5.2):
ka 4C 4C 1 − cos(ka) 2 2 ω (k) = = sin . (5.7) M 2 M 2 The solutions describe plane waves that propagate in the crystal with a phase velocity c = ω/k and a group velocity vg = dω/dk
4C vg = M
1/2
a cos 2
ka 2
.
(5.8)
In the vicinity of the Γ point, i.e. k ≪ π/a the dispersion relation is linear in k ω(k) = a C/M k . (5.9) We are used to such linear relations for sound (and also light) waves. The phase and group velocity are the same and do not depend on k. Thus, such
80
5 Mechanical Properties
(k)
4C / M
0
1
0
k (/a)
1
Fig. 5.2. Dispersion relation for a monoatomic linear chain
solutions are called acoustic. The sound velocity of the medium is given by cs = a C/M . It is characteristic of the nonhomogeneous medium that, when k approaches the boundary of the Brillouin zone, the behavior of the wave is altered. For k = π/a the wavelength is just λ = 2π/k = 2a, and thus samples the granularity of the medium. The maximum phonon frequency ωm is 4C . (5.10) ωm = M The group velocity is zero at the zone boundary, thus a standing wave is present. Since the force constants of the longitudinal and transverse waves can be different, the dispersion relations are different. The transverse branch of the dispersion relation is 2fold degenerate, unless the two directions that are perpendicular to x are not equivalent. 5.2.2 Diatomic Linear Chain Now we consider the case that the system is made up from two different kinds of atoms (Fig. 5.3). This will be a model for semiconductors with a diatomic base, such as zincblende. We note that the diamond structure also needs to be modeled in this way, although both atoms in the base are the same. The lattice will be the same and the lattice constant will be a. Alternating atoms of sort 1 and 2 with a relative distance of a/2 are on the chain. The displacements of the two atoms are labeled u1n and u2n , both belonging to the lattice point n. The atoms have the masses M1 and M2 . The force constants are C1 (for the 1–2 bond within the base) and C2 (for the 2–1 bond between different bases).
5.2 Lattice Vibrations
81
Fig. 5.3. Visualization of acoustic and optical waves in a diatomic linear chain
The total potential energy of the system is then given as U=
2 1 2 2 1 1 un − u2n + C2 un − u1n+1 . C1 2 2 n n
The equations of motion are M1 u ¨1n = −C1 u1n − u2n − C2 u1n − u2n−1 M2 u ¨2n = −C1 u2n − u1n − C2 u2n − u1n+1 .
(5.11)
(5.12a) (5.12b)
With the planewave ansatz u1n (x, t) = v1 exp [i(kna − ωt)] and u2n (x, t) = v2 exp [i(kna − ωt)] and periodic boundary conditions we ﬁnd 0 = −M1 ω 2 v1 + C1 (v1 − v2 ) + C2 (v1 − exp(−ika)v2 ) 0 = −M2 ω 2 v2 + C1 (v2 − v1 ) + C2 (v2 − exp(ika)v1 ) .
(5.13a) (5.13b)
These equations for v1 and v2 can only be solved nontrivially if the determinant vanishes, i.e. M ω 2 − (C1 + C2 ) C1 + e−ika C2 0 = 1 C1 + eika C2 M2 ω 2 − (C1 + C2 )
= M1 M2 ω 4 − (M1 + M2 )(C1 + C2 )ω 2 + 2C1 C2 (1 − cos(ka)) . (5.14) √ Using the substitutions C+ = (C1 + C2 )/2, C× = C1 C2 , the arithmetic and geometrical averages, and accordingly for M+ and M× , the solution is
1 − cos(ka) 2C× 2 , (5.15) ω (k) = 1 ± 1 − γ2 γM× 2
82
5 Mechanical Properties
with γ=
C× M× . C+ M+
(5.16)
The dispersion relation, as shown in Fig. 5.4, now has (for each longitudinal and transverse mode) two branches. The lower branch (‘−’ sign in (5.15)) is related to the acoustic mode; neighboring atoms have similar phase (Fig. 5.3). For the acoustic mode ω = 0 at the Γ point and the frequency increases towards the zone boundary. The maximum phonon frequency ωm is in the upper branch (‘+’ sign in (5.15)) at the zone center 4C× 4C+ M+ ωm = = . (5.17) 2 γM× M× In the vicinity of the Γ point the dispersion is parabolic with negative curvature: 1 γa 2 2 k . (5.18) ω(k) ∼ = ωm 1 − 2 4 The upper branch is called the optical mode (since it can interact strongly with light, see Sect. 9.7) and neighboring atoms have opposite phase. Thus, four different vibrations exist that are labeled TA, LA, TO, and LO. Both the TA and TO branches are degenerate. At the zone boundary (X point) a frequency gap exists. The gap center is at ωm (5.19) ω ¯X = √ , 2
(k)
4C M / M 2
2C M / M 2
0 1
0
k ( /a)
1
Fig. 5.4. Dispersion relation for a diatomic linear chain.
5.2 Lattice Vibrations
and the total width is ΔωX
C+ M+ − C× M× . = ωm 1 − γ = 2 2 M×
83
(5.20)
The group velocity is zero for optical and acoustic phonons at k = π/a and for optical phonons at the Γ point. Usually two cases are treated explicitly: (i) atoms with equal mass (M = M1 = M2 ) and different force constants or (ii) atoms with unequal mass and identical force constants C = C1 = C2 . For the case C1 = C2 and M1 = M2 , γ = 1 and thus ΔωX = 0. Then the dispersion relation is the same as for the monoatomic chain, except that the k space has been folded since the actual lattice constant is now a/2. M1 = M2 In this case, M+ = M× = M and the dispersion relation is
2 C× 1 − cos(ka) 2C + 2 1± 1− 2 . ω = M C+ 2
(5.21)
At the zone boundary the frequencies for the acoustic and the optical branch are ωX,1 = 2C1 /M with v1 = v2 and ωX,2 = 2C2 /M with v1 = −v2 , respectively (assuming C2 > C1 ). The motion for k = π/a is phase shifted by 180◦ for adjacent bases. Additionally, for the acoustic branch the atoms of the base are in phase, while for the optical branch the atoms of the base are 180◦ out of phase. The vibration looks as if only one of the springs is strained. C1 = C2 In this case, C+ = C× = C and the dispersion relation is
2 M 1 − cos(ka) 2CM + × . ω2 = 1± 1− 2 2 M× M+ 2
(5.22)
At the zone boundary the frequencies for the acoustic and the optical branch are ωX,1 = 2C/M1 with v2 = 0 and ωX,2 = 2C/M2 with v1 = 0, respectively (assuming M2 < M1 ). In the vibration for k = π/a thus only one atom species oscillates, the other does not move. Close to the Γ point the atoms are in phase in the acoustic branch, i.e. v1 = v2 . For the optical branch, the frequency at the Γ point is given by ω = 2C/Mr (with the 2 reduced mass Mr−1 = M1−1 + M2−1 = 2M+ /M× ) and the amplitude ratio is given by the mass ratio: v2 = −(M1 /M2 )v1 , i.e. the heavier atom has the smaller amplitude.
84
5 Mechanical Properties
5.2.3 Lattice Vibrations of a ThreeDimensional Crystal When calculations are executed for a threedimensional crystal with a monoatomic base, there are 3N equations of motion. These are transformed to normal coordinates and represent 3 acoustic branches (1 LA phonon mode and 2 TA phonon modes) of the dispersion relation. In a crystal with a base with p atoms, there are also 3 acoustic branches and 3(p−1) optical branches. For a diatomic base (as in the zincblende structure) there are 3 optical phonon branches (1 LO phonon mode and 2 TO phonon modes). The total number of modes is 3p. The dispersion ω(k) now has to be calculated for all directions of k. In Figs. 5.5 and 5.6, the phonon dispersion in silicon and GaAs is shown along particular lines in the Brillouin zone (cf. Fig. 3.31b). The main differences are: (i) the degeneracy of the acoustic and optical branch at the X point for the groupIV semiconductor is lifted for the III–V semiconductor due to the different mass of the constituents, (ii) the degeneracy of the LO and TO energies at the Γ point for the groupIV semiconductor is lifted for the III–V semiconductor due to the ionic character of the bond and the macroscopic electric ﬁeld connected with the longwavelength LO phonon (see Sect. 5.2.7). We note that the degeneracy of the TA phonon is lifted for propagation along the 110 directions (Σ) because the two transverse directions 001 and 1¯ 10 are not equivalent. The dependence of the phonon frequency on the mass of the atoms (∝ M −1/2 ) can be demonstrated with the isotope effect, visualized for GaAs
Fig. 5.5. Phonon dispersion in Si, experimental data and theory (solid lines: bond charge model, dashed lines: valence force ﬁeld model). Adapted from [93]
5.2 Lattice Vibrations
85
Fig. 5.6. Phonon dispersion in GaAs, experimental data and theory (solid lines, 14parameter shell model). ‘L’ and ‘T’ refer to longitudinal and transverse modes, respectively. ‘I’ and ‘II’ (along [ζ, ζ, 0]) are modes whose polarization is in the (1, ¯ 1, 0) plane. Adapted from [93], based on [94]
in Fig. 5.7. The dependence of the phonon frequencies on the stiffness of the spring can be seen from Fig. 5.8; the smaller lattice constant provides the stiffer spring.
(a)
(b)
Fig. 5.7. (b) Energy of optical phonons in GaAs with diﬀerent isotope content [usc ing the Raman spectra shown in (a)]. Reprinted with permission from [95], 1999 APS
86
5 Mechanical Properties
Fig. 5.8. Optical phonon frequencies (TO: ﬁlled squares, LO: empty squares) for a number of III–V compounds with diﬀerent lattice constant a0 . 1 meV corresponds to 8.065 wave numbers (or cm−1 ). From [100]
5.2.4 Phonons Phonons are the quantized quasiparticles of the lattice vibrations (normal modes). The energy of a phonon can take the discrete values of a harmonic oscillator
1 Eph = n + ω , (5.23) 2 where n denotes the quantum number of the state, which corresponds to the number of energy quanta ω in the vibration. The amplitude of the vibration can be connected to n via the following discussion. For the classical oscillation u = u exp[i(kx − ωt)] the space and time average for the kinetic energy yields Ekin =
1 ρV 2
∂u ∂t
2
=
1 ρV ω 2 u20 , 8
(5.24)
where ρ is the density and V the volume of the (homogeneous) solid. The energy of the oscillation is split in half between kinetic and potential energy. From 2Ekin = Eph we ﬁnd
4 1 2 . (5.25) u0 = n + 2 ρV ω The number of phonons with which a vibrational mode is populated is thus directly related to the classical amplitude square.
5.2 Lattice Vibrations
87
Phonons act with a momentum k, the socalled crystal momentum. When phonons are created, destroyed or scattered the crystal momentum is conserved, except for an arbitrary reciprocalspace vector G. Scattering with G = 0 is called a normal process, otherwise (for G = 0) it is called an umklapp process. 5.2.5 Localized Vibrational Modes A defect in the crystal can induce localized vibrational modes (LVM). The defect can be a mass defect, i.e. one of the masses M is replaced by Md , or the force constants in the neighborhood are modiﬁed to Cd . A detailed treatment can be found in [101]. LVM are discussed, e.g., in [102–104]. First we consider the LVM for the onedimensional, monoatomic chain. If the mass at lattice point i = 0 is replaced by Md = M +ΔM (ǫM = ΔM/M ), the displacements are given by ui = AK i , A being an amplitude, with K=−
1 + ǫM , 1 − ǫM
and the defect phonon frequency ωd is ωd = ωm
1 . 1 − ǫ2M
(5.26)
(5.27)
A real frequency is obtained for ǫM  < 1. ωd is then higher than the highest frequency of the bulk modes ωm = 4C/M (5.10). For ǫM < 0, i.e. the mass of the defect is smaller than the mass of the host atoms, K is negative and K < 1. Thus, the displacement can be written as ui ∝ (−K)i = (−1)i exp (+i log K) .
(5.28)
The numerical value of the exponent is negative, thus the amplitude decreases exponentially from the defect and indeed makes a localized vibrational mode. For small mass Md ≪ M (5.27) yields approximately ωd = 2C/Md . This approximation is the socalled oneoscillator model. Since typically the extension of the localized mode is only a few lattice constants, the picture of LVM remains correct for impurity concentrations up to ∼ 1018 − 1020 cm−3 . For higher concentrations the concept of alloy modes has to be invoked (see Sect. 5.2.6). For the case of groupIII or V substitutional impurities in groupIV semiconductors the change in force constants (treated below) can be neglected to some extent. For silicon (M = 28) and germanium (M = 73) the effect of various substitutions is shown in Fig. 5.9. Now, additionally the force constants left and right of the defect are replaced by Cd = C + ΔC (ǫC = ΔC/C). The displacements are still given by ui = AK i , now with
88
5 Mechanical Properties
Fig. 5.9. Energy of local vibrational modes in Si and Ge. Experimental values at T = 300 K (B in Ge: T = 80 K) taken from [101] and references therein and from [105] (C in Ge). The dashed lines are the mass dependence according to (5.27) scaled to the experimental frequency of the 10 B LVM
K=−
(1 + ǫM )(1 + ǫC ) . 1 − ǫM − 2ǫC
(5.29)
An exponential decrease of the LVM amplitude occurs for negative K that is ensured for ǫM + 2ǫC < 0 (and ǫM > −1 and ǫC > −1). The defect frequency is given by
ωd = ω m
(1 + ǫC )(2 + ǫC (3 + ǫM )) . 2(1 + ǫM )(2ǫC + 1 − ǫM )
(5.30)
We note that for ǫC = 0 (5.26) and (5.27) are recovered. For a given mass defect, the change of frequency with ΔC is (in linear order, i.e. for ǫC ≪ 1) ∂ωd (ǫM , ǫC ) 1 − 4ǫM − ǫ2M = ǫC . ∂ǫC 4(1 − ǫM ) 1 − ǫ2M
(5.31)
The linear coeﬃcient diverges for ǫM → −1. For ǫM between −0.968 and 0 the linear coeﬃcient varies between 2 and 1/4. Therefore, a larger force constant (ǫC > 0) increases the LVM frequency of the defect, as expected for a stiffer spring. In a binary compound the situation is more complicated. We assume here that the force constants remain the same and only the mass of the substitution atom Md is different from the host. The host has the atom masses M1 and M2 with M1 < M2 . Substitution of the heavy atom with a lighter one creates a LVM above the optical branch for Md < M2 . Additionally, a level in the
5.2 Lattice Vibrations
89
Relative transmission (%)
0 27
(b)
28
BP
SiGa
12
CGa
40
10
BP
60 14
80 100 400
(a)
11
AlGa
20
NP
GaP 450
500 550 Energy (cm1)
600
Fig. 5.10. (a) Numerical simulation of a linear chain model for GaP (M1 = 31, M2 = 70). Energy of local vibrational modes (dashed (solid ) line): substitution on P (Ga) site) in units of the optical phonon frequency at Γ (ωm = 45.4 meV). The grey areas indicate the acoustic and optical phonon bands. Solid squares are experimental data (from [101]), scaled to the theoretical curve for the 27 AlGa LVM frequency. (b) Diﬀerential transmission spectrum of GaP structure (nitrogendoped layer on zincdoped compensated substrate) against pure crystal (T = 77 K). Data from [106]
gap between the optical and acoustic branch is induced. Such LVM is called a gap mode. Substitution of the lighter atom of the binary compound induces a LVM above the optical branch for Md < M1 . A gap mode is induced for Md > M1 . The situation for GaP is depicted in Fig. 5.10. The energy position of a local vibrational mode is sensitive to the isotope mass of the surrounding atoms. In Fig. 5.11, a highresolution (0.03 cm−1 ) spectrum of the 12 CAs LVM in GaAs is shown together with a theoretical simulation. The various theoretical peak positions are given as vertical bars, their height indicating the oscillator strength. Five experimental peaks are obvious that are due to a total of nine different transitions. The C atom can experience ﬁve different surroundings (see Table 3.7) with the four neighbors being 69 Ga or 71 Ga. The natural isotope mix is an ‘alloy’ 69 Gax 71 Ga1−x As with x = 0.605. The conﬁgurations with Td symmetry contribute one peak each, the lowest (71 Ga surrounding) and highest (69 Ga surrounding) energy transitions. The conﬁgurations with C3v and C2v symmetry contribute each with 2 and 3 nondegenerate modes, respectively. 5.2.6 Phonons in Alloys In an alloy of the type AB1−x Cx the phonon frequencies will depend on the ternary composition. For the binary end materials AB and AC clearly TO and LO frequencies exist. The simplest behavior of the alloy is the onemode behavior (Fig. 5.12d) where the mode frequencies vary continuously (and approximately linearly) with the composition. The oscillator strength (LO–
90
5 Mechanical Properties
GaAs 12
Absorbance (arb. units)
CAs
Exp. Th.
582.0
582.4 582.8 1 Energy (cm )
583.2
Fig. 5.11. Experimental (Exp., T = 4.2 K, resolution 0.03 cm−1 ) and theoretical (Th., artiﬁcial Lorentzian broadening) infrared spectra of LVM of 12 CAs in GaAs. The positions and oscillator strengths of the theoretical transitions involving different conﬁgurations with 69 Ga and 71 Ga isotopes are shown as vertical bars. Data from [102]
TO splitting, (9.61)) remains approximately constant. In many cases, the twomode behavior is observed where the LO–TO gap closes (accompanied by decreasing oscillator strength) and a localized vibrational mode and a gap mode occur for the binary end materials (Fig. 5.12a). Also, a mixedmode behavior (Fig. 5.12b,c) can occur. The masses of the three constituent atoms will be MA , MB , and MC . Without limiting the generality of our treatment, we assume MB < MC . From the considerations in Sect. 5.2.5 on LVM and gap modes, the condition MB < MA , MC
(5.32)
for twomode behavior can be deduced. This ensures a LVM of atom B in the compound AC and a gap mode of atom C in the compound AB. However, it turns out that this condition is not suﬃcient, e.g. Na1−x Kx Cl fulﬁlls (5.32) but exhibits onemode behavior. From a modiﬁed REI model (for k ≈ 0 modes) it has been deduced that MB < μAC =
MA M C < MA , MC M A + MC
(5.33)
is a necessary and suﬃcient condition (unless the force constants between A– B and A–C are signiﬁcantly different) for twomode behavior [107]. A detailed discussion is given in [108]. Equation (5.33) is a stronger condition than the
5.2 Lattice Vibrations
LO1
localized mode
localized mode
LO1
91
LO1
Frequency
LO TO1
TO1
LO2
TO1
LO2
LO2 TO
gap mode
TO2
TO2
(a) 0
gap mode
(b)
0.5 1 Composition
0
TO2
(c)
0.5 1 Composition
0
(d)
0.5 1 Composition
0
0.5 1 Composition
Fig. 5.12. Schematic behavior of phonon modes in an alloy. (a) Twomode behavior with gap mode and localized mode, (b,c) mixedmode behavior, (b) only localized mode allowed, (c) only gap mode allowed, (d) onemode behavior with neither localized mode nor gap mode allowed
previous one (5.32). If (5.33) is not fulﬁlled the compound exhibits onemode behavior. As an example, we show the mass relations for CdS1−x Sex and Cdx Zn1−x S in Table 5.1 and the experimental phonon energies in Fig. 5.13. Also in Table 5.1 the masses for GaP1−x Asx (GaAs1−x Sbx ) exhibiting two(one) mode behavior are shown. Table 5.1. Atomic masses of the constituents of various ternary compounds, reduced mass μAC (5.33), fulﬁllment of the relation from (5.33) (‘+’: fulﬁlled, ‘−’: not fulﬁlled) and experimental mode behavior (‘2’: twomode, ‘1’: onemode) Alloy
A
B
C
MA
MB
MC
μAC
Rel.
Modes
GaP1−x Asx GaAs1−x Sbx CdS1−x Sex Cdx Zn1−x S
Ga Ga Cd S
P As S Zn
As Sb Se Cd
69.7 69.7 112.4 32.1
31.0 74.9 32.1 65.4
74.9 121.8 79.0 112.4
36.1 44.3 46.4 25.0
+ − + −
2 1 2 1
5.2.7 Electric Field Created by Optical Phonons Adjacent atoms oscillate with opposite phase in an optical phonon. If the bond has (partial) ionic character, this leads to a timedependent polarization and subsequently to a macroscopic electric ﬁeld. This additional ﬁeld will inﬂuence the phonon frequencies obtained from a purely mechanical approach. We consider in the following the case k ≈ 0. The phonon frequency for TO and LO vibrations is given by
92
5 Mechanical Properties 360
320
CdxZn1xS
Wave number (cm1)
Wave number (cm1)
320 300 280 260 240 220
0 ZnS
CdS1xSex
300
340
280 260 240 220 200 180
0.5 x
1.0 CdS
160 0 CdS
0.5 x
1.0 CdSe
Fig. 5.13. Phonon energies of Cdx Zn1−x S and CdS1−x Sex as a function of the ternary composition. Experimental data (solid circles) are from [107], dashed lines are guides to the eye
ω0 =
2C Mr
1/2
,
(5.34)
where Mr is the reduced mass of the two different atoms (cf. Sect. 5.2.2). u is the relative displacement u1 − u2 of the two atoms in a diatomic base. When the interaction with the electric ﬁeld E (which will be calculated selfconsistently in the following) is considered, the Hamiltonian for the longwavelength limit is given by [109]: 1 ˆ H(p, u) = 2
1 2 p + b11 u2 + 2b12 u · E + b22 E2 Mr
.
(5.35)
The ﬁrst term is the kinetic energy (p stands for the momentum of the ˙ the second the porelative motion of the atoms 1 and 2 in the base, p = Mr u), tential energy, the third the dipole interaction and the fourth the electricﬁeld energy. The equation of motion for a plane wave u = u0 exp [−i(ωt − k · r)] (¨ u = −ω 2 u) yields Mr ω 2 u = b11 u + b12 E .
(5.36)
Mr u. b12
(5.37)
Thus, the electric ﬁeld is 2 ) E = (ω 2 − ωTO
2 Here, the substitution ωTO = b11 /Mr was introduced that is consistent with (5.34) and b11 = 2C. ωTO represents the mechanical oscillation frequency of the atoms undisturbed by any electromagnetic effects. Already now
5.2 Lattice Vibrations
93
the important point is visible: If ω approaches ωTO , the system plus electric ﬁeld oscillates with the frequency it has without an electric ﬁeld. Therefore the electric ﬁeld must be zero. Since the polarization P = (ǫ − 1)ǫ0 E is ﬁnite, the dielectric constant ǫ thus diverges. The polarization is ˆ = − (b12 u + b22 E) . P = −∇E H
(5.38)
The displacement ﬁeld is
b212 /Mr D = ǫ0 E + P = ǫ0 E − b22 − 2 E = ǫ0 ǫ(ω)E . ωTO − ω 2
(5.39)
Therefore, the dielectric constant is ǫ(ω) = ǫ(∞) +
ǫ(0) − ǫ(∞) . 2 1 − ωω2
(5.40)
TO
Here, ǫ(∞) = 1 − b22 /ǫ0 is the highfrequency dielectric constant and ǫ(0) = ǫ(∞) + b212 /(b11 ǫ0 ) the static dielectric constant. The relation (5.40) is shown in Fig. 5.14. From the Maxwell equation ∇ · D = 0 for zero free charge we obtain the relation ǫ0 ǫ(ω)∇ · E = 0 .
(5.41)
Thus, either ǫ(ω) = 0 or ∇ · E = 0, i.e. u is perpendicular to k. In the latter case we have a TO phonon and, neglecting retardation effects, using
Dielectric function ()
4 3
(0) ()
2 1 0
1
2
3 0
1 2 Frequency ( / T)
Fig. 5.14. Dielectric function according to (5.40) with (0) = 3 and (∞) = 2 (without damping). Grey area denotes the region of negative
94
5 Mechanical Properties
∇ × E = 0 we ﬁnd E = 0 and therefore ω = ωTO , justifying our notation. In the case of ǫ(ω) = 0, we call the related frequency ωLO and ﬁnd the socalled Lyddane–Sachs–Teller (LST) relation 2 ωLO ǫ(0) = . 2 ωTO ǫ(∞)
(5.42)
This relation holds reasonably well for optically isotropic, heteropolar materials with two atoms in the basis, such as NaI and also GaAs. Since at high frequencies, i.e. ω ≫ ωTO , only the individual atoms can be polarized, while for low frequencies the atoms can also be polarized against each other, ǫ(0) > ǫ(∞) and therefore also ωLO > ωTO . For GaAs, the quotient of the two phonon energies is 1.07. Using the LST relation (5.42), we can write for the dielectric constant 2
ωLO − ω 2 ǫ(ω) = ǫ(∞) . (5.43) 2 − ω2 ωTO The (longwavelength) TOphonon does not create a longrange electric ﬁeld. Using ∇ · D = 0 and (5.39) and looking at the longitudinal ﬁelds, we have ǫ0 E = b12 u + b22 E . This can be rewritten as
1/2
1/2 1 1 Mr − u ∝ −u . E = −ωLO ǫ0 ǫ(∞) ǫ(0)
(5.44)
(5.45)
The (longwavelength) LOphonon thus creates a longrange electric ﬁeld acting against the ion displacement and represents an additional restoring force. This effect is also consistent with the fact that ωLO > ωTO .
5.3 Elasticity The elastic properties of the semiconductor are important if the semiconductor is subjected to external forces (pressure, temperature) or to lattice mismatch during heteroepitaxy. 5.3.1 Stress–Strain Relation In this section, we recall the classical theory of elasticity [110]. The solid is treated as a continuous medium (piecewise homogeneous) and the displacement vector is thus a continuous function u(r) of the spatial coordinates. When the spatial variation ∇u of u is small, the elastic energy can be written as
5.3 Elasticity
U=
1 2
∂ul ∂un 3 Cklmn d r, ∂xm ∂xk
95
(5.46)
where Cklmn is the (macroscopic) tensor of the elastic coeﬃcients. 21 components of this tensor can be independent. For crystals with cubic symmetry the number of independent constants is reduced to 3. An exchange k ↔ l and m ↔ n does not matter, only six indices have to be considered (xx, yy, zz, yz, xz, and xy). The strain components ǫij are symmetrized according to
∂ui 1 ∂uj + . (5.47) ǫij = 2 ∂xi ∂xj The strains ǫxx are along the main axes of the crystal as visualized in Fig. 5.15.
(a)
(b)
(c)
(d)
Fig. 5.15. Deformation of a square (a). (b) Pure hydrostatic deformation (xx = yy = 0.2, xy = 0), (c) pure shear deformation (xx = yy = 0, xy = 0.2), and (d) mixed deformation (xx = yy = 0.1, xy = 0.1)
The stresses1 σkl are then given by σkl = Cklmn ǫmn .
(5.48)
The inverse relation is mediated by the stiffness tensor S. ǫkl = Sklmn σmn .
(5.49)
Typically, the strain components eij or ei are used with the convention xx → 1, yy → 2, zz → 3, yz → 4, xz → 5, and xy → 6: eij = ǫij (2 − δij ) .
(5.50)
Then, σm = Cmn en with the Cij being the elastic constants, i.e. C11 = C1111 , C12 = C1122 and C44 = C1212 . The x, y, and z directions are the main axes of the cubic solid, i.e. the 100 directions. Then, we have explicitly ⎛ ⎞ ⎛ ⎞⎛ ⎞ e1 C11 C12 C12 0 0 0 σ1 ⎜ σ2 ⎟ ⎜ C12 C11 C12 0 0 0 ⎟ ⎜ e2 ⎟ ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎜ σ3 ⎟ ⎜ C12 C12 C11 0 0 0 ⎟ ⎜ e3 ⎟ ⎜ ⎟=⎜ ⎟⎜ ⎟ (5.51) ⎜ σ4 ⎟ ⎜ 0 0 0 C44 0 0 ⎟ ⎜ e4 ⎟ . ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎝ σ5 ⎠ ⎝ 0 0 0 0 C44 0 ⎠ ⎝ e5 ⎠ e6 σ6 0 0 0 0 0 C44
1 The stress is a force per unit area and has the dimensions of a pressure or energy density.
96
5 Mechanical Properties
Values for some semiconductors are given in Table. 5.2. The inverse relation is given by the matrix ⎞ ⎛ S11 S12 S12 0 0 0 ⎜ S12 S11 S12 0 0 0 ⎟ ⎟ ⎜ ⎜ S12 S12 S11 0 0 0 ⎟ ⎟ ⎜ (5.52) ⎜ 0 0 0 S44 0 0 ⎟ , ⎜ ⎟ ⎝ 0 0 0 0 S44 0 ⎠ 0 0 0 0 0 S44
with the stiffness coeﬃcients in this notation given by C11 + C12 (C11 − C12 )(C11 + 2C12 ) C12 = 2 −C C 2 −C11 11 12 + 2C12 1 . = C44
S11 =
(5.53a)
S12
(5.53b)
S44
(5.53c)
We emphasize that in this convention (also called the engineering convention), e.g. e1 = ǫxx and e4 = 2ǫyz . There is also another convention (the physical convention) without this factor of two; in this case the matrix in (5.51) contains the elements 2C44 . We note that for an isotropic material the isotropy parameter ξ is zero ξ=
C0 2C44 + C12 − C11 = =0. C44 C44
(5.54)
This isotropy condition is not obeyed by real semiconductors as shown in Table 5.2. Another relation, known as the Keating criterion [111, 112] Table 5.2. Elastic constants of some cubic semiconductors at room temperature. ξ refers to (5.54) and is a measure for the isotropy, IK refers to the Keating criterion (5.55). For MgO, the Keating criterion is not fulﬁlled because it has (sixfold coordinated) rocksalt structure and is thus not tetrahedrally bonded Material
C11 (1010 Pa)
C12 (1010 Pa)
2C44 (1010 Pa)
ξ
IK
C Si Ge BN GaAs InAs AlAs ZnS MgO
107.64 16.58 12.85 82.0 11.9 8.33 12.05 10.46 29.7
12.52 6.39 4.83 19.0 5.34 4.53 4.686 6.53 15.6
57.74 7.96 6.68 48.0 5.96 3.96 5.94 4.63 9.53
−1.3 −0.56 −0.40 −0.63 −0.20 0.08 −0.48 0.30 −0.96
1.005 1.004 1.08 1.11 1.12 1.22 1.03 1.33 0.80
5.3 Elasticity
IK =
2C44 (C11 + C12 ) =1 (C11 − C12 )(C11 + 3C12 )
97
(5.55)
stems from the consideration of bending and stretching of the tetrahedral bonds in the valence force ﬁeld (VFF) model. It is closely fulﬁlled (Table 5.2), in particular for the covalent semiconductors. If C0 = 0, the Young’s modulus (σnn = Y (n)ǫnn ) is nonspherical (see Fig. 5.16a for GaAs). Typically, the 100 directions are the softest. In terms of the Euler angles (Fig. A.1) the angular dependence of the stiffness constant S11 is (Fig. 5.16b,c) S11 (φ, θ) C11 − C12 C0 (21C11 + 10C12 ) + = (5.56) 0 S11 C0 + C11 − C12 32(C0 + C11 − C12 )(C11 + C12 ) C0 (C11 + 2C12 ) × + 32(C0 + C11 − C12 )(C11 + C12 ) (4 cos 2θ + 7 cos 4θ + 8 cos 4φ sin4 θ) , [001]
[010]
[100]
(a)
(b)
(c)
Fig. 5.16. The directional dependence of the inverse of the Young’s modulus (1/Y (n)) for uniaxial stress (along the direction n) in GaAs. (a) 3D view, arbitrary units, (b) dependence on polar angle θ in the (01–1) plane (for φ = π/4, normalized to S11 ), (c) dependence on polar angle θ in the (010) plane (for φ = 0, normalized to S11 )
98
5 Mechanical Properties
0 where S11 is the stiffness along the 100 directions as given in (5.53a). We note that the Young’s modulus Y (Y of (5.57a) is equivalent to 1/S11 of (5.53a)) and the Poisson ratio ν used for isotropic materials are related to the constants of cubic material by
Y = C11 − ν=
2 2C12 C11 + C12
(5.57a)
C12 . C11 + C12
(5.57b)
For isotropic materials Lam´e’s constants λ and μ are also used. They are given by C11 = λ + 2μ, C12 = λ and C44 = μ. Beyond the dependence of the elastic constants on the bond length (as materialized in the phonon frequencies in Fig. 5.8), they depend on the ionicity. In Fig. 5.17, the elastic constants of various zincblende semiconductors are shown as a function of the ionicity fi . The values for the elastic constants are normalized by e2 /a4 , a being the average nearestneighbor distance. For wurtzite crystals, ﬁve elastic constant are necessary for the stress– strain relation that reads ⎛
C11 ⎜ C12 ⎜ ⎜ C13 Cij = ⎜ ⎜ 0 ⎜ ⎝ 0 0
(a)
C12 C11 C13 0 0 0
(b)
C13 C13 C33 0 0 0
0 0 0 C44 0 0
⎞ 0 0 ⎟ 0 0 ⎟ ⎟ 0 0 ⎟ . ⎟ 0 0 ⎟ ⎠ C44 0 0 21 (C11 − C12 )
(5.58)
(c)
Fig. 5.17. Elastic constants as a function of ionicity for various semiconductors, normalized by e2 /a4 , a being the average nearestneighbor distance. (a) Bulk modulus, B = (C11 + 2C12 )/3, (b,c) shear moduli, (b) Cs = (C11 − C12 )/2. Solid lines are a simple model as discussed in [113]. Reprinted with permission from [114], c 1972 APS
5.3 Elasticity
99
5.3.2 Biaxial Strain In heteroepitaxy (cf. Sect. 11.3.1), a biaxial strain situation arises, i.e. layered material is compressed (or expanded in the case of tensile strain) in the interface plane and is expanded (compressed) in the perpendicular direction. Here, we assume that the substrate is inﬁnitely thick, i.e. that the interface remains planar. Substrate bending is discussed in Sect. 5.3.4. The simplest case is epitaxy on the (001) surface, i.e. e1 = e2 = ǫ . The component e3 is found from the condition σ3 = 0 (no forces in the z direction). All shear strains are zero. For zincblende material it follows ǫ100 ⊥ = e3 = −
2C12 C12 (e1 + e2 ) = − ǫ . C11 C11
(5.59)
For other crystallographic directions the formula is more involved [115]: 2C12 − C0 /2 ǫ C11 + C0 /2 2C12 − 2C0 /3 ǫ . =− C11 + 2C0 /3
ǫ110 ⊥ = −
(5.60)
ǫ111 ⊥
(5.61)
In Fig. 5.18 the strain around misﬁt dislocations at a GaAs/CdTe heterointerface, as calculated from a TEM image (Fig. 4.3), is shown.
xx xz of the strain tensor (with respect to the zx zz GaAs lattice constant) of the dislocation array shown in Fig. 4.3, red /blue: positive/negative value, white: zero. From [77] Fig. 5.18. Components
100
5 Mechanical Properties
For wurtzite crystals and pseudomorphic growth along [00.1] the strain along the caxis is given by ǫ0001 =− ⊥
C13 2C13 (e1 + e2 ) = − ǫ , C33 C33
(5.62)
where ǫ⊥ = (c − c0 )/c0 and ǫ = (a − a0 )/a0 . 5.3.3 ThreeDimensional Strain The strain distribution in twodimensional or threedimensional objects such as quantum wires and dots (see also Chap. 13) is more complicated. A simple analytical solution for the problem of a strained inclusion is only possible for isotropic material parameters [116]. The solution for a sphere can be extended to yield the strain distribution of an inclusion of arbitrary shape. This scheme applies only for isotropic materials and identical elastic properties of the inclusion and the surrounding matrix. The solution will be given in terms of a surface integral of the boundary of the inclusion, which is fairly easy to handle. Several disconnected inclusions can be treated by a sequence of surface integrals. The strain distribution for the inner and outer parts of a sphere with radius ρ0 is given (in spherical coordinates) by 2 1 − 2ν in ǫ0 = ǫin θθ = ǫφφ 3 1−ν 3 2 1 + ν ρ0 out = −2ǫout = ǫ0 θθ = −2ǫφφ , 3 1−ν ρ
ǫin ρρ = ǫout ρρ
(5.63) (5.64)
where ρ denotes the radius, ν the Poisson ratio, and ǫ0 the relative lattice mismatch of the inclusion and the matrix. The radial displacements are 2 1 − 2ν ǫ0 ρ 3 1−ν 2 1 − 2ν 3 1 ρ = ǫ0 . 3 1 − ν 0 ρ2
uin ρ = uout ρ
(5.65) (5.66)
Dividing the displacement by the sphere’s volume, we obtain the displacement per unit volume of the inclusion. From the displacement we can derive 0 per unit volume. the stress σij 1 Y ǫ0 2x2i − xj − xk 4π 1 − ν ρ5 3 1 Y ǫ0 xi xj = , 2 4π 1 − ν ρ5
0 σii =
(5.67)
0 σij
(5.68)
where i, j and k are pairwise unequal indices. Due to the linear superposition V of stresses, the stress distribution σij for the arbitrary inclusion of volume V can be obtained by integrating over V
5.3 Elasticity V σij =
V
0 σij (r − r0 )d3 r .
101
(5.69)
The strains can be calculated from the stresses. When ǫ0 is constant within V , the volume integral can be readily transformed into an integral over the surface ∂V of V using Gauss’ theorem. With the ‘vector potentials’ Aij we fulﬁll divAij = σij . 1 Y ǫ0 xi ei 4π 1 − ν ρ3 1 1 Y ǫ0 xi ej + xj ei =− . 2 4π 1 − ν ρ3
Aii = −
(5.70)
Aij
(5.71)
Equation (5.71) is valid for the case i = j. ei is the unit vector in the ith direction. However, special care must be taken at the singularity r = r0 if r0 lies within V because the stress within the ‘δinclusion’ is not singular (in contrast to the electrostatic analog of a δcharge). Thus, we ﬁnd Y ǫ0 V Aij dS + δij (r0 ) = δ(r − r0 )d3 r . (5.72) σij 1 − ν ∂V V As an example, we show in Fig. 5.19 the numerically calculated strain components [117] (taking into account the different elastic properties of the dot and matrix materials) in the cross section of a pyramidal InAs quantum dot in a GaAs matrix on top of a twodimensional InAs layer. The strain component ǫzz is positive in the 2D layer, as expected from (5.59). However, in the pyramid ǫzz exhibits a complicated dependence and even takes negative values at the apex.
Fig. 5.19. Strain components in an InAs pyramid (quantum dot with {101} faces), embedded in GaAs. The cross section is through the center of the pyramid. The lattice mismatch between InAs and GaAs amounts to ≈ −7%. Reprinted with c permission from [117], 1995 APS
102
5 Mechanical Properties au d
compressive
tensile
ai R
(a)
(b)
Fig. 5.20. (a) Schematic bending of a ﬁlm/substrate system for compressive (left) and tensile (right) ﬁlm strain. (b) Schematic deformation of curved ﬁlm of thickness d. The lattice constants at the inner and outer surface are ai and au , respectively.
5.3.4 Substrate Bending If a latticemismatched layer is pseudomorphically grown on top of a substrate it suffers biaxial strain. For ﬁnite substrate thickness part of the strain will relax via substrate bending. If the substrate is circular, a spherical cap is formed. If the lattice constant of the ﬁlm is larger (smaller) than that of the substrate, the ﬁlm is under compressive (tensile) strain and the curvature is convex (concave) with respect to the outward normal given by the growth direction (Fig. 5.20a). Substrate bending can also be induced by a mismatch f s of the thermal expansion coeﬃcients αth and αth of the ﬁlm and substrate, respectively. If a ﬁlm/substrate system is ﬂat at a given temperature, e.g. growth temperature, a decrease of temperature, e.g. during cooling, will lead f s to compressive (tensile) strain if αth is smaller (larger) than αth . In a curved structure, the lattice constant in the tangential direction increases from ati at the inner surface (r = R = κ−1 ) to atu at the outer surface (r = R + d). Thus, the tangential lattice constant varies with the radial position at (r) = ati (1 + rκ) ,
(5.73)
where d is the layer thickness (Fig. 5.20b). Therefore au = ai (1 + d/R). We note that (5.73) holds in all layers of a heterostructure, i.e. the ﬁlm and the substrate. The lattice constant in the radial direction ar , however, depends on the lattice constant a0 of the local material and is calculated from the biaxial strain condition, such as (5.59). The inplane strain is ǫ = (at − a0 )/a0 (we assume a spherical cap with ǫ = ǫθθ = ǫφφ ). For an isotropic material we ﬁnd ar = a0 (1+ǫ⊥ ) with ǫ⊥ = −2νǫ /(1−ν). The local strain energy density U is given by U=
Y ǫ2 . 1−ν
(5.74)
The total strain energy per unit area U ′ of a system of two layers with lattice constants a1 , a2 , Young’s moduli Y1 , Y2 and thickness d1 , d2 (we assume the same Poisson constant ν in both layers) is
5.3 Elasticity
U′ =
d1
U1 dr +
103
d2
U2 dr .
(5.75)
d1
0
The total strain energy needs to be minimized with respect to ai and R in order to ﬁnd the equilibrium curvature κ. We ﬁnd 6a1 a2 (a2 − a1 )d1 d2 (d1 + d2 )Y1 Y2 a32 d41 Y12 + αY1 Y2 + a31 d42 Y24 α = a1 a2 d1 d2 −a2 d1 (2d1 + 3d2 ) + a1 (6d21 + 9d1 d2 + 4d22 ) . κ=
(5.76)
For a2 = a1 (1 + ǫ) we develop κ to ﬁrst order of ǫ and ﬁnd (χ = Y2 /Y1 ) [118, 119] κ=
d41
+
6χd1 d2 (d1 + d2 ) ǫ. + 6χd21 d22 + 4χd1 d32 + χ2 d42
4χd31 d2
(5.77)
In the case of a substrate (ds ) with a thin epitaxial layer (df ≪ ds ), the radius of curvature is approximately (Stoney’s formula [120]) κ = 6ǫ
df Yf . d2s Ys
(5.78)
Conversely, if the radius of curvature is measured [121], e.g. optically, the ﬁlm strain can be determined during epitaxy. 5.3.5 Scrolling In some cases cylindrically scrolled structures are important, e.g. for thinﬁlm ﬂexible electronics, nanotubes and nanoscrolls. The scrolling of thin layers must be avoided by suitable strain management for thin layers that are lifted off from their substrate for transfer to somewhere else. If the ﬁlm remains attached to its substrate, a scroll can be fabricated as schematically shown in Fig. 5.21. Such structures were ﬁrst reported in [122].
(a)
(b)
(c)
Fig. 5.21. Schematic representation of nanoscroll formation. (a) Strained heterostructure (grey) that is planar due to large substrate thickness, (b) starting removal of sacriﬁcial layer (black ), (c) release of thin ﬁlm into nanoscroll geometry
104
5 Mechanical Properties
y t r
(b)
(a)
Fig. 5.22. (a) Schematic representation of a cylindrically rolled sheet with radial direction r, tangential direction t and direction along the cylinder axis y. (b) SEM images of multiwall InGaAs/GaAs nanoscroll rolled up over about 50 µm. Part (b) from [123]
If bending strain occurs only in one of the tangential directions, the energy density is given by U=
Y (ǫ2 + ǫ2y + 2νǫt ǫy ) , 2(1 − ν 2 ) t
(5.79)
where ǫy is the strain in the unbent direction (cylinder axis) as shown in Fig. 5.22a. For a strained heterostructure made up from two layers the curvature is given by (calculated analogous to (5.77), χ = Y2 /Y1 [119]) κ=
6(1 + ν)χd1 d2 (d1 + d2 ) ǫ, d41 + 4χd31 d2 + 6χd21 d22 + 4χd1 d32 + χ2 d42
(5.80)
which differs from (5.77) only by the factor 1 + ν in the denominator. For cubic material and a (001) surface the energy is given as U100 =
C11 − C12 C12 (ǫt + ǫy )2 + C11 (ǫ2t + ǫ2y ) 2C11
(5.81)
for a scrolling direction along 100. When the (001)oriented ﬁlm winds up along a direction hk0 having an angle φ with the [100] direction (φ = 45◦ for 110), the strain energy is given by (C0 is given by (5.54))
2 ǫt − ǫy sin2 (2φ) . (5.82) Uφ = U100 + C0 2 The strain energy vs. bending radius (= κ−1 ) is shown for a SiGe nanoscroll in Fig. 5.23. First, the relaxation along the cylinder axis plays a minor role. The smallest strain energy is reached for scrolling along 100, also yielding the smaller bending radius (larger curvature). Therefore, the ﬁlm preferentially scrolls along 100. This explains the observed ‘curl’ behavior of scrolls winding up for φ = 0 (Fig. 5.23b).
5.3 Elasticity
105
=14° [010]
[100]
(a)
(b)
30 μm
Fig. 5.23. (a) Strain energy (in units of the strain energy of the ﬂat pseudomorphic layers) of a scroll of a 4layer SiGe structure (Si0.3 Ge0.7 , Si0.6 Ge0.4 and Si0.8 Ge0.2 , each 3 nm thick and a 1nm Si cap) as a function of radius for winding directions along 100 and 110. Top (bottom) curves without (with complete) strain relaxation along the cylinder axis. Vertical lines indicate the positions of the respective energy minima [119]. (b) SEM image of curled InGaAs/GaAs nanoscroll rolled φ = 14◦ oﬀ 100. The stripe from which the ﬁlm was rolled oﬀ is indicated by white dashed lines. Part (b) from [125]
5.3.6 Critical Thickness Strained epitaxial ﬁlms are called pseudomorphic when they do not contain defects and the strain relaxes elastically, e.g. by tetragonal distortion. When the layer thickness increases, however, strain energy is accumulated that will lead at some point to plastic relaxation via the formation of defects. In many cases, a grid of misﬁt dislocations forms at the interface (Figs. 4.6 and 5.24). The average distance p of the dislocations is related to the misﬁt f = (a1 − ◦ a2 )/a2 and √ the edge component b⊥ of the Burger’s vector (for a 60 dislocation b⊥ = a0 / 8) p=
b⊥ . f
(5.83)
Two mechanisms have been proposed for the formation of misﬁt dislocations (Fig. 5.25), the elongation of a grownin threading dislocation [127] and the nucleation and growth of dislocation halfloops [128]. For the modeling of such systems a mechanical approach based on the forces on dislocations [127] or an energy consideration based on the minimum strain energy necessary for defect formation [128–130] can be followed. Both approaches have been shown to be equivalent [131] (if a periodic array of dislocations is considered). In [132] it was pointed out that the ﬁnite speed of plastic ﬂow also has to be considered to explain experimental data. Temperature affects the observed critical thickness and a kinetic model is needed.
106
5 Mechanical Properties
(b)
(a)
1 μm
g 002
Fig. 5.24. (a) Series of crosssectional TEM images of 100nm thick Gex Si1−x layers on Si(001) with diﬀerent ternary compositions x = 0.1, 0.2, 0.5, and 1.0. The growth temperature was 550◦ C. The transition from commensurate to incommensurate growth is obvious. From [124]. (b) Plan view 022 TEM bright ﬁeld image of a 250nm Ge0.15 Si0.85 layer on Si (001), annealed at about 700◦ C. The arrow denotes c the position of a dislocation loop. Reprinted with permission from [126], 1989 AVS
c
h3
a
b
c
b
h2
a
h1
c
b
(a)
a
(b)
Fig. 5.25. Schematic formation of misﬁt dislocations by (a) elongation of a grownin threading dislocation and (b) by the nucleation and growth of dislocation halfloops. (a) depicts a threading dislocation. Initially, for thickness h1 the interface is coherent ‘a’, for larger thickness h2 the interface is critical and the force of the interface on the dislocation is equal to the tension in the dislocation line, ‘b’. For larger thickness, e.g. h3 , the dislocation line is elongated in the plane of the interface, ‘c’. In (b) ‘a’ denotes a subcritical dislocation halfloop, ‘b’ depicts a halfloop being stable under the misﬁt stress and for ‘c’ the loop has grown under the misﬁt stress into a misﬁt dislocation line along the interface
In the following, isotropic materials and identical elastic constants of substrate and thin ﬁlm are assumed, following [131]. The interface plane is the (x,y)plane, the growth direction is z. The energy Ed of a periodic dislocation array with period p and Burgers vector b = (b1 , b2 , b3 ) is
5.3 Elasticity
Y β2 8π(1 − ν 2 )
p [1 − exp(−4πh/p)] β 2 = b21 + (1 − ν)b22 + b23 ln 2πq 2 4πh exp(−4πh/p) + b1 − b23 p 1 − exp(−4πh/p)
4πh 2 exp(−4πh/p) 1 2 2 − b 1 + b3 2 2 p [1 − exp(−4πh/p)]
Ed =
+b23
107
(5.84)
2πh exp(−2πh/p) , p 1 − exp(−2πh/p)
where h is the ﬁlm thickness and q denotes the cutoff length for the dislocation core, taken as q = b. The misﬁt strain including the relaxation due to disloˆ in the two orthogonal interface 110 cations with Burger’s vectors b and b ˆ . We chose the coordinate system such that n = (1, 0, 0) directions n and n ˆ = (0, 1, 0) (the and n With respect to these axes the z direction remains). √ 1 1 √1 Burger’s vectors are ± 2 , 2 , 2 a0 / 2. The misﬁt strain ǫm ij is reduced due r to the dislocation formation to the ‘relaxed’ misﬁt strain ǫij with ǫrij = ǫm ij +
ˆ j + ˆbj n ˆi bi nj + bj ni ˆbi n + , 2p 2p
(5.85)
with an associated stress σij . The strain energy Es of the layer due to the relaxed misﬁt is then 1 hσij ǫrij 2 Y (1 + ν) 2 f . lim Es = 2h p→∞ 1−ν Es =
(5.86) (5.87)
The total strain energy E is given by pE = 2Ed + 2Ec + pEs
(5.88)
E∞ = lim E ,
(5.89)
p→∞
with the core energy Ec of the dislocation that needs to be calculated with an atomistic model (not considered further here). This energy is shown in Fig. 5.26a for the material parameters of Ge0.1 Si0.9 /Si(001) (misﬁt −0.4%) for various layer thicknesses as a function of 1/p. This plot looks similar to that for a ﬁrstorder phase transition (with 1/p as the order parameter, cmp. Fig. 14.7a). For a certain critical thickness hc1 the energy of the layer without any dislocation and the layer with a particular dislocation density p1 are identical (E − E∞ = 0) and additionally ∂E/∂pp=p1 = 0. However, between p → ∞ and p = p0 there is an energy barrier. The critical thickness hc2 is reached when
108
(a)
5 Mechanical Properties
(b)
Fig. 5.26. (a) Theoretical calculation for the strain energy vs. inverse dislocation density for various thicknesses of Ge0.1 Si0.9 layers on Si (001). The ordinate is b/2p, b/2 being the edge component of the Burgers vector and p being the dislocation spacing. The abscissa is the strain energy E scaled with E∞ (5.89). (b) Critical thickness for Gex Si1−x layers on Si (001). The solid line is theory (hc2 ) according to (5.91). Data points are from [135] (squares, growth temperature of 750◦ C) and from [124] (triangles for growth temperature of 550◦ C)
∂E/∂p p→∞ = 0 ,
(5.90)
i.e. the energy decreases monotonically for increasing dislocation density up to the global energy minimum at a certain equilibrium dislocation spacing p2 . Equation (5.90) leads to the following implicit equation for the determination of hc2 : b −16 + 3b2 + 8(−4 + ν) ln (2hc2 /q) , (5.91) hc2 = 128f π(1 + ν) √ with the length of the Burgers vector b = a0 / 2. The theoretical dependence of hc2 for Gex Si1−x /Si(001) with varying composition is shown in Fig. 5.26b together with experimental data. The critical thickness for a fairly high growth temperature is much closer to the energetic equilibrium than that deposited at lower temperature. This shows that there are kinetic limitations for the system to reach the mechanical equilibrium state. Also, the experimental determination of the critical thickness is affected by ﬁnite resolution for large dislocation spacing, leading generally to an overestimate of hc . In zincblende materials two types of dislocations are possible, α and β, with Ga and Asbased cores, respectively. They have [¯110] and [110] line directions for a compressively strained interface. The α dislocation has the larger glide velocity. Therefore, strain relaxation can be anisotropic with regard to the 110 directions for zincblende material, e.g. InGaAs/GaAs [133, 134].
5.4 Cleaving
109
5.4 Cleaving The cleavage planes of the diamond structure are {111} planes. It is easiest to break the bonds connecting the double layers in the 111 directions. The cleavage planes of the zincblende structure are {110} planes. Due to the ionic character, breaking the bonds connecting the double layers in the 111 directions would leave charged surfaces, which is energetically unfavorable. The {100} planes contain only one sort of atom and would also leave highly charged surfaces. The {110} planes contain equal amounts of A and B atoms and are neutral. Ideally, the cleaving plane is atomically ﬂat or exhibits large monoatomically ﬂat terraces. However, certain dopants in high concentrations, e.g. GaAs:Te, can induce a rough surface due to lattice distortion [136].
6 Band Structure
Silicon is a metal. A.H. Wilson, 1931 [14]
6.1 Introduction Valence electrons that move in the crystals feel a periodic potential U (r) = U (r + R)
(6.1)
for all vectors R of the direct lattice. The potential1 is due to the effect of the ion cores and all other electrons. Thus a serious manybody problem is present. In principle, the band structure can be calculated from the periodic arrangements of the atoms and their atomic order number. We note that for some problems, e.g. the design of optimal solar cells, a certain band structure is known to be ideal and a periodic atomic arrangement, i.e. a material, needs to be found that generates the optimal band structure. This problem is called the inverse band structure problem.
6.2 Bloch’s Theorem First, we will deduce some general conclusions about the structure of the solution as a consequence of the periodicity of the potential. We ﬁrst investigate the solution of a Schr¨ odinger equation of the type
2 2 ∇ + U (r) Ψ (r) = EΨ (r) (6.2) HΨ (r) = − 2m for an electron. U will be periodic with the lattice, i.e. it will obey (6.1). 1
In this book the form of the potential will never be explicitly given.
112
(a)
6 Band Structure
(b)
(c)
Fig. 6.1. Zone schemes for a band structure: (a) extended, (b) reduced and (c) repetitive zone scheme
Bloch’s theorem says that the eigenstates Ψ of a oneparticle Hamiltonian as in (6.2) can be written as the product of plane waves and a latticeperiodic function, i.e. Ψnk (r) = Aeikr unk (r) .
(6.3)
The√normalization constant A is often omitted. If unk (r) is normalized, A = 1/ V , where V is the integration volume. The wavefunction is indexed with a quantum number n and the wavevector k. The key is that the function unk (r), the socalled Bloch function, is periodic with the lattice, i.e. unk (r) = unk (r + R)
(6.4)
for all vectors R of the direct lattice. The proof is simple in one dimension and more involved in three dimensions with possibly degenerate wavefunctions, see [137]. If Enk is an energy eigenvalue, then Enk+G is also an eigenvalue for all vectors G of the reciprocal lattice, i.e. En (k) = En (k + G) .
(6.5)
Thus the energy values are periodic in reciprocal space. The proof is simple, since the wavefunction (for k + G) exp (i(k + G)r) un(k+G) (r) is for un(k+G) (r) = exp (−iGr) unk (r) obviously an eigenfunction to k. A band structure along one kdirection can be displayed in various zone schemes as depicted in Fig. 6.1. The most frequently used scheme is the reduced zone scheme. In three dimensions, the band structure is typically shown along particular paths in the Brillouin zone, as depicted, e.g., in Fig. 6.2c.
6.3 FreeElectron Dispersion If the entire wavefunction (from (6.3)) obeys the Schr¨ odinger equation (6.2), the Bloch function unk fulﬁlls the equation
6.3 FreeElectron Dispersion
113
Energy (EX)
4 3 2 1
(b)
(a)
(c)
0
X W
L
K X
Fig. 6.2. Dispersion of free electrons (empty lattice calculation, U = 0, shown in the ﬁrst Brillouin zone) in (a) a onedimensional lattice (G = n 2π/a), (b) a simple cubic lattice (G = (h, k, l) 2π/a) and (c) in a fcc lattice. The energy is measured in units of the energy at the Xpoint, EX = (2 /2m)(π/a)2 . The shaded circle in (c) represents the region where the bandgap develops for ﬁnite periodic potential U = 0
−
1 (p + k)2 + U (r) unk (r) = Enk unk (r) , 2m
(6.6)
which is easy to see from p = −i∇. First, we discuss the simplest case of a periodic potential, U ≡ 0. This calculation is also called the empty lattice calculation. The solution of (6.6) is then just constant, i.e. uk = c and Ψk (r) = c exp (ikr). The dispersion of the free electron is then given by E(k) =
2 2 k , 2m
(6.7)
where k is an arbitrary vector in the reciprocal space. k′ is a vector from the Brillouin zone such that k = k′ + G with a suitable reciprocal lattice vector G. Because of (6.5) the dispersion relation can be written also as E(k) =
2 ′ (k + G)2 , 2m
(6.8)
where k′ denotes a vector from the Brillouin zone. Thus, many branches of the dispersion relation arise from using various reciprocal lattice vectors in (6.8). The resulting dispersion relation for the free electron is shown in Fig. 6.2a for a onedimensional system (k′ and G are parallel) and in Fig. 6.2b for the simple cubic lattice (in the socalled reduced zone scheme). In Fig. 6.2c, the (same) dispersion of the free electron is shown for the fcc lattice.
114
6 Band Structure
6.4 Kronig–Penney Model The Kronig–Penney model [13] is a simple, analytically solvable model that visualizes the effect of the periodic potential on the dispersion relation of the electrons, i.e. the formation of a band structure. A onedimensional periodic hardwall potential of ﬁnite height is assumed (Fig. 6.3a). The well width is a, the barrier width b and thus the period P = a + b. The potential is zero in the well (regions (0, a) + nP ) and +U0 in the barrier. The Schr¨ odinger equation −
2 ∂ 2 Ψ + U (x)Ψ (x) = EΨ (x) 2m ∂x2
(6.9)
has to be solved. The solutions for a single hardwall potential well are well known. In the well, they have oscillatory character, i.e. Ψ ∝ exp (±ikx) with real k. In the barrier, they have exponential character, i.e. Ψ ∝ exp (±kx) with real k. Thus we chose Ψ (x) = A exp (iKx) + B exp (−iKx) Ψ (x) = C exp (κx) + D exp (−κx) .
(6.10a) (6.10b)
The wavefunction from (6.10a) is for the well between 0 and a with E = 2 K 2 /2m. The wavefunction from (6.10b) is for the barrier between a and a + b with U0 − E = 2 κ2 /2m. From the periodicity and Bloch’s theorem the wavefunction at x = −b must have the form Ψ (−b) = exp (−ikP )Ψ (a), i.e. between the two wavefunctions is only a phase factor. The wavevector k of the Bloch function (planewave part of the solution) is a new quantity and must be carefully distinguished from K and κ. Both K and κ are real numbers. As boundary conditions, the continuity of Ψ and Ψ ′ are used.2 At x = 0 and x = a this yields A+B = C +D iKA − iKB = κC − κD A exp(iKa) + B exp(−iKa) = C exp(κa) + D exp(−κa)
(6.11a) (6.11b) (6.11c)
iKA exp(iKa)− iKB exp(−iKa) = κCexp(κa) − κDexp(−κa). (6.11d) The continuity of Ψ and Ψ ′ at x = −b is used in the left sides of (6.11c,d). A nontrivial solution arises only if the determinant of the coeﬃcient matrix is zero. This leads (after some tedious algebra) to 2 κ − K2 cos(kP ) = sinh(κb) sin(Ka) + cosh(κb) cos(Ka) . (6.12) 2κK 2 Generally, Ψ ′ /m should be continuous, however, in the present example the mass is assumed constant throughout the structure.
6.4 Kronig–Penney Model
115
(a)
(b)
(c)
(d)
(e)
Fig. 6.3. (a) Onedimensional periodic hardwall potential (Kronig–Penney model). (b) Transcendental function B(K) from (6.13) for β = 5. The dashed lines indicate the [−1, 1] interval for which solutions exist for (6.13). (c) Bandgap between ﬁrst and second subband (in units of EX = (2 /2m)(π/a)2 ) as a function of β. For smaller β the bandgap is ∝ β. For thick barriers (β → ∞) the bandgap saturates towards 3EX as expected for uncoupled wells. (d,e) The resulting energy dispersion (in units of EX ) as a function of the superlattice wavevector k for (d) β = 5 and (e) β = 20 in (6.13). The dashed lines are the freeelectron dispersion (for β = 0) (cf. Fig. 6.2a)
Further simpliﬁcation can be reached by letting the barrier thickness b → 0 and U0 → ∞. Then P → a. The limit, however, is performed in such a way that the barrier ‘strength’ U0 b ∝ κ2 b remains constant and ﬁnite. Equation (6.12) then reads (for κb → 0: sinh(κb) → κb and coth(κb) → 1): cos(ka) = β
sin(Ka) + cos(Ka) = B(K) . Ka
(6.13)
116
6 Band Structure
The coupling strength β = κ2 ba/2 represents the strength of the barrier. Equation (6.13) only has a solution if the right side is in the interval [−1, 1] (Fig. 6.3b). The function sin(x)/x oscillates with decreasing amplitude such that for suﬃciently high values of Ka a solution can always be found. The resulting dispersion is shown in Fig. 6.3c. The dispersion is different from the freeelectron dispersion and has several separated bands. The bandgaps are related to the K values, i.e. energies for which (6.13) cannot be fulﬁlled. At the zone boundary (k = π/a) the bands are split and the tangent is horizontal (dE/dk = 0). The form of the dispersion is similar to the arccos function. For large coupling between the potential wells (small β, β 1) the bandgap E12 between the ﬁrst and the second subband at the Xpoint is E12 = β(4/π 2 )EX with EX = (2 /2m)(π/a)2 . In this case, the width of the subbands is wide. For small coupling (large β) the bandgap E12 converges towards 3EX as expected (Fig. 6.3c) for decoupled potential wells with energy levels En = EX n2 and the width of the bands is small.
6.5 Electrons in a Periodic Potential In this section, we will discuss the solution of a general wave equation for electrons in a periodic potential. The solution is investigated particularly at the zone boundary. The potential U is periodic with the lattice (6.1). It can be represented as a Fourier series with the reciprocal lattice vectors (cf. (3.16)): U (r) =
UG exp (iGr) .
(6.14)
G
∗ Since U is a real function, U−G = UG . The deeper reason for the success of such an approach is that for typical crystal potentials, the Fourier coeﬃcients decrease rapidly with increasing G, e.g. for the unscreened Coulomb potential UG ∝ 1/G2 . The wavefunction is expressed as a Fourier series (or integral) over all allowed (Bloch) wavevectors K,
Ψ (r) =
CK exp (iKr) .
(6.15)
K
The kinetic and potential energy terms in the Schr¨ odinger equation (6.6) are ∇2 Ψ = − UΨ =
K2 CK exp (iKr)
G
(6.16a)
K
UG CK exp [i(G + K)r] .
K
With K′ = K + G, (6.16b) can be rewritten as
(6.16b)
6.5 Electrons in a Periodic Potential
UΨ =
G
K
UG CK −G exp (iK′ r) .
117
(6.17)
Now, the Schr¨ odinger equation can be written as an (inﬁnite) system of algebraic equations: UG CK−G = 0 , (6.18) (λK − E)CK + G
with λK = 2 K2 /(2m). 6.5.1 Approximate Solution at the Zone Boundary We assume that the potential energy has only one important Fourier coeﬃcient U for the shortest reciprocal lattice vector G. Also, we have U−G = UG . Thus, the (onedimensional) potential has the form U (x) = 2U cos(Gx). We consider the solution at the zone boundary, i.e. in the vicinity of K = G/2. The kinetic energy is then the same for K = ±G/2, i.e. λK = λK−G = (2 /2m) (G2 /4). CG/2 is an important coeﬃcient of the wavefunction, thus C−G/2 will also be important. We will now limit the K vectors
for the series of CG/2 (6.15) to just these two. For the coeﬃcient vector the determinant C−G/2 is λ − E U 2 2 (6.19) U λ − E = (λ − E) − U = 0 ,
Fig. 6.4. Periodic potential U (onedimensional cosine, solid line) and the squares of the wavefunctions Ψ+ (dashed line) and Ψ− (dotted line) for the wavevector at the zone boundary, K = G/2 = π/a
118
6 Band Structure
with λ = λK = λ−K = (2 /2m) (G2 /4) for K = G/2. Thus the energy values are 2 G2 ±U . (6.20) E± = λ ± U = 2m 4 At the zone boundary, a splitting of the size E+ − E− = 2U occurs. The center of the energy gap is given by the energy λK of the freeelectron dispersion. The ratio of the coeﬃcients is CG/2 /C−G/2 = ∓1. The ‘−’ solution of (6.20) (lower energy) is a standing cosine wave (Ψ− ), the ‘+’ solution (Ψ+ ) is a standing sine wave as visualized in Fig. 6.4. For the lowerenergy (binding) state the electrons are localized at the potential minima, i.e. at the atoms, for the upper state (antibinding) the electrons are localized between the atoms. Both wavefunctions have the same periodicity since they belong to the same wavevector K = G/2. We note that the periodicity of Ψ is 2a, while the periodicity of Ψ 2 is equal to the lattice constant a. 6.5.2 Solution in the Vicinity of the Zone Boundary In the vicinity of the zone boundary we rewrite (6.19) as λK − E U =0. U λK−G − E
(6.21)
We ﬁnd two solutions
1/2 1 1 2 2 (λK − λK−G ) + U E± = (λK + λK−G ) ± . 2 4
(6.22)
For K in the vicinity of the zone boundary these solutions can be developed. Therefore, we use the (small) distance from the zone boundary ! = K − G/2. With λ = (2 /2m) (G2 /4) we rewrite still exactly (6.22): K 1/2
!2 2 K 2 1 2 ! 2 2 ! G + K ± 4λ +U E± K = . (6.23) 2m 4 2m ! with 2 GK/(2m) ! ≪ U , the energy is then approximately For small K given by
2!2 ! ≈ λ ± U + K 1 ± 2λ . E± K (6.24) 2m U
Thus the energy dispersion in the vicinity of the zone boundary is parabolic. The lower state has a negative curvature, the upper state a positive curvature. The curvature is U 1 ≈ ±m , (6.25) m∗ = m 1 ± 2λ/U 2λ
and will be later related to the effective mass. The approximation in (6.25) is valid for U  ≪ 2λ. We note that in our simple model m∗ increases linearly with increasing bandgap 2U (see Fig. 6.20 for experimental data).
6.6 Band Structure of Selected Semiconductors
119
6.5.3 Kramer’s degeneracy En (k) is the dispersion in a band. The timereversal symmetry (Kramer’s degeneracy) implies En↑ (k) = En↓ (−k) ,
(6.26)
where the arrow refers to the direction of the electron spin. If the crystal is symmetric under inversion, we have additionally En↑ (k) = En↑ (−k) .
(6.27)
With both time reversal and inversion symmetry the band structure fulﬁlls En↑ (k) = En↓ (k) .
(6.28)
6.6 Band Structure of Selected Semiconductors In the following, the band structures of various important and prototype semiconductors are discussed. The band below the fundamental energy gap is called the valence band, the band above it the conduction band. The bandgap ΔEcv , mostly denoted as Eg , is the energy separation between the highest valenceband state and the lowest conductionband state. The maximum of the valence band is for most semiconductors at the Γ point. 6.6.1 Silicon For silicon, an elemental semiconductor, (Fig. 6.5a) the minimum of the conduction band is located close to the X point at 0.85π/a in the 100 direction. Thus, it is not at the same point in kspace as the top of the valence band. Such a band structure is called indirect. Since there are six equivalent 100 directions, there are six equivalent minima of the conduction band. 6.6.2 Germanium Germanium, another elemental semiconductor, (Fig. 6.5b) also has an indirect band structure. The conduction minima are at the L point in the 111 direction. Due to symmetry there are eight equivalent conductionband minima. 6.6.3 GaAs GaAs (Fig. 6.6a) is a compound semiconductor with a direct bandgap since the top of the valence band and the bottom of the conduction band are at the same position in kspace (at the Γ point). The next highest (local) minimum in the conduction band is close to the L point.
120
6 Band Structure
(a)
(b)
Fig. 6.5. Band structure of (a) silicon (indirect) and (b) germanium (indirect). In Si, the minima of the conduction band are in the 100 direction, for germanium in the 111 direction. From [93], based on [138]
(a)
(b)
Fig. 6.6. Band structure of (a) GaAs (direct) and (b) GaP (indirect). For GaAs the minimum of the conduction band is at Γ , for GaP in the 100 direction. From [93], based on [138]
6.6.4 GaP GaP (Fig. 6.6b) is an indirect compound semiconductor. The conductionband minima are along the 100 directions. 6.6.5 GaN GaN (Fig. 6.7) is a direct semiconductor that has wurtzite structure but can also occur in the metastable cubic (zincblende) phase.
6.6 Band Structure of Selected Semiconductors
X
Energy (eV)
15
W
15
GaN
10
10
5
5
0
0
5
5
10 A
121
zb L M
A
H K
w
A
L M
A
H K
Fig. 6.7. Band structure of GaN (direct) in zincblende modiﬁcation (left) and wurtzite modiﬁcation (right), both displayed in the wurtzite Brillouin zone to facilitate comparison
6.6.6 Lead Salts The band structures of PbS, PbSe and PbTe are shown in Fig. 6.8.
(a)
(b)
(c)
Fig. 6.8. Calculated band structures of (a) PbS, (b) PbSe and (c) PbTe. From [139]
The bandgap is located at the L point. The lead chalcogenide system shows the anomaly that with increasing atomic weight the bandgap does not decrease monotonically. At 300 K, the bandgaps are 0.41, 0.27 and 0.31 eV for PbS, PbSe and PbTe, respectively.
122
6 Band Structure
6.6.7 Chalcopyrites The experimental bandgaps of a number of chalcopyrite semiconductors are listed in Table 6.1. The band structures of CuAlS2 , CuAlSe2 , and CuGaSe2 are compared in Fig. 6.9. CuAlS2
T
N
CuGaSe2
CuAlSe2
T
N
T
N
Fig. 6.9. Calculated band structures of CuAlS2 , CuAlSe2 , and CuGaSe2 . Absolute values of gaps are incorrect due to LDA. Adapted from [140], reprinted with c permission, 1983 APS
Table 6.1. Bandgaps of various chalcopyrite semiconductors Eg (eV) CuAlS2 CuAlSe2 CuAlTe2 AgAlS2 AgAlSe2 AgAlTe2 ZnSiP2 ZnSiAs2 CdSiP2 CdSiAs2
3.5 2.71 2.06 3.13 2.55 2.2 2.96 2.12 2.45 1.55
Eg (eV) CuGaS2 CuGaSe2 CuGaTe2 AgGaS2 AgGaSe2 AgGaTe2 ZnGeP2 ZnGeAs2 CdGeP2 CdGeAs2
2.5 1.7 1.23 2.55 1.83 1.11.3 2.34 1.15 1.72 0.57
Eg (eV) CuInS2 CuInSe2 CuInTe2 AgInS2 AgInSe2 AgInTe2 ZnSnP2 ZnSnAs2 CdSnP2 CdSnAs2
1.53 1.0 1.01.15 1.87 1.24 1.0 1.66 0.73 1.17 0.26
6.6 Band Structure of Selected Semiconductors
123
In Fig. 6.10, the theoretical band structure of GaN and its closest related chalcopyrite ZnGeN2 are compared, both shown in the chalcopyrite (orthorhombic) Brillouin zone. The bandgap of ZnGeN2 is smaller than that of GaN and the difference of 0.4 eV is fairly well reproduced by the calculation3 (giving 0.5 eV). ZnGeN2
GaN
15
Energy (eV)
10 5 0 5
10 15 X
Z
U
R
S
Y
X
Z
U
R
S
Y
Fig. 6.10. Calculated (within LDA) band structures of ZnGeN2 and its related III– V compound GaN, both displayed in the chalcopyrite (orthorhombic) Brillouin zone c to facilitate comparison. Adapted from [141], reprinted with permission, 1999 MRS
6.6.8 Delafossites In Fig. 6.11, the theoretical band structures of the delafossites CuAlO2 , CuGaO2 , and CuInO2 are shown. The maximum of the valence band is not at Γ but near the F point. The direct bandgap at Γ decreases for the sequence Al → Ga → In, similar to the trend for AlAs, GaAs and InAs. The direct bandgap at F and L, causing the optical absorption edge, increases, however (experimental values are 3.5, 3.6, and 3.9 eV). 6.6.9 Perovskites The calculated band structure of BaTiO3 in the tetragonal phase is shown in Fig. 6.12. The minimum of the conduction band is at the Γ point. The maximum of the valence band is not at the Γ point but at the M point. The bandgap of the LDA calculation is too small (2.2 eV) compared to the experimental value ∼ 3.2 eV. 3 Due to the local density approximation (LDA) the absolute values of the bandgaps are too small by about 1 eV.
124
6 Band Structure CuAlO2
CuGaO2
CuInO2
Energy (eV)
6 4 2 0 2
Fig. 6.11. Band structures of CuAlO2 , CuGaO2 , and CuInO2 , calculated with LDA (underestimating the absolute value of the bandgaps). The arrows denote the maximum of the valence band that has been set to zero energy for each material. c Adapted from [59], reprinted with permission, 2002 APS
Fig. 6.12. Calculated energy band structure of BaTiO3 along the major symmetry directions. The Fermi level (EF ) is set at zero energy. Reprinted with permission c from [142], 2001 AIP
6.7 Alloy Semiconductors In alloy semiconductors, the size of the bandgap and the character of the bandgap will depend on the composition. The dependence of the bandgap on the ternary composition is mostly nonlinear and can usually be expressed with a bowing parameter b that is mostly positive. For a compound Ax B1−x C the bandgap is written as Eg (Ax B1−x C) = Eg (BC) + x [Eg (AC) − Eg (BC)] − bx(1 − x) .
(6.29)
6.9 Systematics of Semiconductor Bandgaps
125
Even on the virtual crystal approximation (VCA) level (Sect. 3.7.3) a nonzero bowing parameter b is predicted. However, a more thorough analysis shows that the bowing cannot be treated adequately within VCA and is due to the combined effects of volume deformation of the band structure with the alloy lattice constant, charge exchange in the alloy with respect to the binary end components, a structural contribution due to the relaxation of the cation– anion bond lengths in the alloy and a small contribution due to disorder [143]. The Six Ge1−x alloy has diamond structure for all concentrations and the position of the conductionband minimum in kspace switches from L to X at about x = 0.15 (Fig. 6.13a). However, for all concentrations the band structure is indirect. The Inx Ga1−x As alloy has zincblende structure for all compositions. The bandgap is direct and decreases with a bowing parameter of b = 0.6 eV [144] (Fig. 6.13b). This means that for x = 0.5 the bandgap is 0.15 eV smaller than expected from a linear interpolation between GaAs and InAs, as reported by various authors [145]. If one binary end component has a direct band structure and the other is indirect, a transition occurs from direct to indirect at a certain composition. An example is Alx Ga1−x As where GaAs is direct and AlAs is indirect. For all concentrations the crystal has zincblende structure. In Fig. 6.13c, the Γ , L and X conductionband minima for ternary Alx Ga1−x As are shown. Up to an aluminum concentration of x = 0.4 the band structure is direct. Above this value the band structure is indirect with the conductionband minimum being at the X point. The particularity of Alx Ga1−x As is that the lattice constant is almost independent of x. For other alloys lattice match to GaAs or InP substrates is only obtained for speciﬁc compositions, as shown in Fig. 6.14. If the two binary end components have different crystal structure, a phase transition occurs at a certain composition (range). An example is Mgx Zn1−x O, where ZnO has wurtzite structure and MgO has rocksalt structure. The bandgap is shown in Fig. 6.13d. In this case, each phase has its own bowing parameter. A discontinuity arises when the crystal changes from fourfold to sixfold coordination.
6.8 Amorphous Semiconductors In a perfectly crystalline semiconductor the eigenenergies of the states in the bands are real. An amorphous semiconductor can be modelled using a spectrum of complex energies [150]. In Fig. 6.15 the band structure of crystalline silicon is shown next to that calculated for amorphous silicon with α = 0.05.
6.9 Systematics of Semiconductor Bandgaps The trends with regard to the size of the bandgap for elemental, III–V and II–VI semiconductors can essentially be understood in terms of the bond
126
6 Band Structure 1.1
1.5
InxGa1xAs
SixGe1x 1.3 1.1
L
0.9
Eg (eV)
Eg (eV)
1.0
X 0.8
0.9 0.7
0.7
0.5
0.6 0.0
0.2
0.4
x
0.6
0.8
1.0
(a)
0.3 0.0
0.2
0.4
x
0.6
0.8
1.0
(b)
2.6 AlxGa1xAs
1
2.4
L1
Eg (eV)
2.2 2.0
X1 Edd
1.8 1.6 1.4 0.0
0.2
0.4
0.6
0.8
1.0
x
(c)
(d)
Fig. 6.13. (a) Bandgap of Six Ge1−x alloy (T = 296 K) with a change from the conductionband minimum at L (Gerich) to X. Adapted from [146]. (b) Bandgap (at room temperature) of Inx Ga1−x As. The solid line is an interpolation with bowing (b = 0.6 eV) and the dashed line is the linear interpolation. Data from [144]. (c) Bandgap (at room temperature) in the ternary system Alx Ga1−x As. For x < 0.4 the alloy is a direct, for x > 0.4 an indirect, semiconductor. Edd denotes the energy position of a deep donor (see Sect. 7.7.4). Adapted from [147]. (d) Bandgap (at room temperature) in the ternary system Mgx Zn1−x O. Data (from spectroscopic ellipsometry [148, 149]) are for hexagonal wurtzite phase (circles), and Mgrich cubic rocksalt phase (squares). Dashed lines are ﬁts to data with a bowing parameter for each phase
6.9 Systematics of Semiconductor Bandgaps
(a)
127
(b)
Fig. 6.14. Bandgap vs. lattice constant for (a) Gax In1−x P and Alx In1−x P (lattice matched to GaAs) as well as for (b) Inx Al1−x As and Inx Ga1−x As alloys (lattice matched to InP)
Fig. 6.15. (a) Calculated band structure of crystalline silicon. (b) Calculated band structure of amorphous silicon with α = 0.05 (cf. (3.6)). The solid lines denote the real part of the energy, the shaded areas denote the regions with a width of twice the imaginary part of the energies centered around the real part. Adapted from [151]
strength and ionicity. In Fig. 6.16, the bandgaps of many important semiconductors are shown as a function of the lattice constant. For elemental semiconductors, the bandgap decreases with reduced bond strength, i.e. lattice constant (C→Si→Ge). A similar trend exists both for the III–V and the II–VI semiconductors. For the same lattice constant, the bandgap increases with increasing ionicity, i.e. IV–IV→III–V→II–VI. The best example is the sequence Ge→ GaAs→ZnSe for which all materials have almost the same lattice constant. This behavior can be understood within the framework of a modiﬁed Kronig–Penney model [152] (Sect. 6.4). Double potential wells (b/a = 3) are chosen to mimic the diatomic planes along the 111 direction in the zincblende structure (Fig. 6.17a). Symmetric wells (depth P0 ) are chosen to model covalent semiconductors and asymmetric wells with depths P0 ± ΔP
128
6 Band Structure
Fig. 6.16. Bandgaps as a function of the lattice constant for various IV–IV, III–V and II–VI semiconductors. (lattice constant of wurtzite semiconductors has been recalculated for a cubic cell)
60 50 40
2md2 E/h2
30 20 10 0 10
Eg
20 30 40 50
(c)
0
0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5 P
Fig. 6.17. Kronig–Penney model (along 111, b/a = 3) for a (a) IV–IV semiconductor and (b) for a III–V (or II–VI) semiconductor, (c) resulting band structure (P0 = −3). d is the lattice constant (b + a). Adapted from [152]
6.10 Temperature Dependence of the Bandgap
129
to model partially ionic semiconductors. Results are shown in Fig. 6.17a for P0 = −3. With increasing asymmetry, i.e. ionicity, the bandgap increases, mostly due to a downward shift of the valence band. The case of III–V (II– VI) semiconductors is reached for ΔP ≈ 2 (4).
6.10 Temperature Dependence of the Bandgap The bandgap typically decreases with increasing temperature (see Fig. 6.18 for Si and ZnO). The reasons for this are the change of electron–phonon interaction and the expansion of the lattice. The temperature coeﬃcient may be written as
∂Eg ∂Eg α ∂Eg − , (6.30) = ∂T V β ∂p T ∂T p where α is the volume coeﬃcient of thermal expansion and β is the volume compressibility. An anomaly is present for the lead salts (PbS, PbSe, PbTe) for which the temperature coeﬃcient is positive (Fig. 6.19a). Theoretical calculations [153] show that both terms in (6.30) are positive for the lead − salts. The L+ 6 and L6 levels (see Fig. 6.8) shift as a function of temperature in such a way that their separation increases (Fig. 6.19b). 0
Si
Eg (meV)
50
100
150
200
(a)
0
100 200 300 400 500 600 700 800 Temperature (K)
(b)
Fig. 6.18. Temperature dependence of the bandgap of (a) Si (data from [154]) and (b) ZnO (experimental data from photoluminescence (triangles) and ellipsometry (circles)). The solid lines are ﬁts with (6.33) and the parameters given in Table 6.2
For many semiconductors the temperature dependence can be described with the empirical, threeparameter Varshni formula [155], Eg (T ) = Eg (0) −
αT 2 , T +β
(6.31)
130
6 Band Structure 0.35 0.34
8.0
PbS
PbTe 7.5
Energy (eV)
Eg (eV)
0.33 0.32 0.31 0.30
L6
7.0 L+6 6.5
0.29 0.28 0
(a)
50 100 Temperature (K)
6.0 0
150
100 200 Temperature (K)
(b)
300
Fig. 6.19. (a) Bandgap vs. temperature for PbS. (b) Theoretical position of L+ 6 and L− 6 as a function of temperature for PbTe. Adapted from [139]
where Eg (0) is the bandgap at zero temperature. A more precise and physically motivated formula (based on a Bose–Einstein phonon model) has been given in [156]
ΘB −1 , (6.32) Eg (T ) = Eg (0) − 2αB ΘB coth 2T where αB is a coupling constant and kΘB is a typical phonon energy; typical values are given in Table 6.2. This model reaches a better description of the fairly ﬂat dependence at low temperatures. However, experimentally the dependence at low temperatures is rather quadratic. Table 6.2. Parameters for the temperature dependence of the bandgap (6.32) and (6.33) for various semiconductors
Si Ge GaAs InP InAs ZnSe ZnO
α (10−4 eV/K)
Θ (K)
Δ
αB (10−4 eV/K)
ΘB (K)
3.23 4.13 4.77 3.96 2.82 5.00 3.8
446 253 252 274 147 218 659
0.51 0.49 0.43 0.48 0.68 0.36 0.54
2.82
351
5.12
313
The more elaborate model of [157] takes into account a more variable phonon dispersion, including optical phonons, and proposes the four
6.11 Equation of Electron Motion
131
parameter formula 3Δ2 1 − 3Δ2 6 + 1+β−1 exp (2/γ) − 1 2 2 2 π 3Δ − 1 3 8 4 γ2 + γ + γ + γ6 β= 3(1 + Δ2 ) 4 3 γ = 2T /Θ ,
Eg (T ) = Eg (0) − αΘ
(6.33)
where α is the hightemperature limiting magnitude of the slope (of the order of several 10−4 eV/K), Θ is an effective average phonon temperature and Δ is related to the phonon dispersion (typically between zero (Bose–Einstein model) and 3/4).
6.11 Equation of Electron Motion The equation of motion for the electron in the band structure is no longer given by Netwon’s law F = d(mv)/dt as in vacuum. Instead, the propagation of quantummechanical electron wave packets has to be considered. Their group velocity is given by vg =
1 dE dω = . dk dk
(6.34)
Through the dispersion relation the inﬂuence of the crystal and its periodic potential on the motion enters the equation. An electric ﬁeld E acts on an electron during the time δt the work δE = −eEvg δt. This change in energy is related to a change in k via δE = dE/dkδk = vg δk. Thus, we arrive at dk/dt = −eE. For an external force we thus have
dk = −eE = F . dt
(6.35)
Thus, the crystal momentum p = k takes the role of the momentum. A more rigorous derivation can be found in [137]. In the presence of a magnetic ﬁeld B the equation of motion is:
e dk = −ev × B = − ∇k E × B . dt
(6.36)
The motion in a magnetic ﬁeld is thus perpendicular to the gradient of the energy, i.e. the energy of the electron does not change. It oscillates therefore on a surface of constant energy perpendicular to B.
132
6 Band Structure
6.12 Electron Mass 6.12.1 Effective Mass From the freeelectron dispersion E = 2 k 2 /(2m) the mass of the particle is inversely proportional to the curvature of the dispersion relation, i.e. 1/m = (d2 E/dk 2 )/2 . This relation will now be generalized for arbitrary dispersion relations. The tensor of the effective mass is deﬁned as (m∗−1 )ij =
1 ∂2E . 2 ∂ki ∂kj
(6.37)
The equation F = m∗ v˙ must be understood as a tensor equation, i.e. for the components of the force Fi = m∗ij aj . Force and acceleration must no longer be collinear. In order to ﬁnd the acceleration from the force, the inverse of the effectivemass tensor must be used, a = (m∗ )−1 F. In (6.25) the ratio of the effective mass and the freeelectron mass is of the order of m∗ /m ≈ U/λ, the ratio of the free particle energy and the bandgap. For typical semiconductors, the width of the (valence) band is of the order of 20 eV, and the gap is about 0.2–2 eV. Thus, the effective mass is expected to be 10–100 times smaller than the freeelectron mass. Additionally, the relation m∗ ∝ Eg is roughly fulﬁlled (Fig. 6.20).
Fig. 6.20. Eﬀective mass (in units of the freeelectron mass m0 ) as a function of the (lowtemperature) bandgap for several semiconductors. The dashed line fulﬁlls m∗/m0 = Eg /20 eV
From socalled k · p theory [158] (see Appendix E) the effective electron mass is predicted to be related to the momentum matrix element pcv pcv = cpv ,
(6.38)
6.12 Electron Mass
133
with the Bloch functions c and v of the conduction and valence band, respectively, given as c = uc,kc (r) exp (ikc r) v = uv,kv (r) exp (ikv r) .
(6.39a) (6.39b)
Typically, the kdependence of the matrix element is small and neglected. The momentum matrix element will also be important for optical transitions between the valence and conduction bands (Sect. 9.3). Other related quantities that are often used are the energy parameter EP 2
EP =
2 pcv  , m0
(6.40)
and the bulk momentum matrix element Mb2 that is given by Mb2 =
m0 1 2 EP . pcv  = 3 6
(6.41)
The electron mass is given by4
EP 1 2 m0 = 1 + + m∗e 3 Eg Eg + Δ 0 Eg + 2Δ0 /3 EP EP ≈1+ ≈ . = 1 + EP Eg (Eg + Δ0 ) Eg + Δ0 /3 Eg
(6.42)
Comparison with the ﬁt from Fig. 6.20 yields that EP is similar for all semiconductors [159] and of the order of 20 eV (InAs: 22.2 eV, GaAs: 25.7 eV, InP: 20.4 eV, ZnSe: 23 eV, CdS: 21 eV). In silicon there are six conductionband minima. The surfaces of equal energy are schematically shown in Fig. 6.21c. The ellipsoids are extended along the 100 direction because the longitudinal mass (along the Δ path) is larger than the transverse mass in the two perpendicular directions. For example, the dispersion relation around the [100] minimum is then given as (kx0 denotes the position of the conductionband minimum) E(k) = 2
"
ky2 + kz2 (kx − kx0 )2 + 2ml 2mt
#
.
(6.43)
For germanium surfaces of constant energy around the eight conductionband minima in the 111 directions are depicted in Fig. 6.21d. The longitudinal and the transverse masses are again different. For GaAs, the conductionband dispersion around the Γ point is isotropic, thus the surface of constant energy is simply a sphere (Fig. 6.21a). In wurtzite semiconductors the conductionband minimum is typically at the Γ point. However, the mass
134
6 Band Structure
(b)
(a)
(c)
(d)
Fig. 6.21. Ellipsoids of constant energy in the vicinity of the conductionband minima for (a) GaAs with isotropic minimum at Γ point, (b) ZnO with anisotropic minimum at Γ point (anisotropy exaggerated), (c) silicon with six equivalent anisotropic minima (ml /mt = 5 not to scale) along 100 and (d) germanium with eight equivalent anisotropic minima along 111. The cube indicates the 100 directions for the cubic materials. For the wurtzite material (part (b)) the vertical direction is along [00.1]
along the caxis is slightly different from the inplane mass (ml /mt = 1.08 for ZnO), see Fig. 6.21b. The directional dependence of the mass can be measured with cyclotron resonance experiments with varying direction of the magnetic ﬁeld. In Fig. 6.22, the ﬁeld B is in the (110) plane with different azimuthal directions. When the (static) magnetic ﬁeld makes an angle θ with the longitudinal axis of the energy surface, the effective mass is given as [160]
4
1 m∗
2
=
sin2 θ cos2 θ + . m2t mt ml
Δ0 is the spinorbit splitting discussed in Sect. 6.13.2.
(6.44)
6.12 Electron Mass [110]
[001]
0.44
0.40
0.40
0.36
0.36
0.32
0.32
0.28 0.24 0.20 0.16 0.12
0.20 0.16 0.12
0.04
0.04
30 60 Angle (deg)
0
90 (b)
[110]
0.24
0.08
0
[111]
0.28
0.08
0 (a)
[111]
Effective mass m*/m0
Effective mass m*/m0
[001]
0.44
135
0
30 60 Angle (deg)
90
Fig. 6.22. Cyclotron mass (at T = 4 K) in (a) Si and (b) Ge for the magnetic ﬁeld in the (110) plane and various azimuthal directions θ. Experimental data and ﬁts (solid lines) using (6.44) with (a) ml = 0.98, mt = 0.19 and (b) ml = 1.58, mt = 0.082. Data from [161].
6.12.2 Polaron Mass In an ionic lattice, the electron polarizes the ions and causes a change of their equilibrium position. When the electron moves, it must drag this ion displacement with it. This process it called the polaronic effect and requires additional energy. It leads to an increase of the electron mass to the ‘polaron mass’ mp ,5 (6.45) mp = m∗ 1 + α/6 + 0.025α2 , with m∗ being the band mass as deﬁned in Sect. 6.12.1 and α the Fr¨ ohlich coupling constant6 5
For the calculation, manyparticle theory and techniques are needed; the best solution is still given by Feynman’s calculation [162, 163]. 6 This constant is part of the matrix element in the Hamiltonian of the electron– phonon interaction and is related to the electric ﬁeld created by LO phonons, as given in (5.45).
136
6 Band Structure
α=
e2
m∗ 2ωLO
1/2
1 1 − ǫ(∞) ǫ(0)
.
(6.46)
Often, the polaron mass is given as mp = m∗ /(1 − α/6). Polarons in semiconductors are typically ‘large’ or Fr¨ ohlichtype polarons, i.e. the dressing with phonons (as the ion displacement is called in a quantummechanical picture) is a perturbative effect and the number of phonons per electron (≈ α/2) is small. If α becomes large (α > 1, α ∼ 6), as is the case for strongly ionic crystals such as alkali halides, the polaron becomes localized (selftrapped) by the electron–phonon interaction7 and hopping occurs infrequently from site to site. 6.12.3 Nonparabolicity of Electron Mass The dispersion around the conductionband minimum is only parabolic for small k. The further away the wavevector is from the extremum, the more the actual dispersion deviates from the ideal parabola (see, e.g., Fig. 6.6). This effect is termed nonparabolicity. Typically, the energy increases less quickly with k than in the parabolic model. This can be described in a socalled twolevel model with the dispersion relation
2 k 2 E =E 1+ ∗ , 2m∗0 E0
(6.47)
where E0∗ > 0 parameterizes the amount of nonparabolicity (a parabolic band corresponds to E0∗ = ∞). The nonparabolic dispersion for GaAs is shown in Fig. 6.23a. The curvature is reduced for larger k and thus the effective mass is energy dependent and increases with the energy. Equation (6.47) leads to the energydependent effective mass
2E (6.48) m∗ (E) = m∗0 1 + ∗ , E0 where m∗0 denotes here the effective mass at k = 0. Theory and experimental data for the effective electron mass of GaAs are shown in Fig. 6.23b.
6.13 Holes 6.13.1 Hole Concept Holes are missing electrons in an otherwise ﬁlled band. This concept is useful to describe the properties of charge carriers at the top of the valence band. The hole is a new quasiparticle whose dispersion relation is schematically
6.13 Holes N (1018 cm3) 5 10
0.1 1
20 [001] [111]
GaAs 0.3
0.1
(a)
EF (meV) 50
10
100
200
GaAs
0.2
0
5
0.12
m*/m0
E (eV)
0.14
137
0
0.10
0.08
1
2
3 4 5 6 k2 (1013 cm2)
7
0.06 16 10
8
10
(b)
17
10 N (cm3)
18
10
19
Fig. 6.23. (a) Dispersion relations for the conduction band of GaAs. The solid line is parabolic dispersion (constant eﬀective mass). The dashed (dashdotted) line denotes the dispersion for k along [001] ([111]) from a ﬁvelevel k · p model (5LM). (b) Cyclotron resonance eﬀective mass of electrons in GaAs as a function of the Fermi level (upper abscissa) and the corresponding electron concentration (lower abscissa). The dashed line is from a 2LM according to (6.48) with E0∗ = 1.52 eV. The solid lines are for a 5LM for the three principal directions of the magnetic ﬁeld. The symbols represent experimental data from diﬀerent sources. Data from [164]
E
ke kh
k
Fig. 6.24. Hole dispersion (dashed line) in relation to the electron dispersion in the valence band (solid line)
shown in Fig. 6.24 in relation to the dispersion of electrons in the valence band. The wavevector of the hole (ﬁlled circle in Fig. 6.24) is related to that of the ‘missing’ electron (empty circle in Fig. 6.24) by kh = −ke . The energy is Eh (kh ) = −Ee (ke ), assuming that EV = 0, otherwise Eh (kh ) = −Ee (ke ) + 2EV . The hole energy is larger for holes that are further away from the top of 7 One can think about it in the way that the electron strongly polarizes the lattice and digs itself a potential hole out of which it can no longer move.
138
6 Band Structure
the valence band, i.e. the lower the energy state of the missing electron. The velocity of the hole, vh = −1 ∇kh Eh , is the same, vh = ve , and the charge is positive, +e. The effective mass of the hole is positive at the top of the valence band, m∗h = −m∗e . Therefore, the drift velocities of an electron and hole are opposite to each other. The resulting current, however, is the same. 6.13.2 Hole Dispersion Relation The valence band at the Γ point is 3fold degenerate. The band developed from the atomic (bonding) p states; the coupling of the spin s = 1/2 electrons with the orbital angular momentum l = 1 leads to a total angular momentum j = 1/2 and j = 3/2. The latter states are degenerate at Γ in zincblende bulk material and are called heavy holes (hh) for mj = ±3/2 and light holes (lh) for mj = ±1/2 due to their different dispersion (Fig. 6.25a). The two (mj = ±1/2) states of the j = 1/2 state are splitoff from these states by an energy Δ0 due to spinorbit interaction and are called splitoff (so) holes. E
electrons
EC=EV+Eg
EV
k
EV
(a)
light holes
heavy holes
splitoff holes
(b)
Fig. 6.25. (a) Simpliﬁed band structure with conduction band and three valence bands and (b) threedimensional visualization (E vs. (kx , ky )) of the valence bands of Ge (including warping). Part (b) from [165]
All holes have different mass. In the vicinity of the Γ point the dispersion for heavy and light holes can be described with (+:hh, −:lh) E(k) = Ak 2 ± B 2 k 4 + C 2 kx2 ky2 + ky2 kz2 + kx2 kz2
1/2
.
(6.49)
6.13 Holes
139
2
0 10 20 30 40
4 0
2
4
0 2
2 2
0 2
4
4 4
(a)
(b)
4
2
0
2
4
4
2
0
2
4
2
0 100 200 300 400 4
4 0
2 0
2
2 2
0 2
(c)
4
4
4
(d)
Fig. 6.26. Dispersion in the (kx , ky ) plane at the valence band edge of GaAs. (a,b): hh, (c,d): lh. Dispersion as (a,c): 3D plot and (b,d) as isolines
For heavy and light holes there is a dependence of the dispersion, i.e. the mass, in the (001) plane. This effect, sketched in Fig. 6.25b, is called warping. The warping at the GaAs valenceband edge is shown in Fig. 6.26. The so holes have the dispersion E(k) = −Δ0 + Ak 2 .
(6.50)
Values for A, B, C 2 and Δ0 for a number of semiconductors are given in Table 6.3. The valenceband structure is often described with the Luttinger parameters γ1 , γ2 , and γ3 that can be represented through A, B, and C via Table 6.3. Valenceband parameters (for (6.49)) A and B in units of (2 /2m0 ), C 2 in units of (2 /2m0 )2 , and Δ0 in eV. From [93, 166] Material
A
B
C2
Δ0
Si Ge GaAs InP InAs ZnSe
−4.28 −13.38 −6.9 −5.15 −20.4 −2.75
−0.68 −8.5 −4.4 −1.9 −16.6 −1.0
24 173 43 21 167 7.5
0.044 0.295 0.341 0.11 0.38 0.43
140
6 Band Structure
2 γ1 = A 2m0 B 2 γ2 = − 2m0 2 2 B 2 + C 2 /3 . γ3 = 2m0 2
(6.51a) (6.51b) (6.51c)
The mass of holes in various directions can be derived from (6.49). The mass along the [001] direction, i.e. 2 / ∂ 2 E(k)/∂kx2 for ky = 0 and kz = 0, is 1 2 = 2 (A + B) 100 mhh 1 2 = 2 (A − B) . 100 mlh
In [110] and [111] directions the masses are " 1 # 1 C2 2 2 = 2 A+B 1+ m110 4B 2 hh " 1 # 1 C2 2 2 = 2 A−B 1+ m110 4B 2 lh 1 # C2 2 A+B 1+ 3B 2 " 1 # C2 2 2 . = 2 A−B 1+ 3B 2
1 2 = 2 111 mhh 1 m111 lh
"
(6.52a) (6.52b)
(6.53a) (6.53b)
(6.54a) (6.54b)
For C 2 = 0 the hole bands are isotropic, as is obvious from (6.49). In this case γ2 = γ3 , the socalled spherical approximation. The average of the hole masses over all directions is
1 2C 2 2 = A + B 1 + (6.55a) mav 2 15B 2 hh
1 2 2C 2 = 2 A−B 1+ . (6.55b) mav 15B 2 lh 6.13.3 ValenceBand Fine Structure In Fig. 6.27, the schematic structure of the band edges for zincblende structure semiconductors is shown. The so holes in the zincblende structure are splitoff due to the spinorbit interaction Δso , the Γ8 band is degenerate
6.13 Holes
141
Fig. 6.27. Schematic band structure of zincblende and the valenceband splitting due to spinorbit interaction Δso and crystal ﬁeld splitting Δcf for chalcopyrites (typically Δcf < 0, see Fig. 6.28) and wurtzites. For the wurtzites the situation is schematically shown for CdS (Δso =67 meV, Δcf =27 meV) (or GaN) and ZnO (Δso = −8.7 meV, Δcf =41 meV)
(heavy and light holes). Degeneracies for the holes are removed in the wurtzite and chalcopyrite structures by the additional crystal ﬁeld splitting Δcf due to the anisotropy between the a and caxes. Typically, e.g. for CdS, the topmost valence band in the wurtzite structure has Γ9 symmetry (allowed optical transitions only for E ⊥ c); an exception is ZnO for which the two upper bands are believed to be reversed. In the chalcopyrite structure optical transitions involving the Γ6 band are only allowed for E ⊥ c. The three hole bands are usually labeled A, B, and C from the top of the valence band. The energy positions of the three bands (with respect to the position of the Γ15 band) in the presence of spinorbit interaction and crystal ﬁeld splitting are given within the quasicubic approximation [167] by Δso + Δcf 2
1/2
2 Δso + Δcf 2 . − Δso Δcf =± 2 3
E1 = E2,3
(6.56a) (6.56b)
In chalcopyrites the crystal ﬁeld splitting is typically negative (Fig. 6.28). It is approximately linearly related to 1 − η (for η = c/2a see Sect. 3.4.6). In certain compounds the bandgap can shrink to zero and even become negative in the sense that the Γ6 symmetry (conduction) band is below the valenceband edge (Fig. 6.29).
142
6 Band Structure 0.3 AgGaS2 AgGaSe2
cf (eV)
0.2 AgInS2 CuAlS2
0.1
CuGaS2 CuGaSe2
AgGaTe2 AgAlTe2
AgInSe2
AgInS2(w)
0
CuInS2 CuInSe2
0.0
0.1 2 c/a
0.2
Fig. 6.28. Crystal ﬁeld splitting Δcf for various chalcopyrite compounds vs. the tetragonal distortion 2 − c/a = 2(1 − η). Dashed line represents Δcf = 1.5b(2 − c/a) for b = 1 eV. Data from [168] positive gap
zero gap
6 0>0
6
8 0 0 is the valenceband hydrostatic deformation potential. Therefore the bandgap increases by ΔEg = aTr(ǫ) = a (ǫxx + ǫyy + ǫzz ) ,
(6.59)
with a = ac − av . Biaxial and shear strains affect the valence bands and lead to shifts and splitting of the heavy and light holes at the Γ point: 1/2 Ev,hh/lh = Ev0 ± Eǫǫ $ % 2 2 2 2 Eǫǫ = b2 /2 (ǫxx − ǫyy ) + (ǫyy − ǫzz ) + (ǫxx − ǫzz ) +d2 ǫ2xy + ǫ2yz + ǫ2xz ,
(6.60a)
where Ev0 denotes the bulk valenceband edge. b and d are the optical deformation potentials. For compressive strain the heavyhole band is above the lighthole band. For tensile strain there is strong mixing of the bands (Fig. 6.30). In Table 6.4 the deformation potentials for some III–V semiconductors are listed. Typical values are in the eV regime. In a wurtzite crystal, ﬁve deformation potentials are needed that are termed a and D1 – D4 [173, 174]. In Si and Ge four deformation potentials are needed that are termed a, b, d, Ξu and Ξd [175]. The energy position of the ith conductionband edge (with unit vector ai pointing to the valley, e.g. [111]) is 0 + Ξd Tr(ǫ) + Ξu ai ǫai , EC,i = EC,i
(6.61)
0 denotes the energy of the unstrained conductionband edge. where EC,i
144
6 Band Structure E
E
E
electrons
k
k
k
mj=3/2 mj=1/2
mj=1/2 mj=3/2
mj=3/2 mj=1/2
unstrained
compressive
tensile
Fig. 6.30. Schematic band structure of GaAs in unstrained state (center ) and under compressive and tensile biaxial strain as labeled. Dashed lines indicate shift of band edges due to hydrostatic part of strain Table 6.4. Deformation potentials (in eV) for some III–V semiconductors material
a
b
d
GaAs InAs
−9.8 −6.0
−1.7 −1.8
−4.6 −3.6
6.14.2 Strain Effect on Effective Masses In the presence of strain the band edges are shifted (see Sect. 6.14). Since the electron mass is related to the bandgap, it is expected that the mass will also be effected. In the presence of hydrostatic strain ǫH the electron mass is [176] (cf. to (6.42) for ǫH → 0)
EP m0 3a 2 + 1 − ǫ , (6.62) = 1 + H m∗e Eg + Δ0 /3 Eg + Δ0 /3 with a being the hydrostatic deformation potential and ǫH = Tr(ǫ). In [176], formulas are also given for biaxial and shear strain and also for hole masses.
6.15 Density of States 6.15.1 General Band Structure The dispersion relation yields how the energy of a (quasi) particle depends on the k vector. Now we want to know how many states are at a given energy. This quantity is called the density of states (DOS) and is written as D(E). It
6.15 Density of States
145
is deﬁned in an inﬁnitesimal sense such that the number of states between E and E + δE is D(E)δE. In the vicinity of the extrema of the band structure many states are at the same energy such that the density of states is high. The dispersion relation of a band will be given as E = E(k). If several bands overlap, the densities of state of all bands need to be summed up. The ˜ for the given band is density of states at the energy E ˜ D E dE = 2
d3 k ˜ − E(k)) , δ(E (2π/L)3
(6.63)
where (2π/L)3 is the kspace volume for one state. The factor 2 is for spin degeneracy. The integral runs over the entire kspace and selects only those ˜ The volume integral can be converted to a surface instates that are at E. ˜ with E(k) = E. ˜ The volume element tegral over the isoenergy surface S(E) ˜ and prod3 k is written as d2 Sdk⊥ . The vector k⊥ is perpendicular to S(E) portional to ∇k E(k), i.e. dE = ∇k E(k)dk⊥ . ˜ D E =2
˜ S(E)
1 d2 S . (2π/L)3 ∇k E(k)
(6.64)
In this equation, the dispersion relation is explicitly contained. At band extrema the gradient diverges, however, in three dimensions the singularities are integrable and the density of states takes a ﬁnite value. The corresponding peak is named a vanHove singularity. The concept of the density of states is valid for all possible dispersion relations, e.g. for electrons, phonons or photons. The density of states for the silicon band structure (cf. Fig. 6.5a) is shown in Fig. 6.31. If disorder is introduced, the density of states is modiﬁed as shown in Fig. 6.32 for amorphous germanium. The defects, as compared to the perfect lattice, introduce states in the bandgap and generally wash out the sharp features from the crystalline DOS. 6.15.2 FreeElectron Gas In M dimensions, the energy states of a freeelectron gas are given as E(k) =
M 2 2 k . 2m∗ i=1 i
(6.65)
The ki can take the values ±πn/L (in the ﬁrst Brillouin zone) with n ≤ N , N being the number of unit cells in one dimension. These values are equidistant in kspace. Each M dimensional kpoint takes a volume of (2π/L)M . 2 2 The number of states N (EF ) up to the energy EF = 2m kF (later used as Fermi energy EF and Fermi vector kF ) is
146
6 Band Structure
Fig. 6.31. Density of states in the silicon valence and conductionband (theoretical calculation using empirical pseudopotentials). From [93], based on [177]
Density of states
= 0.0 0.07 0.09
8
6
4 2 0 Energy (eV)
Ge
2
4
Fig. 6.32. Theoretical calculation for the density of states of amorphous Ge models as obtained for various degrees of disorder α (3.6). α = 0.09 corresponds to a mean shortrange order distance of about 2.4 lattice constants. From [52]
N (EF ) =
2 (2π/L)M
k=kF
dM k .
(6.66)
k=0
The factor 2 is for spin degeneracy, the integration runs over M dimensions. The density of states is the derivative D(E) = dN/dE. In the following, the density of states for M = 3, 2, 1 and zero dimensions is derived. A visualization is given in Fig. 13.1. M =3 This case relates to bulk material in which electrons are free to move in all three dimensions. Performing the integral (6.66) for M = 3 yields
6.15 Density of States
N 3D =
V 3 V k = 3π 2 F 3π 2
2mEF 2
3/2
Therefore, kF and EF are given by 2 1/3 3π N kF = V 2 2/3 3π N 2 , EF = 2m∗ V
and the density of states in three dimensions is ∗ 3/2 √ 2m V D3D (E) = E. 2 2 2π
.
147
(6.67)
(6.68) (6.69)
(6.70)
M =2 This case is important for thin layers in which the electron motion is conﬁned in one direction and free in a plane. Such structures are called quantum wells (see Sect. 11.5). We ﬁnd for the 2D density of states (for each subband over which it is not summed here, including spin degeneracy) A m∗ A 2 kF = E, (6.71) 2π π 2 where A is the area of the layer. The density of states is thus constant and given by N 2D =
D2D (E) =
A m∗ . π 2
(6.72)
M =1 The case M = 1 describes a quantum wire in which the electron motion is conﬁned in two dimensions and free in only one dimension (see Sect. 13.2). For this case, we ﬁnd for a wire of length L
1/2 2L 2m∗ E 2L kF = N 1D = . (6.73) π π 2 The density of states becomes singular at E = 0 and is given by (for one subband)
1/2 1 L 2m∗ 1D √ . (6.74) D (E) = π 2 E M =0 In this case electrons have no degrees of freedom, as, e.g., in a quantum dot (see Sect. 13.3), and each state has a δlike density of states at each of the quantized levels.
7 Electronic Defect States
¨ Uber Halbleiter sollte man nicht arbeiten, das ist eine Schweinerei, wer weiß ob es u ¨ berhaupt Halbleiter gibt.1 W. Pauli, 1931 [178]
7.1 Introduction One cm3 of a semiconductor contains about 5 × 1022 atoms. It is practically impossible to achieve perfect purity. Typical low concentrations of impurity atoms are in the 1012 − 1013 cm−3 regime. Such a concentration corresponds to a purity of 10−10 , corresponding to about one alien in the world’s human population. In the beginning of semiconductor research the semiconductors were so impure that the actual semiconducting properties could only be used ineﬃciently. Nowadays, thanks to large improvements in highpurity chemistry, the most common semiconductors, in particular silicon, can be made so pure that the residual impurity concentration plays no role in the physical properties. However, the most important technological step for semiconductors is doping, the controlled incorporation of impurities, in order to manage the semiconductor’s conductivity. Typical impurity concentrations used in doping are 1015 − 1020 cm−3 .
7.2 Fermi Distribution In thermodynamic equilibrium, the distribution function for electrons is given by the Fermi–Dirac distribution (Fermi function) fe (E) (see Appendix D) fe (E) =
exp
1 E−EF kT
+1
,
(7.1)
1 One should not work on semiconductors. They are a mess. Who knows whether semiconductors exist at all.
150
7 Electronic Defect States
where k (or kB ) denotes the Boltzmann constant, T is the temperature, and EF is the Fermi level, which is called the chemical potential μ in thermodynamics. The Fermi distribution is shown in Fig. 7.1. The distribution function gives the probability that a state at energy E is populated in thermodynamic equilibrium. For E = EF the population is 1/2 for all temperatures. At (the unrealistic case of) T = 0, the function makes a step from 1 (for E < EF ) to 0.
(a)
(b)
(c)
(d)
Fig. 7.1. Fermi function for (a,b) diﬀerent temperatures (for EF = 1.0 eV) and (c) for diﬀerent chemical potentials (for T = 300 K). (d) Fermi function (solid lines) compared with Boltzmann approximation (dashed lines) for various temperatures and EF = 1.0 eV on semilogarithmic plot
The highenergy tail of the Fermi distribution, i.e. for E − EF ≫ kT , can be approximated by the Boltzmann distribution:
E − EF fe (E) ≈ exp − kT
.
(7.2)
If the Boltzmann distribution is a good approximation, the carrier distribution is called nondegenerate. If the Fermi distribution needs to be invoked, the carrier ensemble is called degenerate. If the Fermi level is within the band the ensemble is highly degenerate.
7.3 Carrier Concentration
151
7.3 Carrier Concentration Generally, the density of electrons in the conduction band is given by ∞ De (E)fe (E)dE , (7.3) n= EC
and accordingly the density of holes in the valence band is EV p= Dh (E)fh (E)dE .
(7.4)
−∞
The energy of the top of the valence band is denoted by EV , the bottom of the conduction band as EC . The distribution function for holes is fh = 1−fe . Thus, fh (E) = 1 −
exp
1 E−EF kT
+1
=
exp
1 F − E−E kT
+1
.
(7.5)
We assume parabolic band edges, i.e. effective masses me and mh for electrons and holes, respectively. The density of states in the conduction band (per unit volume) is given (for E > EC ) as (cf. (6.70)) De (E) =
1 2π 2
2me 2
3/2
1/2
(E − EC )
.
(7.6)
If, in the previous consideration the Boltzmann approximation cannot be applied, i.e. at high temperatures or for very small bandgaps, the integral over Df cannot be explicitly (or analytically) evaluated. In this case the Fermi integral is needed that is deﬁned2 as ∞ yn 2 dy . (7.7) Fn (x) = √ π 0 1 + exp(y − x) In the present case of bulk materials n = 1/2. For large negative argument, i.e. x < 0 and x ≫ 1, F1/2 (x) ≈ exp(x), which is the Boltzmann approximation. F1/2 (0) ≈ 0.765 ≈ 3/4. For large argument, i.e. x ≫ 1, √ F1/2 (x) ≈ (2 π)(2/3)x3/2 . Such fairly simple approximations are plotted in Fig. 7.2 in comparison with the Fermi integral. For computations, numerical approximations are used [179, 180]. The derivative of the Fermi integral is given by Fn′ (x) = nFn−1 (x), n > 0. For n = 0, i.e. a twodimensional system, the integral can be executed explicitly, F0 (x) = ln [1 + exp(x)]. With the Fermi integral F1/2 (7.15) and (7.16) then have the following expressions for the freecarrier densities: 2
Equation (7.7) is restricted to n > −1. A form without restriction is Fn (x) = ∞ yn dy. 0 1+exp(y−x)
1 Γ (n+1)
152
7 Electronic Defect States
(a)
(b)
Fig. 7.2. Fermi integral F1/2 with approximations in three regions of the argument: A1 (x) = exp(x) for x < 2, A2 (x) = (1/4 + exp(−x))−1 for −2 < x < 2, A3 (x) = √ (2/ π)(2/3)x3/2 for x > 2. (a) linear, (b) semilogarithmic plot
EF − E C kT
EF − E V p = NV F1/2 − , kT
n = NC F1/2
(7.8) (7.9)
with NC = 2 NV = 2
me kT 2π2 mh kT 2π2
3/2
3/2
(7.10) ,
(7.11)
where NC (NV ) is called the conductionband (valenceband) edge density of states. If the conductionband minimum is degenerate, a factor gv (valley degeneracy) must be included, i.e. gv = 6 for Si and gv = 8 for Ge (gv = 1 for GaAs). This factor is typically included in the mass used in (7.10) that then becomes the density of states mass md,e . If the conductionband minimum has cylindrical symmetry in kspace, such as for Si and Ge, the mass that has to be used is 1/3 . (7.12) md,e = gv2/3 m2t ml
In the case of a degeneracy of the valence band, the states of several bands need to be summed for NV . In bulk material, typically the heavy and light hole bands are degenerate at the Γ point. If the splitoff band is not populated because of insuﬃcient temperature, the valenceband edge density of states is given by
3/2 kT 3/2 3/2 . (7.13) m NV = 2 + m hh lh 2π2
7.4 Intrinsic Conduction
153
Alternatively, the mass mh in (7.11) can be taken as the density of states hole mass 3/2
3/2
md,h = (mhh + mlh )2/3 .
(7.14)
Values of NC,V for Si, Ge and GaAs are given in Table 7.1. Now, we assume that the Boltzmann approximation (7.2) can be used, i.e. the probability that a band state is populated is ≪ 1. Then, the integral (7.3) can be executed analytically and the concentration n of electrons in the conduction band is given as
3/2 E F − EC EF − EC me kT exp exp = N . (7.15) n=2 C 2π2 kT kT For the Boltzmann approximation and a parabolic valence band, the density of holes is given by
3/2
mh kT EF − E V EF − EV exp − = NV exp − . (7.16) p=2 2π2 kT kT The product of the electron and hole density is
Eg EC − E V n p = NV NC exp − = NV NC exp − kT kT
3 kT Eg =4 (md,e md,h )3/2 exp − . 2π2 kT
(7.17)
Thus, the product np is independent of the position of the Fermi level, as long as the Boltzmann approximation is fulﬁlled, i.e. the Fermi level is not in the vicinity of one of the band edges within several kT : EV + 4kT < EF < EC − 4kT .
(7.18)
The relation (7.17) is called the mass–action law. In Fig. 7.3, the product np is shown for silicon over a wide range of Fermi energies. If EF is within the bandgap, np is essentially constant. If the Fermi level is in the valence or conduction band, np decreases exponentially.
7.4 Intrinsic Conduction First, we consider the conductivity of the intrinsic, i.e. an ideally pure, semiconductor. At T = 0 all electrons are in the valence band, the conduction band is empty and thus the conductivity is zero (a completely ﬁlled band cannot conduct current). Only at ﬁnite temperatures the electrons have a ﬁnite probability to be in a conductionband state and contribute to the conductivity. Due to neutrality, the electron and hole concentrations in the intrinsic
154
7 Electronic Defect States
(b)
(a)
Fig. 7.3. (a) np for silicon at T = 300 K as a function of the position of the Fermi level. The valenceband edge EV is chosen as E = 0. np is constant for the range √ of Fermi energies given by (7.18) (4kT ≈ 0.1 eV). (b) n, p and np as a function of the Fermi level
semiconductors are the same, i.e. each electron in the conduction band comes from the valence band, −n + p = 0 ,
(7.19)
or ni = pi . Therefore
Eg ni = pi = NV NC exp − 2kT
3/2
kT Eg 3/4 (m m ) exp − . =2 e h 2π2 2kT
(7.20)
The massaction law n p = ni pi = n2i = p2i
(7.21)
will be essential also for doped semiconductors. The intrinsic carrier concentration is exponentially dependent on the bandgap. Thus, in thermodynamic equilibrium intrinsic widegap semiconductors have much smaller electron concentrations than intrinsic smallgap semiconductors (see Table 7.1). The intrinsic carrier concentration of Si has been determined to be (within 1%, T in K)
Eg (T ) 15 1.706 (7.22) = 1.640 × 10 T exp − nSi i 2kT for temperatures between 77 and 400 K [181, 182]. As we will see later in Part II, many semiconductor devices rely on regions of low conductivity (depletion layers) in which the carrier concentration is
7.4 Intrinsic Conduction
155
(b)
(a)
Fig. 7.4. (a) Bandgap and (b) intrinsic carrier concentration of silicon vs. temperature Table 7.1. Bandgap, intrinsic carrier concentration, conduction band and valenceband edge density of states at T = 300 K for various semiconductors
InSb InAs Ge Si GaAs GaP GaN
Eg (eV)
ni (cm−3 )
NC (cm−3 )
NV (cm−3 )
0.18 0.36 0.67 1.124 1.43 2.26 3.3
1.6 × 1016 8.6 × 1014 2.4 × 1013 1.0 × 1010 1.8 × 106 2.7 × 100 ≪1
1.04 × 1019 7.28 × 1019 4.35 × 1017
6.0 × 1018 1.05 × 1019 5.33 × 1018
small. Since the carrier concentration cannot be smaller than the intrinsic concentration (n + p ≥ 2ni ), an increase of temperature leads to increasing ohmic conduction in the depletion layers and thus to a reduction or failure of device performance. The small bandgap of Ge leads to degradation of bipolar device performance already shortly above room temperature. For silicon, intrinsic conduction limits operation typically to temperatures below about 300◦ C. For higher temperatures, as required for devices in harsh environments, such as close to motors or turbines, other semiconductors with wider bandgaps need to be used, such as GaN, SiC or even diamond. From the neutrality condition for the intrinsic semiconductor (7.19) and (7.15) and (7.16), the Fermi level of the intrinsic semiconductor can be determined as
NV mh kT 3 EV + E C EV + EC EF = + ln + kT ln = . (7.23) 2 2 NC 2 4 me Since the hole mass is perhaps a factor of ten larger than the electron mass, the second term has the order of kT . Thus, for typical semiconductors
156
7 Electronic Defect States E
E
EC ED
EF
E
n
EC
EV
EV
p
(a) D(E) E
n,p
f(E) E
E
EC
EC
n
EV
p
EF EV (b) D(E)
f(E) E
E
n,p E
EC
EC
n
EF
EA EV
EV
p
(c) D(E)
f(E)
n,p
Fig. 7.5. Density of states (left column), Fermi distribution (center column) and carrier concentration (right column) for (a) ntype, (b) intrinsic and (c) ptype semiconductors in thermal equilibrium
where Eg ≫ kT , the intrinsic Fermi level, denoted by Ei , is close to the middle of the bandgap, i.e. EF ≈ (EC + EV )/2. The situation for an intrinsic semiconductor is schematically shown in Fig. 7.5a.
7.5 Shallow Impurities, Doping The electronic levels of an impurity can be within the forbidden gap of the bulk host material. These levels can be close to the band edges or rather in the middle of the bandgap. In Fig. 7.6, the positions of the energy levels
7.5 Shallow Impurities, Doping
157
of a variety of impurities are shown for Ge, Si and GaAs. An impurity for which the longrange Coulomb part of the ioncore potential determines the energetic level is termed a shallow impurity. The extension of the wavefunction is given by the Bohr radius. This situation is in contrast to a deep level where the shortrange part of the potential determines the energy level. The extension of the wavefunction is then of the order of the lattice constant.
Fig. 7.6. Energetic position (ionization energy) of various impurities in Ge, Si and c GaAs. Reprinted with permission from [183], 1981 Wiley
We will consider ﬁrst a groupIV semiconductor, Si, and (impurities) dopants from the groups III and V of the periodic system. When these are incorporated on a lattice site (with tetrahedral bonds), there is one electron too few (group III, e.g. B) or one electron too many (group V, e.g. As). The ﬁrst case is called an acceptor , the latter a donor . The doping of III–V semiconductors is detailed in [184]. 7.5.1 Donors Silicon doped with arsenic is denoted as Si:As. The situation is schematically shown in Fig. 7.7. The arsenic atom has, after satisfying the tetrahedral bonds, an extra electron. This electron is bound to the arsenic atom via the Coulomb interaction since the ion core is positively charged compared to the silicon cores. If the electron is ionized, a ﬁxed positive charge remains at the As site.
158
7 Electronic Defect States
Si
Si As
Si
Si
Si
Si
Si
Fig. 7.7. Arsenic impurity in silicon. Arsenic donates one electron, and a ﬁxed positive charge remains
A free arsenic atom has an ionization energy of 9.81 eV. However, in the solid the Coulomb interaction is screened by the (static) dielectric constant ǫr of the material, which is of the order of 10 for typical semiconductors. Additionally, the mass is renormalized (effective mass) by the periodic potential to a value that is smaller than the freeelectron mass. Within effective mass theory (Appendix F) the hydrogen problem is scaled with the (isotropic) effective mass m∗e and the dielectric constant ǫr , the binding energy (ionization b energy) ED of the electron to the shallow donor is (relative to the continuum given by the conductionband edge EC ) b ED =
m∗e 1 m0 e4 . m0 ǫ2r 2(4πǫ0 )2
(7.24)
b . The ﬁrst The absolute energy position of the level is ED = EC − ED factor in the right side of (7.24) is the ratio of effective and freeelectron mass, typically 1/10, the second factor is typically 1/100. The third factor is the ionization energy of the hydrogen atom, i.e. the Rydberg energy of 13.6 eV. Thus, the binding energy in the solid is drastically reduced by about 10−3 to the 10 meV regime. The extension of the wavefunction of the electron bound to the ﬁxed ion is given by the Bohr radius
aD =
m0 ǫr aB , m∗e
(7.25)
where aB = 0.053 nm denotes the hydrogen Bohr radius. For GaAs aD = 10.3 nm. For semiconductors with a nonisotropic band minimum, such as Si, Ge or GaP, an ‘elliptically deformed’ hydrogen problem with the masses ml and mt has to be treated [185]. An impurity that fulﬁlls (7.24) is called an effectivemass impurity. For silicon we ﬁnd, from (7.24), a donor binding energy of 6 meV. Using the correct tensor of the effective masses, the result for the effectivemass donor binding energy is 9.05 meV. Some experimentally observed values are summarized in Table 7.2. For GaAs, the effectivemass donor has a binding energy of 5.715 meV, which is fulﬁlled for several chemical species (Table 7.3). In
7.5 Shallow Impurities, Doping
159
GaP, experimental values deviate considerably from the effective mass donor (59 meV). b Table 7.2. Binding energies ED of groupV donors in Si and Ge. All values in meV
Si Ge
P
As
Sb
45 12.0
49 12.7
39 9.6
b Table 7.3. Binding energies ED of donors in GaAs (data from [186]), GaP (data from [187]) and GaN (low concentration limits, data from [188, 189]). All values in meV
V site
III site
GaAs
S Se Te
5.854 5.816 5.786
C Si Ge
5.913 5.801 5.937
GaP
O S Se Te
897 107 105 93
Si Ge Sn
85 204 72
GaN
O
39
Si
22
The donors are typically distributed statistically (randomly) in the solid. Otherwise their distribution is called clustered. The concentration of donors is labeled ND and usually given in cm−3 . The concentration of donors populated with an electron (neutral donors) is denoted by ND0 , the concentration of ionized donors (positively charged) is ND+ . Other conventions in the literature label the concentrations N1 and N0 , respectively: N1 = ND0 = ND fe (ED ) N0 = ND+ = ND (1 − fe (ED )) , −1
with fe (ED ) = [1 + exp(ED − EF )] condition
. For the sum of these quantities the
ND = ND+ + ND0 holds.
(7.26a) (7.26b)
(7.27)
160
7 Electronic Defect States
The ratio of the two concentrations is ﬁrst given as (caveat: this formula will be modiﬁed below) ND0 f N1 = = exp + = N0 1−f ND
E F − ED kT
.
(7.28)
Now, the degeneracy of the states has to be considered. The donor charged with one electron has a 2fold degeneracy g1 = 2 since the electron can take the spin up and down states. The degeneracy of the ionized (empty) donor is g0 = 1. Additionally, we assume here that the donor cannot be charged with a second electron. Due to Coulomb interaction the energy level of the possible ND− state is in the conduction band. Otherwise, a multiply charged center would be present. We also do not consider excited states of ND0 that might be in the bandgap as well. In the following, we will continue with gˆ = g1 /g0 = 2. Considering the degeneracy, (7.28) needs to be modiﬁed to ND0 N1 = gˆ exp + = N0 ND
E F − ED kT
.
(7.29)
This can be understood from thermodynamics (see Sect. 4.3), a rate analysis or simply the limit T → ∞. The probabilities f 1 and f 0 for a populated or empty donor, respectively, are 1 N1 ED −EF = −1 ND +1 gˆ exp kT N0 1 . = f0 = −EF ND +1 gˆ exp − EDkT f1 =
(7.30a) (7.30b)
First, we assume that no carriers in the conduction band stem from the valence band (no intrinsic conduction). This will be the case at suﬃciently low temperatures when ND ≫ ni . Then the number of electrons in the conduction band is equal to the number of ionized donors, i.e. ND −ED 1 + gˆ exp EFkT n 1 ND , ND = = n + n1 1 + n1 /n
n = f 0 ND = N0 =
(7.31)
7.5 Shallow Impurities, Doping
b with n1 = (NC /ˆ g ) exp −ED /kT . The neutrality condition is −n + ND+ = −n + N0 = 0 .
Thus the equation (n is given by (7.15))
EF − EC ND −ED = 0 − NC exp kT 1 + gˆ exp EFkT
needs to be solved to obtain the Fermi level.3 The result is ⎤ ⎡$ b %1/2 ED ND exp − 1 1 + 4ˆ g NC kT ⎥ ⎢ b + kT ln ⎣ EF = E C − E D ⎦ . 2ˆ g
161
(7.32)
(7.33)
(7.34)
For T → 0 the Fermi level is, as expected, in the middle between the b populated and unpopulated states, i.e. at EF = EC − ED /2. In Fig. 7.8a the position of the Fermi level is shown for a donor with 45 meV binding energy in Si. For low temperatures the solution can be approximated as (dashed curve in Fig. 7.8b)
ND 1 1 b ∼ . (7.35) EF = EC − ED + kT ln 2 2 gˆNC
The freezeout of carriers in ntype silicon has been discussed in detail in [191], taking into account the effects of the ﬁne structure of the donor states. We note that the fairly high donor binding energy in silicon leads to freezeout of carriers at about 40 K and is thus limiting for the lowtemperature performance of devices. Ge has smaller donor ionization energies and subsequently a lower freezeout temperature of 20 K. For ntype GaAs, conductivity is preserved down to even lower temperatures. For higher temperatures, when the electron density saturates towards ND , the approximate solution is (dashdotted curve in Fig. 7.8a)
ND . (7.36) EF ∼ = EC + kT ln NC The electron density n is given (still in the Boltzmann approximation) by b %1/2 $ ED
1 + 4ˆ D gN −1 b NC exp kT ED n = NC exp − kT 2ˆ g 2ND = $ b %1/2 . ED D 1 + 1 + 4ˆ gN exp NC kT
(7.37)
3 As usual, the Fermi level is determined by the global charge neutrality, see also Sect. 4.3.
162
7 Electronic Defect States
(a)
(b)
b = 45 meV, no Fig. 7.8. (a) Position of the Fermi level in Si:P (ND = 1015 cm−3 , ED acceptors) as a function of temperature without consideration of intrinsic carriers. Zero energy refers to the (temperaturedependent, Table 6.2) conductionband edge EC with approximative solutions for low (dashed line, (7.35)) and high (dashdotted line, (7.36)) temperatures. (b) Corresponding density of conductionband electrons as a function of temperature
The electron density as a function of temperature is shown in Fig. 7.8b. For low temperatures, the solution is close to n∼ =
ND NC gˆ
1/2
Eb exp − D = n1 ND . 2kT
(7.38)
For high temperatures, n ∼ = ND . This regime is called exhaustion or saturation since all possible electrons have been ionized from their donors. We note that even in this case np = ni pi holds, however, n ≫ p. While the characteristic energy for the ionization of electrons from donors b is ED , at high enough temperatures electrons are transferred also from the valence band into the conduction band. Thus, in order to make the above consideration valid for all temperatures the intrinsic conduction also has to be considered. The neutrality condition (still in the absence of any acceptors) is −n + p + ND+ = 0 .
(7.39)
Using (7.15) and p = n2i /n, the equation
E F − EC ND n2i NC exp − − =0 −EC −ED kT NC exp( EFkT ) 1 + gˆ exp( EFkT )
(7.40)
needs to be solved. The result is ⎡
with
b + kT ln ⎣ EF = EC − E D
β γ
+
γ 2 NC
3ˆ g
−1
⎤
⎦ ,
(7.41)
7.5 Shallow Impurities, Doping
#1/3 (NC4 α)2 − 4(NC2 β)3 γ= 2
ED 2ED 2 2 2 g NC ND exp β = NC + 3ˆ + 3ˆ g ni exp kT kT
2ED E D 2 2 2 α = 2NC + 9ˆ − 18ˆ g ni exp . g NC ND exp kT kT "
−NC4 α +
163
(7.42)
The temperaturedependent position of the Fermi level is shown in Fig. 7.9.
(a)
(b)
b Fig. 7.9. (a) Position of the Fermi level in Si:P (ND = 1015 cm−3 , ED = 45 meV, no acceptors) as a function of temperature. The temperature dependence of the bandgap (as given in Table 6.2) has been taken into account. Zero energy refers to the conductionband edge for all temperatures. The dotted curve shows Eg /2. The dashed (dashdotted) line shows the low (high) temperature limit according to (7.35) and (7.23), respectively. (b) Corresponding electron concentration as a function of temperature. The dashed line shows the intrinsic carrier density
The carrier concentration is given by
Eb n = NC exp − D kT
β γ
+
γ 2 NC
3ˆ g
−1
,
(7.43)
with α, β and γ having the same meaning as in (7.41). The three important regimes are the intrinsic conduction at high temperatures when ni ≫ ND , the exhaustion at intermediate temperatures when ni ≪ ND and kT > ED , and ﬁnally the freezeout regime for kT ≪ ED at low temperatures when the electrons condense back into the donors. The rates for these processes will be discussed in Sect. 10.10. A similar plot as in Fig. 7.9b is shown in Fig. 7.10. With increasing temperature the Fermi level shifts from close to the band edge towards the band center. At higher doping the shift begins at higher temperatures.
164
7 Electronic Defect States
Fig. 7.10. Fermi level in silicon as a function of temperature for various doping levels (ntype and ptype) of 1012 , 1013 , . . . , 1018 cm−3 . The intrinsic Fermi level is chosen as zero energy for all temperatures. The (temperaturedependent) conduction and valence band edges are shown as dashed lines
The electronic states of individual donors can be directly visualized by scanning tunneling microscopy (STM) as shown in Fig. 7.11 for Si:P. For small negative bias, tunneling occurs through the charged dopant that is located within the ﬁrst three monolayers. At high negative bias the large contribution from the ﬁlled valence band masks the effect of the donor. This image, however, shows that the contrast attributed to the dopant atom is not due to surface defects or absorbates. 7.5.2 Acceptors A groupIII atom in Si has one electron too few for the tetrahedral bond. Thus, it ‘borrows’ an electron from the electron gas (in the valence band) and thus leaves a missing electron (termed hole) in the valence band (Fig. 7.12). The energy level is in the gap close to the valenceband edge. The latter consideration is made in the electron picture. In the hole picture, the acceptor ion has a hole and the hole ionizes (at suﬃcient temperature) into the valence band. After ionization the acceptor is charged negatively. Also, for this system a hydrogenlike situation arises that is, however, more complicated than for donors because of the degeneracy of the valence bands and their warping. b In Table 7.4 the acceptor binding energies EA for groupIII atoms in Ge b and Si are listed. The absolute acceptor energy is given as EA = EV + EA . In Table 7.5 acceptor binding energies are listed for GaAs and GaP. While in GaAs some acceptors are close to the effective mass value of 27 meV, in GaP the deviation from the effective mass value ≈50 meV is large.
7.5 Shallow Impurities, Doping
(a)
165
(b)
Si
tip
EF
D EF
low negative bias
high negative bias
Fig. 7.11. Filledstate image of a phosphorus atom underneath a Si (001) surface at a tunneling current of 110 pA. The doping level is 5 × 1017 cm−3 . (a) Sample bias −0.6 V, (b) sample bias −1.5 V between Si:P and tip. Image sizes are 22 × 22 nm2 . c Reprinted with permission from [192], 2004 APS. Lower row : Schematic band diagrams for the two bias situations
Si
Si
B
Si
Si
Si
Si
Si
Fig. 7.12. Boron impurity in silicon. Boron accepts one electron and a ﬁxed negative charge remains
When the conductivity is determined by holes or electrons, the material is called ptype or ntype, respectively. We note that some metals also show hole conduction (e.g. Zn). However, for metals the conductivity type is ﬁxed, while the same semiconductor can be made n or ptype with the appropriate doping.
166
7 Electronic Defect States
b of groupIII acceptors in Si and Ge. All values in Table 7.4. Binding energies EA meV
Si Ge
B
Al
Ga
In
45 10.4
57 10.2
65 10.8
16 11.2
b Table 7.5. Binding energies EA of acceptors in GaAs, GaP and GaN (low concentration value, data from [193]). All values in meV
V site
III site
GaAs
C Si Ge Sn
27 34.8 40.4 167
Be Mg Zn Cd
28 28.8 30.7 34.7
GaP
C Si Ge
54 210 265
Be Mg Zn Cd
57 60 70 102
Mg
220
GaN
The acceptor concentration is denoted by NA . The concentration of neutral acceptors is NA0 , the concentration of charged acceptors is NA− . Of course NA = NA0 + NA− .
(7.44)
The ratio of the degeneracy of the (singly) ﬁlled and empty acceptor level is gˆA . gˆA = 1/2 for the spin degeneracy of the states in the electron picture.4 Thus, similar to the considerations for electrons and donors,
NA0 EF − EA = gˆA exp − . (7.45) kT NA− The population of the acceptor levels is given by NA− =
NA . −EA 1 + gˆA exp − EFkT
(7.46)
The formulas for the position of the Fermi level and the hole density are analogous to those obtained for electrons and donors and will not be 4 For donors the neutral state is degenerate, for acceptors the charged state is degenerate.
7.5 Shallow Impurities, Doping
167
explicitly given here. In Fig. 7.10, the temperature dependence of the Fermi level is included for ptype Si. With increasing temperature the Fermi level b shifts from the valenceband edge (For T = 0, EF = EV + EA /2) towards the middle of the bandgap (intrinsic Fermi level). Also, the wavefunction at acceptors can be imaged using scanning tunneling microscopy [194]. In [195] images of ionized and neutral Mn in GaAs have been reported (Fig. 7.13b). The tunneling I–V characteristics are shown in Fig. 7.13a. At negative bias, the acceptor is ionized and appears spherically symmetric due to the effect of the A− ion Coulomb potential on the valenceband states. At intermediate positive voltages, tunneling is through the neutral state. The wavefunction of A0 looks like a bowtie due to the admixture of dwavefunctions [196]. The Mn atom is presumably in the third subsurface atomic layer. At even higher positive bias the contrast due to the dopant is lost because the image is dominated by a large tunneling current from the tip to the empty conduction band. (b)
Current (pA)
40
(c)
GaAs:Mn
Mn A0 channel 20 GaAs
UFB 0
tip EF
MnGa
A
GaAs
A
EF
100 meV 0.8
(a)
0.4
0.0 0.4 0.8 Bias voltage (V)
1.2
1.6 negative bias
positive bias
Fig. 7.13. (a) Tunneling I–V characteristic of GaAs:Mn sample. Solid (dashed) line is for pure GaAs (subsurface Mn on Ga site). UFB denotes the simulated ﬂatband voltage. Adapted from [195]. (b,c) STM images of a Mn atom underneath a GaAs (110) surface. The doping level is 3 × 1018 cm−3 . (b) Sample bias −0.7 V, (c) sample bias +0.6 V. Below the images are schematic band diagrams of GaAs:Mn and tip. Image sizes are (b) 8×8 nm2 and (c) 5.6×5 nm2 . Reprinted with permission c from [195], 2004 APS. Lower row under parts (b,c): Schematic band diagrams for the two bias situations
7.5.3 Compensation When donors and acceptors are simultaneously present, some of the impurities will compensate each other. Electrons from donors will recombine with
168
7 Electronic Defect States
holes on the acceptors. Depending on the quantitative situation the semiconductor can be n or ptype. This situation can be invoked by intentional doping with donors or acceptors or by the unintentional background of donors (acceptors) in pdoped (ndoped) material. The chargeneutrality condition (now ﬁnally in its most general form) reads −n + p − NA− + ND+ = 0 .
(7.47)
We will now investigate the case of the presence of donors and acceptors, but limit ourselves to suﬃciently low temperatures (or wide bandgaps) such that the intrinsic carrier density can be neglected. We assume Boltzmann statistics and assume here ND > NA . Then it is a very good approximation to use NA− = NA since there are enough electrons from the donors to recombine with (and thus compensate) all acceptors. Under the given assumptions regarding the temperature p = 0 and the material is ntype. Thus, in order to determine the position of the Fermi level, the following equation (chargeneutrality condition n + NA − ND+ = 0 ) must be solved (compare to (7.33))
EF − EC ND + NA − =0. (7.48) NC exp −ED kT 1 + gˆ exp( EFkT ) The solution is ⎡$
2 A exp g NDN−N C ⎢ α + 4ˆ b EF = EC − ED + kT ln ⎣ 2ˆ g
α = 1 + gˆ
NA exp NC
b ED kT
b ED kT
% 21
.
⎤ − α⎥ ⎦
(7.49)
For NA = 0 we have α = 1 and (7.34) is reproduced, as expected. For T = 0 the Fermi energy lies at EF = ED since the donor level is partially ﬁlled (ND0 = ND −NA ). For low temperatures the Fermi level is approximated by
ND /NA − 1 b ∼ EF = EC − ED + kT ln . (7.50) gˆ The corresponding carrier density is (α has the same meaning as in (7.49))
n = NC exp −
b ED
kT
$ b % 21 ED
α2 + 4ˆ A g NDN−N exp −α kT C 2ˆ g
.
(7.51)
For very low temperatures (n < NA ), the exponential slope of n(T ) is b : given by ED
7.5 Shallow Impurities, Doping
(a)
169
(b)
Fig. 7.14. (a) Position of Fermi level in partially compensated Si:P,B (ND = b b 1015 cm−3 , ED = 45 meV, EA = 45 meV, solid line: NA = 1013 cm−3 , dashed line: NA = 0, dashdotted line: NA = 1012 cm−3 , shortdashed line: NA = 1014 cm−3 , dashdouble dotted line: NA = 5 × 1014 cm−3 ) as a function of temperature. (b) Corresponding electron concentration for NA = 1013 cm−3 as a function of temperature (neglecting intrinsic carriers), dashed line for NA = 0 according to (7.38), dashdotted line approximation for n ≪ NA as in (7.52)
n∼ =
Eb ND − NA NC exp − D . NA gˆ kT
(7.52)
b /2 as in the For higher temperatures (n > NA ) the slope is given by ED uncompensated case (7.38). For suﬃciently high temperatures in the exhaustion regime (but still ni < n) the electron density is given by
n ≈ ND − NA .
(7.53)
At even higher temperatures the electron density will be determined by the intrinsic carrier concentration. An experimental example is shown in Fig. 7.15 for partially compensated pSi (with ND ≪ NA ). If donors are added to a ptype semiconductor, ﬁrst the semiconductor remains pconducting as long as ND ≪ NA . If the donor concentration becomes larger than the acceptor concentration, the conductivity type switches from p to nconduction. If the impurities are exhausted at room temperature, the lowest carrier concentration is reached for ND = NA . Such a scenario is shown for ptype Inx Ga1−x As1−y Ny doped with various concentrations of Si in Fig. 7.16. At high Si incorporation, the number of charge carriers saturates due to autocompensation (see next section) and the formation of Si precipitates. Since the ionization energies of donors and acceptors are typically different, the situation for ND ≈ NA needs, in general, to be investigated carefully and will depend on the temperature.
170
7 Electronic Defect States 10
15
NA
Hole concentration (cm3)
1014 ^ slope = 23 meV
1013 1012 1011
ND ^ slope = 46 meV
1010 109
Si
108 0
0.01
0.02
0.03 0.04 1/T (1/K)
0.05
0.06
b Fig. 7.15. Hole density in ptype silicon (NA = 7.4 × 1014 cm−3 , EA = 46 meV (probably boron) and partial compensation with ND = 1.0 × 1011 cm−3 ). Adapted from [197]
7.5.4 Amphoteric Impurities
Carrier concentration (cm 3 )
If an impurity atom can act as a donor and acceptor it is called amphoteric. This can occur if the impurity has several levels in the bandgap (such as Au in Ge or Si). In this case, the nature of the impurity depends on the position of the Fermi level. Another possibility is the incorporation on different lattice sites. For example, carbon in GaAs is a donor if incorporated on the Gasite. On the Assite carbon acts as an acceptor.
10
10 10
10
19
n
17
15
p
13
10
5
10
4
10
3
10
2
10
1
pSi H / pgroupIII 2
6
Fig. 7.16. Carrier concentration and conductivity type (empty squares: p, solid squares: n) for MOVPEgrown Inx Ga1−x As1−y Ny layers on GaAs (001) (layer thickness ≈ 1 µm, x ≈ 5%, y ≈ 1.6%) doped with diﬀerent amounts of silicon. The ordinate is the ratio of the partial pressures of disilane and the groupIII precursors (TMIn and TMGa) in the gas phase entering the MOVPE reactor. Solid lines are guides to the eye. Experimental data from [198]
7.5 Shallow Impurities, Doping
171
Thus, e.g., crystal growth kinetics can determine the conductivity type. In Fig. 7.17 the conductivity due to carbon background is shown for GaAs grown using MOVPE under various growth conditions. At high (low) arsine partial pressure incorporation of carbon on Assites is less (more) probable, thus the conductivity is ntype (ptype). Also, growth on different surfaces can evoke different impurity incorporation, e.g., ntype on (001) GaAs and ptype on (311)A GaAs, since the latter is Gastabilized.
Carrier concentration (cm3)
10
18
ptype ntype
10
17
GaAs (001) 10
16
10
0
1
10 AsH3/TMG ratio
10
2
Fig. 7.17. Background doping of GaAs due to carbon in MOVPE for diﬀerent ratios of the partial pressures of AsH3 and TMG (trimethylgallium). The conductivity type (squares: ntype, circles: ptype) depends on the incorporation of C from CH3 radicals on Ga or Assite. Lines are guides to the eye. Experimental data from [199]
Deviation from the ideal stoichiometry introduces point defects that can be electrically active and change conductivity type and carrier concentration. In the case of CuInSe2 , excess Cu could go on interstitial positions or promote selenium vacancies, both leading to ntype behavior. This material is particularly sensitive to deviations from ideal stoichiometry for both Cu/In ratio (Fig. 7.18) and Se deﬁciency [200]. 7.5.5 High Doping For low doping concentrations, the impurity atoms can be considered to be decoupled. At low temperature, only hopping from one impurity to the next is possible due to thermal emission or tunneling and the semiconductor becomes an insulator. With increasing concentration, the distance between impurities decreases and their wavefunctions can overlap. Then, an impurity band develops (Fig. 7.19). A periodic arrangement of impurity atoms would result in welldeﬁned band edges as found in the Kronig–Penney model. Since the impurity atoms are randomly distributed, the band edges exhibit tails. For high doping, the impurity band overlaps with the conduction band. In the case of
172
7 Electronic Defect States
Carrier concentration (cm3)
102
CuInSe2
1019 1018 1017 1016 ptype ntype
1015 1014 1013
0.5
1.0 Cu/In
1.5
Fig. 7.18. Carrier concentration and conductivity type (squares: ntype, circles: ptype) as a function of stoichiometry (Cu/In ratio) for CuInSe2 thin ﬁlms. Lines are guides to the eye. Experimental data from [200]
compensation, the impurity band is not completely ﬁlled and contains (a new type of) holes. In this case, conduction can take place within the impurity band even at low temperature, making the semiconductor a metal. This metal–insulator transition has been discussed by Mott [201]. E
E
EC ED
EC
EV
EV
E
EV
D(E) (a)
D(E) (b)
D(E) (c)
Fig. 7.19. Principle of the formation of a (donor) impurity band. (a) Small doping concentration and sharply deﬁned impurity state at ED , (b) increasing doping and development of an impurity band that (c) widens further and eventually overlaps with the conduction band for high impurity concentration. The shaded areas indicate populated states at T = 0 K
(a)
15 b
ED
173
1020
Ge:As
10
5 0 13 14 15 16 17 18 12 10 10 10 10 10 10 10 3 NDNA (cm ) (b)
Electron concentration (cm3)
Ionization energy (meV)
7.5 Shallow Impurities, Doping (iii)
10
19
10
18
10
17
10
16
(ii)
(i)
Si:P 10
15
0
2
4
6 8 10 1/T (1000/K)
12
14
Fig. 7.20. (a) Donor ionization energy in ntype Ge for various doping concenb trations. Dashed line is a guide to the eye. The arrow labeled ED denotes the lowconcentration limit (cf. Table 7.2). Experimental data from [202]. (b) Electron concentration vs. inverse temperature for Si:P for three diﬀerent doping concentrations ((i): 1.2 × 1017 , (ii): 1.25 × 1018 , (iii): 1.8 × 1019 cm−3 ). Experimental data from [203]
The formation of the impurity band leads to a reduction of the impurity ionization energy as known from (7.24). A typical result is shown in Fig. 7.20a for ntype Ge [202]. At the critical doping concentration of Nc = 1.5 × 1017 , the activation energy for the carrier concentration disappears. The freezeout of the carrier concentration (cf. Fig. 7.8) disappears as shown in Fig. 7.20b. Similar effects have been observed for Si [203] and GaAs [204]. The critical doping concentrations are listed in Table 7.6. The decrease of the ionization energy E b (donor or acceptor) follows the dependence [202, 203]
1/3 Ni 1/3 b b b , (7.54) E = E0 − αNi = E0 1 − Nc where Ni is the concentration of ionized dopants. The critical density can be estimated from the Mott criterion when the distance of the impurities becomes comparable to their Bohr radius (7.25) 2aD =
3 1/3 N . 2π c
(7.55)
The prefactor 3/(2π) stems from the random distribution of impurities and disappears for a periodic arrangement. The Mott criterion is (rewriting (7.55)) aD Nc1/3 ≈ 0.24 .
(7.56)
For GaAs with aD = 10.3 nm, the criterion yields Nc = 1.2 × 1016 cm−3 , in agreement with experiment.
174
7 Electronic Defect States
Table 7.6. Critical doping concentration for various semiconductors (at room temperature) material
type
Nc (cm−3 )
Ref.
Ge:As Si:P Si:B GaAs GaP:Zn GaN:Si GaN:Mg
n n p n p n p
1.5 × 1017 1.3 × 1018 6.2 × 1018 1 × 1016 2 × 1019 2 × 1018 4 × 1020
[202] [203] [203] [204] [205] [206] [193]
The achievable maximum concentration of electrically active dopants is limited by the concentration dependence of the diffusion coeﬃcient, Coulomb repulsion, autocompensation and the solubility limit [184]. In Table 7.7 the maximum carrier concentrations for GaAs with various dopants are listed. Table 7.7. Maximum electrically active doping concentration for GaAs material
type
Nc (cm−3 )
Ref.
GaAs:Te GaAs:Si GaAs:C GaAs:Be
n n p p
2.6 × 1019 1.8 × 1019 1.5 × 1021 2 × 1020
[207] [208] [209] [210]
7.6 QuasiFermi Levels The carrier concentrations were given by (7.8) and (7.9). So far, we have only considered semiconductors in thermodynamic equilibrium for which np = n2i . In a nonequilibrium situation, e.g. for external excitation or carrier injection in a diode, the electron and hole densities can each take arbitrary values, in principle. In particular, np will no longer be equal to n2i and there is no Fermi level constant throughout the structure. In this case, however, quasiFermi levels Fn and Fp for electrons and holes, respectively, are deﬁned via
Fn (r) − EC (7.57a) n(r) = NC F1/2 kT
Fp (r) − EV p(r) = NV F1/2 − . (7.57b) kT
7.7 Deep Levels
175
A quasiFermi level is sometimes called imref5 and can also be denoted as EFn or EFp . We emphasize that the quasiFermi levels are only a means to describe the local carrier density in a logarithmical way. The quasiFermi levels can be obtained from the density via (for Boltzmann approximation)
n Fn = EC + kT ln (7.58a) NC
p . (7.58b) Fp = EV − kT ln NV The quasiFermi levels do not imply that the carrier distribution is actually a Fermi distribution. This is generally no longer the case in thermodynamical nonequilibrium. However, in ‘wellbehaved’ cases the carrier distribution in nonequilibrium can be approximated locally as a Fermi distribution using a local quasiFermi level and a local temperature, i.e. fe (r, E) ∼ =
exp
1 E−Fn (r) kT (r)
.
(7.59)
+1
Using the quasiFermi levels, np is given by (for Boltzmann approximation)
Fn (r) − Fp (r) . (7.60) n(r) p(r) = n2i exp kT We note that for an inhomogeneous semiconductor or a heterostructure (see Chap. 11), ni may also depend on the spatial position. In the case of thermodynamic equilibrium the difference of the quasiFermi levels is zero, i.e. Fn − Fp = 0 and Fn = Fp = EF .
7.7 Deep Levels For deep levels the shortrange part of the potential determines the energy level. The longrange Coulomb part will only lead to a correction. The term ‘deep level’ implies that the level is within the bandgap and not close to the band edges. However, some deep levels (in the sense of the potential being determined by the ion core) have energy levels close to the band edges or even within a band. Details can be found in [72, 211, 212]. The wavefunction is strongly localized. Thus, it cannot be composed of Bloch functions, as has been done for the shallow levels for the effectivemass impurity. The localization in r space leads to a delocalization in k space. The wavefunction might thus have components far away from the Γ point. 5 W. Shockley had asked E. Fermi for permission to use his name reversed. Fermi was not too enthusiastic but granted permission.
176
7 Electronic Defect States
Examples are Si:S, Si:Cu or InP:Fe, GaP:N, ZnTe:O. Deep levels can also be due to defects such as vacancies or antisite defects. Due to the larger distance to the band edges, deep levels are not eﬃcient at providing free electrons or holes. Quite the opposite, they rather capture free carriers and thus lead to a reduction of conductivity. Centers that can capture electrons and holes lead to nonradiative recombination of electrons through the deep level into the valence band (see also Chap. 10). This can be useful for the fabrication of semiinsulating layers with low carrier concentration and fast time response of, e.g., switches and photodetectors. 7.7.1 Charge States The level can have different charge states depending on the occupancy of the levels with electrons. The energy position within the gap varies with the charge state due to the Coulomb interaction. Also, the lattice relaxation around the defect depends on the charge state and modiﬁes the energy level. The localized charge qd at the defect is the integral over the change Δρ of the charge density compared to the perfect crystal over a suﬃciently large volume V∞ around the defect ne . (7.61) Δρ(r)d3 r = qd = ǫr V∞ In semiconductors, the charge qd ǫr is an integer multiple of the elementary charge. The defect is said to be in the nth charge state. Each charge state has a certain stable atomic conﬁguration Rn . Each charge state has a ground state and excited states that can each have different stable atomic conﬁgurations. Now, we discuss how the concentration of the various charge states depends on the position of the Fermi level. The overall constraint of global charge neutrality determines the chemical potential of the electron, i.e. the Fermi level in Fermi–Dirac statistics. We use the approximation that the defect concentration is small and their interactions become negligible. As an example, we treat the possible reaction V 0 ⇋ V + + e− , where V 0 denotes a neutral vacancy and V + is a positively charged vacancy, created by the ionization of an electron from the vacancy into the conduction band. The free energy G depends on the numbers n0 of neutral and n+ of positively charged vacancies. The minimum condition is met by dG =
∂G ∂G dn0 + dn+ = 0 . ∂n0 ∂n+
(7.62)
The neutrality constraint is dn0 + dn+ = 0 and therefore the minimum condition reads ∂G ∂G = . ∂n0 ∂n+
(7.63)
7.7 Deep Levels
177
For noninteracting defects and using (4.9) we write
n0 ∂G 0 = Gf (V ) + kT ln (7.64a) ∂n0 N0
+ n+ ∂G ∂G(V + ) ∂G(e− ) = + = GVf + kT ln + μe− , (7.64b) ∂n+ ∂n+ ∂n+ N+ where N0 = N Z0 and N+ = N Z+ are the number of available sites, given by the number N of atomic sites and including possible internal degeneracies Z0 and Z+ , respectively. Gf denotes the free enthalpy of formation of the respective defect, as in (4.3). We have written the free enthalpy of the separated − ) pair V + and e− as the sum G(V + ) + G(e− ). μe− = ∂G(e is (by deﬁnition) ∂n+ the chemical potential of the electron, i.e. the Fermi energy EF of Fermi– Dirac statistics.6 From (7.64a,b) we ﬁnd for the ratio of the concentrations of defects c0 = n0 /N and c+ = n+ /N # "
+ 0 Z+ Et (V 0 ) − EF Z+ GVf − GVf + EF c0 = , (7.65) = exp − exp c+ Z0 kT Z0 kT +
0
where −Et (V 0 ) = GVf − GVf is the negative free enthalpy of ionization of V 0 . We note that c0 can be obtained from (4.9) and EF is determined by the chargeneutrality condition. 7.7.2 Jahn–Teller Effect The lattice relaxation can reduce the symmetry of the defect. Many defects, such as a vacancy, a tetrahedral interstitial or an impurity, occupy initially tetrahedral sites in the zincblende structure. The lattice relaxation reduces the symmetry, e.g. to tetragonal or trigonal, and therefore causes initially degenerate levels to split. Such splitting is called the static Jahn–Teller effect [211,213]. The energy change in terms of the atomic displacement Q can be denoted (using perturbation theory for the simplest, nondegenerate case) as −IQ (I > 0). Including the elastic contribution with a force constant C, the energy of a conﬁguration Q is 1 E = −IQ + CQ2 . 2
(7.66)
The stable conﬁguration Qmin , for which the energy is minimal (Emin ), is therefore given by Qmin =
I C
(7.67a) 2
Emin = −
I . 2C
(7.67b)
6 The chemical potential in a onecomponent system is μ = ∂G/∂n = G/n. In a multicomponent system it is, for the ith component, μi = ∂G/∂ni = G/ni .
178
7 Electronic Defect States
Several equivalent lattice relaxations may exist, e.g. a 3fold minimum for remaining C3v symmetry. The energy barrier between them has a ﬁnite height. Therefore, e.g. at suﬃcient temperature, the defect can switch between different conﬁgurations and eventually again becomes isotropic (dynamic Jahn–Teller effect). The experimental observation depends on the relation between the characteristic time of the experiment and the reorientation time constant of the defect.
7.7.3 NegativeU Center We explain the principle of a socalled negativeU center for the Si vacancy (cf. Fig. 4.1). Coulomb energy and the Jahn–Teller effect compete for the position of the occupancy level for different charge states. U refers to the additional energy upon charging of the defect with an additional electron. The Coulomb repulsion of electrons leads to an increase of the energy, i.e. positive U , which has been calculated to be 0.25 eV for the Si vacancy [214] for all charge states. The occupation level (see Sect. 4.3) E0 (1, 2) (the index 0 indicates effects only due to manyelectron Coulomb interaction), separating the domination of V ++ and V + (Fig. 7.21) is 0.32 eV above the valanceband edge. Therefore, the occupation level E0 (0, 1) is expected to lie at about 0.57 eV above EV .
V0 E0(0,1) E0(1,2)
V V
E(1,2) V0 E(0,2) E(0,1) V
Fig. 7.21. Charge states of the vacancy in silicon. Left: level scheme without lattice relaxation, right: level scheme including the Jahn–Teller eﬀect. For a Fermi level below (above) E(0, 2) the charge state V ++ (V 0 ) is dominant
The Jahn–Teller effect may lead to a splitting of the otherwise 4fold degenerate states of the vacancy. The schematic level diagram for the Jahn– Teller splitting is shown in Fig. 7.22. The V ++ state (A1 is always populated with two electrons) is resonant with the valence band. The T2 state lies in the bandgap. When the Jahn–Teller effect (now on the T2 state) is included, the energies of the different charge states depend on the conﬁguration coordinate (a mostly tetragonal distortion in the case of the Si vacancy).
7.7 Deep Levels
1 EV 0 = E(0, Q) = E(0, Q = 0) − 2IQ + CQ2 2 1 EV + = E(1, Q) = E(1, Q = 0) − IQ + CQ2 2 1 2 EV ++ = E(2, Q) = E(2, Q = 0) + CQ . 2
179
(7.68a) (7.68b) (7.68c)
T2
A1 V
V
V0
V
Fig. 7.22. Jahn–Teller splitting for diﬀerent charge states of the vacancy. A1 and T2 refer to irreducible representations of the Td point symmetry group. A1 is nondegenerate and therefore does not exhibit a Jahn–Teller eﬀect. T2 is triply degenerate. The arrows represent electrons and their spin orientation
For the n = 2 state the T2 gap state is empty and thus no degeneracy and Jahn–Teller term arises. For n = 1 there is a linear Jahn–Teller term. The occupation with two electrons (V 0 ) causes an approximately twice as large Jahn–Teller splitting for the n = 0 state. The force constant is assumed to be independent of the charge state. The energies for the minimum conﬁgurations Qnmin are therefore I2 2C I2 1 E(1, Qmin ) = E(1, Q = 0) − 2C E(2, Q2min ) = E(2, Q = 0) .
E(0, Q0min ) = E(0, Q = 0) − 4
(7.69a) (7.69b) (7.69c)
The Jahn–Teller energy EJT = I 2 /2C lowers the position of the occupancy levels E0 calculated with Coulomb terms only. The occupancy levels including the Jahn–Teller contribution are therefore given as E(1, 2) = E0 (1, 2) − EJT
E(0, 1) = E0 (0, 1) − 3EJT .
(7.70a) (7.70b)
For the vacancy in silicon the Jahn–Teller energy EJT is about 0.19 eV. Thus the E(1, 2) level is lowered from 0.32 eV to 0.13 eV. The E(0,1) occupancy level, however, is reduced from 0.57 eV to 0 eV, i.e. the valenceband
180
7 Electronic Defect States
edge below E(1,2) (see Fig. 7.21). The occupancy level E(0, 2) is in the middle between E(0, 1) and E(1, 2). It lies experimentally between 0.16 eV (Si:In) and 0.065 eV (Si:Ga). The relative concentrations of the three charge states are determined by (7.65) (degeneracy and entropy terms have been neglected)
E(1, 2) − EF c(V ++ ) = exp (7.71a) c(V + ) kT
c(V + ) E(0, 1) − EF . (7.71b) = exp c(V 0 ) kT Therefore, V ++ dominates if EF < E(0, 1) and V 0 dominates for EF > E(1, 2). In the intermediate range E(0, 1) < EF < E(1, 2) we know from (7.71a,b) that V + is dominated by V 0 and V ++ . However, at this point it is not clear whether V ++ or V 0 dominates overall. The ratio of the concentrations of V ++ and V 0 is given by
2 E(1, 2) + E(0, 1) − 2EF E(0, 2) − EF c(V ++ ) = exp . = exp c(V 0 ) kT kT (7.72) The occupancy level E(0, 2) is thus given as E(0, 2) =
1 [E(0, 1) + E(1, 2)] , 2
(7.73)
and is shown in Fig. 7.21. V ++ dominates if EF < E(0, 2) and V 0 dominates for EF > E(0, 2). V + is, for no position of the Fermi level, the dominating charge state of the Si vacancy. We note that for ndoped Si the V − and V −− can also be populated. The population of the V 0 state with an extra electron introduces another Jahn–Teller splitting (Fig. 7.22) that has trigonal symmetry. Generally, the Jahn–Teller effect can make the addition of an electron cause an effectively negative charging energy; in this case the center is termed a negativeU center. 7.7.4 DX Center The DX center is a deep level that was ﬁrst investigated for ndoped (e.g. Sidoped) Alx Ga1−x As. It dominates the transport properties of the alloy for x > 0.22. For smaller Al concentrations and GaAs the DX level lies in the conduction band. DXtype deep levels have also been found for other alloys and dopants, e.g. GaAsP:S. It is experimentally found that the capture process of electrons into the DX center is thermally activated. The capture energy Ec depends on the AlAs mole fraction (Fig. 7.23). The (average) barrier for electron capture has
7.7 Deep Levels
181
a minimum of 0.21 eV for x ≈ 0.35, near the crossover point between direct and indirect bandgap (cf. Fig. 6.13). For lower Al concentrations, the capture barrier increases to 0.4 eV for x = 0.27; for x > 0.35 the capture barrier increases to about 0.3 eV for x around 0.7 [215]. The barrier for thermally releasing carriers from the DX center has been determined to be about 0.43 eV, independent of the Al mole fraction [215].
Capture energy (eV)
0.5 AlxGa1xAs:Si 0.4 0.3 0.2 0.1
0.3
0.4 0.5 0.6 0.7 AlAs mole fraction x
Fig. 7.23. Energy barrier for electron capture Ec at the SiDX center in Alx Ga1−x As for various compositions. Experimental data from [215]
Carriers can be removed from the DX center by optical absorption of photons with energy larger than about 1.2 eV. If carriers are removed by optical excitation at low temperatures the (re)capture is so slow (σ < 10−30 cm2 ) that the carriers remain in the conduction band and cause persistent photoconductivity (PPC). The PPC is only reduced upon increasing the sample temperature. The concentration of the DX center is about the same as the net doping concentration. The properties of the DX center are reviewed in [216,217]. So far, no deﬁnite microscopic model of the DX center has been agreed on. Lang [218] proposed that the DX center involves a donor and an unknown defect (probably a vacancy). It probably involves large lattice relaxation as in the conﬁgurab with tion coordinates model of Fig. 7.24 where the donor binding energy ED respect to the conductionband minimum, the barrier for electron capture Ec , the barrier for electron emission Ee and the optical ionization energy Eo are labeled. The donor binding energy is measured with Hall effect (see Sect. 8.4) at temperatures suﬃcient to overcome the capture and emission barriers, the emission barrier is measured with deep level transient spectroscopy (DLTS). The capture barrier manifests itself in PPC experiments. We note that the DX center is related to the Lconduction band. For small Al mole fraction, the DX level is degenerate with the Γ related conduction band (see Fig. 7.24b).
182
7 Electronic Defect States
Theoretical models and experimental evidence hint at a vacancyinterstitial model for the SiDX center [219]. The donor (Si) is displaced along the 111 direction from the Ga substitution site. The displacement is predicted to be 0.117 nm and the distorted geometry can be viewed as a Ga vacancy and a Si interstitial. The charge state of the (ﬁlled) DX center is proposed to be a twoelectron negativeU state.
E
E
Eopt EC EDX (a)
Ec EbD
EL EDX EC
Ee
q0
qt
q (b)
L
DX
Ec
Ee
q0
qt
q
Fig. 7.24. (a) Schematic conﬁguration coordinate diagram for the DX level with large lattice relaxation. q0 is the conﬁguration of the empty defect, qt is the conﬁgb uration of the ﬁlled defect. The donor binding energy ED , the barrier for electron capture Ec , the barrier for electron emission Ee and the optical ionization energy Eo are labeled. EC denotes the conductionband edge. We note that in AlGaAs the DX level is associated with the L conduction band (see Fig. 6.13). (b) Schematic conﬁguration coordinate diagram for the DX level in Al0.14 Ga0.86 As with the DX level being degenerate with the (Γ related) conduction band
7.7.5 EL2 Defect The EL2 defect is a deep donor in GaAs. It is not related to impurities but occurs for intrinsic material, in particular grown under Asrich conditions. It has similar physical properties to the DX center. The bleaching of absorption due to EL2, i.e. the optical removal of electrons from the defect at low temperatures, is shown in Fig. 7.25. The microscopic model [221] describes the EL2 defect as an arsenic antisite defect, i.e. an arsenic atom on a Ga site, AsGa . In the charged state the arsenic atom is displaced from the lattice position and a complex of a Ga vacancy (symmetry T3d ) and an interstitial As (symmetry C3v ) with 0.14 nm displacement along 111 forms (VGa Asi ). The charged state is ﬁlled with two electrons.
7.7 Deep Levels
183
Absorption coefficient (cm1)
4 GaAs 3
2
1
0 0.8
1.0 1.2 Energy (eV)
1.4
Fig. 7.25. Below bandgap absorption spectrum of GaAs at low temperatures (T = 10 K) when cooled in the dark (solid line). The dashed (dashdotted) line is the absorption after illuminating the sample for 1 min (10 min) with white light, leading to quenching of the EL2related absorption. Adapted from [220]
7.7.6 Semiinsulating Semiconductors Semiconductors with high resistivity (107 –109 Ω cm) are called semiinsulating or ‘si’ for short. Semiinsulating substrates are needed for highspeed devices. The high resistivity should stem from a small freecarrier density at ﬁnite temperature.7 For suﬃciently wide bandgap, the intrinsic carrier concentration is small and such pure material is semiinsulating, e.g. GaAs with ni = 1.47 × 106 cm−3 and 5.05 × 108 Ω cm [222]. Since shallow impurities are hard to avoid, another route is used technologically. Impurities that form deep levels are incorporated in the semiconductor in order to compensate free carriers. For example, a deep acceptor compensates all electrons if NA > ND . b Since the acceptor is deep (EA ≫ kT ), it does not release holes for reasonable temperatures. Examples of suitable impurities for compensation of electrons are Si:Au [223], GaAs:Cr [224] and InP:Fe [225]. A deep donor, e.g. InP:Cr [226], is necessary to compensate ptype conductivity. Figure 7.26a shows the terms of Fe in InP [227,228]. An overview of transition metals in III–V semiconductors can be found in [230]. The electron conﬁguration of neutral Fe atoms is 3d6 4s2 (cf. Table 15.2). The Fe is incorporated on the In site and thus has a Fe3+ state as a neutral acceptor (A0 ). The Fe3+ state has the electron conﬁguration 3d5 . The arrow in Fig. 7.26a 7
Not from a small mobility due to poor crystal quality.
7 Electronic Defect States 1.34
EC T2
1.14
5
0.78
5
InP:Fe E
Electron concentration (cm3)
184
0.25 0
(a)
Fe
3+
Fe
2+
InP:Sn
(b)
InP:Sn
1017 n
10
EV
InP:Sn,Fe
16
0
0.2
0.4 0.6 Depth (μm)
0.8
1.0
Fig. 7.26. (a) Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrow denotes capture of an electron (from the conduction band or a shallow donor) on the deep acceptor. Compare this ﬁgure also with Figs. 9.32 and 10.15. (b) Depth proﬁle of electron concentration in an InP:Sn/InP:Fe,Sn/InP:Sn structure. The change Δn ≈ 4.5 × 1016 cm−3 of electron concentration is due to the compensation by Fe and corresponds to the chemical iron concentration determined by SIMS, [Fe]=4.9 × 1019 cm−3 . Part (b) adapted from [235]
represents the capture of an electron from the conduction band or from a shallow donor. The charge state of the Fe becomes Fe2+ (charged acceptor, A− ) with the electron conﬁguration 3d6 . The cubic crystal ﬁeld (Td symmetry) splits this 5 D Fe state8 into two terms [231] that exhibit further ﬁne structure [228]. The large thermal activation energy of 0.64 eV found in the Hall effect on semiinsulating InP:Fe [225] corresponds to the energy separation of the 5 E level and the conduction band. The maximum electron concentration that can be compensated in this way is limited by the solubility of Fe in InP [232], about 1 × 1017 cm3 . Higher Fe incorporation leads to the formation of Fe (or FeP) precipitates and degrades the crystal quality. Only a fraction of the incorporated Fe may then be electrically active and contribute to the compensation. The maximum electrically active Fe concentration is found to be 5–6×1016 cm−3 [233]. The compensation can be directly visualized via the depth proﬁle of the electron concentration in a nsin structure (Fig. 7.26b). The poor thermal stability of Fe, i.e. high diffusion coeﬃcient, has evoked proposals for more stable dopants such as InP:Ru [234]. 7.7.7 Surface States The investigation of (semiconductor) surfaces is a large ﬁeld with sophisticated methods that allow realspace imaging with atomic resolution by scanning probe microscopy and highly depth resolved electronic studies. The surface represents ﬁrst of all a break in the periodic crystal potential and 8 The notation is 2S+1 J (multiplicity), with S being the total spin and J being the total angular momentum.
(b)
Work function (eV)
7.8 Hydrogen in Semiconductors
185
4.26 (d) =42 meV 4.24
4.22
Height (nm)
(a) 2 (c) 1 0 0
z=1.56nm 100
200 300 Position (nm)
400
Fig. 7.27. Image of (a) topography (Δz = 2.8 nm) and (b) work function (Δφ = 4.21–4.26 eV) of a surface step along [111] on a nGaP(110) surface cleaved in c UHV. Reprinted with permission from [237], 2004 APS. (c) and (d) show the corresponding linescans. Adapted from [237]
thus a defect of the bulk crystal. The unsatisﬁed bonds partly rearrange, e.g. by building dimers, forming a surface reconstruction or remain as dangling bonds. The surface exhibits a surface density of states. Such states can lie in the bandgap and capture electrons, leading to recombination and a depletion layer. In this book, we will not get into details of semiconductor surface physics and refer the reader to [236]. As an example of the formation of electronic states at surface defects we show in Fig. 7.27 the comparison of topography and work function (measured by Kelvin probe force microscopy [237]) at a surface step on a GaP(110) surface that has been prepared by cleaving insitu in ultrahigh vacuum (UHV). The depletiontype band bending of the surface is about 0.4 eV. The further increase of the position of the vacuum level at the step edge shows the presence of trap states in the bandgap causing the conduction band to bend upwards (cf. Sect. 18.2.1). Modeling of the effect shows that the charge density at the surface is 6 × 1011 cm−2 and at the step edge 1.2 × 106 cm−1 .
7.8 Hydrogen in Semiconductors The role of hydrogen in semiconductors was ﬁrst recognized in studies of ZnO [238]. It is now clear that hydrogen plays an important role in the passivation of defects9 . As a ‘small’ atom, it can attach easily to dangling bonds and form an electronpair bond. Thus, surfaces, grain boundaries, dislocations and shallow (donor and acceptor) and deep impurity levels become passivated. A good overview and many details of the physics and technological 9
Just not in ZnO where hydrogen is a shallow doner.
186
7 Electronic Defect States Si
Si/B
0.5 Td
Energy (eV)
0.0 0.5 1.0 AB
1.5 2.0 0.5
(a)
Td
+
H in Si 0 H in Si:B
BM 0.25 0.0 0.25 Coordinate u along (b)
Fig. 7.28. (a) Energy for positions u of the hydrogen atom along the 111 direction for H+ in pure Si (Si atom at u = √ −0.25) and neutral hydrogen (B atom at u = −0.25). u is measured in units of 3a0 . For all positions of the hydrogen atom the positions of the other atoms have been relaxed in the calculation. Data from [246]. (b) Adiabatic potential energy in the (110) plane for hydrogen in Si:B. ‘BM’ denotes the bond minimum site (high valence electron density), C and C’ are equivalent for c pure Si. Reprinted with permission from [246], 1989 APS
use of hydrogen in semiconductors can be found in [239, 240]. The hydrogen must be typically introduced as atomic species into semiconductors, e.g. from a plasma in the vicinity of the surface or by ion irradiation. With regard to silicon it is important to note that the Si–H bond is stronger than the Si–Si bond. Thus a silicon surface under atomic hydrogen exhibits Si–H termination rather than Si–Si dimers [241]. Due to the stronger bond, the hydrogenation leads to an increase of the silicon bandgap, which can be used for surface passivation [243], leading to reduced reverse diode current. The hydrogen concentration in amorphous Si (aSi) can be as high as 50% [242]. Electronic grade aSi contains typically 10–30 atomic % hydrogen and is thus rather a silicon–hydrogen alloy. Hydrogen in crystalline silicon occupies the bondcenter interstitial position (cf. Fig. 3.17b) as shown in Fig. 7.28a. The complexes formed by hydrogen with shallow acceptors and donors have been studied in detail. It is now generally accepted that for acceptors (e.g. boron) in silicon the hydrogen is located close to the bondcenter position of the Si–B pair (BM, bond minimum) as sketched in Fig. 7.29a. The boron atom forms an electronpair bond with three silicon atoms of the tetrahedra, the fourth silicon bonds to the hydrogen atom. The complex therefore no longer acts as an acceptor. The silicon atoms and the acceptor relax their positions. The adiabatic potential energy surface of hydrogen in Si:B is shown in Fig. 7.28b. The hydrogen can sit on four equivalent sites (BM) along the 111 directions of the initial B–Si4 tetrahedron. This reduces the symmetry, e.g. of H–B vibrations [244]. The energetic barrier for the hydrogen orientation has been determined to be
7.8 Hydrogen in Semiconductors
187
(110)
Si
H
H
Si
B
B
(a)
(b)
Fig. 7.29. Schematic model for hydrogen in silicon forming a complex with (a) a shallow acceptor (boron, empty orbital) and (b) a shallow donor (phosphorus, doubleﬁlled orbital)
[001]
(a)
[110]
[110]
(b)
Fig. 7.30. (a) Structure of the V–O complex (A center) in silicon. The black sphere c represents the oxygen atom. Reprinted with permission from [249], 2004 APS. (b) Calculated groundstate structure for the V–O–H2 center in silicon. Oxygen is over the C2 axis, and the two white spheres represent hydrogen. Reprinted with c permission from [247], 2000 APS
0.2 eV theoretically [246] for a hydrogen motion along the path BM–C–BM in Fig. 7.28b. Stress (along [100] and [112]) reduces the symmetry and leads to splitting of the local vibrational modes, now showing axial symmetry [245]. However, this preferential orientation disappears with an activation energy of 0.19 eV, close to the theoretical value. Hydrogen has experimentally been found to also passivate shallow donors. The microscopic conﬁguration is sketched in Fig. 7.29b. The hydrogen atom sits on the Si–AB (antibonding) position and forms an electronpair bond with the silicon atom. The donor, e.g. phosphorus, is left with a doubleﬁlled porbital (lone pair) whose level is in the valence band and thus no longer contributes to conductivity. Molecular hydrogen can passivate the socalled A center in Si, an oxygen–vacancy complex [247]. The atomistic conﬁguration of the V–O–H2 complex is shown in Fig. 7.30. The deep double donor S in Si with a level at 0.3 eV below the conductionband edge can also be passivated by two hydrogen atoms [248].
8 Transport
8.1 Introduction
Charge and heat energy can be transported through the semiconductor in the presence of appropriate (generalized) forces. Such a force can be an electric ﬁeld or a temperature gradient. Both transport phenomena are coupled since electrons can transport energy and charge through the crystal. First, we will treat the charge transport as a consequence of a gradient in the Fermi level, then the heat transport upon a temperature gradient and ﬁnally the coupled system, i.e. the Peltier and Seebeck effects. Practically all important semiconductor devices are based on the transport of charge, such as diode, transistor, photodetector, solar cell and laser. Carriers move in the semiconductor driven by a gradient in the Fermi energy. We distinguish • drift, as a consequence of an electrical ﬁeld E, • diffusion, as a consequence of a concentration gradient ∇n or ∇p. In inhomogeneous semiconductors for which the position of the band edges is a function of position, another force occurs. This will not be treated here, since later (see Chap. 11) it will be included as an additional, internal electrical ﬁeld. Many semiconductor properties, such as the carrier concentration and the bandgap, depend on the temperature. Thus, device properties will also depend on temperature. During operation of a device typically heat is generated, e.g. by Joule heating due to ﬁnite resistivity. This heat leads to an increase of the device temperature that subsequently alters the device performance, mostly for the worse. Ultimately, the device can be destroyed. Thus cooling of the device, in particular of the active area of the device, is essential. Mostly the thermal management of device heating limits the achievable performance (and lifetime) of the device. In highpower devices quite high energy densities can occur, e.g. the facet of a highpower semiconductor laser has to withstand an energy density beyond 10 MW cm−2 .
190
8 Transport
8.2 Conductivity Under the inﬂuence of an electric ﬁeld the electrons accelerate according to (cf. (6.35)) F = m∗
dk dv = = qE = −eE . dt dt
(8.1)
In the following, q denotes a general charge, while e is the (positive) elementary charge. After the time δt the k vector of all conduction electrons (and the center of the Fermi sphere) has been shifted by δk δk = −eE δt/ .
(8.2)
In the absence of scattering processes this goes on further (similar to an electron in vacuum). This regime is called ballistic transport. In a (periodic) band structure, the electron will perform a closed cycle as indicated in Fig. 8.1. Such motion is called a Bloch oscillation. However, in a bulk crystal the period T of such an oscillation eET / = 2π/a0 is of the order of 10−10 s for E = 104 V/cm. This time is much longer than a typical scattering time of 10−14 s. Thus, in bulk material the Bloch electron cannot reach the zone boundary. However, in artiﬁcial superlattices (see Chap. 11) with larger periodicity (≈ 10 nm), high electric ﬁelds (≈ E = 106 V/cm) and high quality (reduced collision time) such motion is possible. We note that in the absence of scattering, electrons also perform a periodic oscillation in a magnetic ﬁeld (cyclotron motion).
/a
/a
Fig. 8.1. Schematic representation of a Bloch oscillation
In a real semiconductor, at ﬁnite temperatures, impurities, phonons and defects (ﬁnally also the surface) will contribute to scattering. In the relaxationtime approximation it is assumed that the probability for a scattering event, similar to friction, is proportional to the (average) carrier velocity. The average relaxation time τ is introduced via an additional term v˙ = −v/τ that sums up all scattering events. Thus, the maximum velocity that can be reached in a static electric ﬁeld is given by (steadystate velocity) v = −eEτ /m∗ .
(8.3)
8.3 LowField Transport
191
The current density per unit area is then linear in the ﬁeld, i.e. fulﬁlls Ohm’s law j = nqv = ne2 Eτ /m∗ = σE .
(8.4)
The conductivity σ in the relaxationtime approximation is given by σ=
ne2 τ 1 = . ρ m∗
(8.5)
The speciﬁc resistivity is the inverse of the conductivity. Metals have a high conductivity, e.g. for Cu at room temperature σ = 5.88 × 105 Ω−1 cm−1 . At low temperatures (4 K) the conductivity is even a factor of 105 higher. The mean free path is then 3 mm (and thus susceptible to the sample geometry) while at room temperature the mean free path is only 30 nm. In semiconductors, the carrier concentration depends strongly on the temperature. At zero temperature the conductivity is zero. Also, the scattering processes and thus the relaxation time constant exhibit a temperature dependence.
8.3 LowField Transport First we consider small electric ﬁelds. The real meaning of this will only become clear in Sect. 8.5 on highﬁeld transport. In the lowﬁeld regime the velocity is proportional to the electric ﬁeld. 8.3.1 Mobility The mobility is deﬁned (scalar terms) as μ=
v . E
(8.6)
By deﬁnition, it is a negative number for electrons and positive for holes. However, the numerical value is usually given as a positive number for both carrier types. In an intrinsic semiconductor the mobility is determined by scattering with phonons. Further scattering is introduced by impurities, defects or alloy disorder. The conductivity is (8.4) σ = qnμ
(8.7)
for each carrier type. The mobility in the relaxation time approximation is μ=
qτ . m∗
(8.8)
192
8 Transport
Thus, in the presence of both electrons and holes, σ = −enμn + epμp ,
(8.9)
where μn and μp are the mobilities for electrons and holes, respectively. In the relaxationtime approximation these are given by μn = −eτn /m∗e and μp = eτp /m∗p . As a unit, usually cm2 /V s is used. While Cu at room temperature has a mobility of 35 cm2 /V s, semiconductors can have much higher values. In twodimensional electron gases (see Chap. 11), the mobility can reach several 107 cm2 /V s at low temperature (Fig. 11.25). In bulk semiconductors with small bandgap, a high electron mobility is caused by its small effective mass. Some typical values are given in Table 8.1. Table 8.1. Mobilities (in cm2 /V s) for electrons and holes at room temperature for various semiconductors
Si Ge GaAs GaN InSb InAs InP ZnO
μn
μp
1300 4500 8800 300 77 000 33 000 4600 230
500 3500 400 180 750 460 150 8
8.3.2 Microscopic Scattering Processes The relaxation time constant summarizes all scattering mechanisms. If the relaxation times τi of various processes are independent, the Matthiesen rule can be used to obtain the mobility (μi = qτi /m∗ ) 1 1 . = μ μi i
(8.10)
The different scattering mechanisms have quite different temperature dependences such that the mobility is a rather complicated function of temperature.
8.3 LowField Transport
193
8.3.3 Ionized Impurity Scattering Theoretically, this problem is treated similar to Rutherford scattering. A screened Coulomb potential is assumed, as the scattering potential
Ze 1 r exp − V (r) = − , (8.11) 4πǫ0 ǫr r LD where LD is the screening length. The problem has been treated classically by Conwell and Weisskopf [250] and quantum mechanically by Brooks [251] and Herring. An expression for the mobility that encompasses the Conwell– Weisskopf and Brooks–Herring results is derived in [252]. Further details can be found in [253, 254]. For the mobility it is found that μion.imp. =
1 27/2 (4πǫ0 ǫr )2 (kT )3/2 √ . 2 ) − β 2 (1 + β 2 ) 3/2 2 3 ∗ N ln(1 + β π Z e m ion
(8.12)
8.3.4 Deformation Potential Scattering Acoustic phonons with small wavevector, i.e. a wavelength large compared to the unit cell, can have TA or LA character. The TA phonons represent a shear wave (with zero divergence), the LA phonons are a compression wave (with zero rotation). The LA phonon is a plane wave of displacement δR parallel to the kvector q, δR = A sin (q · R − ωt) .
(8.13)
The strain tensor is given by ǫij =
1 (qi Aj + qj Ai ) cos (q · R − ωt) . 2
(8.14)
It has a diagonal form ǫij = qi Aj for q and ω → 0. Therefore, the LA phonon creates an oscillatory volume dilatation (and compression) with amplitude q · A. This volume modulation affects the position of the band edges (Sect. 6.14). For the conductionband edge the energy change is related to the volume change by the hydrostatic deformation potential Eac.def. = V ∂EC /∂V . Since the modulation is small compared to the energy of the charge carriers, it is mostly an elastic scattering process. The Hamilton operator for the LA scattering is ˆ = Eac.def. (q · A) . H
(8.15)
The size of the LA amplitude is given by the number of phonons in the mode that is given by the Bose–Einstein distribution, Nph (ω) = ω −1 exp kT . The mobility due to acoustic deformation potential scattering is found to be
194
8 Transport
μac.def. =
√
3/2 1 2 2πe4 cl , 2 kT 3m∗ 5/2 Eac.def.
(8.16)
where cl = ρcLA s , ρ being the density and cs being the sound velocity. The acoustical deformation potential scattering is therefore important at high temperatures. It is dominating in nonpolar semiconductors (Ge, Si) at high temperatures (typically at and above room temperature). 8.3.5 Piezoelectric Potential Scattering In piezoelectric crystals, i.e. crystals that show an electric polarization upon strain, certain acoustic phonons lead to piezoelectric ﬁelds. In GaAs this is the case for shear waves. In strongly ionic crystals, e.g. II–VI semiconductors, the piezoelectric scattering can be stronger than the deformation potential scattering. The mobility due to piezoelectric potential scattering is μpz.el. with K =
e2p /cl ǫ0 ǫr +e2p /cl ,
√
1/2 1 16 2π ǫ0 ǫr , = 3 m∗ 3/2 eK 2 kT
(8.17)
ep being the piezoelectric coeﬃcient.
8.3.6 Polar Optical Scattering LO phonons are connected with an electric ﬁeld antiparallel to the displacement (5.45). In the scattering mechanism the absorbed or emitted phonon energy ω0 is comparable to the thermal energy of the carriers. Therefore, the scattering is inelastic and the relaxationtime approximation does not work. The general transport theory is complicated. If the temperature is low compared to the Debye temperature, T ≪ ΘD
ΘD e , (8.18) exp μpol.opt. = 2m∗ αω0 T , 1 1 1 m∗ c2 is the dimensionless polar constant. − where α = 137 2kΘD ǫ(∞) ǫ(0) 8.3.7 Temperature Dependence The sum of all scattering processes leads to a fairly complicated temperature dependence of the mobility μ(T ). In covalent semiconductors (Si, Ge) the most important processes are the ionized impurity scattering (μ ∝ T 3/2 ) at low temperatures and the deformation potential scattering (μ ∝ T −3/2 ) at high temperatures (Fig. 8.2a). In polar crystals (e.g. GaAs) at high temperatures the polar optical scattering is dominant (Fig. 8.2b).
8.3 LowField Transport
(a)
195
(b)
Fig. 8.2. Temperature dependence of the electron mobility in ndoped (a) Ge (for various doping levels from ND ≈ 1018 for sample A to 1013 cm−3 for sample F in steps of a factor of ten) and (b) GaAs (ND ≈ 5 × 1013 cm−3 , NA ≈ 2 × 1013 cm−3 ). Part (a) adapted from [202], part (b) adapted from [255]
(a)
(b)
Fig. 8.3. Temperature dependence of the electron mobility in ntype (a) bulk ZnO and (b) ZnO thin ﬁlm. In the latter, grainboundary scattering is limiting the mobility
In Fig. 8.3 the electron mobility of bulk and thinﬁlm ZnO is compared. Since ZnO is polar the mobility at room temperature is limited by polar optical phonon scattering. In the thin ﬁlm, grainboundary scattering [256] additionally occurs. Since the carrier concentration increases with increasing temperature and the mobility decreases, the conductivity has a maximum, typically around 70 K (see Fig. 8.4). At very high temperature, when intrinsic conduction starts, σ shows a strong increase due to the increase in n. The mobility decreases with increasing dopant concentration as shown in Figs. 8.2a and 8.5. Thus, for bulk material high carrier density and high mobility are contrary targets. A solution will be provided with the concept of modulation doping where the dopants and the (twodimensional) carrier gas will be spatially separated (see Sect. 11.5.3).
196
8 Transport Temperature (K)
Temperature (K) 10
300 78
33.3
18
20.4
14.3
10
10
300
3
78
33.3
20.4
14.3
10
ND~1018 cm3 A
Ge:As
B
14
10
13
10
12
B
Conductivity ( 1 cm 1 )
Electron concentration (cm 3)
C
15
10
3
102
1016
10
18
ND~10 cm
A
1017
101
Ge:As
D
100 E
101
F
C D
13
ND~10 cm
3
102 E 13
10
(a)
ND~10 cm
11
0
20
40 60 1000/T (1/K)
80
3
F
10
100
(b)
3
0
20
40 60 1000/T (1/K)
80
100
Fig. 8.4. (a) Carrier concentration and (b) conductivity of ntype Ge as a function of temperature. The doping level varies from ND ≈ 1013 to 1018 (samples A–F as in Fig. 8.2a where the mobility of the samples is shown). Adapted from [202]
Fig. 8.5. Roomtemperature mobility as a function of dopant concentration for Ge, Si, and GaAs. Solid lines (dashed lines) represent the electron (hole) mobility. Adapted from [183]
8.4 Hall Eﬀect
B
197
z y
v F
B w
x I
VH Fig. 8.6. Scheme of the Halleﬀect geometry. The movement of one electron in the longitudinal electric current I is shown schematically. The coordinate system (x, y, z) and the directions of the magnetic ﬁeld B, the drift velocity of an electron v and the resulting Lorentz force F are given. The transverse ﬁeld Ey is given by VH /w
8.4 Hall Effect An electrical current along the x (longitudinal) direction in a perpendicular magnetic ﬁeld B = (0, 0, B) along z induces an electric ﬁeld Ey along the transverse (y) direction. The charge accumulation is due to the Lorentz force. The related transverse voltage is called the Hall voltage and the resistivity ρxy = Ey /jx the Hall resistivity [257]. For the Hall geometry see Fig. 8.6. For thinﬁlm samples typically the vanderPauw geometry (Fig. 8.7) and method is used [258–260]. The steadystate equation of motion is v (8.19) m∗ = q (E + v × B) . τ We note that this equation of motion is also valid for holes, given the convention of Sect. 6.13.1, i.e. positive charge. With the cyclotron frequency ωc = qB/m∗ the conductivity tensor is (j = σE = qnv) ⎛ ⎞ σxx σxy 0 σ = ⎝ σyx σyy 0 ⎠ (8.20a) 0 0 σzz 1 1 σxx = σyy = σ0 (8.20b) = σ0 2 2 1 + ωc τ 1 + μ2 B 2 ωc τ μB (8.20c) = σ0 σxy = −σyx = σ0 2 2 1 + ωc τ 1 + μ2 B 2 q 2 nτ = qnμ . (8.20d) σzz = σ0 = m∗ If only one type of carrier (charge q, density n) is considered, the condition jy = 0 leads to Ey = μBEx and jx = σ0 Ex . The Hall coeﬃcient RH = Ey /(jx B) is therefore given by
198
8 Transport
(a)
(b)
(c)
(d)
(e)
Fig. 8.7. (a–d) Geometry for vanderPauw Hall measurements. (a) Best geometry (cloverleaf), (b) acceptable square geometry with small contacts on the corners, (c,d) not recommended geometries with contacts on the edge centers or inside the square, respectively. (e) Current distribution, as visualized by lockin thermography [190], in epitaxial ZnO layer on sapphire with Hall geometry as in part (b). Grey dashed line indicates the outline of the 10 × 10 mm2 substrate, grey areas indicate gold ohmic contacts
RH =
1 . qn
(8.21)
If both types of carriers are present, again the condition jy = 0 yields the Hall constant RH =
−nμ2e (1 + μ2h B 2 ) + pμ2h (1 + μ2e B 2 ) 1 . 2 2 2 e n μe (1 + μh B 2 ) − 2npμe μh (1 + μe μh B 2 ) + p2 μ2h (1 + μ2e B 2 ) (8.22)
Under the assumption of small magnetic ﬁelds,1 i.e. μB ≪ 1, the Hall coeﬃcient is −nμ2e + pμ2h np(−n + p)μ2e μ2h (μe − μh )2 2 1 RH = + B + . . . . (8.23) e (−nμe + pμh )2 (−nμe + pμh )4 For small magnetic ﬁeld this can be written as RH =
1 −nβ 2 + p , e (−nβ + p)2
(8.24)
with β = μe /μh . For large magnetic ﬁelds, i.e. μB ≫ 1, the Hall coeﬃcient is given by RH = 1
1 −n + p . e (n + p)2
We note that for a mobility of 104 cm2 /V s, μ−1 is a ﬁeld of B = 1 T.
(8.25)
8.4 Hall Eﬀect
199
In Fig. 8.8, the absolute value of the Hall coeﬃcient for InSb samples with different doping concentrations is shown. The pdoped samples exhibit a reverse of the sign of the Hall coeﬃcient upon increase of temperature when intrinsic electrons contribute to the conductivity. The zero in RH occurs for n = pμ2h /μ2e . For high temperatures, the Hall coeﬃcient for n and pdoped samples is dominated by the electrons that have much higher mobility (Table 8.1).
104 8 6
4000
InSb 2000
4 1000 800 600
F E
200
1.310
Hall coefficient RH (cm3 C1)
1.01017
400
Conductivity (1cm1)
2
A
103 8 6
E
3
NAND (cm )
16
100 80 60 40
D
2.01017
20
C
10 8 6
B
6.010
16
2.210
16
4
B
2
C
102 8 6
F D
4 2
4 2 1 1
(a)
A 2
4.010
3 4 5 6 7 1/Temperature (1000/K)
8
10 8 6
15
4 1
9
(b)
2
3
4 5 6 1/Temperature (1000/K)
7
8
9
Fig. 8.8. (a) Conductivity and (b) absolute value of the Hall coeﬃcient vs. inverse temperature for four pdoped (A–D) and two ndoped (E,F) InSb samples. The doping levels are given in (a). Adapted from [261]
In the derivation of the Hall coeﬃcient we had assumed that all carriers involved in the transport have the same properties, in particular that they are subject to the same scattering time. This assumption is generally not the case and we need to operate with the ensemble average of the discussed quantities. The ensemble average of an energydependent quantity ζ(E) over the (electron) distribution function f (E) is denoted as ζ and is given as2 ζ(E)f (E)dE ζ = . (8.26) f (E)dE
In particular τ 2 is now different from τ 2 . Considering the equation j = σE for the ensemble averaged current densities we ﬁnd (for one type 2
For this consideration it is assumed that the energy dependence is the decisive one. Generally, averaging may have to be performed over other degrees of freedom as well, such as the spin or, in the case of anisotropic bands, the orbital direction.
200
8 Transport
of carrier, cf. (8.21)) RH =
1 rH , qn
(8.27)
with the socalled Hall factor rH given by γ α2 + ωc2 γ 2 . τ α= 1 + ωc2 τ 2 . τ2 γ= . 1 + ωc2 τ 2
rH =
(8.28)
The Hall factor depends on the scattering mechanisms and is of the order of 1. For large magnetic ﬁelds the Hall factor approaches 1. For small magnetic ﬁelds we have RH =
1 τ 2 . qn τ 2
(8.29)
The mobility calculated from (cf. (8.20d)) σ0 RH is called the Hall mobility μH and is related to the mobility via μH = rH μ .
(8.30)
8.5 HighField Transport 8.5.1 DriftSaturation Velocity In the case of small electric ﬁelds the scattering events are elastic. The drift velocity is linearly proportional to the electric ﬁeld. The average thermal energy is close to its thermal value 3kT /2. The scattering eﬃciency, however, is reduced already at moderate ﬁelds. Then, the electron temperature becomes larger than the lattice temperature. If the carrier energy is large enough it can transfer energy to the lattice by the emission of an optical phonon. This mechanism is very eﬃcient and limits the maximum drift velocity. Such behavior is nonohmic. The limiting value for the drift velocity is termed the driftsaturation velocity. It is given by [262] vs =
8 3π
1/2
ωLO m∗
1/2
.
(8.31)
This relation can be obtained from an energybalance consideration. The energy gain per unit time in the electric ﬁeld is equal to the energy loss by the emission of an optical phonon.
8.5 HighField Transport 10
201
8
Electron drift velocity (107 cm/s)
ZnO
Drift velocity (cm/s)
GaAs 107
Ge 10
6
electrons holes
Si 5
10 2 10
(a)
103
104 105 Electric field (V/cm)
3.0 GaN
InGaAs
(b)
GaAs
1.0 Si 0 0
106
InP
2.0
100 200 Electric field (kV/cm)
300
Fig. 8.9. Drift velocity at room temperature as a function of applied electric ﬁeld for (a) highpurity Si, Ge, and GaAs on a doublelogarithmic plot and (b) on linear plots for Si [263], Ge [264], GaAs [222], InP [265], InGaAs [266], GaN and ZnO [267]
ωLO , (8.32) τ where τ is the typical relaxation time constant for LO phonon emission. Together with (8.3) we ﬁnd (8.32) except for the prefactor, which is close to 1. The exact prefactor results from a more exact quantummechanical treatment. For Ge the driftsaturation velocity at room temperature is 6 × 106 cm/s, for Si it is 1 × 107 cm/s (Fig. 8.9a). In GaAs there is a maximum drift velocity of about 2 × 107 cm/s and following a reduction in velocity with increasing ﬁeld (1.2 × 107 cm/s at 10 kV/cm, 0.6 × 107 cm/s at 200 kV/cm) as shown in Fig. 8.9a. This regime is called negative differential resistivity (NDR). This phenomenon can be used in oscillators, e.g. the Gunn diode. The effect occurs in a multivalley band structure (see Fig. 8.10), e.g. in GaAs or InP, when the carrier energy is high enough to scatter (Fig. 8.10c,d) from the Γ minimum (small mass, m∗ =0.065 m0 , high mobility μ ≈ 8000 cm2 /V s) into the L minimum (large mass, m∗ =1.2 m0 , low mobility μ ≈ 100 cm2 /V s). The temperature dependence of the saturation velocity is shown in Fig. 8.11. With increasing temperature the saturation velocity decreases since the coupling with the lattice becomes stronger. qv · E =
8.5.2 Velocity Overshoot When the electric ﬁeld is switched on, the carriers are at ﬁrst in the Γ minimum (Fig. 8.10a). Only after a few scattering processes are they scattered into the L minimum. This means that in the ﬁrst moments transport occurs with the higher mobility of the lowest minimum (Fig. 8.10e). The velocity is then larger than the (steadystate) saturation velocity in a dc ﬁeld. This phenomenon is called velocity overshoot and is a purely dynamic effect (Fig. 8.12) on a subps timescale.
202
8 Transport E
(a)
E
L
k
(b)
E
(c)
L
k
E
L
k
(d)
E
L
k
(e)
L
k
Fig. 8.10. Chargecarrier distribution in a multivalley band structure (e.g. GaAs, InP) for (a) zero, (b) small (E < Ea ), (c) intermediate and (d) large (E > Eb ) ﬁeld strength. The situation shown in (e) is reached temporarily during velocity overshoot (see also Fig. 8.12)
Fig. 8.11. Temperature dependence of the saturation velocity for Si (following vs = vs0 (1 + 0.8 exp(T /600 K))−1 with vs0 = 2.4 × 107 cm/s from [263]) and GaAs [222, 268, 269]
8.5.3 Impact Ionization If the energy gain in the ﬁeld is large enough to generate an electron–hole pair, the phenomenon of impact ionization occurs. The energy is ∝ v 2 . Momentum and energy conservation apply. Thus, at small energies (close to the threshold for impact ionization) the vectors are short and collinear to fulﬁll momentum
8.5 HighField Transport
In0.53Ga0.47As
8
Electron velocity (107 cm/s)
203
6
4
InP
2 GaAs 0
0
0.2
0.4 Time (ps)
0.6
0.8
Fig. 8.12. Time dependence of the electron velocity at room temperature upon a steplike electric ﬁeld (40 kV/cm) for GaAs (dashdotted line), InP (dashed line) and In0.53 Ga0.47 As (solid line)
conservation. At higher energy, larger angles between the velocity vectors of the impact partners can also occur. If the process is started by an electron (Fig. 8.13a) the threshold energy is given by Eethr =
2me + mhh Eg . me + mhh
(8.33)
The threshold for impact ionization triggered by a so hole (shown schematically in Fig. 8.13b) is mso (1 − Δ0 /Eg ) thr Eg . (8.34) Eh = 1 + 2mhh + me − mso The generation rate G of electron–hole pairs during impact ionization is given by G = αn nvn + αp pvp ,
(8.35)
where αn is the electron ionization coeﬃcient. It describes the generation of electron–hole pairs per incoming electron per unit length. αp denotes the hole ionization coeﬃcient. The coeﬃcients depend strongly on the applied electric ﬁeld. They are shown in Fig. 8.14. They also depend on the crystallographic direction. The ionization rate increases with decreasing bandgap.
204
8 Transport e
E
E vi
e
Eg Eg
lh
lh
hh
hh
vi so
(a)
so
k (b)
k
Fig. 8.13. Electron and hole transitions for impact ionization close to the threshold energy. Ionization is triggered by (a) an electron and (b) a splitoﬀ hole of velocity vi
Fig. 8.14. Impact ionization rates for electrons and holes as a function of the inverse electric ﬁeld for Si, Ge, GaAs and some other semiconductors at 300 K. c Reprinted with permission from [183], 1981 Wiley
8.7 Diﬀusion
205
8.6 HighFrequency Transport The above consideration pertained to dc (or slowly varying) ﬁelds. Now, we consider an ac ﬁeld. It accelerates the carriers but at the same time the dissipative force in the relaxationtime approximation is present, i.e. m∗ v˙ = −eE − m∗
v . τ
(8.36)
For a harmonic ﬁeld E ∝ exp(−iωt) the complex conductivity (j = σE = nqv) is σ=
ne2 τ ne2 1 i = , ∗ ∗ m 1 − iωτ m ω + iγ
(8.37)
with γ = 1/τ being the damping constant. Splitting into real and imaginary parts yields
ne2 τ 1 ωτ +i σ= . (8.38) m∗ 1 + ω2 τ 2 1 + ω2 τ 2 For small frequencies (ω → 0) the dc conductivity from (8.5) is recovered, i.e. σ = ne2 τ /m∗ . For high frequencies (ωτ ≫ 1)
1 ne2 τ 1 +i σ= . (8.39) m∗ ω2 τ 2 ωτ
8.7 Diffusion A gradient of a particle concentration n leads to a particle current proportional to −∇n. This diffusion law (Fick’s law) corresponds microscopically to a random walk. The gradients of the semiconductor carrier densities ∇n or ∇p thus lead to electron and hole currents, respectively: jn = eDn ∇n jp = −eDp ∇p .
(8.40a) (8.40b)
The coeﬃcients Dn and Dp are called the electron and hole diffusion coefﬁcient, respectively. Thus the total electron and hole currents in the presence of an electric ﬁeld E and diffusion are jn = −eμn nE + eDn ∇n jp = eμp pE − eDp ∇p .
(8.41a) (8.41b)
This relation can also be deduced more generally from the gradient of the Fermi level as
206
8 Transport
jn = −eμn nE − nμn ∇EF jp = eμp pE − pμp ∇EF .
(8.42a) (8.42b)
Using (7.8) and (7.9) for the concentrations (valid also in the case of degeneracy) and using dFj (x)/dx = Fj−1 (x) we obtain jn = −eμn nE − kT μn jp = eμp pE − kT μp
F1/2 (η) ∇n F−1/2 (η)
F1/2 (ζ) ∇p , F−1/2 (ζ)
(8.43a) (8.43b)
with η = (EF − EC )/kT and ζ = −(EF − EV )/kT . If the prefactor of the density gradient is identiﬁed as the diffusion coeﬃcient we ﬁnd the socalled ‘Einstein relations’: Dn = − Dp =
F1/2 (η) kT μn e F−1/2 (η)
F1/2 (ζ) kT μp . e F−1/2 (ζ)
(8.44a) (8.44b)
In the case of nondegeneracy, i.e. when the Fermi level is within the bandgap and not closer than about 4kT to the band edges, the equation simpliﬁes to D = kT q μ, i.e. kT μn e kT μp . Dp = e
Dn = −
(8.45a) (8.45b)
In this case, (8.41a,b) read jn = −eμn nE − kT μn ∇n jp = eμp pE − kT μp ∇p .
(8.46a) (8.46b)
We recall that both diffusion coeﬃcients are positive numbers, since μn is negative. Generally, the diffusion coeﬃcient depends on the density. A Taylor series of the Fermi integral yields
2 n n kT −3 μn 1 + 0.35355 Dn = − − 9.9 × 10 + . . . . (8.47) e NC NC
8.8 Continuity Equation The balance equation for the charge is called the continuity equation. The temporal change of the charge in a volume element is given by the divergence
8.9 Heat Conduction
207
of the current and any source (generation rate G), e.g. an external excitation, or drain (recombination rate U ). Details about recombination mechanisms are discussed in Chap. 10. Thus, we have ∂n = Gn − Un − ∂t ∂p = Gp − Up − ∂t
1 1 ∇ · jn = Gn − Un + ∇ · jn q e 1 ∇ · jp . e
(8.48a) (8.48b)
In the case of nondegeneracy we ﬁnd, using (8.41ab) ∂n = Gn − Un − μn n∇ · E − μn E∇n + Dn Δn ∂t ∂p = Gp − Up − μp p∇ · E − μp E∇p + Dp Δp . ∂t
(8.49a) (8.49b)
In the case of zero electric ﬁeld these read ∂n = Gn − Un + Dn Δn ∂t ∂p = Gp − Up + Dp Δp , ∂t
(8.50a) (8.50b)
and if the stationary case also applies: Dn Δn = −Gn + Un
Dp Δp = −Gp + Up .
(8.51a) (8.51b)
8.9 Heat Conduction We consider here the heat transport [270] due to a temperature gradient. The ˆ , is proporheat ﬂow q, i.e. energy per unit area per time in the direction q tional to the local gradient of temperature. The proportionality constant κ is called the heat conductivity, q = −κ∇T .
(8.52)
In crystals, the heat conductivity can depend on the direction and thus κ is generally a tensor of rank 2. In the following, κ will be considered as a scalar quantity. The quite generally valid Wiedemann–Franz law connects the thermal and electrical conductivities 2 π2 k κ= Tσ . (8.53) 3 e
208
8 Transport
The balance (continuity) equation for the heat energy Q is ∇·q=−
∂T ∂Q = −ρC +A, ∂t ∂t
(8.54)
where ρ denotes the density of the solid and C the heat capacity. A denotes a source or drain of heat, e.g. an external excitation. Combining (8.52) and (8.54), we obtain the equation for heat conductivity ΔT =
ρC ∂T A − , κ ∂t κ
(8.55)
which simply reads ΔT = 0 for a stationary situation without sources. The random mixture of various isotopes in natural elements represents a perturbation of the perfectly periodic lattice. Since the mass of the nuclei varies, in particular lattice vibrations will be perturbed. Thus we expect an effect on the heat conductivity. In Fig. 8.15, the thermal conductivity of crystals from natural Ge and enriched 74 Ge are compared [272], the latter having, as expected, the higher heat conductivity, i.e. less scattering. The thermal conductivity of isotopically pure 28 Si thin ﬁlms has been measured to be 60% greater than natural silicon at room temperature and at least 40% greater at 100◦ C, a typical chip operating temperature [273, 274].
100 3
T
50
74
enriched Ge
(W cm1 K1)
20 10 5
natural Ge
2 1 0.5 0.2 1
2
5
10 20 50 100 200 Temperature (K)
500
Fig. 8.15. Thermal conductivity of Ge vs. temperature. The enriched Ge consists of 96% 74 Ge while the natural isotope mix is 20% 70 Ge, 27% 72 Ge, 8% 73 Ge, 27% 74 Ge and 8% 76 Ge. The dashed line shows the κ ∝ T 3 dependence at low temperatures (Debye’s law). Adapted from [272]
8.10 Coupled Heat and Charge Transport
209
8.10 Coupled Heat and Charge Transport The standard effect of coupled charge and heat transport is that a current heats its conductor via Joule heating. However, more intricate use of thermoelectric effects can also be employed to cool certain areas of a device. For further details see [271]. For the analysis of coupled charge and heat transport we ﬁrst sum the ˆ = E + ∇EF /e. electric ﬁeld and the concentration gradient to a new ﬁeld E Then, the heat ﬂow and charge current are ˆ + L∇T j = σE ˆ + N ∇T , q = ME
(8.56) (8.57)
ˆ and ∇T are the stimulators for the currents. From the experimental where E point of view there is interest to express the equations in j and ∇T since these quantities are measurable. With new coeﬃcients they read ˆ = ρj + S∇T E
(8.58)
q = Πj − κ∇T ,
(8.59)
where ρ, S and Π are the speciﬁc resistance, thermoelectric power and Peltier coeﬃcient (transported energy per unit charge), respectively. The relations with the coeﬃcients σ, L, M , and N are given by ρ=
1 σ
(8.60a)
L σ M Π= σ ML −N . κ= σ S=−
(8.60b) (8.60c) (8.60d)
8.10.1 Seebeck Effect Assume a semiconductor with a temperature gradient and in an open circuit, ˆ = S∇T will arise. This effect is called the thermoi.e. j = 0. Then a ﬁeld E electric or Seebeck effect. The voltage can be measured and used to determine the temperature at one end if the temperature at the other end is known. Electrons and holes have different sign of the thermoelectric coeﬃcient (see Fig. 8.16). A famous relation from irreversible thermodynamics connects it to the Peltier coeﬃcient via S=
Π . T
(8.61)
210
8 Transport 0.6
Si
Thermoelectric force (V)
0.4 0.2 ptype 0 ntype 0.2 intrinsic
0.4 0.6 0.8 200
300
400
500 600 700 Temperature (K)
800
900 1000
Fig. 8.16. Thermoelectric force Π of n and psilicon as a function of temperature. Adapted from [275]
With the Seebeck effect the conductivity type of a semiconductor can be determined. If the cold substrate is grounded, the sign of the voltage at a hot solder tip pressed (carefully) on the surface of the semiconductor yields the conductivity type, ntype (ptype) for a negative (positive) voltage. However, the semiconductor should not be heated so strongly that intrinsic conduction arises. 8.10.2 Peltier Effect In a semiconductor with a temperature gradient a current ﬂow will be allowed now (short circuit). The current leads via the charge transport also to a heat (or energy) transport. This effect is called the Peltier effect. The Peltier coeﬃcient is negative (positive) for electrons (holes). The total amount of energy P that is transported consists of the generation term and the loss due to transport: ˆ −∇·q. P =j·E
(8.62)
With (8.58) and (8.59) we ﬁnd P =
j·j + Sj · ∇T − Π∇ · q + κΔT . σ
(8.63)
The ﬁrst term is Joule heating, the second term is Thomson heating. The third exists only when carriers are generated or when they recombine. The fourth term is the heat conduction. In the Thomson term Sj · ∇T heat is
8.10 Coupled Heat and Charge Transport
211
generated in an ntype semiconductor if j and ∇T are in the same direction. This means that electrons that move from the hotter to the colder part transfer energy to the lattice. The effect can be used to construct a thermoelectric cooler, as shown in Fig. 8.17, that generates a temperature difference due to a current ﬂow. For optimal performance σ should be large to prevent excess Joule heating and κ should be small such that the generated temperature difference is not rapidly equalized.
j heat sink
ntype T
heat sink
ptype j
Fig. 8.17. Schematic Peltier cooler. The heat sinks (grey) and the cold junction (black ) on the right are metals that make ohmic contacts with the semiconductors. The current ﬂow is such that electrons move through the ntype semiconductor from right to left
9 Optical Properties
The interaction of semiconductors with light is of decisive importance for photonic and optoelectronic devices as well as for the characterization of semiconductor properties.
9.1 Spectral Regions and Overview When light hits a semiconductor ﬁrst reﬂection, transmission and absorption are considered, as for any dielectric material. The response of the semiconductor largely depends on the photon energy (or wavelength) of the light. In Table 9.1 an overview of the electromagnetic spectrum in the optical range is shown. The energy and wavelength of a photon are related by E = hν = hc/λ, i.e. E =
1240 eV nm λ
(9.1)
Table 9.1. Spectral ranges with relevance to semiconductor optical properties Range deep ultraviolet ultraviolet visible near infrared midinfrared far infrared THz region
DUV UV VIS NIR MIR FIR THz
wavelengths
energies
< 250 nm 250–400 nm 400–800 nm 800 nm–2 µm 2–20 µm 20–80 µm > 80 µm
> 5 eV 3–5 eV 1.6–3 eV 0.6–1.6 eV 60 meV–0.6 eV 1.6–60 meV < 1.6 meV
In Fig. 9.1 a schematic absorption spectrum of a semiconductor is depicted. The transition of electrons from the valence to the conduction band is at the bandgap energy. The bandgaps of Si, Ge, GaAs, InP, InAs, InSb are in the IR, those of AlAs, GaP, AlP, InN in the VIS, those of GaN and ZnO in the UV, MgO and AlN are in the deep UV. The Coulomb correlation of
214
9 Optical Properties
Fig. 9.1. Schematic absorption spectrum of a typical semiconductor. With permisc sion from [278], 1989 PrenticeHall
electrons and holes leads to the formation of excitons that leads to absorption below the bandgap. The typical exction binding energy is in the range of 1–100 meV (see Fig. 9.15). Optical transitions from valenceband electrons into donors and from electrons on acceptors into the conduction band lead to band–impurity absorption. In the region from 10–100 meV the interaction with lattice vibrations (phonons) leads to absorption if the phonons are infrared active. Further in the FIR are transitions from impurities to the closest band edge (donor to conduction and acceptor to valence band). A continuous background is due to freecarrier absorption.
9.2 Reﬂection and Diffraction From Maxwell’s equations and the boundary conditions at a planar interface between two media with different index of refraction for the components of the electric and magnetic ﬁelds the laws for reﬂection and diffraction are derived. We denote the index of refraction as n and also nr in the following. The interface between two media with refractive indices n1 and n2 is depicted in Fig. 9.2. In the following we assume ﬁrst that no absorption occurs. Snellius’ law for the angle of diffraction is n1 sin φ = n2 sin ψ .
(9.2)
When the wave enters the denser medium, it is diffracted towards the normal. If the wave propagates into the lessdense medium (reversely to the situation shown in Fig. 9.2), a diffracted wave occurs only up to a critical angle of incidence n2 sin φTR = . (9.3) n1
9.2 Reﬂection and Diﬀraction
215
normal reflected wave
incident wave
medium 1
interface
medium 2
diffracted wave
Fig. 9.2. Reﬂection and diﬀraction of an electromagnetic wave at the transition between medium ‘1’ and ‘2’, n2 > n1 . The polarization plane is deﬁned by the surface normal and the kvector of the light (plane of incidence). The parallel (‘p’) polarized wave (TMwave, electric ﬁeld vector oscillates in the plane) is shown as ‘↔’; perpendicular (‘s’) polarization (TEwave, electric ﬁeld vector is perpendicular to plane) is depicted as ‘·’
For larger angles of incidence, total internal reﬂection occurs and the wave remains in the denser medium. Thus, the angle in (9.3) is called the critical angle for total reﬂection. For GaAs and air the critical angle is rather small, φTR = 17.4◦ . The reﬂectivity depends on the polarization (Fresnel formulas). The index ‘p’ (‘s’) denotes parallel polarized/TM (perpendicular polarized/TE) waves.
2 tan(φ − ψ) (9.4) Rp = tan(φ + ψ)
2 sin(φ − ψ) Rs = . (9.5) sin(φ + ψ) The situation for GaAs and air is shown for both polarization directions and unpolarized radiation in Fig. 9.3 for a wave going into and out of the GaAs. When the reﬂected and the diffracted wave are perpendicular to each other, the reﬂectivity of the ppolarized wave is zero. This angle is the Brewster angle φB , n2 . (9.6) tan φB = n1 If a wave has vertical incidence from vacuum on a medium with index of refraction nr , the reﬂectivity is given (both polarizations are degenerate) as
216
9 Optical Properties
Fig. 9.3. Reﬂectivity of the GaAs/vacuum interface (close to the bandgap, nr = 3.347) for radiation from vacuum/air and from the GaAs, respectively, as a function of incidence angle and polarization
R=
1 − nr 1 + nr
2
.
(9.7)
For GaAs, the reﬂectivity for vertical incidence is 29.2%. If absorption is considered additionally, the reﬂectivity is (with the complex index of refraction n∗ = nr + iκ) R=
1 − n∗ 1 + n∗
2
=
(nr − 1)2 + κ2 . (nr + 1)2 + κ2
(9.8)
9.3 Electron–Photon Interaction The absorption process is quantum mechanically described by the coupling of electrons and photons. The process is described with timedependent perturbation theory. If H ′ = Hem is the perturbation operator (electromagnetic ﬁeld), the transition probability per time wﬁ for electrons from (unperturbed) state ‘i’ (initial) to state ‘f’ (ﬁnal) is given (with certain approximations) by Fermi’s golden rule wﬁ (ω) =
2π 2 Hﬁ′  δ(Ef − Ei − ω) ,
(9.9)
where ω is the photon energy, Ei (Ef ) is the energy of the initial (ﬁnal) state. Hﬁ′ is the matrix element Hﬁ′ = Ψf H′  Ψi ,
(9.10)
where Ψi (Ψf ) are the wavefunctions of the unperturbed initial (ﬁnal) state.
9.3 Electron–Photon Interaction
217
˙ A is the vector potential for the electromagnetic ﬁeld, i.e. E = −A, μH = ∇ × A, ∇ · A = 0 (Coulomb gange). The Hamiltonian of an electron in the electromagnetic ﬁeld is H=
1 2 (k − qA) . 2m
(9.11)
When terms in A2 are neglected (i.e. twophoton processes), the perturbation Hamiltonian is thus Hem = −
iq q A·p= A · ∇ ≈ qr · E . m m
(9.12)
The latter approximation is valid for small wavevectors of the electromagnetic wave and is termed the electric dipole approximation. In order to calculate the dielectric function of the semiconductor from its band structure we assume that A is weak and we can apply (9.9). The transition probability R for the photon absorption rate at photon energy ω is then given by1 2π 2 cHem v δ (Ec (kc ) − Ev (kv ) − ω) dkc dkv , (9.13) R(ω) = kc kv with the Bloch functions c and v of the conduction and valence band, respectively, as given in (6.39b). The vector potential is written as A = Aˆ e with a unit vector ˆ e parallel to A. The amplitude is connected to the electricﬁeld amplitude E via A=−
E [exp (i(qr − ωt)) + exp (−i(qr − ωt))] . 2ω
(9.14)
In the electricdipole approximation the momentum conservation q+kv = kc , q being the momentum of the light wave is approximated by kv = kc . The matrix element is then given by 2
cHem v =
e2 A2 2 cˆ e · pv , m2
(9.15)
1 pcv 2 = Mb2 , 3
(9.16)
with 2
c ˆ e · pv =
and the momentum matrix element pcv given in (6.38). A kindependent matrix element pcv 2 is often used as an approximation. In Fig. 9.4 the matrix elements for valence to conduction band transitions in GaN are shown as a function of k. 1
Here we assume that the valenceband states are ﬁlled and the conductionband states are empty. If the conductionband states are ﬁlled and the valenceband states are empty, the rate is that of stimulated emission.
218
9 Optical Properties
pcv2 (eV)
30
60
GaN
Ec
20
40
10
20
0 A
L M
A
H K
Ec
0 A
C B A
L M
A
H K
2
Fig. 9.4. Theoretical momentum matrix elements pcv  along highsymmetry directions in the Brillouin zone (cf. Fig. 3.31d) for transitions between valence and conduction bands in GaN and light polarized perpendicular (left panel ) and parallel (right panel ) to the caxis. The transitions are A: Γ9 (A)→ Γ7c , B: Γ7 (B)→ Γ7c , C: Γ7 (C)→ Γ7c (cf. Fig. 6.27). Adapted from [276]
In terms of the electricﬁeld amplitude E(ω) the transition probability is 2 2π e 2 E(ω) 2 p  δ (Ec (k) − Ev (k) − ω) dk . (9.17) R(ω) = cv mω 2 k
If the integration over k is restricted to those values allowed in unit volume, the power that is lost from the ﬁeld in unit volume is given by Rω. The dielectric function ǫ = ǫr + iǫi is given by
2 1 2πe 2 ǫi = pcv  δ (Ec (k) − Ev (k) − ω) dk (9.18a) 4πǫ0 mω k 1 e2 2pcv 2 ǫr = 1 + dk , (9.18b) 2 mω 2 /ω 2 ǫ mω 1 − ω cv k 0 cv cv with ωcv = Ec (k) − Ev (k). The second equation has been obtained via the Kramers–Kronig relations2 (see Appendix B). Comparison with (C.7) yields that the oscillator strength of the band– band absorption is given by f=
e2 2pcv 2 , 2 mω ǫ0 mωcv cv
(9.19)
with Ncv =
2pcv 2 mωcv
(9.20)
being the classical ‘number’ of oscillators with the frequency ωcv . 2 The real and imaginary parts of the dielectric function are generally related to each other via the Kramers–Kronig relations.
9.4 Band–Band Transitions
219
9.4 Band–Band Transitions 9.4.1 Joint Density of States The strength of an allowed optical transitions between conduction and valence bands is, apart from the matrix element (9.15), proportional to the joint density of states (JDOS) Dj (Ecv ) (cf. (6.63), (6.64) and (9.18a)) Dj (Ecv ) = 2
˜ S(E)
1 d2 S , (2π/L)3 ∇k Ecv 
(9.21)
where Ecv is an abbreviation for Ec (k)−Ev (k) and d2 S is a surface element of ˜ = Ecv . The spin is assumed to generate the constant energy surface with E doubly degenerate bands and accounts for the prefactor 2. Singularities of the JDOS (vanHove singularities or critical points) appear where ∇k Ecv vanishes. This occurs when the gradient for both bands is zero or when both bands are parallel. The latter generates particularly large JDOS because the condition is valid at many points in kspace. Generally, the (threedimensional) energy dispersion E(k) around a threedimensional critical point (here developed at k = 0) can be written as E(k) = E(0) +
2 ky2 2 kz2 2 kx2 + + . 2mx 2my 2mz
(9.22)
The singularities are classiﬁed as M0 , M1 , M2 and M3 with the index being the number of masses mi in (9.22) that are negative. M0 (M3 ) describes a minimum (maximum) of the band separation. M1 and M2 are saddle points. For a twodimensional kspace there exist M0 , M1 and M2 points (minimum, saddle point and maximum, respectively). For a onedimensional kspace there exist M0 and M1 points (minimum and maximum, respectively). The functional dependence of the JDOS at the critical points is summarized in Table 9.2. The resulting shape of the dielectric function is visualized in Fig. 9.5. 9.4.2 Direct Transitions Transitions between states at the band edges at the Γ point are possible (Fig. 9.6). The k conservation requires (almost) vertical transitions in the E(k) diagram because the length of the light k vector, k = 2π/λ, is much smaller than the size of the Brillouin zone k ≤ π/a0 . The ratio of the lengths of the k vectors is ∼ 2a0 /λ and typically about 10−3 for NIR wavelengths. For parabolic bands, i.e. bands described with an energyindependent effective mass, the absorption coeﬃcient is (M0 critical point) α ∝ (E − Eg )1/2 .
(9.23)
220
9 Optical Properties
Table 9.2. Functional dependence of the joint density of states for critical points in 3, 2 and 1 dimensions. E0 denotes the energy (band separation) at the critical point, C stands for a constant value. The type of critical point is given (min.: minimum, saddle: saddle point, max.: maximum) Dim.
label
type
Dj for E < E0
Dj for E > E0
3D
M0 M1 M2 M3
min. saddle saddle max.
0 √ C − E0 − E C √ E0 − E
E − E0 C √ C − E − E0 0
2D
M0 M1 M2
min. saddle max.
0 − ln(E0 − E) C
C − ln(E − E0 ) 0
1D
M0 M1
min. max.
0 √
√
√ E0 − E
0
E − E0
r M0
M1
i M2
M3
M0
M1
M2
M3
3D M0
M1
M2
M0
M1
M2
2D M0
M1
M0
M1
1D Fig. 9.5. Shape of the real (left panel ) and imaginary (right panel ) parts of the dielectric function in the vicinity of critical points in 3, 2 and 1 dimensions (for labels see Table 9.2). The dashed line in each graph indicates the energy position of the critical point E0 . Adapted from [277].
The absorption spectrum of GaAs is shown in Fig. 9.7a for photon energies close to the bandgap. The rapid increase, typical for direct semiconductors, is obvious. At low temperatures, however, the absorption lineshape close to the bandgap is dominated by an excitonic feature, discussed in Sect. 9.4.7. Due to the increasing density of states, the absorption increases with the photon energy (Fig. 9.7c). At 1.85 eV there is a step in the absorption spectrum of GaAs due to the beginning of the contribution of transitions
9.4 Band–Band Transitions E
221
E
EC=EV+Eg
EC=EV+Eg
hph
h
h EV
(a)
k
EV
0
kph
k
(b)
Fig. 9.6. (a) Direct optical transition and (b) indirect optical transitions between valence and conduction bands. The photon energy is ω. The indirect transition involves a phonon with energy ωph and wavevector kph .
between the so hole band and the conduction band (see E0 + Δ0 transition in Fig. 9.7e). When bands go parallel, i.e. with the same separation, in the E(k) diagram, the absorption processes contribute at the same transition energy. In this way higher peaks in the absorption spectrum due to the E1 or E0′ transitions originate as indicated in the band structure in Fig. 9.7e. The selection rules for transitions from valence to conduction band must take into account the angular momentum and spin states of the wavefunctions. The optical transitions are circularly polarized as shown in Fig. 9.8. A lifting of the energetic degeneracies of these states occurs, e.g. by magnetic ﬁelds or spatial conﬁnement. 9.4.3 Indirect Transitions In an indirect band structure the missing k difference (across the Brillouin zone) between valence and conductionband state needs to be provided by a second particle. A phonon can provide this and additionally contributes a small amount of energy ωph . Due to energy conservation this absorption starts already at an energy Eg −ωph below the bandgap. But the twoparticle process is less probable than the direct absorption that only involves the photon. Also there are several processes involving various phonons (or combinations of them). The perturbation calculation yields an absorption coeﬃcient with a quadratic dependence on energy (9.24). However, the strength close to the bandgap is about 10−3 smaller than for the direct transition. α ∝ (E − Eg − ωph )2 .
(9.24)
The dependence is shown for Si and GaP in Fig. 9.9. The complicated form is due to the contribution of different phonons.
222
9 Optical Properties
(a)
(d)
GaAs
GaAs
1.0
0.5
0
D ,X
Eg
0
(b)
23
Absorption coefficient (104 cm1)
Absorbtion coefficient (104 cm1)
n=1
1.515
1.520 Energy (eV)
10
E0+0 5 E0
0
(c)
1.5
2.0 Energy (eV)
2.5
(e)
Fig. 9.7. (a) Absorption of GaAs close to the bandgap at diﬀerent temperatures. Adapted from [279]. (b) Highresolution absorption spectrum of highly pure GaAs at T = 1.2 K in the exciton region. Dashed line is theory without excitonic correlation. Adapted from [280]. (c) Absorption spectrum of GaAs at T = 21 K in the vicinity of the bandgap. Adapted from [279]. (d) Complex dielectric function of GaAs at T = 300 K, dashed (solid ) line: real (imaginary) part of dielectric constant. Peak labels relate to transitions shown in part (e). (e) Band structure of GaAs with bandgap transition (E0 ) and higher transitions (E0 + Δ0 , E1 , E1 + Δ1 , E0′ , and E2 ) indicated
9.4 Band–Band Transitions
1/2
1/2
3/2
1/2
1/2
3/2
hh
lh
lh
hh
mj
mj
223
electrons
holes
Fig. 9.8. Optical selection rules for band–band transitions in bulk material 8
GaP
6 Absorption coefficient (cm1)
( E)
1/2
( (eV/cm)1/2 )
Si 5 4 3 2 1
(a)
0 1.00 1.04 1.08 1.12 1.16 1.20 1.24 1.28 Energy (eV)
77K 6
1.6K 4 218K 120K 2
0 2.15
(b)
296K
2.18
2.21
2.24
2.27 2.30 Energy (eV)
2.33
2.26
2.39
2.42
Fig. 9.9. Absorption edge of (a) Si and (b) GaP at various temperatures. Part (a) adapted from [93], based on [281], part (b) adapted from [93] based on [282]
We note also that the indirect semiconductors have an optical transition between Γ valence and conductionband states. However, this transition is at higher energies than the fundamental bandgap, e.g. for Si (Eg = 1.12 eV) at 3.4 eV (see Fig. 6.5a). In Fig. 9.10, the absorption scheme for indirect and direct absorbtion processes starting with an electron at the top of the valence band is shown together with an experimental absorption spectrum for Ge with the direct transition (Γ8 → Γ7 ) at 0.89 eV. In Fig. 9.11, the absorption edge of BaTiO3 is shown. An indirect transition with an increase of (weak) absorption ∝ E 2 and an indirect gap of Ei = 2.66 eV and a direct transition with an increase of (strong) absorption ∝ E 1/2 and a direct gap of Ed = 3.05 eV are observed. These transitions could be due to holes at the M (indirect gap) and Γ (direct gap) points (see Sect. 6.6.9), respectively. 9.4.4 Urbach Tail Instead of the ideal (E − Eg )1/2 dependence of the direct bandedge absorption, often an exponential tail is observed (see Fig. 9.12). This tail is called
224
9 Optical Properties
E Absorption coefficient (cm1)
10
7 L6
8
L
k
4
103 102 101 100 101 102
(b)
(a)
Ge
0.76 0.78 0.80 0.82 0.84 0.86 0.88 0.90 Energy (eV)
Fig. 9.10. (a) Scheme of indirect and direct optical transitions starting at the top of the valence band in Ge. Vertical solid lines represent the involved photon, the horizontal dashed line the involved phonon. (b) Experimental absorption spectrum of Ge (T = 20 K). Adapted from [281] 1/2
k2
k
4
10
15
15
10
10
5
5
0 2.5
2.75 3.0 Energy (eV)
0 3.0
3.25
3.05 3.1 Energy (eV)
3.15
Fig. 9.11. Absorption of BaTiO3 at room temperature. Experimental data (circles) from [283] with ﬁts (dashed lines) ∝ E 2 and ∝ E 1/2 , respectively
the Urbach tail [284] and follows the functional dependence α(E) = αg exp
E − Eg E0
,
(9.25)
where E0 is the characteristic width of the absorption edge, the socalled Urbach parameter. The Urbach tail is attributed to transitions between band tails below the band edges. Such tails can originate from disorder of the perfect crystal, e.g. from defects or doping, and the ﬂuctuation of electronic energy bands due to
10
4
10
3
10
2
10
225
GaAs Urbach parameter (meV)
Absorption coefficient (cm1)
9.4 Band–Band Transitions
1
15
10
GaAs 0
10 1.3
1.4
(a)
1.5 Energy (eV)
1.6
5 0
1.7
(b)
500 Temperature (K)
1000
Fig. 9.12. (a) Experimental absorption spectrum (circles) of GaAs at room temperature on a semilogarithmic plot. The exponential tail below the bandgap is called the Urbach tail (the dashdotted line corresponds to E0 = 10.3 meV). The dashed line is the theoretical dependence from (9.23). Adapted from [287]. (b) Temperature dependence of Urbach parameter E0 for two GaAs samples. Experimental data for undoped (solid circles) and Sidoped (n = 2 × 1018 cm−3 , empty circles) GaAs and theoretical ﬁts (solid lines) with onephonon model. Adapted from [285]
lattice vibrations. The temperature dependence of the Urbach parameter E0 is thus related to that of the bandgap as discussed in [285, 286]. 9.4.5 IntravalenceBand Absorption Besides optical interband transitions between the valence and the conduction band there are also optical transitions within the valence band. In ptype material holes from the valenceband edge can undergo absorption and end up in the splitoff hole band (Fig. 9.13a). Such intravalenceband absorption occurs at photon energies close to Δ0 as shown in Fig. 9.13b for ptype GaAs:Zn. Also, hh → lh transitions are possible. 9.4.6 Amorphous Semiconductors The sharp features in the dielectric function due to critical points in the band structure of crystalline semiconductors are washed out in amorphous material. As an example the spectra of the imaginary part of the dielectric function for crystalline (trigonal) and amorphous selenium are shown in Fig. 9.14. 9.4.7 Excitons An electron in the conduction band and a hole in the valence band form a hydrogenlike state due to the mutual Coulomb interaction. Such a state is called an exciton. The centerofmass motion is separated and has a dispersion
226
9 Optical Properties E
400
Absorption coefficient (cm1)
GaAs:Zn
8
EV Fp
k
6
EV 0
200 100 60 40 0 20 10
0.1
0.2
(b)
(a)
0.3 0.4 Energy (eV)
0.5
0.6
Fig. 9.13. (a) Schematic optical transitions within the valence band. Holes (empty circles) are shown to start at the hole quasiFermi level, transitions are from left to right: ‘hh → so’, ‘lh → so’ and ‘hh → lh’. (b) Experimental absorption spectrum of GaAs:Zn with p = 2.7 × 1017 cm−3 at T = 84 K. The absorption above the splitoﬀ energy Δ0 is due to the hh/lh → so process. Adapted from [288]
Se
20 trigonal
2nk
15 Ec
10
E c
5
0
amorphous 2
4 6 8 Energy (eV)
10
Fig. 9.14. Imaginary part of the dielectric function of amorphous (solid line) and crystalline (trigonal) selenium (dashdotted lines for two diﬀerent polarization directions). From [289] 2
K2 , where M = me + mh is the total mass and K is the centerofE = 2M mass momentum
K = ke + kh .
(9.26)
The relative motion yields hydrogenlike quantized states En ∝ n−2 (n ≥ 1):
9.4 Band–Band Transitions n EX =−
1 m∗r 1 m0 e4 , 2 2 m0 ǫr 2(4πǫ0 ) n2
227
(9.27)
where m∗r denotes the reduced effective mass m∗−1 = m∗−1 +m∗−1 r e h . The third factor is the atomic Rydberg energy (13.6 eV). The exciton binding energy ∗ 1 −3 b 1 EX . A more detailed theory of excitons = −EX is scaled by m m0 ǫ2r ≈ 10 beyond the simple hydrogen model presented here, taking into account the valenceband structure, can be found in [290] for direct and [291] for indirect cubic and in [292] for wurtzite semiconductors. The exciton binding energies for various semiconductor are shown in Fig. 9.15a. n= n=3 n=2
E continuum
Eg E
b X
EX
(b)
(a)
0
n=1
K
Fig. 9.15. (a) Exciton binding energy vs. bandgap for various semiconductors. (b) Schematic dispersion of excitonic levels. The Kvector refers to the centerofmass motion
The radius of the exciton is n rX = n2
m0 ǫr aB , m∗r
(9.28)
where aB = 0.053 nm denotes the hydrogen Bohr radius.3 The Bohr radius 1 of the exciton is aX = rX (14.6 nm for GaAs). The exciton moves with the centerofmass Kvector through the crystal. The complete dispersion is (see Fig. 9.15b) n E = Eg − EX +
2 2 K . 2M
(9.29)
3 Cf. (7.25); an electron bound to a donor can be considered as an exciton with an inﬁnite hole mass.
228
9 Optical Properties
2PA (arb. units)
1PA (a.u.)
The oscillator strength of the exciton states decays ∝ n−3 . The absorption due to excitons is visible in Fig. 9.7a for GaAs at low temperatures. If inhomogeneities are present, typically only the n = 1 transition is seen. However, under special conditions also higher transitions of the exciton Rydberg series are seen (e.g. n = 2 and 3 in Fig. 9.7b). The exciton concept was introduced ﬁrst for absorption in Cu2 O [293]. The J = 1/2 absorption spectrum (‘yellow series’) is shown in Fig. 9.16. In this particular material both the valence and conduction bands have s character, thus the 1s transition of the exciton is forbidden and the np transitions are observed in normal (onephoton) absorption. Only with twophoton absorption can the s (and d) transitions also be excited.
Cu2O (a)
4 green
(b) 2.030
2.035 2.14 2.15 Energy (eV)
2.16
2.17
Fig. 9.16. Onephoton (top) and twophoton (bottom) absorption spectra of Cu2 O at T = 4.2 K. Arrows denote theoretical peak positions. Adapted from [294]
The scattering (unbound) states of the exciton [295] for E > Eg contribute to absorption above the bandgap. The factor by which the absorption spectrum is changed is called the Sommerfeld factor. For bulk material it is S(η) = η
exp(η) , sinh(η)
(9.30)
b 1/2 EX with η = π E−E . The change of the absorption spectrum due to the g Coulomb correlation is shown in Fig. 9.17. There is a continuous absorption between the bound and unbound states. At the bandgap there is a ﬁnite absorption (S(E → Eg ) → ∞). The detail to which exciton peaks can be resolved depends on the spectral broadening.
9.4 Band–Band Transitions
(a)
(b)
(c)
(d)
229
Fig. 9.17. Modiﬁcation of the absorption edge of a direct transition by excitonic eﬀects for diﬀerent spectral (Lorentzian) broadening (∝ (E 2 + Γ 2 /4)−1 ), (a) Γ = b b b 0.01EX , (b) Γ = 0.1EX , (c) Γ = EX . (d) is (c) in linear scale. Dashed lines are electron–hole plasma absorption according to (9.23)
In Fig. 9.18 the energy separations of the A, B, and Cexcitons in GaN are shown [174]. Thus, the ordering of the valence bands depends on the strain state of the semiconductor. 9.4.8 Exciton Polariton Electrons and holes are particles with spin 1/2. Thus, the exciton can form states with total spin S = 0 (paraexciton, singlet) and S = 1 (orthoexciton, triplet). The exchange interaction leads to a splitting of these states, the singlet being the energetically higher. The singlet state splits into the longitudinal and transverse exciton with respect to the orientation of the polarization carried by the Bloch functions and the centerofmass motion K of the exciton. Dipole transitions are only possible for singlet excitons (bright excitons). The triplet excitons couple only weakly to the electromagnetic ﬁeld and are thus also called dark excitons. The coupling of these states to the electromagnetic ﬁeld creates new quasiparticles, the exciton polaritons [297]. The dielectric function of the exciton
230
9 Optical Properties
Transition energy difference (meV)
100
GaN
50 ECEA
0
EBEA
50
0.2
0.1 0 0.1 0.2 caxis strain zz (%)
Fig. 9.18. Theoretical dependency (lines) for the the diﬀerences of the Cline and Aline as well as Bline and Aline exciton transition energies in GaN as a function of the caxis strain. Symbols are experimental data from [296]. Adapted from [174]
(with background dielectric constant ǫb ) is ǫ(ω) = ǫb
β 1+ 2 1 − ωω2
X
∼ = ǫb 1 +
1−
ω2 2 ωT
β + MωT K 2
,
(9.31) 2
K 2 . ωT where β is the oscillator strength and the energy is ωX = ωT + 2M is the energy of the transverse exciton at K = 0. With this dispersion the wave dispersion must be fulﬁlled, i.e.
c2 k 2 = ω 2 ǫ(ω) ,
(9.32)
where k is the k vector of the light that needs to be k = K due to momentum conservation. The dependence of the dielectric function on k is called spatial dispersion [303]. Generally, up to terms in k 2 it is written as ǫ(ω) = ǫb
β 1+ 2 1− ω + Dk 2 ω2 0
.
(9.33)
The term k 2 with curvature D (for the exciton polariton D = /(M ωT )) 2 − ω 2 = 0. For k = 0 even a cubic material plays a role in particular when ωT ˆ = Dk 2 should fulﬁll D ˆ = is anisotropic. The dimensionless curvature D
9.4 Band–Band Transitions
231
(/(M c) ≪ 1 in order to make k 4 terms unimportant. For exciton polaritons4 ˆ = 2 ωT ≈ 2 × 10−5 for ωT = 1 eV and m∗ = 0.1. typically D c m From (9.32) together with (9.33) two solutions result: 2ω 2 = c2 k 2 + (1 + β + Dk 2 )ω02 ± −4c2 k 2 (1 + Dk 2 )ω02 + (c2 k 2 + (1 + β + Dk 2 )ω02 )2
(9.34) 1/2
.
The two branches are shown schematically in Fig. 9.19a. Depending on the k value they have a photonic (linear dispersion) or excitonic (quadratic dispersion) character. The anticrossing behavior at k ′ ≈ ωT /c (for ωT = 1 eV k ′ ≈ 0.5 × 10−5 cm−1 ) creates a bottleneck region in the lower polariton branch. This name stems from the small emission rate of acoustic phonons (i.e. cooling) in that region, as predicted in [298] and experimentally found, e.g. in CdS [299]. The polaritons decay into a photon when they hit the surface. The effect of the oscillator strength of the dispersion is shown in Fig. 9.20 for twoexciton resonance. In the case of several excitons (9.33) reads ⎡ ⎤ n β i ⎦ . (9.35) ǫ(ω) = ǫb ⎣1 + ω2 + Di k 2 1 − 2 ω i=1 0,i
For k = 0 either ω = 0 (lower polariton branch) or ǫ(ωL ) = 0. We ﬁnd from (9.33) ωL = (1 + β)1/2 ωT .
(9.36)
Therefore, the energy splitting ΔELT , mostly denoted as ΔLT , between the L and Texciton energy given by $ % (9.37) ΔELT = (ωL − ωT ) = (1 + β)1/2 − 1 ωT ≈ βωT /2
is proportional to the exciton oscillator strength (for experimental values see Table 9.3). We note that if (C.9) is used for the dielectric function, β in (9.37) needs to be replaced by β/ǫb . The effect of spatial dispersion on the reﬂection at the fundamental exciton resonance is depicted in Fig. 9.19b. For nonnormal incidence an additional feature due to the longitudinal wave is observed for ppolarization [303]. For a detailed discussion additional effects due to anisotropy in wurtzite crystals, an exciton free layer at the semiconductor surface, additional boundary conditions and damping need to be considered [304, 305]. The polariton dispersions of ZnO and GaN are shown in Fig. 9.21. 4
The dependence of the opticalphonon energies on k is typically too small to ˆ = − a0 ωTO 2 ≈ make spatial dispersion eﬀects important. According to (5.18) D 4c 4 × 10−11 for typical material parameters (lattice constant a0 = 0.5 nm, TO phonon frequency ωTO = 15 THz).
232
9 Optical Properties
ZnSe 0.8
UPB Reflectivity
Energy
1.0
ELX ETX
(a)
LPB
k
0.6
0.4
0.2
0.0 0.999
1.000
(b)
1.001 / T
1.002
Fig. 9.19. (a) Schematic dispersion of exciton polaritons. The lower polariton branch (‘LPB’) is at small k photonlike, at large k excitonlike. The upper branch (‘UPB’) is excitonlike at small k and photonlike at larger k. The limit of the UPB for k → 0 is the energy of the longitudinal exciton. The dashed lines represent the pure exciton dispersions. (b) Theoretical eﬀect of spatial dispersion on the reﬂectivity at the fundamental exciton resonance at normal incidence for ZnSe material parameters (ωT =2.8 eV, β = 1.0 × 10−3 and a background dielectric constant of b = 8.1, damping was set to Γ = 10−5 ωT ). The arrow denotes the position of ωL . The solid (dashed) line is with (without) spatial dispersion for ˆ = 0.6 × 10−5 (D ˆ = 0). Data from [303] D Table 9.3. Exciton energy (low temperature), LT splitting and exciton polariton oscillator strength for various semiconductors. Values for ZnO from [300], values for GaAs from [301], all other values from [302] CdS A CdS B ZnO A ZnO B ZnSe
GaN A GaN B GaAs
ωT (eV) 2.5528 2.5681 3.3776 3.3856 2.8019 3.4771 ΔLT (meV) 2.2 1.4 1.45 5 1.45 1.06 β (10−3 ) 1.7 1.1 0.9 3.0 1.0 0.6
3.4816 1.5153 0.94 0.08 0.5 0.11
9.4.9 BoundExciton Absorption Excitons can localize at impurities or inhomogeneities. Such excitons are called bound excitons. Here, the absorption due to such complexes is discussed. The recombination is discussed in Sect. 10.4. In GaP:N excitons are bound to the isoelectronic N impurities (substituting P) that results in the ‘A’ line at 2.3171 eV (at T = 4.2 K). At suﬃciently high nitrogen doping, there exist nitrogen pairs, i.e. a complex where a nitrogen impurity has an
9.4 Band–Band Transitions 3
3
2
2
2
1
1
1
Energy
3
233
(a) 0
0
1
2
k
3
4
(b) 5
0
0
1
2
k
3
4
(c) 5
0
0
1
2
k
3
4
5
Fig. 9.20. Schematic polariton dispersion for a twoexciton resonance (curvature ˆ = 10−2 ) at ωT,1 = 1 and ωT,2 = 1.5 of exciton dispersion greatly exaggerated, D for three diﬀerent oscillator strengths (a) f = 10−3 , (b) f = 10−2 , (c) f = 10−1 . The dashed lines in (c) represent the pure exciton dispersions 3.395
ZnO
Ec
GaN
B L
5
Energy (eV)
3.390 B T B 3.380
5
6
E c
A L
5
A T 3.375 A 5
1,2
0
(a)
10 k (105 cm1)
20
0
(b)
5
10 k (105 cm1)
15
Fig. 9.21. (a) Exciton polariton dispersion (k ⊥ c) of ZnO with experimental data (T = 1.8 K). Solid (dotted ) lines are for polaritons with E c (E ⊥ c). The dashed lines refer to excitons. Adapted from [306]. (b) Exciton polariton dispersion c (T = 2 K) in GaN (on sapphire) for E ⊥ c. Reprinted from [307], 1998, with permission from Elsevier, originally in [308]
234
9 Optical Properties
other nitrogen impurity in the vicinity. The pair is labeled NNn if the second nitrogen atom is in the nth shell around the ﬁrst. For example, NN1 relates to a N–Ga–N complex having 12 equivalent sites for the second N atom. The transitions due to excitons bound to NNn , as shown in Fig. 9.22 give a series of lines (see Table 9.4) that fulﬁll limn→∞ NNn = A. n=
12
3
4
5 67 8
Transmission
NN1' NN2
NN1
NN3 BA
GaP:N 2.18
2.20
2.22
2.24 2.26 Energy (eV)
2.28
2.30
2.32
Fig. 9.22. Transmission spectrum of GaP:N with a nitrogen concentration of about 1019 cm−3 at 1.6 K (thickness: 1.1 mm). n is indicated for the ﬁrst eight transitions due to excitons bound to nitrogen pairs. NNn ’ indicate phonon replica. The ‘A’ line denotes the position of the transition due to excitons bound to a single nitrogen atom (observable for samples with low N doping). The ‘B’ line is forbidden and due to the J = 2 exciton. Adapted from [309]
Table 9.4. Spatial separation d of nitrogen pairs NNn (in nm) and energy separation ΔE of boundexciton transitions from the freeexciton line (in meV) for n = 1 . . . 10 and the ‘A’ line n
1
2
3
4
5
6
7
8
9
10
A
d ΔE
0.385 143
0.545 138
0.667 64
0.771 39
0.862 31
0.945 25
10.2 22
10.9 20
11.56 18
12.19 ∞ 17 11
9.4.10 Biexcitons Similar to two hydrogen atoms forming a hydrogen molecule two excitons can also form a bound complex, the biexciton involving two electrons and two holes. The energy of the biexciton is smaller than 2EX . While the exciton density increases linearly with external excitation, the density of biexcitons increases quadratically.
9.4 Band–Band Transitions
235
9.4.11 Trions The complexes ‘eeh’ and ‘ehh’ are called trions. Also, the notation X− and X+ is common. X− is typically stable in bulk material but hard to observe. In quantum wells or dots, trions are easier to observe. In quantum dots excitons with higher charge, e.g. X2− , have also been observed (see Fig. 13.29). 9.4.12 Burstein–Moss Shift In the discussion so far it has been assumed that all target states in the conduction band are empty. In the presence of free carriers the absorption is modiﬁed by the • •
change of the distribution function manybody effects (bandgap renormalization)
The latter is discussed in the next section. For a degenerate electron distribution all states close to the conductionband edge are populated. Thus a transition from the valence band cannot take place into such states. This shift of the absorption edge to higher energies is called the Burstein–Moss shift [310, 311]. kconserving optical transitions between parabolic hole and electron bands have the dependence E = Eg +
2 k 2 2 k 2 2 k 2 , + = E + g 2m∗e 2m∗h 2mr
(9.38)
where mr is the reduced mass of electron and hole. About 4kT below the Fermi level all levels in the conduction band are populated (Fig. 9.23). Thus the k value at which the absorption starts is given as 1/2 2mr . (9.39) (E − E − 4kT ) kˆ = F 2
Besides the energy shift in the conduction band, the corresponding energy shift in the valence band k 2 /(2mh ) must be considered. Thus, the Burstein– Moss shift of the absorption edge is
me ΔE = ω − Eg = (EF − 4kT − EC ) 1 + . (9.40) mh
The relation between n and the Fermi level is given by (7.8). If EF −EC ≫ −E 3/2 C (Sect. 7.3). kT the Fermi integral can be approximated by √2π 32 EFkT Using (7.10) for NC , the Burstein–Moss shift can be written for this case (low T ) as 2/3
2 3 me h2 2/3 2/3 h ΔE = n n . (9.41) 1+ ≈ 0.97 8me π mh 8mr
Originally, the Burstein–Moss shift was evoked to explain the absorption shift in InSb with varying carrier concentration (Fig. 9.24).
236
9 Optical Properties E
E
EF EF4kT EC
EV
k
fe
k
Fig. 9.23. Principle of Burstein–Moss shift. Left panel : Schematic band structure with completely ﬁlled electron states shown in grey. The kvector for the lowest ˆ Right panel : Electron photon energy optical absorption process is indicated as k. distribution function for a degenerate electron gas with Fermi level in the conduction band
Energy gap (eV)
h E F E c E F E c 4kT
0.8
1.5
0.6
2
0.4
3 4 7
0.2
Eg
gap
Absorption edge (μm)
1
InSb 1.0
10 17 10 18 1019 Electron density (cm 3 )
Fig. 9.24. Burstein–Moss eﬀect at InSb (Eg = 0.18 eV) at room temperature. Theoretical dependence and data points for intrinsic InSb and 5 × 1018 cm−3 ntype. Data from [310]
9.4.13 Bandgap Renormalization The band structure theory has been developed so far for small carrier densities. If the carrier density is large the interaction of free carriers has to be considered. The ﬁrst step was exciton formation. However, at high temperatures (ionization) and at large carrier density (screening) the exciton is not
9.4 Band–Band Transitions
237
stable. Exchange and correlation energy leads to a decrease of the optical absorption edge that is called bandgap renormalization (BGR). An effect due to signiﬁcant carrier density is to be expected when the density is of the order of the exciton volume, i.e. n ∼ a−3 B (Mott criterion). For aB ∼ 15 nm (GaAs) this means n ∼ 3 × 1017 cm−3 . The dimensionless radius rs is deﬁned via 1 4π 3 rs = . (9.42) 3 na3B The sum of exchange and correlation energies Exc is found to be mostly independent of material parameters [312] (Fig. 9.25a) and follows the form a + brs , c + drs + rs2
Exc =
(9.43)
with a = −4.8316, b = −5.0879, c = 0.0152 and d = 3.0426. Thus the density dependence of the bandgap at small carrier density is ∝ n1/3 . Experimental data for a number of II–VI semiconductors roughly follow such a dependence (Fig. 9.25b). 0
0
Ge Si model system
5
Energy (Ryd)
Exc (Ry)
1 2 3 CdS CdSe CdTe ZnO
4
(a)
10 0
5 1
rs
2
3
(b)
0
1
2
3
4
5
rs
Fig. 9.25. (a) Theoretical exchange and correlation energies in units of the exciton Rydberg energy as a function of the dimensionless variable rs for Ge, Si and a model system (with one isotropic conduction and valence band each). The solid line is a ﬁt according to (9.43). Adapted from [312]. (b) Bandgap renormalization in terms of the excitonic Rydberg for various II–VI semiconductors. Solid line is the relation according to (9.43), dashed line is the dependence predicted in [313] for T = 30 K. Data are compiled in [314]
In Fig. 9.26, a theoretical calculation of the absorption spectrum of bulk GaAs for various carrier densities [315] is shown. With increasing density the excitonic resonance broadens and vanishes. The shape approaches the electron–hole plasma shape. The absorption edge shifts to smaller energies. At high density the absorption becomes negative, i.e. ampliﬁcation.
238
9 Optical Properties
1.2
Absorption (cm1)
1.0 0.8 0.6
GaAs n=0 n=51015 cm3 n=31016 cm3 n=81016 cm3
0.4 0.2 0.0 0.2
1.490
1.495 Energy (eV)
1.500
Fig. 9.26. Absorption of GaAs (low temperature, T = 10 K) as a function of the electron–hole density n (theory). Adapted from [315]
9.4.14 Electron–Hole Droplets At low temperature and high density, electron–hole pairs in Ge and Si can undergo a phase transition into a liquid state. This electron–hole liquid (EHL) was suggested in [316] and is a Fermi liquid exhibiting the high conductivity of a metal and the surface and density of a liquid. The condensation is due to exchange interaction and correlation. The formation is fostered by the band structure of Ge [317] and the long lifetime of carriers in the indirect band structure. In unstressed Ge typically a cloud of electron–hole droplets with diameter in the µm range exists. The phase diagram is shown in Fig. 9.27a. In suitably stressed Ge electron–hole droplets with several hundred µm diameter form around the point of maximum shear strain in inhomogeneously strained crystals, as shown in Fig. 9.27b. The pair density in such a liquid is of the order of 1017 cm−3 . We note that the metallic EHL state hinders observation of the Bose– Einstein condensation (BEC) of (bosonic) excitons. The lightexciton mass offers a high condensation temperature in the 1 K range (compared to the mK range for atoms). Recent experiments with spatially indirect excitons in coupled quantum wells lead towards BEC [321, 322]. A suﬃciently long lifetime ensures cooling of the excitons close to the lattice temperature. Another potential candidate for BEC are longliving excitons (msrange) in Cu2 O [323]. The condensation of polaritons (see Sect. 9.4.8) in microcavities to welldeﬁned regions of kspace has been discussed in [324] and compared to bosonic condensation in bulk.
9.4 Band–Band Transitions
EHG
T
sp
6
EHL
5
T (K)
screw
Ge
exp
c
7 exp c
239
4 3 droplets of EHL in EHG
2
EHL
1 0
(a)
0
0.5
1.0 1.5 2.0 17 3 (10 cm )
2.5
Ge disk
(b)
Fig. 9.27. (a) Temperature–density phase diagram of electrons and holes in Ge. The regions of electron–hole gas (EHG) and liquid (EHL) and the droplet phase are labeled. Solid line is theoretical calculation, symbols are experimental data from [318]. The dashdotted line denoted ρsp is the experimentally obtained temperature dependence of the liquid density due to singleparticle excitations. ρexp c and Tcexp denote the experimental critical density and temperature, respectively. Adapted from [319]. (b) Photographic image of radiative recombination (at 1.75 µm wavelength) from a 300µm diameter droplet of electron–hole liquid (EHL) in a stressed (001) Ge disk (diameter 4 mm, thickness 1.8 mm) at T = 2 K. The stress is applied from the top by a nylon screw along a 110 direction. Adapted from [320], c reprinted with permission, 1977 APS
9.4.15 TwoPhoton Absorption So far, only absorption processes that involve one photon have been considered. The attenuation of the intensity I of a light beam (of frequency ω0 ) along the z direction can be written as dI = −αI − βI 2 , dz
(9.44)
where α is due to the (linear) absorption coeﬃcient (and possibly scattering) and β is the twophoton absorption coeﬃcient. A twophoton process can occur in two steps, e.g. via a midgap level, which is not considered any further here. Here, we consider twophoton absorption (TPA) via the population of a state at 2ω0 higher energy than the initial state with a nonlinear optical process. The TPA coeﬃcient is related to the nonlinear thirdorder electric dipole susceptibility tensor [325] χijkl . Within the twoband approximation theory predicts [326] 3/2
β ∝ (2ω0 − Eg )
.
(9.45)
240
9 Optical Properties
Transition rate (W/V)
10
GaAs
22
1021
~(2h  Eg)1/2 ~(2h  Eg)3/2
10
20
1019 3 10
2
10 10 2h  Eg (eV)
1
1
Fig. 9.28. Experimental (dots) twophoton absorption of GaAs (T = 4 K) as a function of the diﬀerence of the doublephoton energy 2ω from the GaAs band edge Eg . The solid line is a theoretical calculation, the dashed lines represent slopes with exponent 1/2 and 3/2, respectively. Adapted from [327]
The exponent 3/2 is indeed found experimentally, as shown in Fig. 9.28 for GaAs. The strength of absorption depends on the relative orientation of the light polarization with respect to the main crystallographic directions, e.g. TPA for polarization along 110 is about 20% larger than for the 100 orientation.
9.5 Impurity Absorption Charge carriers bound to shallow impurities exhibit a hydrogenlike term scheme En =
m∗ 1 1 × 13.6 eV , m0 ǫ2r n2
(9.46)
with the ionization limit E∞ being the conduction (valence) band edge for donors (acceptors), respectively. They can be excited by light to the nearest band edge. Such absorption is typically in the FIR region and can be used for photodetectors in this wavelength regime. The actual energies can deviate from (9.46) due to deviation of the potential close to the impurity from the pure Coulomb potential. Such an effect is known as the chemical shift or central cell effect and is characteristic of the particular impurity. In GaAs such shifts are small (∼ 100 µeV) [328]. The term scheme for P in Si is shown in Fig. 9.29a. The ground state (1s) is split because of a reduction of the tetrahedral symmetry due to intervalley
9.5 Impurity Absorption
0
241
5p0 4p±, 5p±
cond. band
3p± 4p0 3p0 2p±
2p0
...
cond. band
hph
4p 3p
11.62
1s(E) 1s(T1)
1.33
2p
(a)
44.09 43.25 42.41 42.25 40.07 39.14 34.08
45.31
1s(A1)
h (b)
1s
Fig. 9.29. (a) Term scheme of phosphorus donor in silicon, all energies in meV. After [329]. (b) Schematic sequence for photothermal ionization, here absorption of a photon with ω = E3p − E1s and subsequent absorption of a phonon with energy ωph ≥ E∞ − E3p
coupling. The anisotropic mass at the Xvalley in Si causes the p states (and states with higher orbital momentum) to split into p0 and p± states. Such an effect is absent in a direct semiconductor with an isotropic conductionband minimum such as GaAs (Fig. 9.30). Optical transitions between the 1s and various p states are observed because the missing energy to the ionization into the continuum is supplied by a phonon at ﬁnite temperature (photothermal ionization) (Fig. 9.29b). The splitting of the 2p transition in Fig. 9.30a is the chemical shift due to different donors incorporated in the GaAs (Si, Sn, and Pb). Peak broadening is mostly Stark broadening due to neighboring charged impurities. The application of a magnetic ﬁeld induces Zeemanlike splittings and increases the sharpness of the peaks. The peak width can be further increased by illuminating the sample with light having a higher energy than the bandgap. The additional charge carriers neutralize charged impurities and allow higher resolution (Fig. 9.30b).
9 Optical Properties Energy (meV) 5 6
4
Photoconductive response
Si 2p
GaAs 2p0
Sn Pb
2p
2p
ED 0T 1.9T
30
(a)
7
3p 4p 2s
3p 3p0
40 50 1 Energy (cm )
GaAs
Photoconductive response
242
1s3p
illuminated
dark 48
60
(b)
1s3p0
50 52 Energy (cm1)
54
Fig. 9.30. (a) Farinfrared photoconductivity response (Lymantype s→p series) of not intentionally doped GaAs with residual donors Pb, Sn, and Si, NA = 2.6 × 1013 cm−3 , ND − NA = 8 × 1012 cm−3 . The upper (lower ) curve is for a magnetic ﬁeld of 0 (1.9) T. Measurement temperature is 4.2 K. (b) Photoconductive response of a (diﬀerent) GaAs sample with the same impurities (ND = 1 × 1013 cm−3 ) with (upper curve) and without (lower curve) illumination with abovebandgap light (B = 1.9 T, T = 4.2 K). Adapted from [330]
In Fig. 9.31 absorption spectra of highly doped ntype GaAs are shown. For doping concentrations larger than the critical concentration of ∼ 1 × 1016 cm−3 (cf. Table 7.6) signiﬁcant broadening is observed due to the formation of an impurity band (Sect. 7.5.5). The absorption of deep levels is typically in the infrared. In Fig. 9.32a the possible optical absorption processes involving the Fe levels in InP (cf. Sect 7.7.6) during the charge transfer Fe3+ → Fe2+ are shown. These transitions and their ﬁne structure (Fig. 9.32b) have been observed in calorimetric absorption spectroscopy (CAS) experiments [228].
9.6 FreeCarrier Absorption A timedependent electric ﬁeld accelerates the charge carriers. The excess energy is subsequently transferred to the lattice via scattering with phonons. In the relaxationtime approximation energy is relaxed with a time constant τ . Thus energy is absorbed from the electromagnetic wave and dissipated. The complex conductivity (8.38) is given by
1 ωτ ne2 τ + i . (9.47) σ = σr + iσi = m∗ 1 + ω2 τ 2 1 + ω2 τ 2 We note that a static magnetic ﬁeld introduces birefringence as discussed in more detail in Sect. 12.2.1. The wave equation for the electric ﬁeld is
9.6 FreeCarrier Absorption
243
b
1s 2p ED
Absorption coefficient (cm1)
GaAs:Te
500 ND (cm3) 2.11016 14 1.010 15 6.710 15 1.010
0 50 1 Energy (cm )
0
100
Fig. 9.31. Lowtemperature (T = 1.35 K) absorption spectra of highly doped ntype GaAs:Te with doping concentrations as labeled (circles: ND = 2.1×1016 cm−3 , stars: 6.7 × 1014 , triangles: 1.0 × 1015 ). A sharp photoconductivity spectrum (in arbitrary units) from lowdoped GaAs:Te (crosses, ND = 1.0 × 1014 cm−3 ) is shown for comparison (cf. Fig. 9.30a). The energy of the 1s→2p transition and the donor binding energy (onset of continuum absorption) are indicated. Adapted from [331]
1.34
EC 1.14
5
0.78
InP:Fe E
InP:Fe Absorption (arb. units)
T2
5
0.25 0 (a)
Fe
3+
Fe2+
EV
TA
5
VB E 0.77
0.78
(b)
5
VB T2 1.14 Energy (eV)
1.15
Fig. 9.32. (a) Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrows denote the optical transition of a valenceband electron to the Fe center, Fe3+ + ω → Fe2+ + h. (b) Calorimetric absorption spectra (at T = 1.3 K) of InP:Fe, [Fe]=5 × 1016 cm−3 . Part (b) adapted from [228]
¨ + σμ0 E ˙ . ∇2 E = ǫμ0 E For a plane wave ∝ exp [i(kr − ωt)] the wavevector obeys
1/2 σ∗ ω , ǫr + i k= c ǫ0 ω
(9.48)
(9.49)
where c = (ǫ0 μ0 )−1/2 is the velocity of light in vacuum, ǫr is the background dielectric constant (for large ω).
244
9 Optical Properties
The tensor of the dielectric function from free carriers is ǫ=
i ∗ σ . ǫ0 ω
(9.50)
The complex index of refraction is ∗
n = nr + iκ =
σ∗ ǫr + i ǫ0 ω
1/2
.
(9.51)
Taking the square of this equation yields τ2 σi ne2 = ǫr − ∗ ǫ0 ω ǫ0 m 1 + ω 2 τ 2 2 τ σr ne = 2nr κ = . ∗ ǫ0 ω ǫ0 ωm 1 + ω 2 τ 2
n2r − κ2 = ǫr + i
(9.52a) (9.52b)
The absorption coeﬃcient (damping of E2 ) of the plane wave is ω α=2 κ. c
(9.53)
For the case of higher frequencies, i.e. ωτ ≫ 1, the absorption is α=
ne2 1 . ∗ ǫ0 cnr m τ ω 2
(9.54)
The absorption decreases with increasing frequency. For semiconductors it is particularly important in the mid and farinfrared regions when carriers are present due to doping or thermal excitation. The index of refraction is given by (also for ωτ ≫ 1) ω 2 ne2 ǫ2 ωp 4 1 p 2 + κ = ǫ (9.55) + r2 1 − n2r = ǫr − r ∗ 2 ǫ0 m ω ω 4nr ω ω2 τ 2 ω 2 p ≈ ǫr 1 − , ω where ωp =
ne2 ǫr ǫ0 m∗
1/2
(9.56)
is the plasma frequency. The approximation is valid for small absorption and when (ωτ )−2 can be neglected. A graphical representation is given in Fig. 9.33a. For coupling to electromagnetic waves (still ωτ ≫ 1) ω 2 c2 k 2 p (9.57) = 2 ǫ(ω) = ǫr 1 − ω ω
9.7 Lattice Absorption
245
2
1
0
1
1
2
(a)
0
1
/p
2
(b)
0 0
1
k
2
Fig. 9.33. (a) Dielectric constant for plasmon oscillations. Shaded area represents region of attenuation (negative ). (b) Dispersion relation (k in units of ωp /c, ω in units of ωp ) in the presence of free carriers (9.58, for r = 1). Shaded area represents forbidden frequency range for propagating solutions. Dashed line is photon dispersion ω = ck
must be fulﬁlled. It follows that the dispersion relation in the presence of free carriers (Fig. 9.33b) is ω 2 = ωp2 +
c2 k 2 . ǫ2r
(9.58)
For ω > ωp , ǫ > 0, thus waves can propagate. For ω < ωp , however, the dielectric constant is negative, i.e. ǫ < 0. For such frequencies waves are exponentially damped and cannot propagate or penetrate a layer. This effect can be used in a plasmon waveguide. The expected dependence of the plasmon wavelength on the carrier density λp ∝ n−1/2 is depicted in Fig. 9.34 for GaAs. For semiconductors the plasmon frequency is in the midor farinfrared spectral region.5
9.7 Lattice Absorption 9.7.1 Dielectric Constant The dielectric constant (with damping parameter Γ ) in the vicinity of the optical phonon energies is given by (cf. (5.43))
2 ωLO − ω 2 − iωΓ . (9.59) ǫ(ω) = ǫ(∞) 2 − ω 2 − iωΓ ωTO 5
The much higher freeelectron density in metals shifts the plasma frequency to the UV, explaining the reﬂectivity of metals in the visible and their UV transparency.
246
9 Optical Properties
Fig. 9.34. Plasmon wavelength for GaAs with various electron concentrations due to diﬀerent doping levels. Filled circles: experimental values, dashed line: n−1/2 dependence
The dispersion relation (without damping) can be written as ǫ(0) − ǫ(∞) f ǫ(ω) = ǫ(∞) + = ǫ(∞) 1 + . 2 2 1 − ω 2 /ωLO 1 − ω 2 /ωLO Thus the oscillator strength (compare with (C.10)) is f = the LST relation (5.42) the oscillator strength is f=
2 2 ωLO ωLO − ωTO − ωTO , ≈2 2 ωTO ωTO
(9.60)
ǫ(0)−ǫ(∞) . ǫ(∞)
With
(9.61)
and thus proportional to the splitting ΔLT = ωLO −ωTO between the longitudinal and transverse optical phonon frequency. The approximation in (9.61) is valid for ΔLT ≪ ωTO . The oscillator strength increases with the ionicity, i.e. the electronegativity difference of the atoms in the base (Fig. 9.35). Additionally, the oscillator strength depends on the reduced mass and the highfrequency polarizability; this can be seen, e.g., for the series of the Zn compounds that all have similar ionicity. For the series of the nitrides, the mass effect is small since the reduced mass is dominated by the light N mass. 9.7.2 Reststrahlenbande The absorption of electromagnetic radiation by optical phonons is governed by the dielectric function that has been derived in (9.59). For small damping, i.e. Γ ≪ ΔLT , the dielectric constant is negative between ωTO and ωLO . From ǫr = n2r − κ2 it follows that κ2 is much larger than n2r . Therefore, the reﬂectivity (9.8) will be close to 1. This energy range is the socalled
9.7 Lattice Absorption
247
Fig. 9.35. Lattice absorption oscillator strength f from (9.61) for various IV–IV, III–V and II–VI compounds as a function of their ionicity fi . Dashed line is linear dependence on ionicity for similar (reduced) mass, dashdotted line is a guide to the eye for similar ionicity and varying mass
reststrahlenbande. This term stems from multiple reﬂections in this wavelength regime that suppresses neighboring spectral regions and thus achieves a certain monochromatization in the farinfrared spectral region. Within the semiconductor the absorption is large in the reststrahlenbande (Fig. 9.36).
GaAs
0
25
50 Energy (meV)
75
Fig. 9.36. Farinfrared absorption of GaAs. In the region around 35 meV is the reststrahlenbande with high absorption due to optical phonons. Adapted from [93], based on [229]
248
9 Optical Properties
9.7.3 Polaritons The coupled propagation of phonons and electromagnetic radiation is related to the equation (without phonon damping) ǫ(ω) = ǫ(∞)
2 ωLO − ω2 2 − ω2 ωTO
=
c2 k 2 . ω2
(9.62)
There are two branches of propagating waves (real k): 1 ω2 = 2
c2 k 2 2 + ωLO ǫ(∞)
2 2 2 2 2 1/2 2 2 c k ωTO k c 1 2 + − . ± ωLO 4 ǫ(∞) ǫ(∞)
(9.63)
ǫ(0). For large k we For k = 0 we ﬁnd the solutions ω = ω and ω = kc/ LO ﬁnd ω = ωTO and ω = kc/ ǫ(∞). These solutions are shown in Fig. 9.37. Both branches have a phonon and a photonlike part. The coupled state between the phonon and the photon ﬁeld is called the (phonon) polariton.
Fig. 9.37. Dispersion of the polariton. The dotted line displays the dispersion for a purely imaginary wavevector with the absolute value k
In the interval [ωTO , ωLO ] the wavevector is purely imaginary, i.e. k = ik˜ ˜ For this case there is only one solution that is depicted in Fig. 9.37 with real k. as dotted line,
ω2 =
1 2
"
2 ωLO +
2 ˜2
c k ǫ(∞)
#
⎡ " #2 " #2 ⎤1/2 2 ˜2 2 ˜2 2 1 c k c k ωTO ⎦ 2 +⎣ ωLO . + + 4 ǫ(∞) ǫ(∞)
(9.64)
9.7 Lattice Absorption
249
9.7.4 Phonon–Plasmon Coupling The coupling of phonons and plasmons in the spectral region of the reststrahlenbande leads to the development of two new branches, the longitudinal phonon plasmon modes (LPP+ and LPP−), in the common dispersion. The dielectric function is " # 2 ωp2 − ω2 ωLO ǫ(ω) = ǫ(∞) 1 + 2 (9.65) − 2 . ωTO − ω 2 ω For ǫ(ω) = 0 for k = 0 (coupling to photons) the two solutions ωLPP+ and ωLPP− do not cross as a function of ωp (Fig. 9.38), ωLPP± =
1/2 % 2 1$ 2 2 ωLO + ωp2 ± (ωLO + ωp2 )2 − 4ωTO ωp2 . 2
(9.66)
For small plasma frequencies ωLPP+ = ωLO , i.e. the optical phonons couple to the electromagnetic ﬁeld without change. Also ωLPP− = ωp . For large carrier density, i.e. ωp ≫ ωLO , we ﬁnd ωLPP− = ωTO and ωLPP+ = ωp . Thus, the carriers have effectively screened the electric ﬁeld of the phonon that had led to the increase of the TO to the LO frequency.
Fig. 9.38. Frequency of the coupled longitudinalphonon plasmon (LPP) modes as a function of the plasma frequency
10 Recombination
10.1 Introduction In thermodynamic nonequilibrium excess charges can be present in the semiconductor. They can be created by carrier injection through contacts, an electron beam or the absorption of light with wavelength smaller than the bandgap. After the external excitation is turned off, the semiconductor will return to the equilibrium state. The relaxation of carriers into energetically lower states (and energy release) is called recombination. The term stems from the electron recombining with the hole created after absorption of a photon. However, there are other recombination mechanisms. In the simplest picture an excitation generates carriers with a rate G (carriers per unit volume and unit time). In the steady state (after all turnon effects) a constant excess charge n carrier density is present. Then the generation exactly compensates the recombination processes. The principle of detailed balance even says that each microscopic process is balanced by its reverse process. If the time constant of the latter is τ , n is given by n = Gτ . This follows from the steadystate solution n˙ = 0 of n dn =G− . dt τ
(10.1)
10.2 Band–Band Recombination The band–band recombination is the relaxation from an electron in the conduction band into the valence band (the empty state there is the hole). In a direct semiconductor, electrons can make an optical transition between the bottom of the conduction band to the top of the valence band. In an indirect semiconductor, this process is only possible with the assistance of a phonon and is thus much less probable. 10.2.1 Spontaneous Emission We consider the spontaneous recombination of an electron of energy Ee and a hole of energy Eh (Fig. 10.1a). C(Ee , Eh ) is a constant proportional to the matrix element of the optical transition (see Sect. 9.3). The spontaneous
252
10 Recombination
Ec E=h
Eg
E=h
E=h
E=h E=h
Ev
(a)
(b)
(c)
Fig. 10.1. Processes of band–band recombination: (a) spontaneous emission, (b) absorption and (c) stimulated emission. A full (empty) circle represents an occupied (unoccupied) electron state
recombination rate rsp at photon energy E ≥ EC − EV = Eg is (assuming energy conservation, i.e. E = Ee − Eh , but without kconservation in a dense plasma [332]), ∞ EV dEh C(Ee , Eh ) (10.2) dEe rsp (E) = EC
−∞
×De (Ee )fe (Ee )Dh (Eh )fh (Eh )δ(E − Ee + Eh ) E+EV = dEe C(Ee , Ee − E) EC
×De (Ee )fe (Ee )Dh (Ee − E)fh (Ee − E) ,
where fh denotes the hole occupation fh = 1 − fe . The lineshape of the band–band recombination with kconservation1 is proportional to the joint density of states (9.21) and the Fermi distribution function. At small excitation and at low doping it can be approximated by the Boltzmann distribution function and the lineshape is given as
E 1/2 . (10.3) exp − I(E) ∝ (E − Eg ) kT An experimental spectrum is shown in Fig. 10.2 together with a ﬁt according to (10.3). The expected FWHM of the peak is 1.7954 kT , which is about 46 meV at T = 300 K. 10.2.2 Absorption A similar consideration is made for the absorption process (Fig. 10.1b). An electron is transferred upon light absorption from a valenceband state (occupied) to a conductionband state that must be empty. The coeﬃcient is 1
b Excitonic eﬀects are neglected here, e.g. for temperatures kT ≫ EX .
10.2 Band–Band Recombination
PL Intensity (arb. units)
5
253
GaAs
4 3
E= 46meV
2 Eg= 1.423eV
1 0 1.35
1.40
1.45 1.50 Energy (eV)
1.55
Fig. 10.2. Photoluminescence spectrum of an undoped LPEgrown epitaxial GaAs layer at room temperature and low cw (λ = 647 nm) excitation density (10 W/cm2 ). The solid line is a lineshape ﬁt with (10.3) and Eg =1.423 eV and T = 293 K
B1 . Also, the process is proportional to the light intensity, represented by the density of occupied photon states Nph (E), rabs (E) =
E+EV
dEe B1 (Ee , Ee − E)
EC
(10.4)
De (Ee )(1 − fe (Ee ))Dh (Ee − E)(1 − fh (Ee − E))Nph (E) . 10.2.3 Stimulated Emission In this case, an incoming photon ‘triggers’ the transition of an electron in the conduction band into an empty state in the valence band. The emitted photon is in phase with the initial photon (Fig. 10.1c). The rate is (with coeﬃcient B2 ): rst (E) =
E+EV
EC
dEe B2 (Ee , Ee − E)
(10.5)
De (Ee )fn (Ee )Dh (Ee − E)fp (Ee − E)Nph (E) . 10.2.4 Net Recombination Rate In thermodynamical equilibrium the rates fulﬁll rsp (E) + rst (E) = rabs (E) .
(10.6)
The population functions are Fermi functions with quasiFermi levels Fn and Fp . The photon density is given by Planck’s law and the Bose–Einstein distribution (Appendix D)
254
10 Recombination
Nph = N0
exp
1 E kT
−1
.
(10.7)
The prefactor is N0 = ω 3 n2r /(π 2 c3 ). Since for absorption and stimulated emission the same quantummechanical matrix element is responsible, B1 = B2 . The detailed balance (10.6) yields
E − (Fn − Fp ) −1 . (10.8) C(E1 , E2 ) = B1 (E1 , E2 )Nph exp kT In thermodynamic equilibrium, i.e. Fn = Fp , C(E1 , E2 ) = N0 B1 (E1 , E2 ) = B .
(10.9)
If the constant B, the bimolecular recombination coeﬃcient, is independent of the energy E, the integration for the net recombination rate R can be executed analytically and we ﬁnd ∞ rB = [rsp (E) + rst (E) − rabs (E)] dE (10.10) Eg
Fn − Fp . = Bnp 1 − exp − kT
In thermodynamic equilibrium, of course, rB = 0. The recombination rate Bnp is then equal to the thermal generation rate Gth Gth = Bn0 p0 .
(10.11)
The bimolecular recombination rate typically used in Shockley–Read–Hall (SRH) [333, 334] kinetics is rB = B(np − n0 p0 ) .
(10.12)
Values for the coeﬃcient B are given in Table 10.1. In the case of carrier injection, np is larger than in thermodynamical equilibrium, i.e. np > n0 p0 , and the recombination rate is positive, i.e. light is emitted. If the carrier density is smaller than in thermodynamical equilibrium, e.g. in a depletion region, absorption is larger than emission. This effect is also known as ‘negative luminescence’ [335] and plays a role particularly at elevated temperatures and in the infrared spectral region. 10.2.5 Recombination Dynamics The carrier densities n and p, are decomposed into the densities n0 and p0 in thermodynamic equilibrium and the excesscarrier densities δn and δp, respectively n = n0 + δn p = p0 + δp .
(10.13a) (10.13b)
10.2 Band–Band Recombination
255
Table 10.1. Bimolecular recombination coeﬃcient B at room temperature for a number of semiconductors. Data for GaN from [336], Si from [337], SiC from [338], other values from [339] Material
B (cm3 /s)
GaN GaAs AlAs InP InAs 4HSiC Si GaP
1.1 1.0 7.5 6.0 2.1 1.5 1.1 3.0
×10−8 ×10−10 ×10−11 ×10−11 ×10−11 ×10−12 ×10−14 ×10−15
Here, only neutral excitations are considered, i.e. δn = δp. Obviously the ∂ δn time derivative fulﬁlls ∂n ∂t = ∂t , and correspondingly for the hole density. The equation for the dynamics n˙ = p˙ = −Bnp + Gth = −B(np − n0 p0 ) = −B(np − n2i )
(10.14)
can be written as ∂ δp = −B (n0 δp + p0 δn + δn δp) . ∂t
(10.15)
The general solution of (10.15) is given by δp(t) =
(n0 + p0 )δp(0) . [n0 + p0 + δp(0)] exp (Bt(n0 + p0 )) − δp(0)
(10.16)
In the following, we discuss some approximate solutions of (10.15). First, we treat the case of a small (neutral) excitation, i.e. δn = δp ≪ n0 , p0 . The dynamic equation is in this case ∂ δp = −B (n0 + p0 ) δp . ∂t
(10.17)
Then the decay of the excesscarrier density is exponential with a time constant (lifetime) τ given by τ=
1 . B (n0 + p0 )
(10.18)
In an ntype semiconductor additionally n0 ≫ p0 , and thus the minority carrier lifetime τp is
256
10 Recombination
τp =
1 . Bn0
(10.19)
If the nonequilibrium carrier densities are large, i.e. n ≈ p ≫ n0 , p0 , e.g. for strong injection, the kinetics obeys ∂ δp = −B(δp)2 , ∂t
(10.20)
and the transient has the form δp(t) =
δp(0) , 1 + Btδp(0)
(10.21)
where δp(0) is the excess hole density at time t = 0. Such a decay is called hyperbolic and the recombination is bimolecular. The exponential decay time is formally τ −1 = Bδp(t) and is thus time and density dependent. 10.2.6 Lasing The net rate for stimulated emission and absorption is
E − (Fn − Fp ) (10.22) rst (E) − rabs (E) = 1 − exp kT E+EV dEe BDe (Ee )fe (Ee )Dh (Ee − E)fh (Ee − E)Nph (E) . × EC
The net rate at photon energy E = ω is only larger than zero (i.e. dominating stimulated emission) when Fn − Fp > E ≥ Eg .
(10.23)
When the difference of the quasiFermi levels is larger than the bandgap, the carrier population is inverted, i.e. close to the band edges the conductionband states are more strongly populated with electrons than the valenceband states, as shown in Fig. 10.3. An incoming optical wave of energy E will then be net ampliﬁed by stimulated emission. Equation (10.23) is also called the thermodynamic laser condition. We note that lasing requires further conditions as discussed in Sect. 20.4.
10.3 FreeExciton Recombination The observation of freeexcitons is limited for semiconductors with a small exciton binding energies (such as in GaAs) to low temperatures. However, for large exciton binding energy, recombination from freeexcitons is observed even at room temperature, as shown in Fig. 10.4 for ZnO.
10.3 FreeExciton Recombination
257
E Fn EC
EV Fp
D(E) Fig. 10.3. Chargecarrier distribution during inversion, necessary for lasing. Shaded areas are populated with electrons. A stimulated transition between an electron and a hole is indicated
ZnO
PL Intensity (arb. units)
295 K 249 K 220 K 191 K 158 K 131 K 111 K 89 K 73 K 54 K 41 K 0
D ,X
3.20
3.25 3.30 Energy (eV)
3.35
XA
19 K 10 K 4.4 K
3.40
Fig. 10.4. Temperaturedependent luminescence spectra of a ZnO thin ﬁlm (on sapphire). At low temperatures, the spectra are dominated by donorbound exciton transitions (Al0 ,X)). The vertical dashed line indicates the lowtemperature position of the donorbound exciton transition (D0 ,X). The curved dashed line visualizes the energy position of the freeexciton transition (XA ) that becomes dominant at room temperature
258
10 Recombination
10.4 BoundExciton Recombination Excitons can localize at impurities or other potential ﬂuctuations and subsequently recombine. Excitons can be bound to neutral or ionized impurities (donors and acceptors). The transition energy ω of an exciton bound to a neutral impurity is b −Q, ω = Eg − EX
(10.24)
where Q is the binding energy of the exciton to the impurity. A transition involving an exciton bound to a neutral donor is denoted (D0 ,X); correspondingly (D+ ,X), also denoted as (h,D0 ), and (A0 ,X). In Si, the binding energy to the impurity is about one tenth of the binding energy of the impub b rity (Haynes’s rule [340]), i.e. Q/ED and Q/EA ≈ 0.1 (Fig. 10.5a). In GaP b b + 3 meV the approximate relations Q = 0.26ED − 7 meV and Q = 0.056EA b have been found [341]. For donors in ZnO Q = 0.40ED − 5.34 meV holds (Fig. 10.5b) [342]. 20
Si In
Q (meV)
15
10
Bi As Ga P Sb Al B
5
0
(a)
0
50
150 100 b ED, A (meV)
200
(b)
Fig. 10.5. Energy Q required to remove an exciton from a neutral impurity (10.24) b b as a function of the ionization energy ED (open circles) or EA (solid circles) of the involved impurity in (a) silicon (experimental data from [340]) and (b) ZnO (experimental data from [342])
In Fig. 10.6, the recombination spectrum of GaAs:C is shown that exhibits recombination from excitons bound to the acceptor (carbon) and shallow donors. The exciton is more strongly bound to an ionized donor (D+ ) than to a neutral donor. The peak labeled (D0 ,X)2s in Fig. 10.6 is called a twoelectron satellite (TES) [344]. Highresolution spectra of the TES in GaAs [186,345] are shown in Fig. 10.7a. The TES recombination is a (D0 ,X) recombination that leaves the donor in an excited state as schematically shown in Fig. 10.7b. Therefore a hydrogenlike series with n = 2, 3, . . . is observed with energies
Photoluminescence Intensity (arb. units)
10.4 BoundExciton Recombination
259
0
(A ,X)
GaAs:CAs
0
(h,D ) 0 (D ,X) 0
(e,A ) X (n=1) 0
0
0
(D ,A )
(h,D2s)
0
(D ,X)2s
X (n=2) 20
1.49
1.50 1.51 Energy (eV)
1.52
Fig. 10.6. Photoluminescence spectrum (T = 2 K, D = 10 mW cm−2 ) of GaAs:CAs (NA = 1014 cm−3 ) with donor and acceptorrelated boundexciton recombination around 1.512 eV, (e,A0 ), (h,D0 ) and (D0 ,A0 ) pair and freeexciton recombination. Adapted from [343]
(D0,X)
Photoluminescence Intensity (arb. units)
TES
EC
20
0
0
X
D* n=3 n=2
4
ED
40
n=1
1
1.510
(a)
D
exc.
1.515 Energy (eV)
(b)EV
Fig. 10.7. (a) Photoluminescence spectrum (T = 1.5 K, D = 50 mW cm−2 ) of highpurity GaAs with two donors (Ge and Se/Sn). The lower spectrum has been excited 6 meV above the bandgap, the upper spectrum has been resonantly excited with the laser set to the (D0 ,X) transition and exhibits n = 2, 3, 4, and 5 TES transitions. α,β,γ denote excited (hole rotational) states of the (D0 ,X) complex. Adapted from [345]. (b) Schematic representation of the n = 2 TES process, left: initial, right: ﬁnal state
260
10 Recombination n ETES
= E(D0 ,X) −
b ED
1 1− 2 n
.
(10.25)
The effect of isotope disorder on the sharpness and splitting of impurity states has been investigated in [346, 347]. The recombination of excitons bound to Al, Ga and In in natural silicon (92.23% 28 Si, 4.67% 29 Si, 3.10% 30 Si) is split into three lines due to the valleyorbit splitting [348] of electron states at the band minimum. Each of these (A0 ,X) lines is split by 0.01 cm−1 for Si:Al due to a symmetry reduction of the 4fold degenerate A0 ground state, as observed in the presence of applied axial strain or an electric ﬁeld. The comparison to spectra from enriched 28 Si shows that the observed splitting without external perturbation is due to isotope disorder that causes random strains and splits the A0 ground state into two doublets [347]. Similarly, the (unsplit) phosphorusinduced (D0 ,X) transition in enriched Si is found to be much sharper (< 40 µeV) than in natural Si (330 µeV) [346].
10.5 Alloy Broadening The boundexciton recombination peak in a binary compound is spectrally fairly sharp (Sect. 10.4), even in the presence of isotope disorder. In an alloy (see Sect. 3.7), the random distribution of atoms (with different atomic order number Z) causes a signiﬁcant broadening effect of the luminescence (and absorption) line, the socalled alloy broadening [349]. As an example, we treat Alx Ga1−x As. The exciton samples, at different positions of the lattice, different coordinations of Ga and Al atoms. If the experiment averages over these conﬁgurations, an inhomogeneously broadened line is observed. The cation concentration cc for the zincblende lattice is given as cc = 4 a−3 0 ,
(10.26)
where a0 is the lattice constant. cc = 2.21 × 1022 cm−3 for Alx Ga1−x As in the entire composition range 0 ≤ x ≤ 1 since the lattice constant does not vary signiﬁcantly. In a random alloy, the probability p(N ) to ﬁnd exactly N Ga atoms in a given volume V (with a total of cc V cations) is given by the binomial distribution
c V p(N ) = c xN (1 − x)cc V −N . (10.27) N The sampling volume for a luminescence event is the exciton volume (cf. (9.28)) that is given for the freeexciton as Vex
4π 4π 3 aX = = 3 3
m0 ǫs aB m∗r
3
.
(10.28)
10.6 Phonon Replica
261
PL intensity (arb. units)
Si:Al 0
AX A0
natural Si 28
Si
1.1508
1.1509 1.1510 Photon energy (eV)
Fig. 10.8. Highresolution photoluminescence (PL) spectra of (A0 ,X) recombination in natural and 28 Sienriched silicon doped with aluminum (T = 1.8 K). The 28 Si PL spectrum is shifted up in energy by 0.114 meV, as indicated by the arrow, to compensate for the shift in bandgap. The inset shows a level scheme for the recombination in natural silicon. Adapted from [347], reprinted with permission, c 2002 APS
In GaAs there are about 1.6 × 105 cations in the exciton volume. In Alx Ga1−x As, there are on average xcc Vex Al atoms in the exciton volume. The ﬂuctuation is given by the standard deviation of the binomial distribution σx2 =
x(1 − x) . cc Vex
(10.29)
The corresponding energetic broadening (full width at halfmaximum) of the spectral line ΔE is 1/2 ∂Eg x(1 − x) ∂Eg σx = 2.36 . ΔE = 2.36 ∂x ∂x cc Vex
(10.30)
This theoretical dependence is shown for Alx Ga1−x As in Fig. 10.9 together with experimental data.
10.6 Phonon Replica The momentum selection rule for freeexciton recombination allows only excitons with K ≈ 0 (for K cf. (9.26)) to recombine. The ﬁne structure of this recombination is connected to polariton effects (cf. Sect. 9.4.8). Excitons with large K can recombine if a phonon or several phonons are involved that provide the necessary momentum q = K1 − K2 , with K1 (K2 ) being the wavevector of the initial (intermediate) exciton state (Fig. 10.10). A socalled
262
10 Recombination
9
FWHM (meV)
7
AlxGa1xAs
5 4 3 2
1 0.0
0.1 0.2 0.3 Al concentration x
0.4
Fig. 10.9. Spectral width of the (A0 ,X) recombination photoluminescence line of excitons bound to carbon acceptors in Alx Ga1−x As with various Al content within the directbandgap regime. Full circles are experimental data at T = 2 K and low excitation density from various sources, solid line is theory according to (10.30). Experimental data from [349]
E
n=3 n=2 continuum n=1
hph
E1
K Fig. 10.10. Schematic representation of 1 LO exciton scattering of an exciton at K = 0 to an intermediate state with K ≈ 0 and subsequent radiative decay. ωph represents the phonon energy and E1 the energy of the emitted photon
10.6 Phonon Replica
263
zerophonon line at energy E0 is then accompanied by phonon replica below E0 at integer multiples (at low temperature) of the (LO) phonon energy ωph En = E0 − nωph .
(10.31)
Phonon replica have been observed in many polar semiconductors such as CdS [350] and ZnSe [351]. A sequence of such phonon replica, as observed in GaN [352], is depicted in Fig. 10.11a. BE FE
GaN PL Intensity (arb. units)
10
0
1LO 10
1
10
2
2LO
5LO
4LO
103
92meV
3.1
(a)
3LO
3.2 3.3 Energy (eV)
3.4
3.5
(b)
Fig. 10.11. (a) Photoluminescence spectrum of GaN (grown on SiC substrate) at T = 50 K. In addition to emission from free (FE) and bound (BE) excitons several phonon replica (labeled as 1LO–5LO) are observed. Vertical dashed lines indicate energy positions of multiple LOphonon energies (ωLO = 92 meV) below the FE peak. Adapted from [352]. (b) Photoluminescence spectrum of 1LO phononassisted recombination peak at T = 103 K (from the data of Fig. 10.4). Data points (dots) and lineshape ﬁt (solid line) according to (10.32) with the parameters L1 = 1.00 ± 0.05 and E1 = 3.2947 eV (and background)
The lineshape of the nth phononassisted line is proportional to the exciton population at a given excess energy, which is proportional to the density of states and the Boltzmann distribution function [353]
Eex 1/2 wn (Eex ) . (10.32) In (Eex ) ∝ Eex exp − kT Here, Eex represents the exciton kinetic energy. The factor wn (Eex ) accounts for the qdependence of the matrix element. It is typically expressed as Ln . wn (Eex ) ∝ Eex
(10.33)
Accordingly, the energy separation ΔEn of the energy of the peak maximum of phonon replica from E0 is given by
1 ΔEn = En − E0 = nωph + Ln + kT . (10.34) 2
264
10 Recombination
It is found theoretically that L1 = 1 and L2 =0. These relations are experimentally veriﬁed and, e.g., fulﬁlled for the peaks of Fig. 10.11a. A lineshape ﬁt for the 1 LO phononassisted transition in ZnO is shown in Fig. 10.11b. In Fig. 10.12a the ‘green band’ emission of ZnO is shown as presented in [354]. This band is mostly attributed to a Cu impurity; recently, evidence has grown from isotope decay and annealing studies that it is related to the zinc vacancy [355] (Fig. 10.12b). The zero phonon line is followed by many replica with a maximum at about 6 LO phonons. The intensity IN of the N th replica is given by [356, 357] SN , (10.35) N! where S is the socalled Huang–Rhys parameter. In [355], a coupling parameter of S = 6.9 has been determined. Equation (10.35) is obtained from the consideration of transitions in the conﬁguration diagram [356, 358] (Fig. 10.13), using the Born–Oppenheimer approximation, i.e. the electronic wavefunctions are separated from the vibrational wavefunctions, the Frank–Condon principle, i.e. that optical transitions occur with the positions of the nuclei ﬁxed and thus vertical in the conﬁguration diagram Fig. 10.13 and assuming low temperatures, i.e. only the lowest state is (partially) occupied. The Huang–Rhys parameter, the average number of phonons involved in the transition, is related to the displacement δq = q1 − q0 of the two conﬁgurations IN ∝ exp(−S)
S=
Cδq 2 , 2ωph
(10.36)
where C is the curvature of the parabola, C = d2 E/dq 2 .
PL Intensity (arb. units)
650
600
ZnO
8 9
450
4 3 2 1
2.0
(a)
Wavelength (nm) 550 500 6 5 7
2.2 2.4 Energy (eV)
2.6
2.8
(b)
Fig. 10.12. (a) Luminescence spectrum of ZnO in the visible. The arrow denotes the zerophonon line at 2.8590 eV. The numbers of the phonon replica are labeled. Adapted from [354]. (b) Luminescence spectra (solid lines) of a ZnO bulk crystal before (‘untreated’) and after annealing in O2 atmosphere at T = 1073 K. After annealing in Zn atmosphere at the same temperature, the green band disappears again (dashed line). From [355]
10.7 Donor–Acceptor Pair Transitions
E
absorption
emission
S= 0
S h E1
1
E
2
h
4 8
E0 (a)
265
q0 q1
q
ZPL
(b)
E
Fig. 10.13. (a) Conﬁguration diagram of two states that diﬀer in their conﬁguration coordinate by δq = q1 − q0 . Both are coupled to phonons of energy ω. The absorption maximum (solid vertical line) and emission maximum (dashed vertical line) are shifted with respect to the zerophonon line (dotted vertical line) with energy E1 − E0 . The Huang–Rhys parameter is S ∼ 4. (b) Intensity of zerophonon line (‘ZPL’) and phonon replica (10.35) for emission and absorption processes with diﬀerent values of the Huang–Rhys parameter S as labeled
For small S ≪ 1, we are in the weak coupling regime and the zerophonon line is the strongest. In the strong coupling regime, S > 1, the maximum is (red) shifted from the zerophonon line. We note that in absorption, phonon replica occur on the highenergy side of the zerophonon absorption. For large S the peak intensities are close to a Gaussian.
10.7 Donor–Acceptor Pair Transitions Optical transitions can occur between neutral donors and acceptors. The (spatially indirect) donor–acceptor pair (DAP) recombination is present in (partially) compensated semiconductors and follows the scheme D0 A0 → D+ A− eh → D+ A− + γ, where γ is a photon with the energy ω. The energy of the emitted photon is given by b b ω = Eg − ED − EA −
1 e2 , 4πǫ0 ǫr R
(10.37)
where R is the distance between the donor and the acceptor for a speciﬁc pair. Since R is discrete, the DAP recombination spectrum consists of several discrete lines. If the donor and acceptor occupy the same sublattice, e.g. O and C both substituting Psites in GaP, the spatial distance of the donor and acceptor is R(n) = a0 n/2, where a0 is the lattice constant and n is an integer. However, for certain ‘magic’ numbers n = 14, 30, 46, . . . no lattice points exist and therefore the corresponding lines are missing (labeled ‘G’
10 Recombination
Transition energy (eV)
266
1.57 1.56 1.55 1.54 1.53 1.52 1.51 1.50 1.49 1.48 1.47 1.46 1.45 1.44 1.43 1.42 1.41 1.40
C O
Zn O
GaP
Cd O
15.5 meV 32.5 meV
0
0.5
1.0
1.5 R (nm)
2.0
2.5
3.0
Fig. 10.14. Transition energies in GaP (T = 1.6 K) of the donor–acceptor recombination involving the deep oxygen donor and C, Zn, and Cd acceptors, respectively. b The lines follow (10.37) for EgGaP =2.339 eV, r = 11.1 and (ED )O = 893 meV, b b b (EA )C = 48.5 meV, (EA )Zn = 64 meV, and (EA )Cd = 96.5 meV. Predicted missing modes for GaP:C,O are labeled with ‘G’. Adapted from [359]
in Fig. 10.14). No such gaps exist in DA spectra where donors and acceptors occupy different sublattices, e.g. GaP:O,Zn (see also Fig. 10.14). In this case, the spatial separation is given by R(n) = a0 n/2 − 5/16. If signiﬁcant broadening is present, the lines are washed out and a donor–acceptor pair band forms. 1.34 1.14
5
0.78
InP:Fe E
PL Intensity (arb. units)
EC T2
5
0.25 0 (a)
Fe
3+
Fe2+
EV
InP:Fe 5
0.340
(b)
T25E
0.345 Energy (eV)
0.350
Fig. 10.15. (a) Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrow denotes the optical transition from an excited Fe2+ state to the Fe2+ ground state. (b) Photoluminescence spectrum (at T = 4.2 K) of InP:Fe sample with [Fe]=5 × 1016 cm−3 . Part (b) adapted from [361].
10.9 Auger Recombination
267
10.8 InnerImpurity Recombination The transitions of electrons between different states of an impurity level can be nonradiative or radiative. As an example, the radiative transition of electrons in the Fe2+ state in InP 5 T2 →5 E (Fig. 10.15) and its ﬁne structure were observed ﬁrst in [360] at around 0.35 eV.
10.9 Auger Recombination In competition with the radiative, bimolecular recombination is the Auger recombination (Fig. 10.16). In the Auger process, the energy that is released during the recombination of an electron and hole is not emitted with a photon but, instead, transferred to a third particle. This can be an electron (eeh, Fig. 10.16a) or a hole (hhe, Fig. 10.16b). The energy is eventually transferred nonradiatively from the hot third carrier via phonon emission to the lattice. The probability for such process is ∝ n2 p if two electrons are involved and ∝ np2 if two holes are involved. The Auger process is a threeparticle process and becomes likely for high carrier density, either through doping, in the presence of many excess carriers, or in semiconductors with small bandgap. Auger recombination is the inverse of the impact ionization (see Sect. 8.5.3). e
E
e
Eg
Eg
lh
(a)
E
lh
hh
k (b)
hh
k
Fig. 10.16. Schematic representation of Auger recombination. An electron recombines with a hole and transfers the energy to (a) another electron in the conduction band, (b) another electron in the valence band
268
10 Recombination
In thermodynamic equilibrium the rates for Auger recombination and thermal Auger generation must be equal, thus Gth = Cn n20 p0 + Cp n0 p20 ,
(10.38)
where Cn and Cp denote the Auger recombination coeﬃcients. The equation for the dynamics in the presence of excess carriers (if solely Auger recombination is present) is given as ∂ δn = Gth − R = −Cn (n2 p − n20 p0 ) − Cp (np2 − n0 p20 ) . ∂t
(10.39)
The Auger recombination rate typically used in SRH kinetics is rAuger = (Cn n + Cp p)(np − n0 p0 ) .
(10.40)
Typical values for the Auger recombination coeﬃcients are given in Table 10.2. Table 10.2. Auger recombination coeﬃcients for some semiconductors. Data for InSb from [362], SiC from [338], others from [339] Material
Cn (cm6 /s)
Cp (cm6 /s)
4HSiC Si, Ge GaAs, InP InSb
5 ×10−31 2 ×10−31 −31 2.8 ×10 9.9 ×10−32 −30 5.0 ×10 3.0 ×10−30 −26 1.2 × 10
10.10 Band–Impurity Recombination Another recombination process is the capture of carriers by impurities. This process is in competition with all other recombination processes, e.g. the radiative recombination and the Auger mechanism. The band–impurity recombination is the inverse process to the carrier release from impurities. It is particularly important at low carrier densities, for high dopant concentration and in indirect semiconductors since for these the bimolecular recombination is slow. The theory of capture on and recombination involving impurities is called Shockley–Read–Hall (SRH) kinetics [333,334]. An example of radiative band–impurity recombination (of the type shown in Fig. 10.17a) is shown in Fig. 10.6 for the (e,A0 ) recombination at the carbon acceptor in GaAs. We consider electron traps (see Fig. 10.17) with a concentration Nt with an energy level Et . In thermodynamic equilibrium they have an electron population
10.10 Band–Impurity Recombination
269
EC Et EV (a)
(b)
(c)
(d)
Fig. 10.17. Bandtoimpurity processes at an impurity with one level (left: initial, right: ﬁnal state in each part): (a) electron capture (from conduction band), (b) electron emission (into conduction band), (c) hole capture (from valence band), (d) hole emission (into valence band). The arrows indicate the transition of the electron
ft0 =
exp
1 Et −EF kT
+1
,
(10.41)
where ft is the nonequilibrium population of the trap. Then the capture rate rc is proportional to the density of unoccupied traps and the electron concentration, rc ∝ nNt (1 − ft ). The proportionality factor has the form vth σn , where vth is the thermal velocity vth = (3kT /m∗ )1/2 ≈ 107 cm/s at room temperature and σn is the capture cross section that is of the order of the lattice constant a20 , typically ∼ 10−15 cm2 . In order to make the following 1/2 calculation more transparent, we put the effectivemass ratio (m0 /m∗ ) into σ in the following and thus have the same thermal velocity vth = (3kT /m0 )1/2 for electrons and holes. The capture rate of electrons is rc = vth σn nNt (1 − ft ) .
(10.42)
The emission rate from ﬁlled traps is gc = en Nt ft ,
(10.43)
where en denotes the emission probability. In a similar way, the emission and capture rates for holes can be written: rv = vth σp pNt ft gv = ep Nt (1 − ft ) .
(10.44) (10.45)
In thermodynamical equilibrium, capture and generation rates are equal, i.e. rc = gc and rv = gv . Thus, the emission probability is en = vth σn n0
1 − ft0 . ft0
(10.46)
270
10 Recombination 1−f 0
Using f 0 t = exp t can be written as
Et −EF kT
, (7.15) and (7.16) the emission probabilities
en = vth σn nt ev = vth σp pt , with nt = NC exp (7.20))
E
t −EC
kT
(10.47) (10.48)
−EV and pt = NV exp − EtkT . We note that (cf.
EC − EV nt pt = NC NV exp − kT
= n0 p0 .
(10.49)
The temperature dependence of the thermal velocity is ∝ T 1/2 , the temperature dependence of the bandedge density of states is ∝ T 3/2 (7.10) and (7.13). Thus, the temperature dependence of the emission rate is (apart from the exponential term) ∝ T 2 if σ is temperature independent. Charge conservation requires rc − rv = gc − gv , also in nonequilibrium. From this we obtain the population function in nonequilibrium: ft =
σn n + σp p . σn (n + nt ) + σp (p + pt )
(10.50)
The recombination rate rb−i of the band–impurity recombination is then rb−i = −
∂δn = r c − gc ∂t =
(10.51)
σn σp vth Nt (np − n0 p0 ) . σn (n + nt ) + σp (p + pt )
Using the ‘lifetimes’ τp0 = (σn vth Nt )−1 and τn0 = (σp vth Nt )−1 , this is typically written as rb−i =
1 (np − n0 p0 ) . τp0 (n + nt ) + τn0 (p + pt )
(10.52)
For an ntype semiconductor the Fermi level is above Et and the traps are mostly full. Thus hole capture is the dominating process. The equation for the dynamics simpliﬁes to p − p0 ∂δp . =− ∂t τp0
(10.53)
Thus, an exponential decay with minoritycarrier lifetime τp0 (or τn0 for ptype material) occurs. A recombination center is most effective when it is close to the middle of the bandgap (midgap level). The condition ∂rb−i /∂Et = 0 leads to the trap energy Etmax with the maximum recombination rate being located at
10.10 Band–Impurity Recombination
Etmax =
EC + E V − kT ln 2
σn NC σp NV
.
271
(10.54)
The curvature ∂ 2 rb−i /∂Et2 at Etmax is proportional to −(np − n0 p0 ) and thus indeed is negative in the presence of excess carriers. The maximum recombination rate (for Et = Etmax ) is σn σp vth Nt (np − n2i ) 2ni (σn σp )1/2 + nσn + pσp
np np − n2i 1/2 − ni ≈ σvth Et , (10.55) = (σn σp ) vth Nt γ ni n + p + 2ni
max rb−i =
with γ −1 = 2 +
nσn + pσp n+p , ≈2+ ni ni (σn σp )1/2
(10.56)
where the approximations are for σ = σn = σp . The energetic width (FWHM) ΔEt for which the recombination rate has dropped by a factor of 2 from this maximum value is
1 + 2γ + (1 + 4γ)1/2 . (10.57) ΔEt = 2kT ln 2γ For large excess carrier concentration n + p ≫ ni and γ ≈ ni /(n + p) ≪ 1, the width is
n+p ΔEt ≈ 2kT ln γ −1 ≈ 2kT ln (10.58) ni which can be signiﬁcant for suﬃciently high temperature. In the case of a constant density of impurity states (per energy) Dt around midgap the total recombination rate is (for ΔEt ≪ Eg ) 1 max Dt ˆ dE rb−i = rb−i ˆ Et 1 + γ [2 sinh(E/(2kT ))]2 √ max Dt arctanh( 1 − 4γ) √ = 4kT rb−i , (10.59) Et 1 − 4γ ˆ = E − Et . For large excess carrier concentration γ ≪ 1: with E max rb−i ≈ 2kT rb−i
Dt ln γ −1 . Et
(10.60)
With σ = σn = σp we ﬁnd rb−i
np ≈ 2kT σvth Dt ln n+p
n+p ni
.
(10.61)
272
10 Recombination
For a neutral excitation n = p ≫ ni the rate is
2n rb−i ≈ kT σvth Dt n ln , ni
(10.62)
dominated by n. In the case of an unipolar excitation (np ≫ ni und n ≫ p, ni ), the minority carrier density p is the dominating factor,
n rb−i ≈ 2kT σvth Dt p ln . (10.63) ni In the case of small carrier density n + p ≪ ni (10.59) becomes [364] max rb−i ≈ πkT rb−i
Dt π ≈ − kT σvth Dt ni . Et 2
(10.64)
A typical example is gold in silicon. The minority carrier lifetime decreases from 2 × 10−7 s to 2 × 10−10 s upon increase of the Au concentration from 1014 to 1017 cm−3 . The incorporation of recombination centers is an important measure for the design of highfrequency devices [363]. A reduction in minoritycarrier lifetime can also be achieved by irradiation with highenergy particles and the subsequent generation of point defects with energy levels at midgap.
10.11 Field Effect The emission of electrons from a trap is thermally activated with an ionization energy Ei = EC − Et . If the trap is in a strong electric ﬁeld E, the emission probability can change. An acceptorlike trap after removal of the electron is neutral and its potential is short range. A donor has a longrange Coulomb potential after ionization. In an electric ﬁeld, these potentials are modiﬁed as visualized in Fig. 10.18. Various additional processes can now occur. 10.11.1 Thermally Activated Emission For the δlike potential the ionization energy remains unchanged. For the Coulomb potential the barrier in the ﬁeld direction is lowered by ΔEi = e
eE πǫr
1/2
.
(10.65)
The emission probability is increased in the ﬁeld by exp (ΔEi /kT ). This effect is called the Poole–Frenkel effect and can be quite important. For silicon and E = 2 × 105 V/cm and ΔEi = 100 meV a 50fold increase of emission rate results at room temperature.
10.12 Multilevel Traps
273
Ei Ei
(a)
(b)
Fig. 10.18. Field eﬀect at (a) a δlike potential and (b) a Coulomb potential
10.11.2 Direct Tunneling Carriers can tunnel from the trap level through the barrier in the ﬁeld direction into the conduction band. This process is temperature independent. The transmission factor of a barrier is (in WKB approximation) proportional to exp − 2 2m[V (x) − E]dE . The emission probability for a triangular barrier is then # " 3/2 eE 4(2m∗ )1/2 Ei . (10.66) exp − en = 3eE 4(2m∗ Ei )1/2 In the case of a Coulomblike potential the argument of the exponent in (10.66) needs to be multiplied by a factor 1 − (ΔEi /Ei )5/3 with ΔEi from (10.65). 10.11.3 Assisted Tunneling In a thermally assisted tunneling process the electron on the trap level is ﬁrst excited to a virtual level Et +Eph by phonon absorption and then tunnels out of the trap (photonassisted tunneling). From the energetically higher level the tunneling rate is higher. The probability is proportional to exp (Eph /kT ). The additional energy can also be supplied by a photon (photonassisted tunneling).
10.12 Multilevel Traps Traps with multiple levels in the bandgap have generally similar but more complicated dynamics as compared to singlelevel traps. Lifetimes are an average over negatively and positively charged states of the trap.
274
10 Recombination
10.13 Surface Recombination A surface is typically a source of recombination, e.g. by midgap levels induced by the break of crystal symmetry. The recombination at surfaces [364] is modeled as a recombination current js = −eS(ns − n0 ) ,
(10.67)
Recombination rate S (cm/s)
where ns is the carrier density at the surface and S is the socalled surface recombination velocity. The surface recombination velocity for GaAs is shown in Fig. 10.19. For InP, if the surface Fermi level is pinned close to midgap, the surface recombination velocity increases from ∼ 5 × 103 cm/s for a doping level of n ∼ 3×1015 cm−3 to ∼ 106 cm/s for a doping level of n ∼ 3×1018 cm−3 [365]. For Si, the surface recombination rate depends on the treatment of the surface and lies in the range between 10–104 cm/s [366, 367]. The SiSiO2 interface can exhibit S ≤ 0.5 cm/s. Timeresolved measurements and detailed modeling for Si have been reported in [368]. 10
7
GaAs 10
6
105
104 15 10
1016 1017 1018 3 Concentration n (cm )
1019
Fig. 10.19. Surface recombination velocity for GaAs as a function of ntype doping concentration. Diﬀerent experimental points correspond to diﬀerent surface treatment methods. Dashed line is a guide to the eye. Experimental data from [369]
10.14 ExcessCarrier Proﬁles In this section, some typical excesscarrier proﬁles (in onedimensional geometry) are discussed that arise from certain excitation conditions. The excesscarrier density Δp (here holes in an ntype semiconductor, i.e. Δp = pn −pn0 ) is determined by the diffusion equation (cf. (8.51a)) Dp
∂ 2 Δp Δp = −G(x) . + ∂x2 τp
(10.68)
10.14 ExcessCarrier Proﬁles
275
The generation of excess carriers in a semiinﬁnite piece of semiconductor occurs only at the surface at x = 0. The generation is zero everywhere and the excitation is incorporated via the boundary condition Δp(x = 0) = Δp0 . The general solution for the homogeneous equation (10.68), i.e. G = 0, is
x x Δp(x) = C1 exp − + C2 exp , (10.69) Lp Lp with the diffusion length Lp = Δpn (x → ∞) = 0 the solution is
Dp τp . Taking the boundary condition
x Δp(x) = Δp0 exp − . Lp
(10.70)
In order to connect Δp0 with the total generation rate per unit area Gtot , we calculate ∞ Δp(x) Dp Δp0 Lp dx = = Δp0 . (10.71) Gtot = τ τ τp p p 0 Now, the generation is taken as G(x) = G0 exp (−αx) ,
(10.72)
i.e. due to light absorption with the (wavelengthdependent) absorption coeﬃcient α. The total generation rate is ∞ G0 . (10.73) Gtot = G(x)dx = α 0 The solution of (10.68) is the sum of the homogeneous solution (10.69) and a particular solution that is given by Δp(x) = C exp (−αx) .
(10.74)
The constant C is determined to be C=
G 0 τp . 1 − α2 L2p
(10.75)
Therefore, the solution is
x x G 0 τp + C2 exp + Δp(x) = C1 exp − exp (−αx) . (10.76) Lp Lp 1 − α2 L2p Using again Δpn (x → ∞) = 0 (leading to C2 = 0) and a recombination velocity S at the front surface, i.e.
276
10 Recombination
−eSΔp0 = −eDp
dΔp dx
.
(10.77)
x=0
The solution is given as
x G0 τp S + αDp exp − . exp (−αx) − Δp(x) = 1 − α2 L2p S + Dp /Lp Lp
(10.78)
For S = 0 the solution is Δp(x) =
G 0 τp x exp − , exp (−αx) − αL p 1 − α2 L2p Lp
(10.79)
and then for αLp ≫ 1, (10.70) is recovered. This dependence is the excesscarrier proﬁle if the absorption is strong, which is a tendency for short wavelengths.
11 Heterostructures
11.1 Introduction Heterostructures consist of (at least two) different materials. The geometry of the interfaces between the two materials can be complicated. The simplest case is a planar interface, i.e. a layered system. A metal–semiconductor junction is generally a heterostructure. However, we will use the term mostly for structures of various semiconductors. Most of the heterostructures discussed here are epitaxial, i.e. fabricated by the successive epitaxy of the various layers on a substrate. Another method to fabricate heterostructures of different (and dissimilar) materials is wafer bonding that is brieﬂy discussed in Sect. 11.8. Many modern semiconductor devices rely on heterostructures, such as the heterobipolar transistor (HBT), the high electron mobility transistor (HEMT), lasers and nowadays also lightemitting diodes. Shockley had already considered heterostructures in his 1951 patent for pnjunctions. For the development and the realization of heterostructures H. Kroemer and Zh.I. Alferov were awarded the 2000 Physics Nobel Prize. The properties of charge carriers in layers that are part of heterostructures can be quite different from those in bulk material, e.g. extremely high mobility, high radiative recombination eﬃciency or novel states of matter, as revealed in the quantum Hall effects.
11.2 Growth Methods Since the thickness of layers in the active part of heterostructures has to be controlled to monolayer precision and the thickness of layers can go down to the single monolayer range, special growth methods have been developed. Among these molecular beam epitaxy (MBE), chemical vapor deposition (CVD) and metalorganic vapor phase epitaxy (MOVPE) are the most common for Si, Ge, III–V and II–VI semiconductors. In particular, oxide semiconductors are also fabricated with pulsed laser deposition (PLD). Liquid phase epitaxy (LPE) used to be very important for the fabrication of LEDs but has lost its role largely to MOVPE.
278
11 Heterostructures
MBE is performed in an ultrahigh vacuum (UHV) chamber, pumped by getter pumps and cryoshrouds. The source materials are evaporated from effusion cells and directed towards the heated substrate. If the source materials are supplied as a gas stream, the method is called gassource MBE (GSMBE). If metalorganic compounds are used as precursors, the method is denoted as MOMBE. The atoms impinge on the substrate with thermal energy and are ﬁrst physisorbed. After diffusion on the surface they either desorb or they are chemisorbed, i.e. incorporated into the crystal. In order to obtain high spatial homogeneity of material properties such as composition, thickness and doping, the substrate is rotated during deposition. During CVD and MOVPE the heated substrate is in a gaseous environment. The transport gas is typically H2 , N2 or O2 . Precursor materials are hydrides such as silane, germane, arsine or phosphine (SiH4 , GeH4 , AsH3 , PH3 ) and (for MOVPE) metalorganic compounds, such as, e.g. trimethylgallium (TMG). Due to the toxicity of the hydrides, alternative, i.e. lesstoxic and lessvolatile compounds are used, such as TBAs ((CH3 )3 CAsH2 ). The crystal growth occurs after pyrolysis and catalysis of the compounds close to or on the substrate surface. All remaining C and H atoms (and whatever else that is not incorporated into the crystal) leave the reactor and are neutralized and stopped in a scrubber. Thinﬁlm epitaxy is mostly performed on wafers, i.e. thin circular slices of substrate material. The most common substrate materials are Si (currently up to 300 mm diameter), GaAs (up to 6 inch), InP (up to 4 inch) and sapphire (up to 6 inch). Typical wafer thickness is 300–500 µm. Also, very thin, ﬂexible Si wafers (8–10 µm) have been developed. A wafer is cut from a large single cylindrical crystal that is fabricated with suitable growth techniques such as Czochralski (CZ) growth (1918) modiﬁed by Teal and Little [370]. In CZ growth the crystal is pulled from a seed crystal out of a melt of previously polycrystalline, pure or doped material. All dislocations stop in the narrow neck between the seed and the main body of the cylinder. The diameter of the crystal is controlled by the pulling rate and the heating power. For the growth of III–V compound semiconductors liquid encapsulated CZ (LEC) growth has been developed to counteract the high volatility of the growthV component. During LEC growth the melt is completely covered with molten boric oxide (B2 O3 ). The keys to optimization of the crystal growth process are numerical modeling and computer control. In Fig. 11.1 a large CZ silicon crystal and a smaller LEC GaAs crystal (boule) are shown. For details on other important fabrication methods for bulk crystals, including ﬂoatzone (FZ) or vertical gradient freeze (VGF), we refer to the literature [371]. Signiﬁcant expertise is necessary for cutting, grinding and polishing (lapping) wafers for epitaxy. For semiconductors, the wafer is marked with ﬂats to indicate orientation and doping. In Fig. 11.2 the standard ﬂats are shown for (001) and (111)oriented material. The primary ﬂat is longer than the secondary ﬂat, e.g. 32
11.2 Growth Methods
279
(b)
(a)
Fig. 11.1. (a) Silicon single crystal for 300mm diameter wafers after opening of the crucible. From [372] with permission. (b) GaAs single crystal (boule) for 4inch wafers and some cut and polished wafers
S S P
P
(100) ntype
(100) ptype
S
P
P
(111) ntype
(111) ptype
Fig. 11.2. Schematic semiconductor wafer geometry for various orientations and doping with the primary (P) and secondary (S) ﬂats indicated.
and 12 mm, respectively, for a 4inch (100mm) diameter wafer. The front surface, on which the epitaxy is performed, typically undergoes an elaborate cleaning and polishing process. One prerequisite for making highquality heterostructures with thin layers is a ﬂat surface. Even if the polished substrate is not perfect, ﬂat interfaces can be achieved with the growth of appropriate superlattice buffer layers (Fig. 11.3). Roughness can exist on all length scales and is typically investigated using atomic force microscopy scans. However, it is possible to create surfaces that exhibit large, essentially monoatomically ﬂat terraces between individual surface steps. Insitu monitoring is of importance to obtain information about the growth process while it is underway. Using the information in a feedback
280
11 Heterostructures
loop it is possible to achieve insitu control of the process, e.g. for precise determination of growth rates or layer thickness. Techniques are RHEED (reﬂection highenergy electron diffraction) [373] (only for UHV systems) and RAS (reﬂection anisotropy spectroscopy) [374, 375].
(a)
(b)
Fig. 11.3. Crosssectional TEM of MBEgrown Alx Ga1−x As/GaAs heterostructures for (a) x = 0.41 and (b) x = 1.0. Using an AlAs/GaAs superlattice an excellent ﬂattening of substrate roughness is achieved. From [376]
11.3 Material Combinations 11.3.1 Pseudomorphic Structures Heterostructures can generally be made from any sequence of materials. However a mismatch in lattice constant (or a different crystal structure) leads to strains and stresses that are of the order of 103 atmos for strains of 1% (σ ∼ Cǫ, C ≈ 5 × 1010 Pa) as discussed in Sect. 5.3.2. The total strain energy is ∝ Cǫ2 . Above a critical thickness dc ∝ ǫ−1 (see Sect. 5.3.6) defects, e.g. misﬁt dislocations (relaxing strain with their edge components), are generated. The crosshatch pattern due to misﬁt dislocations is shown in Fig. 11.4. There are a number of semiconductor combinations that are lattice matched and thus can be grown with arbitrary thickness. Alx Ga1−x As is closely lattice matched to GaAs for all Al concentrations. See Fig. 6.14 for latticematched pairs, e.g. In0.53 Ga0.47 As/InP. Often, thin layers of latticemismatched materials with thickness smaller than the critical thickness are used. 11.3.2 Heterosubstrates If homosubstrates are not available or very expensive, semiconductors are also grown on dissimilar substrates, e.g. GaN and ZnO on sapphire (Al2 O3 ) or SiC. For ZnO, homosubstrates have recently been produced with 3inch diameter [377]. In many cases, the integration of III–V or II–VIbased semiconductors for optoelectronic applications on silicon for electronic devices
11.3 Material Combinations
281
(b)
(a)
Fig. 11.4. Surface (a) of a supercritical, plastically relaxed and (b) of a pseudomorphic Inx Ga1−x As ﬁlm on GaAs. In (a) the crosshatch pattern is due to misﬁt dislocations along [110] and [1¯ 10]
is desirable, such as GaAs/Si, InP/Si, GaN/Si or ZnO/Si. For such combinations the epitaxial relationship, i.e. the alignment of the crystallographic directions of both materials, which can have different space groups, has to be considered [378]. Some examples are given in Table 11.1. In Fig. 11.5, Xray diffraction data are shown from a ZnO layer on coriented sapphire. The hexagonal ZnO lattice is rotated by 30◦ with respect to the trigonal sapphire lattice. In the case of growth of ZnO on Si(111) an amorphous SiOx layer forms at the interface such that the crystallographic information of the substrate is lost. The ZnO grains exhibit random inplane orientation (Fig. 11.6). Table 11.1. Epitaxial relationship for various ﬁlm/substrate combinations, ZnO (or GaN) on c, a and rsapphire and Si(111) ZnO
Al2 O3 [00.1]
ZnO
Al2 O3 [11.0]
ZnO
Al2 O3 [¯ 10.2]
ZnO / GaN
Si [111]
[00.1] [11.0]
[00.1] [01.0]
[00.1] [11.0]
[11.0] [00.1]
[11.0] [00.1]
[¯ 10.2] [0¯ 1.1]
[00.1] — / [2¯ 1.0]
[111] [¯ 110]
The initial growth steps can determine the orientation in polar materials. GaN directly grown on cAl2 O3 grows with Nface orientation (see Fig. 3.18). The high surface mobility of Ga allows nitrogen to take its preferred position in the ﬁrst atomic layer. Even under Garich conditions the N atoms can kick
282
11 Heterostructures ZnO [10.0]
Tilt (deg)
0.4
=30°
0.2 0 0.2 0.4
ZnO (1 0.4)
Tilt (deg)
0.4 0.2 0 0.2 0.4 180
Al2O3 (1 0.10) 90 0 90 Azimuthal orientation (deg)
180
Fig. 11.5. Xray diﬀraction intensity from the asymmetric ZnO (10.4) (upper panel ) and the sapphire (10.10) (lower panel ) reﬂections as a function of the azimuthal sample orientation (rotation angle φ around the [00.1] axis). The peaks appear at diﬀerent tilt angles ω due to an overall tilt of the mounted sample (dashed sinusoidal lines). The ZnO [00.1] axis is not tilted with respect to the sapphire [00.1] direction
off the Ga from its favorite site on the surface. If an AlN buffer is used the strong bond between Al and oxygen leads to an Al atomic layer at the interface and subsequent GaN grows with a Gaface [379]. On a sapphire substrate with lateral AlN patterns, laterally orientationmodulated GaN can be grown. At the juncture of the phases an inversion domain boundary forms [380]. Now, the nucleation and the initial ﬁlm growth are important and determine the ﬁlm quality. Several techniques have been developed to overcome common problems. A typical strategy is the growth of a lowtemperature nucleation layer. The defect density can be reduced in parts of the structure using epitaxial lateral overgrowth (ELO) [382]. The defects thread only from the limited contact area of the layer with the substrate and the part of the layer away from the mask (‘wing’) is free of defects (Fig. 11.8). The cracking of thick ﬁlms during cooling due to the mismatch of the thermal expansion coeﬃcients (Fig. 11.9) can be avoided by the introduction of suitable stressrelaxing layers [383, 384].
11.3 Material Combinations
283
500 nm
(a)
ZnO
Si 500 nm
(b) Si
SiOx
ZnO
(2.5 ... 3) nm
(c)
5 nm
Fig. 11.6. (a) Planview TEM image (inset: electron diﬀraction diagram averaged over several grains) of ZnO on Si(111). (b) Crosssectional TEM of the same sample. (c) Highresolution crosssectional image of the ZnO/SiOx /Si interface region
284
11 Heterostructures
(a)
180
(c)
(d)
0
phase (deg)
(b)
0
x (μm)
10
Fig. 11.7. Side view of the heterointerfaces between AlN and coriented sapphire with nitrogen (a) and Al (b) being the ﬁrst layer. Adapted from [379]. (c) Phase image of piezoresponse force microscopy (PFM) of lateral polarity GaN heterostructure. (d) Linescan of phase signal along white line in part (c), adapted from [381]. c Part (c) reprinted with permission from [381], 2002 AIP
Fig. 11.8. SEM crosssectional image of GaN grown on a structured Si(111) substrate. The laterally grown wings extend about 2.5 µm over the grooves. The thickness of the GaN layer is 0.5 µm on the bottom of the grooves, while it is 1.4 µm on c top of the ridges. Reprinted with permission from [382], 2001 AIP
11.4 Band Lineup in Heterostructures
285
Fig. 11.9. 1×1 mm2 top view with a diﬀerential interference contrast microscope of a 1.3µm thick GaN layer grown on Si(111). Reproduced with permission from [383], c 2000 IPAP
11.4 Band Lineup in Heterostructures In heterostructures, semiconductors with different bandgaps are combined. The relative position of conduction and valence band (band alignment) is determined by the electron aﬃnities as shown in Fig. 11.10. It can lead to different types of heterostructures. In Fig. 11.11, the band alignment for typeI and typeII heterostructures are shown. In the typeI structure (straddeled band lineup) the lower conductionband edge and the higher valenceband edge are both in the material with smaller bandgap. Thus, electrons and holes will localize there. In the typeII structure a staggered lineup is present and electrons and holes will localize in different materials. The technologically most relevant are typeI structures. In a typeI heterostructure, the conduction and valenceband discontinuities are given, respectively, by ΔEC = χ1 − χ2 ΔEV = (χ1 + Eg1 ) − (χ2 + Eg2 ) .
(11.1a) (11.1b)
Depending on the layer sequence of high and lowbandgap materials various conﬁgurations, as shown in Fig. 11.12 have obtained special names, such as single heterointerface, quantum well (QW), multiple quantum well (MQW), superlattice (SL). In the extreme case the layer is only one monolayer thick (Fig. 11.13) and the concept of layer and interface blurs. Such atomically precise layer sequences are mastered nowadays for a variety of material systems such as AlGaAs/GaAs/InAs, InP/InGaAs, Si/SiGe and also BaTiO3 /SrTiO3 . The design of heterostructures to fulﬁll a certain device functionality or to have certain physical properties is called ‘bandgap engineering’.
11 Heterostructures
0 1
Si Ge SiC AlN GaN InN AlP GaP InP AlAs GaAs InAs AlSb GaSb InSb ZnO ZnS CdS ZnSe CdSe ZnTe CdTe
286
Energy (eV)
2 3 4 5 6 7 8 9 Fig. 11.10. Position of conduction and valenceband edges for a variety of semiconductors. Based on values from [385]
vacuum
vacuum
(a)
2
EC Eg2
Eg1 EV Spatial coordinate
1
Electron energy
Electron energy
2 1
(b)
Eg2 Eg1
EC, V
Spatial coordinate
Fig. 11.11. Position of band edges (band alignment) in a (a) typeI and a (b) typeII heterostructure.
11.5 Energy Levels in Heterostructures 11.5.1 Quantum Well The energy in a single quantum well of thickness Lz (along the growth direction z) can be calculated with the quantummechanical particleinabox model. In the envelope function approximation (Appendix F) the wavefunction is written as a product of the Bloch function and the envelope function χ(z).
11.5 Energy Levels in Heterostructures
(a)
(b)
(d)
287
(c)
(e)
Fig. 11.12. Heterostructures with diﬀerent layer sequences (bandgap engineering). (a) quantum well (QW), (b) multiple quantum well (MQW), (c) superlattice (SL), (d) singlebarrier tunneling structure, (e) doublebarrier tunneling structure InAs
Fig. 11.13. Crosssectional TEM of a MOVPEgrown shortperiod superlattice (SPS) of InAs layers in GaAs1−x Nx . In high resolution (right image), the individual rows of atoms can be seen. The InAs layers are indicated by arrows. From [386]
Ψ A,B (r) = exp (ik⊥ r) unk (r)χn (z) ,
(11.2)
where ‘A’ and ‘B’ denote the two different materials. The envelope function χ fulﬁlls, approximately, the onedimensional Schr¨ odingertype equation,
−
2 ∂ 2 + V (z) χn (z) = En χn (z) , c 2m∗ ∂z 2
(11.3)
where m∗ denotes the effective mass. Vc is the conﬁnement potential determined by the band discontinuities. Typically, Vc = 0 in the well and V0 > 0 outside in the barrier. En are the resulting energy values of the quantized
288
11 Heterostructures
levels. In the case of inﬁnite barriers (V0 → ∞, Fig. 11.14a) the boundary conditions χ(0) = χ(Lz ) = 0 yield 2 nπ 2 En = (11.4) 2m∗ Lz
nπz χn (z) = An sin , (11.5) Lz where En is called the conﬁnement energy. For ﬁnite barrier height (Fig. 11.14b) the calculation leads to a transcendental equation
1/2
1/2 mb V 0 − E mw EL2z = , (11.6) tan 22 mw E where mw (mb ) is the effective masses in the well (barrier). The wavefunction tunnels into the barrier. While for inﬁnite barrier height the lowest level diverges for Lz → 0, for ﬁnite barrier height E1 → V0 . In the plane the carriers are still free and have a twodimensional dispersion. Thus, each quantized level contributes m∗ /(π2 ) (6.72) to the density of states at each subband edge En .
n=3
(a)
Lz
n=2
n=2
n=1
n=1
(b)
Lz
Fig. 11.14. Schematic energy levels and wavefunctions in (a) a potential well with inﬁnite barriers, and (b) for ﬁnite barrier height
For holes, the situation is a little more complicated than that for electrons (Fig. 11.15). First, the degeneracy of heavy and light holes is lifted since their mass enters the conﬁnement energy. The effective hole masses along the z direction, i.e. those that enter (11.3), are 1 = γ1 − 2γ2 mzhh 1 = γ1 + 2γ2 . mzlh
(11.7a) (11.7b)
11.5 Energy Levels in Heterostructures
289
Fig. 11.15. Schematic representation of the development of hole levels in a quantum well: (a) bulk, (b) splitting at the subband edge, (c) dispersion (mass reversal), (d) anticrossing behavior. From [376]
The light holes have the higher quantization energy. The angular momentum is quantized along the z direction. The transverse masses for the dispersion in the interface plane are 1 = γ1 + γ2 mxy hh 1 = γ1 − γ2 . mxy lh
(11.8a) (11.8b)
Now the heavy hole, i.e. the Jz = ± 23 state, has the smaller mass and the light hole (Jz = ± 21 ) the larger (Fig. 11.15c). However, this consideration is only an approximation since the lifting of degeneracy and the dispersion have to be treated on the same level. Higher terms of the perturbation calculation lead to band mixing and remove the band crossing that seems to originate from the situation at the Γ point. In reality, the bands show anticrossing behavior and are strongly deformed. The hole dispersion in a superlattice and the anticrossing behavior is shown in Fig. 11.16. Experimentally observed transition energies in quantum wells of varying thickness are shown in Fig. 11.17 and are in good agreement with the theoretical calculation. We note that for inﬁnite barriers optical transitions are only allowed between conﬁned electron and hole states with the same quantum number n. For ﬁnite barriers this selection rule becomes relaxed, and other transitions become partially allowed, e.g. e1 –hh3 . The optical matrix element from the Bloch part of the wavefunction, which was isotropic for (cubic) bulk
290
11 Heterostructures 0
hh1
Subband energy (meV)
hh2
10
GaAs/ AlGaAs
lh1
hh3
20
hh4 lh2
30
0.04 0.03 0.02 0.01 0 0.01 0.02 0.03 0.04 [100] [110] Transverse electron wavevector (2/a)
Fig. 11.16. Hole dispersion in a 68ML GaAs/71 ML Al0.25 Ga0.75 As superlattice (numerical calculation). The double curves originate from a lifting of timereversal c symmetry at k = 0. Reprinted with permission from [387], 1985 APS
Ee nh m Ee 1h h 1(meV)
200 100 70 50
e6hh6
30 20
e4hh4
10 7 5
e2lh2
3 2 1 3
e5hh5
e3hh3
e2hh2 e1hh3
GaAs/AlGas
e1lh1
e1hh2
5 7 10 20 30 50 70 100 QW thickness (nm)
Fig. 11.17. Observed electron–hole transitions (energy diﬀerence to the ﬁrst e–h transition from excitation spectroscopy) in GaAs/AlGaAs quantum wells of varying thickness. Lines are theoretical model. Data from [389]
material (9.16), is anisotropic for quantum wells. TE (TM) polarization is deﬁned with the electromagnetic ﬁeld in (perpendicular to) the plane of the quantum well (Fig. 11.18a). At the subband edge, i.e. for inplane wavevector k = 0 the matrix elements for the various polarizations and propagation directions are given in Table 11.2. The matrix elements averaged over all in
11.5 Energy Levels in Heterostructures mj
1/2
1/2
291
electrons
TM
TE mj
TE (b)
(a)
3/2 hh
1/2
1/2
lh
lh
3/2
holes
hh
Fig. 11.18. (a) Directions of electricﬁeld vector relative to the quantumwell plane for TE and TM polarization. (b) Optical selection rules for band–band transitions in a quantum well. If the (inplane averaged) relative strength of the e–hh transitions (solid lines) is 1, the relative strength of the TEpolarized e–lh transitions (dashed lines) is 1/3 and that of the TMpolarized e–lh transitions (dashdotted lines) is 4/3 Table 11.2. Squared momentum matrix elements cˆ e · pv2 in a quantum well 2 for various propagation directions in units of Mb . The quantumwell normal is along z propagation
ˆ ex (TE)
ˆ ey (TE)
ˆ ez (TM)
e–hh
x y z
– 1/2 1/2
1/2 – 1/2
0 0 –
e–lh
x y z
– 1/6 1/6
1/6 – 1/6
2/3 2/3 –
e–so
x y z
– 1/3 1/3
1/3 – 1/3
1/3 1/3 –
plane directions for TEpolarization are 3/2Mb2 (1/2Mb2 ) for the electron to heavy (light) hole transition. For TM polarization the values are 0 and 2Mb2 , respectively [388]. The optical selection rules are shown in Fig. 11.18 (cf. Fig. 9.8 for bulk material). For propagation along the quantumwell plane, the ratio between the strength of the TE polarized e–hh and e–lh transitions is 3:1. The conﬁnement potential squeezes charge carriers bound to impurities closer to the ion. Therefore, the binding energy increases as shown in Fig. 11.19. This behavior can be modeled theoretically with good precision.
11 Heterostructures C acceptor binding energy (meV)
292
GaAs/Al0. 3Ga0. 7As
40
35
30
25
0
5
10 15 20 25 30 Quantum well width (nm)
35
Fig. 11.19. Experimental values for the acceptor binding energy in GaAs/Al0.3 Ga0.7 As quantum wells (solid circles) from [390] as a function of well width. Solid line is theory (variational calculation) for the wellcenter acceptor including top four valence bands and ﬁnite barriers, dashed line is hydrogenlike model with inﬁnite barrier height. Adapted from [391]
15 Al0.4Ga0.6As/GaAs
10
5 0
(a)
mbmw , b w mbmw , b= w mb=mw , b w mb=mw , b= w
Exciton binding energy (meV)
X(e,hh) binding energy (meV)
It makes a difference whether the impurity is located at the center or the interface of the quantum well. The conﬁnement potential also squeezes electrons and holes in the exciton closer together and thus increases their Coulomb interaction. The binding energy of the quantumwell exciton is thus larger than in bulk material and depends on the well width (Fig. 11.20). In the simple hydrogenlike model with inﬁnite barriers the exciton binding energy is 4 times the bulk binding
10 15 5 Quantum well thickness Lz (nm) (b)
InGaAs/ GaAs
10 9 8 7 6 0
5 10 Well width (nm)
Fig. 11.20. (a) Theoretical (variational) calculation (solid line) of the heavyhole exciton binding energy vs. QW thickness in a GaAs/Al0.4 Ga0.6 As quantum well (using also diﬀerent approximations, other lines). Adapted from [392]. (b) Experimental exciton binding energy in Inx Ga1−x As/GaAs quantum wells of diﬀerent thickness. Circles: data and error bars from [393], x unspeciﬁed, squares: data from [394], x = 0.18
11.5 Energy Levels in Heterostructures
293
energy in the limit Lz → 0. In a realistic calculation the effect of different dielectric constants in the well and barrier (image charge effect) need to be considered. 11.5.2 Superlattices In a superlattice, the barrier thickness is so small that carriers can tunnel in neighboring wells or, in other terms, that there exists a signiﬁcant wavefunction overlap between adjacent wells. This leads to a band structure (Fig. 11.21), similar to the Kronig–Penney model (Sect. 6.4). For the superlattice the bands are called minibands, the gaps are called minigaps. The density of states does not make a step at the subband edge but follows an arccos function. The modiﬁcation of the density of states, as seen in the absorption spectrum, are shown in Fig. 11.22 for 1, 2, 3 and 10 coupled wells. 0.45 0.40 E4
0.35
Energy (eV)
0.30 0.25
E3
0.20 0.15 E2
0.10 0.05
E1 0 0
1
2
3
4
5 6 w (nm)
7
8
9
10
Fig. 11.21. Band structure of a superlattice with a potential depth of 0.4 eV and well and barrier width w (LQW = Lbarr ). Adapted from [395]
11.5.3 Single Heterointerface Between Doped Materials We consider a single heterointerface between ndoped materials. As an example we take nAlGaAs/nGaAs (Fig. 11.23). First, we consider the materials without contact, forming a typeI structure. In thermodynamic equilibrium the system must have a constant Fermi level. Thus, charge is transferred from the region close to the interface from AlGaAs to GaAs. This results in the formation of a triangular potential well in the GaAs close to the interface. A twodimensional electron gas (2DEG) forms in this potential well (Fig. 11.24). The charge transfer in thermodynamic equilibrium adjusts the
294
11 Heterostructures Lz
1.5
Lz
LB
1 QW Lz=5.0nm
3 QW's Lz=6.0nm LB=1.6nm
1.0
Optical density
lh
hh
0.5 0
LB
Lz
1.0 lh
2 QW's Lz=5.0nm LB=1.5nm
10 QW's Lz=4.2nm LB=1.2nm
1.70
1.55
hh
0.5 0
1.55
1.60
1.65
1.60
1.65
1.70
Photon energy (eV) Fig. 11.22. Absorption spectra of a single, double, triple and ten coupled quantum wells. Theoretically predicted transitions with heavy (light) holes are labeled with ﬁlled (empty) bars at their respective transition energies. Adapted from [396]
band bending and the charge density (quantized levels in the well) in such a way that they are selfconsistent. The Poisson equation and the Schr¨ odinger equation are simultaneously fulﬁlled. Numerically, both equations are iteratively solved and the solution is altered until it is selfconsistent, i.e. it fulﬁlls both equations.
AlGaAs
Ec
GaAs
Ec
Ev
Ev (a)
(b)
Fig. 11.23. Schematic formation of a triangular potential well in a nAlGaAs/nGaAs heterostructure, (a) before and (b) after equilibration of Fermi levels
11.6 Recombination in Quantum Wells
295
Fig. 11.24. (a) Conductionband edge at a GaAs/Al0.3 Ga0.7 As heterointerface (T = 0 K) with two conﬁned states at E0 and E1 marked with solid horizontal lines. In the GaAs channel there are 5 × 1011 cm−2 electrons. The barrier height is GaAs 300 meV, ND = 3 × 1014 cm−3 . The position of the Fermi level EF is at E = 0 and indicated with a dashdotted line. (b) Envelope wavefunctions φ0 and φ1 of the two conﬁned states, dashdotted line: calculation without exchange and correlation for state at E0 . Adapted from [398]
If the region of the 2DEG is not doped, the electron gas exists without any dopant atoms and ionized impurity scattering no longer exists. This concept is called modulation doping. Mobilities up to 3.1×107 cm2 /V s have been realized (Fig. 11.25). The theoretical limits of mobility in a 2DEG at modulationdoped AlGaAs/GaAs heterointerfaces are discussed in detail in [397].
11.6 Recombination in Quantum Wells The energy of exciton recombination in quantum wells is blueshifted with respect to that in bulk material due to the quantumconﬁnement energies of electrons and holes (Fig. 11.26). The electron–hole recombination lineshape in quantum wells is given by the product of the joint density of states and the Boltzmann function (when Boltzmann statistics apply). The JDOS is given by a step function (Heavyside function H(E)).
E I(E) ∝ H(E − E11 ) exp − , (11.9) kT where E11 = Eg + Ee1 + Eh1 represents the energy separation of the E1–H1 subband edges as shown in Fig. 11.26. An experimental spectrum
296
11 Heterostructures
Fig. 11.25. Progress in the achievement of high electron mobility in GaAs, annotated with the technical innovation responsible for the improvement. Reprinted c from [399], 2003, with permission from Elsevier
(Fig. 11.27a) shows that excitonic effects inﬂuence the recombination lineshape even at room temperature [400]. At high carrier densities when the electron (quasi) Fermi level is above the electron subband edge, the spectrum broadens and reﬂects the Fermi– Dirac distribution (Fig. 11.27b). At low temperatures a manybody effect, multiple electron–hole scattering with electrons at the Fermi edge, leads to an additional peak, termed Fermiedge singularity that is discussed in [401]. Inhomogeneous broadening effects the recombination lineshape. Since the interfaces of the QW are not ideally ﬂat, the exciton averages over different quantumwell thicknesses within its volume. Also, e.g. for the GaAs/AlGaAs system, the wavefunction in the (binary) quantum well tunnels into the barrier, the amount depending on the QW width, and there ‘sees’ the alloy broadening (see Sect. 10.5). The problem of exciton dynamics in a potential with random ﬂuctuations has been treated in detail [402, 403]. A simpliﬁed picture is as follows: At low temperatures the excitons populate preferentially the potential minima. A simple lineshape1 of the QW absorption or joint density of states is given by a step function (cf. Table 9.2) 1
neglecting excitonic enhancement
11.6 Recombination in Quantum Wells
297
AlGaAs QW1 AlGaAs
E
QW2
Ee2
GaAs AlGaAs
Ee1
GaAs substrate
EC (b)
Egbarr
Eh1 Eh2
EV
(c) PLintensity (arbitrary units)
Eg E11 E22
QW2
QW1 AlGaAs *1000
1.5
(a)
GaAs/AlGaAs
1.6
1.7 Energy (eV)
1.8
1.9
Fig. 11.26. (a) Schematic energy diagram of a quantum well with conﬁned electron (e1, e2) and hole (h1, h2) states and recombination between them at energies E11 and E22 . (b) Schematic sample structure with two GaAs/Alx Ga1−x As quantum wells with thicknesses 3 nm and 6 nm. (c) Photoluminescence spectrum (T = 300 K) of the structure from part (b). A small amount of barrier luminescence appears at 1.88 eV, according to x = 0.37 (cf. Fig. 6.13c)
at the QW band edge E0 . The inhomogeneous broadening has a Gaussian probability distribution p(δE) ∝ exp[−(δE)2 /2σ 2 )] with δE being the deviation from the QW band edge δE = E − E0 . The resulting lineshape is given by the convolution of the Gaussian with the unperturbed absorption spectrum yielding an errorfunctionlike spectrum2 as shown in Fig. 11.28a. For complete thermalization the level population is given by the Boltzmann function. The recombination spectrum is given by the product of the absorption spectrum (or JDOS) and the Boltzmann function. It is (red) shifted with respect to E0 by about3 ΔE(T ) = −σ 2 /kT .
(11.10)
This shift between emission and absorption is also called the Stoke’s shift. z The error function is deﬁned as erf(x) = √2π 0 exp −t2 dt. 3 Formula (11.10) is exact for the product of a Gaussian and the Boltzmann function. 2
298
11 Heterostructures
Photoluminescence intensity (arb. units)
InGaAs/InP
104
PL Intensity (arb. units)
GaAs/AlGaAs 103
10
2
10
1
T=80K
T=25K
E11
44.1 meV T=4.7K
10
(a)
0
1.50
1.55
1.60 Energy (eV)
1.65
1.70
0.82
(b)
0.84
0.86 0.88 Energy (eV)
0.90
0.92
Fig. 11.27. (a) Photoluminescence spectrum of a 5nm GaAs/AlGaAs quantum well at T = 300 K. The solid (dashed) line is ﬁt with (without) excitonic eﬀects. The two peaks are due to transitions involving heavy and light holes. Adapted from [400]. (b) Photoluminescence spectra at three diﬀerent temperatures as labeled of a 10nm modulationdoped InGaAs/InP quantum well with an electron sheet density ns = 9.1 × 1011 cm−2 . The electron quasiFermi level is Fn − (EC + Ee1 ) = 44.1 meV from the subband edge. The dashed line in the T = 80 K spectrum is the lineshape from JDOS and a Fermi–Dirac distribution without enhancement at the Fermi edge. Adapted from [401]
Within their lifetime, limited at least by radiative recombination, the excitons are typically unable to reach the energy position required by the Boltzmann function, but only a local minimum. Thus, their thermalization may be incomplete due to insuﬃcient lateral diffusion. This effect is particularly important at low temperatures when thermal emission into adjacent deeper potential minima is suppressed. In this case the redshift is smaller than expected from (11.10). A numerical simulation [402] yields such behavior of the energy position of the recombination line as shown in Fig. 11.28b. Simultaneously, the width of the recombination spectrum also exhibits a minimum (Fig. 11.28c). These ﬁndings are in agreement with experiments [404, 405]. A potential ﬂuctuation can localize an exciton laterally at low temperatures [400] and behave like a quantum dot (see Sect. 13.3). Localized and delocalized excitons are separated by a boundary called the mobility edge [406]. The transition between the two regimes is a Mott transition [407]. Under certain growth conditions, quantum wells with piecewise very ﬂat interfaces can be fabricated. The thickness difference between such regions (with lateral extension in the µm range) is an integer monolayer. Accordingly, the recombination spectrum yields several, typically two or three, discrete lines.
11.7 Isotope Superlattices
299
(a)
(b)
(c)
Fig. 11.28. (a) Recombination spectra (solid lines, scaled to same height) of a model quantum well for diﬀerent temperatures as labeled and complete thermalization, dashed (dashdotted) line is unperturbed (inhomogeneously broadened by σ = 20 meV) shape of the QW absorption edge. The energy scale is relative to the energy position of the unperturbed QW absorption edge at E0 . (b) Theoretical energy position and (c) linewidth of exciton recombination from a model disordered quantum well. The hightemperature limits are marked by arrows. Parts (b,c) adapted from [402]
11.7 Isotope Superlattices A special type of heterostructure is the modulation of the isotope content. The ﬁrst kind of heterostructures made like this were 70 Gen /74 Gen symmetric superlattices [408]. Figure 11.29 shows phonon energies determined from Raman spectroscopy for various layer numbers n. The modes are classiﬁed by 70 LOm and 74 LOm denoting the material in which the amplitude is maximal and m being the number of maxima in that medium.4 Such modes are visualized in Fig. 11.30a for a (69 GaP)16 /(71 GaP)16 superlattice. Theoretical mode energies as a function of the superlattice period are shown in Fig. 11.30b. 4
Only modes with odd m are Ramanactive.
300
11 Heterostructures
320
Phonon energy (cm1)
70
74
Gen/ Gen SL
70
LO1 LO3 LO5 70 LO7 74 LO1 74 LO3 74 LO5
310
70
70
300
70 Ge alloy 74
Ge
290 280 270 0
10 20 30 Layer thickness n (ML)
40
bulk
Fig. 11.29. Measured (full circles) and theoretical (solid lines) conﬁned LO phonon energies in 70 Gen /74 Gen superlattices vs. the layer thickness (number of monolayers) n. The dashed lines represent a calculation that considers intermixing at the interfaces. On the right, the energies of bulk modes for isotopically pure 70 Ge and 74 Ge are shown together with that of an 70 Ge0.5 74 Ge0.5 alloy. Adapted from [408]
11.8 Wafer Bonding Wafer bonding is a fairly recently developed method to join different and dissimilar materials. Two wafers of the respective materials are put together face to face and are adequately fused. The idea is to not only ‘glue’ the wafers together with a sticky (and compliant) organic material, but to form strong atomic bonds between the two materials with possibly a perfect interface. In some cases, the interface needs to allow chargecarrier transport through it. Less stringent conditions need to be met for photon transport. Mechanical deﬁciencies such as surface roughness, dust particles and the like must be avoided in the waferbonding process since they result in voids. Several methods have been developed for bonding various materials [96, 97]. Such processes are successful for large substrate sizes. With proper processing, ideal interfaces can be created, as shown in Fig. 11.31. Such structures, if made between a pdoped and a ndoped semiconductor, show diode characteristics.
11.8 Wafer Bonding
(a)
301
(b)
Fig. 11.30. (a) Atomic displacements [Ga (ﬁlled dots) and P (open circles)] of oddindex LO modes in a (69 GaP)16 /(71 GaP)16 superlattice unit cell. These modes have even parity with respect to midlayer planes, which are at atom numbers 16 and 48 in this example. The labels on the left identify the predominant character of the mode, those on the right give the relative Raman intensities with respect to that of the 69 LO1 mode. The tick marks on the vertical axis indicate zero displacement of the respective mode. (b) Upper panel : Energies and characters of oddindex LO phonon modes in GaP isotope SLs as calculated within the planar bond charge model for the case of ideal interfaces. 69 LOm modes are shown as open symbols; 71 LOm modes as full symbols. The shaded area marks n = 16 for which the atomic displacements of the modes are shown in part (a). Lower panel : Calculated intensities of the modes relative to that of the 69 LO1 phonon mode. Adapted from [95], reprinted c with permission, 1999 APS
Fig. 11.31. Highresolution TEM images of waferbonded (a) SiSi and (b) GaAsSi interfaces. White circles indicate the position of misﬁt dislocations. Part (a) c reprinted from [98], 2003, with permission from Elsevier. Part (b) reprinted with c permission from [99], 1998 AIP
12 External Fields
The energy levels of the solid and its optical and electronic properties depend on external electric and magnetic ﬁelds. In high magnetic ﬁelds and at low temperatures the quantum Hall effects give evidence for new states of matter in manybody systems.
12.1 Electric Fields 12.1.1 Bulk Material The centerofmass motion of the exciton is not inﬂuenced by an electric ﬁeld. The Hamilton operator for the relative motion of an electron–hole pair of reduced mass μ along z in the presence of an electric ﬁeld E along the z direction is 2
ˆ = − Δ − eEz . H 2μ
(12.1)
Here, the Coulomb interaction, leading to the formation of bound exciton states, is neglected. In the plane perpendicular to the ﬁeld (here the z direction) the solutions for the relative motion are just plane waves. In the electric ﬁeld the bands are tilted (Fig. 12.1), i.e. there is no longer an overall bandgap. Accordingly, the wavefunctions are modiﬁed and have exponential tails in the energy gap. After separation of the motion in the (x,y) plane the Schr¨ odinger equation for the motion in the z direction is
2 2 d − eEz − Ez φ(z) = 0 , (12.2) − 2μ dz 2 which is of the type d2 f (ξ) − ξf (ξ) = 0 , dξ 2
(12.3)
2 2 2 1/3 1/3 − z 2μe and the optoelectronic energy Θ = e E2μ . 2 E The solution of (12.3) is given by the Airy function Ai (see Fig. 12.2):
with ξ =
Ez Θ
304
12 External Fields
E=0 e2
e2
e1
e1
h
EC h
E0
h
Eg h1
EV (b)
(a)
h1 h2 h3 h4
h2 h3 h4
h5
h5
Fig. 12.1. Impact of an electric ﬁeld on (a) bulk material (tilt of bands) and (b) a quantum well (quantum conﬁned Stark eﬀect, QCSE)
0.4 0.5 0.2 0
0
0.5
0.2 0.4
(a)
10
8
6
4
2
0
2
4
(b)
1 10
8
6
4
2
0
2
4
Fig. 12.2. (a) Airy function Ai(x), (b) Ai’(x)
φEz (ξ) =
(eE)1/2 Ai(ξ) . Θ
(12.4)
The prefactor guaranties the orthonormality (with regard to the Ez ). The absorption spectrum is then given by α(ω, E) ∝
% 1 1/2 $ 2 Θ π Ai (η) − ηAi2 (η) , ω
(12.5)
with η = (Eg − E)/Θ and Ai′ (x) = dAi(x)/dx. Optical transitions below the bandgap become possible that are photonassisted tunneling processes. The belowbandgap transitions have the form of an exponential tail. Additionally, oscillations develop above the bandgap, the socalled Franz–Keldysh oscillations (FKO) (Fig. 12.3a).
12.1 Electric Fields
305
The absorption spectrum scales with the optoelectronic energy Θ. The energy position of the FKO peaks En is periodic with (ν ∼ 0.5) 3/2
(En − Eg )
∝ (n − ν)Eμ−1/2 .
(12.6)
A nonperiodicity can indicate a nonparabolicity of the mass. For a given mass the electric ﬁeld strength can be determined. Wellpronounced oscillations are only present for homogeneous ﬁelds.
30
0.10
ehh
25
(103 cm1)
0.05
=(E)(0)
0 2
0.005
4
0 3
0.005
5
elh
15 10 5
0.3V 0.2V 0V
0.5V
2.0V
1
0.80 (a)
20
0.84 0.88 E (eV) (b)
InGaAs
0 0.80 0.81 0.82 0.83 0.84 Energy (eV)
Fig. 12.3. (a) Theoretical absorption (top panel ) with (solid line) and without (dashdotted line) electric ﬁeld for a volume semiconductor (without Coulomb interaction) and theoretical change of absorption (bottom panel ). (b) Experimental absorption spectra of InGaAs on InP at T = 15 K for various applied voltages as labeled. Adapted from [410]
Experimental spectra show additionally the peaks due to excitonic correlation (Fig. 12.3b) at low ﬁeld strength. At higher ﬁelds the FKO evolve and the amplitude of the excitonic peaks decreases because the excitons are ionized in the ﬁeld. 12.1.2 Quantum Wells In a quantum well an electric ﬁeld along the conﬁnement direction (z direction) causes electrons and holes to shift their mean position to opposite interfaces (Fig. 12.1b). However, excitons are not ionized due to the electric ﬁeld. With increasing ﬁeld (for both ﬁeld directions) the energy position of the absorption edge and the recombination energy is reduced. This is the
306
12 External Fields
AlGaAs/ GaAs
(i)
(iii)
(iv) (v)
1.42
(a)
(ii)
Absorption coefficient (arb. units)
Absorption coefficient (arb. units)
quantum conﬁned Stark effect (QCSE). Corresponding experimental data are shown in Fig. 12.4a(i–v). The shift depends quadratically on the electric ﬁeld since the exciton has no permanent dipole moment (mirror symmetry of the quantum well). Thus, only the secondorder Stark effect is present in which the ﬁeld ﬁrst induces a dipole p = αE. This dipole interacts with the ﬁeld with an energy E = −p · E = −αE 2 .
1.46 Energy (eV)
AlGaAs/ GaAs
1.43
1.50
(b)
(iii)
(ii) (i)
1.45 Energy (eV)
1.47
Fig. 12.4. Impact of electric ﬁelds on the absorption spectrum of a 9.4nm AlGaAs/GaAs quantum well. (a): Electric ﬁeld along the [001] growth direction, (i)– (v): E = 0, 0.6, 1.1, 1.5, and 2 × 105 V/cm. (b): Electric ﬁeld within the interface plane, (i,ii,iii): E = 0, 1.1, and 2×105 V/cm
If the ﬁeld is within the quantumwell interface plane, the ﬁeld leads to the ionization of excitons. The loss of the excitonic peak is visualized in the spectra in Fig. 12.4b(i–iii).
12.2 Magnetic Fields In magnetic ﬁelds, electrons (or holes) perform a cyclotron motion with frequency ωc = eB/m∗ , i.e. a motion perpendicular to the magnetic ﬁeld on a line of constant energy in kspace. This line is the intersection of a plane perpendicular to the magnetic ﬁeld and the respective isoenergy surface in kspace. For semiconductors with anisotropic mass, such as Si and Ge, the quantum theory of cyclotron resonance has been given in [409]. The ‘free’ cyclotron motion can only occur between two scattering events. Thus, a signiﬁcant cyclotron motion and the connected magnetotransport properties are only possible when –
ωc τ ≫ 1, i.e. when the average scattering time τ is suﬃciently large. This requires high mobility.
12.2 Magnetic Fields
307
– the magnetic ﬁeld is suﬃciently strong and the temperature suﬃciently low, i.e. ωc ≫ kT , such that thermal excitations do not scatter electrons between different Landau levels. – the cyclotron path is free of geometric obstructions. An external magnetic ﬁeld also produces a splitting of the spin states. For the electron, the energy splitting ΔE is given by ΔE = ge∗ μB B ,
(12.7)
where B is the magneticﬁeld amplitude and ge∗ the (effective) electron gfactor. This value differs from the freeelectron value in vacuum of ge = 2.0023 due to the presence of spinorbit interaction. Values for ge∗ at low carrier density and low temperatures are 2 for Si, 1.2 for InP and ZnSe, −1.65 for CdTe, −0.44 for GaAs, and −50 for InSb. In [411] the temperature dependence of ge∗ in GaAs, InP and CdTe is also measured and discussed. The electron gfactor increases in thin GaAs/AlGaAs quantum wells [412]. 12.2.1 FreeCarrier Absorption The absorption of free carriers was treated in Sect. 9.6 without the presence of a static magnetic ﬁeld. Solving (8.19) for a static magnetic ﬁeld B = μ0 H with H = H (hx , hy , hz ) and a harmonic electric ﬁeld E ∝ exp(−iωt) yields for the dielectric tensor (cf. (9.50)) ǫ=
i σ, ǫ0 ω
by comparing j = σE = qN v ⎡
⎛
⎞⎤−1 0 −hz hy ǫ(ω) = −ωp∗2 ⎣(ω 2 + iωγ)1 − iωc ⎝ hz 0 −hz ⎠⎦ , −hy hz 0
(12.8)
(12.9)
where 1 denotes the (3 by 3) unity matrix and γ = 1/τ = m∗ μ/q is the damping parameter with μ representing the optical carrier mobility. The (unscreened) plasma frequency is given by e2 . ǫ0 m∗
(12.10)
μ0 H . m∗
(12.11)
ωp∗2 = n The freecarrier cyclotron frequency is ωc = e
If the effective mass is treated as a tensor, 1/m∗ is replaced by m∗ −1 in (12.10) and (12.11). For zero magnetic ﬁeld the classical Drude theory for one carrier species is recovered (cf. (9.52a))
308
12 External Fields
ǫ(ω) = −
ωp∗2 . ω(ω + iγ)
(12.12)
With the magnetic ﬁeld perpendicular to the sample surface, i.e. B = μ0 (0, 0, H) the magnetooptic dielectric tensor simpliﬁes to (cf. (8.20d)) ⎛ ⎞ ǫ˜xx i˜ ǫxy 0 −ωp∗2 ⎝ −i˜ ǫxy ǫ˜xx 0 ⎠ ǫ(ω) = ω2 0 0 ǫ˜zz 1 + iγ/ω (1 + iγ/ω)2 − (ωc /ω)2 1 = (1 + iγ/ω) ωc /ω = . (1 + iγ/ω)2 − (ωc /ω)2
(12.13a)
ǫ˜xx =
(12.13b)
ǫ˜zz
(12.13c)
ǫ˜xy
(12.13d)
The inplane component ǫxx provides information about ωp∗ and γ, i.e. n and μ, the effective mass, are known. Additionally, the antisymmetric tensor component ǫxy is linear in the cyclotron frequency and provides q/m. This subtle but ﬁnite birefringence depends on the strength (and orientation) of the magnetic ﬁeld and can be experimentally determined in the infrared using magnetoellipsometry [413, 414]. Such ‘optical Hall effect’ experiment allows the determination of the carrier density n, the mobility μ, the carrier mass1 m∗ and the sign of the carrier charge sgn(q) with optical means. The electrical Hall effect (Sect. 8.4) can reveal n, μ and sgn(q) but cannot reveal the carrier mass. 12.2.2 Energy Levels in Bulk Crystals In a 3D electron gas (the magnetic ﬁeld is along z, i.e. B = [0, 0, B]) the motion in the (x, y) plane is described by Landau levels. Quantum mechanically they correspond to levels of a harmonic oscillator. The magnetic ﬁeld has no impact on the motion of electrons along z, such that in this direction a free dispersion relation ∝ kz2 is present. The energy levels are given as
2 2 1 k . Enkz = n + (12.14) ωc + 2 2m z Thus, the states are on concentric cylinders in kspace (Fig. 12.5a). The populated states of the 3D electron gas (at 0 K) lie within the Fermi vector of length kF . For the 3D system the density of states at the Fermi energy 1
We note that mobility and eﬀective mass deﬁned and measured in this way may be referred to as ‘optical’. Other deﬁnitions and approaches to the mobility or eﬀective mass may give diﬀerent results.
12.2 Magnetic Fields
309
is a square root function of the Fermi energy (6.70). In the presence of a magnetic ﬁeld the density of states diverges every time that a new cylinder (with a onedimensional density of states, (6.74)) touches the Fermi surface at EF . In real systems, the divergence will be smoothed, however, a pronounced peak or the periodic nature of the density of states is often preserved. kz
B
hc
n=0 n=1 n=...
3D
n=nm
ky
kx EF (a)
(b)0
1/2
3/2
5/2
7/2 EF
E
Fig. 12.5. 3D electron gas in an external magnetic ﬁeld. (a) Allowed states in kspace for magnetic ﬁeld along the z direction. (b) Density of states (DOS) ρ vs. energy (in units of ωc ). Dashed line is threedimensional DOS without magnetic ﬁeld. Based on [376]
The period is given by the number nm of cyclotron orbits (Landau levels) within the Fermi surface.
1 nm + ωc = EF . (12.15) 2 If the number of carriers is constant, the density of states at the Fermi energy at varying the condi magnetic ﬁeldvaries periodically eB with 1/B. From 1 1 1 1 1 2 = E and n + 1 + = E with = tions nm + 21 eB F m F m 2 m B2 B1 + ΔB we ﬁnd e 1 = ∗ . ΔB m EF
(12.16)
This periodicity is used to determine experimentally, e.g., the properties of the Fermi surface in metals using the Shubnikov–de Haas oscillations (of the magnetoresistance) or the de Haas–van Alph´en effect (oscillation of the magnetic susceptibility). 12.2.3 Energy Levels in a 2DEG In a 2D electron gas (2DEG), e.g. in a quantum well or a potential well at a modulationdoped heterointerface, a free motion in z is not possible and
310
12 External Fields
ky
hc
2D
kx n=0 n=1 n=2 (a)
EF(0)
(b)
E1 E1+hc/2
E EF(0)
Fig. 12.6. 2D electron gas in an external magnetic ﬁeld. (a) Allowed states in kspace. (b) Density of states (DOS) ρ vs. energy. Dashed line is twodimensional DOS without magnetic ﬁeld. Thick vertical lines: δlike DOS without broadening, curves: broadened DOS. Based on [376]
kz is quantized. The energy levels (for each 2D subband) are only given by the cyclotron energy (Fig. 12.6a). The density of states is a sequence of δlike peaks (Fig. 12.6b). Each peak contributes (degeneracy gˆ of a Landau level) a total number of gˆ =
eB h
(12.17)
states (per unit area without spin degeneracy and without the degeneracy of the band extremum). In reality, disorder effects lead to an inhomogeneous broadening of these peaks. The states in the tails of the peaks correspond to states that are localized in real space. Also, in a 2D system several physical properties exhibit an oscillatory behavior as a function of Fermi level, i.e. with varying electron number, and as a function of the magnetic ﬁeld (periodic with 1/B) at ﬁxed Fermi energy, i.e. at ﬁxed electron number (Fig. 12.7). 12.2.4 Shubnikov–de Haas Oscillations From the 2D density of states (per unit area including spin degeneracy) D2D (E) = m∗ /π2 (6.72) the sheet density of electrons ns can be expressed as a function of the Fermi level (at T = 0 K without spin degeneracy) ns =
m∗ (EF − EC ) . 2π2
(12.18)
Using (12.16) we thus ﬁnd (without spin degeneracy, without valley degeneracy), that the period of 1/B is ∝ ns :
Specific heat (arb. units)
Magnetization (arb. units)
Fermi energy (meV)
12.2 Magnetic Fields
35
(a)
30 25 30 (b) 20 10 0 10 20 30 15 (c) 10 5 0
Thermoelectric power (arb. units)
311
(d)
0.3 0.2 0.1 0 0
2 4 6 8 Magnetic field (T)
10
Fig. 12.7. Oscillatory (theory, T = 6 K) behavior of a 2DEG (GaAs/AlGaAs) in a magnetic ﬁeld: (a) Fermi level, (b) magnetization, (c) speciﬁc heat, (d) thermoelectric power. A Gaussian broadening of 0.5 meV was assumed. Adapted from [376,415]
e 1 = ns . ΔB h
(12.19)
The carrier density of a 2DEG can therefore be determined from the oscillations of magnetoresistance, and is proportional to the density of states at the Fermi level (Shubnikov–de Haas effect). A corresponding measurement with varying ﬁeld and ﬁxed electron density is shown in Fig. 12.8. The periodicity with 1/B is obvious. Since only the component of the magnetic ﬁeld
12 External Fields Magnetoresistance (arb. units)
312
H layers
AlGaAs/GaAs
H  layers
0
2
4 H (T)
6
8
Fig. 12.8. Shubnikov–de Haas oscillations at a modulationdoped AlGaAs/GaAs heterostructure with a 2DEG, n = 1.7 × 1017 cm−2 and μ = 11 400 cm2 /V s. Data from [416]
perpendicular to the layer affects the (x, y) motion of the carriers, no effect is observed for the magnetic ﬁeld parallel to the layer. In another experiment the carrier density was varied at constant ﬁeld (Fig. 12.9). The electron density in an inversion layer in ptype silicon is (linearly) varied with the gate voltage of a MOS (metal–oxide–semiconductor) structure (inset in Fig. 12.9, for MOS diodes see Sect. 21.5). In this experiment, the Fermi level was shifted through the Landau levels. The equidistant peaks show that indeed each Landau level contributes the same number of states.
Conductance (arb. units)
aluminum gate oxide n+
n+ silicon
0
20
40 60 Gate voltage (V)
80
100
Fig. 12.9. Shubnikov–de Haas oscillations of a 2DEG at the (100) surface of ptype silicon (100 Ω cm) at a magnetic ﬁeld of 33 kOe and T = 1.34 K. The inset shows schematically the contact geometry. Data from [417]
12.3 Quantum Hall Eﬀect
313
12.3 Quantum Hall Effect In high magnetic ﬁelds, at low temperatures and for highmobility, 2D electron gases exhibit a deviation from the classical behavior. We recall that the classical Hall effect (i.e. considering the Lorentz force, classical Drude theory), the generation of a ﬁeld Ey perpendicular to a current ﬂow jx (see Sect. 8.4), was described with the conductivity tensor σ (here, for the (x, y)plane only)
σ0 1 ωc τ (12.20a) σ= 1 + ωc2 τ 2 −ωc τ 1 1 →0 (12.20b) σxx = σ0 1 + ωc2 τ 2 ωc τ ne σxy = σ0 → , (12.20c) 1 + ωc2 τ 2 B where σ0 is the zeroﬁeld conductivity σ0 = ne2 τ /m∗ (8.5). The arrows denote the limit for ωc τ → ∞, i.e. large ﬁelds. The resistivity tensor ρ = σ −1 is given by
ρxx ρxy ρ= (12.21a) −ρxy ρxx σxx →0 (12.21b) ρxx = 2 2 σxx + σxy B −σxy . (12.21c) →− ρxy = 2 2 σxx + σxy ne 12.3.1 Integral QHE Experiments yield strong deviations from the linear behavior of the transverse resistivity ρxy = Ey /jx = BRH with the Hall coeﬃcient RH = −1/(ne) with increasing magnetic ﬁeld is observed at low temperatures for samples with high carrier mobility, i.e. ωc τ ≫ 1 (Fig. 12.10). In Fig. 12.11a,b, Hall bars are shown for 2DEGs in silicon metal–oxide–semiconductor ﬁeldeffect transistor (SiMOSFET) electron inversion layers and at GaAs/AlGaAs heterostructures, respectively. The Hall resistivity exhibits extended Hall plateaus with resistivity values that are given by ρxy =
1 h , i e2
(12.22)
i.e. integer fractions of the quantized resistance ρ0 = h/e2 =25812.807 Ω, which is also called the vonKlitzing constant. In Fig. 12.10, a spin splitting is seen for the n = 1 Landau level (and a small one for the n = 2). We note
314
12 External Fields
Fig. 12.10. Hall resistivity ρxy and longitudinal resistivity ρxx for a modulationdoped GaAs/AlGaAs heterostructure (n = 4 × 1011 cm−2 , μ = 8.6 × 104 cm2 /V s) at 50 mK as a function of magnetic ﬁeld (10 kG=1 T). The numbers refer to the quantum number and spin polarization of the Landau level involved. The inset shows schematically the Hall bar geometry, VL (VH ) denotes the longitudinal (Hall) c voltage drop. Reprinted with permission from [421], 1982 APS
that the topmost Hall plateau is due to the completely ﬁlled n = 0 Landau level; the resistance is ρ0 /2 due to the spin degeneracy of 2. The integral quantum Hall effect, ﬁrst reported in [418,419], and the value for ρ0 are found for a wide variety of samples and conditions regarding sample temperature, electron density or mobility of the 2DEG and the materials of the heterostructure. Within the plateau the resistivity is well deﬁned within 10−7 or better up to 4 × 10−9 . A precise determination allows for a new normal for the unit Ohm [422], being two orders of magnitude more precise than the realization in the SI system, and an independent value for the ﬁnestructure constant e2 1 α = c 4πǫ0 . At the same time, the longitudinal resistivity, starting from the classical value for small magnetic ﬁelds, exhibits oscillations and eventually it is zero for the plateaus in ρxy . For ρxx values of 10−10 Ω/2 have been measured, which corresponds to 10−16 Ω/cm for bulk material, a value three orders of magnitude smaller than for any nonsuperconductor. The simplest explanation is that the conductivity is zero when a Landau level is completely ﬁlled and the next is completely empty, i.e. the Fermi level
12.3 Quantum Hall Eﬀect
(a)
315
(b)
Fig. 12.11. (a) Silicon MOS (metal–oxide–semiconductor) structure of K. v. Klitzing’s et al. original experiments. (b) GaAs/AlGaAs heterostructure sample grown with molecular beam epitaxy for QHE measurements, chip carrier and bond wires. Reprinted with permission from [423]
lies between them. The temperature is small, i.e. kT ≪ ωc τ , such that no scattering between Landau levels can occur. Thus no current, similar to a completely ﬁlled valence band, can ﬂow. The sheet carrier density ns is given by counting the i ﬁlled Landau levels (degeneracy according to (12.17)) as ns = i
eB . h
(12.23)
In the transverse direction energy dissipation takes place and the Hall resistivity ρxy = B/(ns e) takes the (scatteringfree) values given in (12.22). However, this argument is too simple as it will not explain the extension of the plateaus. As soon as the system has one electron more or less, the Fermi energy will (for a system with δlike density of states) be located in the upper or lower Landau level, respectively. Then, the longitudinal conductivity should no longer be zero and the Hall resistivity deviates from the integer fraction of ρ0 . Therefore (in the localization model) an inhomogeneous (Gaussian) broadening of the density of states is assumed. Additionally, the states in the tails of the distribution are considered nonconducting, i.e. localized, while those around the peak are considered conductive. This mobility edge is schematically shown in Fig. 12.12a–c. When the Fermi level crosses the density of states of the broadened Landau level (upon increase of the magnetic ﬁeld), it ﬁrst populates localized states and ρxx remains at zero. When the Fermi level crosses the delocalized, conducting states, the longitudinal conductivity shows a peak and the Hall conductivity increases from the plateau value by e2 /h to the next plateau.
316
12 External Fields
D(E)
filling factor
Magnetic field (T)
Normalized Hall potential
xx
(a)
(b) 2
xy
e /h
(c)
0
Filling factor
1 (d)
Tip scanning position y (μm)
Fig. 12.12. (a) Density of states D(E), (b) longitudinal conductivity σxx and (c) Hall conductivity σxy for a Landau level as a function of the ﬁlling factor μ = n/d, where n is the electron density and d the degeneracy of the level. In (a) the ﬁlling factor relates via the position of the Fermi level to an energy scale. The grey areas in (a) denote localized states. The slanted dashed line in (c) has a slope of ne/B. Adapted from [420]. (d) Normalized Hall potential proﬁle for diﬀerent magnetic ﬁelds around ﬁlling factor ν = 2. The overall voltage drop corresponds to 20 mV. The insets show the sample geometry and transport data. The 2DEG is from a GaAs/Al0.33 Ga0.67 As modulationdoped heterostructure, ns = 4.3 × 1011 cm−2 , μ = 5 × 105 cm2 /V s, T = 1.4 K. Adapted from [427]
When the Fermi level lies within the upper nonconducting states, the Hall resistivity remains constant in the next plateau. For the sample in Fig. 12.10 it has been estimated that 95% of the Landau level states are localized [421]. In the localization model it is still astonishing that the samples exhibit the step of e2 /h in the conductivity as if all electrons on the Landau level contribute to conduction, cf. (12.23). According to the calculations in [425] the Hall current lost by the localized states is compensated by an extra current by the extended states. The behavior of the electrons in the quantum
12.3 Quantum Hall Eﬀect
317
Hall regime (‘quantum Hall liquid’) can be considered similar to that of an incompressible ﬂuid where obstructions lead the ﬂuid to move with increased velocity. Nevertheless, the single particle picture seems to be insuﬃcient to model the IQHE. Another model for the explanation of the QHE, supported now with plenty of experimental evidence, is the edge state model where quantized onedimensional conductivity of edge channels, i.e. the presence of conductive channels along the sample boundaries, is evoked [426]. Due to depletion at the boundary of the sample, the density of the 2DEG varies at the edge of the sample and ‘incompressible’ stripes develop for which ∂μ/∂ns → ∞. When the ﬁlling factor is far from an integer, the Hall voltage is found to vary linearly across the conductive channel and the current is thus homogeneous over the sample (Fig. 12.12d). In the Hall plateau, the Hall voltage is ﬂat in the center of the channel and exhibits drops at the edges, indicating that the current ﬂows along the boundary of the sample (edge current) [427] in agreement with predictions from [428]. Although the current pattern changes with varying magnetic ﬁeld, the Hall resistivity remains at its quantized value. The most fundamental arguments for the explanation of the IQHE come from gauge invariance and the presence of a macroscopic quantum state of electrons and magnetic ﬂux quanta [429]. This model holds as long as there are any extended states at all. 12.3.2 Fractional QHE For very low temperatures and in the extreme quantum limit, novel effects are observed when the kinetic energy of the electrons is smaller than their Coulomb interaction. New quantum Hall plateaus are observed at various fractional ﬁlling factors ν = p/q. We note that the effects of the fractional quantum Hall effect (FQHE) in Fig. 12.13 mostly arise for magnetic ﬁelds beyond the n = 1 IQHE plateau. The ﬁlling factor ν = n/(eB/h) is now interpreted as the number of electrons per magnetic ﬂux quantum φ0 = h/e. The effects of the FQHE cannot be explained by singleelectron physics. The plateaus at fractional ﬁllings ν occur when the Fermi energy lies within a highly degenerate Landau (or spin) level and imply the presence of energy gaps due to manyparticle interaction and the result of correlated 2D electron motion in the magnetic ﬁeld. A decisive role is played by the magnetic ﬂux quanta. The presence of the magnetic ﬁeld requires the manyelectron wavefunction to assume as many zeros per unit area as there are ﬂux quanta penetrating it. The decay of the wavefunction has a length scale of the magnetic length l0 = /(eB). Since the magnetic ﬁeld implies a 2π phase shift around the zero, such an object is also termed a vortex, being the embodiment of the magnetic ﬂux quanta in the electron system. Such a vortex represents a charge deﬁcit (compared to a homogeneous charge distribution) and thus electrons and vortices attract each other. If a vortex and an electron are placed onto each other, considerable
12 External Fields
Rxx
Rxy (h/e2)
318
B (T)
Fig. 12.13. Hall resistance Rxy and magnetoresistance Rxx of a twodimensional electron system (GaAs/AlGaAs heterostructure) of density n = 2.33 × 1011 cm−2 at a temperature of 85 mK, vs. magnetic ﬁeld B. Numbers identify the ﬁlling factor ν, which indicates the degree to which the sequence of Landau levels is ﬁlled with electrons. Plateaus are due to the integral (ν = i) quantum Hall eﬀect (IQHE) and fractional (ν = p/q) quantum Hall eﬀect (FQHE). Adapted from [424], reprinted c with permission, 1990 AAAS
Coulomb energy is gained. At ν = 1/3, there are three times more vortices than there are electrons, each vortex representing a charge deﬁcit of 1/3 e. Such a system is described with manyparticle wavefunctions, such as the Laughlin theory for ν = 1/q [429] and novel quasiparticles called composite fermions [430, 431] for other fractional ﬁllings. For further reading we refer readers to [432] and references therein. 12.3.3 Weiss Oscillations In Fig. 12.14, measurements are shown for a Hall bar in which an array of antidots (in which no conduction is possible) has been introduced by dry etching. The antidot size is 50 nm (plus depletion layer) and the period is 300 nm. These obstructions for the cyclotron motion lead to a modiﬁcation of the magnetotransport properties. Before etching of the antidot array the 2DEG has a mean free path length of 5–10 µm at 4 K for the mobility of ≈ 106 cm2 /V s. At low magnetic ﬁelds there is a strong deviation of the Hall resistivity from the straight line to which the QHE levels converge. Similarly, ρxx shows a strong effect as well. These effects are related to commensurability effects between the antidot lattice and the cyclotron resonance path. When the cyclotron orbit is equal to the lattice period, electrons can fulﬁll a circular motion around one antidot (pinned orbit, Fig. 12.14b) that leads to a reduction of conductivity. At
12.3 Quantum Hall Eﬀect
319
(a)
(b)
(a)
B (T)
(b)
Fig. 12.14. Weiss oscillations: (a) magnetoresistance and (b) Hall resistance of an antidot lattice (inset in (a)) with pattern (solid lines) and without pattern (dashed lines) at T = 1.5 K. (b) Schematic of the diﬀerent orbits: ‘p’: pinned, ‘d’: drifting, c ‘s’: scattered. Reprinted with permission from [433], 1991 APS
high ﬁelds, drifting orbits for which the cyclotron orbit is much smaller than the lattice period occur. At small ﬁelds, scattering orbits also contribute for which the cyclotron radius is large and the electron has antidots from time to time. Resonances in the Hall resistivity have been found due to pinned orbits enclosing 1, 2, 4, 9 or 21 antidots.
13 Nanostructures
The principles of physics, as far as I can see, do not speak against the possibility of maneuvering things atom by atom. R.P. Feynman, 1959 [434]
13.1 Introduction When the structural size of functional elements enters the size range of the de Broglie matter wavelength, the electronic and optical properties are dominated by quantummechanical effects. The most drastic impact can be seen from the density of states (Fig. 13.1). The quantization in a potential is ruled by the Schr¨ odinger equation with appropriate boundary conditions. These are simplest if an inﬁnite potential is assumed. For ﬁnite potentials, the wavefunction leaks out into the barrier. Besides making the calculation more complicated (and more realistic), this allows electronic coupling of nanostructures. Via the Coulomb interaction, a coupling is even given if there is no wavefunction overlap. In the following, we will discuss some of the fabrication techniques and properties of quantum wires (QWR) and quantum dots (QD). In particular for the latter, several textbooks can also be consulted [435, 436].
13.2 Quantum Wires 13.2.1 Preparation Methods Many methods have been proposed and realized to fabricate quantum wires. In the following, we will restrict ourselves to the growth of QWRs on corrugated substrates, fabrication using cleavededge overgrowth (CEO) and nanowhiskers.
322
13 Nanostructures
bulk material
D(E)
Ec
E
quantum film D(E)
Ec
E
quantum wire D(E)
Ec
E
quantum dot D(E)
Ec
E
Fig. 13.1. Schematic geometry and density of states for 3D, 2D, 1D and 0D electronic systems
Vgroove Quantum Wires Quantum wires with high optical quality, i.e. high recombination eﬃciency and welldeﬁned spectra, can be obtained by employing epitaxial growth on corrugated substrates. The technique is shown schematically in Fig. 13.2. A Vgroove is etched, using, e.g., an anisotropic wet chemical etch, into a GaAs substrate. The groove direction is along [1¯ 10]. Even when the etched pattern is not very sharp on the bottom, subsequent growth of AlGaAs sharpens the apex to a selflimited radius ρl of the order of 10 nm. The side facets
13.2 Quantum Wires
323
of the groove are {111}A. Subsequent deposition of GaAs leads to a larger upper radius ρu > ρl of the heterostructure. The GaAs QWR formed in the bottom of the groove is thus crescentshaped as shown in Fig. 13.3. A thin GaAs layer also forms on the side facets (sidewall quantum well) and on the top of the ridges. Subsequent growth of AlGaAs leads to a resharpening of the Vgroove to the initial, selflimited value ρl . The complete resharpening after a suﬃciently thick AlGaAs layer allows vertical stacking of crescentshaped QWRs of virtually identical size and shape, as shown in Fig. 13.4. In this sense, the selflimiting reduction of the radius of curvature and its recovery during barrierlayer growth leads to selfordering of QWR arrays whose structural parameters are determined solely by growth parameters. The lateral pitch of such wires can be down to 240 nm.
Fig. 13.2. Schematic cross section of a GaAs/AlGaAs heterostructure grown on a channeled substrate, illustrating the concept of selfordered quantumwire fabrication. From [437]
To directly visualize the lateral modulation of the bandgap, a lateral cathodoluminescence (CL) linescan perpendicular across the wire is displayed in Fig. 13.5. In Fig. 13.5a, the secondary electron (SE) image of the sample from Fig. 13.3 is shown in plan view. The top ridge is visible in the upper and lower parts of the ﬁgure, while in the middle the sidewalls with the QWR in the center are apparent. In Fig. 13.5b, the CL spectrum along a linescan perpendicular to the wire (as indicated by the white line in Fig. 13.5a) is displayed. The xaxis is now the emission wavelength, while the yaxis is the lateral position along the linescan. The CL intensity is given on a logarithmic scale to display the full dynamic range. The top QW shows almost no variation in bandgap energy (λ = 725 nm); only directly at the edge close to the sidewall does a second peak at lower energy (λ = 745 nm) appear, indicating a thicker region there. The sidewall QW exhibits a recombination
324
13 Nanostructures
Fig. 13.3. Transmission electron microscopy crosssectional image of a crescentshaped single GaAs/AlGaAs quantum wire. From [438]
Fig. 13.4. TEM crosssectional image of a vertical stack of identical GaAs/AlGaAs crescentshaped QWRs. From [437]
13.2 Quantum Wires
325
Fig. 13.5. (a) Planview SE image of single QWR (sample A), showing top and sidewall with QWR in the center. The white line indicates the position of the linescan on which the CL spectra linescan (b) has been taken at T = 5 K. The CL intensity is given on a logarithmic grey scale to display the full dynamic range as a function of wavelength and position along the white line in (a). From [438]
wavelength of 700 nm at the edge to the top QW, which gradually increases to about 730 nm at the center of the Vgroove. This directly visualizes a linear tapering of the sidewall QW from about 2.1 nm thickness at the edge to 3 nm in the center. The QWR luminescence itself appears at about 800 nm. After fast capture from the barrier into the QWs and, to a much smaller extent corresponding to its smaller volume, into the QWR, excess carriers will diffuse into the QWR via the adjacent sidewall QW and the vertical QW. The tapering of the sidewall QW induces an additional drift current. CleavedEdge Overgrowth Quantum Wires Another method to create quantum wires of high structural perfection is cleavededge overgrowth (CEO) [439], shown schematically in Fig. 13.6. First, a layered structure is grown (single or multiple quantum wells or superlattice).
326
13 Nanostructures CEO QWRs (110)
[110]
(001) AlGaAs GaAs AlGaAs
[001] [110]
(a)
(b)
(c)
CEO QD
[110] 2nd growth
50nm
QW
cleavage plane
(d)
QW
[001] 1st growth
Fig. 13.6. Principle of CEO quantum wires and 2fold CEO quantum dots. Part (a) depicts a layered structure (quantum wells or superlattice), (b) describes the growth on the cleaved facet used for fabrication of quantum wires. In (c) a second cleave and growth on top of the plane allows the fabrication of quantum dots. From [440]. (d) Crosssectional TEM image of CEO GaAs/AlGaAs quantum wires. Two quantum wells (QW) and the QWR at their junction are labeled. The ﬁrst epitaxy was from left to right. The second epitaxy step was on top of the cleavage plane (dashed line) in the upward direction. Adapted from [441], reprinted with c permission, 1997 APS
Then, a {110} facet is fabricated by cleaving (in vacuum) and epitaxy is continued on the cleaved facet. At the junctures of the {110} layer and the original quantum wells QWRs form. Due to their crosssectional form they are also called Tshaped QWRs. A second cleave and another growth step allow fabrication of CEO quantum dots [440, 441] (Fig. 13.6c). Nanowhiskers Whiskers are primarily known as thin metal spikes and have been investigated in detail [442]. Semiconductor whiskers can be considered as (fairly short) quantum wires. They have been reported for a number of materials, such as
13.2 Quantum Wires
327
1μm Fig. 13.7. Array of ZnO nanowhiskers on sapphire, fabricated using thermal evaporation
Si, GaAs, InP and ZnO. A ﬁeld of ZnO whiskers is shown in Fig. 13.7. If heterostructures are incorporated along the whisker axis [443], quantum dots or tunneling barriers can be created (Fig. 13.8). The nanocrystal can also act as a nanolaser [444, 445].
Au InAs InP InAs InP InAs
Fig. 13.8. TEM image of a part of an InAs whisker 40 nm in diameter that contains InP barriers. The zooms show sharp interfaces. On top of the whisker is a gold droplet from the socalled vapor–liquid–solid growth mechanism. The whisker axis is [001], the viewing direction is [110]. Adapted from [443], reprinted with permission, c 2002 AIP
328
13 Nanostructures
13.2.2 Quantization in TwoDimensional Potential Wells The motion of carriers along the quantum wire is free. In the crosssectional plane the wavefunction is conﬁned in two dimensions. The simplest case is for constant cross section along the wire. However, generally the cross section along the wire may change and therefore induce a potential variation along the wire. Such potential variation will impact the carrier motion along the longitudinal direction. Also, a twist of the wire along its axis is possible. In Fig. 13.9, the electron wavefunctions in a Vgroove GaAs/AlGaAs QWR are shown. Further properties of Vgroove QWRs have been reviewed in [446]. In Fig. 13.10, the excitonic electron and hole wavefunctions are shown for a (strained) Tshaped QWR.
n=1
n=2
n=3
Fig. 13.9. Electron wavefunctions (Ψ 2 on logarithmic grey scale) for the ﬁrst three conﬁned levels for the QWR of Fig. 13.3. From [438]
13.3 Quantum Dots 13.3.1 Quantization in ThreeDimensional Potential Wells The solutions for the ddimensional (d = 1, 2, or 3) harmonic oscillator, i.e. the eigenenergies for the Hamiltonian d
2 1 ˆ = p + H mω02 x2i 2m i=1 2
(13.1)
13.3 Quantum Dots
329
hh
e [110] (a) [110]
[001]
[110] (b) [001] Fig. 13.10. (a) Threedimensional view of the electron and (heavy) hole part of the excitonic wavefunction in a 4 nm × 5 nm Tshaped In0.2 Ga0.8 As/GaAs QWR. The orbitals correspond to 70% probability inside. (b) Cross section through the electron and hole orbitals in their center along the wire direction. Reprinted with c permission from [447], 1998 APS
are given by
En =
d n+ 2
ω0 ,
(13.2)
with n = 0, 1, 2, . . . . More detailed treatments can be found in quantummechanics textbooks. Next, we discuss the problem of a particle in a centrosymmetric ﬁnite potential well with different masses m1 in the dot and m2 in the barrier. The Hamiltonian and the potential are given by 2 ˆ = ∇ ∇ + V (r) H 2m −V0 , r ≤ R0 . V (r) = 0 , r > R0
(13.3) (13.4)
The wavefunction can be separated into radial and angular components Ψ (r) = Rnlm (r) Ylm (θ, φ), where Ylm are the spherical harmonic functions. For the ground state (n = 1) the angular momentum l is zero and the solution for the wavefunction (being regular at r = 0) is given by
330
13 Nanostructures
R(r) =
sin(kR0 ) kR0
sin(kr) kr
, r ≤ R0 exp (−κ(r − R0 )) , r > R0
2m1 (V0 + E) 2 2m2 E κ2 = − 2 . k2 =
(13.5a) (13.5b) (13.5c)
1 ∂R(r) are continuous From the boundary conditions that both R(r) and m ∂r across the interface at r = R0 , the transcendental equation
kR0 cot (kR0 ) = 1 −
m1 (1 + κR0 ) m2
(13.6)
is obtained. From this formula the energy of the single particle ground state in a spherical quantum dot can be determined. For a given radius, the potential needs a certain strength V0,min to conﬁne at least one bound state; this condition can be written as V0,min
3. Adapted from [457], reprinted with permission from c Nature, 2000 Macmillan Magazines Limited
In a QD ensemble, optical transitions are inhomogeneously broadened due to ﬂuctuations in the QD size and the size dependence of the conﬁnement energies (Fig. 13.30). Interband transitions involving electrons and holes suffer from the variation of the electron and hole energies:
σE ∝
∂Ee ∂Eh + ∂L ∂L δL .
(13.17)
Fig. 13.30. Ensemble photoluminescence spectrum (T = 293 K, excitation density 500 W/cm2 ) of InAs/GaAs QDs
344
13 Nanostructures
A typical relative size inhomogeneity of σL /L of 7% leads to several tens of meV broadening. Additional to broadening due to different sizes ﬂuctuations of the quantum dot shape can also play a role. The conﬁnement effect leads to an increase of the recombination energy with decreasing quantumdot size. This effect is nicely demonstrated with colloidal quantum dots of different size as shown in Fig. 13.31.
Fig. 13.31. Luminescence (under UV excitation) from ﬂasks of colloidal CdTe quantum dots with increasing size (from left to right). From [458]
14 Polarized Semiconductors
14.1 Introduction Semiconductors can have an electric polarization. Such polarization can be induced by an external electric ﬁeld (Fig. 14.1a). This phenomenon, i.e. that the semiconductor is dielectric, has been discussed already in Chap. 9. In this chapter, we discuss pyroelectricity, i.e. a spontaneous polarization without an external ﬁeld (Fig. 14.1b), ferroelectricity, i.e. pyroelectricity with a hysteresis (Fig. 14.1c) and piezoelectricity, i.e. a polarization due to external stress.
P
P
P
Psp
Psp
Psp=0 Eext (a)
Eext (b)
Eext (c)
Fig. 14.1. Schematic representation of the polarization vs. external electric ﬁeld dependence for (a) dielectric, (b) pyroelectric and (c) ferroelectric semiconductors
14.2 Spontaneous Polarization The reason for a spontaneous polarization Psp (without external electric ﬁeld) is the static, relative shift of positive and negative charges in the unit cell. For a slab of semiconductor material (thus ignoring depolarization effects present in other geometries), the polarization causes polarization charges located at the upper and lower surfaces (Fig. 14.2a). The polarization vector P points from the negative to the positive charge. The electric ﬁeld due to the polarization charges has the opposite direction. In the absence of free charges, the Maxwell equation ∇ · D = 0 yields for piecewise constant ﬁelds at a planar
346
14 Polarized Semiconductors
interface (Fig. 14.2b) (D2 − D1 ) · n12 = 0 where n12 is the surface normal pointing from medium 1 to medium 2. Therefore, the polarization charge σP = ǫ0 ∇ · E is given by σP = −(P2 − P1 ) · n12 .
(14.1)
Polarization charges develop at interfaces where the polarization is discontinuous, e.g. an interface between two semiconductors with different spontaneous polarization. Vacuum (at a surface) represents a special case with P = 0.
         P
P1
P
P
n 12
E
P2 (a)
+ + + + + + + + + +
P
(b)
Fig. 14.2. (a) Surface polarization charges σP on a slab of semiconductor material with polarization. The electric ﬁeld is given by E = −P/0 . (b) Polarization charge σP at an interface between two semiconductors with diﬀerent polarization. In the depicted situation σ is negative
For cubic zincblende structure semiconductors, Psp is typically fairly small. The anisotropy of the wurtzite structure allows for sizeable effects. The main cause is the nonideality of the cellinternal parameter u (see Sect. 3.4.5).
14.3 Ferroelectricity Ferroelectric semiconductors exhibit a spontaneous polarization in the ferroelectric phase and zero spontaneous polarization in the paraelectric phase. As a function of temperature, the ferroelectric material undergoes a phase transition from the hightemperature paraelectric phase into the ferroelectric phase. There can be further phase transitions between different ferroelectric phases that differ in the direction of the polarization. The literature until 1980 is summarized in [504]. A more recent treatment can be found in [505]. PbTiO3 has perovskite structure (cf. Sect. 3.4.8). It exhibits a phase transition at TC = 490 ◦ C from the cubic into the (ferroelectric) tetragonal phase as shown in Fig. 14.4a. Mostly the cell symmetry changes, while the cell volume remains almost constant. A more complicated situation arises for BaTiO3 . At 120 ◦ C the transition into the ferroelectric phase occurs (Fig. 14.4b) that is tetragonal with the polarization in the [100] direction. At −5 ◦ C and −90 ◦ C transitions occur into an orthorhombic and a rhombohedral (trigonal) phase, respectively. The largest polarization is caused by
14.3 Ferroelectricity
347
0.04 0.02
BP BAs
GaP
0
Psp (C/m 2 )
BP BSb BAs GaP
BSb
TlP 2HSiC
AlSb 2HSiC
0.02
AlAs
AlP AlAs TlP
GaN
InN
GaN
0.04
AlP
BN
BN
TlN
TlN
ZnO
InN ZnO
0.06 0.08 AlN
AlN
0.10 0.20 0.25
0.30
0.35
0.40
0.50
0.45
0.373
0.375
0.377
0.379
0.381
0.383
u
a (nm)
Fig. 14.3. Spontaneous polarization Psp for various semiconductors as a function of the lattice constant a (left) and the cellinternal parameter u (right). Based on [503]
a displacement of the negatively (O) and positively (Ba, Ti) charged ions of the unit cell by δ ≈ 0.02 nm (Fig. 14.5). Such an origin of the spontaneous polarization is called a displacement transition. However, other mechanisms (not discussed here) can also be responsible for ferroelectricity. tetragonal
0.415
cubic PbTiO3
c
0.405
20
0.400
PS (102 C/m2)
Cell parameters (nm)
0.410
(a2c)1/ 3 0.395
a=b
0.390
15
10
5
trigonal
orthorhombic
tetragonal
Tc
0.385 0
(a)
BaTiO3
100
200
300 T (°C)
400
500
600
(b)
0 200
150
100
0 50 50 Temperature (°C)
100
150
Fig. 14.4. (a) Cell parameters of PbTiO3 as a function of temperature. Adapted from [506]. (b) Phase transitions of BaTiO3 as a function of temperature. The spontaneous polarization PS points along 100, 110 and 111 in the tetragonal (C4v ), orthorhombic (C2v ) and trigonal (C3v , rhombohedral) phase, respectively. Adapted from [507]
348
14 Polarized Semiconductors
Ba2
O2
2
O
Ti
4
(a)
(b)
Fig. 14.5. (a) Crystal structure of BaTiO3 (cf. Fig. 3.23). (b) Schematic tetragonal deformation below the Curie temperature, generating a dipole moment
14.3.1 Materials A large class of ferroelectric semiconductors are of the type ABO3 , where A stands for a cation with larger ionic radius and B for an anion with smaller ionic radius. Many ferroelectrics have perovskite (CaTiO3 ) struc1+ 5+ 2− ture. They are A2+ B4+ O2− B O3 , e.g. 3 , e.g. (Ba,Ca,Sr) (Zi,Zr)O3 or A (Li,Na,K) (Nb,Ta)O3 . Ferroelectrics can also be alloyed. Alloying in the B component yields, e.g. PbTix Zr1−x O3 also called PZT. PZT is widely used for piezoelectric actuators. Also, alloying in the A component is possible, e.g. Bax Sr1−x TiO3 . Another class of ferroelectrics are AV BVI CVII compounds, such as SbSI, SbSBr, SbSeI, BiSBr. These materials have a width of the forbidden band in VI the ∼ 2 eV range. A further class of ferroelectric semiconductors are AV 2 B3 compounds, such as Sb2 S3 . 14.3.2 Soft Phonon Mode The ﬁnite displacement of the sublattices in the ferroelectric means that the related lattice vibration has no restoring force. The displacement is, however, ﬁnite due to higherorder terms (anharmonicity). Thus, for T → TC ωTO → 0. Such a mode is called a soft phonon mode. The decrease of the phonon frequency is shown in Fig. 14.6a for SbSI. From the LST relation (5.42), it follows that the static dielectric function must increase strongly. The increase is ∝ (T − TC )−1 (Fig. 14.6b). 14.3.3 Phase Transition In the case of ferroelectrics, the order parameter for the Ginzburg–Landau theory of phase transitions is the spontaneous polarization P . The free energy F of the ferroelectric crystal is written in terms of the free energy of the paraelectric phase F0 and is expanded in powers of P (here up to P 6 ) as
14.3 Ferroelectricity Ba0. 5Sr0. 5TiO3
SbSI
50
Dielectric constant
SrTiO3
40
TO (cm1)
349
TC 30 20
BaTiO3 KTaO3
Ca0. 2Sr0. 8TiO3 CaTiO3
10 0 0
(a)
100 200 Temperature (K)
300
(b)
1000/(TTC)
(1/K)
Fig. 14.6. (a) Decrease of the transverse phonon mode of SbSI close to the Curie temperature of TC = 288 K. The dashed curved line represents a T − TC 1/2 dependence. Adapted from [508]. (b) Dielectric constant of various perovskites vs. 1/(T − TC ) in the paraelectric phase (T > TC ). Adapted from [509]
1 1 1 F = F0 + αP 2 + βP 4 + γP 6 . 2 4 6
(14.2)
In this equation, we have neglected effects due to charge carriers, an external electric ﬁeld or external stresses and we assume homogeneous polarization. In order to obtain a phase transition, it has to be assumed that α has a zero at a certain temperature TC and we assume (expanding only to the linear term) α = α0 (T − TC ) .
(14.3)
SecondOrder Phase Transition For modeling a secondorder phase transition, we set γ = 0. Thus, the free energy has the form (Fig. 14.7a) 1 1 F = F0 + αP 2 + βP 4 . 2 4
(14.4)
The equilibrium condition with regard to the free energy yields a minimum for ∂F = αP + βP 3 = 0 ∂P ∂2F = α + 3βP 2 > 0 . ∂P 2
(14.5a) (14.5b)
Equation (14.5a) yields two solutions. P = 0 corresponds to the paraelectric phase. P 2 = −α/β is the spontaneous polarization in the ferroelectric phase. The condition from (14.5b) yields that α > 0 in the paraelectric phase,
350
14 Polarized Semiconductors
60
PS (102 C/m2)
>0 Free energy
LiTaO3
50
=0
40 30 20 10
0 (α < 0) corresponds to the paraelectric (ferroelectric) phase. (b) Spontaneous polarization of LiTaO3 as a function of temperature exhibiting a secondorder phase transition. The dashed line is theory with suitable parameters. Adapted from [510]
while α < 0 in the ferroelectric phase. Also, β > 0 below the Curie temperature (β is assumed to be temperature independent in the following). Using (14.3), the polarization is given as (Fig. 14.7b) P2 =
α0 (T − TC ) . β
(14.6)
Therefore, the entropy S = − ∂F ∂T and the discontinuity ΔCp of the heat ∂S at the Curie point TC are given by capacity Cp = T ∂T p S = S0 + ΔCp =
α02 (T − TC ) β
α02 TC , β
(14.7a) (14.7b)
0 with S0 = − ∂F ∂T being the entropy of the paraelectric phase. This behavior is in accordance with a secondorder phase transition with vanishing latent heat (continuous entropy) and a discontinuity of the heat capacity. The dielectric function in the paraelectric phase is ∝ 1/α and in the ferroelectric phase ∝ −1/α. The latter relation is usually written as the Curie–Weiss law
ǫ=
C . T − TC
(14.8)
FirstOrder Phase Transition When the P 6 term is included in (14.2) (γ = 0), a ﬁrstorder phase transition is modeled. However, in order to obtain something new, compared to the
14.3 Ferroelectricity
351
previous consideration, now β < 0 (and γ > 0) is necessary. The dependence of the free energy on P is schematically shown in Fig. 14.8a for various values ∂F = 0 yields of α. The condition ∂P αP + βP 3 + γP 5 = 0 ,
(14.9)
with the solutions P = 0 and β P =− 2γ 2
1+
1−
4αγ β2
.
(14.10)
25
PS (102 C/m2)
20 15 10 5
BaTiO3
(b)
(a)
0 20
30
40
50 60 70 80 Temperature (°C)
90
100 110
Fig. 14.8. (a) Schematic plot of the free energy vs. spontaneous polarization for a ﬁrstorder phase transition. The lowest curve is for α = 0, the others are for α > 0. (b) Spontaneous polarization in BaTiO3 as a function of temperature exhibiting a ﬁrstorder phase transition. The dashed line is a guide to the eye. Adapted from [511]
For a certain value of α, i.e. at a certain temperature T = T1 , the free energy is zero for P = 0 and also for another value P = P0 (second curve from the top in Fig. 14.8a). From the condition 1 1 1 α(T1 )P02 + βP04 + γP06 = 0 , 2 4 6
(14.11)
the values for P0 and α at the transition temperature T = T1 are given by 3β 4γ 3 β2 >0. α(T1 ) = 16 γ P02 = −
(14.12a) (14.12b)
The schematic dependence of P at the phase transition temperature T1 is depicted in Fig. 14.8b. For T ≤ T1 the absolute minimum of the free energy is reached for ﬁnite polarization P > P0 . However, between F (P = 0) and the minimum of the
352
14 Polarized Semiconductors
free energy an energy barrier (second lowest curve in Fig. 14.8) is present for T close to T1 . The energy barrier disappears at the Curie–Weiss temperature T0 . At the phase transition temperature, the entropy has a discontinuity ΔS = α0 P02 ,
(14.13)
that corresponds to a latent heat ΔQ = T ΔS. Another property of the ﬁrstorder phase transition is the occurrence of hysteresis in the temperature interval between T1 and T0 ΔT ≈ T1 − T0 =
1 β2 , 4α0 γ
(14.14)
in which an energy barrier is present to hinder the phase transition. For decreasing temperature, the system tends to remain in the paraelectric phase. For increasing temperature, the system tends to remain in the ferroelectric phase. Such behavior is observed for BaTiO3 , as shown in Fig. 14.4b. 14.3.4 Domains Similar to ferromagnets, ferroelectrics form domains with different polarization directions in order to minimize the total energy by minimizing the ﬁeld energy outside the crystal. The polarization can have different orientations, 6 directions for P along 100 (tetragonal phase), 12 directions for P along 110 (orthorhombic phase) and 8 directions for P along 111 (rhombohedral phase). In Fig. 14.9, such domains are visualized for BaTiO3 . Due to the restricted geometry, domain formation in thin ﬁlms is different from that in bulk material. Domains can also be artiﬁcially created by socalled poling. The ferroelectric semiconductor is heated to the paraelectric phase. With electrodes,
Fig. 14.9. Ferroelectric domains in a BaTiO3 single crystal visualized by birefrinc gence contrast. Reprinted with permission from [512], 1949 APS
14.4 Piezoelectricity
353
appropriate electric ﬁelds are applied and the material is cooled. The polarization is then frozen in the ferroelectric phase. The domains of a periodically poled structure in LiNbO3 (PPLN) are shown in Fig. 14.10b. The nonlinear optical properties in such structures can be used for eﬃcient second harmonic generation (SHG).
PPLN
(a)
Input light
(b)
Fig. 14.10. (a) Scheme of PPLN (perodically poled lithium niobate), arrows denote the direction of spontaneous polarization. (b) Polarization microscopy image (vertical stripes are domains, horizontal dark lines are scratches)
14.3.5 Optical Properties The ﬁrstorder phase transition of BaTiO3 manifests itself also in a discontinuity of the bandgap (Fig. 14.11). The coeﬃcient ∂Eg /∂T for the temperature dependence of the bandgap is also different in the para and ferroelectric phases.
14.4 Piezoelectricity External stress causes atoms in the unit cell to shift with respect to each other. In certain directions, such a shift can lead to a polarization. Generally, all ferroelectric materials are piezoelectric. However, there are piezoelectric materials that are not ferroelectric, e.g. quartz, GaAs and GaN. Piezoelectricity can occur only when no center of inversion is present. Thus, e.g., GaAs is piezoelectric along 111, but Si is not. Also, the cubic perovskite structure (in the paraelectric phase) is not piezoelectric. Generally, the piezoelectric polarization is related to the strains via the tensor eijk of the piezoelectric modules Pi = eijk ǫjk .
(14.15)
354
14 Polarized Semiconductors
Fig. 14.11. Temperature dependence of the bandgap in BaTiO3 (for polarized light with E ⊥ c). Experimental data from [513]
In zincblende semiconductors, the polarization (with respect to x = [100], y = [010], z = [001]) is due to shear strains only and is given as ⎛ ⎞ ǫyz ⎜ ⎟ Ppe = 2e13 ⎝ ǫxz ⎠ . (14.16) ǫxy
The strain in pseudomorphic heterostructures (see Sect. 5.3.2) can cause piezoelectric polarization in a piezoelectric semiconductor. In zincblende, the main effect is expected when the growth direction is along [111] and the strain has a purely shear character. In this case, the polarization is in the [111] direction, i.e. perpendicular to the interface (P⊥ ). For the [001] growth direction, no piezoelectric polarization is expected. For the [110] growth direction, the polarization is found to be parallel to the interface (P ). The situation is shown for various orientations of the growth direction in Fig. 14.12. In wurtzite crystals, the piezoelectric polarization (with respect to x = [2–1.0], y = [01.0], z = [00.1]) is given by ⎞ ⎛ 2e15 ǫyz ⎟ ⎜ Ppe = ⎝ (14.17) 2e15 ǫxz ⎠ . e31 (ǫxx + ǫyy ) + e33 ǫzz
Therefore, the polarization (along c) for biaxial strain in heteroepitaxy (5.62) on the [00.1] surface is
C13 (14.18) PPE = 2ǫ e31 − e33 , C33
14.4 Piezoelectricity
(d)
355
(e)
(f) Fig. 14.12. Threedimensional view of the (a) total, (b) longitudinal and (c) transverse polarization in uniaxially compressed GaAs. Reprinted with permission c from [516], 1994 APS. (d) Longitudinal electric ﬁeld E⊥ (perpendicular to the interface) and (e) transverse polarization P (parallel to the interface) in the InGaAs layer of a GaAs/In0.2 Ga0.8 As superlattice with joint inplane lattice constant (obtained from energy minimization, 1.4% lattice mismatch, the InGaAs is under compressive and the GaAs under tensile strain). The layer thicknesses of the GaAs and InGaAs layers are identical. The quantities are shown for various orientations of the growth direction. The vector of the growth direction varies in the (01–1) plane (φ = π/4) with polar angle θ reaching from [100] (0◦ ) over [111] to [011] (90◦ ). Image (f ) depicts the transverse polarization P (P⊥ = 0 in this geometry) for growth directions in the (001) plane (φ = 0). Parts (d,e,f ) reprinted with c permission from [514], 1988 AIP
where ǫ = (a − a0 )/a0 is the inplane strain. The dependence of the magnitude for GaN on the inplane strain is shown in Fig. 14.13 together with the polarization for uniaxial stress along [00.1] and hydrostatic strain. In the latter two cases, the polarization is smaller.
356
14 Polarized Semiconductors 10
GaN Gaface
0
Px
biaxial
Py
1
10
2
Ppee (C/m )
Psp Pz
2
uniaxial
10
Pz
3
10
Px Py
hydrostatic 4
10 0.10
0.08
0.06 0.04 0.02
0
 Fig. 14.13. Piezoelectric polarization Ppe in GaN (Gaface) vs. inplane strain = (a − a0 )/a0 for biaxial, uniaxial and hydrostatic strain. The value of the spontaneous polarization Psp is indicated by an arrow. From [515]
Fig. 14.14. (a) Electric ﬁeld and (b) additional conﬁnement potential for electrons due to piezoelectric charges for a strained In0.2 Ga0.8 As/GaAs quantum wire. c Reprinted with permission from [516], 1994 APS
14.4 Piezoelectricity charges
piezoelectric potential (mV) 42
(c) (a)
357
(b)
around the QD
42
25
(d)
21
in the QD
Fig. 14.15. (a) Piezoelectric charges and (b)–(d) resulting Coulomb potential for InAs/GaAs quantum dot with base length b = 12 nm. (a) Isosurfaces corresponding to volume charges ±0.3 e nm−3 . (b) Isosurfaces for the Coulomb potential at ±30 meV. (c,d) Cross section through the Coulomb potential somewhat above the wetting layer in two diﬀerent magniﬁcations, (d) is a zoom into (c). The InAs/GaAs interface is visible in (d) due to the image charge eﬀect. Parts (a) and (b) reprinted c with permission from [117], 1995 APS
The strain distribution around zincblende strained quantum wires [516] and quantum dots [117] contains shear components and thus generates piezoelectric ﬁelds. In Fig. 14.14, the electric ﬁeld and potential due to the piezoelectric charges are shown for a strained In0.2 Ga0.8 As/GaAs quantum wire. In Fig. 14.15, the piezoelectric charges and potential are shown for the quantum dot from Fig. 5.19. The piezoelectric potential has quadrupole character and thus reduces the symmetry of the QD (to C2v ) [117].1 Piezoelectric effects are particularly important in wurtzite nanostructures [517].
1
The strain distribution has C2v symmetry for a squarebased pyramid for zincblende materials. The energy levels and wavefunctions are more strongly impacted by the piezoelectric eﬀects than by the strain asymmetry [448, 450]
15 Magnetic Semiconductors
15.1 Introduction Magnetic semiconductors exhibit spontaneous magnetic order. Even ferromagnetism, important for spin polarization, as needed in spinelectronics (also called spintronics), can occur below the Curie temperature that is characteristic of the material. Magnetic semiconductors can be binary compounds such as EuTe (antiferromagnetic) or EuS (ferromagnetic). Another class of magnetic semiconductors contains paramagnetic ions in doping concentration (typically < 1021 cm−1 ) or alloy concentration x (typically x ≥ 0.1%). Such materials are termed diluted magnetic semiconductors (DMS). The incorporation of the magnetic atoms leads ﬁrst to conventional alloy effects, such as the modiﬁcation of the lattice constant, the carrier concentration or the bandgap. The status of the ﬁeld up to the mid1980s can be found in [518], mostly focused on II–VI DMS. A review of work on III–V based materials for spintronics, mostly GaAs:Mn, can be found in [519]. A 2003 review of widebandgap ferromagnetic semiconductors is given in [520].
15.2 Magnetic Semiconductors In a magnetic semiconductor, one sublattice is populated with paramagnetic ions. The ﬁrst two ferromagnetic semiconductors discovered were CrBr3 [521] in 1960 and EuO [522] one year later. Europium monoxide has an ionic Eu2+ O2− character, such that the electronic conﬁguration of europium is [Xe]4f7 5d0 6s0 and that of oxygen is 1s2 2s2 2p6 . Some properties of europium chalcogenides are summarized in Table 15.1. EuO can be modeled as a Heisenberg ferromagnet with dominant nearestand nextnearest Eu–Eu interactions [523]. The Heisenberg exchange parameters J1 and J2 for these four compounds are shown in Fig. 15.1. In the nearestneighbor interaction a 4f electron is excited to the 5d band, experiences an exchange interaction with the 4f spin on a nearest neighbor and returns to the initial state. This mechanism generally leads to ferromagnetic exchange. The nextnearestneighbor interaction is weakly ferromagnetic (EuO) or antiferromagnetic (EuS, EuSe, EuTe). In the superexchange process, electrons
360
15 Magnetic Semiconductors
are transferred from the anionic p states to the 5d states of the Eu2+ cations, resulting in an antiferromagnetic coupling.
Fig. 15.1. Heisenberg nearest (J1 , squares) and nextnearest (J2 , circles) exchange parameters (in units of J1,2 /kB ) for the Eu chalcogenides vs. the Eu–anion distance. Dashed lines are guides to the eye. Experimental data from [524]
Table 15.1. Material properties of Eu chalcogenides. ‘F’ (‘AF’) denotes ferromagnetic (antiferromagnetic) order. TN (TC ) denotes the N´eel (Curie) temperature. Data collected in [524] material
Eg (eV)
magnetic order
TN , TC (K)
EuO EuS EuSe
1.12 1.65 1.8
EuTe
2.00
F F AF F AF
69.3 16.6 4.6 2.8 9.6
15.3 Diluted Magnetic Semiconductors
361
15.3 Diluted Magnetic Semiconductors In Table 15.2, the transition metals and their electron conﬁgurations are summarized. The 3d transition metals are typically used for magnetic impurities in DMS due to their partially ﬁlled 3d shell. Due to Hund’s rule, the spins on the 3d shell are ﬁlled in parallel for the ﬁrst ﬁve electrons up to half ﬁlling (in order to allow the electrons to get out of their way in real space). Thus, the atoms have a sizeable spin and a magnetic moment. The spin of Mn is S = 5/2. Most transition metals have a 4s2 conﬁguration that makes them isovalent in II–VI compounds. We note that Zn has a complete 3d shell and thus no net spin. In Fig. 15.2, an overview of the crystallographic properties is given for Mnalloyed II–(Se,S,Te,O) based DMS [525] (DMS with Se, S, and Te have been discussed in [526]). As an example, the properties of Hg1−x Mnx Te are discussed. This alloy is semiconducting (positive bandgap ǫ0 ) for x > 0.075 and a zerogap material (negative interaction gap ǫ0 ) for smaller Mn concentration (cf. Fig. 6.29). The transitions between the Γ6 and Γ8 bands can be determined with magnetoabsorption spectra in the infrared [527]. In Fig. 15.3a, the magnetic ﬁeld dependence of transition energies between different Landau levels is shown that can be extrapolated to yield the interaction gap. The interaction gap is shown in Fig. 15.3b as a function of the Mn concentration. For small Mn concentrations, the DMS behaves like a paramagnetic material. For larger concentrations, the Mn atoms have increasing probability to be directly neighbored by another Mn atom and suffer superexchange interaction (cf. Eq. (3.19b)). At a certain critical concentration xc , the cluster size becomes comparable with the size of the sample. If interaction up to the ﬁrst, second or third neighbor are taken into account for a fcc lattice, the critical concentrations are given by xc =0.195, 0.136, and 0.061, respectively [528]. The nearestneighbor interaction between Mn atoms in such DMS
Table 15.2. 3d, 4d and 5d transition metals and their electron conﬁgurations. Note that Hf72 has an incomplete 4fshell with 4f14 Sc21
Ti22 2
V23
3d 4s
3d
3d
3d
4s2
4s2
4s2
Y
39
4d 5s
2
Zr
40
4d2 5s
2
Cr24
3
41
5
Mn25 5
3d
4s2 42
43
Fe26 6
3d
4s2 Ru
Co27 7
3d
4s2 44
Rd
45
Ni28
Cu29
8
3d
4s2
4s
3d
Pd
46
10
Ag
Zn30 3d10 4s2
47
Cd48
Nb
Mo
Tc
4d4
4d5
4d6
4d7
4d8
4d10
4d10
4d10
5s
5s
5s
5s
5s
−
5s
5s2
Pt78
Au79
Hg80
La57
Hf 72
Ta73
W74
Re75
Os76
Ir77
5d
5d2
5d3
5d4
5d5
5d6
5d9
5d9
5d10
5d10
2
2
2
2
2
−
6s
6s
6s2
6s
2
6s
6s
6s
6s
6s
362
15 Magnetic Semiconductors
VI Fig. 15.2. Diagrammatic overview of AII alloys and their crystal struc1−x Mnx B tures. The bold lines indicate ranges of the molar fraction x for which homogeneous crystal phases form. ‘Hex’ and ‘Cub’ indicate wurtzite and zincblende, respectively. From [525]
as (Zn,Cd,Hg)Mn(S,Se,Te) was found to be antiferromagnetic,1 i.e. neighboring spins are aligned antiparallel. Due to frustration of antiferromagnetic longrange order on a fcc lattice, an antiferromagnetic spin glass forms. The transition temperature TC between the paramagnetic and spinglass phases of Hg1−x Mnx Te is shown in Fig. 15.4. In III–V compounds, the 3d transition metals represent an acceptor if incorporated on the site of the groupIII element as, e.g., in the much investigated compound Ga1−x Mnx As. This material will be used in the following to discuss some properties of magnetic semiconductors. It seems currently well understood and has a fairly high Curie temperature of TC ≈ 160 K. Ferromagnetism in a diluted magnetic semiconductor is believed to be caused by indirect exchange through itinerant charge carriers. The ferromagnetic coupling can be invoked by the Ruderman–Kittel–Kasuya–Yoshida (RKKY) interaction, i.e. the spins of the paramagnetic ions are aligned via interaction with the free carriers in the semiconductor. A related concept is the double exchange2 [529–531] in which carriers move in a narrow Mnderived dband (for dwave character cf. Fig. 7.13c). Such a mechanism was ﬁrst invoked for PbSnMnTe [532]. Later, ferromagnetism was discovered in InMnAs [533] and GaMnAs [534]. In (In,Ga)MnAs a Mn ion (spin up) spin polarizes the surrounding hole gas (spin down), which has been supplied from the Mn 1
Such superexchange leads to antiferromagnetic interaction if the bond angle is ‘close’ to 180◦ . 2 This model is also called the Zener model.
15.3 Diluted Magnetic Semiconductors
363
300
Hg1xMnxTe 200
370
0 (meV)
100
Hg1xMnxTe x=0.004
E (meV)
350
100
330
200
310 290
0 270 0
(a)
0
1
2
3 H (T)
4
300 0
5
(b)
0.05
0.1
0.15
x
Fig. 15.3. (a) Energies of Γ6 → Γ8 transitions vs. magnetic ﬁeld for Hg0.996 Mn0.004 Te at T = 2 K. Symbols are experimental values for two polarization directions as indicated. Numbers denote quantum numbers of transitions. Solid lines are theoretical ﬁts. (b) Interaction gap vs. Mn concentration for Hg1−x Mnx Te at T = 4.2 K. Various symbols represent data from diﬀerent authors and methods. Dashed line is a guide to the eye. Adapted from [527]
acceptors. This mechanism lowers the energy of the coupled system. The interaction H = −βN0 Ss
(15.1)
between the Mn dshell electrons (S = 5/2) and the plike free holes (s = 1/2) is facilitated by p–d hybridization of the Mn states. N0 denotes the concentration of cation sites. The coupling via electrons is much weaker (coupling coeﬃcient α). The holes interact with the next Mn ion and polarize it (spin up), thus leading to ferromagnetic order. The ferromagnetic properties are evident from the hysteresis shown in Fig. 15.6a. Without the carrier gas such interaction is not present and the material is only paramagnetic. Theoretical results for the Curie temperature of various ptype semiconductors are shown in Fig. 15.5. Generally, the quest for higher Curie temperatures (well above room temperature) is underway and widebandgap materials such as GaN or ZnO doped with transition metals have shown some encouraging results. Mnsubstituted chalcopyrite semiconductors are analyzed theoretically
364
15 Magnetic Semiconductors
25 Hg1xMnxTe
TC (K)
20 15
P
10 SG 5 0
0.1
0.2
0.3 x
0.4
0.5
Fig. 15.4. Magnetic phase diagram of Hg1−x Mnx Te, ‘P’ (‘SG’) denotes the paramagnetic (spin glass) phase. Various symbols represent data from diﬀerent authors and methods. Dashed line is a guide to the eye. Adapted from [527]
Fig. 15.5. Computed values of the Curie temperature TC for various ptype semiconductors plotted vs. the bandgap (dashed lines are guides to the eye). All materials contain 5% Mn on the cation sublattice and a hole concentration of p = 3.5 × 1020 cm−3 . Values for TC taken from [531]
in [535] and are predicted to exhibit lessstable ferromagnetism than III–V semiconductors of comparable bandgap. The carrier density and thus magnetic properties in a DMS can be controlled in a spacecharge region (cf. Sect. 18.2.2) as demonstrated in [536]. In Fig. 15.6, results are shown for hydrogen (deuterium) passivated GaMnAs that exhibits ferromagnetism as ‘asgrown’ thin ﬁlm. The deuterium is incorporated in similar concentration as the Mn, assumes a backbond position (forming a H–As–Mn complex) and compensates the hole gas from the Mn
15.4 Spintronics
365
(cf. Sect. 7.8). The lowtemperature conductivity drops nine orders of magnitude [537]. Such material displays only paramagnetic behavior. An optimal Mn concentration for ferromagnetic Ga1−x Mnx As is around x = 0.05. For smaller Mn concentrations, the hole density is too small and the Curie temperature drops; for larger Mn concentrations, the structural properties of the alloy degrade (phase separation into GaAs and MnAs.3 )
Fig. 15.6. Magnetization M vs. magnetic ﬁeld H for Ga0.963 Mn0.037 As at low temperature. (a) Comparison of asgrown (full squares) and deuterated (open circles) thin ﬁlm with magnetic ﬁeld in the layer plane at T = 20 K. (b) Magnetization of the deuterated sample at T = 2 K for larger magnetic ﬁelds. Solid line is Brillouin function for g = 2 and S = 5/2. Adapted from [537]
Magnetic hysteresis has been found in nconducting Mndoped ZnO [538, 539] (Fig. 15.7). Such material is interesting due to its small spinorbit coupling. The exchange mechanism is under debate.
15.4 Spintronics Spintronics (as opposed to electronics) is an emerging ﬁeld that uses the electron spin rather than its charge for transport, processing and storage of information. Prototype devices are the spin transistor and the spin LED. It remains to be seen whether spintronics can be developed to its theoretically envisioned potential and will play a commercially important role in the course of microelectronics. The spin degree of freedom also promises potential for quantum information processing due to its weak coupling to charge and phonons and the resulting long dephasing time.
3 MnAs is a ferromagnetic metal. MnAs clusters can be a problem since they create ferromagnetic properties but not in the way the DMS is supposed to work.
366
15 Magnetic Semiconductors 0.08 10K
Zn0. 935Mn0. 065O
M (emu/g)
0.04 300K 0
0.04
0.08 7
3.5
0 H (kOe)
3.5
7
Fig. 15.7. Magnetization M vs. magnetic ﬁeld H for Zn0.935 Mn0.065 O thin ﬁlm at T = 10 and 300 K. A hysteresis is obvious for both temperatures
15.4.1 Spin Transistor In this device (for regular transistors cf. Chap. 21), spinpolarized electrons are injected from contact 1, transported through a channel and detected in contact 2. During the transport, the spin rotates (optimally by π) such that the electrons cannot enter contact 2 that has the same magnetization as contact 1. The spin rotation is caused by spinorbit interaction due to the electric ﬁeld under the gate contact. This effect is called the Rashba effect and is purely relativistic [540]. As channel material, a semiconductor with strong spinorbit coupling such as InAs or (In,Ga)Sb is preferable. However, the use of narrowgap semiconductors and the increase of spin scattering at elevated temperatures [541] make the realization of such a transistor at room temperature diﬃcult.
source
gate
drain
Fig. 15.8. Scheme of spin transistor after the proposal of [542]. Source and drain are ferromagnets with their magnetization shown schematically as arrows. The channel under the gate transports electrons whose spin rotates in the electric ﬁeld under the gate
15.4 Spintronics
367
15.4.2 Spin LED In a spin LED (for LEDs see Sect. 20.3), the injection of spinpolarized carriers into the active layer leads to circularly polarized luminescence. The spin alignment can be achieved with semimagnetic semiconductors grown on top of the active layer or via spin injection from a ferromagnetic metal into the semiconductor (for metal–semiconductor junctions see Sect. 18.2). In Fig. 15.9a, a Fe/AlGaAs interface is shown. Ideally, the spinpolarized electrons from the ferromagnetic metal tunnel into the semiconductor and transfer to the recombination region. Subsequently, the emission is circularly polarized (Fig. 11.18b). The degree of circular polarization is Pσ =
Iσ+ − Iσ− , Iσ+ + Iσ−
(15.2)
with Iσ± being the intensity of the respective polarization. The degree of polarization depends on the magnetization of the metal. For the saturation magnetization of Fe, the maximum polarization is about 30% at T = 4.5 K (Fig. 15.9b) [543]. The interface and its structural nonideality of the interface presumably prevent the spin injection from being 100% eﬃcient [544]. MFe Fe/ AlGaAs/ GaAs
Fe
AlGaAs (a) (110)
[001]
(b)
Fig. 15.9. (a) Transmission electron microscopy image of the (110) cross section of the Fe/AlGaAs interface of a spin LED. The vertical lines in Fe are the (110) planes with 0.203 nm distance. (b) Magneticﬁeld dependence of the circular polarization ratio Pσ at T = 4.5 K (15.2) (ﬁlled and empty circles) and the outofplane component of the Feﬁlm magnetization (dashed line, scaled to the maximum of Pσ ). Reproduced from [544] by permission of the MRS Bulletin
16 Organic Semiconductors
Organic semiconductors are based on carbon compounds. The main difference from inorganic semiconductors is the sp2 bond (see Sect. 2.2.3) as present in graphite. Diamond, although consisting of 100% carbon, is not considered an organic semiconductor. We note that carbon can form further interesting structures based on sp2 bonds, such as carbon nanotubes or fullerenes. Carbon nanotubes are graphene sheets rolled up to form cylinders. Their walls can consist of a single graphene sheet (SWNT, singlewall carbon nanotube) or of several sheets (MWNT, multiwall carbon nanotube). Fullerenes are soccerballlike molecules such as C60 .
16.1 Materials The prototype organic molecule is the benzene molecule with its ringlike structure (Fig. 2.8). The pz orbitals are partially ﬁlled and there is a separation between HOMO and LUMO (Fig. 2.11). A similar consideration is valid for polymers. The coupling of orbitals along the polymer chain leads to broadening of the π and π ∗ states into a (ﬁlled) valence and an (empty) conduction band, respectively (Fig. 16.1).
conduction band
valence band
6 pz 18 sp2
Fig. 16.1. Schematic band structure of a polymer originating from the states of the benzene molecule (cf. Fig. 2.11)
370
16 Organic Semiconductors
Fig. 16.2. Various organic compounds: 1: naphtalene, 2: anthracene, 3: tetracene, 4: pentacene, 5: pyrene, 6: perylene, 7: anthanthrene, 8: chrysene, 9: ovalene, 10: coronene, 11: violanthrene, 12: isoviolanthrene, 13: pyranthrene, 14: mdinaphthanthrene, 15: pterphenyl, 16: anthanthrone, 17: violanthrone, 18: isoviolanthrone, 19: pyranthrone, 20. mdinaphthanthrone
(a)
(b)
(c)
(d)
O
N
Al
N
(e)
O
O
N
(f)
Fig. 16.3. Organic compounds: (a) thiophene, (b) pyridine, (c) poly(pphenyl), (d) poly(pphenylvinyl), (e) Alq3 (tris(8hydroxyquinolate)aluminum) and (f ) a threedimensional view of the Alq3 molecule. Part (f ) reprinted with permission c from [466], 1998 AIP
16.2 Properties
371
There is a large number of organic, semiconducting molecules that differs by the number of benzene rings (Fig. 16.2), the substitution of carbon atoms by nitrogen or sulfur (Fig. 16.3a,b), the polymerization (Fig. 16.3c) or the substitution of hydrogen atoms by side groups (Fig. 16.3d). Since PPV is insoluble, typically derivatives such as MEHPPV1 [465] that are soluble in organic solvents are used. Compared to benzene, the substitution of one carbon atom by nitrogen (pyridine) represents doping with one electron. In Fig. 16.4, the most important building blocks of organic molecules are shown. R
RHC
H
alkane
CHR
alkene
O
R RC
CR
OH
carboxylic acid
O
alkyne
ester R
OR
aromatic
O
amide R
OH
alcohol
R
OR
ether
R
NHR O
O
R
ketone R
Cl R
acid chloride
NH 2
amine
NH
imine
N
nitrile
R O
RHC
aldehyde R
H
RC
Fig. 16.4. Building blocks of organic molecules, ‘R’=alkyl group, i.e. CH 3 (methyl), CH3 CH2 (buthyl), . . .
Small organic molecules can crystallize into solids due to vanderWaals interaction. In Fig. 16.5, the monoclinic unit cell of an anthracene crystal is shown.
16.2 Properties For organic semiconductors, the conductivity within a molecule, e.g. a long polymer chain, and the conductivity between different molecules have to be distinguished. A magnetic ﬁeld induces a circular current within the benzene 1
2ethoxy,5(2’ethylhexyloxy)1,4phenylene vinylene
372
16 Organic Semiconductors
Mobility (cm2/Vs)
Fig. 16.5. Monoclinic unit cell of anthracene crystal 10
3
10
2
10
1
10
0
10
1
10
2
10
3
10
4
10
5
Si wafers polySi aSi:H
pentacene thiophene oligomers polythiopenes
6
10 1985
1990
1995 Year
2000
Fig. 16.6. Historic development of the experimentally achieved mobility of organic semiconductors
molecule. This current will ﬂow unhindered (diamagnetic effect) as long as the HOMO/LUMO gap is large enough to prevent thermal excitations. The conduction between different molecules occurs via hopping. Typically, the conductivity is thermally activated according to
E σ = σ0 exp − , (16.1) kT where E is an energy of the order of 1 eV. The photoconductivity is related to the absorption spectrum (Fig. 16.7). The mobility is mostly much smaller than 1 cm2 /V s (Fig. 16.6) and thus much smaller than that of crystalline silicon and rather comparable to that of amorphous silicon. The density of excited (empty) states of the Alq3 molecule is shown in Fig. 16.8 together with the orbitals associated with the four prominent states.
16.2 Properties
373
Projected DOS
Fig. 16.7. Photoconductivity and absorption spectrum of anthracene
(a)
(b)
Fig. 16.8. (a) Projected density of states (for C, N, and O) of excited states in an Alq3 molecule. The origin of the energy axis is the HOMO level. (b) Orbitals for c the four states labeled I–IV in (a). Reprinted with permission from [466], 1998 AIP
The lowest orbital is the LUMO and leads to the visible luminescence of the Alq3 in the red. Organic molecules can emit light eﬃciently and are thus useful for light emitters. In Fig. 16.9, the photoluminescence (PL) and the PL excitation (PLE) spectra of polythiophene are shown. The recombination is below the bandgap of 2.1–2.3 eV on an excitonic level at 1.95 eV. There are several phonon replica whose separation of 180 meV corresponds to the C–C stretching mode. The PLE demonstrates that the PL at 1.83 eV can be excited via the exciton level. The theoretical band structure of polythiophene is shown in Fig. 16.10a. The Brillouin zone is onedimensional. The situation I corresponds to a single molecular chain, the situation II pertains to the chain embedded in a medium
374
16 Organic Semiconductors
(b)
(a)
Fig. 16.9. (a) Photoluminescence (PL) and absorption spectra, (b) PL excitation (PLE) spectrum (Edet = 1.83 eV) of polythiophene. Reprinted with permission c from [467], 1987 APS
(a)
(b)
(c)
Fig. 16.10. (a) Band structure of polythiophene (‘I’: naked chain, ‘II’: chain in a dielectric medium ( = 3)), (b) singleparticle energies and bandgap, (c) exciton c levels (‘E’: experimental values). Reprinted with permission from [468], 2002 APS
with a dielectric constant ǫ = 3. The predicted bandgaps are 3.6 and 2.5 eV, respectively. The exciton binding energy is about 0.5 eV. The exciton is a Frenkel exciton that has a small extension and is localized. The high binding energy is favorable for radiative recombination since the exciton is stable at room temperature. For photovoltaic applications, it is unfavorable since it has to be overcome in order to separate electrons and holes (after absorption). Generally, intrachain excitons (as here) and interchain excitons, where electron and the hole are localized on different chains, are distinguished.
17 Dielectric Structures
17.1 PhotonicBandgap Materials 17.1.1 Introduction A structure with a socalled photonic bandgap (PBG) exhibits an energy range (color range) in which photons cannot propagate in any direction. In the photonic bandgap, there are no optical modes, no spontaneous emission and no vacuum (zeroﬁeld) ﬂuctuations. We recollect that spontaneous emission is not a necessary occurrence: Looking at Fermi’s golden rule (9.9) for the transition probability integrated over all ﬁnal states w(E) =
2π M 2 ρf (E) ,
(17.1)
we see that the decay rate depends on the density ρf of ﬁnal states at energy E. In the case of spontaneous emission, this is the (vacuum) density Dem of electromagnetic modes (per energy per volume) that varies ∝ ω 2 : Dem (E) =
8π E2 . (hc)3
(17.2)
In a homogeneous optical medium c must be replaced with c/n. If the bandgap of a PBG is tuned to the electronic gap of a semiconductor, the spontaneous emission, and also induced emission, can be suppressed. Thus, one mode has to be left by ‘doping’ the structure. In this mode all emission will disappear and an eﬃcient singlemode (monochromatic) LED or ‘zerothreshold’ laser could be built. A schematic comparison of the band structure (dispersion) of electrons and photons is given in Fig. 17.1. 17.1.2 General 1D Scattering Theory The formation of a photonic bandgap in a onedimensional dielectric can be calculated to a large extent analytically and thus with direct insight. Let n(x) be the spatially varying index of refraction (no losses or nonlinear optical effects). The onedimensional wave equation (Helmholtz equation) reads for the electric ﬁeld E
376
17 Dielectric Structures
Fig. 17.1. Right: electromagnetic dispersion with a forbidden gap at the wavevector of the periodicity. Left: Electronwave dispersion typical of a directgap semiconductor, the dots representing electrons and holes. When the photonic bandgap straddles the electronic bandgap, electron–hole recombination into photons is inhibited since the photons have no place to go (zero ﬁnal density of states)
∂ 2 E(x) ω2 2 + n (x) E(x) = 0 . ∂x2 c2 A comparison with a onedimensional Schr¨ odinger equation
(17.3)
∂ 2 Ψ (x) 2m − 2 [V (x) − E] Ψ (x) = 0 (17.4) ∂x2 shows that the Helmholtz equation corresponds to the quantummechanical wave equation of zero external potential V and a spatially modulated mass, i.e. a case that is usually not considered in quantum mechanics. Let us consider now the amplitude ak of the k eigenvector. The eigenvalue is ωk . The onedimensional mode density ρ(ω) (per energy and per unit length) is dk , (17.5) dω which is the inverse of the group velocity. We follow onedimensional scattering theory as presented in [469]. At this point we do not rely on any speciﬁc form of n(x) (Fig. 17.2a). The (complex) transmission coeﬃcient t for any index structure is √ (17.6) t = x + iy = T exp(iφ) , ρ(ω) =
where tan φ = y/x. φ is the total phase accumulated during propagation through the structure. It can be written as the product of the physical thickness of the structure d and the effective wave number k. Hence we have the
17.1 PhotonicBandgap Materials
377
n 1
t
r
0
n
x
d
0
(a)
1
tN ...
rN (b)
0 n
d
2d
3d
0 x
(N1)d Nd
d 1 d2
n2
1
n1
rN
(c)
tN ...
0
2d
d
3d
0 (N1)d Nd
x
Fig. 17.2. 1D scattering problem: (a) General scattering of an index of refraction distribution, (b) N period stack, (c) twolayer (quarterwave) stack.
dispersion relation d d y tan(kd) = . dω dω x
(17.7)
Evaluating the derivative we ﬁnd 1 cos2 (kd)
d
dk y ′ x − x′ y = , dω x2
(17.8)
where the prime denotes derivation with respect to ω. Using the relation cos2 θ = (1 + tan2 θ)−1 , we obtain the general expression ρ(ω) =
1 y ′ x − x′ y dk = . dω d x2 + y 2
(17.9)
17.1.3 Transmission of an N Period Potential Now, the behavior of N periods of a given index distribution n(x) within a thickness d of one period (Fig. 17.2b) is investigated. The scattering matrix M connects " the intensity at x = 0 with that at x = d. We use the column # u+ containing the right and leftgoing waves (labeled ‘+’ vector u = u− and ‘−’, respectively), u± = f ± exp(±ikx),
378
17 Dielectric Structures
u(0) = M u(d) .
(17.10)
Using the boundary conditions u(0) = (1, r) and u(d) = (t, 0), we ﬁnd that M has the structure # " 1/t r∗ /t∗ . (17.11) M= r/t 1/t∗ The conservation of energy requires that det M = (1 − R)/T = 1. The eigenvalue equation for M is μ2 − 2μRe(1/t) + 1 = 0 .
(17.12)
The two eigenvalues μ± are related by μ+ μ− = det M = 1. If we consider an inﬁnite, periodic structure, we know from Bloch’s theorem that the eigenvector varies between unit cells only via a phase factor, i.e. μ = 1. Therefore, the eigenvalues can be written as μ± = exp(±iβ) ,
(17.13)
where β corresponds to the Bloch phase of a hypothetical inﬁnite periodic structure. This phase β should not be confused with φ deﬁned earlier, which is associated with the unit cell transmission. We ﬁnd the condition Re(1/t) = cos β
(17.14)
for the Bloch phase. Since every matrix obeys its own eigenvalue equation, we have also (1 being the unity matrix) from (17.12) M2 − 2M cos β + 1 = 0 .
(17.15)
By induction one can show that the N period case has the scattering matrix MN = M
sin((N − 1)β) sin(N β) −1 . sin β sin β
(17.16)
The solution for the ﬁnite period case can be written in terms of the Bloch phase of the inﬁnite potential. The transmission and reﬂection of the N period system are given by 1 1 sin(N β) sin((N − 1)β) = − tn t sin β sin β rn r sin(N β) . = tn t sin β The transmission of intensity can be written as (T = t∗ t) 1 sin2 (N β) 1 =1+ − 1 . TN T sin2 β
(17.17a) (17.17b)
(17.18)
17.1 PhotonicBandgap Materials
379
Again, up to this point no speciﬁc distribution of the index of refraction within the unit cell has been speciﬁed. From (17.17a), a general formula for the mode density ρN (ω) (17.9) of the N stack can be obtained as [469] % $ sin(2N β) ηξ ηξξ ′ + −N η 2 2 sin β 1−ξ 1−ξ 2 1 (17.19) ρN = $ %2 , Nd β) cos2 (N β) + η 2 sin(N sin β
where ξ = x/T = cos β and η = y/T . 17.1.4 The QuarterWave Stack
A quarterwave stack, also known as a Bragg mirror, exhibits a onedimensional photonic bandgap. One period consists of two regions with thickness and index of refraction (d1 , n1 ) and (d2 , n2 ), respectively (Fig. 17.2c). In the quarterwave stack each region has an optical thickness of λ/4 (the wave accumulates in each region a phase of π/2) for a particular wavelength λ0 or (midgap) frequency ω0 . Thus, the condition reads n1 d 1 = n2 d 2 =
π c λ0 = . 4 2 ω0
(17.20)
The transmission of an arbitrary twolayer cell is t=
T12 exp(i(p + q)) , 1 + R12 exp(2iq)
(17.21)
where p = n1 d1 ω/c and q = n2 d2 ω/c are the phases accumulated in the two layers, respectively. The values of T12 and R12 are given from the Fresnel formula (9.7) as 4n1 n2 (n1 + n2 )2 (n1 − n2 )2 = . (n1 + n2 )2
T12 =
(17.22a)
R12
(17.22b)
For the quarterwave stack (p = q = π/2), we obtain for (17.21) t=
˜) T12 exp(iπ ω , 1 + R12 exp(iπ ω ˜)
(17.23)
where ω ˜ = ω/ω0 is the frequency scaled to the midgap value. The transmission of a single twolayer cell is T =
2 T12 2 , 1 − 2R12 cos(π ω ˜ ) + R12
(17.24)
380
17 Dielectric Structures
and the Bloch phase is given by cos(π ω ˜ ) − R12 T12 sin(π ω ˜) . η= T12
cos β = ξ =
(17.25a) (17.25b)
For the N period quarterwave stack the transmission is given by TN =
1 + cos β . 1 + cos β + 2(R12 /T12 ) sin2 (N β)
(17.26)
A bandgap forms. Within the bandgap, the density of modes is lowered, at the edges it is enhanced (Figs. 17.3 and 17.4). The transmission at midgap 2N decreases exponentially as ∝ (ni /nj ) , where ni < nj .
(a)
(b) Fig. 17.3. Quarterwave stack with indices of refraction (a) n1 , n2 = 1.0, 1.5 and (b) 1.0, 3.0. Solid lines: dimensionless density of modes ρN (17.19), dashed lines: transmission TN (17.26) for two diﬀerent numbers of pairs N = 5 (left panels) and 10 (right panels) vs. the dimensionless frequency ω ˜
In the limit of large N the complete width Δ˜ ω of the bandgap is
2 π n1 − n2 cos . (17.27) Δ˜ ω =1−2 2 n1 + n2
17.1 PhotonicBandgap Materials
381
(b)
(a)
Fig. 17.4. Quarterwave stack with indices of refraction n1 , n2 = 1.0, 1.5: (a) Transmission TN at midgap (˜ ω = 1, down triangles) and at the band edge (˜ ω = 1 − Δ˜ ω /2, up triangles) vs. number of pairs N . (b) Dimensionless density of modes ρN at maximum near the band edge and at midgap vs. number of pairs N
If n1 − n2  ≪ n1 + n2 , we ﬁnd Δ˜ ω≈
4 n1 − n2  . π n1 + n 2
(17.28)
The principle of the quarterwave stack is scalable to frequencies other than visible light. As an example, a Mo/Si Bragg mirror with a period of 6.7 nm is shown in Fig. 17.5. Such a mirror works in the extreme UV and is used for soft Xray optics, possibly in advanced lithography systems. 0.7
50nm
0.6
Mo/Si
Reflectivity
0.5
Mo Si
0.4 0.3 0.2 0.1
(a)
Si
0 12.2
(b)
12.4
12.6 12.8 Wavelength (nm)
13.0
13.2
Fig. 17.5. (a) Crosssectional TEM of Mo/Si superlattice with 2.7 nm Mo and 4.0 nm Si (period: 6.7 nm) on Si(001) substrate. From [470]. (b) Reﬂection spectrum for a SL with period of 6.5 nm and 88.5◦ angle of incidence. Data points are shown as circles, the solid line is a ﬁt with a period of 6.45 nm. Adapted from [471]
382
17 Dielectric Structures
17.1.5 Formation of a 3D Band Structure For applications, 3D (or at least 2D) photonic bandgap structures are needed. Further details can be found in [472, 473]. In [474] planar, cylindrical and spherical Bragg mirrors are discussed. Since we want a photonic bandgap that is present for all directions of propagation, a Brillouin zone with a shape close to a sphere is preferable. Then, the main directions are at similar kvalues (Fig. 17.6). One of the best suited is the fcc lattice. Since the L point is centered at ≈14% lower frequency than the X point, the forbidden gaps for different directions must be, however, suﬃciently wide to create a forbidden frequency band overlapping at all points along the surface of the Brillouin zone. For example, the bcc lattice has a Brillouin zone that is more asymmetric than that of the fcc lattice (cf. Fig. 3.31) and thus is less suited for the creation of a photonic bandgap. Maxwell’s equations (zero charge density) for monochromatic waves ∝ exp(iωt) ∇·D = 0 μω ∇×E = i H c ω ∇×H = i D c ∇(μH) = 0 ,
(17.29a) (17.29b) (17.29c) (17.29d)
together with D(r) = ǫ(r)E(r) and μ = 1 are combined into the wave equation ω2 ∇ × ǫ−1 (r)∇ × H(r) + 2 H(r) = 0 . c
(17.30)
kz X W
X
L U
X
! kx
(a)
L
ky
K
(b)
L X
k
Fig. 17.6. The facecentered cubic Brillouin zone (a) in reciprocal space. Schematic forbidden gaps (b) at the L and X points
17.1 PhotonicBandgap Materials
383
Fig. 17.7. (a) Calculated photonic bandgap structure along symmetry lines in the fcc Brillouin zone of a dielectric structure composed of air spheres in a dielectric background of refractive index n = 3.5. The ﬁlling ratio is 86% air and 14% dielectric material. Dotted and solid lines represent coupling to s and ppolarized light, c respectively. Reprinted with permission from [475], 1990 APS. (b) Density of states for the band structure of part (a)
This equation is numerically solved for planar waves with wavevector k. In the following, results are shown for various structures. In a fcc lattice of air spheres in a dielectric medium with n = 3.6 (a typical semiconductor), no bandgap can be achieved (Fig. 17.7a), only a pseudogap (Fig. 17.7b) appears. In a diamond lattice (two fcc lattices shifted by 1/4 111), a complete photonic bandgap is possible [475] (Fig. 17.8). Recently, a periodic array of spirals (Fig. 17.9) has been predicted to exhibit a large photonic bandgap [476]. Glancingangle deposition [477] (GLAD) is a way to realize such structures. Another method to fabricate structures with arbitrary geom
Fig. 17.8. (a) Calculated photonic band structure for a diamond dielectric structure consisting of overlapping air spheres in a dielectric material with n = 3.6. Filling ratio of air is 81%. The frequency is given in units of c/a, a being the cubic lattice constant of the diamond lattice and c being the velocity of light. (b) Gaptomidgap frequency ratio for the diamond structure as a function of ﬁlling ratio for dielectric spheres n = 3.6 in air (solid circles) and air spheres in dielectric n. Optimal case: air spheres with 82% ﬁlling ratio. Reprinted with permission from [475], c 1990 APS
384
17 Dielectric Structures
(b)
(a)
(c) Fig. 17.9. (a) Tetragonal squarespiral photonic crystal. The crystal shown here has a solid ﬁlling fraction of 30%. For clarity, spirals at the corners of the crystal are highlighted with a diﬀerent shade and height. The tetragonal lattice is characterized by lattice constants a and b. The geometry of the square spiral is illustrated in the insets and is characterized by its width, L, cylinder radius, r, and pitch, c. The top left inset shows a single spiral coiling around four unit cells. (b) Band structure for the direct structure crystal characterized by [L,C,r]=[1.6,1.2,0.14] and a spiral ﬁlling factor fspiral = 30%. The lengths are given in units of a, the lattice constant. The width of the PBG is 15.2% relative to the center frequency for background dielectric constant b = 1 and spiral dielectric constant s = 11.9. The positions of highsymmetry points are illustrated in the inset. Reprinted with permission c from [476], 2001 AAAS. (c) Oblique and edge views of a tetragonal square spiral structure grown using the GLAD (glancingangle deposition) process. Reprinted c with permission from [477], 2002 ACS
etry within a material is twophoton lithography or twophoton holography. Another path to PBG structures are socalled inverted opals. First, a closepacked structure of spheres, e.g. monodisperse silica spheres, is fabricated by sedimentation or selfassembly. The gaps are ﬁlled with a highindex medium and the template is subsequently removed, e.g. by etching or dissolving. The resulting structure is shown in Fig. 17.10a. Such a structure has a photonic bandgap (Fig. 17.10b) if the refractive index is suﬃciently high (> 2.85) [478].
17.1 PhotonicBandgap Materials
(i)
385
(ii)
(iii) (iv) (v)
(a)
(b)
(c) Fig. 17.10. (a) Cartoon showing, in ﬁve steps, the fabrication of an inverse diamond structure with a full photonic bandgap. First, (i) a mixed bodycentered cubic lattice is assembled (ii) after which the latex sublattice is removed; (iii) then the structure is sintered to a ﬁlling fraction of ∼50% after that (iv) silicon or germanium inﬁltration takes place and ﬁnally (v) silica elimination. (b) Photonic band diagrams of (upper panel) a silicon/silica composite diamond opal and (lower panel) made of air spheres in silicon resulting from the removal of the silica spheres from the former. The ﬁlling fraction for silicon is 50%. The inset shows the correspondc ing real space structures. Reprinted with permission from [479], 2001 AIP. (c) SEM images of internal facets of silicon inverse opal: (i) (110) facet, (ii) (111) facet. c Adapted from [480], reprinted with permission from Nature, 2000 Macmillan Magazines Limited
17.1.6 Defect Modes Similar to a perfect periodic atomic arrangement leading to the formation of the electronic band structure, a perfectly periodic dielectric structure leads to the photonic band structure. As we know from semiconductor physics, much of the interesting physics and numerous applications lie in defect modes, i.e.
386
17 Dielectric Structures
localized electronic states due to doping and recombination at such centers. The equivalent in PBG structures are point defects (one unit missing) or line defects (a line of units, straight, bend or with sharp angles, missing). Such defects create localized states, i.e. regions for light localization. In the case of line defects we deal with waveguides that can be conveniently designed and could help to reduce the size of photonic and optoelectronic integrated circuits. 1D Model We revisit our 1D scattering theory and create now a ‘defect’. A simple defect is the change of the width of the center n2 region in a quarterwave stack. For the numerical example, we choose N = 11, n1 = 1, n2 = 2. In Fig. 17.11, the transmission curves are shown for the undisturbed quarterwave stack and the microcavity with n2 dcenter = 2λ0 /4 = λ0 /2. 2 A highly transmissive mode at ω = ω0 arises that is quite sharp with Δω = 3×10−4 . Thus, the quality factor Q, also called the Qfactor or ﬁnesse, Q=
ω0 , Δω
(17.31)
with ω0 being the resonance frequency and Δω being the linewidth, is 3.3×103 in this case. If the thickness is varied (Fig. 17.12), the mode shifts away from the = center. A similar scenario arises for higherorder nl /2cavities, e.g. n2 dcenter 2 4λ0 /4 = λ0 (Fig. 17.13).
(a)
(b)
Fig. 17.11. Defect mode in 1D photonic bandgap: (a) Transmission of N = 11 quarterwave stack exhibiting a photonic bandgap (n1 = 1, n2 = 2) (dashed line) and of microcavity (solid line) with center n2 region of width λ0 /2 (instead of λ0 /4). (b) Relative width of mode is about 3 × 10−4
17.1 PhotonicBandgap Materials
387
Fig. 17.12. Transmission of N = 11 quarterwave stack (n1 = 1, n2 = 2) with center n2 region of widths 1.8 λ0 /4 (dashed line) and 2.2 λ0 /4 (solid line)
Fig. 17.13. Transmission of N = 11 quarterwave stack (n1 = 1, n2 = 2) with center n2 regions of widths 3 λ0 /4 (solid line), 3.5 λ0 /4 (dashdotted line) and 4 λ0 /4 (dashed line)
2D or 3D Defect Modes An example of 2D waveguiding is shown in Fig. 17.14. Point defects can be used for highﬁnesse wavelength ﬁltering. Emitters surrounded by a photonic bandgap material with a defect mode can emit into the defect mode only, leading to spectrally ﬁltered, highly directional emission. 17.1.7 Coupling to an Electronic Resonance In a verticalcavity surfaceemitting lasers (see Sect. 20.4.14), an optical defect mode in a 1D dielectric structure is coupled to an electronic excitation, such as an exciton in a quantum well or dot. In the simplest picture, the
388
17 Dielectric Structures
(b)
(a)
(c) Fig. 17.14. 2D photonic bandgap waveguide structure. (a) Fabrication principle, (b) SEM image of the structure, (c) light guiding at a 90◦ bend. Reprinted with c permission from [481], 2000 AIP
oscillator must emit its radiation into the cavity mode since other modes do not exist in the Bragg band. Thus, the emission energy is given and ﬁxed by the cavity mode. However, the photon mode (ﬁeld oscillator) and the electronic oscillator form a coupled system that generally must be described using quantum electrodynamics. Energy is periodically exchanged between the two oscillators with the Rabi frequency. An analogous phenomenon is investigated in the ﬁeld of atom–cavity interactions. A necessary condition for the observation of such an oscillation is that the radiation energy remains long enough in the cavity that can be expressed as [482, 483] (cf. (17.37)) αd ≫ 1 − R ≈ π/Q ,
(17.32)
17.1 PhotonicBandgap Materials
389
where α is the absorption coeﬃcient of the electronic transition, d is the length of the absorbing medium, R is the reﬂectivity of the cavity mirror and Q is the ﬁnesse of the cavity given in (17.31). This situation is called the strong coupling regime since it leads to anticrossing behavior of the cavity mode and electronic resonance. In the weak coupling regime for small absorption, the resonances cross (within their linewidth). For resonance, the emission intensity of the oscillator into the cavity mode is enhanced and its lifetime is reduced (Purcell effect), which is discussed in Sect. 17.2.2. The transmission T of a Fabry–Perot cavity with two (equal and lossless) mirrors of transmission Tm = 1 − Rm is given by T (ω) =
2 exp (−2Lα(ω)) Tm 2
1 − Rm exp (i2n∗ Lω/c)
,
(17.33)
√ with the complex index of refraction n∗ = nr + iκ = ǫ and α = 2ωκ/c (cf. (9.53)). For an empty cavity, i.e. a (small) background absorption αB and a background index of refraction nr = nB , the resonances occur when the phase shift 2nB Lω/c is an integer multiple of 2π, i.e. for ωm = m
πc , nB L
(17.34)
with m ≥ 1 being a natural number. In the vicinity of the resonance, i.e. for ω = ωm + δω, we can expand exp (2nB Lω/c) ≈ 1 + i2nB Lδω/c and obtain from (17.33) a Lorentzian for the transmission T (ω) ≈
2 exp (−2Lα(ω)) Tm 2
1 − Rm (1 + i2nB L δω/c)
=
(Tm /Rm )2 exp (2Lα(ω)) . (δω)2 + γc2
(17.35)
The frequency width (HWHM) γc of the emptycavity resonance is given by γc =
1 − R′ c , R′ 2nB L
(17.36)
where R′ = Rm exp (−2Lα). Thus, the decay rate (photon loss from the cavity) is proportional to Tm + αB L if both terms are small. The quality factor of the cavity resonance m is given by Q=
mπ ωm . ≈ 2γc 1−R
(17.37)
Now, the electronic resonance is put into the cavity leading to a change in the dielectric function to (cf. (C.11))
f 2 , (17.38) ǫ = nB 1 + 2 1 − ω +iωΓ ω2 0
390
17 Dielectric Structures
where the √ index of refraction due to the electronic resonance is given by n(ω) = ǫ and (C.13a,b). For resonance of the cavity mode and the electronic oscillator, i.e. ωm = ω0 , the solution for the cavity resonance condition 2nr ωL/c = m2π is obtained, using (17.34), from nr (ω) = m
ωm πc = nB . ωL ω
(17.39)
A graphical solution (Fig. 17.15a) yields three intersections of the left and right hands of (17.39). The very high absorption at the central solution (ω = ω0 ) results in very low transmission. The other two solutions1 yield the frequencies of the coupled normal mode peaks. For f ≪ 1, we use (C.13a) in (17.39) and ﬁnd for the splitting ±Ω0 /2 of the two modes Ω02 = f ω02 − Γ 2 .
(17.40)
This frequency is called the Rabi frequency. If the dielectric function of the oscillator is put into (17.33), the splitting is found to be Ω02 = f ω02 − (Γ − γc )2 .
(17.41)
A splitting will only be observable if Ω0 ≫ Γ, γc . If the two resonances ωc and ω0 are detuned by Δ = ωc −ω0 , the splitting Ω of the transmission peaks shows the typical anticrossing behavior of two coupled oscillators Ω 2 = Ω02 + Δ2 .
(17.42)
In the experiment, typically the electronic resonance remains ﬁxed at ω0 and the cavity resonance is detuned by variation of the cavity length across the wafer (Fig. 17.15b). A detailed theory of cavity polaritons is given in [484]. The nonlinear optics of normal mode coupling in semiconductor microcavities is reviewed in [485].
17.2 Microscopic Resonators 17.2.1 Microdiscs A microdisc is a cylindrical resonator with a thickness d that is small compared to the radius R. It can be fabricated from semiconductors and semiconductor heterostructures using patterning and materialselective etching. With underetching a mostly freestanding disc can be made that resides on a post (Fig. 17.16). 1
These solutions only occur for suﬃcient oscillator strength f > (Γ/ω0 )2 , i.e. in the strong coupling regime where Ω02 > 0. The absorption coeﬃcient at ω0 must be larger than Γ n∞ /c.
17.2 Microscopic Resonators
391
Peak position detuning (meV)
20
(b)
(a)
15
GaAs/ AlGaAs c
10 5 0 0 5 10
15 15 10 5 0 5 10 15 20 Cavity detuning (meV)
Fig. 17.15. (a) Graphical representation of (17.39) with the two solutions marked with circles for n∞ = 1 (dashed line), f = 10−3 , Γ/ω0 = 10−2 and ω0 = ωm . (b) Reﬂectivity peak positions (experimental data (circles) at T = 5 K) vs. cavity detuning ωc − ω0 for a cavity with two GaAs/AlGaAs Bragg mirrors (24/33 pairs for the front/bottom mirror) and ﬁve embedded quantum wells whose resonances are closely matched. Solid lines are a theoretical ﬁt according to (17.42) with Ω0 = 4.3 meV. The dashed lines show the electronic resonance ω0 and the cavity resonance ωc . Part (b) adapted from [483]
500nm (a)
(b)
1μm
Fig. 17.16. (a) Side view of a 3µm diameter disc containing one 10nm InGaAs quantum well between 20nm InGaAsP barriers standing on an InP pillar that has been selectively underetched using HCl. (b) Top view SEM image of a 5µm diameter InGaAsP microdisc. The pedestal shape is a rhombus due to anisotropic c etching of the HCl. Adapted from [486], reprinted with permission, 1992 AIP
The coordinate system is (ρ, φ, z) with the z direction being perpendicular to the disc area. Typically, the disc is so thin that there is only one node along z. Solving the wave equation in this geometry [487], the modes are characterized by two numbers (m, l). m describes the number of zeros along the azimuthal direction φ with the ﬁeld amplitude being proportional to exp(±imφ). Thus, except for m = 0, the modes are simply degenerate. Modes with Ez = 0 are called TE modes. This is the preferred polarization of emission. The number l denotes the number of zeros in the radial direction. Only for modes with m = 1, is the intensity nonzero on the axis, i.e. for ρ = 0. All other modes have vanishing intensity in the disc center.
392
17 Dielectric Structures
Q factor (104)
6 5 4 3 2 1 0 0.0 (a)
(b)
0.05
0.1
Fig. 17.17. (a) Field intensity for whispering gallery mode (10, 0) (TMpolarized) for a circle with 1 µm radius (shown as white line) and n = 1.5. The image size is 4 × 4 µm2 . (b) Theoretical quality factor of a 2µm InP microdisc as a function of the deformation parameter (17.44). The insets show (8,0) whispering gallery modes at a wavelength of 1.55 µm for n = 3.4. Part (b) adapted from [489]
The light intensity in whispering gallery modes is preferentially concentrated along the circumference of the disc as shown in Fig. 17.17a. Since the light can only escape via evanescent waves, the light is well ‘captured’ in such a mode. The Qfactor (17.31) is extremely high and takes values of several 104 . In order to couple light out of such a disc, deformed resonators, e.g. with a defect in the form of protrusions [488], were devised. Deformed resonators are discussed in more detail in the next section. 17.2.2 Purcell Effect According to Fermi’s golden rule (17.1), the probability of an optical transition depends on the density of available optical modes (ﬁnal states). If the density of modes is enhanced compared to its vacuum value (17.2) at a resonance of an optical cavity, the lifetime of the electronic state decreases by the Purcell factor [490] FP =
(λ/n)3 3 , Q 4π 2 V
(17.43)
where n is the refractive index of the medium, Q is the quality factor of the cavity resonance and V is the effective mode volume.2 Experiments on the emission of quantum dots (that generally provide small absorption and thus allow for the weak coupling regime) in etched micropillars containing a microcavity (Fig. 17.18a) have shown that indeed the luminescence decay 2 V is given by the spatial integral of the vacuum ﬁeld intensity for the cavity mode, divided by its maximum value.
17.2 Microscopic Resonators
393
0
35
6 5
"0 / "
4 3 2 1 0
5
(b)
(a)
10 15 20 25 Purcell factor FP
30
Fig. 17.18. (a) Micropillar with MBEgrown GaAs/AlAs DBRs and a cavity containing ﬁve layers of InAs quantum dots as indicated. The pillar has been prepared c by reactive ion etching. Reprinted with permission from [491], 1998 APS. (b) Experimental decay time τ of onresonance quantum dot luminescence scaled by oﬀresonance lifetime τ0 = 1.1 ns (close to lifetime in a QD in bulk) for a variety of micropillars with diﬀerent Purcell factors FP . The error bars correspond to the measurement accuracy of the decay time (±70 ps), the dashed line is a guide to the eye. Adapted from [491]
is faster for cavities with large Purcell factor (Fig. 17.18b) [491]. The resonance of cavity mode and emitter leads to an enhanced emission intensity as shown in Fig. 17.19 for the exciton emission of a single quantum dot in a microdisc [492]. 17.2.3 Deformed Resonators The whispering gallery modes in circular (or spherical) cavities are longlived and emission goes into all angles. Light escape is based only on the exponentially slow process of evanescent leakage (neglecting disorder effects such as surface roughness). In order to overcome the isotropic light emission, the resonator needs to be deformed. This can be accomplished with an ellipsoidal shape, i.e. r(φ) = R [1 + ǫ cos φ] ,
(17.44)
where 1 + 2ǫ is the aspect ratio of the ellipse. The increased radiation leads to a decrease of the Qfactor as shown in Fig. 17.17b. Also, a new decay
17 Dielectric Structures
Energy (eV)
1.322
QDX WGM
WGM intensity (arb. units)
394
1.321
1.320
1.319 0
(a)
10
20
30
40
Temperature (K)
50
7 6 5 4 3 2 1 0 1.5
60
1.0
(b)
0.5 0.0 0.5 Detuning (meV)
1.0
Fig. 17.19. (a) Temperature dependence of the energy positions of the whispering gallery mode (WGM) of a 5µm diameter AlGaAs/GaAs microdisc (Q = 6500) and the singleexciton resonance of a single InAs quantum dot contained within the disc. (b) Intensity of WGM mode as a function of the detuning EWGM − EQD−X from the QD single exciton resonance. The excitation density was 15 Wcm−2 for all data. Adapted from [492]
process, refractive escape, becomes possible. A ray that is initially in a whispering gallery trajectory diffuses in phase space until ﬁnally an angle smaller than the critical angle for total reﬂection (9.3) is reached. The ray dynamics becomes partially chaotic [493]. One other possible deformation of the circular disc geometry is a ‘ﬂattened quadrupole’ as shown in Fig. 17.20a. This shape can be parameterized by a deformation parameter ǫ and the angledependent radius r(φ) given by r(φ) = R 1 + 2ǫ cos2 (2φ)
1/2
.
(17.45)
For small deformation, the whispering gallery modes become chaotic and exhibit preferred emission along the long axis of the resonator (Fig. 17.20b). For larger deformations (ǫ ≥ 0.14), a stronger and qualitatively different directionality occurs in the shape of a bowtie [494] as shown in Fig. 17.20c. The optical laser power extracted from deformed resonators was found to increase exponentially with ǫ; for ǫ = 0.2 it was 50 times larger than for the circular resonator. Another modiﬁcation that can be applied to the microdisc in order to increase outcoupling of light, is the spiral resonator [495] as shown in Fig. 17.21a. The radius is parameterized by $ ǫ % φ . (17.46) r(φ) = R 1 + 2π The experimental emission pattern is displayed in Fig. 17.21b. It exhibits a maximum along the direction of the tangent at the radius step. The simulated nearﬁeld intensity of such an emission mode is shown in Fig. 17.21c. In a spiral laser, ray dynamics is also chaotic [497].
17.2 Microscopic Resonators
395
(a)
(b)
(c)
Fig. 17.20. (a) SEM image of a quadrupolar cylinder laser with deformation parameter ≈ 0.16 on a sloped InP pedestal. The light grey area in the top view is the electrical contact. (b) Simulated nearﬁeld intensity pattern of a chaotic whispering gallery mode for = 0.06 and n = 3.3. (c) Simulated nearﬁeld intensity pattern of a bowtie mode for = 0.15. The length of the minor axis for (b) and (c) is 50 µm. c Reprinted with permission from [494], 1998 AAAS
17.2.4 Hexagonal Cavities Hexagonal cavities develop, e.g., in microcrystals of wurtzite semiconductors (with the caxis along the longitudinal axis of the pillar). In Fig. 17.22a, a ZnO tapered hexagonal resonator (needle) is shown. Whispering gallery modes modulate the intensity of the green ZnO luminescence [499].3 In a simple planewave model, the resonance condition is given by 3
We note that besides the green luminescence as in Fig. 10.12, an unstructured green band also occurs that is observed here. Its origin may be linked to the oxygen vacancy [498].
396
17 Dielectric Structures
(a)
(b)
(c) Fig. 17.21. (a) SEM image of a microcavity disc laser diode with a disc radius of 50 µm. The pcontact ring electrode deﬁnes the areas through which carriers are injected into the microdisc and where stimulated emission can take place. (b) Radial distribution of the light output from the spiralshaped microdisc laser diode measured below and above threshold. The radius of the spiral microdisc was r0 = 250 µm and the deformation parameters were = 0.05 (grey) and = 0.10 (black ). An emission beam at an angle of α = 0◦ corresponds to a direction normal to the notch surface as shown in the inset. Below the laser threshold, the emission pattern is essentially isotropic and independent of the deformation parameter. Above the threshold, directional emission is clearly observed with the emission direction at a tilt angle α ≈ 25◦ . The measured divergence angle of the farﬁeld pattern is ∼ 75◦ c for = 0.10 and ∼ 60◦ for = 0.05. Reprinted with permission from [496], 2004 AIP. (c) Simulated nearﬁeld intensity pattern of an emission mode with nkR ≈ 200 c for deformation = 0.10. Reprinted with permission from [495], 2003 AIP
6Ri =
6 hc , N + arctan β 3n2 − 4 nE π
(17.47)
where Ri is the radius of the inner circle (Fig. 17.22d), n is the index of refraction, N is the mode number and β is given by βTM = 1/n (βTE = n) for TM (TE) polarization, respectively. Due to birefringence, n (n⊥ ) has to be used as the index of refraction for TM (TE) polarization. A detailed numerical
17.2 Microscopic Resonators
397
(d)
(e) Fig. 17.22. (a)–(c) SEM images of ZnO nanoneedle fabricated by pulsed laser deposition. (d) Schematic geometry of crosssectional plane. Ri (R) is the radius of the incircle (circumscribing circle). The circumference of the inscribed white hexagon, representing the path of a whispering gallery mode, has a length of 6Ri . (e) Twodimensional plot of spectra recorded along a linescan along the needle’s longitudinal axis. The left vertical axis shows the linescan position x, the right one refers to the respective needle diameter D. The spectral maxima, i.e. the measured WGM energies, appear as bright belts going from the bottom left corner to the right upper one. With decreasing diameter, all resonances shift systematically to higher energies. The white dots give theoretical TMresonance energy positions obtained from (17.47), white crosses give the same for TEpolarization. Reprinted c with permission from [499], 2004 APS
treatment can be found in [500]. From the energy positions of the TE and TM resonances, the birefringence of the resonator can be determined [501]. A N = 26 whispering gallery mode of a hexagonal resonator is shown in Fig. 17.23c,d. The 6fold symmetric emission stems from the edges of the hexagon. While whispering gallery resonators have typically mode numbers N ≫ 1, in such hexagonal resonators the whispering gallery modes could be followed down to N = 1 [499] as shown in Fig. 17.22a,b,e.
398
17 Dielectric Structures
(a)
(b)
(c)
(d)
(e) Fig. 17.23. Simulated nearﬁeld intensity pattern of modes in a cavity with hexagonal cross section (absolute value of electric ﬁeld in linear grey scale): Modes (N = 4) with (a) symmetry −a and (b) mode 4+ (nomenclature from [502]) for n = 2.1 and kR = 3.1553 − i0.0748. Modes (c) 26− and (d) 26+ for n = 1.466 and kR = 22.8725 − i0.1064. The displayed modes have a chiral pattern. Emission originates mostly from the corners. (e) Microphotoluminescence spectra of a single ZnO nanopillar. The three topmost curves are unpolarized. The curve labeled ‘bulk’ shows the unmodulated luminescence of the green luminescence in bulk. The line labeled ‘exp.’ shows the experimental µPL spectrum of the investigated nanopillar. The experimental spectra recorded for TM and TEpolarization, respectively, are shown in the lowest two curves. The curve labeled ‘theory’ displays the theoretical luminescence spectra. Dashed vertical lines are guides to the eye referring to the spectral position of the dominating WGMs. The inset shows a SEM image of the investigated pillar, the scale bar has a length of 500 nm. The dotted lines show the position of the edges of the hexagonal resonator obtained from topography contrast
Part II
Applications
18 Diodes
18.1 Introduction One of the simplest1 semiconductor devices is the diode. It is a socalled twoterminal device, i.e. a device with two leads. The most prominent property of a diode is the rectifying current–voltage (I–V ) characteristic. This function was initially realized with vacuum tubes (Fig. 18.1); a heated ﬁlament emits electrons that are transferred through vacuum to the anode if it is on a positive potential. The semiconductor diode technology led to a tremendous miniaturization, integration with other devices (in planar technology) and cost reduction. We distinguish2 unipolar diodes, for which the majority carriers cause the effects (e.g. metal–semiconductor diodes), and bipolar diodes in which minority carriers play the decisive role, e.g. in the pnjunction diode.
(a)
(b)
Fig. 18.1. (a) Schematic image of a vacuum diode. The electron current ﬂows from the heated cathode to the anode when the latter is at a positive potential. (b) John A. Fleming’s ﬁrst diode ‘valve’, 1904 1
The simplest device is a resistor made from a homogeneous piece of semiconductor, used, e.g., as a part of an integrated circuit or as a photoresistor as discussed in Sect. 19.2. 2 This distinction is not only made for diodes but also many other semiconductor devices such as transistors, see Chap. 21.
402
18 Diodes
18.2 Metal–Semiconductor Contacts The metal–semiconductor contact was investigated in 1874 by F. Braun (see Sect. 1.1). For metal sulﬁdes, e.g. CuFeS2 , he found nonohmic behavior. We remark here that we treat ﬁrst metal–semiconductor contacts with rectifying properties. Later it becomes understandable that metal– semiconductor contacts can also be used as ohmic contacts, i.e. contacts with a very small contact resistance. Rectifying metal–semiconductor contacts are also called Schottky diodes. A very important variation are metal– insulator–semiconductor diodes for which an insulator, mostly an oxide, is sandwiched between the metal and the semiconductor. Such diodes are treated in Sect. 18.3. Reviews on Schottky diodes can be found in [545–548]. 18.2.1 Band Diagram in Equilibrium The metal and the semiconductor have generally different positions of the Fermi levels relative to the vacuum level. When the metal is in contact with the semiconductor, charges will ﬂow in such a way that in thermodynamic equilibrium the Fermi level is constant throughout the structure.3 In the following we treat two limiting cases: The contact of a metal with a semiconductor without any surface states (Schottky–Mott model) and a contact where the semiconductor has a very high density of surface states (Bardeen model). The position of the Fermi level in the metal is given by the work function Wm = −eφm that is shown in Fig. 18.2 for various metals. The work function reﬂects the atomic shell structure; minima of the work function exist for groupI elements. The work function is the energy difference between the vacuum level (an electron is at rest in an inﬁnite distance from the metal surface) and the metal Fermi level. Since the electron density in the metal conduction band is very high, the position of the metal Fermi level does not change considerably when charge is exchanged between the metal and the semiconductor. Ideal Band Structure When the metal and the semiconductor are not in contact (Fig. 18.3a), the metal is characterized by its work function Wm = Evac − EF = −eφm and the semiconductor by its electron aﬃnity χsc . Evac − EC = −eχsc is deﬁned as the energy difference between the vacuum level and the conductionband edge.4 First, we assume that φm  > χsc . For an ntype semiconductor, the 3
This situation is similar to the heterostructure interface (Sect. 11.5.3), with the metal, however, having a very short screening length. 4 The use of the Fermi level for the semiconductor here is not suitable since it depends strongly on the doping and temperature.
18.2 Metal–Semiconductor Contacts
403
7 Se
Work function (eV)
6 5
Co Ni As
C B
4 3
Al Si
Ru Nb
Ge
V Fe Ga Ti Mn Cu Sc Zn Be Mg Ca
Pt Ag Te Sn
Rb Mo Sb Zr Cd In Y
Sr
Li
2
Cr
Pd
K
Rb
Re
Au Hg W Bi Ir Ta Os Hf La Pb Tl Nd Gd
Tb Ce Ba Eu Sm Cs
Lu
U Th
1 0
0
10
20
30
40 50 60 Atomic number Z
70
80
90
Fig. 18.2. Work function Wm of various metals Table 18.1. Values of the work function Wm of various metals Z
element
Wm (eV)
Z
element
Wm (eV)
Z
element
Wm (eV)
3 4 5 6 12 13 14 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34
Li Be B C Mg Al Si K Ca Sc Ti V Cr Mn Fe Co Ni Cu Zn Ga Ge As Se
2.4 3.4 4.5 4.8 3.66 4.2 4.2 2.2 2.87 3.5 4.1 4.3 4.4 3.89 4.4 5.0 4.9 4.5 4.3 4.2 4.8 5.1 5.9
37 38 39 40 41 42 44 45 46 47 48 49 50 51 52 55 56 57 58 59 60 62 63
Rb Sr Y Zr Nb Mo Ru Rh Pd Ag Cd In Sn Sb Te Cs Ba La Ce Pr Nd Sm Eu
2.1 2.59 3.1 3.8 4.3 4.2 4.71 4.6 5.0 4.7 4.0 4.12 4.3 4.1 4.8 2.14 2.5 3.5 2.9 3.2 2.7 2.5
64 65 66 67 68 69 70 71 72 73 74 75 76 77 78 79 80 81 82 83 90 92
Gd Tb Dy Ho Er Tm Yb Lu Hf Ta W Re Os Ir Pt Au Hg Tl Pb Bi Th U
3.1 3.0 3.3 3.9 4.1 4.55 5.0 4.8 4.6 5.3 4.8 4.49 3.8 4.0 4.4 3.5 3.6
404
18 Diodes Evac Wm=
e m
metal
semiconductor
Evac
Evac
metal
semiconductor
esc
eVn
Evac
EC EF
eVbi
e Bn
EF
EF
EC EF
w
EV
EV
(a)
(b)
neutral
Fig. 18.3. Schematic band structure of a metal–semiconductor junction that is dominated by bulk properties of the semiconductor. (a) no contact, (b) metal and semiconductor in contact. w denotes the width of the depletion layer. Outside the depletion layer the semiconductor is neutral. φB,n denotes the Schottky barrier height, Vbi denotes the builtin voltage
energy difference between the Fermi level and the conduction band is denoted as −eVn = EC − EF (Vn < 0 for nondegenerate semiconductors). Thus, the position of the semiconductor Fermi level is given as EF = Evac + e(χsc + Vn ). The potential difference φm − (χsc + Vn ) is called the contact potential. If the metal and semiconductor are connected to each other via a conductive link,5 the Fermi levels will equilibrate. For the case of Fig. 18.3 electrons will ﬂow from the semiconductor to the metal. The negative surface charge of the metal is compensated by a positive charge (due to D+ ) in the semiconductor in the vicinity of the surface. If the metal to semiconductor distance is reduced to zero (and surface effects such as nonmatching bonds, surface states, etc., play no role), a (Schottky) barrier of height φBn φBn = φm − χsc
(18.1)
forms at the interface. The subscript ‘n’ stands for the contact on an ntype semiconductor. In the semiconductor there exists a positively charged region that is called the depletion layer or spacecharge layer. Its extension (w in Fig. 18.3d) and properties will be discussed in Sect. 18.2.2. For a contact on a ptype semiconductor the barrier φBp (to the valence band) is (see Fig. 18.4a) φBp = −
Eg + φm − χsc . e
(18.2)
Between the surface of the metal and the bulk part of the semiconductor there is a potential drop 5 This consideration is a gedanken experiment and not the metal–semiconductor contact itself.
18.2 Metal–Semiconductor Contacts metal
nsemiconductor
metal
Evac
405
psemiconductor
Evac EC
e(Vbi V) EC EF
e Bn EF
eV
w
EF
w
eV EF EV
e(Vbi V)
e Bp
EV
(a)
(d)
Evac
Evac EC
eVbi
e Bn EF
EC EF
w
EF
e Bp
w
eVbi
EF EV
EV
(b)
(e)
Evac
Evac
e Bn
EC
e(Vbi V)
EF w
eV
EC EF
w
EF
e Bp
eV E F EV
e(Vbi V)
EV
(c)
(f)
Fig. 18.4. Band structures of metal–semiconductor junctions for (a,b,c) an ntype semiconductor and (d,e,f ) a ptype semiconductor. (b,e) in thermodynamic equilibrium, (a,d) with forward bias (V > 0), (c,f ) with reverse bias (V < 0)
Vbi = −(φBn − Vn ) = −φm + χsc + Vn ,
(18.3)
which is termed the builtin potential (or diffusion voltage). The exact form of the voltage drop, the socalled band bending, will be discussed in Sect. 18.2.2. The surface index is deﬁned as S = ∂φBn /∂φm .
(18.4)
From the present consideration, the same semiconductor with metals of varying work function should result in S = 1.
406
18 Diodes 10
S=1
BN
S=0
C
GaP 1.0
0.5
ECEF (meV)
e Bn (eV)
1.5
GaAs
1.0
GaAs Si GaSb Ge
Si
SiC GaP AlAs BP AlSb
InP
CdS InSb
0 3.0
(a)
4.0 Wm (eV)
0.1 0.1
5.0
(b)
1.0
ZnS
1.0 Eg (meV)
10
AlN SnO2 ZnO KTaO3 SiO2 Al2O3 SrTiO3 Ga2O3
GaS
Surface index S
0.8 CdS GaSe
0.6
ZnSe
0.4
SiC GaTe CdTe
0.2 Ge Si
(c)
CdSe
GaP
GaAs InSb
InP
0 0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0 2.2 2.4
X
Fig. 18.5. (a) Experimental Schottky barrier heights φBn vs. metal work function φm for various metal–semiconductor junctions, ﬁlled squares: GaP, empty squares: GaAs, ﬁlled circles: Si, empty circles: CdS. Dashed lines are guides to the eye, dashdotted lines indicate dependencies for S = 1 and S = 0. Data from [549]. (b) EC − EF at the metal–semiconductor interface vs. the bandgap Eg for Au Schottky contacts on various semiconductors. The dashed line represents EC − EF = 2Eg /3. Data from [550]. (c) Surface index S vs. the electronegativity diﬀerence ΔX between the species of compound semiconductors. Dashed line is a guide to the eye. Adapted from [551]
Band Structure in the Presence of Surface States Experimental data shown in Fig. 18.5a, however, show a different behavior with smaller slope. For GaAs, e.g., the barrier height is almost independent of the metal work function. Thus, a different model is needed for realistic Schottky diodes. A rule of thumb for the dominantly covalent semiconductors is that for ntype material the barrier height is 2/3 of the bandgap and for ptype material 1/3 of the bandgap, such that EC −EF ≈ 2Eg /3 (Fig. 18.5b). Only for ionic semiconductors does S ≈ 1 (Fig. 18.5c). If the semiconductor has a large density of states at its surface, there is a spacecharge region already without the metal. Surface traps are ﬁlled up to the Fermi level (Fig. 18.6a). The size of the band bending in the semicon
18.2 Metal–Semiconductor Contacts Evac Wm=
e m
metal
semiconductor Evac
Evac
metal
407
semiconductor
esc
Evac
EC EF
surface states
EF
EF
eVbi
e Bn
EC EF
EV
(a)
EV
w
(b)
w
Fig. 18.6. Schematic band structure of a metal–semiconductor junction that is dominated by surface properties of the semiconductor. (a) no contact; due to pinning of the Fermi level at surface states of the semiconductor, a depletionlayer of width w is already present. (b) Metal and semiconductor in contact
ductor will be denoted as φBn since it will turn out below as the Schottky barrier height. If the density of surface states is very high, the charge carriers moving from the semiconductor into the metal upon contact formation are accommodated in the surface states and the position of the Fermi level at the semiconductor surface changes only very little. Thus, the spacecharge region is not modiﬁed and it is identical to the surface depletion region. The Schottky barrier height is then given by the band bending at the (bare) semiconductor surface φBn (Fig. 18.6d) and does not depend on the metal work function at all. For this case we ﬁnd for the surface index S = ∂φBn /∂φm = 0. For actual metal–semiconductor contacts the surface index S is between 0 and 1 and a theory involving the semiconductor band structure and midgap (surface) states (MIGS) is needed [236]. For Si, the experimental result is S = 0.27. The corresponding density of surface states is Ds = 4 × 1013 cm−2 eV−1 . 18.2.2 SpaceCharge Region The width w of the spacecharge region is calculated next. First, we make the socalled abrupt approximation. In this approximation (Schottky–Mott model), the charge density ρ in the spacecharge region (0 ≤ x ≤ w) is given by the doping, i.e. ρ = eND . Outside the spacecharge region the semiconductor is neutral, i.e. ρ = 0 and the electrical ﬁeld is zero, i.e. dV /dx = 0. As further boundary conditions the potential at the interface is V (0) = −Vbi < 0. The potential drop in the spacecharge region is determined by the onedimensional Poisson equation ρ d2 V =− , d2 x ǫs
(18.5)
where ǫs is the static dielectric constant of the semiconductor. Using the ansatz V = V0 + V1 x + V2 x2 we ﬁnd
408
18 Diodes
eND V (x) = −Vbi + ǫs
1 wx − x2 2
.
(18.6)
The electric ﬁeld strength is E(x) = −
eND eND (w − x) = Em + x, ǫs ǫs
(18.7)
with the maximum ﬁeld strength Em = −eND w/ǫs at x = 0. From the condition V (w0 ) = 0 we obtain w as
2ǫs Vbi w0 = eND
1/2
.
(18.8)
The thermal distribution of the majority carriers must be treated with a little more care. The dependence of the chargecarrier density ρ = ND+ − n on the potential V is (β = e/kT ) ρ = eND [1 − exp (βV )] .
(18.9)
We note that for the depletion layer V ≤ 0 and n ≤ ND . The charge difference Δρ (due to the tail of the thermal distribution of the majority charge carriers in the depletion layer) between the real distribution (18.9) to the abrupt approximation model with constant charge density (ρ = eND ) in the depletion layer is Δρ(x) = −eND exp (βV (x)) .
(18.10)
The integration of Δρ over the depletion layer yields that the voltage drop Vbi across the depletion layer needs to be corrected by ΔV w x −Δρ(x′ ) kT 1 ′ . (18.11) ΔV = dx dx = [1 − exp(−βVbi )] ≈ ǫs β e 0 0 The approximation is valid for βVbi ≫ 1. Therefore, (18.8) is corrected to
2ǫs w0 = eND
kT Vbi − e
1/2
.
(18.12)
When a potential Vext is applied externally to the diode, (18.12) is modiﬁed by the change in the interface boundary condition, V (0) = −Vbi + Vext . The band structure is shown schematically in Fig. 18.4b for a forward bias and in Fig. 18.4c for a reverse bias. Therefore, we ﬁnally obtain for the depletionlayer width
2ǫs w= eND
kT Vbi − Vext − e
1/2
.
(18.13)
18.2 Metal–Semiconductor Contacts
409
Now we can also give explicitly the value of the maximum electrical ﬁeld (at x = 0)
1/2 2eND kT Vbi − Vext − ǫs e
kT 2 =− Vbi − Vext − . w e
Em = −
(18.14)
We note that so far the barrier height is independent of the applied bias voltage. In the next section, it is shown that this is actually not the case. 18.2.3 Schottky Effect The barrier height is reduced by the imagecharge effect that has been neglected so far. An electron (charge q = −e) at position x in the semiconductor is facing a metal surface. The metal surface is at zero position (Fig. 18.7a). The potential distribution of the free charge is modiﬁed since the metal surface is an equipotential surface. The potential distribution outside the metal is identical to that if an image charge −q were located at −x. This image charge exerts a force (image force Fim ) on the electron Fim = −
q2 , 16 πǫ0 ǫs x2
(18.15)
where ǫs is the relative dielectric constant of the semiconductor. In order to bring an electron to x from inﬁnity the work Eim x q2 (18.16) Fim dx = − Eim = 16 πǫ0 ǫs x ∞ is needed. This image potential energy is shown in Fig. 18.7a. The total energy Etot (solid line in Fig. 18.7a) of the electron in the presence of an electric ﬁeld E is given by Etot = qEx −
q2 . 16 πǫ0 ǫs x
(18.17)
The maximum of this function (dEtot /dx = 0) is at xm xm =
e 16 πǫ0 ǫs E
1/2
.
(18.18)
The barrier (now labeled φB0 ) is reduced by Δφ given by
eE Δφ = 4 πǫ0 ǫs
1/2
= 2Exm .
(18.19)
410
18 Diodes xm 1
Energy (e B0)
e
e B0
eVbi
e Bn
V=Vbi/2 0
V=0
EC EF
EF
1
w
0
(a)
(b)
V=Vbi 1 x (w0 )
2
Fig. 18.7. (a) Energy of a particle with respect to the metal surface (dashed line), conduction band in semiconductor depletion layer (dashdotted line) and combined eﬀect (solid line). The image charge energy lowers the potential barrier −eφB0 by the amount −eΔφ to −eφBn . (b) Conduction band on the semiconductor side of a metal–semiconductor junction at various bias voltages (V = 0, V = +Vbi /2, and V = −Vbi as labeled) taking into account the Schottky eﬀect. The width of the depletion layer is indicated with a short vertical dashed line. The barrier height without Schottky eﬀect is φB0 . The dashed line is the situation without Schottky eﬀect for zero bias
With the ﬁeld in the vicinity of the interface given by Em from (18.15), the barrier reduction is6 3
1/4 e ND kT . (18.20) Vbi − Vext − Δφ = 8 π 2 ǫ30 ǫ3s e For ǫs = 1 (vacuum) and a ﬁeld strength of 105 V/cm the maximum position is at xm = 6 nm and the barrier reduction is Δφ = 0.12 V. For 107 V/cm, xm = 1 nm and Δφ = 1.2 V. For semiconductors with ǫs ∼ 10 the effect is smaller (Fig. 18.8). The Schottky effect depends on the bias voltage as visualized in Fig. 18.7b and therefore the barrier height depends on the applied bias voltage. 18.2.4 Capacitance The total space charge Q (per unit area) in the semiconductor is
1/2 kT Q = eND w = 2eND ǫs Vbi − Vext − . e 6
(18.21)
The term 3s is technically s 2d where d is the imageforce dielectric constant. d is equal to s if the transit time of an electron from the metal to the maximum of the potential energy is suﬃciently long to build up the dielectric polarization of the semiconductor [545].
18.2 Metal–Semiconductor Contacts 10
60
3
Electric field E (V/cm) 4 5 10 10 s=1
50
(meV)
411
40 30 20 10
Au/Si
s=12
0 0
400
100 200 300 E1/ 2 ( (V/cm)1/ 2 )
Fig. 18.8. Electricﬁeld dependence of the image charge lowering of the Schottky barrier. Dashdotted line is for vacuum dielectric constant, dashed line is (18.19) for s =12. Adapted from [552]
Therefore, the capacity C = dQ/dV  (per unit area) of the space charge region7 is given by
eND ǫs C= 2 Vbi − Vext −
kT e
1/2
Equation (18.22) can also be written as 2 Vbi − Vext − 1 = C2 eND ǫs
kT e
=
ǫs . w
.
(18.22)
(18.23)
If 1/C 2 is measured as a function of the bias voltage (C–V spectroscopy), it should be linearly dependent on the bias voltage if the doping concentration is homogeneous (Fig. 18.9a). The doping concentration can be determined from the slope via ND = −
−1 d 1 2 , eǫs dVext C 2
(18.24)
(see Fig. 18.9b) and the builtin voltage Vbi from the extrapolation to 1/C 2 = 0. The Schottky barrier height can be determined from this [553] via 7
A dc bias voltage is set and the capacitance is probed with an ac voltage with small amplitude. A typical frequency of the ac voltage is 1 MHz. However, this might correlate to a characteristic time constant of the system. In this case, another ac frequency is preferred. Probing the capacitance as a function of the ac frequency is called admittance spectroscopy.
412
(a)
18 Diodes
(b)
Fig. 18.9. (a) Capacity C (dashed line) and 1/C 2 (solid line) vs. bias voltage dependence for an Au/GaAs Schottky diode (2µm MOVPEgrown GaAs:Si on a nGaAs substrate) at room temperature. From the extrapolation to 1/C 2 = 0 and (18.23) we obtain Vbi = 804 ± 3 meV. (b) Donor concentration (ND = 4.8 × 1016 cm−3 ) determined via (18.24) from the 1/C 2 plot vs. the depletion layer width (calculated using (18.22))
φBn = Vbi + Vn +
kT − Δφ , e
(18.25)
where Δφ is the barrier lowering due to the image force effect between the ﬂatband and the zerobias cases. We note that for inhomogeneous doping the depth proﬁle of the doping can be determined by C–V spectroscopy. The 1/C 2 vs. bias curve is then no longer a straight line and exhibits a varying slope. At a given bias voltage, the charge (ionized donors or acceptors) at the boundary of the spacecharge region is tested by the capacitance measurement. However, this principle works only if the depth of the spacecharge region actually changes with the bias voltage. The method can therefore not be directly applied to such systems like δdoped layers or quantum wells. 18.2.5 Current–Voltage Characteristic The current transport through a metal–semiconductor junction is dominated by the majority charge carriers, i.e. electrons (holes) in the case of an ntype (ptype) semiconductor, respectively. In Fig. 18.10, the possible transport mechanisms are visualized for an ntype semiconductor. Thermionic emission ‘above’ the barrier involves the hot electrons from the thermal distribution and will be important at least at high temperatures. Tunneling ‘through’ the barrier will be important for −1/2 thin barriers, i.e. at high doping (w ∝ ND , cf. (18.13)). ‘Pure’ tunneling for electrons close to the (quasi) Fermi level, also called ﬁeld emission, and thermionic ﬁeld emission, i.e. tunneling of electrons with higher energies, are distinguished. Also, recombination in the depletion layer and hole injection from the metal are possible.
18.2 Metal–Semiconductor Contacts
413
(1) (2) (3) (4) EF
eV
EC EF
EV
Fig. 18.10. Transport mechanisms at metal–semiconductor junctions. (1) Thermionic emission (‘above’ the barrier) (2) tunneling (‘through’ the barrier), (3) recombination in the depletion layer, (4) hole injection from metal
The transport of electrons above the barrier can be described with diffusion theory [554, 555] or thermionicemission theory [556]. In both cases the barrier height is large compared to kT . For thermionic emission (typically relevant for semiconductors with high mobility) the current is limited by the emission process and an equilibrium (constant electron quasiFermi level) is established throughout the depletion layer and ballistic transport is considered. In diffusion theory (for low mobility) a thermal equilibrium between metal and semiconductor electrons is established in the interface plane and the current is limited by diffusion and drift in the depletion region. Thermionic Emission The current density per unit area js→m of electrons that ﬂow from the semiconductor into the metal is due to the hot electrons from the thermal distribution function ∞ −evx dn . (18.26) js→m = EF −eφBn
The integral starts at the lowest possible energy, the top of the Schottky barrier (no tunneling allowed in this model!). The electron density dn in a small energy interval dE is dn = D(E)f (E)dE .
(18.27)
The carrier velocity is obtained from 1 E = E C + m∗ v 2 . 2
(18.28)
414
18 Diodes
For a bulk semiconductor and the Boltzmann distribution (−eφB ≫ kT ) ∗
m eV m∗ v 2 dn = 2 exp exp − 4πv 2 dv . (18.29) h kT 2kT Using 4πv 2 dv = dvx dvy dvz and integrating over all velocities in y and z directions and vx from the minimum velocity necessary to pass the barrier 1/2 to ∞, the current density is found to be vmin,x = (2e(Vbi − V )/m∗ )
eV eφBn js→m = A∗ T 2 exp exp , (18.30) kT kT with A∗ being the Richardson constant given by A∗ =
2 eNC v¯ 4πem∗ kB = , h3 4T 2
(18.31)
where v¯ is the average thermal velocity in the semiconductor. A∗ for electrons in vacuum is 120 A cm−2 K−2 . A similar result is obtained for the thermionic emission of electrons from a metal into vacuum. Since φBn is negative, the saturation current increases with increasing temperature. If the bias is changed, the current from the semiconductor to the metal increases in the forward direction because the energy difference between the quasiFermi level and the top of the barrier is reduced. The current is reduced for reverse bias. The barrier from the metal into the semiconductor remains constant (except for the Schottky effect whose impact on the current–voltage characteristic is discussed next). Therefore the current from the metal into the semiconductor is constant and can be obtained from the condition j = 0 for zero bias. Therefore the current–voltage characteristic in the thermionicemission model is
eV eφBn ∗ 2 exp −1 (18.32) j = A T exp kT kT
eV = js exp −1 . kT The prefactor js = A∗ T 2 exp
eφBn kT
(18.33)
is called the saturation current density. This dependence is the ideal diode characteristic and is shown in Fig. 18.11. The temperature dependence of the saturation current js can be written as
js eφBn (18.34) = ln A∗ + ln 2 T kT
18.2 Metal–Semiconductor Contacts
415
(b)
(a)
Fig. 18.11. Ideal diode I–V characteristics I = Is (exp(eV /kT ) − 1) (a) in linear plot and (b) semilogarithmic plot
by transforming (18.33). The plot of ln js /T 2 to vs. 1/T is called a Richardson plot and allows the barrier height and the Richardson constant to be determined from a linear ﬁt. If the Schottky effect, i.e. the change of barrier height with bias voltage, is considered, the semilogarithmic slope of the forward I–V characteristic is no longer V0−1 = e/kT but can be expressed as V0−1 = e/nkT , n being a dimensionless parameter termed the ideality factor.8 n is given by n=1+
∂φB . ∂V
(18.35)
Values for n obtained this way (using (18.20)) are smaller than 1.03. For GaAs and ND = 1017 cm−3 n = 1.02. With regard to V0 and its temperature dependence we refer also to Fig. 18.13 and the related discussion. In [557] the effect of a spatial inhomogeneity of the diffusion voltage and thus the barrier height is investigated. The barrier height φBn (x, y) across the contact area is assumed to have a Gaussian probability distribution p(φBn ) with a mean value φ¯Bn and a standard deviation σφ . It turns out that the barrier height φC Bn responsible for the capacity, and thus the diffusion voltage determined by C–V spectroscopy, is given by the spatial average, i.e. φC Bn = φ¯Bn . The barrier height φjBn determining the current–voltage characteristics (cf. (18.32)) via
eV eφBn ∗ 2 (18.36) j = A T exp −1 p(φBn )dφBn exp kT kT # "
eφjBn eV ∗ 2 exp = A T exp −1 kT kT is given by 8
Obviously n = 1 for the ideal characteristic. Otherwise n ≥ 1.
416
18 Diodes
eσφ2 . (18.37) 2kT Thus, the barrier height determined from the current–voltage characteristic underestimates the spatial average of the barrier height.9 The Richardson plot (18.34) is now modiﬁed (and is nonlinear in 1/T ) to
e2 σφ2 eφBn js ∗ = ln A − . (18.38) + ln T2 kT 2k 2 T 2 φjBn = φ¯Bn −
Temperature Dependence Figure 18.12a shows the temperaturedependent I–V characteristics of a Pd/ZnO Schottky diode. A straightforward evaluation according to (18.32) results in a barrier height of about 700 meV and a Richardson constant that is orders of magnitude smaller than the theoretical value of 32 A K−2 cm−2 (for m∗e = 0.27). A ﬁt of the temperaturedependent data with (18.37), as shown in Fig. 18.12b, results in φ¯Bn = 1.1 eV, in agreement with the (temperatureindependent) value obtained from CV spectroscopy, and σφ = 0.13 V [558]. The temperature dependence of the ideality factor n is given by [559] n=
1 , 1 − ρ2 + eρ3 /(2kT )
(18.39)
where ρ2 (ρ3 ) is the (temperatureindependent) proportionality coeﬃcient of the bias dependence of the mean barrier height (standard deviation), i.e. ρ2 = ∂ φ¯Bn /∂V (ρ3 = ∂σφ2 /∂V ). The ﬁt of 1/n − 1 vs. 1/T (Fig. 18.12c) yields ρ2 = −0.025 and ρ3 = −0.028 V. The forward I–V characteristic of an Au/GaAs Schottky diode reported in [560, 561] is shown in Fig. 18.13a at various temperatures. The current amplitude decreases with decreasing temperature due to the temperature dependence of the saturation current (18.32). Also, the slope V0−1 of the characteristic j = js exp(V /V0 ) varies with temperature. Looking at the temperature dependence of V0 , it is described as V0 = k(T + T0 )/e rather than with an ideality factor n in the form of V0 = nkT /e. In other words, the ideality factor follows a temperature dependence n = 1 + T0 /T . In view of (18.39), such behavior means for small T0 that n ≈ 1/(1 − T0 /T ) and thus ρ2 = 0 and ρ3 = 2kT0 /e. For T0 = 45 K, ρ3 is 0.008 V, which is a fairly small value. Thus, the temperature behavior of the diode is due to the narrowing of the Gaussian distribution of barrier height with bias voltage [557]. Diffusion Theory In diffusion theory the current density is considered in the presence of a carrierdensity and electricﬁeld gradient. In the Boltzmann approximation 9 This phenomenon is similar to the redshift of luminescence lines (Stoke’s shift) due to thermalization in the presence of disorder, cf. Sect. 11.6.
18.2 Metal–Semiconductor Contacts 10 3
T= 293K
Pd/ZnO
210K
10 5
103
10 7
105 106 107
10 8 10
T=293K
104
6 jd (Acm2)
jd (Acm2)
10 4
10
417
3
2 1 0 Voltage (V)
1
9
0.0
0.2
0.4 0.6 Voltage (V)
0.8
(a) 0.8
0.15
0.775
0.2
0.75
0.25
0.725
0.3
0.7
0.4
0.65
0.45
0.625
0.5 3.5
4.0 4.5 1/T (1000/K)
0.55 3.0
5.0
(c)
n
1.8 1.6 1.4 1.2 200
0.35
0.675
0.6 3.0
(b)
1/n1
#B,eff (eV)
2.0
3.5
250 T (K)
4.0 4.5 1/T (1000/K)
5.0
Fig. 18.12. (a) Forward I–V characteristic of Pd/ZnO Schottky diodes for various temperatures. Diode temperatures are 210 K, 220 K, 230 K, 240 K, 250 K, 260 K, 270 K, and 293 K. The inset shows the current density vs. voltage for 293 K on a semilogarithmic scale. (b) Eﬀective barrier height φjBn vs. the inverse temperature. The solid line is a linear ﬁt according to (18.37) yielding the standard deviation σφ = 0.13 V and the mean barrier height φ¯Bn = 1.1 eV. (c) Plot of 1/n − 1 vs. the inverse temperature. The solid line is a linear ﬁt of the data yielding the voltage deformation coeﬃcients ρ2 = −0.025 and ρ3 = −0.028 V. The inset shows the experimentally determined n factors and the n factors calculated from (18.39) using the voltagedeformation coeﬃcients obtained from the linear ﬁt (dashed line)
the electron current is given by (8.46a). In stationary equilibrium the current density is constant, i.e. independent of x. Assuming that the carrier density has its equilibrium values at x = 0 and x = w, we ﬁnd after integration and using (18.6)
eV eφBn j = −eμn NC Em exp exp −1 (18.40) kT kT
eV = js exp −1 . kT
418
18 Diodes
40 Au/ GaAs
V0 (meV)
30 k V0= e (T+T0) 20 10 0 0
(a)
(b)
k V0= e T
10 20 kT/q (meV)
30
Fig. 18.13. (a) Forward I–V characteristic of Au/GaAs diode for various temperatures. (b) Temperature dependence of the voltage V0 . The experimental data are ﬁtted with T0 = 45 ±8 K. Adapted from [560]
Therefore, also in this case the ideal diode characteristic is obtained, however, with a different saturation current. The ideality factor in diffusion theory is n = 1.06 (for −eφBn 15 kT ) [547]. Combined Theory A combination of both theories [563] considers both mechanisms to be in series. The current can then be expressed as
eφBn eV eNC vr j= exp exp −1 (18.41a) 1 + vr /vD kT kT
eV = A∗∗ T 2 exp −1 (18.41b) kT
eV −1 . = js exp kT Here vr = v¯/4 is a ‘recombination velocity’ [562] at the top of the barrier according to j = vr (n − n0 ), n0 being the equilibrium electron density at the top of the barrier and v¯ is the average thermal velocity in the semiconductor.
18.2 Metal–Semiconductor Contacts
419
vD is an effective diffusion velocity describing the transport of electrons from the edge of the depletion layer (x = w) to the top of the barrier (x = xm ). It is deﬁned as
−1 w −e −eφBn − EC (x) vD = exp − dx . (18.42) kT xm μn kT In [563] μn has been assumed to be independent of the electric ﬁeld. This assumption is potentially not realistic. If vD ≫ vr , thermionic theory applies and we obtain (18.32). The case vr ≫ vD ∼ μn Em relates to diffusion theory and we recover (18.40). The constant A∗∗ in (18.41b) is called the effective Richardson constant. Its calculated dependence on the electric ﬁeld is shown in Fig. 18.14 for Si. At room temperature for most Ge, Si and GaAs Schottky diodes the thermionic emission of majority carriers is the dominating process.
Fig. 18.14. Calculated eﬀective Richardson constant A∗∗ as a function of the electric ﬁeld for a metal–Si diode at T = 300 K for a (ntype, upper curve or ptype, lower curve) doping of 1016 cm−3 . Adapted from [564]
Tunneling Current At high doping the width of the depletion layer becomes small and tunneling processes become more probable. Also at low temperatures, when thermionic emission is very small, tunneling processes can dominate the transport between metal and semiconductor. One process is tunneling of electrons close to the Fermi level of the semiconductor. This process is called ﬁeld emission (F)
420
18 Diodes
and is at least important for degenerate semiconductors at very low temperatures. If the temperature is raised, electrons are excited to higher energies where they encounter a thinner barrier. The tradeoff between thermal energy and barrier width selects an electron energy Em above the conductionband edge for which the current is largest. This process is known as thermionic ﬁeld emission (TF). For very high temperatures enough carriers can overcome the barrier completely and we are back in the thermionic emission regime. The validity of the two regimes is shown in Fig. 18.15 for Au/GaAs Schottky diodes as a function of doping concentration (ntype) and temperature. 12
kT (meV)
10
Au/GaAs
8 6
TF emission
4 2 0 15 10
F emission 10
16
17
10 ND (cm3)
10
18
Fig. 18.15. Calculated conditions for thermionic ﬁeld (‘TF’) and ﬁeld (‘F’) emission in a Au/GaAs Schottky diode as a function of temperature and doping concentration. Adapted from [547]
In the ﬁeldemission regime the forward current is given by
eV j = js exp , E00 with the characteristic energy parameter E00 given by
1/2 e ND E00 = . 2 m∗ ǫs
(18.43)
(18.44)
The saturation current is js ∝ exp (eφBn /E00 ). In Fig. 18.16, the forward characteristic of a highly doped Au/Si is shown. The experimental value of E00 = 29 meV agrees well with the theoretical expectation of E00 = 29.5 meV. In the reverse direction the I–V characteristic under ﬁeld emission is given by
2(−φBn )3/2 4eπm∗ 2 Vbi − V exp − E00 . (18.45) j= h3 φBn 3E00 e(Vbi − V )1/2 From Fig. 18.16b, a barrier height of 0.79 eV is deduced.
18.2 Metal–Semiconductor Contacts 10
421
3
104
106
103 E00=29 meV
7
10
8
10
9
10
4
j VbiV
10
10
(a)
5
105
log10
Current (A)
10
10
Au/Si ND=81018 cm3
6
107 10
8
10
9
10
0
0.2 0.4 0.6 Voltage (V)
0
(b)
0.5
1.0
1.5
(VbiV)1/2 (eV1/2)
Fig. 18.16. (a) Forward and (b) reverse I–V characteristic of a Au/Si Schottky diode at 77 K. The doping concentration of the Si was ND = 8×1018 cm−3 . Adapted from [547]
In the TFemission regime the current–voltage characteristic is given by
eV j = js exp , (18.46) E0 with E0 = E00 coth(E00 /kT ) ,
(18.47)
where E00 is given by (18.44). The energy for maximum TF emission Em is given by Em = e(Vbi − V )/ cosh2 (E00 /kT ). The coth dependence of E0 is shown in Fig. 18.17 for an Au/GaAs diode. A Schottky diode can suffer from nonideality such as series and parallel ohmic resistance [559]. These effects are discussed in some detail below for pndiodes in Sect. 18.4.4 and apply similarly to Schottky diodes. 18.2.6 Ohmic Contacts Although an ohmic contact does not have a diode characteristic, it can be understood from the previous remarks. An ohmic contact will have a small contact resistance for both current directions. The voltage drop across the
422
18 Diodes
40
E0 (meV)
30 20 E00 10 0
0
10
20 30 kT/e (meV)
40
Fig. 18.17. Temperature dependence of E0 of an Au/GaAs diode with ND = 5 × 1017 cm−3 . The solid line is the theoretical dependence for thermionic emission according to (18.47) with ND = 6.5×1017 cm−3 and m∗ = 0.07. Adapted from [547]
contact will be small compared to the voltage drop in the active layer (somewhere else). The contact resistance Rc is deﬁned as the differential resistance at V = 0
−1 ∂I . (18.48) Rc = ∂V V =0 At low doping, the transport is dominated by thermionic emission (18.32). In this case Rc is given by
eφBn k exp − . (18.49) Rc = eA∗ T kT A small barrier height will lead to small contact resistance. For high doping Rc is determined by the tunneling current and is proportional to
eφBn Rc ∝ exp − . (18.50) E00 The contact resistance decreases exponentially with the doping. A theoretical calculation and experimental data are compared in Fig. 18.18 for contacts on Si. The two mechanisms, low barrier height and high doping, for the formation of Ohmic contacts are summarized schematically in Fig. 18.19. Ohmic contacts on widebandgap semiconductors are diﬃcult, since metals with suﬃciently small work function are mostly not available.
18.2 Metal–Semiconductor Contacts
423
3
10 106
20
10
ND (cm )
19
10
18
10
17
Pt/Si Al/Si
104
Rc ( cm2)
B=0.85V 102 0.60V
100 102
0.40V
104 10
6
5
0 ND
1/ 2
(10
10
10 3/ 2 cm )
30
Fig. 18.18. Theoretical and experimental values of speciﬁc contact resistances at T = 300 K for Al/nSi [565] and PtSi/nSi [566] contacts as a function of donor concentration. Solid lines are theoretical dependencies for diﬀerent values of the barrier height as labeled. Adapted from [183]
q B q B
EC
EC
EF
EV
(a)
EF
EV
(b)
Fig. 18.19. Schematic conditions for the formation of an Ohmic contact, (a) low barrier height and (b) high doping (thin depletion layer)
Ohmic contacts are typically prepared by evaporating a contact metal containing the doping material for the semiconductor, e.g. Au/Zn for a contact on ptype GaAs [567] and Au/Ge for a contact [568] on ntype GaAs. The contact is alloyed around 400–500 ◦ C (see Fig. 18.20) above the eutectic temperature of Teu = 360 ◦ C (for Au/Ge) to form a eutectic liquid in which the dopant can quickly diffuse. When the eutectic liquid cools it forms a solid,
424
18 Diodes
a highly doped semiconductor layer underneath the metal. The liquidphase reactions can lead to inhomogeneous contacts. On ntype GaAs Pd/Ge/Au contacts have been reported to have superior structural quality [569]. Ohmic contacts for a number of different semiconductors are reviewed in [570, 571].
Fig. 18.20. Speciﬁc contact resistance for Ni/AuGe on ntype epitaxial GaAs for varying alloying temperatures (2 min). Arrow at Teu denotes the eutectic temperature of AuGe. Adapted from [572]
18.2.7 Metal Contacts to Organic Semiconductors Also, for organic semiconductors the metal contact plays a vital role, either for carrier injection or for manipulation of the spacecharge region. The position of the Fermi level has been determined for various organic semiconductors as shown in Fig. 18.21. These data have been obtained from measurements on metal–semiconductor–metal structures (MSM, see also Sect. 19.3.5) as shown in Fig. 18.22a. The thin (50 nm) organic layer is fully depleted, thus the builtin ﬁeld inside the semiconductor is constant. The builtin ﬁeld is measured by applying an external dc bias and ﬁnding the external potential at which the electroabsorption signal vanishes. Figure 18.22b shows the measured electroabsorption signal ΔT /T (relative change of transmission T ) and the optical density of an MEHPPV ﬁlm as a function of photon energy for an Al/MEHPPV/Al structure. The exciton absorption peak is found at 2.25 eV. The bias at which the builtin ﬁeld vanishes can then be determined for var
18.3 Metal–Insulator–Semiconductor Diodes
425
ious other metals in metal/MEHPPV/Al structures. Figure 18.21 summarizes such results for various metals and three organic semiconductors. The plot of the Fermi level position vs. the metal work function (Figs. 18.22d,e) shows that the metals investigated do not introduce interface states in the singleparticle gap that pin the Schottky barrier (cf. Fig. 18.5 for inorganic semiconductors). An electron trap, such as C60 in MEHPPV, can pin the Fermi level of the ncontact metal and leads to a change of the builtin potential [575]. vacuum level Wm
Pentacene EC 2.4
Ca 2.9
(a)
Al 4.3 Au 4.8 Pt 5.3
EF 3.0 Ca
EV 4.9
4.3 Al 4.8 Au,Pt
vacuum level Wm Sm Ca Mg Al Cu Au Pt
2.7 2.9 3.7 4.3 4.6 4.8 5.3
Alq3
EF
EC 3.0 3.6 4.0 4.6 5.2 5.6
Sm,Ca,Mg Al Cu Au Pt
EV 6.0
(b) vacuum level Wm Sm 2.7 Ca 2.9
(c)
Al,Ag Cu Au Pt
4.3 4.6 4.8 5.3
MEHPPV EC 2.90
EV 5.30
EF 3.0 Sm,Ca 4.3 4.6 5.1 5.2
Al,Ag Cu Au Pt
Fig. 18.21. Measured Fermi energies EF (labeled data in eV) and the work functions Wm of various metals contacting (a) pentacene, (b) Alq3 and (c) MEHPPV. EC (EV ) denotes the energy position of the electron (hole) polaron. Measured data for EF for MEHPPV from [573], other from [574]. Data for Wm from Table 18.1
18.3 Metal–Insulator–Semiconductor Diodes In a metal–insulator–semiconductor (MIS) diode an insulator is sandwiched between the metal and the semiconductor. Subsequently, a MIS contact has
426
18 Diodes metal 2 organic sc. metal 1 glass
(a) 3
1.0
T/T (103) (arb. units)
0.4 0.3
1 0
0.2
1 2
0.1
DC bias
3
(b)
2.2 2.4 Energy (eV)
EF (eV)
0.0
AlAl AuAl
0.0 1.0 Wm (eV)
1.0 0.0 1.0 Bias voltage (V)
2.0
0.0
1.0
Al Cu
2.0
Au
1.0
SmAl 0.5
(c)
Al
1.0
CaAl
0.0 2.0
Ca Sm
1.0
(d)
0.0
2.6
EF (eV)
2.0
Optical density
T/T (103)
2
3.0 (e)
Ag
Pt Au
2.0 1.0 Wm (eV)
0.0
Fig. 18.22. (a) Schematic MSM structure with organic semiconductor (sc.) on transparent glass substrate. Metal 1 is thin and semitransparent. Thickness of organic semiconductor (polymer or small molecules) is about 50 nm. (b) Electroabsorption spectra of Al/MEHPPV/Al structure at four dc bias voltages (solid lines) and optical density spectrum (dashed line). (c) Magnitude of the electroabsorption response at 2.1 eV as a function of bias for metal/MEHPPV/Al structures. (d,e) Calculated (solid lines) and experimental (points) potential diﬀerence across (d) metal/MEHPPV/Al structures and (e) metal/MEHPPV/Ca structures as a function of the workfunction diﬀerence of the contacts. Parts (b)–(e) adapted from [573]
zero dc conductance. The semiconductor typically has an ohmic back contact. As insulator, often the oxide of the respective semiconductor, is used. In particular SiO2 on Si has been technologically advanced (Fig. 18.23). In the latter case, the diode is called a MOS (metal–oxide–semiconductor) diode. This structure has great importance for the investigation of semiconductor surfaces and overwhelming importance for semiconductor technology (planar integration of electronic circuits, CMOS technology). Also, CCDs (Sect. 19.3.8) are based on MIS diodes.
18.3 Metal–Insulator–Semiconductor Diodes
427
polySi gate oxide Si
Fig. 18.23. Highresolution transmission electron microscopy image of a 1.6nm thick gate oxide between polySi (see Sect. 21.5.4) and crystalline Si. From [576]
18.3.1 Band Diagram for Ideal MIS Diode An ideal MIS diode has to fulﬁll the following three conditions: (i) (as shown in Fig. 18.24) without external bias the energy difference φms between the work function of the metal and the semiconductor
Eg φms = φm − χs − ± ΨB (18.51) 2e is zero (φms = 0). The ‘+’ (‘−’) sign in (18.51) applies to a ptype, Fig. 18.24b (ntype, Fig. 18.24a) semiconductor. ΨB is the difference between the intrinsic and actual Fermi level, ΨB = Ei − EF /e > 0. (ii) The only charges present are those in the semiconductor and the opposite charge is on the metal surface close to the insulator. (iii) There is no dc current between the metal and the semiconductor, i.e. the conductivity of the insulator is zero. When an ideal MIS diode is biased, three general cases – accumulation, depletion and inversion – can occur (Fig. 18.25). We discuss these ﬁrst for the ptype semiconductor. Figure 18.25a shows the accumulation case for a negative voltage at the metal.10 Part of the voltage drops across the insulator, the rest across the semiconductor. The valence band is bent upwards towards the Fermi level. The quasiFermi level in the semiconductor, however, is constant since no dc current ﬂows.11 10
This poling is a forward bias of the respective Schottky diode since the positive pole is at the ptype semiconductor. 11 We note that in order to reach the situations shown in Fig. 18.25 from the zero bias case of Fig. 18.24, a current must have ﬂowed since charge carriers are
428
18 Diodes Evac
metal
i
nsemiconductor
Evac
Evac
metal
i
psemiconductor
Evac
esc Wm=
e m
Wm=
e m
esc
e B
EF
e$B
EC EF
EC
e B
e$B
EF
Ei EF EV
Ei EV
(a)
d
(b)
d
Fig. 18.24. Band diagram of an ideal MIS diode with (a) n and (b) ptype semiconductor at external bias V = 0. The insulator (‘i’) thickness is d as labeled. The dashdotted line represents the intrinsic Fermi level Ei
Since the chargecarrier (hole) density depends exponentially on the energy separation EF − EV , a charge accumulation (of holes) occurs in the semiconductor in the vicinity of the interface to the insulator. In Fig. 18.25b the depletion case is shown. Now a moderate reverse voltage, i.e. a positive bias to the metal, is applied. A depletion of majority charge carriers occurs in the semiconductor close to the insulator. The quasiFermi level in the semiconductor remains beneath the intrinsic level (Ei ≈ EC + Eg /2), i.e. the semiconductor remains ptype everywhere. If the voltage is increased further to large values, the quasiFermi level intersects the intrinsic level and lies above Ei close to the insulator. In this region, the electron concentration becomes larger than the hole concentration and we have the inversion case. The inversion is called ‘weak’ if the Fermi level is still close to Ei . The inversion is called ‘strong’ when the Fermi level lies close to the conductionband edge. The corresponding phenomena occur for ntype semiconductors for the opposite signs of the voltage with electron accumulation and depletion. In the inversion case, p > n close to the insulator. 18.3.2 SpaceCharge Region Now we calculate the charge and electric ﬁeld distribution in an ideal MIS diode, following the treatment in [577]. We introduce the potential Ψ that measures the separation of the intrinsic bulk Fermi level and the actual intrinsic level Ei , i.e. −eΨ (x) = Ei (x) − Ei (x → ∞) (see Fig. 18.26). Its value redistributed. Figure 18.25 depicts the stationary equilibrium after transient voltage switchon eﬀects have subsided. The time, however, that is needed in order to reach the stationary equilibrium from zero bias (thermal equilibrium) may be very long (days, see Sect. 19.3.8).
18.3 Metal–Insulator–Semiconductor Diodes metal
i
nsemiconductor
metal
i
429
psemiconductor
EC
V0
Ei
Ei EF EV
EV
(a)
(d)
EC V>0
EC EF V0
EC EF Ei
V 0 and inversion (as shown here) for Ψs > ΨB > 0
at the surface is termed Ψs , the surface potential. The value is positive, i.e. Ψs > 0, if the intrinsic Fermi level at the surface is below the bulk Fermi level. The electron and hole concentrations are given (for a ptype semiconductor) as np = np0 exp(βΨ ) pp = pp0 exp(−βΨ ) ,
(18.52a) (18.52b)
where np0 (pp0 ) are the bulk electron (hole) concentrations, respectively, and β = e/kT > 0. Therefore, the net free charge is given by np − pp = np0 exp(βΨ ) − pp0 exp(−βΨ ) .
(18.53)
The electron and hole concentrations at the surface are denoted with an index ‘s’ and are given by12 ns = np0 exp(βΨs )
(18.54a)
ps = pp0 exp(−βΨs ) .
(18.54b)
We use the Poisson equation
d2 Ψ dx2
= − ǫρs with the charge given by
ρ(x) = e p(x) − n(x) + ND+ (x) − NA− (x) .
(18.55)
As boundary condition we employ that far away from the surface (for x → ∞) there is charge neutrality (cf. (7.47)), i.e. 12
Ψs represents the voltage drop across the semiconductor that will be discussed in more detail in Sect. 18.3.3. In this sense, Ψs for the MIS diode is related to Vbi −V for the Schottky contact.
18.3 Metal–Insulator–Semiconductor Diodes
np0 − pp0 = ND+ − NA− ,
431
(18.56)
and that Ψ = 0. We note that ND+ − NA− must be constant throughout the completely ionized, homogeneous semiconductor. Therefore (18.56) (but not charge neutrality) holds everywhere in the semiconductor. Using (18.53) the Poisson equation reads e ∂2Ψ = − {pp0 [exp(−βΨ ) − 1] − np0 [exp(βΨ ) − 1]} . ∂x2 ǫs
(18.57)
The Poisson equation is integrated and with the notations 1/2 np F(Ψ ) = (exp(−βΨ ) + βΨ − 1) + 0 (exp(βΨ ) − βΨ − 1) (18.58a) pp 0 1/2 1/2 ǫs ǫs kT LD = 2 = , (18.58b) e pp0 eβpp0 with LD being the Debye length for holes, the electric ﬁeld can be written as √ ∂Ψ 2kT E =− =± F(Ψ ) . (18.59) ∂x eLD The positive (negative) sign is for Ψ > 0 (Ψ < 0), respectively. At the surface, Ψs will be taken as the value for Ψ . The total charge Qs per unit area creating the surface ﬁeld √ 2kT ∂Ψ =± F(Ψs ) (18.60) Es = − ∂x eLD is given by Gauss’s law as Qs = −ǫs Es . The dependence of the spacecharge density from the surface potential13 is depicted in Fig. 18.27. If Ψs is negative, F is dominated by the ﬁrst term in (18.58a) and the space charge is positive (accumulation) and proportional to Qs ∝ exp(−βΨ /2). For Ψs = 0 the (ideal) MIS diode has the ﬂatband condition and the space charge is zero. For 0 ≤ Ψs ≤ ΨB the space charge is negative √ (depletion) and F is dominated by the second term in (18.58a), i.e. Ψs ∝ Ψs . For Ψs ≫ ΨB we are in the (weak) inversion regime and the space charge is dominated by the fourth term in (18.58a), Qs ∝ − exp(−βΨ/2). Strong inversion starts at about Ψsinv ≈ 2ΨB = 2kT ln(NA /ni )/e. For the case of strong inversion the band diagram is shown in Fig. 18.28 together with the charge, ﬁeld and potential. The total voltage drop V across the MIS diode is V = Vi + Ψs , 13
(18.61)
We note that we discuss the spacecharge region now only with regard to Ψs , the voltage drop across the semiconductor, and the dependence of Ψs on the bias of the diode will be discussed in the next section.
432
18 Diodes 104
Qs (C/cm2)
105
10
accumulation
weak inversion
depletion
strong inversion
⬀exp(eΨs /2kT)
⬀exp(eΨs /2kT)
6
2ΨB
10
10
Qs0
1/2
⬀Ψs
8
Ei
EV
EC
9
10 0.4 0.2 0.0
0.2
0.4
0.6
0.8
1.0
Ψs (eV)
Fig. 18.27. Dependence of the space charge on the surface potential Ψs for ptype silicon with NA = 4 × 1015 cm−3 at T = 300 K. The ﬂatband condition is present for Ψs = 0
with Vi being the voltage drop across the insulator. In the case of inversion, the charge (per unit area) in the spacecharge region Qs = Qd + Qn
(18.62)
is composed of the depletion charge (ionized acceptors) Qd = −ewNA ,
(18.63)
with w being the width of the depletion region, and the inversion charge Qn , which is present only close to the interface. The metal surface carries the opposite charge Qm = −Qs
(18.64)
due to global charge neutrality. The insulator itself does not contribute charges in the case of an ideal MIS diode. 18.3.3 Capacity The insulator represents a capacitor with the dielectric constant ǫi and a thickness d. Therefore, the capacity is Ci =
ǫi . d
(18.65)
18.3 Metal–Insulator–Semiconductor Diodes
433
semiconductor
metal insulator Vi
EC
eS
eB
V>0
(a)
inversion region Qm
depletion region
neutral region
(x)
0
(b)
Ei EF EV
w
d
x
eNA Qn
Qm/i
(c)
x d
0
w
(x) V Vi s
(d)
x d
0
w
Fig. 18.28. Ideal MIS diode at inversion: (a) band diagram, (b) charge distribution, (c) electric ﬁeld and (d) potential
Between the charges −Qs and Qs the ﬁeld strength Ei in the insulator is Ei =
Qs  . ǫi
(18.66)
The voltage drop Vi across the insulator is given by Vi = Ei d =
Qs  . Ci
(18.67)
The total capacity C of the MIS diode is given by the insulator capacitance in series with the capacitance Cd of the depletion layer C=
Ci Cd . Ci + Cd
(18.68)
434
18 Diodes
The capacity of the spacecharge region varies with the applied bias (Fig. 18.29). For forward bias (accumulation), the capacity of the spacecharge region is high. Therefore, the total capacity of the MIS diode is given by the insulator capacitance C ≈ Ci . When the voltage is reduced, the capacity of the spacecharge region drops to Cd = ǫs /LD for the ﬂatband case (Ψs = 0). For a high reverse voltage, the semiconductor is inverted at the surface and the spacecharge region capacity is high again. In this case, the total capacity is given by C ≈ Ci again. Ci
Ci s=0 CFB flat band capacitance
C/Ci
0.8
1.0
2
s=B
0.4
Cmin Cmin '
0.6
0.6 0.4
(iii)
(a)
0 Vmin VT Bias voltage
10 0 10 Bias voltage (V)
Cmin '
0.2 VT
breakdown
V
10 Hz 5 10 Hz
(ii)
0.2 0
103Hz 4
0.8 s=2B
10 Hz
0.8
20
0.6
10Hz
1.0
Ci
(i)
C/Ci
1.0
0
+V
(b)
4
2
0 2 Bias voltage (V)
4
Fig. 18.29. (a) Schematic dependence of the capacity of a MIS diode on the bias for (i) low frequencies, (ii) high frequencies and (iii) deep depletion. (b) Highfrequency capacity of a Si/SiO2 diode (NA = 1.45 × 1016 cm−3 , d = 200 ν). The inset shows the frequency dependence for various frequencies as labeled. Adapted from [578]
The previous consideration assumes that the charge density in the semiconductor can follow changes of the bias suﬃciently fast.14 The inversion charge must disappear via recombination that is limited by the recombination time constant τ . For frequencies around τ −1 or faster, the charge in the inversion layer cannot follow and the capacitance of the semiconductor is given by the value Cd ∼ = ǫs /wm . wm (Fig. 18.30) is the maximum depletionlayer width present at the beginning of inversion (cf. (18.8))
1/2
1/2 4ǫs kT ln(NA /ni ) 2ǫs inv . (18.69) Ψs = wm ∼ = eNA e2 NA For further increased voltage (into the inversion regime), the electric ﬁeld is screened by the inversion charge and the width of the depletion layer remains constant. Therefore, the total capacity in the inversion regime is given by ǫi C∼ . (18.70) = d + ǫǫsi wm 14 Typically, a dc bias voltage V is set and the capacity is sampled with a small ac voltage of amplitude ΔV , with δV ≪ V
18.4 Bipolar Diodes
435
101
wm (μm)
GaAs 100
10
Si Ge
1
2
10 14 10
1015
1016 NB (cm3)
1017
1018
Fig. 18.30. Maximum width of the depletion layer wm (18.69) at room temperature for deep depletion for GaAs, Si and Ge diodes as a function of bulk doping level
18.3.4 Nonideal MIS Diode In a real, i.e. nonideal, MIS diode, the difference φms in the work functions of the metal and semiconductor (cf. (18.51)) is no longer zero. Therefore, the capacitance vs. voltage relation is shifted with respect to the ideal MIS diode characteristic by the ﬂatband voltage shift VFB VFB = φms −
Qox . Ci
(18.71)
Additionally, the ﬂatband voltage can be shifted by charges Qox in the oxide that have been neglected so far. Such charges can be trapped, i.e. ﬁxed with regard to their spatial position, or mobile, e.g. ionic charges such as sodium. For Al as metal (φm = 4.1 eV) and ntype Si (φs = 4.35 eV), the ﬂatband voltage shift is φms = −0.25 V, as shown schematically in Fig. 18.31a for zero bias. VFB is split into 0.2 eV and 0.05 eV for the oxide and the silicon, respectively. In Fig. 18.31b, the dependence of φms on the doping, conductivity type and metal is shown for various SiO2 –Si MIS diodes. An AuSiO2 –Si diode with ptype Si and NA ≈ 1015 cm−3 fulﬁlls the condition of an ideal MIS diode with regard to φms = 0.
18.4 Bipolar Diodes A large class of diodes is based on pnjunctions. In a homo pnjunction an ndoped region is next to a pdoped region of the same semiconductor. Such
436
18 Diodes
Al
SiO2
nSi Evac
0.2eV
1.0
EC
i
Au/nS
0.6
p + po
0.4
ms (V)
0.05eV
4.1eV 3.2eV
5.25eV
0.8
EC EF
i/nSi
+ S p poly
0.2 0
i
Al/nSi
9.0eV
0.4
i/nSi
+ S n poly
0.6
EV
1.0
Al/pSi n + po lySi/
10 (a)
(b)
pSi
Au/pS
0.2
0.8
lySi/
14
10
pSi
15
1016 1017 1018 3 NB (cm )
Fig. 18.31. (a) Schematic band diagram of an Al–SiO2 –Si (ntype) diode with 50 nm oxide thickness and ND = 1016 cm−3 for zero bias. Based on data from [579]. (b) Diﬀerence of work functions φms for SiO2 –Si MIS diodes and various doping levels and electrode materials (Al, Au and polycrystalline Si). The square represents the situation of part (a). Based on data from [580]
a device is called bipolar. At the junction a depletion region forms. The transport properties are determined by the minority carriers. An important variation is the pindiode in which an intrinsic (or lowly doped) region is between the doped region (Sect. 18.5.8). If the differently doped regions belong to different semiconductor materials, the diode is a heterostructure pndiode (Sect. 18.5.11). 18.4.1 Band Diagram If the doping proﬁle is arbitrarily sharp, the junction is called abrupt. This geometry is the case for epitaxial pnjunctions where the differently doped layers are grown on top of each other.15 For junctions that are fabricated by diffusion, the abrupt approximation is suitable for alloyed, ionimplanted 15 The choices of dopant and the growth conditions, in particular the temperature, need to be made such that no interdiﬀusion of the dopants takes place.
18.4 Bipolar Diodes
437
Fig. 18.32. Schematic fabrication technologies for bipolar diodes: (a) Planar junction with local impurity incorporation (diﬀusion from gas phase or ion implantation) through mask and contact metallization, (b) epitaxial junction NAND
xp
(a)
xn
x
xp
NAND
xn
(b)
x
w/2
x
w/2
(c)
NB
w/2 w/2
x
(d)
Fig. 18.33. Description of doping distribution with (a,b) abrupt approximation and with (c,d) linearly graded junction. (a,c) show real impurity concentration, (b,d) idealized doping proﬁle
and shallowdiffused junctions. For deepdiffused junctions a linearly graded approximation is better, which is treated in more detail in [183]. If one doping level is much higher that the other, the junction is termed a onesided (abrupt) junction. If n ≫ p (p ≫ n), the junction is denoted as an n+ pdiode (p+ ndiode). 18.4.2 SpaceCharge Region We ﬁrst consider the pndiode in thermodynamical equilibrium, i.e. without external bias. No net current ﬂows in this case. The electron current is given by (8.42a) jn = −eμn nE − μn n∇EF ,
(18.72)
438
18 Diodes
and therefore in the absence of electrical ﬁelds and zero net electron and hole currents the Fermi energy is constant: ∇EF = 0 .
(18.73)
The builtin voltage Vbi is given by (see Fig. 18.34d) eVbi = Eg + eVn + eVp ,
(18.74)
where Vn is the difference between conduction band and Fermi level on the nside, −eVn = EC −EF . Vp is the difference between valence band and Fermi level on the pside, −eVp = EF − EV . For the nondegenerate semiconductor Vn , Vp < 0 and (using (7.17), (7.15) and (7.16))
NC NV NC NV eVbi = kT ln − kT ln + kT ln n2i nn0 pp 0
pp0 nn0 pp0 n n0 (18.75a) = kT ln = kT ln = kT ln n2i pn0 n p0
NA ND ∼ . (18.75b) = kT ln n2i The electron and hole densities on either side of the junction (np0 and pp0 at x = −xp and nn0 and pn0 at x = xn ) are related to each other by (from rewriting (18.75a))
eVbi np0 = nn0 exp − (18.76a) kT
eVbi pn0 = pp0 exp − . (18.76b) kT Microscopically, the equilibration of the Fermi levels on the n and pside occurs via the diffusion of electrons and holes to the p and nside, respectively. The electrons and holes recombine in the depletion layer. Therefore, on the nside the ionized donors and on the pside the ionized acceptors remain (Fig. 18.34a). These charges build up an electrical ﬁeld that works against the diffusion current (Fig. 18.34d). At thermal equilibrium the diffusion and drift currents cancel and the Fermi level is constant. Values for the builtin potential are depicted in Fig. 18.35 for Si and GaAs diodes. The spatial dependence of the potential in the depletion layer is determined by the Poisson equation. We assume here the complete ionization of the donors and acceptors. Also, we neglect at ﬁrst majority carriers in the depletion layers on the n and psides.16 With these approximations, the Poisson equation in the depletion layers on the n and pside reads 16 An abrupt decrease of the majority carrier density at the border of the spacecharge region corresponds to zero temperature.
18.4 Bipolar Diodes
Potential (V)
p 1.0
NA
ND
n
0.5
Vbi
0.0 (c)
Energy (eV)
eVbi
0.5 0.0
EF
E (105 V/cm)
EC
0.5
EV
1.0
3 n,pp (cm n, (cm)3)
(a)
(b)
Si
1.0
(d)
0.0 1.0 2.0 3.0 4.0
1019 1016 1013 10
10 107
(e)
n
p
ni
104 10191 10 n+p (cm3) n+p (cm3)
439
(f)
1017 1015 1013 1011 109
ni 40
20
0 x(nm)
20
40
Fig. 18.34. (Symmetric) pnjunction (abrupt approximation) in thermal equilibrium (zero bias) for Si at room temperature and NA = ND = 1018 cm−3 . (a) Schematic representation of pdoped and ndoped region with depletion layer (grey area) and ﬁxed space charges, (b) diﬀusion potential, (c) band diagram with Fermi level (dashed line), (d) electric ﬁeld, (e) freecarrier concentrations n and p and (f ) total freecarrier density n + p
440
18 Diodes
Fig. 18.35. Builtin voltage as a function of doping for onesided Si and GaAs pndiodes
eND ∂2V = , 0 ≤ x ≤ xn 2 ∂x ǫs ∂2V eNA , −xp ≤ x ≤ 0 . =− 2 ∂x ǫs
(18.77a) (18.77b)
One integration yields (together with the boundary conditions that the ﬁeld is zero at the boundaries of the depletion layer) the electrical ﬁeld in the two regions e ND (x − xn ), 0 ≤ x ≤ xn ǫs e E(x) = − NA (x + xp ), −xp ≤ x ≤ 0 . ǫs E(x) =
(18.78a) (18.78b)
The maximum ﬁeld strength Em is present at x = 0 and is given by Em = −
eND xn eNA xp =− . ǫs ǫs
(18.79)
The continuity of the ﬁeld at x = 0 is equivalent to the overall charge neutrality ND xn = NA xp . Another integration yields the potential (setting V (x = 0) = 0)
x2 , 0 ≤ x ≤ xn V (x) = −Em x − 2xn
x2 V (x) = −Em x + , −xp ≤ x ≤ 0 . 2xp
(18.80)
(18.81a) (18.81b)
18.4 Bipolar Diodes
441
The builtin potential Vbi = V (xn ) − V (−xp ) > 0 is related to the maximum ﬁeld via 1 (18.82) Vbi = − Em w , 2 where w = xn + xp is the total width of the depletion layer. The elimination of Em from (18.79) and (18.82) yields
1/2 2ǫs NA + ND Vbi w= . (18.83) e NA ND For p+ n and n+ p junctions, the width of the depletion layer is determined by the lowly doped side of the junction 1/2 2ǫs w= , (18.84) Vbi eNB where NB denotes the doping of the lowly doped side, i.e. NA for a n+ p diode and ND for a p+ n diode. If the spatial variation of the majority carrier density is considered in more detail (and for ﬁnite temperature, cf. (18.11)), an additional term −2kT /e = −2/β is added [577] to Vbi
1/2
2ǫs NA + ND 2kT w= . (18.85) Vbi − V − e NA ND e Also, the external bias V has been included in the formula. If w0 denotes the depletion layer width at zero bias, the depletion layer width for a given voltage V can be written as 1/2 1/2 V V w(V ) = w0 1 − . (18.86) ≈ w0 1 − Vbi − 2/β Vbi Using the Debye length (cf. (18.58b))
1/2 ǫs kT LD = , e2 NB
(18.87)
the depletion layer width for a onesided diode can be written as (with β = e/kT ) (18.88) w = LD 2(βVbi − βV − 2) .
The Debye length is a function of the doping level and is shown for Si in Fig. 18.36. For a doping level of 1016 cm−3 the Debye length in Si is 40 nm at room temperature. For onesided junctions the depletion layer width is about 6 LD for Ge, 8 LD for Si and 10 LD for GaAs. The external bias is counted positive if the ‘+’ (‘−’) pole is at the pside (nside). The reverse voltage has opposite polarity. If a reverse bias is applied, the depletion layer width is increased (Fig. 18.37).
442
18 Diodes
Fig. 18.36. Debye length in Si at room temperature as a function of the doping level NB according to (18.87) 2
10
Depletion layer width (μm)
100V 10
1
10
0
102 13 10
Si 103
10V 1V
101
104
105
0.1V
10
14
2
15
10 10 3 NB (cm )
C (pF/cm2)
10
16
10
17
6 10 18 10
Fig. 18.37. Width of the depletion layer and capacitance per area for onesided, abrupt Si junctions for various values of Vbi − V − 2kT /e as labeled. The dashdotted line is for zero bias, the dashed line is the limit due to avalanche breakdown. Adapted from [183]
18.4.3 Capacitance The capacity of the depletion layer is the charge change upon a change of the external bias. It is given as dQ d(eNB w) ǫs ǫs −1/2 = C= = =√ (βVbi − βV − 2) . (18.89) 2 dV d(w eNB /2ǫs ) w 2LD
Therefore, the capacity of the depletion layer is inversely proportional to the depletionlayer width (see the two scales in Fig. 18.37). A detailed treatment
18.4 Bipolar Diodes
443
has been given in [581]. 1/C 2 is proportional to the external bias 1 2L2D = (βVbi − βV − 2) . C2 ǫ2s
(18.90)
From C–V spectroscopy the doping level can be obtained from the slope 2βL2D d(1/C 2 ) 2 = = . dV ǫ2s eǫs NB
(18.91)
From the extrapolation to the voltage for which 1/C 2 = 0 the builtin voltage can be obtained. 18.4.4 Current–Voltage Characteristics Ideal Current–Voltage Characteristics Now, the currents in thermodynamical equilibrium (V = 0) and under bias are discussed. A diode characteristic will be obtained. We work at ﬁrst with the following assumptions: abrupt junction, Boltzmann approximation, low injection, i.e. the injected minoritycarrier density is small compared to the majoritycarrier density, and zero generation current in the depletion layer, i.e. the electron and hole currents are constant throughout the depletion layer. In the presence of a bias, electrons and holes have quasiFermi levels and the carrier densities are given by (cf. (7.57a and b))
Fn − EC n = NC exp (18.92a) kT
Fp − E V . (18.92b) p = NV exp − kT Using the intrinsic carrier concentration, we can write
Fn − E i e(ψ − φn ) n = ni exp = ni exp kT kT
e(φp − ψ) Fp − E i p = ni exp − = ni exp , kT kT
(18.93a) (18.93b)
where φ and ψ are the potentials related to the (quasi) Fermi level and the intrinsic Fermi levels, −eφn,p = Fn,p and −eψ = Ei . The potentials φn and φp can also be written as
n kT ln (18.94a) φn = ψ − e ni
p kT ln φp = ψ + . (18.94b) e pi
444
18 Diodes
The product np is given by np = n2i exp
e(φp − φn ) kT
.
(18.95)
Of course, at thermodynamical equilibrium (zero bias) φp = φn and np = n2i . For forward bias φp − φn > 0 (Fig. 18.38a) and np > n2i . For reverse bias φp − φn < 0 (Fig. 18.38b) and np < n2i .
Fig. 18.38. (a) Diﬀusion potential, (b) band diagram, (c) electric ﬁeld, (d) electron and hole concentrations and (e) n + p under forward bias +0.4 V (left panel ) and reverse bias (right panel ) −0.4 V for a silicon pndiode at room temperature with NA = ND = 1018 cm−3 (same as in Fig. 18.34). The dashed lines in (b) are the electron and hole quasiFermi levels Fn and Fp . The depletion layer is shown as the grey area. The diﬀusion length in the n and ptype material is taken as 4 nm. This value is much smaller than the actual diﬀusion length (µmrange) and is chosen here only to show the carrier concentration in the depletion layer and the neutral region in a single graph
18.4 Bipolar Diodes
p,n
445
p,n pn pn0
pn0
np np0
(a)
x
xp xn jp,jn
(c)
np xp
pn
np0
x
xn
jp,jn jn jn jp
jp (b) xp xn
x
(d) xp
xn
x
Fig. 18.39. Carrier densities (a,c) and current densities (b,d) (linear scales) in a pndiode under (a,b) forward bias and (c,d) reverse bias
The electron current density (per unit area) is given by (8.46a) that reads here with E = ∇ψ and n given by (18.93a) as17
kT ∇n = enμn ∇φn . (18.96) jn = −eμn nE + e Similarly, we obtain for the hole current density (using (8.46b) and (18.93b))
kT ∇p = −epμp ∇φp . jp = eμp pE − (18.97) e The current through the depletion layer is constant (since no recombination/generation was assumed). The gradient of the quasiFermi levels in the depletion layer is very small and the quasiFermi levels φn,p are practically constant. The change of carrier density is mostly due to the variation of ψ (or Ei ). Therefore, the voltage drop across the depletion layer is V = φp − φn and (18.95) reads
eV 2 . (18.98) np = ni exp kT 17
We remind the reader that μn was deﬁned as a negative number.
446
18 Diodes
The electron density at the boundary of the depletion layer on the pside (at x = −xp ) is (using (18.98))
eV eV n2i exp np = = np0 exp . (18.99) pp kT kT Similarly, the hole density on the nside at x = xn is given by
eV pn = pn0 exp . kT
(18.100)
From the continuity equation and the boundary condition that far away from the depletion layer the hole density is pn0 , the hole density on the nside is given by
eV x − xn − 1 exp − pn (x) − pn0 = pn0 exp , (18.101) kT Lp where Lp = Dp τp is the hole (minoritycarrier) diffusion length. The hole current density at the boundary of the depletion layer on the nside is
eV ∂pn eDp pn0 −1 . (18.102) jp (xn ) = −eDp exp = ∂x xn Lp kT Similarly, the electron current in the depletion layer is
eV eDn np0 jn (−xp ) = −1 . exp Ln kT
(18.103)
The total current due to diffusion is
eV jd = jp (xn ) + jn (−xp ) = js exp −1 , kT
(18.104)
with the saturation current given by jsd =
eDp pn0 eDn np0 + . Lp Ln
(18.105)
This dependence is an ideal diode characteristic and the famous result from Shockley. For a onesided (p+ n) diode, the saturation current is eDp pn0 ∼ jsd ∼ =e = Lp
Dp τp
1/2
n2i . NB
(18.106)
The saturation depends via Dp /τp weakly on the temperature. The term n2i depends on T , proportional to T 3 exp(−Eg /kT ), which is dominated by the exponential function.
18.4 Bipolar Diodes
447
If the minority carrier lifetime is given by the radiative recombination (10.19), the hole diffusion length is Lp =
Dp Bnn0
1/2
.
(18.107)
For GaAs (Tables 8.1 and 10.1) with ND = 1018 cm−3 , we ﬁnd τp = 10 ns and Lp ≈ 3 µm. For Ln we ﬁnd 14 µm, however, the lifetime at room temperature can be signiﬁcantly shorter due to nonradiative recombination and subsequently also the diffusion length will be shorter (by about a factor of 10). For L ∼ 1 µm, the diffusion saturation current is jsd ∼ 4 × 10−20 A/cm2 . The radiative recombination rate (band–band recombination, b–b) in the neutral nregion (as relevant for LEDs, see Sect. 20.3) is B(np − n2i ) ≈ b−b in the neuBnn0 (pn (x) − pn0 ). Therefore, the recombination current jd,n tral nregion is (using (18.101))
∞ eV x − xn b−b 2 Bni exp dx jd,n = e − 1 exp − kT Lp xn
eV = eBLp n2i exp −1 . (18.108) kT For the neutral region on the pside a similar expression results. The total radiative recombination current from the neutral regions is
eV b−b 2 −1 . (18.109) jd = eB(Ln + Lp )ni exp kT For GaAs, the saturation current for the radiative recombination in the neutral region jsr,b−b = eB(Ln + Lp )n2i
(18.110)
is (Tables 7.1 and 10.1) for a diffusion length of 1 µm of jsr,b−b ∼ 4 × 10−21 A/cm2 . Since the (radiative) minoritycarrier lifetime is inversely proportional to the majoritycarrier density, the relevant diffusion length is that of the side with the lower doping level and is given by L=
1 ni
DB NB B
1/2
,
(18.111)
where DB is the minoritycarrier diffusion coeﬃcient on the lowly doped side. The radiative recombination current from the neutral region can be written as
eV 1/2 b−b jd = e (BDB NB ) ni exp −1 . (18.112) kT
18 Diodes
Current (mA)
448
6 5 4 3 Ge Si 2 1 0 0.1 0.2 Si Ge 0.3 0.4 0.5 0.6 120 100 80 60 40 20 0 1 Bias voltage (V)
2
Fig. 18.40. Comparison of the characteristics of Ge and Si diodes at room temperature. Note the diﬀerent scales in the forward and reverse regime
Fig. 18.41. Characteristics of a Si power diode at two temperatures, 25 ◦ C and 100 ◦ C
The I–V characteristic for pndiodes from two semiconductors with different bandgap are shown in Fig. 18.40 (for Ge and Si). Both forward characteristics are exponential functions. The Si diode seems to have the steeper slope, however, the difference is only the smaller saturation current. The saturation current increases at higher temperature (Fig. 18.41). Real I–V Characteristics The ideal I–V characteristics are not observed for real diodes due to several reasons: – besides the diffusion current, also a generation–recombination (G–R) current is present
18.4 Bipolar Diodes
449
– already for fairly small forward voltages, high injection conditions are present, i.e. pn ≪ nn is no longer valid – the series resistance Rs of the diode is ﬁnite (ideally Rs = 0) – the diode has a ﬁnite parallel (shunt) resistance Rp (ideally Rp = ∞ ) – at high reverse voltage the junction breaks down; this phenomenon is treated in Sect. 18.4.5 First, we consider the generation–recombination current due to band– impurity (b–i) processes (see Sect. 10.10). Such recombination is nonradiative or at least does not produce photons with an energy close to the bandgap. The net rate is given by (10.52). For reverse voltage, the generation dominates the G–R current. For n < ni and p < ni , the net recombination rate r is r∼ =
σn exp
n σ σ v N Et −Eni p th t Ei −Et ni ≡ i , τe + σ exp p kT kT
(18.113)
where τe is the effective electron lifetime. The generation current density is given by jg =
eni w . τe
(18.114)
Since the width of the depletion layer varies with the applied reverse bias V , we expect a dependence 1/2
jg ∝ (Vbi + V )
.
(18.115)
The saturation current is given by the sum of the diffusion and generation parts js = e
Dp τp
1/2
n2i eni w + . ND τe
(18.116)
In semiconductors with large ni (narrow bandgap, e.g. Ge) the diffusion current will dominate; in Si (larger bandgap) the generation current can dominate. The maximum of the recombination rate is present for Et ≈ Ei (10.54). Then nt = pt = ni in (10.52). Assuming σ = σn = σp , the recombination rate is rb−i = σvth Nt
np − n2i . n + p + 2ni
(18.117)
Using (18.95) we can write rb−i
eV ni = σvth Nt ni exp −1 . n + p + 2ni kT
(18.118)
450
18 Diodes
The term ζ = by
ni n+p+2ni
is maximal for n = p, which is given (from (18.98))
nmr = pmr = ni exp
eV 2kT
.
(18.119)
Since ζ cannot be analytically integrated, typically as an approximation the maximum rate 1 1 ni eV = nmr + pmr + 2ni 2 1 + exp 2kT
ζmr =
(18.120)
is integrated over the depletion layer [183]. This approximation yields a recombination current
eV eσvth Nt wni exp eV kT − 1 ∼ mr eV jmr = , (18.121) = js exp 2 2kT exp 2kT + 1
with jsmr = eσvth Nt wni /2 and the approximation being valid for eV /kT ≫ 1. Thus the nonradiative band–impurity recombination is often said to cause an ideality factor of n = 2. In order to evaluate the integral of ζ over the depletion layer xn ζ dx (18.122) χ= −xp
in a good approximation, the dependence of the potential can be approximated as linear (constantﬁeld approximation), i.e. using the local ﬁeld Emr at the position where n = p [582]. For a symmetric diode with nn0 = pp0 , this position is at x = 0; for a onesided junction on the lowerdoped side. Emr is given for pp0 ≤ nn0 by
1/2
1/2 √ 2 pp 1 pp . ln 0 1+ 0 Emr = − (Vbi − V ) 1 + β (Vbi − V ) nn0 n n0 w (18.123) For a symmetric diode (18.124a) holds, for a onesided diode the approximation in (18.124b) holds 2 1/2 (Vbi − V ) ∝ (Vbi − V ) w √ 2 1/2 ∼ (Vbi − V ) ∝ (Vbi − V ) . =− w
Emr = −
(18.124a)
Emr
(18.124b)
We note that for V = 0 (18.82) is recovered from (18.124a). Using the above approximation ζ is given by ζ=
1 1 , 2 1 + exp (βV /2) cosh(βEmr x)
(18.125)
18.4 Bipolar Diodes
451
with β = e/kT . Since ζ decreases suﬃciently fast within the depletion layer, the integration over the depletion layer can be extended to ±∞ and we obtain
1/2
1/2 1 exp(βV /2) − 1 2 . (18.126) arctan χ= βEmr exp(βV ) − 1 exp(βV /2) + 1 −1
We note that for V = 0, the integral takes the value χ = (βEmr ) recombination current is now given by [582] jr,b−i
2σvth Nt ni kT = arctan Emr
exp(βV /2) − 1 exp(βV /2) + 1
. The
1/2
1/2 eV −1 . exp kT
(18.127)
For large voltage the arctan term becomes π/4. For eV /kT ≫ 1 the nonradiative recombination current can be written as
eV jr,b−i = jsr,b−i exp , (18.128) nkT with jsr,b−i = eσvth Nt ni kT π/(2Emr ). The voltagedependent ideality factor n (semilogarithmic slope n = βjr (V )/jr′ (V )) is close but not identical to 2 and is shown in Fig. 18.42 for various values of Vbi . The builtin voltage inﬂuences the logarithmic slope via the factor 1/Emr in (18.127).
(a)
(b)
Fig. 18.42. (a) Integral χ (18.122) multiplied by exp(βV /2) in order to extract the diﬀerences on a linear scale. Solid line: Exact numerical calculation, dashdotted line: standard approximation with constant maximum rate, dashed line: this work (approximation with constant ﬁeld). As material parameters we have used room temperature and ni = 1010 cm−3 (Si), nn0 = 1018 cm−3 and pp0 = 1017 cm−3 . (b) Logarithmic slope of band–impurity recombination current in the forward bias regime for various values of the builtin voltage Vbi = 0.6, 1.0, and 1.4 eV and in the limit Vbi → ∞. Adapted from [582]
452
18 Diodes
In the case of radiative band–band (b–b) recombination, the recombination rate is given by (10.14). Together with (18.98) and integrated over the depletion layer, the recombination current in the depletion layer is given by (cf. (18.109))
eV 2 jr,b−b = eBwni exp −1 , (18.129) kT
Potential (V)
Carrier concentration (cm3)
and exhibits an ideality factor of n = 1. Comparing (18.109) and (18.129), the dominating radiativerecombination current is determined by the ratio of w and Ln +Lp . Since in the forward direction, the depletionlayer width tends towards zero (for ﬂatband conditions), the radiativerecombination current is dominated by the recombination in the neutral region(s). 1018
p
1016
p
n
p
1014 10
p
n
n p
n
12
p
1010
n
n
108 2 1 0
(a)
10
(b) 0 x (μm)
10 10
(c) 0 x (μm)
10 10
0 x (μm)
10
Fig. 18.43. Theoretical modeling of chargecarrier concentration, intrinsic Fermi level (potential) ψ and quasiFermi levels (with arbitrary oﬀset) for a Si p+ n diode for various current densities: (a) 10 A cm−2 , (b) 103 A cm−2 and (c) 104 A cm−2 . NA = 1018 cm−3 , ND = 1016 cm−3 , τn = 0.3 ns, τp = 0.84 ns. Adapted from [583]
For high injection current (under forward bias), the injected minoritycarrier density can become comparable with the majoritycarrier density. In this case, diffusion and drift need to be considered. At large current density, the voltage drop across the junction is small compared to the ohmic voltage drop across the current path. In the simulation (Fig. 18.43), the highinjection effects start on the ndoped side because it has been modeled with the lower doping (ND < NA ). The series resistance Rs (typically a few Ohms) also effects the characteristic at low injection. The voltage drop across the junction is reduced by
18.4 Bipolar Diodes
453
Rs I. Thus, the I–V characteristic taking into account the effect of the series resistance is
e(V − Rs I) I = Is exp −1 . (18.130) nkT This equation is implicit with regard to I and can only be solved numerically. At high current, the resistance of the junction becomes very small (Fig. 18.44a) and the I–V characteristic is dominated by the series resistance and becomes linear.
Fig. 18.44. Theoretical I–V characteristic of a diode at room temperature with saturation currents for the n = 1 and n = 2 processes of Isn=1 = 10−12 A and Isn=2 = 10−9 A and resistances Rs = 10 Ω, Rp = 100 MΩ. Dashed line: Ideal diode with n = 1 characteristic only, dashdotted line: only n = 2 process, dotted line: only parallel ohmic resistance, short dashed line: only series resistance, solid line: all eﬀects combined as in (18.132)
The diode can also exhibit a parallel (shunt) resistance Rp , e.g. due to surface conduction between the contacts. Including the shunt resistance, the diode characteristic is
e(V − Rs I) V − Rs I I = Is exp . (18.131) −1 + nkT Rp The shunt resistance can be evaluated best from the differential conductance in the reversevoltage regime [559]. Due to a high surfacestate density, the passivation of GaAs diodes can be diﬃcult. Si can be very well passivated with low leakage current and high reliability. Often, a clear distinction between the n = 1 and n = 2 regimes cannot be made. In this case, an intermediate ideality factor 1 ≤ n ≤ 2 is ﬁtted to the I–V characteristic as in (18.131). If the current can be separated into
454
18 Diodes
a n = 1 (diffusion) and a n = 2 (recombination–generation) process, the characteristic is given by (see Fig. 18.44) (for V ≫ kT /e) e(V − Rs I) e(V − Rs I) V − Rs I n=2 n=1 + Is exp + I = Is exp . kT 2kT Rp (18.132) In summary, the pndiode has the equivalent circuit given in Fig. 18.45; the photocurrent source Iph is discussed below in Sect. 19.3.
Rs Iph
Id
Ir
nr
Rp
Fig. 18.45. Equivalent circuit of a pndiode. Serial (Rs ) and parallel (Rp ) resistance and diode currents: Id (due to diﬀusion, n ≈ 1), Irnr (nonradiative recombination due to band–impurity recombination, n ≈ 2) and an ideal current source due to photogeneration (as discussed in Sect. 19.3)
18.4.5 Breakdown If a large voltage is applied in the reverse direction, the pnjunction breaks down. At breakdown, a small voltage increase leads to a dramatic increase of the current. There are three mechanisms that lead to breakdown: thermal instability, tunneling, and avalanche multiplication [584, 585]. Thermal Instability The reverse current at large applied voltage leads to a power dissipation and heating of the junction. This temperature increase leads to a further increase of the saturation current (18.106). If the heat sink, e.g. the mounting of the chip, is not able to transport the heat away from the device, the current increases indeﬁnitely. If not limited by a resistor, such a current can destroy the device. The thermal instability is particularly important for diodes with high saturation current, e.g. Ge at room temperature.
18.4 Bipolar Diodes
455
Tunneling At large reverse bias, charge carriers can tunnel between conduction and valence band through the junction. A more detailed discussion will be given below in Sect. 18.5.9 about the tunneling diode. Since for the tunneling effect a thin barrier is necessary, breakdown due to tunneling is important for diodes where both sides are highly doped. For Si and Ge diodes, tunneling dominates the breakdown if the breakdown voltage Vbr is Vbr < 4Eg /e. For Vbr > 6Eg /e avalanche multiplication dominates. The intermediate regime is a mixed case. With increasing temperature, the tunneling current can be achieved already with a smaller ﬁeld (since the bandgap decreases with increasing temperature), thus the breakdown voltage decreases (negative temperature coefﬁcient). Avalanche Multiplication Avalanche multiplication due to impact ionization is the most important mechanism for the breakdown of pndiodes. It limits the maximum reverse voltage for most diodes and also the collector voltage in a bipolar transistor or the drain voltage in a ﬁeldeffect transistor. Avalanche multiplication can be used for the generation of microwave radiation or for photon counting (see Sect. 19.3.6). Impact ionization was discussed in Sect. 8.5.3. The most important parameters are the electron and hole ionization coeﬃcients αn and αp . For discussion of the diode breakdown, we assume that at x = 0 a hole current Ip0 enters the depletion layer. This current is ampliﬁed by the ﬁeld in the depletion layer and impact ionization. At the end of the depletion layer (x = w), it is Mp Ip0 , i.e. Mp = Ip (w)/Ip (0). Similarly, an electron current is increased on its way from w to x = 0. The incremental change of the hole current due to electron–hole pairs generated along a line element dx is dIp = (Ip αp + In αn )dx .
(18.133)
The total current in the depletion layer is I = Ip + In and is constant in stationary equilibrium. Therefore, dIp − (αp − αn ) Ip = αn I . dx The solution is Ip (x) = I
1 Mp
+
x αn exp − 0 (αp − αn )dx′ dx x . exp − 0 (αp − αn )dx′
x 0
For x = w we ﬁnd for the multiplication factor x w 1 ′ (αp − αn )dx dx . 1− αn exp − = Mp 0 0
(18.134)
(18.135)
(18.136)
456
18 Diodes
Avalanche breakdown is reached for Mp → ∞, i.e. when x w ′ (αp − αn )dx dx = 1 . αn exp −
(18.137)
0
0
A corresponding and equivalent equation is obtained when the consideration is started with the electron current. If αp = αn = α, (18.137) simpliﬁes to w αdx = 1 . (18.138) 0
103
10
2
10
1
100 14 10
(a)
GaP GaAs Si Ge 10
15
16
10 3 NB (cm )
10
17
10
w at breakdown (μm)
Breakdown voltage (V)
10
101
6
105
100
GaAs GaP Si
1
10
(b)
10 Si Ge
10
18
GaP
GaAs
2
Em at breakdown (V/cm)
This means that per transit of one carrier through the depletion layer, on average another carrier is created such that the process just starts to diverge. The breakdown voltage for various semiconductor materials is shown in Fig. 18.46a as a function of the doping level. The depletionlayer width w at breakdown and the maximum electric ﬁeld Em are depicted in Fig. 18.46b.
14
10
15
16
10 3 NB (cm )
Ge 10
17
10
18
Fig. 18.46. (a) Avalanche breakdown voltage for onesided abrupt junctions in Ge, Si, (100)GaAs and GaP at T = 300 K. The dashed line indicates the limit of avalanche breakdown at high doping due to tunneling breakdown. (b) Depletionlayer width w at breakdown and maximum electric ﬁeld Em for the same junctions. Adapted from [586]
In GaAs, the impactionization coeﬃcients and therefore the breakdown voltage are direction dependent. At a doping of NB = 1016 cm−3 , the breakdown voltage is the same for (001) and (111) orientation; for smaller doping the breakdown voltage of (001)oriented GaAs is smaller, for larger doping that of GaAs (111) [587]. At higher temperatures, the charge carriers release their excess energy faster to the lattice.18 Thus, less energy is available for impact ionization 18
The scattering rate becomes higher with increasing temperature and, e.g., the mobility decreases, see Sect. 8.3.7, and the drift saturation velocity decreases, see Sect. 8.5.1.
18.5 Applications and Special Diode Devices
457
Fig. 18.47. Temperature dependence of a n+ p Sidiode with NB = 2.5 × 1016 cm−3 and a guardring structure (cf. Fig. 18.48d). The temperature coeﬃcient ∂Vbr /∂T is 0.024 V/K. Adapted from [588]
and the required electric ﬁeld is higher. Therefore, the breakdown voltage increases with the temperature (Fig. 18.47). This behavior is opposite to tunneling diodes and the two processes can be distinguished in this way. In planar structures (Fig. 18.48a), high electric ﬁelds are present at the parts with large curvature. At these sites breakdown will occur ﬁrst and at much lower voltages than expected for a perfectly planar (inﬁnite) structure. For devices that require high breakdown voltage, design changes have to be made. These include deep junctions (Fig. 18.48b) with a smaller curvature, a ﬁeldring structure (Fig. 18.48c) in which an additional depletion layer is used to smooth the ﬁeld lines and the often used guard ring (Fig. 18.48d) for which a circular region of low doping (and thus high breakdown voltage) is incorporated.
18.5 Applications and Special Diode Devices In the following, various electronic applications of diodes are discussed. The most important special diode types are introduced. Optoelectronic applications (involving absorption and emission of photons) are treated below (Chap. 19). 18.5.1 Rectiﬁcation In a rectiﬁer, the diode has to supply a high resistivity for one polarity of the bias and a low one to the other polarity. In Fig. 18.49a, a singlepath rectiﬁcation method is shown. Only the positive halfwave can pass the load resistor RL (Fig. 18.49b). In Fig. 18.49c, the characteristic of a Si diode is shown. Of course, the voltage drop across the diode can only range in the
458
18 Diodes
n
+
n+
p
p
(b)
(a)
metal ring contact
n+
n+
n+ n guard ring
n p
p (d)
(c)
p+
Fig. 18.48. (a) Large electric ﬁelds at large curvatures in a shallow junction. Avoidance of regions with large electric ﬁelds by (b) deep junction and (c) ﬁeldring structure. (d) shows a guardring structure with circular, lowdoped n region. Grey area denotes insulating material, arrows indicate ﬁeld lines and the dashed lines indicate the extension of the depletion layers
1V regime. In order to make the setup work, the load resistor has to be considered. The total current is given by I = Is [exp (eUd /nkT ) − 1]. The total voltage U is split between the voltage drop across the diode Ud and that over the load resistance UL = RL I. The current is therefore given by I=
U − Ud . RL
(18.139)
For sizeable currents the voltage drop across the diode Ud is between 0.7 and 1 V. The characteristic is linear between about 1 and 220 V (Fig. 18.49d). Typically, the voltage UL is lowpass ﬁltered with a capacitor parallel to the load resistor. The effective voltage is the peak voltage divided by 2. The drawback of the single diode rectiﬁer is that only the positive halfwave contributes to a dc signal. The setup in Fig. 18.49e (bridge rectiﬁer) allows both halfwaves to contribute to the √ dc signal. The effective voltage in this case is the peak voltage divided by 2. The forward resistance in the static (Rf ) and dynamic (rf ) case are (for βVf > 3)
eVf Vf ∼ Vf exp − = If Is nkT
eVf ∼ nkT nkT ∂Vf = exp . rf = = ∂If eIs nkT eIf
Rf =
(18.140a) (18.140b)
18.5 Applications and Special Diode Devices
459
Fig. 18.49. (a) Singlepath mains rectiﬁer, (b) characteristics of Si diode (BYD127, Philips), (c) load characteristics of the mains rectiﬁer (RL = 400 Ω), (d) voltage output of singlepath mains rectiﬁer. (e) depicts the schematic circuit of a bridge rectiﬁer that works for both halfwaves, (f ) the resulting voltage output
460
18 Diodes
For reverse bias we have (βVr  > 3) Vr ∼ Vr = Ir Is
eVr  nkT ∂Vr = exp . rr = ∂Ir eIs nkT
Rr =
Thus, the dc and ac rectiﬁcations ratios are given by
eVf Rr = exp Rf nkT rr If . = rf I exp eVr  s
(18.141a) (18.141b)
(18.142a) (18.142b)
nkT
Rectiﬁers generally have slow switching speeds. A signiﬁcant time delay arises from the necessary chargecarrier recombination when the diode switches from low (forward) to high (reverse) impedance. This poses typically no problem for linefrequency (50–60 Hz) applications. For fast applications, however, the minoritycarrier lifetime needs to be reduced, e.g. by doping Si with Au (see Sect. 10.10). 18.5.2 Frequency Mixing
The nonlinear characteristic of the diode allows the mixing of frequencies, e.g. for second (or higher) harmonic generation, upconversion or demodulating of radiofrequency (RF) signals. A single balanced mixer is shown in Figs. 18.50a and b. The RF signal consists of a RF carrier frequency f0 modulated with an intermediate frequency (IF) signal fIF (t). It is mixed with a local oscillator (LO) that has a constant frequency fLO outside the RF modulation bandwidth f0 ± fIF . The IF signal can be detected from the setup in Fig. 18.50a if ﬁltered through a lowpass ﬁlter to avoid loss of power to the IF ampliﬁer. The temperature dependence of the diode characteristic (via js and β) on mixing eﬃciency is typically less than 0.5 dB for a change in temperature of 100 K. Problems of singlediode mixers are the radiation of localoscillator power from the RF input port,19 loss of sensitivity by absorption of input power in the local oscillator circuit, loss of input power in the intermediate frequency ampliﬁer, and the generation of spurious output frequencies by harmonic mixing. Some of these problems can be solved by circuit techniques, but these circuits often introduce new problems. Most mixers therefore use multiplediode techniques to provide a better solution of these problems. In Fig. 18.50c, the circuit diagram of a double balance mixer is shown. Evenorder harmonics of both the LO and the signal frequency are rejected. This mixer does not 19
that in military applications could make the mixer detectable by the enemy.
18.5 Applications and Special Diode Devices
461
require a lowpass ﬁlter to isolate the IF circuit. The three ports are isolated from each other by the symmetry of the circuit. These mixers usually cover a broader frequency band than the others. Ratios as high as 1000:1 are available. Microwave equivalents (working at f ≫ 1 GHz) of such mixer circuits are available. Bandwidth ratios as high as 40:1 are available at microwave frequencies in MMICs (millimeterwave integrated circuits). The common drawback of MMIC diodes is that they are obtained from the Schottky barriers used in ﬁeldeffect transistors, that have inferior performance compared to discrete diodes. The use of pHEMT technology20 for millimeterwave applications provides diodes that differently from regular Schottky diodes, since they consist of a Schottky barrier in series with a heterojunction. In Fig. 18.50d, a MMIC 45 GHz mixer is shown using fast GaAsbased pHEMTs.
(a)
(c)
(b)
(d)
Fig. 18.50. (a) Schematic circuit of single balanced mixer with input (RF: radio frequency, LO: local oscillator) and output (IF: intermediate frequency). (b) Optical planview image (300 × 125 µm2 ) of a highspeed single balanced mixer with two GaAs Schottky diodes with opposite poling. The device properties are Rs = 5 Ω, for I = 1 µA a forward and reverse voltage of 0.7 and 6 V, respectively; the capacitance of each diode is 8 fF. Reprinted with permission from [589]. (c) Schematic circuit of a double balanced mixer. (d) Optical image (1.65 mm2 ) of 40–45 GHz MMIC (Gilbert cell) mixer on GaAs basis using pHEMTs. Reprinted with permission from [590] 20
pseudomorphic high electron mobility transistors, see Sect. 21.5.7.
462
18 Diodes
18.5.3 Voltage Regulator In a voltage regulator, the large variation of resistance with applied bias is used. This effect occurs in the forward direction and close to the breakdown voltage. In Fig. 18.51a, a simple circuit is shown. When the input voltage Vin is increased, the current increases. The preresistor R1 = 5 kΩ and the load resistor represent a voltage divider with Vin = IR1 + Vout . The total current I is given by the two currents through the diode and the load resistor I = Is [exp(βVout /n) − 1] + Vout /RL . Therefore, the output voltage is implicitly given by
βVout R1 −1 . = Vin − R1 Is exp Vout 1 + RL n
(18.143)
R1
Vin
RL
Vout
(a)
(b)
(c)
(d)
Fig. 18.51. (a) Circuit diagram of a voltage regulator, (b) diode characteristic (n = 1). The vertical dashed lines show the operation conditions for RL = 2 kΩ and UE = 5 and 9 V and thus the principle of voltage stabilization. (c) Output vs. input voltage and (d) stability (diﬀerential voltage ratio α, see text) for input voltage between 5 and 9 V
18.5 Applications and Special Diode Devices
463
A large current change is related to a fairly small change of the voltage across the diode, which at the same time is the output voltage. Therefore, a change in the input voltage causes only a small change in the output voltage. We assume a diode with n = 1 and IS = 10−14 A with the characteristic shown in Fig. 18.51a. The numerical example in Fig. 18.51c is calculated for RL = 2 kΩ and 4 kΩ, respectively. The output voltage varies by about 0.02 V if the input varies between 5 and 9 V. In Fig. 18.51d, the differential voltage in ∂Vout change α = VVout ∂Vin is shown. In this way, voltage peaks can be ﬁltered from the input voltage. If two antiparallel diodes are used, this principle works for both polarities. Instead of a diode in the forward direction, the very steep slope of the diode I–V characteristic at the breakdown can be used. Just before breakdown, the diode has a high resistance and the voltage drops at the load resistor. If the input voltage increases a little, the diode becomes conductive and shorts the additional voltage (the maximum allowed breakdown current needs to be observed!). Due to its small saturation current, typically Si diodes are used. The breakdown voltage can be designed via the diode parameters. Such diodes with deﬁned breakdown voltage are called Z or Zener diodes (see next section). If the breakdown is due to tunneling (avalanche multiplication), the breakdown voltage decreases (increases) with temperature. If two diodes with positive and negative temperature coeﬃcient are put in series, a very good temperature stability of the breakdown voltage of 0.002%/K can be achieved. Such diodes can be used to realize a reference voltage. 18.5.4 Zener Diodes A Zener diode is designed to have a deﬁned breakdown voltage. Zener diodes are available with a number of different standard breakdown voltages. Their characteristic is shown for reverse bias with the current shown positive. The characteristics of various Zener diodes for different breakdown voltages are shown in Fig. 18.52. 18.5.5 Varactors A diode exhibits a voltagedependent capacitance. This effect can be used to tune an oscillator using the diode bias (voltagecontrolled oscillator, VCO). The equivalent circuit is shown in Fig. 18.53. The capacitance consists of a parasitic capacitance Cp due to mounting and bonding. This effect also causes a parasitic inductance. The series resistance due to mounting can typically be neglected. The variable junction capacitance Cj and the ohmic resistance Rs are bias dependent. The C(V ) dependence has generally a power law with an exponent γ (which itself may depend on the bias voltage)
464
18 Diodes 80 Z3
70
Current (mA)
60 Z4 50
Z5
Z6
40
Z7 Z8
30 20 10 0 0
5mA
1
2
3
4 5 6 7 Reverse voltage (V)
8
9
10
Fig. 18.52. Characteristics of a ﬁeld of Zener diodes (at room temperature)
Lp
Cp
Cj Rs
Fig. 18.53. Equivalent circuit of a varactor diode with parasitic capacitance Cp and inductance Lp and variable capacitance Cj and resistance Rs
C=
C0 , (1 + V /Vbi )γ
(18.144)
where C0 is thezero bias capacitance. Since the frequency f of an LC oscillator circuit depends on C −1/2 the frequency, f depends on the voltage as f ∝ V γ/2 . Therefore, a γ = 2 dependence is most desirable. For uniformly doped proﬁles, the capacitance depends with an inverse square root law on the applied voltage (18.90), i.e. γ = 0.5. Hyperabrupt junctions are typically made by ion implantation or epitaxy with graded impurity incorporation to create a special nonuniform doping proﬁle (Fig. 18.54a). For
18.5 Applications and Special Diode Devices
465
(a)
Frequency (scaled)
L
C (pF)
A L
H A
H
Vr + Vbi (V)
(b)
Bias voltage Vr (V)
(c)
Fig. 18.54. (a) Donordoping proﬁle according to (18.145) in p+ n or Schottky diodes for m = 0 (abrupt junction), m =1 (linearly graded junction) and two values with m < 0 (hyperabrupt junctions). (b) Bias dependence of capacitance for diodes with abrupt junction (‘A’, γ = 0.5), hyperabrupt junction (‘H’, γ > 0.5) and ‘epilinear’ junction (‘L’, γ = 2). (c) Frequency–voltage tuning characteristics (scaled to 1.0 for V = 0) for the three diode types. Parts (b) and (c) adapted from [591], reprinted with permission.
a doping proﬁle ˆB NB (z) = N
z z0
m
(18.145)
the capacitance is given as
ˆB ǫm+1 eN s C= (m + 2)z0m (Vbi − V )
1 m+2
=
C0 1
(1 + V /Vbi ) m+2
.
(18.146)
Ideally, m = −3/2 results is a linear frequency vs. voltage relation. The C– V characteristic of an implanted, hyperabrupt diode exhibits a part that has
466
18 Diodes
an exponent γ = 2 (Fig. 18.54b). A γ = 2 C(V ) dependence and therefore a linear f (V ) curve can be achieved over more than one octave using computercontrolled variable epitaxiallayer doping (Fig. 18.54c). 18.5.6 FastRecovery Diodes Fastrecovery diodes are designed for high switching speeds. The switching speed from the forward to the reverse regime is given by the time t0 = t1 + t2 with t1 being the time to reduce the minority carrier density to the equilibrium value (e.g. pn → pn0 ) and t2 being the time in which the current decreased exponentially. The time t1 can be drastically reduced by incorporation of deep levels that act as recombination centers. A prominent example is Si:Au. However, this concept is limited since the reverse generation current, e.g. (18.127), depends on the trap density. For direct semiconductors, recombination times are short, e.g. 0.1 ns or less for GaAs. In silicon, they can be extremely long (up to ms) or at least 1–5 ns. Schottky diodes are suitable for highspeed applications since they are majoritycarrier devices and minoritycharge carrier storage can be neglected.
Fig. 18.55. Current vs. time trace for a (soft) fastrecovery diode. Reprinted with permission from [592]
18.5.7 StepRecovery Diodes This type of diode is designed to store charge in the forward direction. If polarity is reversed, the charge will allow conductance for a short while, ideally until a current peak is reached (Fig. 18.56a), and then cutoff the current very rapidly during the socalled snapback time Ts (Fig. 18.56b). The cutoff can be quite rapid, in the ps regime. These properties are used for pulse (comb) generation or as a gate in fast sampling oscilloscopes. In Si, only 0.5–5 µs are reached (fastrecovery diode, see previous section) while GaAs diodes can be used in the several tens of GHz regime.
18.5 Applications and Special Diode Devices
467
(b)
(a)
Fig. 18.56. (a) Current vs. time trace for a steprecovery diode and sinusoidal voltage input. The lifetime must be suﬃciently large such that a current peak is reached. (b) Deﬁnition of the snapback time Ts . Reprinted with permission from [593]
Using a heterostructure GaAs/AlGaAs diode (see Sect. 18.5.11), as shown schematically in Fig. 18.57a, a steepening of a 15V, 70ps (10% to 90%) pulse to a fall time of 12 ps was observed (Fig. 18.57c). The forward current of the diode was 40 mA, supplied via a bias tee.
p+ GaAs
300nm
p Al0.3Ga0.7As
200nm
AlxGa1xAs
400nm
n+ Al0.3Ga0.7As
200nm
n+ GaAs
800nm
+
x=00.15
RS
~ VS
n+ GaAs substrate
(a)
If
Id SRD
RL VL
(b)
output
input 0
(c)
20
40
60
80 100 120 140 160 180 200 Time (ps)
Fig. 18.57. (a) Schematic layer sequence for fast GaAs/AlGaAs steprecovery diode. (b) Circuit with input and output pulse. (c) Input (dashed line) and output (solid line) waveforms. Vertical division is 2 V. Adapted from [594]
468
18 Diodes
18.5.8 pinDiodes In a pindiode, an intrinsic (i), i.e. undoped region (with high resistivity) is located between the n and the pregions. Often, also a region with low n or pdoping is used. In this case, the center region is denoted as a ν or πregion, respectively. The fabrication of arbitrary doping proﬁles and an intrinsic region poses little problem for epitaxial diodes.
w
n
(b)
NAND
(c)
(d)
E
(a)
i
( )
p
Fig. 18.58. (a) Schematic layer sequence of pindiode (‘i’: intrinsic, ‘π’: lowly pdoped), (b) net impurity distribution NA − ND , (c) space charge and (d) electric ﬁeld in a pin (solid lines) and a p–π–n (dashed lines) diode
Via the Poisson equation, the charge in the intrinsic layer is related to the electric ﬁeld. If no dopants are present, there is a constant (maximum) ﬁeld in the iregion at zero bias. If there is low doping, a ﬁeld gradient exists. The capacity for reverse bias is ǫs A/w and is constant starting at fairly small reverse bias (10 V). The series resistance is given by Rs = Ri + Rc . The contact resistance Rc dominates the series resistance for large forward bias.
18.5 Applications and Special Diode Devices
469
18.5.9 Tunneling Diodes For the invention of the tunneling diode and the explanation of its mechanism the 1973 Nobel Prize in Physics was awarded to L. Esaki. Eventually, the tunneling diode did not make the commercial breakthrough due to its high basis capacity. It is used for special microwave applications with low power consumption and for frequency stabilization. First, the tunneling diode is a pndiode. While the tunnel effect has already been discussed for Schottky diodes, it has not yet been considered by us for pn–diodes. We expect the tunnel effect to be important if the depletionlayer is thin, i.e. when the doping of both sides is high. The doping is so high that the quasiFermi levels lie within the respective bands (Fig. 18.59). The degeneracy is typically several kT and the depletion layer width is in the 10 nm range. p+
depletion region
n+
EC
qVp EV Fp
qVn Fn EC
EV
Fig. 18.59. Band diagram of a tunneling diode in thermodynamic equilibrium (V = 0). Vn and Vp characterize the degeneracies on the n and pside, respectively
In the forward direction, the I–V characteristic of the tunneling diode exhibits a maximum followed by a minimum and subsequently an exponential increase (Fig. 18.60a). As shown in Fig. 18.60b, the total current consists of three currents, the tunneling current, the excess current and the thermal (normal diode) current. The V = 0 situation is again shown in Fig. 18.61b. Upon application of a small forward bias, electrons can tunnel from populated conductionband states on the ndoped side into empty valanceband states (ﬁlled with holes) on the pdoped side (Fig. 18.61c). We note that this tunneling process is elastic. A similar situation, now with electrons tunneling from the valence band on the pside into the conduction band on the nside, is present for small reverse bias (Fig. 18.61a). Thus the rectifying behavior of the diode is lost. For larger forward bias, the bands are separated so far that the electrons coming from the ndoped side do not ﬁnd ﬁnal states on the pdoped side.
470
18 Diodes
Fig. 18.60. (a) Static current–voltage characteristics of a typical tunneling diode. Peak and valley current and voltage are labeled. (b) The three components of the c current are shown separately. Reprinted with permission from [183], 1981 Wiley I
V
+V +V +V V
(a)
(b)
(c)
(d)
(e)
Fig. 18.61. I–V characteristics (upper row ) and simpliﬁed band structure (lower row ) of a tunneling diode at various bias voltages as indicated with a dot in the I–V plot. (a) Reverse bias, (b) in thermodynamic equilibrium (V = 0), (c) in the maximum of the tunneling current, (d) close to the valley and (e) forward bias with dominating thermal current. The tunneling current is indicated with straight arrows. In (e) the thermionic emission current (curved arrow ) and the excess current with inelastic tunneling (dotted arrow ) are shown.
Thus the tunneling current ceases (Fig. 18.61d). The current minimum is at a voltage V = Vn + Vp > 0. The thermal current is the normal diode diffusion current (Fig. 18.61e). Therefore, a minimum is present in the I– V characteristic. The excess current is due to inelastic tunneling processes through states in the bandgap and causes the minimum to not drop down to almost zero current.
18.5 Applications and Special Diode Devices
471
The peak (Vp , Ip ) and valley (Vv , Iv ) structure of the characteristic leads to a region of negative differential resistance (NDR). Ip /Iv is termed the peaktovalley ratio (Fig. 18.62). Peaktovalley ratios of 8 (Ge), 12 (GaSb, GaAs), 4 (Si), 5 (InP) or 2 (InAs) have been reported (all at room temperature).
Fig. 18.62. Comparison of tunneling diodes based on Ge, GaSb and GaAs. Peaktovalley ratios are 8 (Ge) and 12 (GaSb, GaAs). Reprinted with permission from [183], c 1981 Wiley
18.5.10 Backward Diodes When the doping in a tunneling diode is nearly or not quite degenerate, the peaktovalley ratio can be very small. Then the tunnel current ﬂows mostly in the reverse direction (low resistance) and the forward direction has a higher resistance (with or without the NDR regime). Such diodes are called backward diodes. Since there is no minoritycharge carrier storage, such diodes are useful for highfrequency applications. 18.5.11 Heterostructure Diodes In a heterostructure diode, the n and pregions are made of different semiconductors. Such a diode is important in particular as an injection (emitter–base) diode in transistors. In Fig. 18.63, the band diagram is shown for a typeI heterostructure with the n (p) region having the smaller (larger) bandgap. Additionally to the builtin voltage, the barrier in the valence band is increased if the nregion is made from the semiconductor with larger bandgap Fig. 18.64. In this case, the (mostly undesired) hole current from the p to the nside is reduced. The peak in the conduction band poses potentially a greater barrier than the diffusion potential itself. The spike can be reduced by grading the materials across the heterojunction and creating a smooth transition of Eg between the materials. The effect of grading on the properties of the heterojunction is discussed in detail in [595].
472
18 Diodes
Fig. 18.63. Band diagram of a heterostructure diode (of the type nGaAs/pAlGaAs) (a) without contact of the n and pmaterials, (b) in thermodynamic c equilibrium. Reprinted with permission from [183], 1981 Wiley AlGaAs
Ec
Ec
Ev
Ev
GaAs
Ec
Ev (a)
(b)
(c)
Fig. 18.64. Schematic band diagram of a nAlGaAs/pGaAs diode (a) without contact of the n and pmaterials, (b) in thermodynamic equilibrium, and (c) with graded Al composition at the heterointerface
19 LighttoElectricity Conversion
19.1 Photocatalysis The absorption of light in a semiconductor across the bandgap creates free electrons and holes. In particular, for small particle size in powders1 these charge carriers can reach the surface of the semiconductor. At the surface they can react with chemicals. The hole can form •OH radicals from OH− attached to the bead. The electron can form O2 •− . These radicals can subsequently attack and detoxify, e.g., noxious organic pollutants in the solution surrounding the semiconductor. Such photocatalytic activity has been found, e.g., for TiO2 and ZnO powders. A review of photocatalysis, in particular with TiO2 particles and their surface modiﬁcations with metals and other semiconductors, is found in [596]. The eﬃciency of the photocatalytic activity depends on the eﬃciency of the charge separation (Fig. 19.1a). Any electron–hole pair that recombines within the bulk or the surface of the particle is lost for the catalytic activity. Thus, surfaces must exhibit a small density of recombination centers. Surface traps, however, can be beneﬁcial for chargecarrier separation when they ‘store’ the chargecarrier rather than letting it recombine. Small particles are expected to exhibit more eﬃcient chargecarrier separation than larger ones. Electrons at the surface can be donated and reduce an electron acceptor, typically oxygen, A → A− . A hole at the surface can oxidize a donor species, D → D+ . An example of increased photocatalytic activity are TiO2 powders with deposited metal particles (such as Pt) for H2 evolution and metaloxide particles (such as RuO2 ) for O2 evolution (Fig. 19.1b). Such a system behaves as a shortcircuited microscopic photoelectrochemical cell in which Pt is the cathode and RuO2 is the anode [597]. Excitation with light energy above the bandgap in the TiO2 particle (3.2 eV) injects electrons into the Pt particles and holes into the RuO2 particles. Trapped electrons in Pt reduce water to hydrogen and trapped holes in RuO2 oxidize water to oxygen. The photocatalytic activity is also tied to the geometrical shape of the semiconductor. Generally, powders with nanosized grains have much higher 1 ‘Small’ is here in relation to the diﬀusion length and does not need to be in the range where quantization eﬀects (quantum dots) are present.
474
19 LighttoElectricity Conversion surface recombination
TiO2
H 2O
H2 volume recombination
Pt H2O
(a)
(b)
O2
RuO2
Fig. 19.1. (a) Principle of photocatalytic activity. Light absorption creates an electron–hole pair. The electron and hole diﬀuse and can recombine in the bulk or at the surface. Free carriers can react with species from the surrounding solution. (b) Schematic representation of photocatalytic activity of TiO2 particle with Pt and c RuO2 depositions. Adapted from [596], reprinted with permission, 1995 ACS
activity than those with microsized particles [598]. In Fig. 19.2 it is shown that nanosized object with high surfacetovolume ratio are more effective catalysts than rather compact surfaces. In sunprotection cream only the UV absorption is wanted in UVA (330– 420 nm) and UVB (260–330 nm) ranges. Subsequent photocatalysis on the skin and the presence of radicals are unwanted. Thus the semiconductor particles (∼10–200 nm diameter) are encapsulated in microbeads (∼1–10 µm diameter) of silica, PMMA or urethane, also improving ease of dispersion, aggregation, stability and skin feel.
Fig. 19.2. SEM images of MOCVDgrown (a) ZnO thin ﬁlm and (b) ZnO nanoneedle layer. (c) Comparison of the photocatalytic activity (decoloration of the dye Orange II in aqueous solution) of the ZnO thin ﬁlm (irradiation with a Hg lamp for 5 h and 15 h) and the ZnO nanoneedles (irradiation 5 h). The sample labeled ‘control’ (scaled to 100%) is the start situation (absorption of the dye Orange II) without photocatalytic process. Adapted from [599], reprinted with permission
19.2 Photoconductors
475
19.2 Photoconductors 19.2.1 Introduction Charge carriers can be generated in the semiconductor through the absorption of light with a photon energy above or below the bandgap (Fig. 19.3). Absorption involving impurities occurs typically in the mid and farinfrared spectral regimes (cf. Sect. 9.5). The additional charge carriers cause an increase in the conductivity (8.9).
(a)
(b)
(c)
Fig. 19.3. Absorption and chargecarrier generation in a photoconductor: (a) band–band transition, (b) valenceband to acceptor and (c) donor to conductionband transition
19.2.2 Photoconductivity Detectors In stationary equilibrium for constant illumination of power Popt and photon energy E = hν the generation rate G is given by G=
n Popt /hν =η , τ V
(19.1)
where V is the volume (V = wdL, cf. Fig. 19.4) and τ denotes the chargecarrier lifetime. η is the quantum eﬃciency, i.e. the average number of electron–hole pairs generated per incoming photon. The photocurrent between the electrodes is Iph = σEwd ≈ eμn nEwd ,
(19.2)
assuming that μn ≫ μp and with E = V /L denoting the electric ﬁeld in the photoconductor, V being the voltage across the photoconductor. We can then also write
μn τ E Popt Iph = e η . (19.3) hν L
476
19 LighttoElectricity Conversion
With the primary photocurrent Ip = e η g=
Popt hν
we deduce a gain
τ μn τ E Iph = , = Ip L tr
(19.4)
where tr = L/vd is the transit time through the photoconductor. h
ohmic contact
L semico
w
nduc
tor I
d ohmic contact
(a)
(b)
Fig. 19.4. (a) Scheme of photoconductor. (b) Equivalent circuit of photoconductor
Now we consider a modulated light intensity P (ω) = Popt [1 + m exp(iωt)] ,
(19.5)
where m is between 0 and 1. For m = 0 it is a constant light power, for m = 1 the intensity is sinusoidally modulated between 0 and Pmax = 2Popt . √ 2 The rms optical power is given by 2mP . opt In the case of m = 1 this is √ equal to Pmax / 2. The rms photocurrent is iph ≈
1 eηmPopt τ √ . t 2hν r (1 + ω 2 τ 2 )1/2
(19.6)
The thermal noise at a conductivity G is i2G = 4kT GB ,
(19.7)
with B being the bandwidth over which the noise is integrated. The generation–recombination noise (shot noise) is i2GR =
τ 4qI0 B tr 1 + ω 2 τ 2
(19.8)
for the modulation frequency ω and I0 being the current in stationary equilibrium. The equivalent circuit with the ideal photocurrent source and the noise currents is depicted in Fig. 19.4b. 2
The rms value is the square root of the time average of the square of the power, P 2 .
19.2 Photoconductors
477
The signaltonoise ratio of the power is then given by −1 i2ph kT tr ηm2 (Popt /hν) 2 2 G (1 + ω τ ) S/N = 2 = . 1+ iG + i2GR 8B e τ I0
(19.9)
An important quantity is the noise equivalent power (NEP). This is the √ light power (mPopt / 2) for which the S/N ratio is equal to 1 (for B = 1 Hz). For infrared detectors the typical ﬁgure of merit is the detectivity D∗ that is deﬁned by
∗
D =
√
AB . NEP
(19.10)
A denotes the area of the detector. The unit of D∗ is cm Hz1/2 W−1 . It should be given together with the modulation frequency. It can be given for monochromatic radiation of a particular wavelength λ or a blackbody spectrum of given temperature T0 . 19.2.3 Electrophotography The principle of the Xerox copy machine is based on a photoconductive layer (Fig. 19.5). This layer is normally insulating such that both sides of the layer can be oppositely charged. If light hits the layer it becomes photoconductive and neutralizes locally. This requires a small lateral diffusion of charge carriers. Initially amorphous selenium (Eg = 1.8 eV) was used. The conductivity in the dark of aSe is 1016 Ω/cm. Se was subsequently replaced by organic material. The highest performance is currently achieved with amorphous silicon. On the charged areas of the photosensitive layer toner can be attached. The toner pattern is subsequently transferred to the copy sheet and ﬁxated. A copy takes typically more than one rotation of the drum. The principle was invented in 1938 by Chester F. Carlson (1906–1968) with sulfur as the photoconductor.3 19.2.4 QWIPs Quantumwell intersubband photodetectors (QWIPs) are based on the absorption of photons between two quantum well subbands (Fig. 19.6). A review can be found in [601]. Quantized electron or hole states can be used. Besides 3
In 1947 the Haloid company bought the rights to this process, renamed itself XeroX and brought the ﬁrst copy machine to the market in 1958 based on amorphous selenium. The word ‘xerography’ stems from the Greek word ξ´ ρoς (dry). The last ‘X’ in XeroX was added to mimic the name of the KodaK corporation.
478
19 LighttoElectricity Conversion
(f)
(g)
protective surface layer
0.5 μm
photosensitive layer
30 μm
blocking layer
3 μm
(h)
substrate
Fig. 19.5. Principle of xerography: (a) charging of the seleniumcovered drum, (b) (reﬂection) exposure of the Se, exposed areas become uncharged, (c) toner addition, (d) toner transfer to paper for copy, and (e) ﬁxation of the toner on the copy and preparation of drum for the next cycle. (f ) First xerox copy (Oct. 22nd 1938). (g) Schematic cross section of coating of photosensitive drum. The indicated thicknesses are approximate. (h) Image of drum with photosensitive layer made from amorphous silicon. Part (h) from [600]
an oscillator strength for this transition, the lower level must be populated and the upper level must be empty in order to allow this process. The Fermi level is typically chosen by appropriate doping such that the lower subband is populated.
E
bb bc
0
Lz
growth direction
Fig. 19.6. Schematic level diagram of a quantum well. Optical intersubband transitions between the ﬁrst and second quantized level (b–b) and the ground state and the continuum (b–c)
For inﬁnite barrier height the energy separation between the ﬁrst and second quantized levels (in the effectivemass theory) is (cf. (11.4)) E 2 − E1 = 3
2 π 2 . 2m∗ L2z
(19.11)
19.2 Photoconductors
479
(b)
(a)
Fig. 19.7. (a) AlGaAs/GaAs QWIP absorption spectrum for multiple reﬂection geometry. Adapted from [601]. (b) Transmission of AlGaAs/GaAs QWIP (100 QWs) in double reﬂection geometry (45◦ angle of incidence). The well doping is 1.0×1012 cm−2 (dashed line) and 1.5×1012 cm−2 (solid line). Adapted from [602]
For real materials the barrier height determines the maximum transition energy. Typical absorption and transmission spectra of a QWIP structure are shown in Fig. 19.7. The spectral response is in the mid or farinfrared. The dipole matrix element z = Ψ2 zΨ1 can be easily calculated to be z =
16 Lz . 9π 2
(19.12)
The oscillator strength is about 0.96. The polarization selection rule causes the absorption to vary ∝ cos2 φ, where φ is the angle between the electricﬁeld vector and the z direction (Fig. 19.8). This means that for vertical incidence (φ = 90◦ ) the absorption vanishes. Thus schemes have been developed to allow for skew entry of the radiation (Fig. 19.9a). The strict selection rule can be relaxed by using asymmetric potential wells (breaking of mirror symmetry/parity), strained materials (band mixing) or quantum dots (lateral conﬁnement). Also, a grating can be used to create a ﬁnite angle of incidence (Fig. 19.9b). Besides a useful detectivity (2 × 1010 cm Hz1/2 /W at 77 K) QWIPs have the advantage, e.g. against HgCdTe interband absorbers, that the highly developed GaAs planar technology is available for the fabrication of focal plane arrays (FPA) as shown in Fig. 19.10. A FPA is an image sensor (in the focal plane of an imaging infrared optics) and is used, e.g., for the detection of heat leaks in buildings or night surveillance. In particular, night vision support in cars may become a major market. A competing technology are bolometric arrays with thermally insulated pixels based on MEMS technology. The carriers that have been optically excited into the upper state leave the QW by tunneling or thermionic emission. Also, a QWIP can be made based on the direct transfer from the (populated) subband into the continuum.
Absorbance (arb. units)
19 LighttoElectricity Conversion
Absorbance (arb. units)
480
0
(a)
10
20
30 40 50 60 70 Polarizer angle (deg)
80
90
0
(b)
10
20 30 40 50 60 70 Angle of incidence (deg)
80
90
Fig. 19.8. Dependence of the QWIP response on (a) polarization and (b) angle of incidence. Dashed lines are guides to the eye. Adapted from [601]
MQW AlAs
h GaAs
(a)
GaAs
(b)
h
◦
Fig. 19.9. QWIP geometries: (a) 45 edge coupled with multiple quantumwell (MQW) absorber and (b) grating coupled with GaAs substrate, AlAs reﬂector and metal grating on top. Grey areas are highly ndoped contact layers
Fig. 19.10. Part of a 256×256 QWIP focal plane array (FPA) with grating coupler (area of one pixel: 37 µm2 ). From [603]
19.2 Photoconductors
481
The incoming infrared radiation creates a photocurrent density of iph = eηw Φ ,
(19.13)
where ηw is the quantum eﬃciency of a single quantum well (including the escape rate) and Φ is the photon ﬂux per time and unit area. During the transport of the charge carriers through the barrier they can be (re)captured by the QW with the probability pc . The capture probability decreases exponentially with the applied bias. The total photocurrent density (including generation and recapture) is jph = (1 − pc )jph + iph =
iph . pc
(19.14)
If the quantum eﬃciency is small, the eﬃciency of Nw quantum wells η ≈ Nw ηw . With this approximation the total photocurrent of Nw quantum wells is given by jph = eηΦg ,
(19.15)
where g is termed the gain of the structure and is given by g=
1 1 ηw . ≈ N w pc pc η
(19.16)
10
4
10
5
10
6
8
10
9
10
10
(a)
68
6
46 39 4
10
10
7
58
107 10
T(K) 77
Responsivity (A/W)
Dark current (A)
The dark current can be calculated from thermionic emission and agrees fairly well with experiment (Fig. 19.11a). When the voltage is increased further, avalanche multiplication can occur while the carriers are transported through the barrier(s). This mechanism provides further gain as shown in Fig. 19.11b.
4 3 2 1
11
12
0
5
1
2 3 Bias voltage (V)
4
0
5
(b)
6
7
9 8 10 Bias voltage (V)
11
12
Fig. 19.11. (a) Dark current of a QWIP at 10.7 µm, experimental (solid lines) and theoretical (dashed lines) response. (b) QWIP responsivity as a function of the applied voltage. The solid line (dashed line) is the theoretical dependence with (without) the eﬀect of avalanche multiplication. Adapted from [601]
482
19 LighttoElectricity Conversion
19.2.5 Blocked ImpurityBand Detectors Impurity absorption allows photoconductivity detectors in the mid and farinfrared regions to be made. In particular, for THz spectroscopy in medicine and astronomy the extension to longer wavelengths is interesting. For conventional photoconductors the impurity concentration is well below the critical dopant concentration (cf. Sect 7.5.5). Longwavelength response can be achieved by going to impurity/host systems with smaller ionization energy, such as Si:B (45 meV) → Ge:As (12.7 meV) → GaAs:Te (5.7 meV). By applying stress to Ge the energy separation between impurity and conduction bands can be lowered and subsequently the detector response is shifted towards longer wavelengths. For high doping the impurity level broadens to an impurity band and thus allows smaller ionization energy and thus stronger longwavelength detector response. However, conduction in the impurity band leads to dark current and makes such detectors unfeasible. In a blocked impurity band (BIB) detector [604, 605] an additional intrinsic blocking layer is sandwiched between the absorption layer and the contact (Fig. 19.12a). Such a structure is similar to a MIS diode, the insulator being the intrinsic semiconductor. We assume in the following an ntype semiconductor, such as Si:As or GaAs:Te, but also ptype BIBs can be made, e.g., from Ge:Ga. n
+
n
i n
+
h
(a)
w
0
b
EC (b) EV
0 (c) Ei Fig. 19.12. (a) Structure of BIB photodetectors. Highly doped contact layers (black ), doped semiconductor (white) and blocking (intrinsic) layer (grey). (b) Band diagram under small forward bias. Shaded area represents the donor impurity band. (c) Electric ﬁeld in the structure
19.2 Photoconductors
483
The semiconductor is highly doped (ND ) and partly compensated (NA ). Typically, the acceptor concentration must be small, about 1012 cm−3 , and controls the formation of the electric ﬁeld as shown below. The doping is so high that the impurities form an impurity band. Some of the electrons recombine with the acceptors NA− = NA and leave some donors charged ND+ = NA . For GaAs, e.g., the donor concentration in the doped semiconductor is > 1016 cm−3 and ∼ 1013 cm−3 in the ilayer. Under an external forward bias V , i.e. the positive pole is at the insulator, part of the applied voltage drops over the blocking layer of thickness b. If ideally no charges are present here, the electric ﬁeld is constant. In the ndoped material electrons move in the impurity band towards the insulator, forming neutral donors in an electron accumulation layer of thickness w in the presence of the charged acceptors NA− . This layer is the absorption layer. The mechanism can also be considered as if positive charge (the charged donors, ND+ ) moves (via hopping conduction) towards the back contact. In the literature the layer close to the insulator is thus also termed a ‘depletion layer’. The band diagram and the electric ﬁeld are shown in Fig. 19.12b,c. Due to the blocking layer the carriers on the donors in the ntype material cannot spill via the impurity band into the contact but must be lifted (by infrared photoabsorption) into the conduction band. From the Poisson equation the electric ﬁeld is given by e E(x) = − NA (w + x) , −w ≤ x ≤ 0 (19.17a) ǫs e (19.17b) E(x) = − NA w = Ei , 0 ≤ x ≤ b . ǫs The voltage drops across the blocking layer Vb and the doped semiconductor Vs fulﬁll V = Vb + Vs .
(19.18)
Integration of the ﬁelds yields w2 e NA ǫs 2 e Vb = NA wb . ǫs Vs =
(19.19a) (19.19b)
Substituting (19.19a,b) into (19.18) results in the width of the ‘depletion layer’
1/2 2ǫs V w= + b2 −b. (19.20) eNA The high dopant concentration allows for much thinner absorption layers than in a conventional photoconductivity detector, making it less susceptible to background highenergy cosmic radiation. The recombination in the depletion layer is negligible. Detector performance is modeled in [606].
484
19 LighttoElectricity Conversion
19.3 Photodiodes 19.3.1 Introduction The principle of the photodiode is the interband absorption of light in the depletion layer of a diode (or the izone of a pindiode) and the subsequent separation of electrons and holes by the electric ﬁeld. There are opposite requirements for fast detectors (thin depletion layer) and eﬃcient detectors (complete light absorption, suﬃciently thick depletion layer). For this reason generally semiconductors with high absorption coeﬃcient are most suited (Fig. 19.13). In Fig. 19.14 the quantum eﬃciency and detectivity D∗ of various semiconductor detectors are compared. A diode can be operated without bias (photovoltaic mode) using the builtin ﬁeld. An improvement in the speed of a pndiode is achieved with a reverse bias since it increases the ﬁeld strength in the depletion layer. However, the reverse bias is below the breakdown voltage. Operation near breakdown is exploited in the avalanche photodiode (APD). In the following we will discuss pn, pin, MS (Schottky), MSM and heterostructurediodes and APDs. 19.3.2 pn Photodiodes The most important ﬁgures of merit are the quantum eﬃciency, responsivity, noise equivalent power (NEP) and the response speed. If the depletion layer is hit by a photon ﬂux with a generation rate G0 (i.e. electron–hole pairs per unit volume per unit time) the photogenerated current is added to the diffusion current. The photocurrent density jp (per unit area) is
(a)
(b)
Fig. 19.13. Optical absorption coeﬃcient of various semiconductor materials used for photodetectors in (a) the UV, visible and nearinfrared range and (b) the midinfrared spectral range. From [607]
19.3 Photodiodes
485
(b)
(a)
Fig. 19.14. (a) Quantum eﬃciency and sensitivity of various photodetectors. (b) Detectivity D∗ of various photoconductors and photodiodes. Reprinted with perc mission from [183], 1981 Wiley optical inputs
currents
signal photoelectric effect
thermal noise signal dark interaction output signal circuit plus noise background
background
(a)
(b)
Fig. 19.15. (a) Schematic dark and illuminated I–V characteristics of a photodiode (for the case jp = −2js ). (b) Schematic representation of currents in a photodiode and equivalent circuit. Part (b) adapted from [608]
jph = −eG0 Lp
(19.21)
for a p+ ndiode. In order to obtain this result the diffusion and continuity equations have to be solved for the depletion region4 . Equation (19.21) means that the dark I–V characteristic is shifted by jph as shown in Fig. 19.15a. The number of electron–hole pairs that are generated per photon of energy hν by the absorption of the (monochromatic) light power Popt is 4 This derivation is done in Sect. 19.3.3. Equation (19.21) is obtained from (19.31) for vanishing thickness w and αLp ≪ 1.
486
19 LighttoElectricity Conversion
η=
Iph /e , Popt /(hν)
(19.22)
where Iph = Ajph is the photogenerated current over the √ surface A. For a modulated light intensity Popt must be replaced by mPopt / 2. The equivalent circuit including noise sources for a photodiode is shown in Fig. 19.15b. Random processes lead to shot noise i2S . Besides the photocurrent Iph itself, the background radiation (IB , in particular for infrared detectors) and the thermal generation (dark current, ID ) of carriers contribute: i2S = 2e (Iph + IB + ID ) B ,
(19.23)
with B being the bandwidth. Additionally, the parallel resistances cause thermal noise i2T = 4kT B/Req .
(19.24)
The resistance Req is given by the resistance of the depletion layer −1 = (junction) Rj , the load RL and the input of the ampliﬁer Ri as Req −1 −1 −1 Rj + RL + Ri . The series resistance Rs of the photodiode can be usually ignored in this context. For a fully modulated signal (m = √ 1) the signaltonoise ratio of the photodiode is given by (iph = eηmPopt /( 2hν)) S/N =
2 i2ph (eηPopt /hν) /2 . = i2S 2 + i2T 2 2e (Iph + IB + ID ) B + 4kT B/Req
(19.25)
Therefore the NEP is given by
1/2 Ieq 2hνB 1+ 1+ . NEP = η eB
(19.26)
The current Ieq is given by Ieq = IB + ID + 2kT /(eReq ). If Ieq /eB ≪ 1, the NEP is determined by the shot noise of the signal itself. In the other limit Ieq /eB ≫ 1 the detection is limited by the background radiation or thermal noise. In this case, the NEP is (for B = 1 Hz, in W cm2 Hz1/2 ) √ hν NEP = 2 η
Ieq e
1/2
.
(19.27)
In Fig. 19.16 the situation is shown for a silicon photodiode as a function of Req . The diode has a quantum eﬃciency of 75% at λ = 0.77 µm. A high value of Req ∼ 1 GΩ is necessary to ensure detection limited by dark current.
19.3 Photodiodes 10
10
10
NEP (W Hz1/ 2)
487
background current IB=10μA
11
10
12
10
13
IB=10μA IB=100nA IB=10nA IB=1nA dark current ID=150pA
10
14
10
15
IB=0
thermal noise of load 10
10
3
10
5
10
7
10
9
10
11
Req ( )
Fig. 19.16. NEP as a function of the resistance Req for a Si photodiode. Adapted from [608]
19.3.3 pin Photodiodes The depletion layer in pndiodes is relatively thin such that the incident light is not completely absorbed. An almost complete absorption of light can be achieved by using a thick intrinsic absorption layer. The ﬁeld in the intrinsic region is constant or slowly varying linearly (Fig. 18.58). The generation rate per unit area decreases exponentially (Lambert–Beer’s law) as shown in Fig. 19.17c: G(x) = G0 exp(−αx) .
(19.28)
The initial generation rate G0 = Φ0 α is given by the incident photon ﬂux per unit area Φ0 and the reﬂectivity of the surface R as Φ0 = Popt (1 − R)/(Ahν). The drift current in the iregion collects all those carriers (if recombination in the depletion layer is neglected). The electron drift current is given by w G(x)dx = eΦ0 [1 − exp(−αw)] , (19.29) jdr = −e 0
with w being the thickness of the depletion layer that is approximately the same as the thickness of the iregion. In the bulk (neutral) region (x > w) the minoritycarrier density is determined by drift and diffusion (as in (10.79)). The diffusion current density at x = w is given by jdiff = −eΦ0
Dp αLp exp(−αw) + epn0 . 1 + αLp Lp
The total current jtot = jdiff + jdr is given by Dp exp(−αw) jtot = −eΦ0 1 − . + epn0 1 + αLp Lp
(19.30)
(19.31)
488
19 LighttoElectricity Conversion
Fig. 19.17. (a) Schematic cross section of pindiode, (b) schematic band structure under reverse bias and (c) proﬁle of carrier generation due to light absorption. From [607]
The ﬁrst part is due to the photocurrent, the second is due to the diffusion current known from the pndiode. In normal operation, the second can be neglected compared to the ﬁrst. The quantum eﬃciency is jtot /e exp(−αw) = (1 − R) 1 − η= . Popt /hν 1 + αLp
(19.32)
For a high quantum eﬃciency of course a low reﬂection and a high absorption, i.e. αw ≫ 1, are necessary. However, for w ≫ 1/α the transit time through the depletion layer tr ≈ w/vs (at suﬃciently high ﬁeld, vs being the driftsaturation velocity) increases too much. The 3 dB cutoff frequency f3 dB (Fig. 19.18) is 2.4 ∼ 0.4 vs . f3 dB ∼ = = 2πtr w
(19.33)
Therefore a tradeoff exists between the quantum eﬃciency and the response speed of the pinphotodiode (Fig. 19.18). Choosing w ∼ = 1/α is a good compromise.
19.3 Photodiodes
489
Fig. 19.18. Quantum eﬃciency and 3 dB cutoﬀ frequency of a Si pindiode at T = 300 K for various wavelengths of input radiation. Adapted from [608]
19.3.4 PositionSensing Detector In a positionsensing detector (PSD) two electrodes are placed at opposite edges of a photodetector. The current output depends linearly on the beam position in between the electrodes, similar to a voltage divider. If two pairs of electrodes, one on the front and one on the back of the detector, are fabricated in orthogonal directions (Fig. 19.19a), the beam position can be measured in both x and y directions.
(a)
(b)
Fig. 19.19. (a) Scheme of twodimensional positionsensing detector (PSD), (b) image of PSD. From [609]
490
19 LighttoElectricity Conversion
19.3.5 MSM Photodiodes A MSM photodiode consists of a piece of semiconductor between two Schottky contacts (MS contacts). These are typically arranged laterally (as shown in Fig. 19.24b) but will ﬁrst be considered at the front and back of the semiconductor [610]. The band structure in thermodynamic equilibrium is shown in Fig. 19.20.
Fig. 19.20. Band diagram of a MSM structure with an ntype semiconductor in thermal equilibrium. From [610]
In the general case two different metals with two different barriers φn1 , φn2 and builtin voltage VD1 , VD2 are considered. If a voltage is applied across the MSM diode, one of the junctions is biased in the forward, the other in the reverse direction. We assume in Fig. 19.21 that the voltage biases the ﬁrst contact in the reverse direction, i.e. the ‘+’ pole is on the left contact. The applied voltage V is split between the two contacts, the larger voltage will drop at the reversebiased contact (here: V1 > V2 ) V = V1 + V 2 .
(19.34)
The electron current jn2 arises from thermionic emission at contact 2. Due to current continuity (without recombination since we inject majority charge carriers) this is also the current through contact 1, i.e. jn1 = jn2 .
(19.35)
The reverse current at contact 1 is jn1 = A∗n T 2 exp (−βφn1 ) exp (βΔφn1 ) [1 − exp (−βV1 )] ,
(19.36)
where Δφn1 is the barrier reduction due to the Schottky effect (Sect. 18.2.3 and (18.20)). The forward current at contact 2 is jn2 = −A∗n T 2 exp (−βφn2 ) exp (βΔφn2 ) [1 − exp (βV2 )] .
(19.37)
19.3 Photodiodes
491
Fig. 19.21. (a) Chargecarrier distribution, (b) electric ﬁeld and (c) potential for a MSM structure under bias (V < VRT ). From [610]
For a symmetric structure, i.e. φn1 = φn2 and VD1 = VD2 = VD , (19.35)– (19.37) yield together with (18.20) 3
1/4 $ % e ND 1 exp (βV2 ) − 1 1/4 1/4 = (V + V ) − (V − V ) ln . D 1 D 2 8π 2 ǫ3s β 1 − exp (−βV1 ) (19.38) Together with (19.34) a numerical or graphical solution can be found. Initially (for small voltages) the injected hole current (from contact 2) is much smaller than the electron current and diffusion occurs in the neutral region.
492
19 LighttoElectricity Conversion
(b)
(a)
(c)
Fig. 19.22. Electric ﬁeld (upper parts) and band diagram (lower parts) in a MSM diode for various bias conditions: (a) at reachthrough voltage VRT , (b) at ﬂatband voltage VFB and (c) for V > VFB . From [610]
The reachthrough voltage VRT is reached when the width of the neutral region is reduced to zero (Fig. 19.22a). At the juncture of the two depletion regions inside the semiconductor material the electric ﬁeld is zero and changes sign. For a larger voltage VFB ﬂatband conditions are present at contact 2, i.e. the electric ﬁeld is zero at contact 2 (Fig. 19.22b). At even larger voltage VB breakdown occurs. At V = VRT we have 1/2 2ǫs w1 = (19.39a) (V1 + VD1 ) eND 1/2 2ǫs w2 = (19.39b) (VD2 − V2 ) eND (19.39c) L = w1 + w2 , and therefore (with (19.34)) VRT =
2eND eND 2 L −L (VD2 − V2 ) − ΔVD , 2ǫs ǫs
(19.40)
with ΔVD = (VD1 − VD2 ), vanishing for a symmetric MSM structure. At and after reachthrough the electric ﬁeld varies linearly from 0 to L within the semiconductor. The point of zero electric ﬁeld shifts towards contact 2. At the ﬂatband voltage this point has reached the contact 2 and the width of the depletion layer at contact 2 is zero. This condition leads (as long as no breakdown occurred) to VFB =
eND 2 L − ΔVD . 2ǫs
(19.41)
19.3 Photodiodes
493
The maximum electric ﬁeld is at contact 1 and is given (for V > VFB ) by Em1 =
V + VFB + 2ΔVD . L
(19.42)
If in a part of the structure the critical ﬁeld EB for impact ionization is reached (this will be at contact 1, since the ﬁeld is highest there), the diode breaks down. Therefore the breakdown voltage is given by VB ≈ EB L − VFB − 2ΔVD .
(19.43)
The current–voltage characteristic for a SiMSM structure is shown in Fig. 19.23. At small voltages only small currents ﬂow since one contact is in reverse bias. The hole current is much smaller than the electron current. Only those holes that diffuse through the neutral region contribute to the hole current. After reachthrough the barrier φp2 + VD2 − V2 for hole injection is strongly reduced that leads to strong hole injection. Beyond the ﬂatband voltage the hole current increases only weakly since a lowering of the barrier occurs only via the Schottky effect. For high ﬁelds (V > VFB , before breakdown) the hole current is jp1 = A∗p T 2 exp (−βφp2 ) exp (βΔφp2 ) = jp,s exp (βΔφp2 ) ,
(19.44)
and the total current is 105
105
10
PtSiSiPtSi MSM 4 2 A=5 10 cm
jt ot Current density j (A/cm2)
Current density j (A/cm2)
Si MSM n1=0.85V
0
p2=0.2V p2=1.0V
10
5
10
10
0
5
T=350K 300K 193K
jn
77K
jp VRT VFB 10
(a)
VB
10
103
102
101 100 101 Voltage (V)
102
10
103
(b)
10
10
3
102
101 100 101 Voltage (V)
102
103
Fig. 19.23. Current voltage characteristics of a Si MSM structure, ND = 4 × 1014 cm−3 , L = 12 µm (thin polished, 111oriented wafer). (a) Theory for φn1 = 0.85 V and two diﬀerent values of φp2 for T =300 K. Total current (solid lines), electron current (dashed line) and hole current (dashdotted line). (b) Experiment on PtSiSiPtSi MSM structure (contact area: 5 × 10−4 cm−2 ) for four diﬀerent temperatures as labelled (for φp2 ≈ 0.2 V). Dashed lines are guides to the eye, solid line is high current part of theory from part (a). Adapted from [610]
494
19 LighttoElectricity Conversion (a)
(b)
+V
V
+V InGaAs:Fe active layer
+
InP:Fe substrate
(c)
(d)
Fig. 19.24. Scheme of MSM photodetector with interdigital contacts in (a) plan view and (b) cross section. In part (b), the electrical ﬁeld lines are shown schematically together with an electron–hole pair ready to be separated. (c) Scheme of a MSM mesa structure, (d) SEM image of an InGaAs/InP MSM mesa photodetector. Parts (c) and (d) from [611]
j = jn,s exp (βΔφn1 ) + jp,s exp (βΔφp2 ) ,
(19.45)
with jn,s = A∗n T 2 exp (−βφn1 ) and jp,s = A∗p T 2 exp (−βφp2 ). In a MSM photodetector the metal contacts are typically formed in an interdigitated structure on the semiconductor surface (Fig. 19.24). These contacts shield some of the active area from photons. An increase in quantum eﬃciency can be achieved with transparent contacts (e.g. ZnO or ITO) and an antireﬂection (AR) coating. The dark current is given by (19.45) and is minimal when electron and hole saturation currents are equal. This conditions leads to the optimal barrier height
φn = Eg − φph =
1 kT ln 2 e
me mhh
1 + Eg 2
(19.46)
close to middle of the bandgap. For InP and optimal barrier φn = 0.645 eV a dark current density of 0.36 pA/cm2 is expected for a ﬁeld of 10 V/µm. For deviating barrier height the current increases exponentially. The current– voltage characteristic of an InGaAs:Fe MSM photodetector is shown in Fig. 19.25 for a dark environment and various illumination levels. The timedependent response of a MSM photodetector depends on the drift time of the carriers, i.e. the time that a created electron and hole need
495
Current (μA)
19.3 Photodiodes
Bias voltage (V)
Fig. 19.25. dc I–V characteristic of an InGaAs/InP MSM photodetector (InP:Fe/InGaAs:Fe/InP:Fe, ﬁnger separation 1 µm, λ = 1.3 µm) under illumination for dark environment (0 µW) and various illumination levels as labeled. Adapted from [611]
to arrive at their respective contacts. In Fig. 19.26 a simulation is shown for a MSM detector. The current has two components, a fast one due to the electrons and a slow one due to the holes that have the lower mobility and smaller drift saturation velocity. A similar dependence is found in experiment (Fig. 19.27a). For longer wavelengths the detector is slower since they penetrate deeper into the material and thus the charge carriers have a longer path to the contacts (see scheme in Fig. 19.24b). An important role is played by the ﬁnger separation; smaller ﬁnger separation ensures a more rapid carrier collection (Fig. 19.27b). In [612] a bandwidth of 300 GHz was demonstrated for 100 nm/100 nm ﬁnger width and separation for LTGaAs5 and bulk GaAs, limited by the RC time constant. For 300 nm/300 nm ﬁngers and a LTGaAs a bandwidth of 510 GHz (pulsewidth of 0.87 ps) was reported, which is faster than the intrinsic transit time (1.1 ps) and not limited by the RC time constant (expected pulse width 0.52 ps), due to the recombination time (estimated to be 0.2 ps). 19.3.6 Avalanche Photodiodes In an avalanche photodiode (APD) intrinsic ampliﬁcation due to carrier multiplication (through impact ionization) in a region with high electric ﬁeld is used to increase the photocurrent. The ﬁeld is generated by a high reverse bias in the diode. In an ideal APD only one type of carrier is multiplied, resulting in the lowest noise. If electrons are injected into the ﬁeld region at x = 0 (Fig. 19.28a), the multiplication factor for electrons is Mn = exp(αn w) ,
(19.47)
5 LT: grown at low temperature, i.e. containing many defects that reduce the carrier lifetime.
19 LighttoElectricity Conversion Pulse response (arb. units)
496
electrons and holes
electrons holes
Time (ps)
Fig. 19.26. Simulation of the timedependent response of an InGaAs:Fe MSM photodetector to a short light pulse. Adapted from [611]
(a)
(b) Fig. 19.27. (a) Experimental timedependent response of an InGaAs:Fe MSM photodetector to a short light pulse for three diﬀerent wavelengths, inset shows the frequency response from a Fourier transform. (b) Response of the MSM for two diﬀerent ﬁnger widths and separations (both 1 or 2 µm, respectively), InGaAs layer thickness 2 µm, λ = 1.3 µm and bias voltage 10 V. Adapted from [611]
19.3 Photodiodes
EC
p
jn(0)
n
electron injection
h
n
h
p
n
n
EV h
n substrate
jp(w) 0
(a)
497
w
x
(b)
hole injection
Fig. 19.28. Schematic band structure (a) and schematic device setup (b) of an avalanche photodiode (APD). Adapted from [388]
for αp = 0. Typically, both carrier types suffer multiplication. If the electron and hole impact ionization coeﬃcients are the same (αn = αp = α), the multiplication factor for electrons and holes M is given by M=
1 . 1 − αw
(19.48)
The rms value of the current noise is the same as in the case of the pndiode (19.23), only that now the gain M is added i2S = 2e (Iph + IB + ID ) M 2 B .
(19.49)
The term M 2 is written as M 2 F (M ) with F (M ) = M 2 /M 2 being the excess noise factor that describes the additional noise introduced by the random nature of the impact ionization. For multiplication started with electron injection, it is given by
1 F (M ) = kM + (1 − k) 2 − , (19.50) M with k = αp /αn . For hole injection starting the multiplication (19.50) holds with k substituted by k ′ = αn /αp . In Fig. 19.29a the excess noise factor is shown vs. the average multiplication for various values of k and k ′ . Experimental data are shown in Fig. 19.29b for a Si APD. For short wavelengths absorption is preferential at the surface (nregion) and we have the case of hole injection. The data for the excess noise factor are fairly well ﬁt with k ′ ≈ 5. For longer wavelengths, the data for electron injection are ﬁt by k ≈ 0.2 = 1/k ′ . For a fully modulated signal the signaltonoise ratio is given by S/N =
(eηPopt /hν)2 /2 . 2e (Iph + IB + ID ) F (M )B + 4kT B/(Req M 2 )
(19.51)
498
19 LighttoElectricity Conversion
Excess noise factor F
Excess noise factor F
(a)
10
2
10
1
10
0
long wavelength EC
k, k'=
103
10
0
1
2
10 10 Multiplication M
10
3
10
3
10
2
theory hole injection electron injection
short wavelength
n/p 10 5 / 0.2 p n 0.1
10
1
10
0
100
(b)
101 102 Multiplication M
103
Fig. 19.29. (a) Excess noise factor for various values of the ratio of ionization coeﬃcients k or k′ . Adapted from [613]. (b) Experimental results for F for a Si APD with 0.1 µA primary current. The empty (full ) symbols are for short (long) wavelengths [primary hole (electron) current]. The inset shows the schematic band diagram of the npdiode under reverse bias. Adapted from [614]
If S/N is limited by thermal noise, the APD concept leads to a drastic improvement of noise. A particular APD structure is known as a solidstate multiplier. It has separate absorption and ampliﬁcation regions (SAM structure). In the lowﬁeld region the light is absorbed. One type of carrier is transported with the drift ﬁeld Ed to the multiplication region in which a large ﬁeld Em is present and multiplication occurs. In Fig. 19.30a a homoAPD with SAM structure is shown. Regions with different electric ﬁeld are created by a special doping proﬁle.6 A πpπ structure leads to regions with homogeneous low and high ﬁeld strengths. In the case of a heterostructureAPD with SAM structure (Fig. 19.30b) absorption (of light with suﬃciently long wavelength with an energy smaller the the InP bandgap) takes place only in the InGaAs layer. Since no light is absorbed in the multiplication region, the device functions similarly for front and back illumination. 19.3.7 TravelingWave Photodetectors In a standard photodetector there was a tradeoff between the thickness of the absorption layer and the speed of the detector. In a travelingwave photodetector the light absorption occurs in a waveguide such that for suﬃcient length L all incident light is absorbed. Complete absorption is achieved (‘long’ waveguide) if L ≫ (Γ α)−1 , α being the absorption coeﬃcient and Γ ≤ 1 be6
employing Poisson’s equation ∂(s (x)E(x))/∂x = ρ(x).
19.3 Photodiodes
499
NAND
p+
p+
n+
h
substrate
(i)
E multiplication region
Em
drift region
p+ InP
Ed
(ii)
n InP
InGaAs
+
n InP
h
h
(i)
Vr
NAND
(1R)0 exp(x)
(iii)
(ii) E
creation drift
multiplication
E
Vr small bias
EC EF
(a) (iv)
EV
drift region
(iii)
(b)
large bias
multiplication region
Fig. 19.30. (a) HomoAPD with SAM structure. (i) doping proﬁle, (ii) electrical ﬁeld, (iii) photon ﬂux or electron–hole pair generation rate and (iv) schematic band diagram under reverse voltage Vr with chargecarrier transport. The multiplication is for αn ≫ αp . Adapted from [183]. (b) (i) Scheme of an InP/InGaAs heteroAPD with SAM structure, (ii) doping proﬁle and (iii) electric ﬁeld for small (dashed line) and large (solid line) reverse bias Vr . Adapted from [388]
ing the optical conﬁnement factor, the geometrical overlap of the optical mode with the cross section of the absorbing medium (see also Sect. 20.4.4). The electrical connections are designed along this waveguide on the sides (coplanar layout, Fig. 19.31a) or above and below (Fig. 19.31b). The limitation due to a RC time constant is now replaced by the velocity match of the light wave √ vopt = c/n and the traveling electric wave in the contact lines vel ≈ 1/ LC. While the two waves travel along the waveguide, energy is transferred from the light wave to the electric wave. The 3 dB bandwidth due to velocity mismatch Bvm (for impedance matched, long waveguides) is given by
500
19 LighttoElectricity Conversion
Bvm =
Γ α vopt vel . 2π vopt − vel
(19.52)
For a MSM structure, whose electrode separation has been designed with a selfaligned process (without extensive effort in lateral patterning) by an etch depth of a few 100 nm (Fig. 19.32), 3 dB cutoff frequencies beyond 500 GHz have been achieved (Fig. 19.33). The quantum eﬃciency of this detector was still 8.1%.
Fig. 19.31. Scheme of a travelingwave photodetector (with pin structure). (a) coplanar contacts and (b) contacts as parallel plates. Reprinted with permission c from [615], 1992 IEEE
Fig. 19.32. Scheme of a MSM travelingwave photodetector in (a) cross section c and (b) plan view. Reprinted with permission from [616], 2001 IEEE
19.3 Photodiodes
501
Fig. 19.33. (a) Pulse response and (b) frequency response (Fourier transform of time response) of a MSM travelingwave photodetector (bias 5 V) for various illumination intensities, A: 1 mW, B: 1.8 mW and C: 2.2 mW. From [616]
19.3.8 Charge Coupled Devices The concept of the charge coupled device (CCD), an array of connected photodetectors serving as an image sensor, was devised by W.S. Boyle and G.E. Smith [617] (Fig. 19.34). As textbook for further details [618] may serve.
Fig. 19.34. First 8bit charge coupled device (1970). The chip (size: 1.5 × 2.5 mm2 ) consists of 24 closely packed MOS capacitors (narrow rectangles in the center grid). The thick rectangles at either end of the grid are input/output terminals.
A MIS diode (mostly a siliconbased MOS diode) can be designed as a light detector. The diode is operated in deep depletion. When a large reverse voltage is applied, initially a depletion layer is formed and the bands are strongly bent as shown in Fig. 19.35b. We note that in this situation the semiconductor is not in thermodynamic equilibrium (as it is in Fig. 19.35d) when the quasiFermi level is constant throughout the semiconductor. The inversion charge has yet to build up. There are three mechanisms to generate the inversion charge. (a) generation–recombination, (b) diffusion from the depletionlayer boundary and (c)
502
19 LighttoElectricity Conversion metal insulator
semiconductor
EC
eB
Ei EF EV
(a) EC
eB eS V>0
Ei EF EV
(b) Vi
EC
eS
eB
V>0
Ei EF EV
(c) Vi EC
eS
eB
V>0
(d)
inversion region
depletion region
Ei EF EV
neutral region
Fig. 19.35. Ideal MISdiode (with ptype semiconductor) as photodetector (principle of a CCD pixel). (a) Without bias (cf. Fig. 18.24b). (b) Immediately after an external (reversely poled) voltage V > 0 has been applied, the surface potential is Ψs = V and no charges have moved yet. (c) Strong depletion (still not in thermodynamic equilibrium) with signal charge and reduced surface potential Ψs < V . (d) The semiconductor in equilibrium (EF is constant) with depletion and inversion layer (cf. Fig. 18.28). For all diagrams, V = Vi + Ψs
19.3 Photodiodes
503
carrier generation by light absorption. Mechanisms (a) and (b) represent dark currents for the photodetector. The conductivity due to these two processes is shown in Fig. 19.36 and slowly builds up the inversion charge. Two temperature regimes are obvious; at low temperatures the generation dominates (∝ ni ∝ exp (−Eg /2kT )), at high temperatures the diffusion (∝ n2i ∝ exp (−Eg /kT )). The latter process can be strongly suppressed by cooling the device. 103
Si 10
4
10
5
10
6
G ( )
(a)
(b)
107 2.0
2.2
2.4
2.6 2.8 3.0 1000/T (1/K)
3.2
3.4
Fig. 19.36. Conductivity of a nSi/SiO2 diode as a function of temperature (1/T ). The slope of the dashed lines is (a) ∼ 0.56 eV (≈ Eg /2) and (b) ∼ 1.17 eV (≈ Eg ). Adapted from [619]
The gate voltage VG and the surface potential Ψs are related to each other via VG − VFB = Vi + Ψs =
eNA w eNA w2 + , Ci 2ǫs
(19.53)
where w is the width of the depletion layer. w will be larger than wm in thermodynamic equilibrium. The ﬁrst term in the sum is Qs /Ci and the second is obtained by integrating the Poisson equation for the constant charge density −eNA across the depletion layer. The elimination of w yields 1 2eǫs NA Ψs . (19.54) VG − VFB = Ψs + Ci
If light is absorbed in the depletion layer (process (c)), the hole (for pSi) drifts towards the bulk material. The electron is stored as part of the signal charge Qsig close to the oxide semiconductor interface (Fig. 19.35b). VG − VFB =
Qsig eNA w + + Ψs . Ci Ci
(19.55)
As a consequence of the increase in signal charge the potential well becomes shallower (19.55). For each gate voltage there is a maximum charge
504
19 LighttoElectricity Conversion Si 15V
s (V)
10
10V 5
5V 0 0
2 1 Qsig (1012 e/cm2)
3
Fig. 19.37. Surface potential as a function of the signal charge Qsig for various values of the bias VG − VFB as labeled for a SiO2 /pSi diode with NA = 1015 cm−3 and an oxide thickness of 100 nm. The dashed line represents the limit for inversion given by Ψs = 2ΨB ≈0.6 V. Adapted from [620]
(well capacity). The maximum signal charge is reached for Ψs ≈ 2ΨB (Fig. 19.37). In a charge coupled device (CCD) many lightsensitive MIS diodes, as described above, are fabricated in matrix form to create an image sensor. Upon application of a gate voltage they accumulate charge depending on the local exposure to light. The read out of this charge occurs by shifting the charge through the array to a readout circuit. Therefore charge is transferred from one pixel to the next. Several schemes have been developed for this task. The threephase clocking is shown schematically in Fig. 19.38. Other clocking schemes involve four, two or only one electrode per pixel [621]. Since the CCD sensor has many pixels (e.g. up to 4096) along a line, the charge transfer must be highly eﬃcient. The transfer of charge carriers occurs via thermal (regular) diffusion, selfinduced drift and the effect of the fringing ﬁeld (inset of Fig. 19.39). The time constant with which the charge carriers move due to diffusion (in a ptype semiconductor) is τth =
4L2 , π 2 Dn
(19.56)
where L is the length of the electrode. For a suﬃciently large charge packet the selfinduced drift due to Coulomb repulsion is important. The decay of charge is then given by t0 Q(t) = , Q(0) t + t0
(19.57)
with t0 = πL3 We Ci /(2μn Q(0)). We is the width of the electrode. This dependence is shown as a dashed line in Fig. 19.39a. The last electrons are eﬃciently
19.3 Photodiodes
505
(b)
(a)
(c)
(e)
(d)
(f)
(g)
(h)
Fig. 19.38. (a) Threephase CCD. Each pixel has three electrodes that can be switched independently (phases 1–3). (b,e,f ) Schematic of CCDs with four, two or one phase, respectively. (c) (t1 ) Charge accumulated after light exposure. A lateral potential well is formed along the row of pixels by the voltages at the three electrodes, e.g. P1 = P3 = 5 V, P2 = 10,V. (t2 –t7 ) transfer of charge, (t7 ) has the same voltages as (t1 ), the charge has been moved one pixel to the right. (d,g,h) Timing schemes for 4, 2 and 1phase CCDs, respectively. From [621]
transferred by the drift induced by the fringing ﬁeld of the electrodes (solid line in Fig. 19.39a). The origin of the fringing ﬁeld is schematically shown in Fig. 19.39b; the minimum fringing ﬁeld shown is 2 × 103 V/cm. In about
19 LighttoElectricity Conversion 10
0
0
0.9
10
2
0.99
10
3
0.999
10
4
0.9999
Si 105 0
2V
500
(a)
1500
1000 Time (ps)
7V
12V
0
s (V)
N(t) / N(0)
101
Efficiency
506
5
(b) 10
Fig. 19.39. (a) Eﬃciency of charge transfer with (solid line) and without (dashed line) the eﬀect of the fringing ﬁeld. (b) Schematic plot of the CCD electrodes and bias with the fringing ﬁeld for a threeelectrode CCD, oxide thickness 200 nm, doping ND = 1015 cm−3 . The electrode pitch is 4 µm and the gap between electrodes is 200 nm wide. Adapted from [622]
1–2 ns practically all (1 − 10−5 ) charges are transferred. This enables clock rates of several 10 MHz. For the clocking of the CCD the lateral variation of potential depth with the applied gate voltage is used. In Fig. 19.40 it is shown how a lateral variation of doping or oxide thickness creates a lateral potential well. Such structures are used to conﬁne the row of pixels against the neighboring rows (channel stops, Fig. 19.41). In order to avoid carrier loss at the interface between the oxide and the semiconductor a buriedchannel structure is used (Fig. 19.42).
V
V
NA
metal insulator
N'A>NA
s
NA
semiconductor
s
(a)
(b)
Fig. 19.40. Creation of a lateral potential well (barrier) in a MIS structure with (a) varying doping via diﬀusion or implantation and (b) varying (stepped) oxide thickness. Upper row shows schematic geometry, lower row depicts schematic lateral variation of the surface potential
19.3 Photodiodes
signal silicon (b) charge substrate
channel stops (a)
507
transfer electrode thick field oxide light channel stop depletion region
field shield channel stopping diffusion (c)
(d)
Fig. 19.41. (a) Schematic image of channel isolation. Cross section for channel isolation by (b) variation of oxide thickness, (c) highly doped region and (c) ﬁeld eﬀect. Adapted from [623]
SiO2 nSi
VG
pSi
(a) EC EV
EF Qsig=0
VGVFB
(b) EC
Qsig
EV
EF VGVFB (c)
Fig. 19.42. (a) Schematic layers of MIS diode with buriedchannel structure. Band diagram (b) after application of reverse voltage VG and (c) with signal charge Qsig . Adapted from [624]
508
19 LighttoElectricity Conversion
For front illumination parts of the contact electrodes shield the active area of the device. Higher sensitivity (in particular in the UV) is achieved for back illumination. For this purpose the chip is thinned (polished). This process is expensive and makes the chip mechanically less stable. For red/infrared wavelengths typically interference fringes occur for such thinned chips due to the small thickness. An increase in eﬃciency for front illumination can be achieved with an onchip microlens (Fig. 19.43).
(b)
(a)
Fig. 19.43. (a) Scheme for enhancement of CCD eﬃciency for front illumination by application of an onchip microlens. (b) SEM image of an array of such microlenses. From [625]
For color imaging the CCD is covered with a threecolor mask (Fig. 19.44a). On average there are one blue and one red pixel and two green pixels since green is the most prominent color in typical lighting situations. Thus each pixel delivers monochromatic information; RGB images are generated using suitable image software. Alternatives in highend products are the use of a beam splitter, static color ﬁlters and three CCD chips, one for each color (Fig. 19.44b), or the timesequential recording of three monochromatic images using one CCD chip and a rotating colorﬁlter wheel (Fig. 19.44c).
R G R G R (a) G
G B G B G B
R G R G R G
G B G B G B
R G R G R G
G B G B G B (b)
(c)
Fig. 19.44. (a) Arrangement of colors in a CCD color ﬁlter (‘R’: red, ‘G’: green, ‘B’: blue). Color splitting with (b) static color ﬁlters and (c) rotating color wheel. Parts (b) and (c) from [621]
19.3 Photodiodes
509
19.3.9 Photodiode Arrays An array of photodiodes is also suitable to create an image sensor. During illumination each diode charges a capacitor that is read out with suitable electronics. Based on CMOS technology (see Sect. 21.5.4) cheap image sensors can be made that show currently, however, inferior performance to CCDs. The builtin electronics allows simple outward connections (Fig. 19.45).
(a)
(b)
Fig. 19.45. (a) CMOS linear array sensor in a 8pin package. (b) Block diagram, the builtin timing generator allows operation only with start and clock pulse inputs. Reprinted with permission from [626]
The threecolor CCD image sensor did not offer RGB color information at each pixel. Therefore the spatial resolution of a color image is not directly given by the pixel distance. This is not a very dramatic drawback since human vision is more sensitive to intensity contrast than color contrast. However, RGB color information for each pixel would be desirable, giving higher resolution, in particular in professional photography. Such a sensor has been fabricated employing the wavelength dependence of the silicon absorption coeﬃcient (Fig. 19.13). Blue light has the shortest and red light the largest penetration depth. By stacking three photodiodes on top of each other (Fig. 19.46) photocurrents at different penetration depth are recorded that can be used to generate a RGB value for each pixel. In Fig. 19.47a a 16channel array of silicon avalanche photodiodes is shown. It features a quantum eﬃciency of > 80% between 760 and 910 nm. The pixel size is 648 × 208 µm2 on a 320 µm pitch. The gain is 100 and the rise time 2 ns. The InGaAs photodiode array in Fig. 19.47b is hybridized with CMOS readout integrated circuits. It is useful for detection in the spectral range 0.8–1.7 µm. The asymmetric diode size of 25 × 500 µm is designed for use in the focal plane of a monochromator. Another special type of photodiode array is the fourquadrant detector. A light beam generates four photocurrents Ia , Ib , Ic , Id of the respective parts (Fig. 19.48a). A beam deviation in the horizontal or vertical direction can be detected from the (signed) signals (Ia + Id ) − (Ib + Ic ) or (Ia + Ib ) − (Ic + Id ), respectively. We note that these signals can also be normalized to the total beam intensity Ia + Ib + Ic + Id .
510
19 LighttoElectricity Conversion
(b)
(a)
Fig. 19.46. (a) Scheme of image sensor with depthdependent light detection. From [627]. (b) Schematic layer sequence for threecolor pixel. ib , ig and ir denote the photocurrents for blue, green and red light, respectively. Adapted from [628]
(b)
(a)
Fig. 19.47. (a) Array of 16 silicon APDs. From [629]. (b) 1024pixel InGaAs photodiode array. From [630]
(a)
a
b
d
c (b)
Fig. 19.48. (a) Scheme of fourquadrant photodetector with sections ‘a’, ‘b’, ‘c’ and ‘d’, (b) image of fourquadrant silicon photodetector with circuit board. Part (b) from [631].
19.4 Solar Cells
511
19.4 Solar Cells Solar cells are light detectors, mostly photodiodes, that are optimized for the (largearea) conversion of solar radiation (light) into electrical energy. 19.4.1 Solar Radiation
.13 AM 1
AM1
The sun has three major zones, the core with a temperature of 1.56 × 107 K and a density of 100 g/cm3 in which 40% of the mass is concentrated and 90% of the energy is generated, the convective zone with a temperature of 1.3 × 105 K and a density of 0.07 g/cm3 , and the photosphere with a temperature of 5800 K and low density (∼ 10−8 g/cm3 ). The radius is 6.96 × 108 m and is about 100 times larger than that of the earth (6.38 × 106 m). The distance sun–earth is 1.496 × 1011 m. The angle under which the sun disk appears on earth is 0.54◦ . An energy density of 1367 ± 7 W/m2 arrives at the earth in front of its atmosphere. This value and the according spectrum of the sun’s emission, which is similar to a blackbody with temperature 5800 K (Fig. 19.50), is termed air mass zero (AM0). The total energy that reaches the earth from the sun is 1.8 × 1017 W per year. This value is 104 times the world’s primary energy need. Air mass zero (AM0) is important for solar cells in satellites. When the solar spectrum passes the earth’s atmosphere, it is changed with regard to its shape and the total energy density due to gas absorption (ozone, water, CO2 , . . . ). Depending on the meridian of the sun γ (Fig. 19.49), the spectrum on the surface of the earth is termed AMx with x = 1/ sin γ. In spring and fall (March 21st and September 21st), Leipzig (51◦ 42′ N latitude) has about AM1.61. At the summer (June 21st) and winter (December 21st) solstices the air mass in Leipzig is AM1.13 (γ = 61.8◦ ) and AM3.91 (γ = 14.8◦ ), respectively. Additionally, the duration of sunshine and thus the light power density is regionally different across the earth due to climate and weather (Fig. 19.51). For AM1.5, the incident power density is 844 W/m2 .
5
1.
AM
2
AM
.91
AM3 =14.8°
horizon
earth Fig. 19.49. Schematic path of sunlight through the atmosphere and deﬁnition of the air mass AMx
512
19 LighttoElectricity Conversion
Fig. 19.50. Solar spectra (power per area and wavelength interval) for AM0 (black line, extraterrestrial irradiance) and AM1.5 (sun at 41.8◦ elevation above horizon) for direct normal irradiance (blue line) and global total irradiance (red line) on a sun facing surface (tilted 37◦ towards the equator). Left (right) graph in loglog (linear) scales
(a)
(b) Fig. 19.51. Global sunshine distribution in (a) January and (b) July. The sunshine fraction is the actual number of bright sunshine hours over the potential number, and is thus expressed as a percentage ﬁgure. The color scale reaches from 0 to 100%. The sunshine data are in a 0.5 degree grid based on data from [632]
19.4 Solar Cells
513
19.4.2 Ideal Solar Cells When a solar cell made from a semiconductor with a bandgap Eg is irradiated by the sun, only photons with hν ≥ Eg contribute to the photocurrent and the output power. The I–V characteristic under illumination (Fig. 19.52) is given by
eV I = Is exp − 1 − IL , (19.58) kT with IL being the current due to generation of excess carriers by the absorption of the sunlight. The saturation current density is given by (18.105) and (18.106)
Dn Dp 1 Eg 1 + exp − js = Is /A = eNC NV , (19.59) N A τn N D τp kT with A being the cell area. The voltage at I = 0 is termed the opencircuit voltage Voc , the current at V = 0 is termed the shortcircuit current Isc = IL (Fig. 19.52). Only a part of the rectangle Isc × Voc can be used for power conversion. By choice of the load resistance RL , the work point is set. At Im and Vm , the generated power Pm = Im Vm is maximal. The ﬁlling factor F is deﬁned as the ratio F =
Im Vm . Isc Voc
The opencircuit voltage is given by
IL IL kT kT ∼ ln ln Voc = +1 = e Is e Is
(19.60)
(19.61)
and increases with increasing light power and decreasing dark current. The output power is
eV P = IV = Is V exp (19.62) − 1 − IL V . kT The condition dP/dV = 0 yields the optimal voltage at which the solar cell has to be operated and is given by the implicit equation (β = e/kT )
IL /Is + 1 1 1 (19.63) = Voc − ln (1 + βVm ) . Vm = ln β 1 + βVm β The current at maximum power is
1 − βVm Is /IL ∼ 1 Im = IL 1 − . = IL 1 − 1 + βVm βVm
(19.64)
514
19 LighttoElectricity Conversion
1.0
0.5 Pm
Current (A)
0.5 0.0
Power (W)
Vm Voc
0.0
0.5 Im
1.0
Isc 0.0
0.5 Voltage (V)
Fig. 19.52. Schematic I–V characteristics of a solar cell under illumination (left scale) and extracted power (right scale). The grey area is the maximum power rectangle with Pm = Im Vm .
Em is the energy that is delivered per photon at the load resistor at the power maximum. The maximum power is Pm = IL Em /e and Em is given by 1 1 Em ∼ . (19.65) − ) − e V ln (1 + βV = oc m β β The ideal solar cell has a (power) conversion eﬃciency η = Pm /Pin that can be determined from Fig. 19.53a. The right curve (1) in Fig. 19.53a shows the integral number nph of photons in the solar spectrum (per area and time) with an energy larger than a given one (Eg ). For a given value of nph , the left curve (2) represents the value of Em . The eﬃciency is the ratio of Em nph and the area under curve (1). The eﬃciency as a function of the bandgap is shown in Fig. 19.54a. It has a fairly broad maximum such that many semiconductors can be used for solar cells, in principle. The maximum theoretical eﬃciency for a single junction is 31% for nonconcentrated sunlight (AM1.5). This limit corresponds to the classic Shockley–Queisser limit [633], assuming radiative recombination as the only chargecarrier recombination mechanism. In [634], the limit for a single material is found to be 43% for an optimally tailored band structure that allows carrier multiplication by optically excited hot carriers. When the sunlight is concentrated, e.g. by a lens, the eﬃciency increases (Fig. 19.54b). The shortcircuit current increases linearly. The effect is mostly due to the increase of the opencircuit voltage. For C = 1000, the maximum theoretical eﬃciency for a singlejunction solar cell is 38%. A further increase of eﬃciency can be achieved with multiple junctions using various materials for absorption. In a tandem cell (two junctions), the
19.4 Solar Cells C=1 AM 1.5
4
515
64
(1)
(2)
48
hEg
32
2
jL (mA cm2)
nph (1017 cm2s1)
3
Em
1
(31%)
16 EgEm
0 0
1 Em= Eg= 0.9eV 1.35eV
(a)
2
0
3 Energy (eV)
(b)
Fig. 19.53. (a) Number of photons nph per area and time in the sun spectrum (AM1.5, C = 1 sun) with an energy larger than a cutoﬀ energy (curve 1) and graphical method to determine the quantum eﬃciency (from curve 2). Adapted from [635]. (b) Number of photons in concentrated solar spectrum (AM1.5, C =1000 sun) with an energy larger than a given energy and graphical method to determine the quantum eﬃciency of multijunction solar cells. Adapted from [183] after [635]
40
CuGaS2
Si GaAs Cu2O CdS CdTe
Fill factor
Ge
CuInS2 CuGaSe2
Efficiency (%)
Efficiency (%)
C=1000
20
C=1
Vo c(V)
10
(a)
FF
0.75
102
0.70 24
30
0 0
0.80
1
2 Eg (eV)
3
22 20
10
2
projected
18 16
14 0.8 0.7
Voc
0.6 10
(b)
1
jsc
Isc (A/cm2)
CuInSe2
0
1
2
10 10 Concentration C
10
3
Fig. 19.54. (a) Ideal quantum eﬃciency of solar cells (single junction) as a function of bandgap and light concentration C. The bandgaps of some important semiconductors are denoted by arrows. Adapted from [635]. (b) Properties of a silicon solar cell (water cooled) as a function of light concentration. Solid line is theoretically projected eﬃciency, dashed lines are guides to the eye. Adapted from [183].
516
19 LighttoElectricity Conversion
upper layer absorbs the higherenergy photons in a widebandgap material. The lowerbandgap material makes use of the lowenergy photons. Thus, the cell works with two different values of Em (Fig. 19.53b). With bandgaps of 1.56 eV and 0.84 eV, an eﬃciency of 50% can be reached theoretically. With three materials 56%, and for a large number of materials 72% is the limit. Between the junctions, tunneling diodes (Sect. 18.5.9) must be used to allow carrier transport through the entire structure. It is a nontrivial task to fabricate multiple heterojunctions due to incompatibilities of the lattice constants. Besides heteroepitaxy, wafer bonding can also be used for fabrication. A latticematched InGaP/GaAs/InGaAsN cell seems a viable solution for higheﬃciency solar cells. 19.4.3 Real Solar Cells For a real solar cell, the effect of parallel resistance Rsh (shunt resistance due to leakage current, e.g. by local shorts of the solar cell) and serial resistance Rs (due to ohmic loss) must be considered. The I–V characteristic is then (cf. (18.131))
I + IL V − IRs e (V − IRs ) . − +1 = (19.66) ln Is Is Rsh kT The serial resistance affects the ﬁlling factor more strongly than the shunt resistance (Fig. 19.55). Therefore, it is frequently enough to consider Rs only and use (cf. (18.130))
e(V − IRs ) I = Is exp − 1 − IL . kT
(19.67)
In the example of Fig. 19.55, a serial resistance of 5 Ω reduces the ﬁlling factor by a factor of about four. 19.4.4 Design Reﬁnements In order to collect electrons most eﬃciently, a back surface ﬁeld is used (Fig. 19.56). A higherdoped region at the back contact creates a potential barrier and reﬂects electrons back to the front contact. An important point for optimization is the management of the reﬂection at the solar cell surface. First, dielectric antireﬂection (AR) multilayers can be used. These layers should have a broad AR spectrum. Additionally, a textured surface, as schematically shown in Fig. 19.57a, e.g. created by anisotropic etching of Si (001) (Fig. 19.57c), reduces reﬂection (Fig. 19.57d), giving reﬂected photons a second chance for penetration (Fig. 19.57b). The reﬂectivity of bare Si, 35%, can be reduced to 2%. An AM0 eﬃciency of 15% was reached using textured cells.
19.4 Solar Cells 100
517
Rs=5 Rsh=100
Current (mA)
50 Rs=5 Rsh=
0
50 Rs=0 Rsh=100 Rs=0 Rsh=
100 0.5
0
0.5
1.0
Voltage (V)
Fig. 19.55. I–V characteristics of a solar cell considering shunt and series resistances Rs and Rsh , respectively. The eﬃciency of the real cell (shaded power rectangle) is less than 30% of that of the ideal cell. Adapted from [636] n
+
p
p
+
EF
metal
front surface
base
back metal surface
Fig. 19.56. Increase of the carrier collection eﬃciency by a back surface ﬁeld. Adapted from [637]
During its course over the sky during the day, the sun changes its angle towards a ﬁxed solar cell.7 A tracking mechanism can optimize the angle of incidence during the day and increase the overall eﬃciency of the solar cell (Fig. 19.58). 19.4.5 SolarCell Types Silicon is the most frequently used material for solar cells. Cells based on singlecrystalline silicon (wafers) have the highest eﬃciency but are the most expensive (Fig. 19.59a). Polycrystalline silicon (Fig. 19.59b) is cheaper but offers less performance. Material design is oriented towards increasing the grain size. These solar cells are also called ‘ﬁrstgeneration’ photovoltaics. Thin sheets of crystalline silicon drawn from a melt between two seed crystals in a modiﬁed CZ growth (sheet silicon or ribbon silicon) allow cheaper 7
We are of course aware that the earth rather rotates around the sun.
518
19 LighttoElectricity Conversion
incident reflected
(b)
(a)
0.6
Reflectivity
AR, flat 0.4
0.2
xt.
AR, te 0 0.3
(c)
(d)
0.5 0.7 0.9 Wavelength (μm)
1.1
Fig. 19.57. (a) Schematic surface topology of a textured solar cell. (b) Exemplary light path. (b) SEM image of a textured surface (pyramid base: ∼ 5 µm). (c) Reﬂectivity of antireﬂectioncoated ﬂat (dashed line) and textured (solid line) surface). Parts (a) and (d) adapted from [638]
Power (scaled units)
1.0 0.8 0.6 0.4 0.2 0.0
8
9 10 11 12 13 14 15 16 Daytime (h)
Fig. 19.58. Power generation of a solar cell vs. time (in daytime hours) for a stationary setup facing the sun at constant angle (solid line) and mounting with tracking (dashed line) to optimize the angle towards the sun. Adapted from [639]
production compared to cells based on ‘traditional’ polished wafers cut from a large silicon rod. Even cheaper are solar cells from amorphous silicon (Fig. 19.59c). Since silicon is an indirect semiconductor, a fairly thick layer is needed for light absorption. If direct semiconductors are used, a thin layer (d ≈ 1 µm) is
19.4 Solar Cells
519
suﬃcient for complete light absorption. Such cells are called thinﬁlm solar cells. A typical material class used in this type of cell are chalcopyrites, such as CuInSe2 (CIS). The bandgap is around 1 eV, which is not optimal. An improvement can be achieved by adding Ga and/or S that increases the band gap, Cu(In,Ga)(Se,S)2 (CIGS), to 1.2–1.6 eV. Using CIGS, an eﬃciency of 15% has been reported. Thinﬁlm solar cells can be fabricated on glass substrate or on ﬂexible polymer substrate such as Kapton8 (Fig. 19.60a,b). Also here, optimization of the grain size is important (Fig. 19.60b). As the front contact, a transparent conductive oxide (TCO), such as ITO (InSnO2 ) or ZnO:Al, is used. Thinﬁlm and amorphous silicon solar cells are also termed ‘secondgeneration’ photovoltaics.
(b)
(a)
(c) Fig. 19.59. Various types of solar cells: (a) monocrystalline silicon solar cell, (b) polycrystalline solar cell, (c) amorphous silicon solar cell. From [639]
In order to cover a large area and supply certain values of output voltage and current, several solar cells are connected into modules. Arrays are built up from several modules (Fig. 19.61). If solar cells are connected in parallel, the total current increases; if they are connected in series, the output voltage increases. ‘Thirdgeneration’ photovoltaics attempt to go beyond the 30% limit and comprise of multijunction solar cells, concentration of sunlight, use of hotcarrier excess energy as discussed above and possibly other concepts including photon conversion [641, 642]. 8
Kapton is a polyimide and a product and registered trademark of DuPont.
520
19 LighttoElectricity Conversion transparent contact antireflection coating window (ntype)
junction
absorber (ptype) Ohmic contact substrate
(a)
nZnO
pCuInSe2
Mo polyimide
(c)
(b)
1 µm
Fig. 19.60. (a) Schematic cross section of a polycrystalline thinﬁlm solar cell. (b) Rolled sheets of CIS thin ﬁlm solar cell on ﬂexible Kapton foil. (c) SEM cross section of CIS thinﬁlm solar cell. Parts (b) and (c) reprinted with permission from [640].
cell
module
array
Fig. 19.61. Schematic drawing of a solar cell (with contact grid), a module (36 cells) and an array of ten modules
19.4.6 Commercial Issues The cost9 of producing photovoltaic (PV) modules, in constant dollars, has fallen from as much as $50 per peak watt in 1980 to as little as $3 per peak watt in 2004. A projected cost of 0.2 €/kWh in 2020, a third of the current cost, is realistic and competitive in many applications. In 2002, photovoltaic power of 560 MW was installed worldwide. By the end of 2003, a total photovoltaic power of about 350 MW was installed in Germany. Thus, the PV power is 0.33% of the total installed electric power of 106 GW in Germany. 9
The following information is taken from [643] and [644].
19.4 Solar Cells
521
The current market growth of 30% (worldwide) is driven by crystalline silicon cells (95% in 2002). The energy payback period is also dropping rapidly. For example, it takes today’s typical crystalline silicon module about 4 years to generate more energy than went into making the module in the ﬁrst place. The next generation of silicon modules, which will employ a different grade of silicon and use thinner layers of semiconductor material, will have an energy payback of about 2 years. And thinﬁlm modules will soon bring the payback down to one year or less. However, market growth of thinﬁlm modules is currently slow. This means that these modules will produce ‘free’ and clean energy for the remaining 29 years of their expected life. PV technology can meet electricity demand on any scale. The solar energy resource in a 100 milesquare area of Nevada could supply the United States with all its electricity (about 800 GW), using modestly eﬃcient (10%) commercial PV modules. A more realistic scenario involves distributing these same PV systems throughout the 50 states. Currently available sites, such as vacant land, parking lots, and rooftops, could be used. The land requirement to produce 800 GW would average out to be about 17 × 17 miles per state. Alternatively, PV systems built in the ‘brownﬁelds’, the estimated 5 million acres of abandoned industrial sites in the US, could supply 90% of America’s current electricity. Solar power is expected to contribute 10% of the US energy need in 2030. For Germany, more than 2% in 2020 is probable. In 2001, PV module shipments in the US approached the 400 MW mark, representing a $2.5 to $3 billion market. The USbased industry itself is now approaching $1 billion per year and provides 25 000 jobs. It is expected to grow to the $10–$15 billion level in the next 20 years, providing 300 000 jobs by 2025.
20 ElectricitytoLight Conversion
20.1 Radiometric and Photometric Quantities 20.1.1 Radiometric Quantities The radiometric quantities are derived from the radiant ﬂux (power) Φe (or usually simply Φ) that is the total power (energy per time) emitted by a source, measured in Watts. The radiant intensity Ie is the radiant ﬂux emitted by a point source into a solid angle,1 measured in Watts per steradian (or W/sr). The irradiance Ee is the radiant ﬂux per area incident on a given plane, measured in W/m2 . The radiance Le is the radiant ﬂux per area and solid angle as, e.g., emitted by an extended source, measured in W/(m2 sr). 20.1.2 Photometric Quantities The photometric quantities are related to the visual impression and are derived from the radiometric quantities by weighting them with the V (λ) curve. The luminous ﬂux (luminosity or visible brightness) Φv of a source with the radiant ﬂux (spectral power distribution) Φ(λ) is given by ∞ Φ(λ)V (λ)dλ , (20.1) Φv = Km 0
with Km = 683 lm/W. This formula is also the deﬁnition of the unit ‘lumen’. In Fig. 20.1b, the conversion function2 V (λ) is shown for light and dark adapted vision.3 1
A solid angle Ω is the ratio of the spherical surface area A and the square of the sphere’s radius r, i.e. Ω = A/r2 . 2 The V (λ) curve has been experimentally determined by letting several observers adjust (decrease) the perceived brightness of a monochromatic light source at 555 nm to that of light sources of the same absolute radiation power at other wavelengths with socalled heterochromatic ﬂicker photometry. The ‘relative sensitivity curve for the CIE Standard Observer’ was determined in 1924. The ‘standard observer’ is neither a real observer nor an average human observer. The curve has shortcomings, e.g., due to the used spectral band width (20–30 nm) of the light sources and the comparison of spectral power instead of the photon ﬂux. 3 While photopic vision is due to cones, the scotopic (darkadapted) vision is due to rods. Rods are more than one thousand times as sensitive as the cones and
524
20 ElectricitytoLight Conversion
Further derived photometric quantities are luminous intensity (luminous ﬂux per solid angle), measured in candela (cd), the illuminance (luminous ﬂux per area), measured in lux (lx), and the luminance (luminous ﬂux per area and solid angle). The latter is particularly important if the radiation enters an optical system, e.g. for refocusing. The radiometric and photometric quantities are summarized in Table 20.1. Table 20.1. Radiometric and photometric quantities and units. The photometric units are lumen (lm), lux (lx=lm/m2 ) and candela (cd=lm/sr) quantity
Radiometric symbol
radiant ﬂux radiant intensity irradiance radiance
Φe Ie Ee Le
(a)
unit W W/sr W/m2 W/m2 /sr
quantity
Photometric symbol
luminous ﬂux luminous intensity illuminance luminance
Φv Iv Ev Lv
unit lm cd lx lm/m2 /sr
(b)
Fig. 20.1. (a) Relative eye sensitivity curves for photopic (light adapted, solid line) and (dark adapted, dashed line) vision. (b) Conversion of lumen to Watt for light(solid line) and darkadapted (dashed line) vision
20.2 Scintillators A scintillator (or phosphor) is a material that converts impacting highenergy radiation into photons [645]. Besides a high conversion eﬃciency, the spectrum and decay time constant of the scintillator are important for display can reportedly be triggered by individual photons under optimal conditions. Rods predominate in the peripheral vision and are not color sensitive.
20.2 Scintillators
525
applications. For display purposes, the photons are directly used for forming the image for the observer. For radiation detection, the photons are fed to a photomultiplier tube and counted. The most prominent applications, involving the conversion of electrons, are the screens of cathode ray tubes (CRT) (acceleration voltage > 10 kV) and of ﬂat panel devices, such as ﬁeldeffect displays (using a low voltage for excitation, typically < 1 kV) or plasma displays (using the UV light from the discharge of a plasma placed between two electrodes for excitation). Further details on electroluminescent displays can be found in [646]. Other forms of radiation detected with scintillators are α, β, and γradiation, Xrays and neutrons [647]. Different excitation conditions require different phosphors for optimal performance. 20.2.1 CIE Chromaticity Diagram The CIE4 procedure converts the spectral power distribution (SPD) of light from an object into a brightness parameter Y and two chromaticity coordinates x and y. The chromaticity coordinates map the color5 with respect to hue and saturation on the twodimensional CIE chromaticity diagram. The procedure for obtaining the chromaticity coordinates for a given colored object involves determination of its spectral power distribution P (λ) at each wavelength, multiplication by each of the three colormatching functions x ¯(λ), y¯(λ), and z¯(λ) (Fig. 20.2a) and integration (or summation) of the three tristimulus values X, Y , Z 780 nm P (λ)¯ x(λ)dλ (20.2a) X= 380 nm 780 nm
Y = Z=
380 nm 780 nm
P (λ)¯ y (λ)dλ
(20.2b)
P (λ)¯ z (λ)dλ .
(20.2c)
380 nm
Y gives the brightness. The tristimulus values are normalized to yield the chromaticity coordinates, e.g. x = X/(X + Y + Z). x and y obtained in this 4 ´ Commission Internationale de l’Eclairage. The color space can be described by diﬀerent coordinate systems, and the three most widely used color systems, Munsell, Ostwald, and CIE, describe the color space with diﬀerent parameters. The Munsell system uses hue, value, and chroma and the Ostwald system uses dominant wavelength, purity, and luminance. The more precise CIE system uses a parameter Y to measure brightness and parameters x and y to specify the chromaticity that covers the properties hue and saturation on a twodimensional chromaticity diagram. 5 This deﬁnition is motivated by the color vision of the eye. Two light sources will have the same color, even if they have diﬀerent SPDs, when they evoke the same color impression to the human eye.
526
20 ElectricitytoLight Conversion
(b)
(a)
Fig. 20.2. (a) Colormatching functions x ¯, y¯, and z¯ for the calculation of the CIE chromaticity, (b) colormatching functions r¯, g¯, and ¯b for the calculation of RGB values
way are the chromaticity coordinates. The third coordinate z = 1 − x − y offers no additional information and is redundant. Therefore, the color is represented in a twodimensional diagram, the CIE chromaticity diagram6 as shown in Fig. 20.3a. White is represented by x = y = z = 1/3. In order to relate the differences between colors as perceived by the human eye more closely to the geometrical distance in the chart, a revision was made (Fig. 20.3b) with new coordinates u′ = 4x/(−2x + 12y + 3) ′
v = 9y/(−2x + 12y + 3) .
(20.3a) (20.3b)
For CRTs the redgreenblue (RGB) color space is used.7 The color matching functions for RGB values are shown in Fig. 20.2b. The RGB values are related to the XYZ values according to ⎛ ⎞ ⎛ ⎞⎛ ⎞ R X 2.36461 –0.89654 –0.46807 ⎜ ⎟ ⎜ ⎟⎜ ⎟ (20.4) ⎝ G ⎠ = ⎝ –0.51517 1.42641 0.08876 ⎠ ⎝ Y ⎠ . B Z 0.00520 –0.01441 1.00920
6 The coloring of the chart is provided for an understanding of color relationships. CRT monitors and printed materials cannot reproduce the full gamut of the color spectrum as perceived in human vision. The color areas that are shown only depict rough categories and are not precise statements of color. 7 RGB is an additive color system. However, printing devices use a subtractive color system. This means that the ink absorbs a particular color, and the visible impression stems from what is reﬂected (not absorbed). When inks are combined, they absorb a combination of colors, and hence the reﬂected colors are reduced, or subtracted. The subtractive primaries are cyan, magenta and yellow (CMY) and are related to RGB via (C, M, Y ) = (1 − R, 1 − G, 1 − B).
20.2 Scintillators
527
(b)
(a)
(c) Fig. 20.3. CIE chromaticity diagram from 1931 (a) in the coordinates x and y and from 1976 (b) in the coordinates u′ and v ′ (20.3b). The curved upper boundary is called the ‘spectrum locus’ and contains monochromatic colors, the straight line at the lower left is termed the ‘purple boundary’. In the graph also the color of blackbody radiation is given, T = 5440 K corresponds to x = y = 1/3. ‘A’, ‘B’, ‘C’, and ‘E’ are standard illuminants, ‘D65’ denotes daylight with color temperature T = 6500 K. (c) CIE chart with the color ranges of sRGB, CIE and NTSC. Part (c) adapted from [648]
The CIE RGB primaries from 1931 are at 700, 546.1, and 435.8 nm with the relative intensities 1.0, 4.5907, and 0.0601. A display device using three phosphors can only display colors in the triangular area of the CIE chart be
528
20 ElectricitytoLight Conversion
tween the three chromaticity coordinates. For sRGB8 , the 1931 CIE primaries and the NTSC9 norm the coordinates are given in Table 20.2 and visualized in Fig. 20.3c. An optimal coverage of the CIE chart involves monochromatic sources (for laser TV or LED displays) at about 680, 520 and 440 nm. Table 20.2. Primaries and white points for sRGB, CIE and NTSC primary CIE NTSC sRGB
red
green
blue
white
0.73467 0.26533 0.27376 0.71741 0.16658 0.00886 0.33333 0.33333 0.6700 0.3300 0.2100 0.7100 0.1400 0.0800 0.3100 0.3160 0.6400 0.3300 0.3000 0.6000 0.1500 0.0600 0.3127 0.3290
20.2.2 Display Applications The once ubiquitous ambercolored monochrome displays are mostly fabricated using ZnS:Mn [646], having broad emission (540–680 nm) with its spectral peak at 585 nm (x = 0.50, y = 0.50) with an eﬃciency of 2–4 lm/W. In color television (and similar applications such as color computer monitors, tubes for aviation use, projection television) the image is reproduced by selective and timemultiplexed cathode excitation of three phosphors (blue, green and red) deposited on the internal face of the screen. The chromaticity coordinates of the standard CRT phosphors P22B, P22G and P22R are given in Table 20.3. They cover about the color range labeled ‘sRGB’ in Fig. 20.3c. For blue and green ZnS:Ag (x = 0.157, y = 0.069), ZnS:Ag,Cl, ZnS:Ag,Al and ZnS:Cu,Al (x = 0.312, y = 0.597), ZnS:Cu,Au,Al are used as phosphors, respectively. Y2 O2 S:Eu (x = 0.624, y = 0.337) activated with trivalent europium (Eu3+ ) facilitated such a gain in the brilliance of red over ZnS:Ag (more than doubled it) that it has totally replaced it at about one ﬁfth of the cost. For reproducible image quality, precise grainsize control (median size for CRT phosphors is about 8 µm), dispersion control and surface treatment are necessary. Flatpanel displays with their lower excitation voltage require different phosphors for optimal eﬃciency. 20.2.3 Radiation Detection The most commonly used scintillation detector for alpha measurements is ZnS activated with silver, ZnS:Ag. This material is not very transparent to light and is usually prepared as a large number of crystals with submm size attached with an adhesive to a ﬂat piece of plastic or other material. The 8
Standard RGB color space as deﬁned mainly by HewlettPackard and Microsoft, almost identical to PAL/SECAM European television phosphors. 9 National television standard colors, US norm.
20.2 Scintillators
529
Table 20.3. CIE color coordinates, peak emission wavelength and decay time (10%) of standard CRT phosphors phosphor
x
y
λp (nm)
decay time
P22B P22G P22R
0.148 0.310 0.661
0.062 0.594 0.332
440 540 625
∼20 µs ∼60 µs 1 ms
ﬂat screen is optically coupled to a photomultiplier tube that is attached to associated electronics. The voltage and discriminator levels are selected so that the detector is sensitive to the rather large pulses from alpha interactions but insensitive to beta or gammainduced pulses. The alpha particles deposit all of their energies in a small thickness of material compared to beta and gamma radiations. Scintillation detectors for beta radiation are often made from organic materials. In an organic scintillator, the light emission occurs as a result of ﬂuorescence when a molecule relaxes from an excited level following excitation by energy absorption from ionizing radiation. Molecules such as anthracene, transstilbene, paraterphenyl, and phenyl oxazole derivatives are among the many organic species that have useful scintillation properties. The organic molecules are dissolved in organic solvents and used as liquid scintillators. A classic application is in the measurement of lowenergy beta radiation from, e.g. tritium, 14 C, or 35 S. In such cases, the sample containing the radioactive beta emitter is dissolved in, or in some cases suspended in, the liquid scintillation solution. The emitted beta radiation transfers energy through the solvent to the scintillator molecule that emits light, subsequently detected by photomultiplier tubes. Organic scintillator molecules can also be dissolved in an organic monomer that can then be polymerized to produce a plastic scintillator in a wide variety of shapes and sizes. Very thin scintillators have been used for alpha detection, somewhat thicker scintillators for beta detection. Largevolume plastic scintillators have been used in gamma detection, particularly for doserelated measurements. Other inorganic crystalline scintillators, especially sodium iodide activated with thallium, NaI:Tl, have been used for gammaray energy measurements. Such detectors can be grown as large single crystals that have a reasonably high eﬃciency for absorbing all of the energy from incident gamma rays. There exists a rather large number of inorganic scintillators; some examples of these include cesium iodide activated with thallium, CsI:Tl, bismuth germanate, Bi4 Ge3 O12 , and barium ﬂuoride, BaF2 . These are mostly used for gamma measurements but can also be prepared with thin windows and have been used for charged particle (e.g. alpha and beta) counting. In Table 20.4, the peak emission wavelength and the characteristic decay time are listed for a variety of scintillator materials. Direct semiconductors,
530
20 ElectricitytoLight Conversion
Table 20.4. Emission peak wavelength and decay time of various scintillator materials material
λp (nm)
decay time
Zn2 SiO4 :Mn ZnS:Cu CdWO4 CsI:Tl CsI:Na Y3 Al5 O12 :Ce Lu2 SiO5 :Ce YAlO3 :Ce ZnO:Ga
525 543 475 540 425 550 400 365 385
24 ms 35–100 µs 5 µs 1 µs 630 ns 65 ns 40 ns 30 ns 2 ns
although not offering the highest eﬃciency, are particularly useful for high time resolution in, e.g., timeofﬂight measurements or fast scanning electron microscopy. 20.2.4 Luminescence Mechanisms SelfTrapped Excitons In a strongly ionic crystal, such as NaI, a hole becomes localized to an atomic site via the polaron effect. A spatially diffuse electron is attracted, and a selftrapped exciton is formed that can recombine radiatively. SelfActivated Scintillator In such material, the luminescent species is a constituent of the crystal. The emission involves an intraionic transition, e.g. 6p→6s in Bi3+ of Bi4 Ge3 O12 , or a chargetransfer transition in the case of (WO4 )2− in CaWO4 . At room temperature, nonradiative competing processes limit the eﬃciency. Activator Ions For dopant ions such as Eu2+ in YO2 S:Eu, Ce3+ in YAlO3 :Ce or Tl+ in NaI:Tl, the hole and electron excited by the radiation are sequentially trapped by the same ion that then undergoes a radiative transition, in the case of Eu and Ce10 5d→4f, for Tl 3 P0,1 →S0 . CsI:Tl has one of the highest eﬃciencies of 64.8 photons/keV [649].
10
This transition is dipole allowed for Ce and partially forbidden for Eu.
20.3 LightEmitting Diodes
531
Core–Valence Luminescence In some materials, e.g., BaF2 , CsF, BaLu2 F8 the energy gap between the valence band and the top core band is less than the fundamental bandgap. A radiative transition occurs when an electron from the valence band ﬁlls a hole in the top core band that has been created by the radiation. The light yield is limited to about 2 photons/keV. Semiconductor Recombination Processes Free excitons or excitons bound to impurities can recombine radiatively. This process is most eﬃcient at low temperatures. At room temperature, the emission is typically much weaker ( 10×) since excitons become unbound or dissociated. Highly doped ntype semiconductors, e.g. CdS:In, exhibit recombination between donorband electrons and holes. ZnO:Ga has an eﬃciency of about 15 photons/keV and a fast response (with 2.4 photons/keV emitted in the ﬁrst 100 ps). Luminescence can also stem from donor–acceptor pair transitions, e.g. in PbI2 with an eﬃciency of 3 photons/keV at 10 K. Isoelectronic impurities such as nitrogen in GaP:N and tellurium in CdS:Te attract an electron and subsequently a hole. In ZnS:Ag and ZnS:Cu (conduction) band to trap recombination is dominant. In a codoping scheme like CdS:In,Te, In supplies electrons in an impurity band that can recombine with holes trapped at Te.
20.3 LightEmitting Diodes 20.3.1 Introduction Lightemitting diodes (LEDs) are semiconductor devices in which injected carriers recombine radiatively. The recombination process leading to light emission can be of intrinsic nature, i.e. band–band recombination, or extrinsic, e.g. impuritybound excitons. Impurityrelated luminescence can also be excited via impact excitation. For an extensive treatment of LEDs see [650]. 20.3.2 Spectral Ranges Applications for LEDs can be sorted by the color of emission. In Fig. 20.4a, the standard sensitivity V (λ) of the human eye is shown (cf. Fig. 20.1a). In the visible spectral region (about 400–750 nm) the perceived brightness of the LED depends on the eye sensitivity. It is largest in the green (at 555 nm) and drops strongly towards the red and blue. The most important spectral regions and applications are: – infrared (λ > 800 nm): remote controls, optocouplers, lowcost data transmission, IR interface
532
20 ElectricitytoLight Conversion
– visible: indicator LED, lighting11 (room, buildings, cars), white LED for broad spectrum – ultraviolet (λ < 400 nm): pumping of phosphors for white LEDs, biotechnology
Fig. 20.4. Spectral coverage by various semiconductor materials. Reprinted with c permission from [183], 1981 Wiley
In Fig. 20.4, potentially useful semiconductors for the various spectral regions are shown. The semiconductors that are currently used for the various colors of the visible spectrum are – – – – –
red–yellow: GaAsP/GaAs, now AlInGaP/GaP yellow–green: GaP:N green–blue: SiC, now GaN, InGaN violet: GaN ultraviolet: AlGaN
20.3.3 Quantum Efficiency The total quantum eﬃciency η is the number of photons emitted from the device per injected electron–hole pair. It is given by the product of the internal quantum eﬃciency ηint and the external quantum eﬃciency ηex : 11
Penetration of white LEDs into the general lighting market could translate (globally) into cost savings of $1011 or a reduction of power generation capacity of 120 GW.
20.3 LightEmitting Diodes
η = ηint ηex .
533
(20.5)
The internal quantum eﬃciency is the number of photons generated (inside the semiconductor) per injected electron–hole pair. High material quality, low defect density and low trap concentration are important for a large value of ηint . The recombination current in the pndiode has been already given in (18.109). The external quantum eﬃciency is the number of photons leaving the device divided by the total number of generated photons. The geometry of the LED is of prime importance to optimize ηex . Due to the large index of refraction of the semiconductors (ns ∼ 2.5–3.5), light can leave the semiconductor only under a small angle θc from the surface normal due to total reﬂection (cf. (9.3) and see right part of Fig. 9.3). Against air (n1 ≈ 1) the critical angle is θc = sin−1 (1/ns ) .
(20.6)
The critical angle for total reﬂection is 16◦ for GaAs and 17◦ for GaP. Additionally, a portion of the photons that do not suffer total reﬂection is reﬂected back from the surface with the reﬂectivity R given by (cf. (9.7))
2 ns − 1 R= . (20.7) ns + 1 We note that the above formula is valid strictly for vertical incidence. For the GaAs/air interface, the surface reﬂectivity (for normal incidence) is about 30%. Thus, the external quantum eﬃciency for a LED is given by (1–R) and the critical angle by ηex ∼ =
4ns 4n1 ns (1 − cos θc ) ≈ (1 − cos θc ) . 2 (n1 + ns ) (ns + 1)2
(20.8)
The latter approximation is valid when the outer medium is air. For GaAs, the external quantum eﬃciency is 0.7 × 4% ≈ 2.7%. Thus, typically only a small fraction of generated photons can leave the device and contribute to the LED emission. 20.3.4 Device Design The following strategies have allowed signiﬁcant improvement of LED eﬃciency: Nonplanar Surfaces With curved surfaces, the problem of total reﬂection can be (partially) circumvented. Spherically polished chips are feasible, but, very expensive. The epoxy seal of the standard LED case (Fig.20.6a) and its shape play a similar role, however, with a smaller index of refraction than the semiconductor, and are important for the beam shape.
534
20 ElectricitytoLight Conversion 20°
semiconductor
10°
0°
10°
30°
(a)
20° 30°
(iii)
metal contact 40°
40°
50°
50°
junction (b)
60°
(c)
(i)
(ii)
60°
70°
70°
80°
80°
(d) 90°
90°
Fig. 20.5. Form of various LED casings with (a) hemispherical, (b) truncated sphere and (c) parabolic geometry. Adapted from [651]. (d) Emission characteristics for rectangular (i), hemispheric (ii) and parabolic (iii) geometry. Adapted from [652] epoxy encapsulation dome lens, transparent LED chip wedge wire bond
mild steel lead frame, solder dipped leads
(a)
lens
cathode post with reflector cup
anode post
flat on side of dome, indicating cathode

+
cathode lead, shorter than anode lead
(b)
heat sink
Fig. 20.6. (a) Standard LED casing (schematic drawing and macrophoto), (b) highpower mounting (schematic drawing and image of Luxeon LED)
transparent active
metal mirror
opaque
(a)
(b)
(c)
(d)
(e)
Fig. 20.7. (a) Standard LED layer sequence with opaque substrate (grey), active layer (checkered ) and transparent top, (b) thick window design with thick top layer (50–70 µm). (c) Transparent substrate (by rebonding, see Fig. 20.8, (d) chip shaping (see also Fig. 20.10). (e) Thinﬁlm LED with metal mirror (black ) and rebonding (see also Fig. 20.11)
ThickWindow Chip Geometry An increase in quantum eﬃciency to about 10–12% can be achieved if the top layer is fabricated with a much larger thickness (Fig. 20.7b) of 50–70 µm instead of a few µm.
20.3 LightEmitting Diodes
535
Transparent Substrate Reﬂection of photons is not so detrimental if they are not lost later due to absorption in the substrate. In Fig. 20.7, the evolution of LED chip design is shown schematically. In Fig. 20.8, the light path is compared for opaque and transparent substrates. The latter provides higher external quantum eﬃciency due to the ‘photon recycling’ effect. Eﬃciencies of 20–25% are possible. In Fig. 20.9, the technological steps are shown to fabricate a GaP LED with an AlGaInP active layer. The active layer is initially grown on GaAs due to latticematch conditions.
Fig. 20.8. Comparison of light path in a LED with (a) opaque and (b) transparent c substrate. Reprinted with permission from [183], 1981 Wiley
GaP window AlGaInP DH AlAs GaAs
substrate
(a)
GaAs
(b)
GaP
(c)
Fig. 20.9. Scheme of fabrication for red high brightness LED: (a) AlGaInP double heterostructure (DH) with GaP window on GaAs substrate (growth with MOCVD). (b) Liftoﬀ using HF etch of sacriﬁcial AlAs layer. (c) Wafer bonding on GaP (transparent for red light)
Nonrectangular Chip Geometry If the chip is made with an inverted structure and mounted on a mirror, a very high external eﬃciency (> 50%) can be achieved. Typical commercial designs are shown in Fig. 20.10.
536
20 ElectricitytoLight Conversion
(a)
(b)
(c)
(d) Fig. 20.10. Optimization of light exit by 3D design of the LED chip, (a) scheme, (b) emission pattern comparison and (c) SEM image of the ATON chip. Reprinted with permission from [653]. (d) Development stages towards the truncated inverted pyramid (Prometheus) chip. The lower row indicates the improvement of photon ﬂux. Adapted from [654]
The increase in quantum eﬃciency allows the devices to run on much higher output power. While initially LEDs delivered power only in the mW regime, now output power in the ∼ 1 W regime is possible (high brightness LEDs). The higher currents made a redesign of the LED mount towards better heat sinks necessary (Fig. 20.6b). While the standard case has a thermal resistance of 220 K/W (chip size (0.25 mm)2 for 0.05–0.1 W and 0.2–2 lm),
20.3 LightEmitting Diodes
537
the highpower case has 15 K/W (chip size (0.5 mm)2 for 0.5–2 W and 10– 100 lm). An epoxyfree technique for encapsulation also enhances the color uniformity and maintains the brightness. ThinFilm LED In the thinﬁlm LED design, as schematically shown in Fig. 20.11a, a metal mirror is evaporated on the LED layers. Subsequently, the metal side is wafer bonded to another metallized substrate and the original substrate is removed. Additionally, the LED surface can be patterned (before bonding) into an (hexagonal) array of (hexagonal) microprism mesas with an insulating (e.g. silicon nitride) layer with openings in order to optimize the current path. The microprisms are optimized to allow eﬃcient reﬂection of light towards the emitting surface. This technology is scalable to large areas without loss in eﬃciency.
(a)
(b)
Fig. 20.11. (a) Scheme of thinﬁlm LED with microprisms. (b) image and luminescence image of thin ﬁlm AlInGaP LED (chip length: 320 µm). Reprinted with permission from [655]
White LEDs There are different possibilities to generate white light with an LED as shown schematically in Fig. 20.12. The highest color gamut and a tunable white point can be achieved by combining a red, a green and a blue LED (Fig. 20.12a). Using a blue LED and a yellow phosphor (Figs. 20.12b and 20.13a,b), a white spectrum can be achieved that is, however, not very close to a blackbody spectrum (Fig. 20.13c). A better color rendering can be obtained with the combination of two phosphors. With an UV LED that is itself invisible (and must be shielded so no UV radiation leaves the LED), phosphors with various colors can be pumped (Fig. 20.12c). The mix of phosphors determines the white point. Using a blueemitting LED based on InGaN material, phosphors (similar to those used in ﬂuorescence lamps) can be pumped. Blue light is converted
538
20 ElectricitytoLight Conversion
into green, yellow or red light such that the resulting total spectrum appears white to the human eye. Also, a broad range of other colors can be designed (color on demand), e.g. pink or particular corporate colors. LumiLeds predicts that its Luxeon LEDs (60 lumen/W, 5 W) will retain upwards of 90% of their light output after 9000 h and 70% through 50. 000 h. Nichia targets 50% after 30 000 h.
(b)
(a)
(c)
Fig. 20.12. Diﬀerent strategies to generate white light with LEDs. (a) Addition of R, G, and B LEDs, (b) blue LED and yellow phosphor, (c) UV LED (invisible) and R, G, and B phosphors. From [654]
(a)
Intensity (arb. units)
(b)
(c)
400
450
500
550
600
650
700
Fig. 20.13. (a) Scheme and (b) image of color conversion Luxeon LED. From [654]. (c) Spectrum (solid line) of white LED with blue LED pumping a yellow phosphor together with eyesensitivity curve V (λ) (dashed line). Adapted from [655]
The color of a white LED depends on the operation conditions. In Fig. 20.14a the intensity vs. dc driving current characteristic of a white LED is shown. In Fig. 20.14b the chromaticity coordinates are shown for various
20.4 Lasers
539
dc currents. In order to avoid this effect, the LED is driven with pulses of a ﬁxed amplitude and a repetition frequency that is high enough to provide a ﬂickerfree image to the human eye, e.g. 100 Hz. The intensity of the LED is modulated via the pulse width, i.e. between 0–10 ms in this case (PWM, pulsewidth modulation).
0.34
IF (mA) 1
0.33
5
0.32
20
y
Luminous intensity (arb. units)
0.35
50
0.31
0
20
(a)
40 60 80 Current (mA)
0.30 0.29
100
(b)
100 0.30
0.31
0.32
0.33
0.34
x
Fig. 20.14. (a) Luminous intensity of white LED (NSCW215) vs. dc forward current. (b) CIE chromaticity coordinates for various dc driving conditions as labeled. Data taken from [656]
Historic Development In Fig. 20.15, the historic development of the LED eﬃciency is shown for various material systems. While the luminosity has increased by a factor of 20 per decade in the last 40 years, the price has decreased by a factor of ten per decade (Fig. 20.16). Currently, there is a need for the development of eﬃcient LEDs in the green spectral range since their luminosity is small compared to devices for the blue and red spectral regions.
20.4 Lasers 20.4.1 Introduction Semiconductor lasers12 [658, 659] contain a zone (mostly called the active layer ) that has gain if suﬃciently pumped and that overlaps with an optical 12 The term ‘laser’ is an acronym for ‘light ampliﬁcation by stimulated emission of radiation’. The ampliﬁcation relies on stimulated emission, theoretically predicted by Einstein in 1917. The laser concept was ﬁrst explored in the microwave wavelength region (1954, MASER using ammonia, Ch.H. Townes, Nobel prize 1964). The ﬁrst optical laser (1958, US patent No. 2,929,922 awarded 1960, A.L. Schawlow, Ch.H. Townes) was the ruby laser developed in 1960 by Th. Maiman.
540
20 ElectricitytoLight Conversion
Fig. 20.15. Historic development of the eﬃciency of semiconductor LEDs. Reproduced from [657] by permission of the MRS Bulletin
Flux (lm) , Cost ($/lm)
103 10
2
10
1
10
0
flux
10
1
10
2
10
3
cost
1970
1980
1990 Year
2000
Fig. 20.16. Historic development of the ﬂux (in lumen) and cost (in $/lm) for semiconductor LEDs. Data from [654]
wave. The wave bounces back and forth in an optical cavity that leads to optical feedback. The part of the wave that exits the semiconductor forms the laser beam. Some of the ﬁrst semiconductor lasers and a mounting design are shown in Fig. 20.18. Generally, two main geometrical laser types, edge emitters (Fig. 20.19a) and surface emitters (Fig. 20.19b), are distinguished. The emission of the edge emitter exits through cleaved {110} side facets13 (≈ 30% reﬂectivity), of which an opposite pair acts as a Fabry–Perot optical cavity. The surface emission is directed along (001), since this is the (standard) growth direction of the heterostructure sequence making up the laser. The mirrors in a verticalcavity surfaceemitting laser (VCSEL) are made from dielectric Bragg mirrors 13
or etched facets in possibly any direction.
20.4 Lasers
541
Fig. 20.17. Luminous performance of various LED materials. Adapted from [657], reprinted by permission of the MRS Bulletin
(a)
(c)
(b)
(d)
Fig. 20.18. Images of the ﬁrst semiconductor lasers, 1962: (a) GaAs laser, Lincoln Laboratories and (b) GaInP laser, N. Holonyak and S.F. Bevacqua, Urbana Champaign. (c) Laser (at the end of gold bond wire) mounted on Peltier heat sink and a TO chip, Universit¨ at Leipzig. (d) Size comparison of an ant with a laser chip (underneath the bond wire)
542
20 ElectricitytoLight Conversion laser light
top contact
insulator
ptype DBR active QW
ptype
laser radiation
ntype
(a)
cleaved facet
ntype DBR
active layer
back contact
ntype substrate
cleaved facet
(b)
laser light
Fig. 20.19. (a) Schematic drawing of edgeemitting semiconductor laser. (b) Schematic drawings of verticalcavity surfaceemitting lasers with top emission (left) and emission through the substrate (right). Black areas are metal contacts
(see Sect. 17.1.4) with typically R > 99.6%. Using antireﬂection coating on one facet, semiconductor lasers can be set up with an external cavity.14 If both facets are antireﬂection coated, feedback is missing and the chip can be used as an optical ampliﬁer (see Sect. 20.5). Most lasers are pndiodes and are then called laser diodes. They rely on the gain of interband transitions and the emission wavelength is determined and (more or less) given by the bandgap of the semiconductor. The cascade laser [660] (Sect. 20.4.16) is a unipolar structure with a superlattice as active layer. Here, the intersubband transitions (mostly in the conduction band but also in the valence band) carry the gain. The emission wavelength depends on the subband separation and lies typically in the far and midinfrared. Extensions to the THz regime and also to shorter wavelengths are possible. A third type of laser is the ‘hothole’ laser (Sect. 20.4.17), typically fabricated with pdoped Ge, which can be viewed as unipolar and functions only in a magnetic ﬁeld; its emission is in the THz regime. 20.4.2 Applications In Fig. 20.20, the revenue in the worldwide diode laser market is shown. The drop after 2000 is due to the burst of the ‘internet bubble’. Nondiode laser (gas, ruby, excimer, . . . ) revenue is currently stable at around 2 billion US$, thus semiconductor lasers account for the largest share of all laser types sold. The following applications rely on semiconductor lasers: – most semiconductor lasers are fabricated for optical communication as senders – optical information storage and retrieval (CD, DVD) with as short of a wavelength as possible, as shown in Fig. 20.21, currently about 400 nm. – pumping of solidstate laser, typically 910 or 940 nm for pumping Nd:YAG 14 Such external cavities can be used for manipulation of the laser properties such as wavelength tuning.
20.4 Lasers
543
Fig. 20.20. Revenue in worldwide diode laser market. Based on numbers from [661]
– laser TV for which eﬃcient red, green and blue lasers will be needed. A mass product can only be developed if cheap laser diodes are available as emitters. – laser pointers, see Fig. 20.22. A red laser pointer simply uses the collimated red emission of a GaAsbased diode. In a green laser pointer, an infrared diode pumps a Nd:YAG or Nd:YVO4 crystal. The emitted beam is then frequency doubled, typically with a KTiOPO4 (KTP) crystal. – medical instruments with a variety of wavelengths. – remote control, position detection, distance measurement. The market for photonic devices is much more dynamic than the electronics market. An example is the rapid change of dominating laser applications. For diode lasers, the most prominent single application moved from telecommunication (77% market share in 2000, 25% in 2003) to optical data storage (17% market share in 2000, 60% in 2003). 20.4.3 Gain Due to current injection,15 a nonequilibrium carrier distribution is created. After fast thermalization processes (phonon scattering), it can mostly described by quasiFermi levels. Suﬃciently strong pumping leads to inversion, i.e. conductionband states are more strongly populated with electrons than valenceband states (Fig. 20.23). In this case, the stimulated emission rate is stronger than the absorption rate (see Sect. 10.2.6). The thermodynamic 15
or due to optical pumping. If electrical contacts are not available, the laser action can be invoked by supplying a highintensity light beam, possibly in a stripelike shape. For optically pumped semiconductor lasers see Sect. 20.4.15.
544
20 ElectricitytoLight Conversion
Fig. 20.21. Evolution of optical data storage technology, ‘CD’: compact disk (laser: 780 nm, pitch: 1.6 µm, capacity: 0.7 GB), ‘DVD’: digital versatile disk (laser: 635– 650 nm, pitch: 0.74 µm, capacity: 4.7 GB for one layer), ‘BD’: ‘Bluray’ disk (laser: 405 nm, pitch: 0.32 µm, capacity: 27 GB for one layer)
(a)
(b)
(c)
(d)
(e)
Fig. 20.22. (a) Scheme of red laser pointer, (b) scheme of green laser pointer. Parts of a green laser pointer: (c) pump laser diode, (d) YVO4 crystal, (e) KTP doubler
20.4 Lasers
E
E
E
Fn
Fn
EC
EC
EC
EV
EV Fp
EV Fp
D(E) (a)
545
D(E) (b)
D(E) (c)
Fig. 20.23. Population (a) in thermodynamic equilibrium T = 0 K, (b) under inversion for T = 0 K, (c) under inversion for T > 0 K. Shaded areas are populated with electrons
laser condition (cf. (10.23)) requires the difference of the quasiFermi levels to be larger than the bandgap. Fn − Fp > Eg
(20.9)
The gain is deﬁned as the (frequencydependent) coeﬃcient g(ω) that describes the light intensity along a path L according to I(L) = I(0) exp (gL) .
(20.10)
The gain spectrum as a function of the photon energy ω is given for nonkconserving recombination by (cf. (10.5) and (10.6)) ω−Eg De (E)Dh (E ′ ) [fe (E)fh (E ′ ) − (1 − fe (E))(1 − fh (E ′ ))] dE , g(ω) = 0
(20.11)
with E ′ = ω−Eg −E. The gain is positive for those photon energies for which light is ampliﬁed and negative for those that are absorbed. In Fig. 20.24a, the electron and hole concentrations are shown for GaAs as a function of the quasiFermi energies. In Fig. 20.24b, the difference of the quasiFermi energies is shown as a function of the carrier density (for neutrality n = p). The gain spectrum is shown in Fig. 20.24c for a twoband model.16 In the case of inversion, the gain is positive for energies between Eg and Fn − Fp . At ω = Fn − Fp , the gain is zero (transparency) and for larger energies negative (positive absorption coeﬃcient). 16 One electron and one hole band are considered; the heavy and light hole bands are taken into account via the mass according to (7.14).
546
20 ElectricitytoLight Conversion
For a given ﬁxed energy, the gain increases with increasing pumping and increasing carrier density n (Fig. 20.24d). For very small density, it is given as g(n → 0) = −α. The gain rises around transparency approximately linearly with the pumping intensity. At transparency carrier density ntr , the gain is zero. Therefore, the relation g(n) can be approximated as (linear gain model) g(n) ≈ α ˆ
n − ntr . ntr
(20.12)
For large carrier density, the gain saturates (at a value similar to α).
(a)
(b)
(c)
(d)
Fig. 20.24. Gain in the twoband model for GaAs. (a) Electron and hole concentrations at T = 300 K as a function of the quasiFermi energies counted relative to the band edges, i.e. Fn − EC and EV − Fp . (b) Diﬀerence of quasiFermi levels as a function of carrier concentration (n = p) for GaAs at two diﬀerent temperatures. (c) Gain spectra according to (20.11) for n = 2 × 1018 and T = 300 K (solid line), increased carrier density n = 2.1 × 1018 and T = 300 K (dashed line), higher temperature n = 2 × 1018 and T = 314 K (dashdotted line) and same diﬀerence of the quasiFermi levels as for the solid line, n = 2.1 × 1018 and T = 314 K (dotted line). (d) Maximum gain (solid line) and gain at a particular energy (dashed line), for photon energy Eg + 26.2 meV for which the gain is maximal for n = 2 × 1018 and T = 300 K, see solid line in part (c)
20.4 Lasers
547
20.4.4 Optical Mode The light wave that is ampliﬁed must be guided in the laser. An optical cavity is needed to provide optical feedback such that the photons travel several times through the gain medium and contribute to ampliﬁcation. We explain the lightwave management for the edge emitter ﬁrst: Vertical mode guiding In the course of the historical development of the semiconductor laser, the most signiﬁcant improvements (reduction of lasing threshold current) have
p GaAs
n n p n p p GaAs GaAs AlGaAs AlGaAs GaAs AlGaAs
E
n
E
n GaAs
(a)
(b) 10
(c)
5
GaAs/AlGaAs homo 4
SHS
jt hr (A/cm2)
10
DHS 103
10
(d)
2
100
150 200 250 Temperature (K)
300
Fig. 20.25. Laser with (a) homojunction, (b) single heterostructure (SHS), (c) double heterostructure (‘DHS’), (d) reduction of threshold current with design progress (‘SHS’: d =2 µm, ‘DHS’: d =0.5 µm). Adapted from [662]
548
20 ElectricitytoLight Conversion
been achieved through the improvement of the overlap of the optical wave with the gain medium, as shown in Fig. 20.25. From homojunctions over the single heterojunction, eventually the double heterostructure (DHS) design could reduce the laser threshold current density to the 1 kA/cm2 level. Evac n
p
p EC EF
EC EF
(a) EF
EV pInP
pInGaAsP
EV nInP
EC EF
(b)
EV EC Fn
Fn
(c)
Fp
Fp EV
Fig. 20.26. Schematic band diagram of a pn double heterostructure (DHS) diode (InP/InGaAsP/InP) (a) before contact of the materials, (b) in thermodynamic equilibrium (zero bias, dashed line is Fermi level EF = const.), (c) with forward bias close to ﬂatband conditions, dashed lines are quasiFermi levels
The band diagram of a double heterostructure is shown in Fig. 20.26 for zero and forward bias. In the DHS, the optical mode is guided by total reﬂection within the lowbandgap center layer, which has a larger index of refraction than the outer, largebandgap layer.17 When the layer thickness is in the range of λ/nr , the form of the optical mode must be determined from the (onedimensional) wave equation (Helmholtz equation) ∂ 2 Ez + ω 2 μ ǫ(z)Ez = 0 . ∂z 2
(20.13)
In Fig. 20.27a, the shape of the optical mode for GaAs/Al0.3 Ga0.7 As DHS with different GaAs thickness is shown. The optical conﬁnement factor Γ is the part of the wave that has geometrical overlap with the gain medium, i.e. is subject to ampliﬁcation. It is 17
A smaller bandgap coincides for many cases with a larger index of refraction.
20.4 Lasers d (μm) 0.2 0.1 0.075
0.5
0
(a)
1.0 AlGaAs/ GaAs
1.0
0.5 0 0.5 Distance (μm)
Optical confineemnt factor
Intensity (scaled)
1.0
549
0.5
x=0.1 AlGaAs/ GaAs 0 0
1.0
0.6 0.3 0.2
(b)
0.5 1.0 1.5 Thickness (μm)
2.0
Fig. 20.27. (a) Optical mode (relative intensity) for various values of the thickness d of the active layer as labeled of a GaAs/Al0.3 Ga0.7 As DHS laser, (b) Optical conﬁnement factor Γ as a function of the thickness of the active layer and the Al concentration x of the barrier as labeled in a GaAs/Alx Ga1−x As DHS laser. Adapted from [658]
shown for GaAs/Alx Ga1−x As DHS with different GaAs thickness and different Al concentration in Fig. 20.27b. The modal gain gmod that is responsible for light ampliﬁcation in the cavity consists of the material gain gmat due to inversion and the optical conﬁnement factor. gmod = Γ gmat .
(20.14)
In order to allow simultaneous optimization of the light mode and the carrier conﬁnement, the separate conﬁnement heterostructure (SCH) has been designed. Here, a single or multiple quantum well of a third material with even smaller bandgap is the active medium (Fig. 20.28a,b,d). A single quantum well has an optical conﬁnement factor of a few per cent only. It offers, however, eﬃcient carrier capture and eﬃcient radiative recombination. An increase in the carrier capture eﬃciency can be achieved using a graded index in the barrier (GRINSCH, Fig. 20.28c). The thin waveguiding layer leads to large divergence of the laser beam along the vertical direction, typically about 90◦ . The strong conﬁnement of light also limits the maximum achievable output power due to catastrophic optical damage (COD). Several ideas have been realized to overcome this problem and achieve much smaller divergence of about 18◦ . The waveguide can be designed to be very thick (large optical cavity, LOC) that leads to an increase of threshold. Other schemes are insertion of a lowindex layer into the conﬁnement layer, insertion of a highindex layer into the cladding layer or the use of highindex quarterwavelength reﬂecting layers [663]. Lateral Mode Guiding Lateral waveguiding can be achieved with gain guiding and index guiding (or a mixture of the two). In the gainguiding scheme (Fig. 20.29), the current
MQWSCH
nAl0.3Ga0.7As
(i)
pAl0.1Ga0.9As pGaAs nAl0.1Ga0.9As
EV
+
(i)
pAl0.3Ga0.7As
EC
+
SCH
n GaAs substrate
20 ElectricitytoLight Conversion
p GaAs
550
Eg
EC
(ii)
(ii)
n
EV
GRINSCH
EC
(iii) E2
(a)
(iii)
EV
(b) (iv)
Fig. 20.28. (a) Various geometries of the active layer of a DHS laser with quantum wells as active medium, (i) single QW (separate conﬁnement heterostructure, SCH), (ii) multiple QW SCH, and (c) GRINSCH (gradedindex SCH) structure. (b) Layer sequence for a separate conﬁnement heterostructure laser
path that is deﬁned by the stripe contact and the current spreading underneath it, deﬁnes the gain region and therefore the volume of ampliﬁcation that guides the optical wave. Since a high carrier density reduces the index of refraction, a competing antiguiding effect can occur. For index guiding, the lateral light conﬁnement is caused by a lateral increase of the index of refraction. This index modulation can be achieved by using a mesalike contact stripe (Fig. 20.30a). A shallow mesa reaches down into the upper cladding,
tungsten wire protons
metal
oxide + p GaAs pAlGaAs n or pGaAs nAlGaAs substrate (GaAs)
protons
p+GaAs pAlGaAs n or pGaAs
S
light
d L
metal
nAlGaAs substrate metal
(a)
(b)
Fig. 20.29. Scheme of gainguided lasers with stripe contact: (a) oxide stripe, (b) proton implanted with shadow mask from tungsten wire (∼ 10 µm). Adapted from [664]
20.4 Lasers
551
a deep mesa reaches down into or through the active layer. Possible problems with surface recombination can be avoided by regrowth of the structure (Fig. 20.30b) with a widebandgap material (compared to the active layer). Optimization of regrowth is targeted to achieve a welldeﬁned surface for subsequent contact processing. A lateral pndiode can be incorporated that avoids current spreading in the upper part of the structure.
pInP nInP
p+InGaAsP p+InGaAsP dielectric InGaAsP InGaAsP active layer nInP
nInP substrate
pInP
nIn
P
pIn
P InGaAsP active region
nInP substrate
(a)
(b)
Fig. 20.30. Schematic cross section of indexguided lasers: (a) shallow ridge, (b) deep etch and regrowth. Black areas are metal contacts
Depending on the width of the lateral mode, it can be monomode or multimode (Fig. 20.31a). For laterally monomode lasers, the stripe width may only be a few µm. In particular for such lasers, the current spreading must be controlled. Problems can arise for wide stripe widths due to current ﬁlamentation and inhomogeneous laser emission from the facet. Since the optical mode is typically more conﬁned in the growth direction than in the lateral direction, the far ﬁeld is asymmetric (Fig. 20.31c). The vertical axis has the higher divergence and is called the fast axis. The lateral axis is called the slow axis. The asymmetric beam shape is detrimental when the laser needs to be coupled into an optical ﬁber or a symmetric beam proﬁle is needed for subsequent optics. The beam can be made symmetric using special optic components such as anamorphic prisms (Fig. 20.31d) and gradedindex lenses. The beam from a laterally monomode laser is diffraction limited and can therefore generally be refocused eﬃciently (beam quality M 2 1). Longitudinal Modes The spectral positions of the laser modes for a cavity with length L is given by the condition (cf. (17.34)) L=
mλ , 2nr (λ)
(20.15)
where m is a natural number and n(λ) is the dispersion of the index of refraction. The distance of neighboring modes is given by (for large m)
552
20 ElectricitytoLight Conversion S=10μm
20μm
20μm
30μm
30μm
50μm
(a)
10μm
(b)
0.1rad
(c)
(d) Fig. 20.31. Lateral near ﬁeld (a) and far ﬁeld (b) of lasers with various width S of the injection stripe as labeled. Adapted from [665]. (c) Typical asymmetric far ﬁeld of an edge emitter. Adapted from [183]. (d) Correction of asymmetric far ﬁeld with a pair of anamorphic prisms
Δλ =
λ2
2nr L 1 −
λ dnr nr dλ
.
(20.16)
The dispersion dnr /dλ can sometimes be neglected. The facets of edgeemitting lasers are typically cleaved. Cleaving bears the danger of mechanical breakage and tends to have poor reproducibility, low yield and therefore high cost. Etched facets are another possibility to form the cavity mirror. The etch process, typically reactive ion dry etching, must yield suﬃciently smooth surfaces to avoid scattering losses. A highly eﬃcient distributed Bragg mirror (see Sect. 17.1.4) with only a few periods can be created by using the large index contrast between the semiconductor and air. As shown in Fig. 20.32, slabs can be etched that make a Bragg mirror with the air gaps [666]. In this way, very short longitudinal cavities can be made (≈ 10 µm). 20.4.5 Loss Mechanisms While the light travels through the cavity, it is not only ampliﬁed but it also suffers losses. The internal loss αi and the mirror loss αm contribute to the
20.4 Lasers
553
(a)
5 μm
(b)
(c)
5 μm
Fig. 20.32. SEM image of (a) an InP microlaser with thirdorder Bragg mirrors, (b) magniﬁed view of the front facet with three slabs, (c) a 12µm long microlaser with ﬁve thirdorder mirrors on the rear side and three ﬁrstorder mirrors on the front side with top contact. From [667]; part (b) reprinted with permission c from [666], 2001 AIP
total loss αtot αtot = αi + αm .
(20.17)
The internal loss is due to absorption in the cladding, scattering at waveguide inhomogeneities and possibly other processes. It can be written as αi = α0 Γ + αg (1 − Γ ) ,
(20.18)
where α0 is the loss coeﬃcient in the active medium and αg is the loss coefﬁcient outside the active medium. The mirror loss is due to the incomplete reﬂection of the optical wave at the laser facets. This condition is necessary, however, to observe a laser beam outside the cavity. R1 and R2 are the reﬂectivities of the two facets, respectively. An ascleaved facet has a reﬂectivity of about 30% (cf. (20.7)). Using dielectric layers on the facets, the reﬂectivity can be increased (high reﬂection, HRcoating) or decreased (antireﬂection, ARcoating). One roundtrip through the cavity of length L has the length 2L. The intensity loss due to reﬂection at the facets is expressed via exp (−2αm L) = R1 R2
1 1 . (20.19) ln αm = 2L R1 R2 If both mirrors have the same reﬂectivity R, we have αm = −L−1 ln R. For R = 0.3 a 1mm cavity has a loss of 12 cm−1 . For the internal loss a typical value is 10 cm−1 , very good waveguides go down to 1–2 cm−1 . Lasing is only possible if the gain overcomes all losses (at least for one wavelength), i.e. gmod = gmat Γ ≥ αtot .
(20.20)
554
20 ElectricitytoLight Conversion
20.4.6 Threshold When the laser reaches threshold, the (material) gain is pinned at the threshold value gthr =
αi + αm . Γ
(20.21)
Since g ∝ n, the carrier density is also pinned at its threshold value and does not increase further with increasing injection current. Instead, additional carriers are quickly converted into photons by stimulated emission. The threshold carrier density is (using the linear gain model, cf. (20.12)) nthr = ntr +
αi + αm . α ˆΓ
(20.22)
For an active layer of thickness d, the threshold current density is ednthr jthr ∼ , = τ (nthr )
(20.23)
where τe (nthr ) is the minority carrier lifetime at the threshold carrier density: τ (nthr ) =
1 A + Bnthr + Cn2thr
.
Using (20.22), we can write (for R = R1 = R2 )
ed 1 jthr = jtr + αi − ln R , τα ˆΓ L
(20.24)
(20.25)
where the transparency current density is jtr = edntr /τ . Thus, the plot of jthr vs. 1/L (or the optical loss) should be linear and can be extrapolated towards the transparency current density (see Fig. 20.33a). Any additional increase of the current j leads to stimulated emission with the rate rst = edvg gthr Nph ,
(20.26)
where vg is the group velocity (mostly c0 /nr ) and Nph is the photon density (per length) in the cavity. The photon density increases linearly beyond the threshold Nph =
1 (j − jthr ) . dvg gthr
(20.27)
The photon lifetime 1 = vg (αi + αm ) = vg Γ gthr τph
(20.28)
20.4 Lasers
555
(b)
(a)
Fig. 20.33. (a) Threshold current density for (threefold InGaAs/GaAs QD stack) laser (λ = 1150 nm) at 10◦ C with diﬀerent cavity length vs. the optical loss (∝ 1/L). The extrapolated transparency current density is 21.5 ± 0.9 A/cm2 . (b) Inverse external quantum eﬃciency for the L = 1 mm QD laser vs. cavity length. The internal quantum eﬃciency determined from the plot is 91% and the internal loss is 1.4 cm−1
is introduced that describes the loss rate of photons. vg αm describes the escape rate of photons from the cavity into the laser beam(s). Therefore, Nph =
τph Γ (j − jthr ) . ed
(20.29)
Since the threshold depends on the carrier density, it is advantageous to reduce the active volume further and further. In this way, the same amount of injected carriers creates a larger carrier density. Figure 20.34 shows the historic development of laser threshold due to design improvements. 20.4.7 Spontaneous Emission Factor The spontaneous emission factor β is the fraction of spontaneous emission (emitted into all angles) that is emitted into laser modes. For Fabry–Perot lasers, β is typically in the order of 104 –105 . The design of a microcavity can increase β drastically by several orders of magnitude to ≈ 0.1 [668] or above and thus reduce the threshold current. The photon number as a function of the pump current can be calculated from the laser rate equations and is depicted in Fig. 20.35. For β = 1, all emitted power goes into the laser mode regardless of whether emission is spontaneous or stimulated. The deﬁnition of threshold in such ‘nonclassical’ lasers with large β is discussed in detail in [669]. 20.4.8 Output Power The output power is given by the product of photon energy, the photon density in the cavity, the effective mode volume and the escape rate:
20 ElectricitytoLight Conversion
Threshold current density (A/cm2)
556
10
4
10
3
10
2
DH
SCHQW
strained QW
10
QD
1
1960
1970
1980 1990 Year
2000
2010
Fig. 20.34. Historic development of threshold current density (at room temperature, extrapolated for inﬁnite cavity length and injection stripe width) for various laser designs, ‘DH’: double heterostructure, ‘SCH–QW’: separate conﬁnement heterostructure with quantum wells. ‘QD’: quantum dots. Dashed lines are guides to the eye 106 105
Photon number
104 103 102 101
=1
100 101
0.5
101 102
3
10 104
10
5
102 103 10 9 8 7 6 5 4 3 2 1 10 10 10 10 10 10 10 10 10 10 Pump current (A)
Fig. 20.35. Photon number vs. pump current for a model laser. Adapted from [670]
Pout = ωNph
Lwd vg αm . Γ
(20.30)
Thus, it is given by Pout = ωvg αm
τph ω αm Lw (j − jthr ) = (I − Ithr ) . e e αm + αi
(20.31)
To this equation, the factor ηint must be added. The internal quantum efﬁciency describes the eﬃciency of the conversion of electron–hole pairs into photons: ηint =
Bn2 + vg gthr Nph . An + Bn2 + Cn3 + vg gthr Nph
(20.32)
20.4 Lasers
557
All in all, now (see Fig. 20.36a) Pout =
ω αm ηint (I − Ithr ) . e αm + αi
(20.33)
The differential (or slope) quantum eﬃciency, also called the external quantum eﬃciency ηext , is the slope of the Pout curve vs. the current in the lasing regime. It is given by ηext =
αm dPout /dI . = ηint ω/e αm + αi
The external quantum eﬃciency can also be written as
1 αi 1 1 = [1 − 2αi L ln (R1 R2 )] . 1+ = ηext ηint αm ηint
(20.34)
(20.35)
−1 is plotted for similar lasers with different cavity length (see Therefore, if ηext Fig. 20.33b), a straight line should arise from which the internal quantum eﬃciency (extrapolation to L → 0) and the internal loss (∝ slope) can be determined experimentally. The threshold current for a given laser is determined from the P –I characteristic via extrapolation of the linear regime as shown in Fig. 20.36a. Record values for the threshold current density are often given for the limit L → ∞. Due to current spreading, the threshold current density also depends on the width of the injection stripe. Record low thresholds are therefore often given for the limit w → ∞. The total quantum eﬃciency is given by
ηtot =
Pout /I . ω/e
(20.36)
This quantity is shown in Fig. 20.36b for a laser as a function of the current. For a linear P –I lasing characteristic, the total quantum eﬃciency converges towards the external quantum eﬃciency for high currents because the low quantum eﬃciency subthreshold regime no longer plays any role. Another important ﬁgure of merit is the wallplug eﬃciency ηw that describes the power conversion: ηw =
Pout . UI
(20.37)
Additionally to the current balance discussed so far, typically a leakage current exists that ﬂows without contributing to recombination or lasing. Carriers not captured into or escaping from the active layers can contribute to this current. The present (2004) record for wallplug eﬃciency of highpower laser diodes is 65%, employing careful control of band alignment (graded
558
20 ElectricitytoLight Conversion
Emission power (arb. units)
InGaAs/ GaAs
It hr 0
(a)
0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 Current (A)
(b)
600
70
500
60 50
Power (W)
400
40 300 30 200
20
100 =940nm 0 0
100
200
300 400 Current (A)
500
Wall plug efficiency (%)
Fig. 20.36. (a) Typical P –I characteristic of a semiconductor laser. Adapted from [183]. (b) Output power and total quantum eﬃciency of a quantum dot laser (3 stacks of InGaAs/GaAs QDs, L = 2 mm, w = 200 µm, λ = 1100 nm, T = 293 K) vs. injection current
10 0 600
Fig. 20.37. Output power (left scale) and wallplug eﬃciency (right scale) vs. driving current for a 10 mm laser bar. Adapted from [673]
junctions, avoiding voltage barriers), optical losses, Joule heating, spontaneous emission and carrier leakage. It seems possible to achieve ηw of 80%. The P –I characteristic is not linear to arbitrary high currents. Generally, the output power will saturate or even decrease for increasing current. These effects can be due to increasing leakage current, increasing internal loss at high current or temperature effects, e.g. an increase of threshold with increasing temperature (see Sect. 20.4.9) and therefore a reduction of total eﬃciency. All nonradiative losses will eventually show up as heat in the laser that must be managed with a heat sink. A radical effect is catastrophical optical damage (COD) at which the laser facet is irreversible (partially) destructed. Antioxidation or protective layers can increase the damage threshold to > 20 MW/cm2 . The record power from a single edge emitter is ∼ 12 W (200 µm stripe width). For a lateral monomode laser, cw power of about 1.2 W has been reached from a 1480nm
20.4 Lasers
559
InGaAsP/InP double quantumwell lasers with 3–5 µm stripes and 3 mm cavity length [671]. About 500 mW can be coupled into a singlemode ﬁber [672]. An array of edge emitters is called a laser bar. The current power record is 509 W (at 540 A) for a 10 mm wide bar (Fig. 20.37). 20.4.9 Temperature Dependence The threshold of a laser typically increases with increasing temperature as shown in Fig. 20.38a. Empirically, in the vicinity of a temperature T1 the threshold follows an exponential law (see Fig. 20.38b)
115°C
2
1
0 0 (a)
95°C
Threshold current (A/cm2)
Power (mW)
GaAs/ 25°C AlGaAs
100 200 Current (mA)
ln( jth r/ (Acm2) )
5.5
300 200
100 80 60
T0=110K
40 30 0
20
(b)
40 60 80 100 120 Temperature (K)
InGaAs/ GaAs
5.0 4.5 4.0 3.5 3.0 50
(c)
100
150 200 250 Temperature (K)
300
Fig. 20.38. (a) P –I characteristic (cw output power per mirror facet) of stripeburied heterostructure laser at various temperatures of the heat sink between 25 ◦ C and 115 ◦ C in steps of 10 K. (b) Threshold current (in logarithmic scale) of this laser as a function of heatsink temperature and exponential ﬁt (dashed line) with T0 = 110 K. Parts (a) and (b) adapted from [674]. (c) Temperature dependence of the threshold current density of a quantum dot laser (3 stacks of InGaAs/GaAs QDs, λ = 1150 nm) with T0 (solid lines are ﬁts) given in the ﬁgure
560
20 ElectricitytoLight Conversion
jthr (T ) = jthr (T1 ) exp
T − T1 T0
∝ exp
T T0
,
(20.38)
with T0 being the socalled characteristic temperature.18 It is the inverse logarithmic slope, T0−1 = d ln jthr /dT . T0 summarizes the temperaturedependent loss and the carrier redistribution in kspace due to the change of the Fermi distribution with temperature. With increasing temperature, populated states below the quasiFermi level become unpopulated and nonlasing states become populated. Therefore, the gain decreases with increasing temperature. This redistribution must be compensated by an increase of the quasiFermi energy, i.e. stronger pumping. This effect is present for (even ideal) bulk, quantum well and quantum wire lasers. Only for quantum dots with a δlike density of states is the change of Fermi distribution irrelevant as long as excited states are energetically well separated from the (lasing) ground state. In Fig. 20.38c, the threshold of a quantum dot laser [675] is indeed temperature independent (T0 = ∞) as long as excited states are not thermally populated (for T < 170 K for the present laser). 20.4.10 Mode Spectrum In Fig. 20.39a, the mode spectrum of a typical edgeemitting laser is shown. Below threshold, the ampliﬁed spontaneous emission (ASE) spectrum exhibits a comblike structure due to the Fabry–Perot modes. Above threshold, some modes grow much faster than others, possibly resulting in single longitudinal mode operation at high injection. The relative strength of the strongest side mode is expressed through the sidemode suppression ratio (SSR) in dB
Imm , (20.39) SSR = 10 log Ism where Imm (Ism ) is the intensity of the maximum (strongest side) mode in the lasing spectrum. 20.4.11 Longitudinal SingleMode Lasers In order to achieve a high SSR or single longitudinal mode lasing, the feedback must offer a higher wavelength selectivity than a simple mirror. A preferential feedback for certain modes can be obtained using a periodic dielectric structure that ‘ﬁts’ to a particular wavelength, similar to a Bragg mirror. The periodic modulation of the refractive index can be made within the cavity (distributed feedback, DFB, Fig. 20.40a) or at the mirror (distributed reﬂection, DBR, Fig. 20.40b). In this way, monochromatic lasers with SSR ≫ 30 dB are possible (Fig. 20.39b). ◦
18 Since T0 has the dimension of a temperature diﬀerence, it can be expressed in C. For the sake of unambiguity it should be given, however, in K.
20.4 Lasers
561
(a)
0.96 Ith
0.59 Ith
0.45 Ith
Laser emission (dB)
Amplified spontaneous emission (arb. units)
1.11 Ith
1.44 1.46 1.48 1.50 1.52 1.54 Energy (eV) (b)
Wavelength (nm)
Fig. 20.39. (a) Mode spectra of a Fabry–Perot laser, under, at and above threshold (Ithr = 13.5 mA). Adapted from [388]. (b) Mode spectra of a cw DFB InGaAs/InP laser with 2 mm cavity length at various currents of 200, 400, . . . , 1400 mA (Ithr = 65 mA), SSR>40 dB at T = 293 K. Adapted from [676], reproduced with permission from SPIE DBR grating
pump region
DBR grating
p
p DFB grating active medium
(a)
n
(b)
n
Fig. 20.40. Schematic drawing of (a) DFB (distributed feedback) and (b) DBR (distributed Bragg reﬂection) lasers. The active medium is schematically shown as a triple quantum well, the waveguide is shown as a grey area
It is possible to couple several hundred mW optical power of a laterally and spectrally monomode laser into a monomode optical ﬁber [677] (Fig. 20.41).
562
20 ElectricitytoLight Conversion 0.8
Power (W)
0.6 0.3 facet
0.4
0.2 fiber
0.2
0.1 0 0
(a)
0.5 1.0 Current (A)
1.5
Coupling efficiency
0.4
0
(b)
Fig. 20.41. (a) Output power of an InGaAsP/InP cw singlemode DFB laser at 1427 nm with 2 mm cavity length from the facet and coupled to a singlemode ﬁber vs. driving current (T = 293 K). The dashed line represents the coupling eﬃciency to the ﬁber (right scale). Adapted from [677]. (b) Package with pigtail of ﬁber coupled 1550 nm DFB laser with 40 mW output power in the ﬁber. From [678]
20.4.12 Tunability The tunability of the emission wavelength [679] is important for several applications such as wavelength division multiplexing19 and spectroscopy. The simplest possibility to tune a laser is to vary its temperature and thus its bandgap. This method is particularly used for lead salt lasers in the midinfrared region,20 as shown in Fig. 20.42. For monomode lasers, mode hopping, i.e. the discontinuous shift of lasing wavelength (or gain maximum) from one mode to the next, poses a problem for continuous tuning, as shown in Fig. 20.43. The continuous shift of emission wavelength is due to the temperature dependence of the index of refraction and subsequently the longitudinal modes. The index of refraction increases with increasing temperature at typically ∼ 3 × 10−4 K−1 . Generally, a redshift is the consequence. Another possibility to vary the index of refraction (and thus the optical path length) is a variation of the carrier density. The coeﬃcient dnr /dn is about −10−20 cm3 . In a twosection laser, separate regions (with separately controlled currents) for gain and tuning are present. The regions are separated with deepetched trenches to avoid crosstalk. The tuning range is limited to about 10 nm. For a modehopping free tuning, the control of the phase in the cavity is important and requires an additional section for the phase control. Such a threesection laser has separate regions (and current control) for the reﬂection, phase and ampliﬁcation (or gain) region. 19
In order to make better use of the high bandwidth of the optical ﬁber several information channels with closely lying wavelengths are transmitted. 20 Note the anomalous positive coeﬃcient dEg /dT as discussed in Sect. 6.10.
nPb0. 88Sn0. 12Te:Bi 0.75 μm nPb0. 782Sn0. 218Te:Bi 1.5 μm MgF2 mask
20
20
15
15
10
10
5
5
pPbTe:Tl
(a) Au
563
jth r(kA/cm2)
In
Wavelength (μm)
20.4 Lasers
PbTe/PbSnTe
(b)
0 0
50 100 Temperature (K)
0
Fig. 20.42. (a) Schematic drawing of PbTe lead salt laser. (b) Tuning characteristics of such laser: Emission wavelength (left scale, ﬁlled circles: emission wavelength at cw threshold, empty circles: emission maximum under pulsed operation) and cw threshold current density (right scale) as a function of the heatsink temperature. Symbols are experimental data, dashed lines are guides to the eye. Adapted from [680]
Fig. 20.43. Wavelength as a function of temperature (with mode hopping) for a GaAsbased DFB laser
Using sampled gratings, the tuning range can be strongly increased to about 100 nm. A sampled grating is a nonperiodic lattice that has several (∼ 10) reﬂection peaks. The laser structure has four sections (Fig. 20.44) with two mirrors that have slightly different sampled gratings. Via the carrier densities in the two mirror sections, different maxima can be brought to overlap (Vernier effect) and the position of the selected maximum can be tuned over a wide spectral range.
564
20 ElectricitytoLight Conversion
Power Reflectivity
0.3 R 1 R2 0.2
0.1
0
(a)
(b)
1.52
1.54 1.56 Wavelength (μm)
1.58
Fig. 20.44. (a) Schematic representation of SGDBR (sampledgrating DBR) laser c with four sections. Reprinted from [681] with permission, 1999 IEEE. (b) Reﬂectivity of two sampled gratings DBR mirrors (R1 : Solid line, R2 : dashed line)
(a)
(b)
Fig. 20.45. (a) Tuning curves of two sampled gratings DBR mirrors for the front and back mirror current. (b) 27 wavelength channels (1531.12 to 1551.72 nm) with c a channel separation of 1 nm. Reprinted from [682] with permission, 1999 IEEE
20.4.13 Modulation For transmission of information, the laser intensity must be modulated. This can be accomplished by direct modulation, i.e. modulation of the injection current, or external modulators, e.g. using, e.g., the voltageinduced shift of the absorption spectrum due to QCSE (see Sect. 12.1.2). For direct modulation, small and largesignal modulation are distinguished. LargeSignal Modulation If a current pulse is fed to the laser, the laser radiation is emitted with a short time delay, the socalled turnon delay (TOD) time. This time is needed to build up the carrier density for inversion. The time dependence of the density is (neglecting the density dependence of the lifetime)
Iτ t n(t) = 1 − exp − . (20.40) eAd τ The TOD time to reach the threshold density (using (20.23)) is
I τTOD = τ ln . I − Ithr
(20.41)
20.4 Lasers
565
We note that τTOD > 0 for I > Ithr . Such a dependence is found experimentally (Fig. 20.46). The turnon delay time decreases with increasing pump current but typically is at least 1 ns. In order to circumvent this limitation for more than about 1 GHz pulse repetition rate, the laser is biased slightly below threshold. 10 8
I / (IIthr)
6 4 3
NA (cm ) 2.0 1017 17 6.5 10 18 2.5 10 18 9.0 10 19 2.7 10
2
1
0
2
4 6 Delay time (ns)
8
10
Fig. 20.46. Variation of turnon delay time with the injected current for a laser at room temperature. Adapted from [683]
In Fig. 20.47a, the response (light emission) of a LED to a short current pulse is shown schematically. The monotonously decreasing transient (that is more or less exponential) corresponds to the carrier recombination dynamics. When a laser is excited with a steep (long) current pulse, the response exhibits socalled relaxation oscillations (RO) before the steadystate (cw) intensity level is reached (Fig. 20.47b). In the laser, ﬁrst the carrier density is built up. It surpasses the threshold density that leads to a buildup of the photon density. The laser pulse depletes the carrier density faster below threshold than the current can supply further (a)
(b)
10ns
1ns
Fig. 20.47. Schematic response of (a) LED to current pulse and (b) of laser to current step
566
20 ElectricitytoLight Conversion
carriers. Therefore, the laser intensity drops below the cw level. From the coupled rate equations for the electron and photon densities n and Nph , the relaxation oscillations have a frequency of
1/2 1 vg g ′ S0 fRO = , (20.42) 2π τph where g ′ is the differential gain g ′ = dg/dn (g(n) = g0 + g ′ (n − n0 )) and S0 is the photon density per volume that is proportional to the laser intensity. 1/2 The dependence fRO ∝ S0 is also found experimentally (Fig. 20.48). 20 f3dB
Frequency (GHz)
15
10 fRO 5
0 0
1
2 3 P1/ 2 (mW 1/ 2)
4
5
Fig. 20.48. Dependence of smallsignal 3 dB cutoﬀ frequency f3dB (ﬁlled symbols) and relaxation oscillation frequency fRO (empty symbols) on the square root of the output power P for a DFBlaser. Adapted from [684]
For digital data transmission, the laser is driven with pulse sequences. The response to a random bit pattern is called an ‘eye pattern’ and is shown in Fig. 20.49. The pattern consists of traces of the type shown in Fig. 20.47b. A clear distinction with welldeﬁned trigger thresholds between ‘on’ and ‘off’states can only be made if the eye formed by the overlay of all possible traces remains open. From the eye patterns in Fig. 20.49, it can be seen that the RO overshoot can be suppressed by driving the laser with a dc offset current well above threshold. SmallSignal Modulation In smallsignal modulation, the injection current I is varied periodically by a small amount δI with δI ≪ I in the lasing regime. The current modulation leads to a corresponding variation of the output intensity. The frequency response is limited by the differential gain and the gain compression coeﬃcient
20.4 Lasers
567
(a)
(b) 100ns Fig. 20.49. Eye pattern of a singlemode VCSEL in response to a 10 Gb/s random bit pattern. The patterns are measured (a) with an oﬀset current well above threshold and (b) with an oﬀset current above but close to threshold. Adapted from [685], c reprinted with permission, 2002 IEEE
ǫ. The latter describes the saturation of gain with increasing photon density S0 according to g(n) = g0 +
g ′ (n − n0 ) . 1 + ǫS0
(20.43)
The frequency response shifts to higher frequency with increasing laser power as shown in Fig. 20.50b. α factor Another important quantity is the α factor, also called the linewidth enhancement factor [686, 687]. Due to the coupling of amplitude and phase ﬂuctuations in the laser, the linewidth Δf is larger than expected. Δf =
ωvg Rspont ln R (1 + α2 ) . 8πPout L
(20.44)
The linewidth enhancement is described via (1 + α2 ) with α=
dnr /dn 4π dnr /dn =− , dκ/dn λ g′
(20.45)
20 ElectricitytoLight Conversion Frequency response (dB)
568
12 9 6 3 0 3 6 9 12
5mW
3
10
6 9 12 Frequency (GHz)
15
20
15
Fig. 20.50. Frequency response of a DFBlaser for various output powers as labeled. Adapted from [684]
where κ denotes the imaginary part of the index of refraction (n∗ = nr +iκ). Typical values for α are between 1 and 10. The linewidth is inversely proportional to the output power (Fig. 20.51). T= 273K
Linewidth f (MHz)
200
150
100
195K
50 77K 0 0
0.5
1.0 1.5 1 1/Pout (mW )
2.0
2.5
Fig. 20.51. Linewidth Δf of a cw GaAs/AlGaAs semiconductor laser at various −1 temperatures as a function of the inverse output power Pout . At room temperature α ≈ 5. Adapted from [688]
20.4.14 Surfaceemitting Lasers Surfaceemitting lasers emit their beam normal to the surface. They can be fabricated from horizontal (edge) emitters by reﬂecting the beam with a suitable mirror into the surface direction. This technology requires tilted facets or microoptical components but allows for high power per area. In
20.4 Lasers
569
Fig. 20.52, a schematic cross section of a horizontalcavity surfaceemitting laser (HCSEL) and the light emission from an array of 220 such lasers are shown. The laser contains a 45◦ mirror that steers the light through the substrate and a Bragg mirror to provide the cavity mirror. The facet can also be fabricated such that the emission is to the top surface (Fig. 20.53). Another possibility to couple the beam out of a horizontal cavity is a surface grating. Now, surfaceemitting lasers with verticalcavity (VCSEL), as shown in Fig. 20.19b, will be discussed. A detailed treatment can be found in [692]. VCSELs are of increasing importance after many issues regarding their technology and fabrication have been solved. VCSEL fabrication is essentially a planar technology and VCSELs can be fabricated as arrays (Fig. 20.55). pmetal SiO2 active medium
SiO2
pAlGaAs nAlGaAs
DBR GaAs substrate AR
(a)
nmetal
(b)
Fig. 20.52. (a) Principle of a surfaceemitting laser. Light generated in the active region is internally reﬂected by the 45◦ angled mirror and directed through the substrate; ‘AR’: antireﬂection coating, ‘DBR’: epitaxial Bragg mirror. (b) Light emission from a 10 × 22 surfaceemitting diode array. The light emission appears as stripes due to the broad beam divergence in the vertical direction. Part (b) reprinted with permission from [689]
laser ridge 45° mirror
(a)
(b)
(c)
Fig. 20.53. (a) Horizontal Fabry–Perot cavity InPbased laser with 1310 nm emission length and 10 mW output power for modulation at 2.5 GB/s. The right facet is formed as DBR, emission is to the left. The trapezoid area in the center bottom of the image is the bond pad for the top contact. (b) Horizontalcavity surfaceemitting laser. Compared to (a), the right facet is replaced with a 45◦ mirror, leading to surface emission. (c) Schematic drawing of the tilted facet. Parts (a) and (b) from [690]
570
20 ElectricitytoLight Conversion
An onwafer test of their properties is possible. They offer a symmetrical (or possibly a controlled asymmetrical) beam proﬁle (Fig. 20.54) with possible polarization control or ﬁxation.
Fig. 20.54. Inplane near ﬁeld of a VCSEL with 6 µm oxide aperture at various currents, (a) 3.0 mA, (b), 6.2 mA, (c) 14.7 mA, (d) 18 mA
(a)
(b)
Fig. 20.55. (a), (b) VCSEL arrays. Part (a) reprinted from [693] with permission, part (b) reprinted from [694] with permission
The cavity is formed by two highly reﬂecting Bragg mirrors with a distance of λ/2 or 3λ/2 forming a microcavity (see Sect. 17.1.6). A high index contrast can be obtained from GaAs/AlAs Bragg mirrors in which the AlAs layers have been selectively oxidized in a hot moist atmosphere. Pure semiconductor Bragg mirrors suffer typically from small index contrast and require many pairs. This poses a problem, e.g. for InPbased VCSELs. In Fig. 20.56, the distribution of light intensity along a 3λ/2 cavity is shown. In the stop band of the mirrors, there is only one optical mode, the cavity mode, that can propagate along the vertical (z) direction. The current path through the active layer can be deﬁned with an oxide aperture. This aperture is fabricated by selective oxidation of an AlAs layer, leaving a circular opening in the center of the VCSEL pillar as shown in
20.4 Lasers
571
Fig. 20.56. Simulation of the longitudinal distribution of the optical ﬁeld in a VCSEL structure. The active medium are ﬁve quantum wells in the center. Reproduced from [691] by permission from the MRS Bulletin
(a)
(b)
Fig. 20.57. (a) Schematic cross section of VCSEL with oxide aperture, (b) TEM image of cross section. Reproduced from [691] by permission from the MRS Bulletin
Fig. 20.57. The current can be injected through the mirrors if they are doped. Alternatively, the current can be directly fed to the active layer by socalled intracavity contacts. The emission wavelength of a VCSEL can be shifted via a variation of temperature or pump power. Tuning of the VCSEL emission can also be accomplished by leaving an air gap between the cavity and the upper mirror [695]. Applying a voltage to the lever arm with the top mirror, the width of the air gap can be varied. This variation leads to a shift of the cavity mode and therefore of the laser emission wavelength. A VCSEL with air gap and particularly a high contrast Bragg mirror is achieved with InP/air as shown in Fig. 20.59. 20.4.15 Optically Pumped Semiconductor Lasers An easy way to pump semiconductor lasers is optical pumping. This technique is similar to diodepumped solidstate lasers (DPSS). A (semiconductor) pump diode illuminates a suitable semiconductor structure (Fig. 20.60). The resonator is built between the bottom Bragg mirror of the semiconductor and the output coupler. The semiconductor structure contains suitable
572
20 ElectricitytoLight Conversion
(b)
(a)
(c) Fig. 20.58. (a) Schematic setup and (b) SEM image of VCSEL with air gap between active layer and top Bragg mirror, (c) spectra for diﬀerent tuning conditions (width of air gap). From [696].
Fig. 20.59. (a) VCSEL with air gap and (b) Bragg mirror with high dielectric c contrast InP/air interfaces. Reprinted with permission from [697], 2002 IEEE
absorption layers (barriers) that absorb the pump light and quantum wells that emit laser radiation. This radiation is intracavity frequency doubled. In order to reach, e.g., a 488nm output laser beam, a standard 808nm pump diode is employed. The InGaAs/GaAs quantum wells are designed to emit at 976 nm. Other design wavelengths of the quantum wells allow for other output wavelengths. This technology allows compact lasers with little heat dissipation [698]. The optically pumped semiconductor laser (OPSL) is also known as a semiconductor disc laser.
20.4 Lasers
573
pump laser
laser beam intracavity SHG crystal
(a)
resonator
heat sink
hemispheric output coupler
semiconductor
focusing optics
(b)
Fig. 20.60. (a) Schematic setup of optically pumped semiconductor laser (OPSL). The semiconductor chip consists of a Bragg mirror on the bottom, multiple quantum wells and an antireﬂection coating on the top. Adapted from [698]. (b) OPSL source (488 nm, 20 mW, footprint: 125 × 70 mm2 ). Reprinted with permission from [699]
20.4.16 Quantum Cascade Lasers In a quantum cascade laser (QCL), the gain stems from an intersubband transition. The concept was conceived in 1971 [700, 701] and realized in 1994 [660]. In Fig. 20.61a, the schematic conductionband structure at operation is shown. The injector supplies electrons into the active region. The electron is removed quickly from the lower level in order to allow inversion. The electron is then extracted into the next injector. The laser medium consists of several such units as shown in Fig. 20.61b. Since every unit can deliver a photon per electron (with eﬃciency η1 ), the total quantum eﬃciency of N units η = N η1 can be larger than 1. The emission wavelength is in the far or midinfrared, depending only on the designed layer thicknesses and not on the bandgap of the material (Fig. 20.61d). In the midinf